Now in its third edition, Fundamentals of Microfabrication and Nanotechnology continues to provide the most complete MEM
122 68 330MB
Pages [1983] Year 2011
Table of contents :
Volume I
Introduction
Historical Note: The Ascent of Silicon, MEMS, and NEMS
Crystallography
Quantum Mechanics and the Band Theory of Solids
Silicon Single Crystal Is Still King
Photonics
Fluidics
Electrochemical and Optical Analytical Techniques
Index
Volume II
Part I: Lithography
Introduction to Part I
Photolithography
NextGeneration Lithographies and Lithography Research
Part II: Pattern Transfer with Subtractive Techniques
Introduction to Part II
Dry Etching
Wet Chemical Etching and Wet Bulk MicromachiningPools as Tools
Thermal EnergyBased Removing
MechanicalEnergyBased Removing
Part III: Pattern Transfer with Additive Techniques
Introduction to Part III
Physical and Chemical Vapor DepositionThin Film Properties and Surface Micromachining
Chemical, Photochemical, and Electrochemical Forming Techniques
Thermal EnergyBased Forming TechniquesThermoforming
10 Micromolding TechniquesLIGA
Index
Volume III
Part I: From Traditional Manufacturing to Nanotechnology
Introduction to Part I
NonlithographyBased (Traditional) and LithographyBased (Nontraditional) Manufacturing Compared
Nature as an Engineering Guide: Biomimetics
Nanotechnology: TopDown and BottomUp Manufacturing Approaches Compared
Packaging, Assembly, and SelfAssembly
Selected Materials and Processes for MEMS and NEMS
6 Metrology and MEMS/NEMS Modeling 285
Part II: Scaling Laws, Actuators, and Power and Brains in Miniature Devices
Introduction to Part II
Scaling Laws
Actuators
Power and Brains in Miniature Devices
Part III: Miniaturization Application
Introduction to Part III
MEMS and NEMS Applications
Index
Third Edition
Fundamentals of
MICRO~ABRICATION
~DNANOTECHNOLOGY VOLUME I
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Third Edition
Fundamentals of
MICROFABRICATION AND
NANOT~CHNOlOGY VOLUME I
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
J. Madou Marc J.
Boca Raton London New York
CRC Press is an imprint of the Taylor & Francis Group, an informa business
CRC Press Taylor & Francis Group 6000 Broken Sound Parkway NW, Suite 300 Boca Raton, FL 334872742 © 2012 by Taylor & Francis Group, LLC CRC Press is an imprint of Taylor & Francis Group, an Informa business No claim to original U.S. Government works Printed in the United States of America on acidfree paper International Standard Book Number: 9781420055115 (Hardback) This book contains information obtained from authentic and highly regarded sources. Reasonable efforts have been made to publish reliable data and information, but the author and publisher cannot assume responsibility for the validity of all materials or the consequences of their use. The authors and publishers have attempted to trace the copyright holders of all material reproduced in this publication and apologize to copyright holders if permission to publish in this form has not been obtained. If any copyright material has not been acknowledged please write and let us know so we may rectify in any future reprint. Except as permitted under U.S. Copyright Law, no part of this book may be reprinted, reproduced, transmitted, or utilized in any form by any electronic, mechanical, or other means, now known or hereafter invented, including photocopying, microfilming, and recording, or in any information storage or retrieval system, without written permission from the publishers. For permission to photocopy or use material electronically from this work, please access www.copyright.com (http://www.copyright.com/) or contact the Copyright Clearance Center, Inc. (CCC), 222 Rosewood Drive, Danvers, MA 01923, 9787508400. CCC is a notforprofit organization that provides licenses and registration for a variety of users. For organizations that have been granted a photocopy license by the CCC, a separate system of payment has been arranged. Trademark Notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identification and explanation without intent to infringe. Visit the Taylor & Francis Web site at http://www.taylorandfrancis.com and the CRC Press Web site at http://www.crcpress.com
I dedicate this third edition of Fundamentals of Microfabrication to my family in the US and in Belgium and to all MEMS and NEMS colleagues in labs in the US, Canada, India, Korea, Mexico, Malaysia, Switzerland, Sweden and Denmark that I have the pleasure to work with. The opportunity to carry out international research in MEMS and NEMS and writing a textbook about it has been rewarding in terms of research productivity but perhaps even more in cultural enrichment. Scientists have always been at the frontier of globalization because science is the biggest gift one country can give to another and perhaps the best road to a more peaceful world.
Contents Roadmap Author Acknowledgments
ix xi xiii
INTRODUCTION MEMS and NEMS Foundations Introduction
1 Historical Note: The Ascent of Silicon, MEMS, and NEMS
2
5
2 Crystallography
37
3 Quantum Mechanics and the Band Theory of Solids
75
4 Silicon Single Crystal Is Still King
215
5 Photonics
299
6 Fluidics
435
7 Electrochemical and Optical Analytical Techniques
517
Index
631
vii
Roadmap In SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology we lay the foundations for a qualitative and quantitative theoretical understanding of micro and nanoelectromechanical systems, i.e., MEMS and NEMS. In integrated circuits (ICs), MEMS, and NEMS, silicon (Si) is still the substrate and construction material of choice. A historical note about the ascent of silicon, MEMS and NEMS is the topic of Chapter 1. The necessary solidstate physics background to understanding the electronic, mechanical, and optical properties of solids relied on in ICs, MEMS and NEMS is covered in Chapters 2–5. Many important semiconductor devices are based on crystalline materials because of their reproducible and predictable electrical properties. We cover crystallography in Chapter 2. The ultimate theory in modern physics today to predict physical, mechanical, chemical, and electrical properties of atoms, molecules, and solids is quantum mechanics. Quantum mechanics and the band theory of solids are presented in Chapter 3. The relevance of quantum mechanics in the context of ICs and NEMS cannot be underestimated, and the profound implications of quantum physics for nanoelectronics and NEMS are a recurring topic throughout this book. Given the importance of singlecrystal Si (SCS) for IC, MEMS, and NEMS applications, we analyze silicon crystallography and band structure in more detail in Chapter 4. This chapter also elucidates all the singlecrystal Si properties that conspired to make Si so important in electronic, optical, and mechanical devices that one might rightly call the second half of the 20th century the Silicon Age. Photonics, treated in Chapter 5, involves the use of radiant energy and uses photons the same way that electronic applications use electrons. We review the distinctive optical properties of bulk 3D metals, insulators, and semiconductors and summarize effects of electron and photon confinement in lowerdimensional structures. We show how evanescent fields on metal surfaces enable the guiding of light below the diffraction limit in plasmonics. Plasmonics is of growing importance for use in submicron lithography, nearfield optical microscopy, enhancement of light/matter interaction in sensors, highdensity data storage, and highly integrated optic chips. We also delve into the fascinating new topic of metamaterials, manmade structures with a negative refractive index, and explain how this could make for perfect lenses and could change the photonic field forever. In Chapter 6 we introduce fluidics, compare various fluidic propulsion mechanisms, and discuss the influence of miniaturization on fluid behavior. Given the high level of interest, fluidics for miniaturized analytical equipment is covered in this chapter as well. Chapter 7 combines a treatise on electrochemical and optical analytical processes whose implementation is often attempted in miniaturized components and systems. Note to the Reader: SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology was originally composed as part of a larger book that has since been broken up into three separate volumes. SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology represents the first volume in this set. The other two volumes include Manufacturing Techniques for Microfabrication and Nanotechnology and From MEMS to BioNEMS: Manufacturing Techniques and Applications. Crossreferences to these books appear throughout the text and will be referred to as Volume II and Volume III, respectively. The interested reader is encouraged to consult these volumes as necessary.
ix
Author Dr. Madou is the Chancellor’s Professor in Mechanical and Aerospace Engineering (MEA) at the University of California, Irvine. He is also associated with UC Irvine’s Department of Biomedical Engineering and the Department of Chemical Engineering and Materials Science. He is a Distinguished Honorary Professor at the Indian Institute of Technology, Kanpur, India and a World Class University Scholar (WCU) at UNIST in South Korea. Dr. Madou was Vice President of Advanced Technology at Nanogen in San Diego, California. He specializes in the application of miniaturization technology to chemical and biological problems (bioMEMS). He is the author of several books in this burgeoning field he helped pioneer both in academia and in industry. He founded several micromachining companies. Many of his students became well known in their own right in academia and through successful MEMS startups. Dr. Madou was the founder of the SRI International’s Microsensor Department, founder and president of Teknekron Sensor Development Corporation (TSDC), Visiting Miller Professor at UC Berkeley, and Endowed Chair at the Ohio State University (Professor in Chemistry and Materials Science and Engineering). Some of Dr. Madou’s recent research work involves artificial muscle for responsive drug delivery, carbonMEMS (CMEMS), a CDbased fluidic platform, solidstate pH electrodes, and integrating fluidics with DNA arrays, as well as labelfree assays for the molecular diagnostics platform of the future. To find out more about those recent research projects, visit http://www.biomems.net.
xi
Acknowledgments I thank all of the readers of the first and second editions of Fundamentals of Microfabrication as they made it worthwhile for me to finish this completely revised and very much expanded third edition. As in previous editions I had plenty of eager reviewers in my students and colleagues from all around the world. Students were especially helpful with the question and answer books that come with the three volumes that make up this third edition. I have acknowledged reviewers at the end of each chapter and students that worked on questions and answers are listed in the questions sections. The idea of treating MEMS and NEMS processes as some of a myriad of advanced manufacturing approaches came about while working on a WTEC report on International Assessment Of Research And Development In Micromanufacturing (http://www.wtec.org/ micromfg/report/Microreport.pdf). For that report we travelled around the US and abroad to visit the leading manufacturers of advanced technology products and quickly learned that innovation and advanced manufacturing are very much interlinked because new product demands stimulate the invention of new materials and processes. The loss of manufacturing in a country goes well beyond the loss of only one class of products. If a technical community is dissociated from manufacturing experience , such as making larger flatpanel displays or the latest mobile phones, such communities cannot invent and eventually can no longer teach engineering effectively. An equally sobering realization is that a country might still invent new technologies paid for by government grants, say in nanofabrication, but not be able to manufacture the products that incorporate them. It is naïve to believe that one can still design new products when disconnected from advanced manufacturing: for a good design one needs to know the latest manufacturing processes and newest materials. It is my sincerest hope that this third edition motivates some of the brightest students to start designing and making things again rather than joining financial institutions that produce nothing for society at large but rather break things.
xiii
INTRODUCTION
MEMS and NEMS Foundations Miniaturization science is the science of making very small things. In topdown micro and nanomachining, one builds down from large chunks of material; in bottomup nanochemistry, one builds up from smaller building blocks. Both require a profound understanding of the intended application, different manufacturing options, materials properties, and scaling laws. The resulting threedimensional structures, ranging in size from subcentimeters to subnanometers, include electronics, photonics, sensors, actuators, micro and nanocomponents, and microand nanosystems.
(a)
(b)
(a) Copper Fermi surface—FCC sixth band with eight short necks touching the eight hexagonal zone faces. (Fermi surface database at http://www.phys.ufl.edu/ fermisurface.) (b) Platinum Fermi surface—FCC fourth, fifth, and sixth bands. (Fermi surface database at http://www.phys.ufl.edu/fermisurface.)
2
MEMS and NEMS Foundations
No one behind, no one ahead. The path the ancients cleared has closed. And the other path, everyone’s path, easy and wide, goes nowhere. I am alone and find my way. Dharmakirti (7th century India)
Introduction Chapter 1 Historical Note: The Ascent of Si, MEMS, and NEMS Chapter 2 Crystallography Chapter 3 Quantum Mechanics and the Band Theory of Solids Chapter 4 Silicon Single Crystal Is Still King Chapter 5 Photonics Chapter 6 Fluidics Chapter 7 Electrochemical and Optical Analytical Techniques
Introduction In Volume I, we lay the foundations for a qualitative and quantitative understanding of micro and nanoelectromechanical systems, i.e., MEMS and NEMS. In integrated circuits (ICs), MEMS, and NEMS, silicon (Si) is still the substrate and building material of choice. A historical note about the history of the ascent of silicon, MEMS, and NEMS is the topic of Chapter 1. The necessary solidstate physics background of electronic, mechanical, and optical properties of solids relied on in MEMS and NEMS is covered in Chapters 2–5. Solidstate physics is the study of solids. A major part of solidstate physics is focused on crystals because the periodicity of atoms in a crystal facilitates mathematical modeling, but more importantly because crystalline materials often have electrical, optical, or mechanical properties that can be easier exploited for engineering purposes. In Chapter 2, we detail crystalline materials in which atoms are arranged in a pattern that repeats periodically in three dimensions. The materials covered here prepare the reader for Chapter 3, which explains the band theory of solids based on quantum mechanics. The relevance of quantum
mechanics in the context of ICs and NEMS cannot be underestimated, and the profound implications of quantum physics for nanoelectronics and NEMS is a recurring topic throughout this book. This is followed in Chapter 4 by a description of the singlecrystal Si band structure, the growth of single crystals of Si, its doping, and oxidation. In this chapter, we also review the singlecrystal Si properties that conspired to make Si so important in electronic, optical, and mechanical devices so that one might rightly call the second half of the 20th century the Silicon Age. Although the emphasis in this book is on nonelectronic applications of miniaturized devices, we briefly introduce different types of diodes and two types of transistors (bipolar and MOSFET). In Chapter 5, we introduce photonics. We compare electron and photon propagation in materials and contrast electron and photonic confinement structures and the associated evanescent wave phenomena. We also delve into the fascinating new topic of metamaterials, artificially engineered materials possessing properties (e.g., optical, electrical) that are not encountered in naturally occurring ones. An introduction to diode lasers, quantum well lasers, and quantum cascade lasers concludes the photonics section. Fluidics and electrochemical and optical analytical techniques are important current applications of MEMS and NEMS. In Chapter 6 we introduce fluidics, compare various fluidic propulsion mechanisms, and discuss the influence of miniaturization on fluid behavior. Given the current academic and industrial interest, fluidics in miniaturized analytical equipment is detailed separately at the end of this chapter. Chapter 7 combines a treatise on
STM image showing standing waves in a 2D electron gas trapped in a “quantum corral” made by positioning Fe atoms on a Cu (111) surface.1
MEMS and NEMS Foundations
electrochemical and optical analytical techniques. Using sensor examples, we introduce some of the most important concepts in electrochemistry, i.e., the electrical double layer, potentiometry, voltammetry, two and threeelectrode systems, Marcus’ theory of electron transfer, reaction rate and diffusion ratecontrolled electrochemical reactions, and ultramicroelectrodes. Many researchers use MEMS and NEMS to miniaturize optical components or whole instruments for absorption, luminescence, or phosphorescence spectroscopy. Optical spectroscopy is concerned with the production, measurement, and interpretation of electromagnetic
3
spectra arising from either emission or absorption of radiant energy by matter. The sensitivity of these optical sensing techniques and the analysis of how amenable they are to miniaturization (scaling laws) are also compared herein. Chapter 7 ends with a comparison of the merits and problems associated with electrochemical and optical measuring techniques.
Reference 1. Crommie, M. F., C. P. Lutz, and D. M. Eigler. 1993. Confinement of electrons to quantum corrals on a metal surface. Science 262:218–20.
1 Historical Note: The Ascent of Silicon, MEMS, and NEMS Outline Silicon in Integrated Circuits MEMS NEMS Acknowledgments Appendix 1A: International Technology Roadmap for Semiconductors (ITRS) Appendix 1B: Worldwide IC and Electronic Equipment Sales
Silicon Valley is the only place on Earth not trying to figure out how to become Silicon Valley (Robert Metcalfe, father of the ethernet). (From PG&E and USGS.)
Questions References
Silicon in Integrated Circuits In 1879, William Crookes recounted his experiments on passing electric discharges through an evacuated glass tube for the Royal Society, thus describing the first cathode ray tube (CRT). Four years later, Thomas Alva Edison and Francis Upton discovered the “Edison effect.” They introduced a metal plate into an incandescent electric light bulb (invented by Edison in 1879) in an attempt to keep the bulb from turning black (Figure 1.1). It did not work, but they discovered that there was a current between the lighted filament and the separate metal plate when the plate was positively charged but not when it was negatively charged. This led Edison and Upton to stumble on the basic principle of the operation of the vacuum tube (rectification!). The first diode tube we owe to John Fleming, who, in 1904, filed a patent for a “valve” vacuum tube, also called a Fleming valve or Fleming diode. 5
6
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
FIGURE 1.1 Edison bulb used to demonstrate the “Edison effect.”
Early researchers thought of electricity as a kind of fluid, leading to the inherited jargon such as current, flow, and valve. Fleming recognized the importance of Edison and Upton’s discovery and demonstrated it could be used for the rectification of alternating currents. Interestingly, Fleming, at first, tried to get reliable rectification from singlecrystal rectifiers used in crystal set radios (Figure 1.2), but could never get them to work well enough, so he switched to tubes! J.J. Thomson, in 1887, convincingly showed that an electrical current was really an electron flow, and Fleming could explain the rectification in his diode tube as electrons boiling of the heated filament and flowing to the metal plate (thermionic emission). Because the plate was not hot enough to emit electrons, no current could go in the opposite direction. Thus, the Edison effect always produced direct
FIGURE 1.2 Early crystal set radio with a galena (lead sulphide) and the “cat’s whisker” (the small coil of wire) that was used to make contact with the crystal.
FIGURE 1.3 Lee De Forest in 1906 with the Audion, the first triode.
current only. In 1906, an American scientist, Lee De Forest (Figure 1.3), invented the vacuum tube amplifier or triode based on the twoelement vacuum tube invented by Fleming. De Forest, reportedly a tireless selfpromoter, added an electrode—the grid—to the Fleming diode, and inserted it between the anode and the cathode. With this grid the diode became an active device, i.e., it could be used for the amplification of signals (say, for example, in radios) and as a switch (for computers). Hence, the amplifying vacuum tube, the ancestor of the transistor, was born. A gate in a dam controls huge amounts of flowing water with relatively small movements. Similarly, a small signal applied to the grid controls the much larger signal between anode and cathode. Vacuum tubes—miniature particle accelerators— dominated the radio and television industries until the 1960s, and were the genesis of today’s huge electronics industry. However, tubes were fragile, large, very power hungry, and costly to manufacture. The industry needed something better. That today’s world is largely electronic—e.g., automobiles, home appliances, even books, writing tablets, and tally sheets—is because of solidstate electronics,* not vacuum tubes. It is true, albeit unfortunate, that World War II and the subsequent Cold War era is what spurred research and development in solidstate electronic devices. Human foibles led to faster development of *
Based on or consisting chiefly or exclusively of semiconducting materials, components, and related devices.
Historical Note
RAdio Detecting And Ranging or RADAR, SOund Navigation And Ranging or SONAR, and many other technological innovations. As we all know, the list of innovations made to feed human aggression did not abate. Alan Turing led the team in England that in 1943 built the Colossus coding and deciphering machine. The Colossus was a specialpurpose computer used to break the German code ULTRA, encrypted using ENIGMA machines. Breaking the German code was one of the keys to the success of the DDay invasion. The Harvard Mark I and later II, III, and IV were generalpurpose electromechanical calculators (sponsored by the U.S. Navy) to compute artillery and navigation tables—the same purpose intended, 100 years earlier, by Babbage for his analytical engine (Figure 1.4). John Mauchly and Presper Eckert started work on the first electronic computer, the ENIAC (Electronic Numerical Integrator and Computer), at the University of Pennsylvania in 1943. The ENIAC, having been a secret during the war, was unveiled in Philadelphia in 1946. This computer featured 17,468 vacuum tubes used as switches and consumed 174 kW of power, enough to light 10 homes! Several tubes would fail every day until the engineers decided to never turn off the machine. This increased the average time until a tube would fail to 2 days. ENIAC was designed to calculate munition trajectory tables for the U.S. Army. It was Ushaped, 25 m long, 2.5 m high, 1 m wide, and weighed more than 30 tons (see Figure 1.5a). Programming was done by plugging cables and setting switches. By the mid1970s, identical ENIAC functions could be achieved by a
(a)
7
FIGURE 1.4 Charles Babbage (1791–1871) first conceived the idea of an advanced calculating machine to calculate and print mathematical tables in 1812. It was a decimal digital machine, with the value of a number being represented by the positions of toothed wheels marked with decimal numbers.
1.5 × 1.5cm silicon die, and the original Pentium processor, if fabricated using ENIAC technology, would cover more than 10 square miles. One of ENIAC’s heirs was a computer called the UNIVAC (Universal Automatic Computer), considered by most historians to be the first commercially successful digital computer (Figure 1.5b). First constructed by the EckertMauchly Computer Corporation (EMCC), it was taken over by SperryRand. At 14.5 ft. long, 7.5 ft. high, and 9 ft. wide, the UNIVAC, priced at $1 million, was physically
(b)
FIGURE 1.5 Electronic Numerical Integrator and Computer (ENIAC), the world’s first largescale, generalpurpose electronic computer (a), and the UNIVAC, the first commercial computer (b). Firstgeneration computers based on vacuum tubes.
8
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
FIGURE 1.6 Von Neumann in his living room. (Photograph by Alan Richards hanging in Fuld Hall, Institute for Advanced Study, Princeton, NJ. Courtesy of the Archives of the Institute for Advanced Study.)
smaller than ENIAC but more powerful. ENIAC and UNIVAC constitute firstgeneration computers based on vacuum tubes. It was the concept of the stored program, invented by John von Neumann in 1945 (Figure 1.6); the magnetic core memory, invented by An Wang at Harvard and used in grids by J.W. Forrester and colleagues at MIT for random access memory (RAM); and William Shockley’s transistor, based on transistors for switches instead of tubes, that would make a second generation of computers possible, thus starting the computer revolution. The year 1940 gave rise to an important milestone in solidstate electronics history with the invention of a siliconbased solidstate pn junction diode by Russell Ohl at Bell Labs.1 This device, when exposed to light, produced a 0.5 V across the junction and represented the first Sibased solar cell. Bell Labs, in 1945, established a group charged with developing an alternative to the vacuum tube. Led by Shockley (1910–1989) and including John Bardeen (1908– 1991) and Walter Brattain (1902–1987), in 1947 the group made an oddlooking device consisting of semiconducting germanium (Ge), gold strips, insulators, and wires, which they called a transistor (subject of U.S. Patent #2,524,035 [1950]2) (Figure 1.7; notice the paper clip!). For this invention Shockley, Bardeen, and Brattain were awarded the 1956 Nobel
FIGURE 1.7 The first pointcontact germanium bipolar transistor. Notice the paper clip! Roughly 50 years later, electronics accounted for 10% ($4 trillion) of the world’s aggregate GDP.
Prize for Physics (Bardeen went on to claim a second Nobel Prize for Physics in 1972 for superconductivity). Bardeen called Ohl’s junction diode fundamental to the invention of the transistor. Brattain was the unassuming experimentalist, Bardeen the theorist, and Shockley* the inventor and leader (Figure 1.8). This trio thus succeeded in creating an amplifying circuit using a pointcontact bipolar transistor that transferred resistance (hence transistor). Two
FIGURE 1.8 Shockley (seated), Bardeen, and Brattain.
*
Unfortunately, Shockley became associated with racist ideas and briefly pursued a U.S. Senate seat (as a Republican).
Historical Note
wires made contact with the germanium crystal near the junction between the p and nzones just like the “cat whiskers”* in a crystal radio set. A few months later, Shockley devised the junction transistor, a true solidstate device that did not need the whiskers of the pointcontact transistor (see also Figure 1.2). Junction transistors were much easier to manufacture than pointcontact transistors, and by the mid1950s the former had replaced the latter in telephone systems. G. Teal and J.B. Little, also from Bell Labs, were able to grow large single crystals of germanium by 1951, which led to the start of commercial production of germanium transistors in the same year. Christmas 1954 saw the first transistor radio (the Regency TR1) built by Industrial Development Engineering Associates, which sold for $49.95 (Figure 1.9). This radio featured four germanium transistors from Texas Instruments. Although germanium was used in early transistors, by the late 1960s silicon, because of its many advantages, had taken over. Silicon has a wider bandgap (1.1 eV for Si vs. 0.66 eV for Ge), allowing for higher operating temperatures (125–175°C vs. 85°C), a higher intrinsic resistivity (2.3 × 105 Ω cm vs. 47 Ω cm), and a better native oxide (SiO2 vs. GeO2 [water soluble!]).
FIGURE 1.9 Movie producer mogul Michael Todd (husband of Elizabeth Taylor in the mid1950s) placed Regency TR1s in gift books to commemorate his movie Around the World in 80 Days. The one pictured was for Shirley MacLaine.
*
A cat whisker is a piece (often springy) of pointed metal wire.
9
The latter results in a higherquality insulator that protects and “passivates” underlying circuitry, helps in patterning, and is useful as a mask for dopants. Finally, silicon is cheaper and much more abundant (sand!) than germanium. Secondgeneration computers relied on transistors instead of vacuum tubes for switches (logic gates). In recent years, germanium is making a comeback based mostly on its higher carrier mobility (three times higher than siliconbased ones), of great interest for faster circuitry, and because Ge has a lattice constant similar to GaAs, making it easier to integrate GaAs optical components with GeCMOS circuits. Transistors perform functions similar to vacuum tubes, but they are much smaller, cheaper, less power hungry, and more reliable. Michael Riordan and Lillian Hoddeson’s Crystal Fire gives, in the author’s opinion, one of the best popular accounts of the invention of the transistor.3 The honeymoon with the transistor was quickly over; by the second half of the 1950s, new circuits on the drawing board were so big and complex that it was virtually impossible to wire that many different parts together reliably. A circuit with 100,000 components could easily require 1 million, mostly manual, soldering operations that were time consuming, expensive, and inherently unreliable. The answer was the “monolithic” idea, in which a single bloc of semiconductor is used for all the components and interconnects, invented by two engineers working at competing companies: Jack Kilby at Texas Instruments (Figure 1.10) and Robert Noyce (Figure 1.11) at Fairchild Semiconductor. In 1958, Jack Kilby at Texas Instruments formed a complete circuit on a piece of germanium, landing U.S. Patent #3,138,743 (1959). His circuit was a simple IC oscillator with three types of components: transistors, resistors, and capacitors (Figure 1.12). Kilby got his welldeserved Nobel Prize for this work only in 2000. Technological progress and engineering feats are not often awarded a Nobel Prize, and if awarded at all they are often belated or controversial (see Kary Mullis, Nobel Laureate Chemistry 1993 for the invention of PCR). Robert Noyce—Mr. Intel (Integrated Electronics)— then at Fairchild, introduced, with Jean Horni, planar technology, wiring individual devices together
10
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
FIGURE 1.12 The first integrated circuit (germanium) in 1958 by Jack S. Kilby at Texas Instruments contained five components of three types: transistors, resistors, and capacitors.
FIGURE 1.10 Jack Kilby with notebook. (TI downloadable pictures.)
on a silicon wafer surface. Noyce’s “planar” manufacturing, in which all the transistors, capacitors, and resistors are formed together on a silicon chip with the metal wiring embedded on the silicon, is still used today. By 1961, Fairchild and Texas Instruments had devised methods whereby large
FIGURE 1.11 Robert Noyce in 1990.
numbers of transistors were produced on a thin slice of Si—and IC production on an industrial scale took off. The transistors on ICs were not the bipolar type but rather field effect transistor devices. The concept of a field effect transistor (FET) was first proposed and patented in the 1930s; however, it was the bipolar transistor that made it first to commercial products. Shockley resurrected the idea of the FET in the early 1950s, but it took until 1962 before a working FET was fabricated. These new FETs proved to be more compatible with both IC and Si technology. Integrated circuits made not only thirdgeneration computers possible but also cameras, clocks, PDAs, RFIDs, etc. The National Academy of Sciences declared ICs the progenitor of the “Second Industrial Revolution,” and Jerry Sanders, founder of Advanced Microdevices, Inc., called ICs the crude oil of the 1980s. A very wellwritten popular account of the invention of the IC is T.R. Reid’s The Chip: How Two Americans Invented the Microchip and Launched a Revolution.4 Robert Noyce, Gordon Moore, and Andrew Grove left Fairchild to start Intel in 1968 with the aim of developing random access memory (RAM) chips. The question these inventors wanted answered was this: since transistors, capacitors, and resistors can be put on a chip, would it be possible to put a computer’s central processor unit (CPU) on one? The answer came swiftly; by 1969 Ted Hoff had designed the Intel 4004, the first generalpurpose 4bit microprocessor. The Intel 4004 microprocessor was a 3chip set with a 2kbit readonly memory (ROM) IC, a 320bit RAM
Historical Note
11
FIGURE 1.13 (a) The Altair 8800 computer and (b) the Intel 8080 microprocessor.
IC, and a 4bit processor, each housed in a 16pin dual inline package (DIP). The processor, made in a 10μm silicon gate pMOS process, contained 2,250 transistors and could execute 60,000 operations per second on a die size of 13.5 mm2. It came on the market in 1971, giving rise to the fourth generation of computers based on microprocessors and the first personal computer (PC). The era of a computer in every home—a favorite topic among science fiction writers—had arrived! The first desktopsize PC appeared in 1975, offered by Micro Instrumentation Telemetry Systems (MITS) as a mailorder computer kit. The computer, the Altair 8800, named after a planet on a Star Trek episode, retailed for $397. It had an Intel 8080 microprocessor, 256 bytes of memory (not 256K), no keyboard, no display, and no auxiliary storage device, but its success was phenomenal, and the demand for the microcomputer kit was overwhelming (Figure 1.13). Scores of small entrepreneurial companies responded to this demand by producing computers for the new market. In 1976, Bill Gates, Paul Allen, and Monte Davidoff wrote their first software program for the Altair—a BASIC (Beginners Allpurpose Symbolic
Instruction Code) interpreter (a highlevel language translator that converts individual highlevel computer language program instructions [source code] into machine instructions). The first major electronics firm to manufacture and sell personal computers, Tandy Corporation (Radio Shack), introduced its computer model (TRS80) in 1977. It quickly dominated the field because of the combination of two attractive features: a keyboard and a cathode ray display terminal. It was also popular because it could be programmed, and the user was able to store information by means of a cassette tape. In 1976, Steve Wozniak, who could not afford an Altair, built his own computer using a cheaper microprocessor and adding several memory chips. As a circuit board alone, it could do more than the Altair. Wozniak and Steve Jobs called it Apple I, and Jobs took on the task of marketing it while Wozniak continued with improvements (Figure 1.14). By 1977, Wozniak had built the Apple II and quit his day job. The Apple II had 16–64K RAM and secondary memory storage in the shape of a cassette tape or a 5.25in. floppy disk drive and cost $1,300. At that time, Wozniak and Jobs formed Apple Computer,
FIGURE 1.14 (a) Jobs and Wozniak with the board for Apple I and (b) the Apple II.
12
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Inc. When it went public in 1980, its stock value was $117 million; three years later it was worth $985 million. Vacuum tubes coexisted with their progeny, the transistor, and even with ICs for a short while. Although solidstate technology overwhelmingly dominates today’s world of electronics, vacuum tubes are still holding out in some areas. You might, for example, still have a CRT (cathode ray tube) as your television or computer screen. Tubes also remain in two small but vibrant areas for entirely different reasons. The first involves microwave technology, which still relies on vacuum tubes for their powerhandling capability at high frequencies. The other—the creation and reproduction of music—is a more complicated story. Tubes distort signals differently than transistors when overdriven, and this distortion is regarded as being more “pleasant” by much of the music community. Extrapolating back to 1961, Gordon Moore in 1965 (Figure 1.15), while at Fairchild, predicted that transistors would continue to shrink, doubling in density on an IC every 18–24 months, while the price would continue to come down—this prediction we know today as Moore’s Law. History has proven Moore right as evidenced by past and projected feature sizes of ICs in the International Technology Roadmap for Semiconductors (ITRS) shown in Appendix 1A and on the Internet at http://public.itrs.net (updated in 2007).5 In this International Technology Roadmap
TABLE 1.1 Integration Scale and Circuit Density IC Evolution Zeroscale integration Smallscale integration Mediumscale integration Largescale integration Very largescale integration Ultralargescale integration Gigascale integration Terascale integration
Number of Logic Gates
Year of Introduction
ZSI
1
1950
SSI
2–30
1965
MSI
30–103
1970
LSI
103–105
1980
VLSI
105–107
1985
ULSI
107–109
1990
GSI
109–1011
2005
TSI
1011–1013
2020
for Semiconductors, technology modes have been defined. These modes are the feature sizes that have to be in volume manufacturing at a fixed date (year of production). The feature size is defined as halfpitch, i.e., half of a dense pair of lines and spaces (see figure in Appendix 1A). In Table 1.1 the increasing numbers of devices integrated on an IC are tabulated. As we will learn in Chapters 1 and 2 on lithography in Volume II, new lithography techniques, novel device structures, and the use of new materials drive Moore’s Law. The state of the art in ICs today is a 2GB DRAM* with 60nm features (Samsung). Intel introduced the Core 2 Quad “Kentsfield” chip in January 2007, a chip featuring a 65nanometer technology mode. The 32nm node should be achieved in 2009. The first Moore’s Law is the good news, but there is a second Moore’s Law that is a bit problematic; this second law states that the cost of building a chip factory doubles with every other chip generation, i.e., every 36 months. Today’s technology involves Si wafers with a 12in. diameter and factories that cost $3–4 billion to construct. With this type of startup costs, few countries can afford to enter the IC market, and the search is on for alternative, lessexpensive *
FIGURE 1.15 Gordon Moore, cofounder of Intel.
Acronym
Dynamic random access memory. A type of memory component used to store information in a computer system. “Dynamic” means the DRAMs need a constant “refresh” (pulse of current through all the memory cells) to keep the stored information.
Historical Note
13
bottomup NEMS techniques (below). From Appendix 1B, the IC market for 2003 was $166 billion worldwide, with 2004 projected at $241 billion (data by the World Semiconductor Trade Statistics [WSTS]; http://www.wsts.org).6 Also from Appendix 1B we learn that the IC business is feeding a trilliondollar electronic equipment business. It is worth pointing out that China is expected to control 5% of the IC market by 2010.
MEMS Singlecrystal silicon is not only an excellent electronic material but it also exhibits superior mechanical properties; the latter gave birth to the microelectromechanical systems (MEMS) field on the coattails of the IC industry. Originally MEMS constituted mostly mechanical types of devices based on singlecrystal silicon with at least one or more of their dimensions in the micrometer range. As MEMS applications broadened, in Europe the acronym MST for microsystem technology became more popular. In Japan one refers to micromachining, and microengineering is popular in the United Kingdom. Development of singlecrystal silicon mechanical MEMS involves the fabrication of micromechanical parts, e.g., a thin membrane in the case of a pressure sensor or a cantilever beam for an accelerometer. These micromechanical parts are fabricated by selectively etching areas of a Si substrate away to leave behind the desired geometries. The terms MEMS and micromachining came into use in 1982 to name these fabrication processes. Around the same time references to “bulk” micromachining techniques also appeared. Richard Feynman’s December 26, 1959 presentation “There’s Plenty of Room at the Bottom” is considered by many to be the starting bongo for MEMS (Figure 1.16) (http://www.its. caltech.edu/~feynman/plenty.html),7 but in a practical sense, it was the invention of the transistor and the processes developed to fabricate transistors, six years earlier, that enabled MEMS. An early milestone for the use of singlecrystal silicon in MEMS was the 1956 discovery of porous Si by Uhlir.8 His discovery eventually led to all types of interesting new, singlecrystal Sibased devices, from reference electrodes for electrochemical sensors,
FIGURE 1.16 Richard Feynman on the bongo drums.
biosensors, quantum structures, and permeable membranes to photonic crystals and photoluminescent and electroluminescent devices. The first impetus for the use of singlecrystal silicon as a micromechanical element in MEMS can be traced to the discovery of its large piezoresistance. Piezoresistance is the change in the resistivity of certain materials as a result of an applied mechanical strain. Charles Smith, of the Case Institute of Technology (now part of the Case Western Reserve University), during a sabbatical leave at Bell Labs in 1953, studied the piezoresistivity of semiconductors and published the first paper on the piezoresistive effect in Si and Ge in 1954.9 The piezoresistive coefficients Smith measured demonstrated that the gauge factor* of Si and Ge strain gauges (see Figure 1.17) was 10–20 times larger than the gauge factor of metal film strain gauges, and, therefore, semiconductor gauges were expected to be much more sensitive. Motivated by these results, companies such as Kulite and Honeywell started developing Si strain gauges commercially from 1958 onward. Pfann and colleagues, in 1961, proposed a dopant diffusion technique for the fabrication of silicon piezoresistive sensors for the measurement of stress, strain, and pressure.10 Based on this idea, Kulite integrated *
A strain gauge is a device used to measure deformation (strain) of an object. The gauge factor of a strain gauge relates strain to change in electrical resistance.
14
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
1.0 mm
FIGURE 1.17 The Si singlecrystal gauge element can be seen as the vertical bar centered between the two solder pads. The singlecrystal silicon strain gauge offers sensitivities 20–50 times greater than metal foil gauges. A microphotograph of the LN100. (BF Goodrich Advanced Micro Machines.)
Si strain gauges on a thin Si substrate with diffused resistors in 1961. As early as 1962, Tufte and coworkers at Honeywell, using a combination of wet isotropic etching, dry etching (using a plasma instead of a solution), and oxidation, made the first thin Si piezoresistive diaphragms for pressure sensors.11 Isotropic etching of Si had been developed earlier for transistor fabrication. In the mid1960s, Bell Labs started work on singlecrystal silicon etchants with directional preferences, i.e., anisotropic etchants, such as mixtures of, at first, KOH, water, and alcohol and later KOH and water.12 Both chemical and electrochemical anisotropic etching methods were pursued. The aspect ratio (heighttowidth ratio) of features in MEMS is typically much higher than in ICs (Figure 1.18). The first highaspectratio cuts in
“CMOS”
Released beam
110 μm
5–50 μm
0.5–1 μm
0.251.0 μm
VLSI/ULSI < 1:1 Aspect ratio (a)
“Bulk MEMS motor” (b) > 1:1 Aspect ratio
MEMS
FIGURE 1.18 Aspect ratio (heighttowidth ratio) typical in (a) fabrication of integrated circuits and (b) microfabricated component.
FIGURE 1.19 Isotropic and anisotropic etching profiles in singlecrystal Si. Isotropic etching of grooves in (100) Si (a) and anisotropic etching of grooves in (100) Si (b) using rectangular mask openings. Features are in the 100μm range.
silicon were used in the fabrication of dielectrically isolated structures in ICs such as those for beam leads. In the mid1970s, a surge of activity in anisotropic etching was associated with the work on Vgroove and Ugroove transistors. Isotropic and anisotropic etching profiles are compared in Figure 1.19. Figure 1.19a shows the isotropic etching of grooves in (100) Si, and Figure 1.19b shows the anisotropic etching of grooves in (100) Si. In both cases, rectangular mask openings are used. Most singlecrystal silicon MEMS devices feature bonding of one Si wafer to another or to a differing substrate, say a glass pedestal, and some MEMS involve cavitysealing techniques, perhaps for a vacuum reference or to accommodate a deflecting cantilever beam. The most prominent techniques developed to achieve these features are fieldassisted bonding, invented by Wallis and Pomerantz in 1969,13 and Si fusion bonding (SFB) by Shimbo in 1986.14 Fieldassisted thermal bonding, as shown in Figure 1.20, also known as anodic bonding, electrostatic bonding, or the Mallory process, is commonly used for joining glass to silicon at high temperatures (e.g., 400°C) and high voltages (e.g., 600 V). The ability to bond two Si wafers directly, at high temperatures (>800°C) in an oxidizing environment, without intermediate layers or applying an electric field, simplified the fabrication of many devices in silicon fusion bonding (SFB).
Historical Note
15
FIGURE 1.20 During anodic bonding, the negative potential applied to the borosilicate glass plate, which has been heated to 500°C, allows the migration of positive ions (mostly Na+) away from the wafer’s interface, creating a strong electric field between the glass and the Si wafer.
The first Si accelerometer was demonstrated in 1970 at Kulite. In 1972, Sensym became the first company to make standalone Si sensor products. By 1974, National Semiconductor Corporation, in California, carried an extensive line of Si pressure transducers as part of the first complete silicon pressure transducer catalog.15 Other early commercial suppliers of micromachined pressure sensor products were Foxboro/ICT, Endevco, Kulite, and Honeywell’s Microswitch. To achieve better sensitivity and stability than possible with piezoresistive pressure sensors, capacitive pressure sensors were first developed and demonstrated by Dr. James Angell at Stanford University around 1977.16 In Figure 1.21 we show a typical piezoresistive singlecrystal silicon pressure sensor, with the silicon sensor anodically bonded to a glass substrate. In many cases, it is desirable to stop the etching process when a certain cavity depth or a certain membrane thickness is reached. Highresolution silicon micromachining relies on the availability of effective etchstop layers rather than the use of a stopwatch to control the etch depth. It was the discovery/development of impuritybased etch stops in silicon that allowed micromachining to become a highyield commercial production process. The most widely used etchstop technique is based on the fact that anisotropic etchants do not attack heavily borondoped (p++) silicon layers. Selective p++ doping is typically implemented using gaseous or solid boron diffusion sources with a mask (such as silicon dioxide). The boron etchstop effect was
FIGURE 1.21 Piezoresistive pressure sensor featuring a Si/glass bond achieved by anodic bonding. The Bosch engine control manifold absolute pressure (MAP) sensor is used in automobile fuel injection systems. By measuring the manifold pressure, the amount of fuel injected into the engine cylinders can be calculated. Micromachined silicon piezoresistive pressure sensors are bonded at the wafer level to a glass wafer using anodic bonding before dicing. The glass pedestal that is created by this process provides stress isolation for the silicon sensor from packageinduced thermal stresses. (Photo courtesy of Robert Bosch GmbH, Germany.)
first noticed by Greenwood in 1969,17 and Bohg in 197118 found that an impurity concentration of about 7 × 1019/cm3 resulted in the anisotropic etch rate of Si decreasing sharply. Innovative, micromachined structures, different from the now mundane pressure sensors, accelerometers, and strain gauges, began to be explored by the mid to late 1970s. Texas Instruments produced a thermal print head in 1977,19 and IBM produced inkjet nozzle arrays the same year.20 In 1980, Hewlett Packard made thermally isolated diode detectors,21 and fiberoptic alignment structures were manufactured at Western Electric. Chemists worldwide took notice when Terry, Jerman, and Angell, from Stanford University, integrated a gas chromatograph on a Si wafer in 1979 as shown in Figure 1.22.22,23 This first analytical chemistry application would eventually lead to the concept of total analytical systems on a chip, or μTAS. An important milestone in the MEMS world was the founding of NovaSensor,
16
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
FIGURE 1.22 Gas chromatograph on a Si wafer. (Courtesy Hall Jerman.)
in 1985, by Kurt Petersen, Janusz Bryzek, and Joe Mallon (Figure 1.23). This was the first company totally dedicated to the design, manufacture, and marketing of MEMS sensors. Kurt Petersen developed the first torsional, scanning micromirror in 1980 at IBM.24 A more recent version of a movable mirror array is shown in Figure 1.24. Mirror arrays of this type led to the infamous stock market optical MEMS bubble of 2000, one of the bigger disappointments befalling the MEMS community. The first disposable blood pressure transducer became available in 1982 from Foxboro/ICT, Honeywell for $40. Active onchip signal conditioning also came of age around 1982. European and Japanese companies followed the U.S. lead more than a
FIGURE 1.23 NovaSensor founders in 2003 at the Boston Transducer Meeting. Left to right: Joe Mallon, Kurt Petersen, and Janusz Bryzek.
FIGURE 1.24 Integrated photonic mirror array from Transparent Networks. MEMSVLSI integration achieved through wafer bonding. There are 1200 3D mirrors on the chip; each is 1 × 1 mm, with a ±10° tilt in two axes. (Courtesy of Janusz Bryzek.)
decade later; for example, Druck Ltd., in the United Kingdom, started exploiting Greenwood’s micromachined pressure sensor in the mid1980s. Petersen’s 1982 paper extolling the excellent mechanical properties of singlecrystalline silicon helped galvanize academia’s involvement in Si micromachining in a major way.25 In MEMS the need sometimes arises to build structures on both sides of a Si wafer; in this case, a doublesided alignment system is required. These systems started proliferating after the EV Group (formally known as Electronic Visions) created the world’s first doubleside mask aligner with bottom side microscope in 1985 (http://www.evgroup.com). In the mid1990s, new highdensity plasma etching equipment became available, enabling directional deep dry reactive ion etching (DRIE) of silicon. Dry plasma etching was now as fast as wet anisotropic etching, and as a consequence the MEMS field underwent a growth spurt. U.S. government agencies started large MEMS programs beginning in 1993. Older MEMS researchers remember the idealistic and inspired leadership of Dr. Kaigham (Ken) Gabriel (Figure 1.25) at Defense Advanced Research Projects Agency (DARPA). Gabriel got many important new MEMS products launched. When the first polysilicon MEMS devices, made in a process called surface micromachining pioneered at University of California, Berkeley by Muller
Historical Note
FIGURE 1.25 Dr. Kaigham Gabriel: Early champion of MEMS work at DARPA.
and Howe, appeared in 1983,26 bulk singlecrystal Si micromachining started to get some stiff competition. This was exacerbated when, from the mid1990s onward, MEMS applications became biomedical and biotechnology oriented. The latter applications may involve inexpensive disposables or implants, and Si is not a preferred inexpensive substrate nor is it biocompatible. Glass and polymers became very important substrates in microfluidics, and many researchers started using a flexible rubber (polydimethylsiloxane or PDMS) as a building material in a process called soft lithography. The latter manufacturing method, which dramatically shortened the time between novel fluidic designs and their testing, was invented in the late 1990s by Harvard’s Whitesides.27 In the early years of MEMS, it was often projected that the overall MEMS market would grow larger than that for ICs. This notion was based on the expectation of many more applications for the former than the latter. This market projection has not been fulfilled. Including nonsilicon devices such as readwrite heads, one can claim a MEMS market of about 10% of the total IC market today. From Appendix 1B we learn that Si sensors and actuators amount to only 4% of IC sales. MEMS never really constituted a paradigm shift away from the IC concept but rather a broadening of it: incorporating more diverse materials, higher aspect ratio structures, and a wider variety of uses in smaller and more fragmented applications. In almost all respects MEMS remained IC’s
17
poor cousin: using secondhand IC equipment, with less than 5% of IC sales, and no Nobel laureates to trumpet breakthrough new concepts. Today, the Si MEMS market prospects are looking much better as MEMS are finally penetrating mass consumer products from projectors, to game controllers, to portable computers to cameras, mobile phones, and iPods with MEMS digital micromirror devices (DMDs), oscillators, accelerometers, gyros, etc. Even MEMS foundries are now thriving inside and outside the United States. This new generation of MEMS products fits highthroughput production lines on large Si substrates and is succeeding in the marketplace. The IC world has started to absorb the SiMEMS world. Over the years, the many MEMS applications did lead to a plethora of MEMS acronyms, some of them perhaps coined by assistant professors trying to get tenure faster. Here are some attempts at 15 minutes of fame: ◾ BioMEMS = MEMS applied to the medical and biotechnology field ◾ Optical MEMS = mechanical objects + optical sources/detectors ◾ PowerMEMS ◾ CMEMS (carbon MEMS for this author but ceramic MEMS for others) ◾ HIMEMS = hybrid insectmicroelectromechanical systems ◾ RFMEMS = radiofrequency MEMS ◾ CifMEMS = CMOS IC Foundry MEMS ◾ COTS MEMS = commercial offtheshelf MEMS ◾ MOEMS = microoptical electromechanical systems ◾ PMEMS = polymer MEMS ◾ CEMS = cellular engineering microsystems ◾ HARMEMS = highaspectratio MEMS We do expect that there are many more MEMS applications yet to be realized and that MEMS will facilitate the handshake between the macro and nano world in nanoelectromechanical systems (NEMS). In Table 1.2 we sketch our attempt at a Si/MEMS history line. Many more MEMS milestones than listed in the preceding text are captured here.
18
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 1.2 MEMS History Year
Fact
1824 1910 1927 1939 1947 (23 December)
Berzelius discovers Si First patent on the MOS transistor concept Field effect transistor patented (Lilienfield) First pn junction transistor (J. Bardeen, W.H. Brattain, W. Shockley) Invention of the transistor made from germanium at Bell Telephone Laboratories
1954 1956
Evidence of piezoresistive effect in Si and Ge by Smith9 An early milestone for the use of singlecrystal silicon in MEMS was the discovery of porous Si by Uhlir8 Jack Kilby of Texas Instruments invents the IC, using GE devices. A patent was issued to Kilby in 1959. A few months later, Robert Noyce of Fairchild Semiconductor announced the development of a planar Si IC
1958
1960s IC (1st Monolithic BJT IC, 4BJT)
1958 1958 1959 1961 1967 1967
Silicon strain gauges commercially available First IC (oscillator) R. Feynman famous talk: “There’s Plenty of Room at the Bottom”7 Fabrication of the first piezoresistive sensor, pressure (Kulite) Anisotropic deep silicon etching (H.A. Waggener12) First surface micromachining process (H. Nathanson28): resonant gate before it was called MEMS
Anodic bonding of glass to Si13 National Semiconductor: commercialize a Si MEMS pressure sensor Gas chromatograph on a Si wafer by S.C. Terry, J.H. Jerman, and J.B. Angell at Stanford University23 First capacitive pressure sensor (Stanford)16 IBM–HP: micromachined inkjet nozzle24
1969–1970 1972 1975 1977 1977
Bubble growth Nucleation
1980
Drop ejection and refill
K.E. Petersen, silicon torsional scanning mirror24
Historical Note
19
TABLE 1.2 MEMS History (Continued) Year
Fact
1982 1982 1982
Review paper “Silicon as a mechanical material” published by K.E. Petersen25 Disposable blood pressure transducer (Foxboro/ICT, Honeywell, $40) The use of xray lithography in combination with electroplating and molding (or LIGA), introduced by Ehrfeld and his colleagues29 Integrated pressure sensor (Honeywell) “First” polysilicon MEMS device (Howe, Muller UCB26); see also Nathanson in 196728 Silicon to silicon wafer bonding (M. Shimbo14) Texas Instrument’s Larry Hornbeck invents the digital micromirror devices (DMDs) Rotary electrostatic side drive motors (Fan, Tai, Muller30) Electrostatic micromotor (UCBerkeley BSAC) First MEMS conference (first transducers conference held in 1987) Lateral comb drive (Tang, Nguyen, Howe31)
1983 1983 1986 1987 1988 1988 1989
1990 1992 1992 1992
1992 1993 1995 1996
The concept of miniaturized total chemical analysis system or μTAS is introduced by Manz et al.32 This may be seen as the beginning of BIOMEMS Grating light modulator (Solgaard, Sandejas, Bloom) First MUMPS process (MCNC) (with support of DARPA). Now owned by MEMSCAP First MEMS CAD tools: MIT, S.D. Senturia, MEMCAD 1.0 Michigan, Selden Crary, CAEMEMS 1.0 Singlecrystal reactive etching and metallization (SCREAM) developed at Process (Cornell) Analog devices: commercialize multiaxis accelerometer integrating electronics (ADXL50) Intellisense Inc. introduces MEMS CAD IntelliSuite. MEMCAD 2.0 is launched, and ISE introduces SOLIDIS and ICMAT The first digital mirror device (DMD)–based products (Texas Instruments) appear on the market
TI’s VGA (640 × 480), the SVGA (800 × 600), and the XGA (1024 × 768)
1996 1997 1998 1998
DRIE (Bosch Process) Printing meets lithography when George M. Whitesides et al. at Harvard discover soft lithography27 First PCRmicrochips Sandia’s ultraplanar multilevel technology SUMMiTIV and V technologies. Four and fivelevel polySi processes (continued)
20
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 1.2 MEMS History (Continued) Year
Fact
1999
DNA microarray techniques
1999 2000 2002
Electrokinetic platforms (Caliper, Aclara, and Agilent) Nortel buys Xros for $3.25 billion The telecom recession puts many things on standby
Lucent 3D optical switch
2004
2006 2007
MEMS rebuilds. First application of accelerometer in consumer electronics (CE) to hard drive protection in notebooks. IBM puts dualaxis accelerometer in the notebook (now Lenovo) Sony (PS3) and Nintendo (Wii) introduce motionbased game controllers Apple announces the iPhone with motionbased features
NEMS The criteria we use in this book for classifying something as a nanoelectromechanical system (NEMS) are not only that the miniaturized structures have at least one dimension that is smaller than 100 nanometers, but also that they are crafted with a novel technique (so beer making is out) or have been intentionally designed with a specific nanofeature in mind (so medieval church stained glass is out). This definition fits well within the one adopted by the National Nanotechnology Institute (NNI; http:// www.nano.gov/html/facts/whatisnano.html): 1. Nanotechnology involves R&D at the 1 to 100nm range. 2. Nanotechnology creates and uses structures that have novel sizebased properties. 3. Nanotechnology takes advantage of the ability to control or manipulate at the atomic scale.
Paul Davis (http://cosmos.asu.edu), a theoretical physicist and wellknown science popularizer, said, “The nineteenth century was known as the machine age, the twentieth century will go down in history as the information age and I believe the twentyfirst century will be the quantum age.” We believe that the current nanotechnology revolution, underpinned by quantum mechanics, is already leading the way toward that reality. The manufacture of devices with dimensions between 1 and 100 nanometers is either based on topdown manufacturing methods (starting from bigger building blocks, say a whole Si wafer, and chiseling them into smaller and smaller pieces by cutting, etching, and slicing), or it is based on bottomup manufacturing methods (in which small particles such as atoms, molecules, and atom clusters are added for the construction of bigger functional constructs). The topdown approach to nanotechnology we call nanofabrication or nanomachining, an extension of
Historical Note
FIGURE 1.26 Master and slave hands on a set of Feynman machines.
viewed the world, the STM impacts our current view of biology, chemistry, and physics. In fast succession, a series of similar instruments, all called scanning proximal probes, followed the introduction of the STM. For example, Binnig, Quate (Stanford), and Gerber (IBM) developed the atomic force microscope (AFM) in 1986. An AFM, in contact mode, measures the repulsive force interaction between the electron clouds on the probe tip atoms and those on the sample—making it possible to image both insulating and conducting surfaces. This results in the visualization of the interactions Control voltages for piezotube Piezoelectric tube with electrodes
the MEMS approach. The bottomup approach we like to refer to as nanochemistry. An example of this second approach is the selfassembly of a monolayer (SAM) from individual molecules on a gold surface. Bottomup methods are nature’s way of growing materials and organisms, and in biomimetics one studies how nature, through eons of time, developed manufacturing methods, materials, structures, and intelligence and tries to mimic or replicate what nature does in the laboratory to produce MEMS or NEMS structures. A historyline with the most important NEMS milestones on it is difficult to put together as so many authors of such charts automatically include themselves or their institution on it first (one author of an early MEMS/NEMS timeline puts himself on it three times and his institution four times!). It sometimes seems that science and engineering are starting to resemble FOX News more by the day. What follows are some milestones toward nanotechnology that many scientists/engineers might agree to. Norio Taniguchi introduced the term nanotechnology in 1974, in the context of traditional machining with tolerances below 1 micron. The 1959 Feynman lecture “There’s Plenty of Room at the Bottom,” which helped launch the MEMS field (see above), was geared more toward NEMS than MEMS (http://www.its.caltech.edu/~feynman/plenty.html).7 Feynman proclaimed that he knew of no principles of physics that would prevent the direct manipulating of individual atoms. In his topdown gedanken experiment, he envisioned a series of machines each an exact duplicate, only smaller and smaller, with the smallest in the series being able to manipulate individual atoms (see Figure 1.26). In 1981, Gerd Binning and Heinrich Rohrer of IBM Zurich invented the scanning tunneling microscope (STM), enabling scientists to see and move individual atoms. Such a microscope, shown in Figure 1.27, measures the amount of electrical current flowing between a scanning tip and the conductive surface that is being measured. This unexpectedly simple instrument allowed for the imaging of micro and nanostructures, catapulted nanotechnology onto the world stage, and got its inventors the 1986 Nobel Prize (http://www. zurich.ibm.com/imagegallery/st/nobelprizes). Just as 350 years before the microscope changed the way we
21
Tunneling current ampliﬁer
Distance control and scanning unit
Data processing and display
Sample Tunneling voltage
FIGURE 1.27 Scanning tunneling microscope (STM). Operational principle of an STM. (Courtesy Michael Schmidt, TU Wien.)
22
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
between molecules at the nanoscale, thus increasing our ability to better understand the mechanism of molecular and biological processes. Other forms of scanning probe microscopes—those that do not depend on tunneling or forces between a probe tip and a sample surface—have also been demonstrated. Examples include the scanning thermal microscope, which responds to local thermal properties of surfaces, the scanning capacitance microscope for dopant profiling, and the nearfield scanning optical microscope (NSOM, also known as SNOM). In the latter instrument,33 the wavelength limitation of the usual farfield optics of a light microscope is avoided by mounting the light detector (say an optical fiber) on an AFM tip, at a distance from the sample that is a fraction of the wavelength used; this way it is possible to increase the resolution of a light microscope considerably. These new tools were an important catalyst behind the surge in nanotechnology activities worldwide, and this illustrates that progress in science is inextricably linked to the development of new measurement tools. The discovery, in the early 1980s at Bell Labs by David L. Allara (now at Pennsylvania State University) and Ralph G. Nuzzo (now at University of Illinois, UrbanaChampaign) of the selfassembly of disulfide and, soon thereafter, of alkanethiol monolayers (SAMs) on metal surfaces coincided with the maturation of STM technology.34,35 SAMs, especially on Au, turned out to be a valuable type of sample for STM investigation, showing these films to spontaneously assemble into stable and highly organized molecular layers, bonding with the sulfur atoms onto the gold and resulting in a new surface with properties determined by the alkane head group. Like SAMs, dendrimers, which are branching polymers sprouting successive generation of branches off like a tree, are an important tool for bottomup nanotechnologists. Dendrimers (from the word dendron, Greek for tree) were invented, named, and patented by Dr. Donald Tomalia (now CTO at Dentritic NanoTechnologies, Inc.) in 1980 while at Dow Chemical.36 In 1970, Arthur Ashkin was the first to report on the detection of optical scattering and gradient forces on micronsized particles.37 In 1986, Ashkin
FIGURE 1.28 Steven Chu (Stanford University), recipient of the 1997 Nobel Prize in Physics for his work on cooling and trapping of atoms.
and colleagues reported the first observation of what is now commonly referred to as an optical trap, i.e., a tightly focused beam of light capable of holding microscopic particles stable in three dimensions.38 One of the authors of this seminal 1986 paper, Steven Chu (Figure 1.28), would go on to make use of optical tweezing techniques in his work on cooling and trapping of atoms. Where Ashkin was able to trap larger particles (10 to 10,000 nanometers in diameter), Chu extended these techniques to the trapping of individual atoms (0.1 nanometer in diameter). This research earned him the 1997 Nobel Prize in Physics (with ClaudeCohen Tannoudji and William D. Phillips). In another heralded experiment, Steven Chu was also the one who demonstrated that by attaching polystyrene beads to the ends of DNA one can pull on the beads with laser tweezers to stretch the DNA molecule (http://www.stanford.edu/group/ chugroup/steve_personal.html). In 1985, Robert F. Curl Jr., Harold W. Kroto, and the late Richard E. Smalley serendipitously (while investigating the outer atmosphere of stars) discovered a new form of carbon: buckminsterfullerene, also known as buckyball or C60, shown in Figure 1.29.39 They were awarded the Nobel Prize in 1996. Perhaps a more important discovery, because of its generality and broader applicability, is the one by NEC’s Sumio Iijima, who, in 1991, discovered
Historical Note
FIGURE 1.29 Buckminsterfullerene C60 or buckyball with 60 atoms of carbon; each is bound to three other carbons in an alternating arrangement of pentagons and hexagons.
carbon nanotubes, with an electrical conductivity that is up to six orders of magnitude higher than that of copper (http://www.nec.co.jp/rd/Eng/innovative/E1/myself.html). Like buckyballs, cylindrical nanotubes each constitute a lattice of carbon atoms, and each atom is again covalently bonded to three other carbons. Carbon nanotubes exist as singlewalled (SWNT) and multiwalled (MWNT); the ones depicted in Figure 1.30a are multiwall nanotubes. Unique among the elements, carbon can bond to itself to form extremely strong twodimensional sheets, as it does in graphite, as well as buckyballs and nanotubes.
23
Cees Dekker demonstrated the first carbon nanotube transistor in 1998 at the Delft University of Technology40 (see Figure 1.30b). In this device, a semiconducting carbon nanotube of only about 1 nm in diameter bridges two closely separated metal electrodes (400 nm apart) atop a silicon surface coated with silicon dioxide. Applying an electric field to the silicon (via a gate electrode) turns on and off the flow of current across the nanotube by controlling the movement of charge carriers in it. By carefully controlling the formation of metal gate electrodes, Dekker’s group (http://www. ceesdekker.net) was able to create transistors with an output signal 10 times stronger than the input. At around the same time, the first nanotransistor was built at Lucent Technologies (1997). The MOS semiconductor transistor was 60 nm wide, including the source, drain, and gate; its thickness was only 1.2 nm. Other companies have since built smaller nanotransistors. At one point, in the late 1990s, it was—with just a bit of exaggeration—hard to find a proposal to a government agency that did not involve carbon nanotubes. But perhaps more real progress was mapped in the meantime in the area of nanocrystals or quantum dots (QD). Quantum dots possess atomlike energy states. The behavior of such small particles was beginning to be understood with work by the Russians Ekimov and Efros from 1980 to 1982.41,42 They recognized that nanometersized particles of CdSe, with their very high surfacetovolume ratio, could Drain electrode
Source electrode Nanotube molecule
Silico
n oxid
Silic
3 nm
(a)
e
on g
ate
(b)
FIGURE 1.30 (a) Multiwall nanotubes with Russian inset doll structure; several inner shells are shown a typical radius of the outermost shell >10 nm. (From S. Iijima, Nature 354, 54, 1991.) (b) First nanotube transistor. This threeterminal device consists of an individual semiconducting nanotube on two metal nanoelectrodes with the substrate as a gate electrode.
24
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
trap electrons and that these trapped electrons might affect the crystal’s response to electromagnetic fields, that is, absorption, reflection, refraction, and emission of light. Louis E. Brus, a physical chemist at Bell Laboratories at the time, and now at Columbia University, put this to practice when he learned to grow CdSe nanocrystals in a controlled manner.43,44 Murray, Norris, and Bawendi synthesized the first highquality quantum dots in 1993.45 Crystallites from −12 to −115 Å in diameter with consistent crystal structure, surface derivatization, and a high degree of monodispersity were prepared in a single reaction based on the pyrolysis of organometallic reagents by injection into a hot coordinating solvent. The confinement of the wavefunctions in a nanocrystal or quantum dot lead to a blue energy shift, and by varying the particle size one can produce any color in the visible spectrum, from deep (almost infra) reds to screaming (almost ultra) violet as illustrated in Figure 1.31. Today, quantum dots form an important alternative to organic dye molecules. Unlike fluorescent dyes, which tend to decompose and lose their ability to fluoresce, quantum dots maintain their integrity, withstanding many more cycles of excitation and light emission (they do not bleach as easily!). Combining a number of quantum dots in a bead conjugated to a biomolecule is used as a spectroscopic signature— like a barcode on a commercial product—for tagging those biomolecules. Carbon nanotubes are only one type of nanowire. In terms of investigating and exploiting quantum confinement effects, semiconductor wires, with
diameters in the 10s of nanometers, often single crystalline, represent the smallest dimension for efficient transport of electrons and excitons and are the logical interconnects and critical devices for nanoelectronics and nanooptoelectronics of the future. Over the past decade, there has been major progress in chemical synthesis technologies for growing these nanoscale semiconductor wires. As originally proposed by R.S. Wagner and W.C. Ellis from Bell Labs for the Aucatalyzed Si whisker growth, a vaporliquidsolid mechanism is still mostly used.46 But the field got a shot in the arm (a rebirth so to speak) with efforts by Charles Lieber (Harvard), Peidong Yang (http://www.cchem.berkeley.edu/pdygrp/main.html), James Heath (http://www.its.caltech.edu/~heathgrp), and Hongkun Park (http://www.people.fas.harvard. edu/~hpark). Lieber’s group at Harvard (http:// cmliris.harvard.edu) reported arranging indium phosphide semiconducting nanowires into a simple configuration that resembled the lines in a ticktacktoe board. The team used electron beam lithography to place electrical contacts at the ends of the nanowires to show that the array was electronically active. The tiny arrangement was not a circuit yet, but it was the first step, showing that separate nanowires could communicate with one another. Molecules are 30,000 times smaller than a transistor (180 nm on a side), so obviously it is of some use to investigate whether molecules can act as switches. Mark Ratner and Ari Aviram had suggested this as far back as 1974.47 The suggestion remained a pipe dream until the advent of scanning probe microscopes in the 1980s, which gave researchers finally
FIGURE 1.31 Differentsized quantum dots in response to nearUV light. Also composition of core affects wavelength. Red: bigger dots! Blue: smaller dots!
Historical Note
master molds of unprecedented aspect ratios and tolerances to replicate microstructures in ceramics, plastics, and metals. The hard xrays used enable nanosized patterns to be printed. At around 1997, Whitesides et al. introduced soft lithography, including the use of pattern transfer of selfassembled monolayers (SAMs) by elastomeric stamping.27 This technique formed a bridge between topdown and bottomup machining; a master mold is made based on “traditional” lithography, and the stamp generated from this master is inked with SAMs to print (stamp) substrates with nanosized patterns. Imposing boundaries on photons, by making them move in a material with a periodic dielectric constant in one, two, or three directions, leads to photonic crystals. Photonic crystals were first studied by Lord Rayleigh in 1887, in connection with the peculiar reflective properties of a crystalline mineral with periodic “twinning” planes.48 He identified a narrow bandgap prohibiting light propagation through the planes. This bandgap was angledependent because of the differing periodicities experienced by light propagating at nonnormal incidences, producing a reflected color that varies sharply with angle. A similar effect is seen in nature, such as in butterfly wings (Figure 1.33) and abalone shells. A onedimensional periodic structure, such as a multilayer film (a Bragg mirror), is the simplest type of photonic crystal, and Lord Rayleigh showed that any such onedimensional system has a bandgap. The possibility of two and threedimensionally periodic crystals with corresponding two and threedimensional bandgaps was suggested 100
the tools to probe and move individual molecules around. This led to a large number of studies in the late 1990s that demonstrated that individual molecules can conduct electricity just like metal wires, and turning individual molecules into switches came not far behind. In 1997, groups led by Robert Metzger (http://bama.ua.edu/~rmmgroup) of the University of Alabama, Tuscaloosa, and Mark Reed of Yale University (http://www.eng.yale.edu/reedlab) created molecular diodes. In July 1999, another group headed by James Heath and Fraser Stoddart of the University of California, Los Angeles (UCLA) (http:// stoddart.chem.ucla.edu) also created a rudimentary molecular switch, a molecular structure that carries current but, when hit with the right voltage, alters its molecular shape and stops conducting. Heath’s team placed molecules called rotaxanes, which function as molecular switches, at each junction of a circuit. By controlling the input voltages the scientists showed that they could make 16bit memory circuits work. The field of moletronics was born. As shown in Figure 1.32, rotaxanes are “mechanically linked” molecules that consist of a dumbbellshaped molecule, with a cyclic molecule linked around it between the two ends. The two ends of the dumbbell molecule are very big and prevent the cyclic molecule from slipping off the end. A number of factors (e.g., charge, light, pH) can influence the position of the cyclic molecule on the dumbbell. The use of xray lithography in combination with electroplating and molding (or LIGA), introduced by Ehrfeld and his colleagues in 1982,29 demonstrated to the world that lithography may be merged with more traditional manufacturing processes to make
Off
On (a)
25
(b)
FIGURE 1.32 (a) A diagram of rotaxane. The usefulness of rotaxanes is because there are a number of positions along the dumbbell molecule that the cyclic molecule can attach to temporarily. The dumbbell can be thought of as a train track, with the positions on the dumbbell molecule as stations and the cyclic molecule as the train. (b) Crystal structure of rotaxane with a cyclobis(paraquatpphenylene) macrocycle.
26
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
2 cm
FIGURE 1.33 A fullgrown Morpho rhetenor butterfly, a native to South America. (From University of Southhampton. Color by nanostructure instead of dyes.)
years after Rayleigh by Eli Yablonovitch49 (http:// w w w.ee.ucla.edu/labs/photon/homepage.html) and Sajeev John50 (http://www.physics.utoronto. ca/~john) in 1987. Yablonovitch (in 1991)51 demonstrated the first microwave photonic bandgap (PBG) structure experimentally with 1mm holes drilled in a dielectric material as illustrated in Figure 1.34 and known today as yablonovite. Since then, several research groups verified this prediction, which has ignited a worldwide rush to build tiny “chips” that control light beams instead of electron streams. In photonic crystals the repeat unit in the lattice is of the same size as the incoming wavelength, so homogeneous (effective) media theory cannot be
FIGURE 1.34 Holes drilled in dielectric: known now as yablonovite, after Yablonivitch (http://www.ee.ucla. edu/~pbmuri). The holes are 1 mm in size, and this photonic crystal is meant to operate in the microwave range.
applied. Photonic crystals feature lattice spacings ranging from the macroscopic (say 1 mm, for operating in the microwave domainlike yablonovite) to the 100s of nanometer range (to operate in the visible range). We cover photonic crystals here under NEMS, although only photonic crystals for the visible range qualify as nanotechnology. The potential applications of photonics are limitless, not only as a tool for controlling quantum optical systems but also in more efficient miniature lasers for displays and telecommunications, in solar cells, LEDs, optical fibers, nanoscopic lasers, ultrawhite pigments, radiofrequency antennas and reflectors, photonic integrated circuits, etc. In 1967 Victor Veselago, a Russian physicist, predicted that composite metamaterials might be engineered with negative magnetic permeability and negative permittivity.52 Metamaterials are artificially engineered materials possessing properties that are not encountered in nature. Whereas photonic materials do exist in nature, metamaterials do not; moreover, in the case of metamaterials, the building blocks are small compared with the incoming wavelength so that effective media theory can be applied. In conventional materials the plane of the electrical field, the plane of the magnetic field, and the direction in which light travels are all oriented at right angles to each other and obey the righthand rule. In Veselago’s imaginary metamaterial, the above quantities obey a lefthand rule (as if they were reflected in a mirror). These materials would interact with their environment in exactly the opposite way from natural materials (see negative refractive index water in Figure 1.35). One intriguing prediction was that the lefthand rule would allow for a flat superlens to focus light to a point and that could image with a resolution far beyond the diffraction limit associated with farfield illumination. Veselago’s prediction that such perfect lenses could be made from metamaterials lay dormant until 1996–2000, when the remarkable John Pendry, a physicist at Imperial College in London, showed that certain metals could be engineered to respond to electric fields as though the field parameters were negative.53–58 In 2001, researchers at Imperial College and Marconi Caswell Ltd. (London) announced a magnetic resonance
Historical Note
27
FIGURE 1.35 Refraction illustrated (a) empty glass: no refraction; (b) typical refraction with pencil in water with n = 1.3; (c) what would happen if the refractive index were negative with n = –1.3 (see metamaterials). (From Gennady Shvets, The University of Texas at Austin; http://www.ph.utexas.edu/~shvetsgr/lens.html.)
imaging system using a magnetic metamaterial based on Pendry’s design.59 Physicist Richard Shelby’s group at the University of California, San Diego demonstrated a lefthanded composite metamaterial that exhibited a negative index of refraction for microwaves.60 The simple arrangement consisted of a planar pattern of copper splitring resonators (SRRs) and wires on a thin fiberglass circuit board. Operating in the microwave range these metal patterns are large (5 mm repeat unit) but progress toward metamaterials operating in the visible was very swift. By 2005, Zhang’s group at University of California, Berkeley made a 35nm thick Ag superlens and imaged objects as small as 40 nm with 365 nm light, clearly breaking the diffraction limit of farfield imaging 61 (find Zhang’s group at http://xlab.me.berkeley.edu). By 2007, a lefthanded material operating in the visible range (780 nm) was demonstrated62 by Soukoulis (http:// cmpweb.ameslab.gov/personnel/soukoulis) at the U.S. Department of Energy’s Ames Laboratory on the Iowa State University campus and Wegener’s group from the University of Karlsruhe (http:// www.aph.unikarlsruhe.de/wegener), Germany. As in the case of photonic crystals, only the metamaterials operating in the visible qualify as nanotechnology, but for comprehensiveness sake we cover all of them together here. In 2000, IBM scientists placed a magnetic cobalt atom inside an elliptical coral of atoms. They observed the Kondo effect, i.e., electrons near the
atom align with the atom’s magnetic moment, effectively canceling it out. When the atom was placed at one focus of the elliptical coral, a second Kondo effect was observed at the other focus, even though no atom was there (see Figure 1.36). Hence some of the properties (info) carried by an atom are transferred to the other focus (www.research.ibm.com). This quantum mirage effect “reflects” information using the wave nature of the electrons rather than transmission of info using electrons in a wire. It has the potential to be able to transfer data within future nanoscale electronic circuits where wires would not work. This would allow miniaturization of circuits well below what is envisioned today.
FIGURE 1.36 Quantum mirage phenomenon (http:// domino.research.ibm.com/comm/pr.nsf/pages/rsc. quantummirage.html).
28
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
FIGURE 1.37 NSF’s Dr. Mike Roco, a photo (a) and a nanograph (b). The nanograph of Dr. M. Roco was recorded at Oak Ridge National Laboratory using piezoresponse force microscopy, one of the members of the family of techniques known as scanning probe microscopy, which can image and manipulate materials on the nanoscale. Each picture element is approximately 50 nanometers in diameter; the distance from chin to eyebrow is approximately 2.5 microns. (Courtesy Dr. Roco.)
In 1999 President Clinton announced the National Nanotechnology Initiative (NNI); this first formal government program for nanotechnology accelerated the pace of nano research (the program had been around unofficially since 1996). In December 2003, George W. Bush signed the 21st Century Nanotechnology Research and Development Act. In this government NEMS program, Dr. Mike Roco (Figure 1.37) played a similar catalyzing role that Dr. Ken Gabriel played earlier in the MEMS field (see above). Two other important nanotech promoters are Ray Kurzweil (http://www.kurzweilai.net/index. html) and K. Eric Drexel (http://www.foresight. org). Whereas Feynman continues to receive almost universal praise for his inspiring 1959 speculative talk, K. Eric Drexel, who in 1981 described mechanochemistry in his speculative paper “Molecular Engineering: An Approach to the Development of General Capabilities for Molecular Manipulation,” continues to receive mostly harsh criticism— sometimes bordering on derision. In this paper and in two books,63,64 Drexel builds nanotechnology, bottomup, atom by atom, rather than whittling down materials as Feynman had suggested. Drexel also makes more of the fact that nature and molecular biology are proof of concept for this type of molecular technology. Drexel’s
early warnings about “gray goo,” his emphasis on assemblers—small machines that would guide chemical bonding operations by manipulating reactive molecules—and building nanotechnology in a dry environment probably explain most of the hostility toward his work (even by those who do not even make an attempt to understand it; see for example Atkinson65 in Nanocosm—we might as well listen to Newt Gingrich talk about nanotechnology). Drexel, unfortunately, has been associated too much with the nano pop culture. Nano! by Ed Regisis is an engaging and entertaining book that describes some of the researchers involved in nanotechnology; he is uncharacteristically positive about Drexler.66 Market projections on NEMS are today even wilder than the early ones on MEMS. Overall, though, this author believes that it is in nanotechnology, especially when considering bottomup manufacturing, that a paradigm shift away from ICtype manufacturing is taking shape, and that it is nanotechnology that holds the potential of having a much larger impact on society than IC technology ever did. Indeed, the nanoscale is unique because at this length scale important material properties, such as electronic conductivity, hardness, or melting point, start depending on the size of the chunk of material in a way they do not at any other scale. Moreover, in biotechnology, molecular engineering already has made major progress, and the confluence of miniaturization science and molecular engineering is perhaps the most powerful new avenue for progress of humankind in general. In this regard, NEMS must be seen as a support technology to extract yet more benefits from the ongoing biotechnology revolution. In Table 1.3 we show a milestone chart in nanotechnology. It can be argued that molecular scientists and genetic engineers were practicing nanotechnology long before the name became popular with electrical and mechanical engineers. Molecular biology or “wet nanotechnology” has been called “nanotechnology that works.” But adding breakthroughs pertaining to molecular biology to this table would make it much too long. For the same reason we also did not list any ICrelated milestones.
Historical Note
29
TABLE 1.3 A Milestone Chart in Nanotechnology 3.5 billion years ago 400 BC 1857 1887 1905
1931 1932 1959 1967
The first living cells emerge. Cells house nanoscale biomachines that perform such tasks as manipulating genetic material and supplying energy Democritus coins the word “atom,” which means “not cleavable” in Greek Michael Faraday introduces “colloidal gold” to the Royal Society Photonic crystals are studied by Lord Rayleigh, in connection with the peculiar reflective properties of a crystalline mineral with periodic “twinning” planes48 Albert Einstein publishes a paper that estimates the diameter of a sugar molecule as 1 nm. JeanBaptist Perrin confirmed these results experimentally and was awarded the 1926 Nobel Prize for this work Max Knoll and Ernst Ruska develop the electron microscope, which enables nanometer imaging Langmuir establishes the existence of monolayers (Nobel Prize in 1932) Richard Feynman gives his famed talk “There’s Plenty of Room at the Bottom,” on the prospects for miniaturization7 Victor Veselago, a Russian physicist, predicted that composite metamaterials might be engineered with negative magnetic permeability and negative permittivity52
Victor Veselago
1968 Early 1970s 1974 1974 1980
1980 1981 Piezoelectric tube with electrodes
Control voltage for piezotube
Alfred Y. Cho and John Arthur of Bell Laboratories and their colleagues invent molecularbeam epitaxy, a technique that can deposit single atomic layers on a surface Groups at Bell Laboratories and IBM fabricate the first twodimensional quantum wells Norio Taniguchi conceives the word nanotechnology to signify machining with tolerances of less than a micron Mark Ratner and Ari Aviram suggest using molecules as switches47 The behavior of quantum dots began to be understood with work by the Russians Ekimov and Efros in 1980–1982.41,42 Louis E. Brus learned to grow CdSe nanocrystals in a controlled manner43,44 Dendrimers (from the word dendron, Greek for tree) were invented, named, and patented by Dr. Donald Tomalia36 Gerd Binnig and Heinrich Rohrer create the scanning tunneling microscope, which can image individual atoms
Distance Tunneling control and current ampliﬁer scanning unit
Data processing and display
Sample Tunneling voltage
Early 1980s 1982 1984 1985
The discovery, in the early 1980s, by David L. Allara and Ralph G. Nuzzo of the selfassembly of disulfide and, soon thereafter, of alkanethiol monolayers (SAMs) on metal surfaces The use of xray lithography in combination with electroplating and molding (or LIGA) is introduced by Ehrfeld and his colleagues29 Pohl develops nearfield scanning optical microscope (NSOM, also known as SNOM)33 Robert F. Curl, Jr., Harold W. Kroto, and Richard E. Smalley discover buckminsterfullerenes, also known as buckyballs, which measure about a nanometer in diameter39
(continued)
30
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 1.3 A Milestone Chart in Nanotechnology (Continued) 1986
Ashkin and colleagues reported the first observation of what is now commonly referred to as an optical trap, i.e., a tightly focused beam of light capable of holding microscopic particles stable in three dimensions38 K. Eric Drexel publishes Engines of Creation, a futuristic book that popularizes nanotechnology The possibility of two and threedimensionally periodic crystals with corresponding twoand threedimensional bandgaps was suggested 100 years after Rayleigh, by Eli Yablonovitch49 and Sajeev John50 Donald M. Eigler of IBM writes the letters of his company’s name using 35 individual xenon atoms on a nickel surface (in high vacuum and at liquid helium temperatures)
1986 1987
1989
1991 1991 1993 1993 1997 1997 1998 1999 OFF
Yablonovitch52 demonstrates the first microwave photonic bandgap (PBG) structure experimentally (holes drilled in dielectric), known now as yablonovite Sumio Iijima of NEC in Tsukuba, Japan, discovers carbon nanotubes. The first singlewalled nanotubes (SWNT) were produced in 1993 The first highquality quantum dots are synthesized by Murray, Norris, and Bawendi45,67 Warren Robinett of the University of North Carolina and R. Stanley Williams of UCLA devise a virtual reality system connected to an STM that lets users see and touch atoms The first complete metal oxide semiconductor transistor (60 nm wide) is invented by Lucent Technologies. The key breakthrough was the 1.2nmthick gate oxide Whitesides et al.27 introduced soft lithography, including the use of pattern transfer of selfassembled monolayers (SAMs) by elastomeric stamping Cees Dekker’s group at the Delft University of Technology in the Netherlands creates a transistor from a carbon nanotube40 James Heath and Fraser Stoddart of UCLA (http://stoddart.chem.ucla.edu/) create rudimentary molecular switches, with molecules called rotaxanes, which function as molecular switches
ON
1999 1999 1999
2000
2000
2001 2004 2005 2007
James M. Tour, now at Rice University, and Mark A. Reed of Yale University demonstrate that single molecules can act as molecular switches68 The Clinton administration announces the National Nanotechnology Initiative, which provides a big boost in funding and gives the field greater visibility Thermomechanical memory device, unofficially known as “Millipede,” first demonstrated at IBM Zurich
Eigler and other IBM scientists devise a quantum mirage—placing a magnetic atom at the focus of an elliptical ring of atoms creates a mirage atom at the other focus—transmitting info without wires John Pendry, a physicist at Imperial College in London, showed that certain metals could be engineered to respond to electric fields as though the field parameters were negative55 Researchers at Imperial College and Marconi Caswell (London) announced a magnetic resonance imaging system using a magnetic metamaterial based on Pendry’s design59 Physicists at the University of Manchester make graphene sheets69 Zhang et al. demonstrate the nearfield superlens—imaging objects in the tens of nanometer range with 365 nm light61 The first lefthanded material in the visible range62
Historical Note
Acknowledgments Special thanks to Xavier Casadevall i Solvas and Drs. Sylvia Daunert and Benjamin Park.
Appendix 1A: International Technology Roadmap for Semiconductors (ITRS) The complete 2003 ITRS and past editions of the ITRS editions are available for viewing and printing as an electronic document at http://public.itrs. net. The International Technology Roadmap for Semiconductors (ITRS) predicts the main trends in the semiconductor industry spanning across 15 years into the future. The participation of experts from Europe, Japan, Korea, and Taiwan as well as the United States ensures that the ITRS is a valid source of guidance for the semiconductor industry as it strives to extend the historical advancement of semiconductor technology and the worldwide integrated circuit (IC) market. The 2003 ITRS edition, used as the source for the tables below, extends to the year 2018. The 2003 ITRS does not predict a further acceleration in the timing of introduction of new technologies as the industry struggles through the worst recession of its history during the past couple of years. As projected, though, the halfpitch of 90 nm (hp90 nm) for DRAMs was introduced in 2004 (Intel’s Prescott Pentium IV). Traditionally, the ITRS has focused on the continued scaling of CMOS (complementary metaloxidesilicon) technology. By 2001, the horizon of the Roadmap started challenging the most optimistic projections for continued scaling of CMOS (e.g., MOSFET channel lengths below 9 nm). By that time it also became difficult for most people in the semiconductor industry to imagine how
31
one could continue to afford the historic trends of increase in process equipment and factory costs for another 15 years! Thus, the ITRS started addressing postCMOS devices. The Roadmap became necessarily more diverse for these devices, ranging from more familiar nonplanar CMOS devices to exotic new devices such as spintronics. Whether extensions of CMOS or radical new approaches, postCMOS technologies must further reduce the cost per function and increase the performance of integrated circuits. Thus, new technologies may involve not only new devices but also new manufacturing paradigms. The ITRS technology nodes in the table below are defined as the minimum metal pitch used on any product, for example, either DRAM halfpitch or Metal 1 (M1) halfpitch in Logic/MPU (see also figure below the tables). In 2003, DRAMs continue to have the smallest metal halfpitch; thus, it continues to represent the technology node. Commercially used numbers for the technology generations typically differ from the ITRS technology node numbers. However, the most reliable technology standard in the semiconductor industry is provided by the above definition, which is quite clear in that the patterning and processing (e.g., etching) capabilities of the technology are represented as the pitch of the minimum metal lines. The above definition is maintained not only for the 2003 version but also as a continuation from previous ITRS editions. Therefore, the official 2003 ITRS metal hpXX node indicator has been added to differentiate the ITRS definition from commercial technology generation numbers. Interim shrinklevel node trend numbers are calculated and included for convenience of monitoring the internode progress of the industry.
NearTerm Years Year of Production
2003
2004
2005
2006
2007
2008
2009
Technology node DRAM halfpitch (nm) MPU/ASIC MI halfpitch (nm) MPU/ASIC Poly Si halfpitch (nm) MPU printed gate length (nm) MPU physical gate length (nm)
100 120 107 65 45
hp90 90 107 90 53 37
80 95 80 45 32
70 85 70 40 28
hp65 65 75 65 35 25
57 67 57 32 22
50 60 50 28 20
32
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
LongTerm Years Year of Production
2010
2012
2013
2015
2016
2018
Technology node DRAM halfpitch (nm) MPU/ASIC MI halfpitch (nm) MPU/ASIC Poly Si halfpitch (nm) MPU printed gate length (nm) MPU physical gate length (nm)
hp45 45 54 45 25 18
35 42 35 20 14
hp32 32 38 32 18 13
25 30 25 14 10
hp22 22 27 22 13 9
18 21 18 10 7
DRAM ½ pitch = DRAM metal pitch/2
MPU/ASIC poly silicon ½ pitch = MPU/ASIC poly pitch/2
Metal pitch
Poly pitch
Typical DRAM metal bit line
Typical MPU/ASIC uncontacted poly
MPU/ASIC M1 ½ pitch = MPU/ASIC M1 pitch/2 Metal 1 (M1) pitch
Typical MPU/ASIC contacted Metal 1
Appendix 1B: Worldwide IC and Electronic Equipment Sales Amounts in US $M
Americas Europe Japan Asia Pacific Total world* Discrete semiconductors Optoelectronics Sensors and actuators Integrated circuits Bipolar Analog Micro Logic Memory Total products* * †
Year on Year Growth in %
2003
2004
2005
2006
2003
2004
2005
2006
32,330.7 32,310.0 38,942.2 62,842.6 166,425.5 13,347.0
39,514.2 40,537.5 47,822.9 85,756.0 213,630.6 16,043.4
41,734.6 43,693.5 51,066.8 95,253.0 231,748.0 17,036.5
40,089.1 43,082.1 50,306.9 96,546.2 230,024.4 16,689.1
3.4 16.3 27.7 22.8 18.3 8.1
22.2 22.5 22.8 36.5 28.4 20.2
5.6 7.8 6.8 11.1 8.5 6.2
−3.9 −1.4 −1.5 1.4 −0.7 −2.0
9,544.7 3,569.2 139,964.7 216.8 26,793.9 43,526.1 36,921.9 32,506.0 166,425.5
13,100.8 4,827.6 179,658.8 239.7 33,652.2 52,412.0 46,421.3 46,933.6 213,630.6
14,851.7 5,739.0 194,120.8 200.8 36,971.8 57,218.6 50,631.8 49,097.9 231,748.0
15,281.2 6,262.1 191,792.0 150.6 36,952.4 57,564.8 49,571.9 47,552.3 230,024.4
40.6
37.3 35.3 28.4 10.6 25.6 20.4 25.7 44.4 28.4
13.4 18.9 8.0 −16.3 9.9 9.2 9.1 4.6 8.5
2.9 9.1 −1.2 −25.0 −0.1 0.6 −2.1 −3.1 −0.7
†
16.1 −4.2 12.0 14.3 18.1 20.2 18.3
All numbers are displayed as rounded to one decimal place, but totals are calculated to three decimal places precision. WSTS included actuators in this category from 2003. Before only sensors were reported. Therefore, a growth rate is not meaningful to show.
Historical Note 400
1,600
1,540 1,395 1,265
Worldwide electronic equipment sales
1,200
350
300
1,160 1,050
1,000
250
960
910 851
200 200.7
800 800
179.0
701
150
157.6
633 585
144.4
600
132.0 137.3
134.7 120.7
120.4
100
104.6
62.3
Worldwide semiconductor sales (billions of dollars)
1,400 Worldwide electronic equipment sales (billions of dollars)
33
Worldwide semiconductor sales
80.0 400
50 1992
1993
1994 1995
1996 1997
1998
1999
2000
2001
2002 2003
11.5
11.6
12.5
12.8
Year Percent semiconductor
10.7
12.6
14.9
18.1
15.5
15.1
Questions 1.1: 1.2: 1.3:
1.4:
1.5:
1.6: 1.7:
1.8: 1.9: 1.10: 1.11:
Why is silicon so important to MEMS and NEMS? Compare the pros and cons of transistors and vacuum tubes. Why was the SiMEMS market at one point in time expected to be much larger than the IC market? Can you list some of the current technological and economic barriers that restrict the wider commercialization of SiMEMS? (a) State Moore’s first law (we are talking about Moore, Intel’s cofounder). (b) What is Moore’s second law? Why did surface micromachining catch on so fast with the IC industry? Why are MEMS market forecasts so difficult to prepare? How would you go about making a better MEMS market forecast? How does radar work? How is it useful? What is the biggest advantage Ge has over Si IC circuits? What is a strain gauge and what is its gauge factor? What is the definition of nanotechnology?
12.6
13.0
1.12:
List at least five commercial products that incorporate nanotechnology. 1.13: What year was the word “nanotechnology” first used? 1.14: What was Feynman’s role in catalyzing the genesis of MEMS and NEMS? 1.15: Why was the honeymoon with the transistor over so quickly? What technology took over very fast? 1.16: What does ITRS stand for? What does it mean? 1.17: List a number of nanostructures that have been fabricated with bottomup methodologies. 1.18: What is a photonic crystal? 1.19: What is a metamaterial? 1.20: What are the important differences between typical devices made in the IC industry and MEMS?
References We took advantage of Google and Wikipedia on numerous occasions and also relied on the following references: 1. Ohl, R. S. 1946. Lightsensitive electric device, Bell Labs. US Patent 2402662. 2. Bardeen, J., and W. Brattain. 1950. Three electrode circuit element utilizing semiconductive materials, Bell Labs. US Patent 2524035.
34
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
3. Riordan, M., and L. Hoddeson. 1998. Crystal fire: the birth of the information age. New York: W. W. Norton & Company. 4. Reid, T. R. 2001. The chip: how two Americans invented the microchip and launched a revolution. New York: Random House Publishing House. 5. ITRS. 2007. International Technology Roadmap for Semiconductors. Presentations from the 2007 ITRS Conference, December 5, 2007, Makuhari Messe, Japan. http://www. itrs.net/Links/2007Winter/2007_Winter_Presentations/ Presentations.html. 6. World Semiconductor Trade Statistics (WSTS). 2004. WSTS Semiconductor Market Forecast Spring 2004. Press release. http://www.wsts.org/plain/content/view/full/869. 7. Feynmann, R. 1959. There is plenty of room at the bottom. http://www.its.caltech.edu/~feynman/plenty.html. 8. Uhlir, A. 1956. Electrolytic shaping of germanium and silicon. Bell Syst Tech J 35:333–47. 9. Smith, C. S. 1954. Piezoresistance effect in germanium and silicon. Phys Rev 94:42–49. 10. Pfann, W. G. 1961. Improvement of semiconducting devices by elastic strain. Solid State Electron 3:261–67. 11. Tufte, O. N., P. W. Chapman, and D. Long. 1962. Silicon diffusedelement piezoresistive diaphragms. J Appl Phys 33:3322–27. 12. Waggener, H. A., R. C. Kragness, and A. L. Taylor. 1967. International Electron Devices Meeting, IEDM ‘67 68. Washington, DC, IEEE. 13. Wallis, P. R., and D. I. Pomeranz. 1969. Field assisted glassmetal sealing. J Appl Phys 40:3946–49. 14. Shimbo, M., K. Furukawa, K. Fukuda, and K. Tanzawa. 1986. Silicontosilicon direct bonding method. J Appl Phys 60:2987–89. 15. National Semiconductor. 1974. Transducers, Pressure, and Temperature (catalog). Sunnyvale, CA: Author. 16. Angell, J. B., S. C. Tery, and P. W. Barth. 1983. Silicon micromechanical devices. Scientific American 248:44–55. 17. Greenwood, J. C. 1969. Ethylene diaminecathecholwater mixture shows preferential etching of a pn junction. J Electrochem Soc 116:1325–26. 18. Bohg, A. 1971. Ethylene diaminepyrocatecholwater mixture shows etching anomaly in borondoped silicon. J Electrochem Soc 118:401–02. 19. Texas Instruments. 1977. Texas Instruments Thermal Character Print Head. Austin, TX: Author. 20. Bassous, E., H. H. Taub, and L. Kuhn. 1977. Ink jet printing nozzle arrays etched in silicon. Appl Phys Lett 31:135–37. 21. O’Neil, P. 1980. A monolithic thermal converter. HewlettPackard J, 12. 22. Terry, S. C., J. H. Jerman, and J. B. Angell. 1979. A gas chromatograph air analyzer fabricated on a silicon wafer. IEEE Trans Electron Devices 26:1880–86. 23. Terry, S. C. 1975. A gas chromatography system fabricated on a silicon wafer using integrated circuit technology. PhD diss., Stanford University. 24. Petersen, K. E. 1980. Silicon torsional scanning mirror. IBM J Res Dev 24:631–37. 25. Petersen, K. E. 1982. Silicon as a mechanical material. Proc IEEE 70:420–57. 26. Howe, R. T., and R. S. Muller. 1983. Polycrystalline silicon micromechanical beams. J Electrochem Soc 130:1420–23. 27. Xia, Y., and G. M. Whitesides. 1998. Soft lithography. Angew Chem Int Ed Engl 37:551–75.
28. Nathanson, H. C., W. E. Newell, R. A. Wickstrom, and J. R. Davis. 1967. The resonant gate transistor. IEEE Trans Electron Devices ED14:117–33. 29. Becker, E. W., W. Ehrfeld, D. Munchmeyer, H. Betz, A. Heuberger, S. Pongratz, W. Glashauser, H. J. Michel, and V. R. Siemens. 1982. Production of separation nozzle systems for uranium enrichment by a combination of xray lithography and galvanoplastics. Naturwissenschaften 69:520–23. 30. Fan, L. S., Y. C. Tai, and R. S. Muler. 1989. ICprocessed electrostatic micromotors. Sensors and Actuators A20:41–48. 31. Tang, W. C., T. C. Nguyen, and R. T. Howe. 1989. Laterally driven polysilicon resonant microstructures. IEEE Micro Electro Mechanical Systems 20:25–32. 32. Manz, A., N. Graber, and H. M. Widmer. 1990. Miniaturized total chemical analysis systems: A novel concept for chemical sensing. Sens Actuators B1:244–248. 33. Pohl, D. W., W. Denk, and M. Lanz. 1984. Optical stethoscopy: image recording with resolution l/20. Appl Phys Lett 44:651–53. 34. Allara, D. L., and R. G. Nuzzo. 1985. Spontaneously organized molecular assemblies; II. Quantitative infrared spectroscopic determination of equilibrium structures of solution adsorbed nalkanoic acids on an oxidized aluminum surface. Langmuir 1:52–66. 35. Allara, D. L., and R. G. Nuzzo. 1985. Spontaneously organized molecular assemblies; I. Formation, dynamics and physical properties of nalkanoic acids adsorbed from solution on an oxidized aluminum surface. Langmuir 1:45–52. 36. Tomalia, D. A., H. Baker, J. R. Dewald, M. Hall, G. Kallos, S. Martin, J. Roeck, J. Ryder, and P. Smith. 1985. A new class of polymers: starburstdendritic macromolecules. Polym J 17:117–32. 37. Ashkin, A. 1970. Acceleration and trapping of particles by radiation pressure. Phys Rev Lett 24:156–59. 38. Ashkin, A., J. M. Dziedzic, J. E. Bjorkholm, and S. Chu. 1986. Observation of a singlebeam gradient force optical trap for dielectric particles. Optics Letters 11:288–90. 39. Kroto, H. W., J. R. Heath, S. C. O’Brien, R. F. Curl, and R. E. Smalley. 1985. C60: buckminsterfullerene. Nature 318:162–63. 40. Tans, S. J., A. R. M. Verschueren, and C. Dekker. 1998. Roomtemperature transistor based on a single carbon nanotube. Nature 393:49–52. 41. Ekimov, A. I., A. L. Efros, and A. A. Onushchenko. 1985. Quantum size effect in semiconductor microcrystals. Solid State Commun 56:921–24. 42. Efros, A. L., and A. L. Efros. 1982. Interband absorption of light in a semiconductor sphere. Sov Phys Semicond 16:772–74. 43. Brus, L. E. 1984. On the development of bulk optical properties in small semiconducting crystallites. J Luminescence 31/32: 381. 44. Brus, L. E. 1984. Electronelectron and electronhole interactions in small semiconductor crystallites: the size dependence of the lowest excited electronic state. J Chem Phys 80:4403–07. 45. Murray, C. B., D. J. Norris, and M. G. Bawendi. 1993. Synthesis and characterization of nearly monodisperse CdE (E=S, Se, Te) semiconductor nanocrystallites. J Am Chem Soc 115:8706–15. 46. Wagner, R. S., and W. C. Ellis. 1964. Vapourliquidsolid mechanism of single crystal growth. Appl Phys Lett 4:89–90.
Historical Note 47. Aviram, A., and M. A. Ratner. 1974. Molecular rectifiers. Chem Phys Lett 29:277. 48. Rayleigh, J. W. S. 1888. On the remarkable phenomenon of crystalline reflexion described by Prof. Stokes. Phil Mag 26:256–65. 49. Yablonovitch, E. 1987. Inhibited spontaneous emission in solid state physics and electronics. Phys Rev Lett 58:2059. 50. John, S. 1987. Strong localization of photons in certain disordered dielectric superlattices. Phys Rev Lett 58:2486. 51. Yablonovitch, E., T. J. Gmitter, and K. M. Leung. 1991. Photonic band structure: the facecentered cubic case employing nonspherical atoms. Phys Rev Lett 67: 2295–98. 52. Veselago, V. G. 1968. The electrodynamics of substances with simultaneously negative values of e and m. Sov Phys Usp 10:509–14. 53. Pendry, J. B. 1999. Photonic gap materials. Curr Sci 76:1311. 54. Pendry, J. B. 2000. Negative refraction makes a perfect lens. Phys Rev Lett 85:3966. 55. Pendry, J. B. 2004. Manipulating the near field with metamaterials. Optics Photonics News 15:33–37. 56. Pendry, J. B. 2007. Metamaterials and the control of electromagnetic fields. Proceedings of the Ninth Rochester Conference on Coherence and Quantum Optics. Washington, DC: Optical Society of America. 57. Pendry, J. B., A. J. Holden, D. J. Robbins, and W. J. Stewart. 1998. Low frequency plasmons in thin wire structures. J Phys Cond Matter 10:4785. 58. Ramakrishna, S. A., J. B. Pendry, M. C. K. Wiltshire, and W. J. Stewart. 2003. Imaging the near field. J Mod Optics 50:1419–30.
35
59. Wiltshire, M. C. K., J. B. Pendry, I. R. Young, D. J. Larkman, D. J. Gilderdale, and J. V. Hajnal. 2001. Microstructured magnetic material for RF flux guides in magnetic resonance imaging (MRI). Science 291:848–51. 60. Shelby, R. A., D. R. Smith, and S. Schultz. 2001. Experimental verification of a negative refractive index. Science 292:77–79. 61. Fang, N., H. Lee, and X. Zhang. 2005. Subdiffractionlimited optical imaging with a silver superlens. Science 308:534–37. 62. Dolling, G., M. Wegener, C. M. Soukoulis, and S. Linden. 2007. Negativeindex metamaterials at 780 nm wavelength. Opt Lett 32:53–55. 63. Drexel, K. E. 1987. Engines of creation. New York: Anchor Books. 64. Drexel, K. E. 1992. Nanosystems, molecular machinery, manufacturing, and computation. New York: John Wiley & Sons, Inc. 65. Atkinson, W. I. 2003. Nanocosm: nanotechnology and the big changes coming from the inconceivable small. New York: AMACOM. 66. Regis, E. 1995. Nano: remaking the world atom by atom. Boston: Little, Brown and Company. 67. Murray, C. B., C. R. Kagan, and M. G. Bawendi. 1995. Selforganization of CdSe nanocrystallites into threedimensional quantum dot superlattices. Science 270:1335–38. 68. Reed, M. A., C. Zhou, C. J. Muller, T. P. Burgin, and J. M. Tour. 1997. Conductance of a molecular junction. Science 278:252–54. 69. Geim, A. K., and K. S. Novoselov. 2007. The rise of graphene. Nature Materials 6:183–191.
2 Crystallography
Outline Introduction Bravais Lattice, Unit Cells, and the Basis Point Groups and Space Groups Miller Indices
The designer Tokujin Yoshioka makes his Venus – Natural Crystal Chair by submerging a block of polyester fibers in the shape of a straightbacked dining chair in a vat of water and then adding a mineral to crystallize it. (Courtesy of Mr. Tokujin Yoshioka.)
XRay Analysis Reciprocal Space, Fourier Space, kSpace, or Momentum Space Brillouin Zones
Introduction
Nothing Is Perfect
Crystallography is the science of analyzing the crystalline structure of materials. The spatial arrangement of atoms within a material plays a most important role in determining the precise properties of that material. Based on the degree of order, materials are classified as amorphous, with no recognizable longrange order; polycrystalline, with randomly ordered domains (10 Å to a few μm); and single crystalline, where the entire solid is made up of repeating units in an orderly array. This classification is illustrated in Figure 2.1. Amorphous solids (e.g., glasses and plastics) are homogeneous and isotropic because there is no longrange order or periodicity in the internal arrangement. Many engineering materials are aggregates of small crystals of varying sizes and shapes. The size of the singlecrystal grains may be as small as a few nanometers but could also be large enough to be seen by the naked eye. Regions between grains are called grain boundaries. These polycrystalline materials have properties determined by both the chemical nature of the individual crystals and their aggregate properties, such as size and shape distribution, and in the orientation relationships between them. In the case of thin polycrystalline films, material properties might deviate significantly from bulk crystalline behavior, as we discover in
Acknowledgments Appendix 2A: Plane Wave Equations Questions Further Reading Reference
37
38
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
(a) Crystalline
(b) Amorphous
(c) Polycrystalline
FIGURE 2.1 Classification of materials as crystalline (a), amorphous (b), and polycrystalline (c). (Drawing by Mr. Chengwu Deng.)
Volume II, Chapter 7, where we deal with thin film properties and surface micromachining. In the case of nanoparticles, deviation from expected bulk theory is even more pronounced (see Chapter 3 on quantum mechanics and the band theory of solids in the current volume). The crystal structure of a nanoparticle is not necessarily the same as that of the bulk material. Nanoparticles of ruthenium (2–3 nm in diameter), for example, have bodycentered cubic (lattice point at each corner plus one at the center; see below) and facecentered cubic structures (lattice points at each corner as well as in the centers of each face; see below) not found in bulk ruthenium. Most important, semiconductor devices are based on crystalline materials because of their reproducible and predictable electrical properties. Crystals are anisotropic—their properties vary with crystal orientation. In this chapter we explain the importance of the symmetry of point groups and space groups in determining, respectively, bulk physical properties and microscopic properties of crystalline solids, properties relied on for building miniaturized electronics, sensors, and actuators. We also launch the concept of reciprocal space (also called Fourier space, kspace, or momentum space), clarify the conditions for xray diffraction in terms of such a reciprocal space, and offer an introduction to Brillouin zones. All these elements are needed for our introduction to the band theory of solids in Chapter 3. We finish Chapter 2 with a description of crystal defects.
Bravais Lattice, Unit Cells, and the Basis Under special conditions almost every solid can be made into a crystal (helium is the only substance that does not form a solid). Atoms organize themselves into crystals because energy can be minimized
Crystal
Lattice: set of points with identical environment
Primary building block: the unit cell
FIGURE 2.2 Any crystal lattice can be simplified to a threedimensional array of periodically located points in space. Such a periodic array, specifying how the repeated units of a crystal are arranged, is called a Bravais lattice. A real crystal is made up of a basis and a lattice. (Drawing by Mr. Chengwu Deng.)
that way. Any crystal lattice can be simplified to a threedimensional (3D) array of periodically located points in space as shown in Figure 2.2 in the case of a twodimensional (2D) crystal. Such a periodic array, specifying how the repeated units of a crystal are arranged, is called a Bravais lattice. Bravais, in 1848, demonstrated that there are only 14 ways of arranging points symmetrically in space that do not lead to voids in a crystal (in 2D there are only five such lattices). All crystalline materials, including nanomaterials, assume one of the 14 Bravais lattices. A real crystal can be described in terms of a Bravais lattice, with one specific atom (or ion) or a group of atoms (a molecule), called a basis, attached to each lattice point (Figure 2.2). The basis superposed on the Bravais lattice renders the complete crystal structure. The 3D Bravais lattice can be mathematically defined by three noncoplanar basis vectors, a1, a 2, and a 3, which are the three independent shortest vectors connecting lattice points. These vectors form a parallelepiped called a primitive cell, i.e., a cell that can reproduce the entire crystal lattice by translation alone. Such a primitive cell is a minimum volume cell with a density of only one lattice point per cell— there are lattice points at each of the eight corners of the parallelepiped, but each corner point is shared among the eight cells that come together there (1/8 of a point at each corner). The lattice translational vector r is given by: r = n1a1 + n2a 2 + n3a 3
(2.1)
39
Crystallography
where n1, n2, and n3 are integers. A displacement of any lattice point by r will result in a new position in the lattice that has the same positional appearance as the original position. A lattice translation vector, r, as described in Equation 2.1, connects two points in the lattice that exhibit identical point symmetry. Nonprimitive unit cells or simple unit cells are also called conventional unit cells or crystallographic unit cells. They are not necessarily unique and need not be the smallest cell possible. Primitive cells are chosen with the shortest possible vectors, whereas unit cells are chosen for the highest symmetry and may contain more than one lattice point per cell. The unit cell in a lattice, like a primitive cell, is representative of the entire lattice. The simplest unit cell belongs to a cubic lattice, which is further divided into simple cubic (SC), facecentered cubic (FCC), and bodycentered cubic (BCC) as illustrated in Figure 2.3. An FCC lattice has the closest atomic packing, then BCC, and then SC. For a simple cubic crystal (SC) unit cell, as shown in Figure 2.3, a1 = a 2 = a 3, and the axes angles are α = β = γ = 90°. The dimension a (= a1 = a 2 = a 3) is known as the lattice constant. For SC the conventional unit cell coincides with the primitive cell. This is not true for FCC and BCC as we shall see in Figure 2.5 below. The 14 possible Bravais lattices can be subdivided into 7 different “crystal classes” based on the choice of conventional unit cells. These 7 crystal classes are cubic, tetragonal, trigonal, hexagonal, monoclinic, orthorhombic, and triclinic. Each of these systems is characterized by a set of symmetry elements, and
a1 = a2 = a3 a1 a2 a3
1. Simple cubic (SC) Conventional cell = primitive cell a3 a2
Add one atom at the center of the cubic
a1
Add one atom at the center of each face
the more symmetry elements a crystal exhibits, obviously, the higher its symmetry. A cubic crystal has the highest possible symmetry and a triclinic crystal the lowest. The 14 Bravais lattices categorized according to the 7 crystal systems are shown in Figure 2.4. A WignerSeitz cell is a primitive cell with the full symmetry of the Bravais lattice. It is an important construct for the understanding of Brillouin zones, the boundaries of which satisfy the Laue conditions for diffraction (see below). To appreciate how WignerSeitz cells are constructed, we illustrate some simple examples for the case of two different types of 2D lattices in Figure 2.5. Lines are drawn passing through the middle points of dotted lines connecting nearest neighbors. In 3D, the WignerSeitz cells
3. Facecentered cubic (FCC) 2. Bodycentered cubic (BCC) Unit cell primitive cell
FIGURE 2.3 The simplest unit cell belongs to a cubic lattice, which is further divided into: simple cubic (SC), facecentered cubic (FCC), and bodycentered cubic (BCC).
FIGURE 2.4 Conventional unit cells for the 14 Bravais lattices arranged according to the 7 crystal systems. P means lattice points on corners only, C means lattice points on corners as well as centered on faces, F means lattice points on corners as well as in the centers of all faces, and lattice points on corners as well as in the center of the unit cell body are indicated by I.
40
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
show conventional unit and primitive unit cells for these lattices.
Point Groups and Space Groups FIGURE 2.5 WignerSeitz primitive cells for two types of simple 2D lattices.
are polyhedra constructed about each atom by drawing planes that are the perpendicular bisectors of the lines between nearest neighbors. The WignerSeitz cell about a lattice point is the region of space that is closer to that point than any other lattice point. WignerSeitz cells for FCC and BCC Bravais lattices are shown in Figure 2.6. In the same figure we also Bodycentered cubic lattice (BCC)
Facecentered cubic lattice (FCC)
Conventional cell: 2 atoms/cell
Conventional cell: 4 atoms/cell
Primitive unit cell: 1 atom/cell
Primitive unit cell: 1 atom/cell
WignerSeitz primitive cell: 1 atom/cell
A lattice translation as described by Equation 2.1 is a type of symmetry operation where a displacement of a crystal parallel to itself carries the crystal structure into itself (Figure 2.7). Rotation and reflection or a combination of rotation and reflection—a socalled compound symmetry operation—about various points are other symmetry operations that may “carry the crystal into itself” (see Figure 2.8). The point around which the symmetry operation is carried out may be a lattice point or a special point within the elementary parallelepiped. There are five types of rotation axes possible, i.e., one (360°), two (180°), three (120°), four (90°), and sixfold (60°) rotation. One sees from Figure 2.8 why fivefold rotational symmetry does not occur in nature; it just cannot be stacked without leaving holes. This explains, for example, why we do not see ice crystals with a pentagon shape (Figure 2.9). Mirror reflection takes place about a plane through a lattice or special point. An inversion operation is an example of a compound symmetry operation and is achieved by rotation of π, followed by a reflection in a plane normal to the rotation axis; the effect is also illustrated in Figure 2.8. The collection of point symmetry elements possessed by a crystal is called a point group and is defined as the collection of symmetry operations which, when applied about a point, leave the lattice invariant. There are 32 crystallographic point groups in all.
WignerSeitz primitive cell: 1 atom/cell
FIGURE 2.6 Conventional unit cells, primitive unit cells, and WignerSeitz primitive cells for BCC and FCC lattices. The BCC WignerSeitz unit cell is a truncated octahedron. The FCC WignerSeitz primitive unit cell is a rhombic dodecahedron.
FIGURE 2.7 The drawing on the left (a) is crystallike and can be carried into itself by a translation that is not possible in the figure on the right (b). The latter is missing a translation vector and is not crystallike.
Crystallography (a)
41
2fold Rotatation 4fold 3fold
5fold 1 full rotation of 360° 1
2 turns of 180° each 2
4 turns of 90° each 4 (b)
3 turns of 120° each 3
6fold
6 turns of 60° each 6
Mirror planes
(c)
Inversion 1
i
i
FIGURE 2.8 Point symmetry operations: (a) rotation, (b) reflection, and (c) a compound symmetry operation: inversion. The latter is made up of a rotation of π followed by reflection in a plane normal to the rotation axis. This is also called inversion through a point (i). The symbol for the inversion axis is 1.
The importance of the 32 point group symmetries and corresponding crystal classes is revealed by the important physical properties of crystalline solids they control, including electrical conductivity, thermal expansion, birefringence, piezoresistance, susceptibility, elastic stiffness coefficient, etc. Some properties that depend on the direction along which they are measured relative to the crystal axes are listed in Table 2.1. This orientation dependence of physical and chemical properties is called anisotropy. Anisotropy also explains why crystals do not grow into spheres but as polyhedra and why certain crystal directions etch faster than others. The reason for this anisotropy is the regular stacking of atoms in a crystal; as one passes along a given direction, one encounters atoms or groups of atoms at different intervals and from different angles than if one travels through the crystal from another direction. Single molecules in a liquid or a gas can also be anisotropic,
but because they are free to move, liquids and gases are isotropic. In a crystal the anisotropy of atoms and groups of atoms is locked into the crystal structure. As a first example we consider a physical quantity such as current density J (column 4), and its cause the electrical field E (column 5). These quantities are linked, to a first approximation, in a linear relationship described by a tensor equation: J = σE
(2.2)
One remembers that a tensor field represents a single physical quantity that is associated with certain places in threedimensional space and instants of time. The crystalline property, in column 1, is a tensor field of the rank listed in column 2. Also recall that a scalar (e.g., mass, temperature, charge) is a tensor of zeroth rank, and a vector (e.g., position, velocity, flow of heat) is a tensor of first rank. Other quantities such as stress inside a solid or fluid may be
42
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
FIGURE 2.9 Ice crystals. No pentagons are found in ice crystal stacking.
characterized by tensors of order two or higher. The physical properties listed in Table 2.1 are exploited to build electronics, sensors, and actuators in MEMS and NEMS. We elaborate a bit further here on the anisotropy of the electrical conductivity σ in a single crystal,
where a causal or forcing term, the electrical field E, causes a current density J. Because both are vectors, this case is referred to as a vectorvector effect. In general, the current vector may not have the same direction as the electric vector. Assuming a linear relationship between electrical field (cause) and
TABLE 2.1 Linear Physical Properties of Solids
Property and Symbol
Rank of Tensor
Number of Independent Components
Pyroelectric coefficient p
1
3
Conductivity σ Resistivity ρ Susceptibility χ Thermal expansion α Piezoelectric coefficient d Elastic stiffness constants χ Elastic compliance σ Piezoresistance π
2 2 2 2 3 4 4 4
6 6 6 6 18 21 21 21
Dependent Physical Quantity Electric polarization dP Current density J Field E Electric polarization P Strain ε Electric polarization Ps Stress S Stress ε Resistivity change ρ
Unfortunately, symbols customarily used for these properties do sometimes overlap.
Causal or Forcing Term Temperature change dT Field E Current density J Electric field E Temperature change dT Stress S Strain ε Stress S Stress S
Crystallography
43
current (effect), we can describe the components of the current relative to an arbitrarily chosen Cartesian coordinate system as:
angle θ between the direction in which ρ is measured and the hexagonal, trigonal, or tetragonal axis. One then finds:
J x S xx E x S xy E y S xz E z
ρ(ϕ) = ρpersin 2ϕ + ρparcos2ϕ
J y S yx E x S yy E y S yz E z
(2.3)
J z S zx E x S zy E y S zz E z The quantities σik are components of a 3 × 3 “conductivity tensor.” The resistivity tensor ρ(= 1/σ) tensor, like the conductivity tensor, is a second rank tensor described by: E = ρJ
(2.4)
Based on the basic symmetry of the equations of motion, Onsager demonstrated that the tensor is symmetric, i.e., σik = σki, so that the nine coefficients are always found to reduce to six. Taking advantage of this symmetry argument and multiplying the expressions in Equation 2.3 by Ex , Ey, and Ez, respectively, one obtains on adding: J x E x J y E y J z E z S xx E 2 x S yy E 2 y S zz E 2 z 2S xy E x E y 2S yz E y E z 2S zx E z E x
(2.5)
To make the mixed terms on the right side of Equation 2.5 disappear, one chooses a new coordinate system with the coordinates along the principal axes of the quadratic surface represented by this righthand side (rhs) term, and in this new coordinate system one obtains: J x S1E x ; J y S 2E y ; J z S 3E z
(2.6)
where σ1, σ2, and σ3 are the principal conductivities. The current and field vectors only have the same direction when the applied field falls along any one of the principal axes of the crystal. From Equation 2.6, no matter how low the symmetry of a crystal, it can always be characterized by three conductivities (σ1, σ2, and σ3) or three specific resistivities (ρ1, ρ2, and ρ3). In cubic crystals the three quantities are equal, and the specific resistivity does not vary with direction. In hexagonal, trigonal, and tetragonal crystals, two of the three principal conductivities (or resistivities) are the same. In such a case, the resistivity only depends on the
(2.7)
where the subscripts stand for perpendicular and parallel to the axis. Another vectorvector effect example in Table 2.1 is the one involving thermal conductivity, where a thermal current vector is caused by a thermal gradient. Scalartensor effects lead to similar relations as vectorvector effects. For example, the deformation tensor of a solid resulting from a temperature change (scalar) involves three principal expansion coefficients, α1, α2, and α3. The latter will again all be equal in the case of a cubic crystal, and the angular dependence of α for hexagonal, trigonal, and tetragonal crystals is given by an expression analogous to Equation 2.7. A simple example of a scalarvector effect from Table 2.1, illustrating the importance of crystal symmetry or lack thereof, involves pyroelectricity (see first row in Table 2.1). Pyroelectricity is the ability of a material to spontaneously polarize and produce a voltage as a result of changes in temperature. It must be a change in temperature: incident light may heat a pyroelectric crystal, thus changing its dipole moment and causing current to flow, but because pyroelectrics respond to the rate of change of temperature only, the light or heat source must be pulsed or modulated! A pyroelectric is a ferroic material, i.e., a class of smart multifunctional materials having both sensing and actuating functions. Ferroic materials is a simplified term to represent ferroelastic, ferromagnetic, and ferroelectric materials. In pyroelectricity, the opposite faces of certain crystals [e.g., tourmaline (Na, Ca)(Li, Mg, Al) (Al, Fe, Mn)6(BO3)3(Si6O18)(OH)4 the “Ceylon magnet,” ZnO, BaTiO3, and PbTiO3] become electrically charged as a result of a change in temperature. This is illustrated for tetragonal BaTiO3 in Figure 2.10. In Table 2.1 we consider the linear relationship between the electric polarization P (a vector) and a temperature change (a scalar). Electric polarization of materials is covered from a theoretical point of view in Chapter 5. For practical applications of pyroelectricity in actuator construction refer to
44
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology (A) Cubic
T > 120°C P
P
P
5°C < T < 120°C
P (coulombs/m2)
20 × 10–2
Tetragonal P aaxis
16 12
–90°C < T < 5°C
8
P parallel with 12 equivalent or P directions
Rhombohedral
Monoclinic
4 0 –200 –160 –120
–80
–40
0
Tetragonal
40
80
120
T< –90°C
P
baxis
P Rhombohedral
P parallel with 8 directions
Temperature(°C)
Orthorhombic
(B) (a)
(b)
Ba2+ O2– Ti4+
4.03 Å 3.98 Å 3.98 Å
FIGURE 2.10 (A) In the pyroelectric crystal BaTiO3, P changes with temperature only when the material is in its tetragonal state. Pyroelectricity only occurs in a crystal lacking an inversion center. This is clear from (B) (a). In cubic BaTiO3 the oxygen ions are at face centers; Ba2+ ions are at cube corners; and Ti4+ is at cube center. (B) (b) In tetragonal BaTiO3, the Ti4+ is offcenter, and the unit cell has a net polarization. (Drawing by Mr. Chengwu Deng.)
Volume III, Chapter 8. The crystalline property, the pyroelectric coefficient p, is a tensor of rank 1 (a vector in other words). One can predict readily that pyroelectricity only occurs in crystals that lack an inversion center or a center of symmetry, i.e., in noncentrosymmetric crystals with one or more polar axes. Indeed, one could not have a crystal with one face positively charged and one negatively charged—i.e., with a polar axis—as a result of a uniform change in temperature if these crystal faces were equivalent. More complicated cases involve vectortensor effects and tensortensor effects. Piezoelectricity is an example of a vectortensor effect; an electric field (vector) causes a mechanical deformation (tensor). Elastic deformation under the influence of a stress tensor is an example of a tensortensor effect. These effects require many more constants than the simple
examples presented above. In discussing actuators in Volume III, Chapter 8, we will find out that an increase in symmetry introduces major simplifications in the coefficient matrices and that to describe the tensors correctly the pointgroup symmetry of the crystal must be known. The combined effects of rotation or reflections from the point groups with translation from the Bravais lattice results in two additional symmetries: screw axes and glide planes. A screw axis combines rotation and translation, and a glide plane combines reflection with translation (Figure 2.11). Considering the various combinations involving the 32 point groups, screw axes, and glide planes, as well as the different Bravais lattices, a total of 230 different possible “space groups” results. In protein crystals there are only 65 space groups because all natural products are chiral so that inversion and mirror symmetry
Crystallography (a)
45
(b)
C
C/3 C/3 120°
Mirror Glide
b
120°
g
0,C
a/2
2C/3
a
a/2
height 3fold axes
FIGURE 2.11 Example of a screw axis and a glide plane. (a) Nfold screw axes C: a combination of a rotation of 360°/n around C and a translation by an integer of C/n. (b) Glide plane: a translation parallel to the glide plane g by a/2.
operations are not allowed. A space group is a group that includes both the point symmetry elements and the translations of a crystal. These space groups are most important when studying the microscopic properties of solids. The space groups for most inorganic substances are known and can be found in tables in the Inorganic Crystal Structure Database (ICSD). These tables make it possible to calculate the exact distances and angles between different atoms in a crystal. The external shape of a crystal is referred to as the habit. Not all crystals have welldefined external faces. Natural faces always have low indices, i.e., their orientation can be described by Miller indices that are small integers as introduced next. The faces that we see are the lowest energy faces as the surface energy is minimized during growth.
Miller Indices To identify a plane or a direction in a crystal, a set of integers h, k, and l, called the Miller indices, are widely used. To determine the Miller indices of a plane, one takes the intercept of that plane with the axes and expresses these intercepts as multiples of the base vectors a1, a 2, and a 3. The reciprocal of these three integers is taken, and, to obtain whole numbers, the (100) plane
z
(110) plane
z
y
three reciprocals are multiplied by the smallest common denominator. The resulting set of numbers is written down as (hkl). By taking the reciprocal of the intercepts, infinities (∞) are avoided in plane identification. Parentheses or braces are used to specify planes. The rules for determining the Miller indices of a direction or an orientation in a crystal are as follows: translate the orientation to the origin of the unit cell, and take the normalized coordinates of its other vertex. For example, the body diagonal in a cubic lattice as shown in the rightmost panel in Figure 2.12 is 1a, 1a, and 1a or the [111] direction. The Miller indices for a direction are thus established using the same procedure for finding the components of a vector. Brackets or carets specify directions. Directions [100], [010], and [001] are all crystallographically equivalent and are jointly referred to as the family, form, or group of directions. A form, group, or family of faces that bear like relationships to the crystallographic axes—e.g., the planes (001), (100), (010), (001), (100), and (010))—are all equivalent, and they are marked as {100} planes (see Figure 2.13). A summary of the typical representation for Miller indices is shown in Table 2.2. The orientation of a plane is defined by the direction
y
[111]
z y
(111) plane [110] [100] x
x
x
FIGURE 2.12 Miller indices for planes and directions in an SC cubic crystal. Shaded planes are from left to right (100), (110), and (111). (Drawing by Mr. Chengwu Deng.)
46
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology (100) on back face
(010) on side face
z
4 3
(001) a3 (100) a1
(364) plane
2
(010)
1
a2 1
1
2
3
4
y
2 3 x (001) on bottom face
4
FIGURE 2.14 The (364) plane in a SC cubic lattice.
FIGURE 2.13 Miller indices for the planes of the {100} family of planes.
and find the differences: r − r1 = (x − 4) a1 + (y − 0) a 2 + (z − 0) a 3
of a normal to the plane or the vector product (A × B = C). For a cubic crystal (such as silicon or gallium arsenide), the plane (hkl) is perpendicular to the direction [hkl]. In other words, the indices of a plane are the same numbers used to specify the normal to the plane. Using a simple cubic lattice as an example, you can check that crystal planes with the smallest Miller indices, such as {100}, {110}, {111}, have the largest density of atoms. Usually crystals are cleaved along these planes and are grown in directions perpendicular to them. When one comes across more complicated planes than the ones considered above, the mathematical vector algebra approach to calculate the Miller indices becomes useful. For examples, consider the plane in Figure 2.14, defined by three points P1, P2, and P3, where P1: (400), P2: (020), and P3: (003).
r2 − r1 = (0 − 4) a1 + (2 − 0) a 2 + (0 − 0) a 3 r3 − r1 = (0 − 4) a1 + (0 − 0) a 2 + (3 − 0) a 3
Step 2. Calculate the scalar triple product of these three vectors [A ∙ (B × C)], which in this case is a plane and its volume is zero because the vectors are coplanar [A ∙ (B × C) = 0]: (r − r1)∙[(r2 − r1) × (r3 − r1)] = 0
A1 A B s C B1 C1
Notation
Interpretation
(hkl ) {hkl } [hkl ]
Crystal plane Equivalent planes Crystal direction Equivalent directions
A3 B3 A 1(B2C 3 B3C 2 ) C3
For our example this leads to: x 4
4
4
r1 = 4a1 + 0a 2 + 0a 3
TABLE 2.2 Miller Indices Symbols
A2 B2 C2
A 2 (B3C1 B1C 3 ) A 3 (B1C 2 B2C1 ) (2.11)
r = xa1 + ya 2 + za 3
r3 = 0a1 + 0a 2 + 3a 3
(2.10)
For vectors A, B, C with coordinates (A1, A2, A3), (B1, B2, B3), and (C1, C2, C3), the requirement in Equation 2.10 is equivalent to:
Step 1. Define the following vectors:
r2 = 0a1 + 2a 2 + 0a 3
(2.9)
(2.8)
y 2 0
z 0 ( x 4)6 12y 8z 0 3
or 3x 6y 4z 12 Once we have the equation for the plane, we easily find the Miller indices. Step 3. Determine the Miller indices. 1. The intercepts with the axes: x = 4 (for y = z = 0), y = 2 (for x = z = 0), and z = 3 (for x = y = 0) 2. The reciprocals 1/4, 1/2, and 1/3, or 3. The Miller indices for the plane are (364)
47
Crystallography
Adjacent planes (hkl) in a simple cubic crystal are spaced a distance dhkl from each other, with dhkl given by: d hkl
a
(2.12)
2
h k 2 l2
where a is the lattice constant. Equation 2.12 provides the magnitude of dhkl and follows from simple analytic geometry. To generalize this expression, notice that for a plane (hkl) with hx + ky + lz = a, the distance from any point (x1, y1, z1) to this plane is:
d hkl =
hx 1 k y 1 lz1 a
h
2
2
k l
1 2 2
(2.13)
Hence when that point is at origin (0, 0, 0) we find Equation 2.12 back. ◾ Example 2.1: With a = 5 Å, we find d = a = 5 Å for (100) planes and d = a/ 2 = 3.535 Å for (110) planes.
Because a, b = ab cos θ the angle between plane (h1, k1, l1) and plane (h2, k2, l2) can be calculated as: cos Q
(h1h 2 k 1k 2 l1l 2 ) 2 1
h k 12 l12 h 22 k 22 l 22
(2.14)
◾ Example 2.2: The angle between a (100) and a (111) plane is cos θ = 1/ 1 3 = 0.58 or θ = 54.74°.
XRay Analysis Introduction Xray analysis reveals the symmetries of crystals (lattice type), distances between atomic planes (lattice parameter), the positions of atoms in crystals, the types of atoms from the intensities of diffracted xrays, and the degree of crystallinity (ordering). To perform xray crystallography, it is necessary to grow crystals with edges of around 0.1–0.3 mm. This is usually not a problem for inorganic materials, but in the case of organic materials, such as proteins (for example, see the crystal structure of the GFP protein
in Figure 7.108) and nucleic acids (see xray diffraction image in Figure 2.17), it often is a challenge: imagine trying to crystallize a molecule with 10,000 atoms! A crystallographer must combine ingenuity and patience to trick these molecules into crystallizing. In this section we learn about diffraction and the allimportant Bragg and Laue xray diffraction laws and how the latter are used to deduce the 3D structure of molecules.
Fourier Transforms Diffraction forms the basis for xray crystallography. The first step toward interpreting diffraction patterns was a mathematical trick discovered by the French mathematician Joseph Fourier, who in 1807 introduced Fourier transforms for solving heat conduction problems. The result of a Fourier transform is that periodic functions in the time domain, e.g., light waves, can be completely characterized by information in the frequency domain, i.e., by frequencies and amplitudes of sine, cosine functions. Fourier analysis provides us with the tools to express most functions as a superposition of sine and cosine waves of varying frequency. For periodic signals a discrete sum of sines/cosines of different frequencies is multiplied by a different weighting coefficient in a socalled Fourier series (FS). For nonperiodic functions, one needs a continuous set of frequencies so the integral of sines/cosines is multiplied by a weighting function in a socalled Fourier transform (FT) (Figure 2.15). One important property of Fourier transforms is that they can be inverted. If you apply a Fourier transform to some function, you can take the result and run it through an inverse Fourier transform to get the original function back. The inverse Fourier transform is essentially just another Fourier transform. Fourier and inverse Fourier transforms, which take the signal back and forth between time and frequency domains, are: From time to frequency: X(f )
1
d
° x( t ) e 2P
2 Pift
d
From frequency to time: x(t )
1
dt
(2.15)
d
° X (f ) e 2P
d
2 Pift
df (2.16)
48
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology Fourier series
Signal Square wave A t
0
A
Spectrum
(4A/)[cos(2ft)(1/3)cos(2(3f)t) +(1/5)cos(2(5f)t)(1/7)cos(2(7f)t) +...]
T
f
3f
5f
7f
9f
f
3f
5f
7f
9f
Triangular wave A t
0 A
(8A/)[cos(2ft)+(1/9)cos(2(3f)t) +(1/25)cos(2(5f)t)+...]
T
(a)
Signal x(t)
Fourier transform X(f )
Spectrum
Rectangular pulse A A t
0 /2
sin(f) f
/2
0
f
3f
5f
0
f
3f
5f
Triangular pulse A 0
A
t
sin(f)
2
f
(b)
FIGURE 2.15 (a) For periodic signals a discrete sum of sines/cosines of different frequencies is multiplied by a different weighing coefficient in a socalled Fourier series (FS). (b) For nonperiodic functions, one needs a continuous set of frequencies so the integral of sines/cosines is multiplied by a weighting function in a socalled Fourier transform (FT).
In Chapter 5 we will see that the formation of an image, according to Abbe’s theory, is a twostage, doublediffraction process: an image is the diffraction pattern of the diffraction pattern of an object. In xray diffraction there is no lens to focus the xrays, so we have to use a computer to reassemble the image: the xray diffraction patterns from a crystal are related to the object diffracting the waves through a Fourier transform. Fourier transforms are actually even more general than revealed here: a FT allows for a description given in one particular “space” to be transformed to a description in the reciprocal of that space, and timefrequency transformation is just one example. It is interesting to note that strong criticism by peers blocked publication of Fourier’s work until 1822 (Theorie Analytique De La Chaleur). Today, Fourier analysis is used in GSM (global system for mobile communications)/cellular phones, most DSP (digital
signal processing)based applications, music, audio, accelerator control, image processing, xray spectrometry, chemical analysis (FT spectrometry), radar design, PET scanners, CAT scans and MRI, speech analysis (e.g., voiceactivated “devices,” biometry), and even stock market analysis.
XRay Diffraction Introduction Wilhelm Conrad Roentgen discovered xrays in 1895 and received the Nobel Prize in Physics in 1901 for his discovery. Xrays are scattered by the electrons in atoms because electromagnetic radiation (including xrays) interacts with matter through its fluctuating electric field, which accelerates charged particles. You can think of electrons oscillating in position and, through their accelerations, reemitting electromagnetic radiation. The scattered radiation
Crystallography
interferes both constructively and destructively, producing a diffraction pattern that can be recorded on a photographic plate. For xrays, electrons, and neutrons incident on a single crystal, diffraction occurs because of interference between waves scattered elastically from the atoms in the crystal. Intensity of scattered radiation is proportional to the square of the charge/mass ratio, and the proton is about 2000 times as massive as the electron. Because electrons have a much higher chargetomass ratio than atomic nuclei or even protons, they are much more efficient in this process. With xrays the interaction is with the electron mantle of the atoms. In the case of electron beams, say in an electron microscope, scattering is from both the electron mantle and the atom nuclei, and neutrons interact with the nucleus only. The final result of a crystallographic experiment is not a picture of the atoms, but a map of the distribution of electrons in the molecule, i.e., an electron density map (Figure 2.16). Because the electrons are mostly tightly localized around the nuclei, the electron density map gives us a pretty good picture of the molecule. As we do not have a lens we do not get the electron density map directly; the xray diffraction patterns from a crystal are related to the object diffracting the waves through a Fourier transform. If one thinks of electron density as a mathematical function: ρ(x, y, z)
(2.17)
49
with x, y, z indices for real space, then the diffraction pattern is the Fourier transform of that electron density function and given as: F(hkl) = T[ρ(x, y, z)]
(2.18)
where F(hkl) is the structure factor (a scattered wave, therefore a complex number with amplitude and phase) with hkl indices in reciprocal space, and T is the forward Fourier transform of ρ(x, y, z). As we saw in Equation 2.16, the reverse relationship holds also, namely: ρ(x, y, z) = T −1 {T[ρ(x, y, z)]}
(2.19)
where T −1 is the inverse Fourier transform. This expression tells us that the inverse Fourier transform of the Fourier transform of an object is the original object. The latter is a rewording of Abbe’s treatment of image generation as presented in Chapter 5. The intensity in an xray diffraction photograph is the square of the amplitude of the diffracted waves, F(X)2, or the recorded diffraction pattern of an object is the square of the Fourier transform of that object. In a diffraction pattern, each point arises from the interference of rays scattered from all irradiated portions of the object. To determine the image, one must measure or calculate the structure factor F(X) at many or all points of the diffraction pattern. Each F(X) is described by an amplitude and a phase, but in recording the intensity of the diffracted xrays, the phase information is lost. This is referred to as the phase problem. Xray phases could be obtained directly if it were possible to rediffract (focus) the scattered rays with an xray lens to form an image; unfortunately, an xray lens does not exist. With xrays we can thus detect diffraction from molecules, but we have to use a computer to reassemble an image as shown in Figure 2.16. The process is summarized in Figure 2.17. We will now learn how the xray diffraction pattern, F(X), comes about and how the expected intensities in the diffraction pattern are calculated to solve Equation 2.19, i.e., how to reconstitute the image that led to the measured xray diffraction pattern. Bragg’s Law
FIGURE 2.16 Electron density map of adenosine triphosphate (ATP).
In 1913 W.H. and W.L. Bragg (a father and son team) proposed that the condition for constructive
50
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
FIGURE 2.17 With xrays, we can detect diffraction from molecules, but we have to use a computer to reassemble the electron density/molecular structure image.
specular reflection of xrays from a set of crystal planes separated by a distance dhkl could be represented as: 2dhkl sin θ = nλ
(2.20)
This expression basically tells us that constructive interference of waves reflected by successive crystal planes occurs whenever the path difference (2dhklsin θ) is an integral multiple (n) of the wavelength λ. Also, for each (hkl) family of planes, xrays will only diffract at one angle θ. The integer n is known as the order of the corresponding reflection. Because Bragg reflection can only occur for λ ≤ 2d, one needs xrays with wavelengths in the Ångstrom range to resolve crystal planes. The Bragg equation is easily derived from an inspection of Figure 2.18. Bragg’s law is a result of the periodicity of the lattice with the atoms in the crystal basis controlling the relative intensity of the various orders (n) of diffraction from a set of parallel (hkl) planes. This basic equation is the starting point for understanding crystal diffraction of xrays, electrons, neutrons, and any other particles that have a de Broglie wavelength Incident beam
Reﬂected beam
Upper plane
(Chapter 3) less than the interatomic spacing. Although the reflection from each plane is specular, only for certain values of θ will the reflections from all planes add up in phase to give a strong reflected beam. Each plane reflects only 10 −3 to 10−5 of the incident radiation, i.e., it is not a perfect reflector. Hence, 103 to 105 planes contribute to the formation of the Braggreflected beam in a perfect crystal. The composition of the basis determines the relative intensity of the various orders of diffraction. Laue Equations In 1912 von Laue predicted that diffraction patterns of xrays on crystals would be entirely analogous to the diffraction of light by an optical grating.* In the von Laue approach there is no ad hoc assumption of specular reflection, as in the case of Bragg’s law. Instead, this more general approach considers a crystal as composed of sets of ions or atoms at the sites of a Bravais lattice that reradiate the incoming xrays. For both optical gratings and crystals only the repeat distances of the periodic structure and the wavelength of the radiation determine the diffraction angles. Let us inquire first into the interference conditions for waves originating from different but identical atoms in a single row—the onedimensional diffraction case. The scattering atoms in a line form secondary, coherent xray sources (scattering from two atoms is shown in Figure 2.19).
d
Lower plane
*
d sin
FIGURE 2.18 Schematic used to derive the Bragg equation.
We will encounter the diffraction of light by an optical grating again in Volume II, Chapter 1 on photolithography, where we discuss patterning of a photoresist with UV light, using a mask with a grating structure on it.
51
Crystallography
the lattice points (see Figure 2.20). Because crystals are periodic in three directions, the Laue equations in 3D are then: a1(cos A cos A 0 ) e L a 2 (cosB cosB0 ) f L a 3 (cos G cos G 0 ) g L
FIGURE 2.19 Two scattering atoms act as coherent secondary sources.
Constructive interference will occur in a direction such that contributions from each lattice point differ in phase by 2π. This is illustrated for the scattering of an incident xray beam by a row of identical atoms with lattice spacing a1 in Figure 2.20. The direction of the incident beam is indicated by wave vector k0 or the angle α0, and the scattered beam is specified by the direction of k or the angle α. Because we assume elastic scattering, the two wave vectors k0 and k have the same magnitude, i.e., 2π/λ but with differing direction. A plane wave* eik.r is constant in a plane perpendicular to k and is periodic parallel to it, with a wavelength λ = 2π/k (see Appendix 2A). The path difference A1B − A2C in Figure 2.20 must equal eλ with e = 0, 1, 2, 3, …. For a fixed incident xray with wavelength λ and direction k, and an integer value of e, there is only one possible scattering angle α defining a cone of rays drawn about a line through k0
For constructive interference from a threedimensional lattice to occur, the three equations above must all be satisfied simultaneously, i.e., six angles α, β, γ, a, α0, β0, and γ0; three lattice lengths a1, a 2, and a 3; and three integers (e, f, and g) are fixed. Multiplying both sides of Equation 2.21 with 2π/λ and rewriting the expression in vector notation we obtain: a1 (k k 0 ) 2Pe a 2 (k k 0 ) 2Pf
(2.22)
a 3 (k k 0 ) 2Pg with a1, a 2, and a 3 being the primitive vectors of the crystal lattice. When two of the conditions in Equation 2.22 are met, one entire plane array scatters in phase. This is depicted in Figure 2.21, where two cones of allowed diffracted rays are depicted. The two conditions are met simultaneously only in two directions along which the cones intersect. To satisfy all three Laue equations simultaneously, the diffracted beam can only have one allowed direction because three cones can mutually intersect along only one line.
C
0
A2 A1
k k
a1
B
k
FIGURE 2.20 Scattering of an incident xray beam (incident direction is k0) by a row of identical atoms with lattice spacing a1. The scattered beam is specified by the direction k. The path difference A1B − A2C must equal eλ, with e = 0,1,2,3,.... (Drawing by Mr. Chengwu Deng.)
*
(2.21)
The complex exponential representation for periodic functions is convenient for adding waves, taking derivatives of wave functions, and so on. It is equivalent to a linear combination of a sine and cosine function, because eiθ = cosθ + i sinθ (Euler) (see also Appendix 2A).
a
k
a
FIGURE 2.21 Each Laue condition produces a cone of allowed rays. In a plane array the entire plane scatters in phase in two directions. These two directions are along the intersection of the two cones. (Drawing by Mr. Chengwu Deng.)
52
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
k
k = k – k0
Reflecting plane
–k0
FIGURE 2.22 Max von Laue (1897–1960).
If we further define a vector Δk = k − k0, Equation 2.22 simplifies to: a1 $k 2Pe a 2 $k 2Pf
(2.23)
a 3 $k 2Pg Dealing with 12 variables for each reflection simultaneously [six angles (α, β, γ, a, α0, β0, and γ0), three lattice lengths (a1, a 2 and a 3), and three integers (e, f, and g)] is a handful; this is the main reason why the Laue equations are rarely referred to directly, and a simpler representation is used instead. The reflecting conditions can indeed be described more simply by the Bragg equation. Historically, von Laue (Figure 2.22) developed his equations first; it was one year after his work that the father and son team William Henry and William Lawrence Bragg (Figure 2.23) introduced
FIGURE 2.24 In case of mirrorlike Bragg reflection, the vector ∆k, the summation of the unit vectors representing incoming (k0) and reflected rays (k), is normal to the plane that intersects the 2θ angle between them. (Drawing by Mr. Chengwu Deng.)
the simpler Bragg’s law. Max von Laue and the Braggs received the Nobel Prize in Physics in 1914 and 1915, respectively. Further below we will learn that constructive interference of diffracted xrays will occur provided that the change in wave vector, Δk = k − k0, is a vector of the reciprocal lattice. Bragg’s law is equivalent to the Laue equations in one dimension as can be appreciated from an inspection of Figures 2.24 and 2.25, where we use a twodimensional crystal for simplicity. Suppose that vector Δk in Figure 2.24 satisfies the Laue condition; because incident and scattered waves have the same magnitude (elastic scattering), it follows that incoming (k0) and reflected rays (k) make the same angle θ with the plane perpendicular to Δk.
a a
a
a
FIGURE 2.23 Father and son Bragg: Sir William Henry and William Lawrence Bragg.
FIGURE 2.25 Connecting Bragg's law with Laue equations and Miller indices. (Drawing by Mr. Chengwu Deng.)
Crystallography
53
The magnitude of vector Δk, from Figure 2.24, is then given as: $k 2k sin Q
(2.24)
We now derive the relation between the reflecting planes to which Δk is normal and the lattice planes with a spacing dhkl (see Figure 2.25 and Bragg’s law in Equation 2.20). The normal unit vector nˆ hk and the interplanar spacing dhk in Figure 2.25 characterize the crystal planes (hk). From Equation 2.23 we deduce that the direction cosines of Δk, with respect to the crystallographic axes, are proportional to e/a1, f/a2, and g/a3 or: e/a1:f/a 2:g/a3
(2.25)
From the definition of the Miller indices, an (hkl) plane intersects the crystallographic axes at the points a1/h, a2/k, and a3/l, and the unit vector nˆ hkl , normal to the (hkl) plane, has direction cosines proportional to: h/a1, k/a 2, and l/a3
(2.26)
Comparing Equations 2.25 and 2.26 we see that Δk and the unit normal vector nˆ hkl have the same directions; all that is required is that e = nh, f = nk, and g = nl, where n is a constant. The factor n is the largest common factor of the integers e, f, and g and is itself an integer. From the above, Laue’s equations can also be interpreted as reflection from the h,k,l planes. From Figure 2.25 it can be seen that the spacing between the (hk) planes, and by extension between (hkl) planes, is given as*: d hkl
nˆ hkl a1 nˆ a nˆ a hkl 2 hkl 3 h k l
(2.27)
Because Δk is in the direction of the normal nˆ hkl and comes with a magnitude given by Equation 2.24, we obtain Bragg’s law from the Laue’s equations as: a1 $k a1 nˆ hkl 2k sin Q 2Pe
(2.28)
or: hd hkl
*
4P sin Q 2Pe L
(2.29)
Notice that in the case of a cubic crystal, Equation 2.27 can be simplified to give the distance between planes as in Equation 2.12.
FIGURE 2.26 Sodium deoxyribose nucleate from calf thymus. (Structure B, Photo 51, taken by Rosalind E. Franklin and R.G. Gosling.) Linus Pauling’s annotations are to the right of the photo (May 2, 1952).
and with e = nh: 2d hkl sin Q nL
(2.30)
In the Bragg equation we treat xray diffraction from a crystal as a reflection from reciprocal lattice planes rather than scattering from atoms. This construction has fewer variables than the Laue equations because reflections are wholly represented in two dimensions only. In Figure 2.26 we reproduce what is possibly the most famous xray diffraction photograph. It was this photograph—photo 51 of DNA taken by Rosalind Franklin and R.G. Gosling—that convinced Watson and Crick that the DNA molecule was helical. The discovery of the double helix followed soon after, as well as an enduring controversy that Franklin probably did not get the credit she deserved in the elucidation of the DNA structure. XRay Intensity and Structure Factor F(hkl) So far we have considered only the condition for diffraction from simple lattices for which only corner points of the unit cell are occupied. The intensity of a beam diffracted from an actual crystal will depend on the grouping of atoms in the unit cell and on the scattering power of these atoms. In this section we discuss the intensity and phase of the diffracted rays and the structure factor, F(hkl). If we treat the incident xray waves as plane waves and the atoms as ideal point scatterers, the scattered waves are spherical waves (Figure 2.19) close to the source, i.e., nearfield or Fresnel diffraction patterns form at finite
54
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
distances from the crystal and Fraunhofer diffraction patterns at infinity (farfield). In a typical xray diffraction experiment, a Fraunhofer diffraction pattern is registered at about 50 to 150 mm behind the specimen. This distance is relatively large compared to the size of the diffracting crystal unit cell (~1–50 nm in dimension) and the wavelength of the incident radiation (typically 1.54178 Å for Cu Kα and 0.71073 Mo Kα). Thus, xray diffraction methods provide a direct way to display the decomposition of xrays in component waves (frequencies), and for this reason xray diffraction may be called spatial frequency spectrum analysis or harmonic analysis. Nearfield and farfield optics are compared in more detail in Chapter 5. The number of scattered xray photons picked up by the detector results in an intensity proportional to the square of the amplitude (peak height) of the diffracted waves. The scattering intensity depends on the number and distribution of electrons associated with the scattering atoms in the basis, i.e., the structure factor F(hkl). The phase of the diffracted rays is the relative time of arrival of the scattered radiation at a particular point in space, say at the emulsion of a photographic film. The phase information is lost when the xray diffraction pattern is recorded on the film—one could say that the film integrates intensity over time—in other words, we cannot measure xray phases directly. When using a lens such as in a microscope, light first strikes the imaged object and is diffracted in various directions. The lens then collects the diffracted rays and reassembles them to form an image. The phase problem is a major concern in structure analysis as we need both intensity and phase to feed into the Fourier transform. Today several techniques exist to regenerate the lost phase information of xray diffraction, but the topic falls outside the scope of this book. We need to extract the structure factor F(hkl) from the intensities and phase of the diffraction spots and then do an inverse Fourier transform (T −1) to obtain the crystal structure/electron density function, ρ(x, y, z) (see Figure 2.17). We now mathematically derive the intensity profile of xrays scattered from a crystal. The result, as Laue predicted, is the same as for visible light diffracted from an optical grating. When an incident
B p
q r
k0
k A
FIGURE 2.27 Scattering of xrays from two nearby atoms A and B with identical scattering density. (Drawing by Mr. Chengwu Deng.)
xray beam travels inside a crystal, we assume that the beam is not much influenced by the presence of the crystal; in other words, the refractive index for xrays is close to unity, and there is not much loss of energy from the beam through scattering, i.e., elastic scattering dominates! With reference to Figure 2.27, we assume two parallel plane xray waves of wavelength λ and frequency v (hence velocity c = λv), scattered elastically from two nearby atoms A and B of identical scattering density. The wave vector for the incoming wave is k0 and that of the diffracted beam is k. Because we assume elastic scattering: k0 = k = k = 2π/λ
(2.31)
Scattering atom A is at the origin, and scattering atom B is at a distance r away from the origin. The path difference, or phase factor, between the waves can be calculated from Figure 2.27 as: p + q = r·(k − k0) = r·Δk
(2.32)
The equations for the wave amplitudes are (for those readers less familiar with wave equations, consult Appendix 2A for more details): Af i( k0 l A W t ) e lA
(2.33)
Af i( k0 lB W t r $k ) e lB
(2.34)
Y ! ( x , t)
and:
Y " ( x , t)
where A is the amplitude and f is the atomic scattering factor defined as the ratio of the amplitude of an electromagnetic wave scattered by atom A and that
55
Crystallography
of a wave scattered by a free electron. The position of the detector with respect to atom A is given by lA , and the position of the detector relative to atom B is lB. The product r ⋅ Δk is the phase factor we calculated in Equation 2.32. Generalizing, an xray wave scattered from the jth atom in a crystal is: Af j i(k0 lj W t rj $k) e lj
9j x,t
(2.35)
Assume now a crystal with base vectors a1, a 2, and a 3 and a total number of atoms along each axis of M, N, and P, respectively, and also accept that there is only a single atom at each lattice point (i.e., fj = 1), then the amplitude of the total wave will be proportional to:
¤
9 ( x,t ) t F(h,k,l)
i(rj $k )
all atoms M–1
where r j is the position of scatterer j relative to scatterer A, and lj is the position of the detector with respect to scatterer j. The total scattered wave amplitude at the detector is the sum of all the contributing atoms: 9 x,t
e
N–1
P–1
¤ ¤ ¤e
m0
n 0
i ¨ª( ma1 +na 2 pa 3 ) $k ·¹
p0
after rearrangement we obtain: M–1
9 ( x,t ) t F(h,k,l)
¤e
N–1 ima1 $k
m0
Af j i(k0 lj W t) i(rj $k) e e all atoms lj
¤e
P–1 ina 2 $k
n 0
¤e
ipa 3 $k
p0
¤
A i(k0 L W t) e L
(2.38) (2.36)
¤
f je
i(rj $k )
all atoms
For a small sample, the distances lj are all about the same (the crystal is small compared to the distance between it and the detector), so in Equation 2.36 we can replace lj with L. Constructive and destructive interference between the scattered waves that reach the detector is the result of the sum of all scatterers and the scattering vector, Δk, and determines where the detector should be put. The term F(hkl):
The intensity of the scattered wave is the square of the wave amplitude, and taking the value of one of the sums in Equation 2.38 for a crystal of dimension Ma1 in the direction of a1, we obtain: M–1
¤e
m0
ima1 $k
1 e iM(a1 $k ) 1 e i(a1 $k )
and I t 9 ( x,t) 2 t
[1 e –iM(a1 $k ) ][1 e iM(a1 $k ) ] [1 e –i(a1 $k ) ][1 e i(a1 $k ) ]
which simplifies to
(2.37)
It
2 e –iM(a1 $k ) e iM(a1 $k ) ] 2 2 cos(Ma1 $k) 2 2 cos(a1 $k) [2 e –i(a1 $k ) e i(a1 $k ) ]
from the expression 2.36 for the wave amplitude, is the geometrical structure factor. It is defined, in analogy with the atomic scattering factor, as the ratio of the amplitude of the wave scattered by all atoms in a unit cell and that scattered by a free electron for the same incident beam. It incorporates the scattering of all atoms of the unit cell and sums up the extent to which interference of the waves scattered from atoms within the basis diminishes the intensity of the diffraction peaks. So even if the Laue condition is met, the structure factor may be zero and no diffraction will be observed. In the case that there is only one type of atom in the basis, the atomic scattering factor fj disappears (fj = 1)—identical atoms have identical scattering factors.
It
1 cos(Ma1 $k) and with the identity 1 cos(a1 $k)
F(hkl)
¤
f je
i(rj $k )
all atoms
cos 2x cos 2 x sin 2 x 1 2sin 2 x ¥1 ´ sin 2 ¦ Ma1 $k µ §2 ¶ It ¥1 ´ sin 2 ¦ a1 $k µ §2 ¶
(2.39)
This is the same result as the light intensity profile expected from an Mslit diffraction grating (see Chapter 5 on photonics). If M is large (~108 for a macroscopic crystal), it has very narrow, intense peaks. Between the peaks the intensity is essentially zero. In Figure 2.28 we have plotted y = sin2Mx/sin2 x.
56
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
reciprocal lattice so that the set of all wave vectors Δk yields plane waves with the periodicity of a given Bravais lattice. From the above, the intensity of the xray diffraction is:
y
¤
I t F(X)2 x=
x=0
x = 2
This function is virtually zero except at the points where x = nπ (n is an integer including zero), where it rises to the maximum value of M2. The width of the peaks and the prominence of the ripples are inversely proportional to M. Remember that there are three sums in Equation 2.38. For simplicity we only evaluated one sum to calculate the intensity in Equation 2.39. The total intensity equals:
i(rj $k )
2
(2.41)
all atoms
x
FIGURE 2.28 Graphical presentation of y = sin2Mx/sin2x. The width of the peaks and the prominence of the ripples are inversely proportional to M.
f je
So what we measure from the xray film is intensity I, and the dependence of that intensity on the atomic position follows from the Fourier expansion of the electron density function in Equation 2.17: R(x,y,z)
¤ ¤ ¤ F(hkl)e h
k
i(rj $k )
(2.42)
l
where F(hkl) is the coefficient to be determined, and h, k, and l are integers over which the series is summed. Because of the 3D periodicity, a triple summation is required: 1 1 1
F(hkl)= ° ° ° R(x,y,z)e
¥1 ´ ¥1 ´ sin ¦ Ma1 $k µ sin 2 ¦ Na 2 $k µ §2 ¶ §2 ¶ It s ¥1 ´ ¥1 ´ sin 2 ¦ a1 $k µ sin 2 ¦ a 2 $k µ §2 ¶ §2 ¶ 2
¥1 ´ sin 2 ¦ Pa 3 $k µ §2 ¶ s ¥1 ´ sin 2 ¦ a 3 $k µ §2 ¶
i(rj $k )
dxdydz
(2.43)
0 0 0
(2.40)
so that the diffracted intensity will equal zero unless all three quotients in Equation 2.40 take on their maximum values at the same time. This means that the three arguments of the sine terms in the denominators must be simultaneously equal to integer multiples of 2π, or the peaks occur only when: a1 $k 2Pe a 2 $k 2Pf a 3 $k 2Pg These are, of course, the familiar Laue equations. As we will see below, to solve for the wave vector Δk it is very convenient to introduce the concept of a
If we knew all the F(hkl) values, we could calculate the electron density, and vice versa. Unfortunately, as remarked above, Equation 2.42 requires values of F(hkl), but the measured intensities only give us F(hkl)2. The apparent impasse is known as the phase problem and arises because we need to know both the amplitude and the phase of the diffracted waves to compute the inverse Fourier transform.
Reciprocal Space, Fourier Space, kSpace, or Momentum Space Introduction The crystal lattice discussed above is a lattice in real space. Practice has shown the usefulness of defining a lattice in reciprocal space for the interpretation of diffraction patterns of single crystals, the simple reason being that a diffraction pattern reveals the reciprocal lattice. We did already consider some reciprocal features when we introduced the Miller indices, which are derived as the reciprocal of the unit cell intercepts. Because the lattice distances
57
Crystallography
between planes are proportional to the reciprocal of the distances in the real crystal (i.e., they are proportional to 1/dhkl), the array is called a reciprocal lattice. We will learn in this section that the condition for nonzero intensity in scattered xrays is that the scattering vector Δk = k − k0 is a translation vector, Ghkl, of the reciprocal lattice, i.e., Δk = Ghkl. One can describe a reciprocal lattice the same way we describe a real one, but one must keep in mind that in one case the points are the position of real objects (atoms or the base), whereas in the other case they mark the positions of abstract points—magnitude and direction of momentum. Reciprocal space, also called Fourier space, kspace, or momentum space, plays a fundamental role in most analytical studies of periodic structures. After the introduction of the reciprocal lattice we will discuss the conditions for xray diffraction in terms of such a lattice and end with an introduction to Brillouin zones. The concepts introduced here are not only needed to understand xray diffraction better, they also are required preparation for Chapter 3, where we deal with band theory of solids.
The Reciprocal Lattice Graphical Presentation of the Reciprocal Lattice Before introducing a reciprocal lattice mathematically, let us learn how to draw one as we demonstrate in Figure 2.29. In this example we start with the twodimensional unit cell of a monoclinic crystal with a1 and a2 in the plane of the paper. The figure also shows the edges of four (hkl) planes: (100), (110), (120), and (010). These planes all are perpendicular to the face of the paper. To construct the reciprocal lattice we draw from a common origin a normal to each plane. Next we place a point on the normal to each plane (hkl) at a distance 2π/dhkl from the origin. Each of the points thus obtained maintains the important features of the stack of parallel planes it represents. The direction of the point from the origin preserves the orientation of the planes, and the distance of the point from the origin preserves the interplanar distance. A doubling of the periodicity in real space will produce twice as many diffraction spots in reciprocal space. It is convenient to let the reciprocal lattice vector, Ghkl, be 2π times the reciprocal of the
b 040
030
220 120
020
210 a 110
(110) a2
010
300 200
(120) 100 (010)
c (100)
a1
FIGURE 2.29 Graphical construction of the reciprocal lattice. (Drawing by Mr. Chengwu Deng.)
interplanar distance, dhkl. This convention converts the units from periods per unit length to radians per unit length. This simplifies comparison of different periodic phenomena, e.g., a crystal lattice and light that interacts with it. For instance, Δk, the wave vector, has an absolute value of 2π/λ. If we choose this scaling factor, we are able to compare the two values directly, and all it really does in our drawing is to expand the size of the reciprocal lattice. Definition of the Reciprocal Lattice Now that we can draw a reciprocal lattice in 2D, let us define what a reciprocal lattice is. Imagine a set of points R constituting a Bravais lattice and a plane wave, eik·r, interacting with that lattice. For most values of k, a plane wave will not have the periodicity of the Bravais lattice of points R. Only a very special * * * set of the wave vectors, G hkl h a 1 k a 2 l a 3 , of the reciprocal lattice satisfies that condition. Mathematically, Ghkl belongs to the reciprocal lattice of points R of the Bravais lattice, if the relation: e iGhkl (r +R ) e iGhkl r
(2.44)
holds for any r, and for all R in the Bravais lattice. From Equation 2.44 it follows that we can describe
58
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
the reciprocal lattice as the set of wave vectors Ghkl satisfying: e iGhkl R 1
R· Δk = 2πm
eiR ⋅ Δk = 1
(2.47)
We see from Equation 2.47 that if Δk is equal to any reciprocal lattice vector Ghkl, then the Laue equations for wave diffraction are satisfied. The diffraction condition is thus simply: Δk G hkl
(2.48)
or from Equation 2.23 (with e = h, f = k and g = l): G hkl a1 2Ph G hkl a 2 2Pk
(2.49)
G hkl a 3 2Pl The expression Δk = Ghkl can be represented in the form of a vector triangle as illustrated in Figure 2.30. Because k and k0 are of equal length, i.e. 2π/λ, the triangle O, O’, O’’ has two equal sides. The angle between k and k0 is 2θ, and the hkl plane dissects it. In the twodimensional reciprocal lattice shown at the bottom of Figure 2.31, the Ghkl vectors give the outline of the unit cell. Vector a1* = G100 and a3* = G 001 and: 2P 2P and a*3 d100 d001
(2.50)
O´ k0
O
k0
Bravais lattice
a1
(002)
(001)
a3 (101)
Reciprocal lattice vectors
a1 = G100
a3 = G001
FIGURE 2.31 Reciprocal lattice vectors a1* = G100 and a3* = G001 in a monoclinic unit cell and their relation to the Bravais lattice. (Drawing by Mr. Chengwu Deng.)
The angle β* between the reciprocal lattice vectors in Figure 2.31 is the complement of β in the Bravais lattice. The components of any vector referred to the reciprocal lattice represent the Miller indices of a plane whose normal is along that vector, whereas the spacing of the plane is given by the inverse of the magnitude of that vector multiplied by 2π. For example, the reciprocal lattice vector u* = [123] is normal to the planes with Miller indices (123) and has an interplanar spacing 2π/u*. Explicit Algorithm for Constructing the Reciprocal Lattice We can write out the change in wave vector, Ghkl = Δk = k − k0, in the following expression: Ghkl = Δk = ea*1 + fa*2 + ga*3
(2.51)
where e, f, and g are the integers from the Laue equations (Equation 2.23) and a1*, a2* and a3* are basis vectors of the reciprocal lattice to be determined. Equation 2.51 is a solution of the Laue Equation 2.23 if all of the following relations are satisfied: a*1 a1 a*2 a 2 a*3 a 3 2P
(102)
(2.46)
with integer m. Because exp[i2π(integer)] = 1, this can be written in the equivalent form:
(hkl) plane
(101)
(2.45)
for all R in the Bravais lattice. Because lattice scatterers are displaced from one another by the lattice vectors R, the condition that all scattered rays interfere constructively is that the Laue equations hold simultaneously for all values of Bravais lattice vectors R, or:
a*1
(100)
k = Ghkl
k O˝
FIGURE 2.30 Vector triangle representation of ∆k = Ghkl. (Drawing by Mr. Chengwu Deng.)
a*1 a 2 a*2 a1 a*3 a 2 a*1 a 3 a*2 a 3 a*3 a1 0
(2.52)
From Equation 2.52, a*1 is perpendicular to primitive lattice vectors a 2 and a 3 of the direct lattice. A vector
Crystallography
59
TABLE 2.3 Bravais Lattice after Fourier Transform Real Space
Fourier Space
Normals to the planes (vectors) Spacing between planes λ is distance, wavelength
Points 2π/distance planes 2π/λ is momentum or wave number WignerSeitz cell
First Brillouin zone (see below)
that is perpendicular to a 2 and a 3 is given by the vector product a 2 × a 3. To construct a*1 of the reciprocal lattice completely, we must normalize a 2 × a 3 to satisfy the expression a*1 ⋅ a1 = 2π. All the equations in 2.52 are thus satisfied when choosing: 2P a 2 s a 3 a1 a 2 s a 3 2P a 3 s a1 a*2 y a1 a 2 s a 3 2P a1 s a 2 a*3 y a1 a 2 s a 3 a*1 y
Reﬂecting planes
O˝ Ghkl k
k0
O´ –Ghkl
O
FIGURE 2.32 The reciprocal lattice and the geometry of diffraction clarified by the Ewald sphere. The sphere with center O intersects the reciprocal lattice center O’. (Drawing by Mr. Chengwu Deng.)
(2.53)
The denominators have been written the same way because of the property of the triple scalar product: a1 ⋅ a 2 × a 3 = a 2 ⋅ a 3 × a1 = a 3 ⋅ a1 × a 2. The magnitude of this triple product is the volume of the primitive cell. In Table 2.3 we summarize the properties of a Bravais lattice before and after a Fourier transform. The Ewald Construction The Ewald construction is a way to visualize the Laue condition that the change in wave vector, Δk, must be a vector of the reciprocal lattice. We reconsider for a moment the vector representation of the von Laue condition Δk = Ghkl represented in the form of a vector triangle in Figure 2.30. Because k and k0 are of equal length (= 2π/λ) the triangle O, O’, O’’ has two equal sides, and we can draw a sphere with k = k0 = 2π/λ as illustrated in Figure 2.32. The angle between k and k0 is 2θ, and the hkl plane dissects it. Diffraction of the incoming beam represented by the vector k0 giving the vector k may be thought of as reflection from the dotted line in this diagram (as in Bragg’s Law). We will now see that with Δk = Ghkl the diffraction vector corresponds to the distance between planes in reciprocal space. We thus superimpose an imaginary sphere of xray radiation on the reciprocal lattice as illustrated
in Figure 2.32. Somewhat confusingly, one might consider two origins: O, which is the center of the sphere and may be considered as the position of the crystal, is the source of the secondary beam k, and O’ is the origin of reciprocal space, the origin of the diffraction vector Δk = Ghkl, and the center of the reciprocal lattice. As the crystal rotates, the reciprocal lattice rotates in exactly the same way. Any points in reciprocal space that intersect the surface of the sphere reveals where diffraction peaks will be observed if the structure factor is nonzero. In other words, reflection is only observed if the sphere intersects a point where Δk = Ghkl. The diffraction angle, θ, is then half the angle between the incident and diffracted wave vectors. It is useful to think of the crystal at the center of the Ewald sphere (O) being linked to the center (origin) of the reciprocal lattice (O’) by something like a bicycle chain—the two “objects” rotate exactly in step with each other. The Ewald construction also makes for a good link with the Brillouin zones discussed in the next section. Notice in Figure 2.32 that both Ghkl and −Ghkl are vectors in reciprocal space. It can be seen that a reflecting plane bisects the vector Ghkl at Ghkl/2 and another reflecting plane cuts −Ghkl at −Ghkl/2. The incident wave vector k0 starting from the Ewald circle’s center O must terminate at the −Ghkl/2 reflecting plane for
60
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology (a) 1.5
(b) 1.5
1.0
1.0
3
0.0
0.5 2
1
ky
ky
0.5
3
–0.5
0.0
2
1
–0.5 4
–1.0
–1.0
–1.5 –1.5 –1.0 –0.5
0.0 kx
0.5
1.0
1.5
–1.5 –1.5 –1.0 –0.5
4 0.0 kx
0.5
1.0
1.5
FIGURE 2.33 The Brillouin zones for (a) a square 2D lattice and (b) a triangular 2D lattice. The solid circles are the lattice points, and the dashed lines are the Bragg lines. The first four Brillouin zones are marked with different gray scales.
diffraction to occur. This observation gives rise to the idea of using the reciprocal lattice to construct Brillouin zones, the boundaries of which satisfy the Laue conditions for diffraction. Bragg planes bisect the lines joining the origin to points of the reciprocal lattice, and one can define the first Brillouin zone as the set of points that can be reached from the origin without crossing any other Bragg planes. Recall that this was also the way we learned how to construct WignerSeitz cells. So the first Brillouin zone is the WignerSeitz cell of the reciprocal lattice.
Brillouin Zones Leon Brillouin (1889–1969) was a FrenchAmerican physicist who was a professor at the Sorbonne, Collège de France, Wisconsin, Columbia, and Harvard. He also worked briefly at IBM. In the previous section
Lattice real space
Lattice kspace
BCC WignerSeitz cell
BCC BZ (FCC lattice in kspace)
FCC WignerSeitz cell
FCC BZ (BCC lattice in kspace)
FIGURE 2.34 The WignerSeitz cell of BCC lattice in real space transforms to a Brillouin zone in an FCC lattice in reciprocal space, whereas the WignerSeitz cell of an FCC lattice transforms to a Brillouin zone of a BCC lattice in reciprocal space.
we used the Ewald sphere (Figure 2.32) as a way to introduce the important concept of Brillouin zones. A Brillouin zone is defined as a WignerSeitz cell in the reciprocal lattice and gives a geometric interpretation of the diffraction condition. The WignerSeitz cell of the reciprocal lattice is the set of points laying closer to Δk = 0 than to any other reciprocal lattice point. The Brillouin construction exhibits all wave vectors k that can be Bragg reflected by the crystal. The constructions divide the Fourier space into zones, out of which the first Brillouin zone is of greatest importance. We have just seen that xray waves traveling in a crystal lattice undergo Bragg reflection at certain wave vectors. The first Brillouin zone is the set of points in kspace that can be reached from the origin without crossing any Bragg reflection plane. The second Brillouin zone is the set of points that can be reached from the first zone by crossing only one Bragg plane. The nth Brillouin zone can be defined as the set of points that can be reached from the origin by crossing n − 1 Bragg planes, but no fewer. Each Brillouin zone is a primitive cell of the reciprocal lattice. In Figure 2.33 we illustrate the first four Brillouin zones in square and triangular twodimensional Bravais lattices. For examples of 3D WignerSeitz cells, corresponding to Brillouin zones, see Figures 2.6 and 2.34.
Nothing Is Perfect Even a crystal having a mass of less than 0.1 g is likely to have more than 1023 ions, and it is unrealistic to
61
Crystallography
expect that the growth of such crystal from solution can lead to zero impurities or imperfections. Successive purification steps may remove impurities, but even in the purest crystal, thermodynamics predicts the existence of some structural intrinsic imperfections. There are at least four types of defects one distinguishes: 1) point defects where the irregularity in structure extends over only a few atoms in size (0D), 2) linear defects where the irregularity extends across a single row of atoms (1D), 3) planar defects with an irregularity extending across a plane of atoms (2D), and 4) volumetric defects with the irregularity taking place over 3D clusters of atoms. In addition, defects can be categorized as either intrinsic, where defects are induced because of physical laws, and extrinsic, where defects are present because of the environment and/or processing conditions. A physical law imposing the presence of intrinsic defects in a crystal is the minimization of the Gibbs free energy (G). The Gibbs free energy is higher in a crystal without vacancies than one with vacancies (G = H − TS = minimum). This is because defects are energetically unfavorable but are entropically favorable. Formation of vacancies (n) does indeed increase the enthalphy H of the crystal because of the energy required to break bonds (ΔH = nΔHf ), but vacancies also increase S of the crystal as a result of an increase in configurational entropy. The configurational entropy is given as: S = klnW
(2.54)
where W is the number of microstates. If the number of atoms in the crystal is N and the number of vacancies is n, then the total number of sites is n + N, and the number of all possible microstates W may be calculated from: W
(N n)! n!N!
(2.55)
and the increase in entropy ΔS is then given by: $S klnW kln
(N n)! n!N!
(2.56)
$G n$Hf T$S
(2.57)
H = nHf
G of a perfect crystal
G = HTS neq
n
TS
FIGURE 2.35 Change in Gibbs free energy G of a crystal as a result of the number of vacancies n.
This expression is plotted in Figure 2.35. It can be seen that for a crystal in equilibrium, vacancies are required to be present at any temperature above 0 K. The equilibrium concentration neq is calculated from: u$G 0 un n neq
(2.58)
n eq ¥ $Hf ´ exp ¦ § kT µ¶ N
(2.59)
or we obtain:
so the neq should increase with increasing temperature. For Al, ΔHf = 0.70 eV/vacancy and for Ni, ΔHf = 1.74 eV/vacancy, leading to the values for neq /N at three different temperatures as shown in Table 2.4. Defects, even in very small concentrations, can have a dramatic impact on the properties of a material. Actually, without defects solidstate electronic devices could not exist, metals would be much stronger, ceramics would be much tougher, and some crystals would have no color. Vacancies even make a small contribution to the thermal expansion of a crystal. Some commonly observed defects are summarized in Table 2.5; they are categorized here as point defects (0D), line defects (1D), and plane defects (2D). The simplest sorts of defects are those based on points (0D). In Figure 2.36 we review point defects, including vacancies, interstitial atoms, small and TABLE 2.4 neq/N Values for Al and Ni at Three Different Temperatures neq/N
and the total free energy change as:
H
G
0K
300 K −12
900 K
Al
0
1.45 10
1.12 10−4
Ni
0
5.59 10−30
1.78 10−10
62
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 2.5 Common Defects in Crystals Type of Imperfection
Description
Point defects: Interstitial
Extra atom in an interstitial site
Schottky defect Frenkel defect
Atom missing from correct site Atom displaced to interstitial site creating nearby vacancy
Line defects: Edge dislocations
Screw dislocations
Plane defects: Lineage boundary
Grain boundary Stacking fault
Row of atoms marking edge of a crystallographic plane extending only part way in crystal Row of atoms about which a normal crystallographic plane appears to be spiral
Boundary between two adjacent perfect regions in the same crystal that are slightly tilted with respect to each other Boundary between two crystals in a polycrystalline solid Boundary between two parts of a closest packing having alternate stacking sequences
large substitutional atoms, and the intrinsic Frenkel and Schottky defects. A missing atom is a vacancy; a dissimilar atom in a nonlattice spot is an interstitial; and a different atom in a lattice position is substitutional. Vacancies are required in ionic solids, just like they are in metals, but the vacancies must be formed in such a way that the solid remains charge neutral. The two main ways
(a)
(b)
(c)
– + – + (d)
(e)
+ – + – – – + + – + – + – +
+ – + –
(f )
FIGURE 2.36 Point defects: vacancy (a), interstitial atom (b), small (c) and large (d) substitutional atom, Frenkel (e), and Schottky defect (f).
to create point defects in ionic solids without causing a charge imbalance are through correlated vacancies (Schottky defects, for the German who described them in 1930) and through correlated vacancy/ interstitial pairs (Frenkel defects, for the Russian who first described them in 1924). Impurities, such as dopants in singlecrystal Si (see Chapter 4), are atom(s) of a type that do not belong in the perfect crystal structure. An impurity atom in a pure crystal will generally raise the enthalpy (H) somewhat and increase the entropy (S = klnW) a lot. In other words, there will always be some impurities present for the same reason as vacancies form in a pure crystal. When doping a crystal we introduce impurities on purpose (see Chapter 4), perhaps turning the material into an extrinsic semiconductor. Because of defects, metal oxides may also act as semiconductors. Some nonstoichiometric solids are engineered to be ntype or ptype semiconductors. Nickel oxide (NiO) gains oxygen on heating in air, producing Ni3+ sites acting as electron traps, resulting in ptype semiconductor behavior. On the other hand, ZnO loses oxygen on heating, and the excess Zn metal atoms in the sample are ready to donate electrons, leading to ntype semiconductor behavior. Color centers are imperfections in crystals that cause color. The simplest color center is found in sodium chloride, normally a colorless crystal. When sodium chloride is bombarded with highenergy radiation, a Cl− can be ejected, creating a vacancy. Momentarily the crystal is no longer electrically neutral, and to regain stability, it grabs an available electron and sticks it in the vacancy previously occupied by the ejected Cl−. With the electron replacing the ejected Cl−, there are now equal numbers of positive and negative charges in the crystal, and the electron is held firmly in its site by the surrounding positively charged Na+ ions. This process turns the colorless salt crystal into an orange/brown. These electrons are color centers, often referred to as Fcenters, from the German word Farben, meaning color. The color center can also exist in an excited state, and the energy needed to reach that excited state is equal to the energy of a visible photon. The color center absorbs a “violet” photon, causing a jump to the excited state, and the crystal appears with the color orange/ brown (the complement of violet). Analogous color
Crystallography
63
FIGURE 2.37 Color centers in some wellknown minerals: (a) the Dresden green diamond, (b) smoky quartz, and (c) amethyst or violet quartz.
centers occur in several minerals. For example, a diamond with C vacancies (missing carbon atoms) absorbs light, and these centers lead to a green color (Figure 2.37). In some cases, impurities are involved in forming the color centers. Replacement of Al3+ for Si4+ in quartz gives rise to the color of smoky quartz (Figure 2.37). An iron impurity is responsible for the violet color in amethyst through the creation of a color center. The color center, not the iron impurity, is responsible for absorbing the “yellow” photon that makes amethyst violet (Figure 2.37). Line defects are 1D imperfections in a crystal structure in which a row of atoms has a local structure that differs from the surrounding crystal. These defects are extrinsic because their presence is not required by thermodynamics. They are created by material processing conditions and by mechanical forces acting on the material. In a typical material, about 5 of every 100 million atoms (0.000005%) belong to a line defect. Line defects or dislocations have a dramatic impact on the mechanical properties of metals and some ceramics. Two Hungarians, Egon Orowan and Michael Polanyi, and an Englishman, G.I. Taylor, discovered dislocations in 1934. As we will see, dislocations really govern the mechanical properties of solids, and their discovery was a very important milestone in the material science field. There are two pure types of dislocations, edge dislocations and screw dislocations, but sometimes a mixed type is displayed. An edge dislocation is the simplest type of dislocation and can be viewed as an extra halfplane of atoms inserted into the crystal. This plane terminates somewhere inside the crystal. The boundary of the halfplane is the dislocation,
shown in Figure 2.38A. A screw dislocation, shown in Figure 2.38B, is a dislocation produced by skewing a crystal so that one atomic plane produces a spiral ramp about the dislocation. A mixed dislocation is a dislocation that contains some edge components and some screws components as illustrated in Figure 2.38C. Line dislocations cannot terminate inside an otherwise perfect crystal but do end at a crystal surface, an internal surface, or interface (e.g., a grain boundary) or they form dislocation loops. Line defects are mostly caused by the misalignment of ions or the presence of vacancies along a line. When lines of ions are missing in an otherwise perfect array of ions, an edge dislocation appears. Dislocations are visible in transmission electron microscopy (TEM) where diffraction images of dislocations appear as dark lines. When a crystal surface is etched the rate of material removal at the location of a dislocation is faster, and this results in an etch pit. Symmetrical strain fields of edge dislocations produce a conical pit, whereas for a screw dislocation a spiral etch pit results. A Burgers vector b is a measure of the magnitude and direction of a dislocation. Imagine going around a dislocation line, and exactly going back as many atoms in each direction as you have gone forward, you will not come back to the same atom where you have started. The Burgers vector points from the start atom to the end atom of your journey. This “journey” is called Burgers circuit in dislocation theory. A Burgers circuit is thus a clockwise trace around the core of a dislocation, going from lattice point to lattice point, and it must go an equal number of steps left and right and an equal number
64
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology Screw dislocation
(A)
x b y
(a)
(b)
(c)
x (B) b y
Edge dislocation (a)
(b)
(c)
(C)
b b Edge Screw
FIGURE 2.38 (A) Edge dislocation: The perfect crystal in (a) is cut, and an extra plane of atoms is inserted (b). The bottom edge of the extra plane is an edge dislocation (c). A Burgers vector b is required to close a loop of equal atom spacings around the edge dislocation. (B) Screw dislocation: The perfect crystal (a) is cut and sheared over one atom spacing (b and c). The line along which shearing occurs is a screw dislocation. (C) A mixed dislocation: The screw dislocation at the front face of the crystal gradually changes to an edge dislocation at the side of the crystal.
of steps up and down. Referring to Figure 2.38A, the extra halfplane of lattice points in the edge dislocation causes the Burgers circuit to be open. The vector that points from the end of the Burgers circuit to its beginning is shown here as the Burgers vector, b. The vector always points from one lattice point to another; it always has the same length and direction for a given dislocation, regardless where the circuit starts. For an edge dislocation, b is always perpendicular to the dislocation line. If b is parallel to the dislocation line, the dislocation is a screw dislocation. If b is neither perpendicular nor parallel to the line, a mixed dislocation is involved. Plastic deformation of a material refers to irreversible deformation or change in shape that remains
even when the force or stress causing it is removed, whereas elastic deformation is deformation that is fully recovered when the stress causing it is removed. Before the discovery of dislocations, materials scientists faced a big theoretical problem; they calculated that plastic deformation of a perfect crystal should require stresses 100 to 1000 times higher than those observed in tensile tests! So the problem was to explain why metals yielded so easily to plastic deformation. How they got these very large theoretical numbers can be understood from Figure 2.39. Planes of atoms in a crystal slip with respect to each other, in contrast to flow in a fluid, where the solid remains crystalline. The theoretical maximal shear stress or yield strength (failure), τmax, needed
Crystallography
A
TABLE 2.6 Theoretical Yield Strengths (Shear and Tensile) of Some Important Materials
d
Shear Strength (GPa)
Material B
Metallic Cu NaCl Quartz Diamond
C
M B
C
A d/2
d x
FIGURE 2.39 Calculation of the theoretical shear stress in a crystal.
to produce slip in an ideal crystal is calculated from the type and strength of the bonds involved, the spacing of the crystal, d, and the crystal symmetry. In yield, atoms slide tangentially from one equilibrium position to another. Thus, the shear stress, τ, is a periodic function: T T max
2P x sin d
65
Tensile Strength (GPa)
1.2 2.84 4.4 121
3.9 0.43 16 205
Calculated values for μ are in the range of 1–150 GPa (see also Table 2.6). But when the experiment is carried out, permanent deformation takes place by a stress as low as 0.5 MPa! The reason is that real materials have lots of dislocations, from 102/cm2 in the best Ge and Si crystals to 1012/cm2 in heavily deformed metals. Therefore, the strength of the material depends on the force required to make dislocations move, not the bonding energy between all atoms in two planes as calculated above. Dislocations can move if the atoms from surrounding planes break their bonds and rebond with the atoms at the terminating edge as shown in Figure 2.41. Instead of all the atoms in Shear stress b
(2.60)
where x is the direction of the shear. With x small this may be rewritten as: 2Px d T 2P T x Gd d < T T max d M d M M T max 2P T T max
(2.61)
(a)
(b)
(c)
(d)
where we have used γ = τ/μ (Hooke’s law) as the shear strain, with μ as the shear modulus (see Figure 2.40). Hooke’s law: = x d
FIGURE 2.40 Shear stress, τ; shear strain, γ; and shear modulus, μ. The shear stress τ produces a displacement Δx of the upper plane as indicated; the shear strain, γ, with Δx/d = tan α is defined γ = τ/μ.
FIGURE 2.41 Dislocation movement: When a shear stress is applied to the dislocation in (a), the atoms are displaced, causing the dislocation to move one Burgers vector b in the slip direction (b). Continued movement of the dislocation eventually creates a step (c), and the crystal is deformed. (d) The caterpillar does not move its complete body at a single time, but it moves one segment at a time as it pulls itself forward.
66
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
(a)
(b)
FIGURE 2.42 Moving a carpet over the floor to illustrate the effect of a line dislocation in a crystal: (a) dislocation; (b) work hardening.
a plane breaking at the same time, atoms are gliding gently in the direction of applied stress normal to dislocation lines. Thus, the direction of movement, i.e., the deformation, is the same as the Burgers vector, b. As a consequence b is also called the slip vector. The interatomic forces in a crystal offer little resistance to the gliding motion of dislocations. An analogy is that of moving a carpet across the floor. This is difficult because of the friction developed from the contact of the whole surface of the carpet with the floor. But with a wrinkle in the carpet, as shown in Figure 2.42, the carpet can now be moved by pushing the wrinkle across the floor. The work involved is much less because only the friction between a small section of carpet and the floor has to be overcome. A similar phenomenon occurs when one plane of atoms moves past another by means of a dislocation defect. Figure 2.43 shows how an applied shear stress, τ, exerts a force on a dislocation and is resisted by a frictional force, F, per unit length. The work done by the shear stress (Wτ) equals the work done by the frictional force (WF), or:
b
F
b l2
l1
FIGURE 2.43 An applied shear stress, τ, exerts a force on a dislocation and is resisted by a frictional force, F, per unit length. The slip vector or Burgers vector is b. (Drawing by Mr. Chengwu Deng.)
WT (T l1l 2 ) s b (2.62)
and WF (F l1 ) s l 2
With Wτ = WF, the lattice friction stress for dislocation motion is: T
F b
(2.63)
where F is the force per unit length of the dislocation and b is its Burgers vector or slip vector. Thus, the applied stress produces a force per unit length everywhere along the dislocation line equal to τb and perpendicular to the line element. It can be shown that: 2 Pa F T Me b b
(2.64)
This lattice friction stress is much less than the theoretical shear strength. Dislocation motion, from Equation 2.64, is most likely on closed packed planes (large a, interplanar spacing) in closed packed directions (small b, inplane atomic spacing). It is thus easiest to create dislocations in the closest packed crystals, and they are typically very soft and ductile. When dislocations move it is said that slip occurred, and the lattice planes that slipped are called—imaginatively—slip planes as elucidated in Figure 2.44 for an edge dislocation and a screw dislocation. As mentioned above, the preferred slip planes are those with the greatest interplanar distance, e.g., (111) in FCC crystals, and the slip directions are those with the lowest resistance, i.e., the closest packed direction. Slip lines are the intersection of a slip plane with a free surface. The motion of dislocations can be blocked by another dislocation, a grain boundary, or a point
Crystallography Dislocation line
67
Dislocation line Slip line F
Slip vector
Slip vector
Slip line Slip plane
Slip plane
(a)
(b)
FIGURE 2.44 Schematic of slip line, slip plane, and slip (Burgers) vector for (a) an edge dislocation and (b) for a screw dislocation. (Drawing by Mr. Chengwu Deng.)
defect. Two dislocations may repel or attract each other, depending on their directions. Atoms near the core of a dislocation have a higher energy because of distortion. To minimize this energy, dislocations tend to shorten as if the line had a line tension, T, i.e., strain energy per unit length. The line tension is given as: Tz
1 2 Mb 2
(2.65)
Dislocations might get pinned by interstitials and bow with a radius R when subjected to a shear stress like the string shown in Figure 2.45: TbL 2 T sin
Q 2
(2.66)
With Equation 2.65 this leads to: R
Mb 2T
(2.67)
Plastic deformation (or yielding) occurs by sliding (or slip) of parallel lattice planes past each other. Pure metals have low resistance to dislocation motion, thus they exhibit low yield strength. Adding impurities in solution strengthening may increase the yield strength. A wellknown example is alloying Zn and Cu to form brass with a strength increase of up to 10 times over pure Cu. The bigger Zn atoms make the slip plane “rougher,” thus increasing the resistance to motion. In general, impurities diffuse to dislocations and form “clouds” that pin dislocations, increasing the elastic limit. Small particles, precipitates, can also promote strengthening by impeding dislocation motion. Precipitates cause bowing of dislocations as illustrated in Figure 2.45. A critical condition is reached when the dislocation takes on
a semicircular configuration between two particles separated by a distance L. Beyond this point a dislocation may loop and escape between the finely dispersed particles in the metal. In the semicircular situation τbL = 2T or τ = 2T/bL, and with Equation 2.67 τ = μb/L; thus, making L smaller will disadvantage dislocation looping. Finally, metals can be hardened by work hardening. Dislocations move when metals are subjected to “cold work,” and their density can increase up to 1012 dislocations/cm2 because of the formation of new dislocations and dislocation multiplication (see below). The consequent increasing overlap between the strain fields of adjacent dislocations gradually increases the resistance to further dislocation motion. This causes a hardening of the metal as the deformation progresses (Figure 2.42b). This effect is known as strain hardening. The effect of strain hardening can be removed by appropriate heat treatment (annealing), which promotes the recovery and subsequent recrystallization of the material. Annealing decreases the dislocation density to around 106 dislocations/cm2. Some dislocations form during the process of crystallization, but more are created during plastic deformation. Frank and Read elucidated one possible mechanism by which dislocations multiply; bL /2
/2 L
T
T R
R
FIGURE 2.45 A pinned dislocation bows under a shear stress.
68
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
(a)
(b)
(c)
(d)
g=011
slip system begins when the shear stress resolved on that system reaches a critical value. Consider a cylindrical crystal of crosssection A0 under the influence of a tensile force F. Let the normal to the active slip plane make an angle α with F, and let the angle between the slip direction and F be β. The resolved shearing force, i.e., the force acting per unit area of the slip plane in the slip direction, is then given by: T
0.25μ
F cos A cos B A
(2.68)
(e)
FIGURE 2.46 A FrankRead source can generate dislocations. (a) A dislocation is pinned at its ends by lattice defects. (b) As the dislocation continues to move, the dislocation bows, eventually bending back on itself. (c) Finally the dislocation loop forms, and (d) a new dislocation is created. (e) Electron micrograph of a FrankRead source (×330,000).
they found that a pinned dislocation (as shown in Figure 2.45), under an applied stress, produces additional dislocations. This mechanism is at least partly responsible for strain hardening. The FrankRead dislocation multiplication mechanism is illustrated in Figure 2.46. First, a dislocation is pinned at its ends by lattice defects, and as the dislocation continues to move, it bows and eventually bends back on itself. Then the dislocation loop forms, and a new dislocation is created. Figure 2.46 also shows an electron micrograph of a FrankRead source. Schmid’s Law, illustrated in Figure 2.47, gives the relationship between shear stress, the applied stress, and the orientation of the slip system. Slip on a given F
Normal to the slip plane
Because the area of the slip plane is A/cosα, the tensile stress per unit area normal to the slip plane is: S
F cos 2A A
(2.69)
When increasing the force F, the rate of plastic flow increases very rapidly when the resolved shear stress τ reaches a critical value τc. In general τc decreases with increasing temperature and increases as a result of alloying or cold working (see above). Besides point and line defects there are also surface defects to reckon with in single crystals. Surface defects include grain boundaries, phase boundaries, and free surfaces. The crystal structure is disturbed at grain boundaries, and different crystal orientations are present in different grains (Figure 2.48). Dislocations are blocked by grain boundaries, so slip is blocked. The smaller the grain size, the larger the surface of the grain boundaries and the larger the elastic limit. The latter is expressed in the empirical HallPetch equation for the maximum elastic yield strength (stress at which the material permanently deforms) of a polycrystalline material:
A0
S Y S0
Slip direction
FIGURE 2.47 Geometry of slip plane, slip direction, and tensile force F. (Drawing by Mr. Chengwu Deng.)
K d
(2.70)
where d is the average diameter of the grains in micrometers, with σ0 the frictionless stress (N/m2) that opposes dislocation, and K a constant. The strength of a material thus depends on grain size. In a small grain, a dislocation gets to the boundary and stops, i.e., slip stops. In a large grain, the dislocation can travel farther. So small grain size equates to more strength. For example, the elastic limit of copper doubles when the grain size falls from 100 μm
69
Crystallography
Grain boundary
(a)
100μm (b)
FIGURE 2.48 Crystal structure is disturbed at grain boundaries. Schematic representation of grain boundaries (a) and microscope picture (b). (From Askeland D. R., and P. P. Phule, The science and engineering of materials, Brooks/Cole, Pacific Grove, CA, 2003.)
to 25 μm. Instead of yield strength one might also plot the hardness (H) of the material as a function of grain size, and a similar relationship is obtained (see Volume II, Figure 7.54): smaller grain size corresponds to a harder material. Indentation (hardness) testing is very common for bulk materials where the direct relationship between bulk hardness and yield strength is well known. As we will learn in Volume II, Chapter 7, in the section on thin film properties, the HallPetch relationship has been well established for grain sizes in the millimeter through submicrometer regimes but is less wellknown in the nano regime. Based on Equation 2.70 one expects that nanosized grains would produce materials with yet greater mechanical integrity, but in reality this is not the case! There is a reverse HallPetch effect, i.e., the strength of materials, from a small grain size on, starts to decrease with decreasing grain size. Plastic deformation occurs at lower and lower stresses as the grains shrink. In other words,
an optimal grain size (dc) exists as suggested by the plot in Volume II, Figure 7.54. The classic HallPetch relationship is based on the idea that grain boundaries act as obstacles to dislocation movement, and because dislocations are carriers of plastic deformation, this manifests itself macroscopically as an increase in material strength. The HallPetch behavior breaks down when the smallest dislocation loop no longer fits inside a grain. Lattice dislocation cannot be the way very smallgrained materials deform. The deformation mechanism for materials with very small grains ( 1/τ, i.e., at very high frequencies
Quantum Mechanics and the Band Theory of Solids
(optical frequencies we will see), where the electrons cannot follow the fast changing electrical field anymore.
J(W)
¨ e 2n · © ¸ E(W) ª me ¹ S(W)E(W) (3.29) 1
iW T
enp(W) me
1. With ω > 1/τ: ¨ eE(W) · p(W , t) © ¸ (W sin Wt iW cos Wt) 2 ª W ¹
¨ eE(W ,t)i · ¨ eE(W)iW · iwt e © © ¸ ¸ 2 ª W ¹ ª W ¹ eE(W ,t) iW
(3.30)
Sa
S0 (Re) 1 W 2T2
(3.31)
S aa
S 0 WT (Im) 1 W 2 T2
(3.32)
and
¨ eE(W)iW · © ¸ (cos Wt isin Wt) 2 ª W ¹
S0 1 iWT
which simplifies to the DC conductivity, i.e., σ0 ne 2 T ( , Equation 3.7), in the case of very low ac me frequencies (ω 1. Under this approximation, we find: E ra (W,k) z 1
W 2p W2
(3.44)
and E raa(W ,k) z
(3.38)
Using Equation 3.36 for the polarization P, we can rewrite Equation 3.37 as: D E(W ,k) E E 0E P E 0E
a material to electromagnetic waves at various frequencies, one divides by ε0 because ε(ω,k)/ε0 = εr(ω,k). The corresponding real and imaginary components of the complex dielectric function are:
(3.37)
In the expression D E 0 E P we have separated the electric displacement D in its materials (P) and vacuum parts (ε0E). The permittivity of a material is usually given as a relative permittivity εr(ω) (also called the dielectric constant). The permittivity ε(ω,k) of a medium is an intensive parameter and is calculated by multiplying the relative permittivity by ε0, or ε(ω) = ε0εr(ω). The permittivity of air is εair = 8.876 pF/m, so the relative permittivity of air is εr,air = 1.0005, and for vacuum it is 1 by definition. From Equation 3.37, it then also follows that εr(ω) = 1 + χ e. The electric displacement field, D, is in turn related to the electric field E (in units of V/m) by the constitutive relation:
87
W 2p W 2p G W 3T W3
(3.45)
This approximation may break down in the farinfrared spectral region, where damping can be significant. Note that damping (γ) is absolutely necessary to have an imaginary part of Er (W). The dispersion of the real part of the dielectric function E ra (W ,k) (Equation 3.44) is plotted in Figure 3.13. The Drude model predicts a monotonous decrease of E ra (W ,k) for decreasing frequency, and experiments confirm ´r
¨ · ne 2 E(W , k) E 0 ©1 ¸ 2 me E 0 (W iGW) ¹ ª
1
¨ · W 2p E 0 ©1 2 ¸ (W iGW) ¸¹ ©ª
(3.40)
0 p
The plasma frequency ωp in Equation 3.40 is defined as: Wp
ne 2 me E 0
(3.41)
where n is the density of electrons in the metal. To obtain εr(ω), the relative dielectric response of
FIGURE 3.13 The dielectric function: ε´r as a function of ω. The dielectric constant ε´r becomes zero when ω = ωp, and this supports free longitudinal collective modes for which all electrons oscillate in phase.
88
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
that E ra (W , k) becomes zero when ω = ωp. When E ra (W) becomes zero at ω = ωp, the material can support free longitudinal collective modes for which all electrons oscillate in phase. Such a collective charge oscillation is called a plasmon. Note that in the limit of γ going to 0, Equation 3.40 leads to the same result as shown in Equation 3.44 (no imaginary component to the dielectric constant at γ = 0). We come back to the field of plasmonics in Chapter 5 on photonics, and at that point we will not only analyze plots of Er (W) for metals but also of n(ω) (refractive index), α(ω) (absorption), and R(ω) (reflectance) for all types of materials. With reference to Figure 3.12, we can derive the plasma frequency ωp in yet another way. Let us look at the case where ε′r(ω) = 0 at ω = ωp; because E ra (W) 1 Cea, this means that at this frequency, Cea z 1, and with the polarization, P(W ,t) Ce E 0 E(W ,t) P (Equation 3.36), this results in P(W ,t) z E 0 E(W , t). The displacement δx of the electron gas of density n creates an electric field E = −P/ε0 = neδx/ε0; this opposing field acts as the restoring force (Fr = −eE) on the electron gas. The equation of motion resulting from this restoring force Fr in such a simple electron gas oscillator is given as: u 2 (Dx) ne 2 Dx Fr eE me 2 2 E0 u t
(3.46)
This results in oscillations at the plasma frequency ne 2 of W p (Equation 3.41). me E 0 The plasma frequency ωp comes with a free space wavelength of: Lp
2Pc Wp
(3.47)
In Table 3.2 we compare the plasma frequency and the free space wavelength for a generic metal and a TABLE 3.2 Plasma Frequency (ωp) and Free Space Frequency (λp) for a Generic Semimetal and Semiconductor Property Electron density: n, cm−3 Plasma frequency: ωp, Hz Space frequency: λp, cm Spectral range
Metal
Semiconductor
1022 5.7 × 1015 3.3 × 10−5 UV
1018 5.7 × 1013 3.3 × 10−3 Infrared region
generic semiconductor. Using Equation 3.41 we can now calculate ωp for a variety of materials. For silver, for example, with a σ of 6.2 × 107 Ωm, one obtains ωp = 9.65 × 1014 Hz (= 311 nm or 4 eV). The lower the resistivity (higher n), the higher the plasma frequency. Consequently, plasma frequencies ωp are in the optical range (UV) for metals and in the THz to the infrared region for semiconductors and insulators. Metals reflect light in the visible region and are transparent at very high frequencies (UV and xrays). With a free space wavelength less than λp, a wave propagates; when it is longer, the wave is reflected (ω > ωp, or λ < λp). In a metal where both bound electrons [εB(ω)] and conduction electrons [εr(ω)] contribute an effective dielectric constant, εEff(ω) must be defined as: E Eff (W) E B (W) E r (W)
(3.48)
where εr(ω) is the complex dielectric constant at ωτ >> 1, given by (see Equations 3.44 and 3.45): E r (W) E ra (W) iE raa (W) 1
W 2p W2
i
W 2p W 3T
(3.49)
Plasma oscillations can be excited in dielectric films as well. A dielectric material is a nonconducting substance whose bound charges are polarized under the influence of an externally applied electric field. In this case, although qualitatively the same effect as in a metal, the oscillations of the bound electrons are with respect to the immobile ions instead of with respect to the films boundary, and a restoring force related to the strength of the bond of the electrons to those ions must be introduced. In Chapter 5 on photonics, after introducing the Maxwell equations, the Drude plasmon model will be upgraded with the more complete DrudeLorentz model that includes such a restoring force term. The restoring force pulls charges back in their equilibrium position. The DrudeLorentz model without the restoring force reduces back to the Drude model, in which conduction electrons are not bound to atoms. There we will also calculate the effective dielectric constant εEff(ω) (with bound and free electron contributions) of Equation 3.48.
Quantum Mechanics and the Band Theory of Solids
Specific Heat Capacity of Metal and Insulators Different materials require different amounts of heat to increase their temperature. Heat capacity per unit mass of a substance is known as specific heat, and as we will see, it is a measure of the number of degrees of freedom of the system. When using classical models, as in the case of electrical conductivity, things went wrong for calculations of the specific heat capacity of metals and insulators. Based on the Drude assumption that electrons in a metal behave as a monatomic gas of N classical particles, they should be able to take up translational kinetic energy when the metal is heated. According to the equipartition principle of energy in a gas with N particles, the electron internal energy U, at temperature T, expressed per mole is: U 3N 3 3 k B T = N A kT = RT n 2n 2 2
(3.50)
with n the number of moles in the system, NA Avogadro’s number, R the ideal gas constant, and kB Boltzmann’s constant. Remember also from thermodynamics that the first derivatives of the fundamental thermodynamic equations, in U (internal energy) or S (entropy), correspond to the intensive parameters T, P, and μ (chemical potential), whereas second derivatives correspond to important materials properties such as the molar heat capacity, or:
89
Atoms in a lattice usually have no translational energy, and as temperature increases only vibrational energy increases. In the case of a monovalent metal, the lattice specific heat contribution, Cv,lat, equals 3R. This follows from the fact that a classical atom oscillator has 3 degrees of freedom in vibration, or U = 3NkT. The vibration of a classical 1 1D harmonic oscillator is U = kT, with kT for 2 1 kinetic and kT for potential energy (Figure 3.14). 2 From the latter we expect Cv,lat to be constant at 3R or 25 J/(mol·k), the socalled DulongPetit law. Experimentally, Cv, the sum of vibrational and electronic contributions (C v = Cv,el + Cv,lat), is proportional to T 3 at low T and approaches a constant 3R at high T (see Figure 3.15). Diamond reaches the DulongPetit value 25 J/(mol·k) only at high temperature, whereas lead reaches the DulongPetit value at relatively low temperature. From the above, at high temperature, electrons are expected to contribute to the lattice heat capacity 9 for a total C v = Cv,el + Cv,lat or R, which is obviously 2 a different result from DulongPetit’s 3R! The total Cv for metals is found to be only slightly higher than that for insulators, which only feature lattice contributions. The question is then: where is the electronic contribution? The absence of a measurable contribution by electrons to the Cv was historically
¥ us ´ T ¥ uS ´ 1 ¥ uQ ´ Cv T ¦ µ ¦ µ ¦ n § uT ¶ v n § uT µ¶ v (3.51) § uT ¶ v This equation basically tells us that the molar heat capacity at constant volume is the quasistatic heat flux per mole required to produce a unit increase in the temperature for a system maintained at constant volume. Materials with high specific heat capacity (Cv) require more energy to reach a given temperature. In the case of a metal, one expects contributions to the heat capacity from both the lattice and the free electrons. The electronic contribution to the molar specific heat capacity at constant volume, Cv, from Equation 3.50, is: C v,el
D ¥ U´ 3 ¦§ µ¶ R DT n v 2
or about 12.5 J/(mol·k).
(3.52)
FIGURE 3.14 Cv: energy needed to raise T of 1 mol by 1 K at constant V, volume. The internal energy resides in vibrations of the solid constituents. The vibration of a classical 1D harmonic oscillator is U = kT. In a solid there are three perpendicular modes of vibration or three harmonic oscillators, and the total energy of a solid is thus U = 3N kT = 3RT.
90
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology DulongPetit value ~ 25 J/(mol·k) Lead
25
Aluminum
Classical theory
Cv Silicon
Cv J/(mol·k)
20
exp. Debye model
Diamond
Einstein model
15
Electronic he
10 0 5
0 0
200
400
600
800
1000
1200
at capacity
300 K
T
FIGURE 3.16 Schematic representation of the temperature dependence of the molar heat capacity, experimental and according to four models. For the Debye and Einstein models, see further below.
T (K)
FIGURE 3.15 DulongPetit law with Cv = 3R or 25 J/(mol·k) at high temperatures.
one of the major objections to the classical free electron model: because electrons are free to carry current, why would they not be free to absorb heat energy? Conduction electrons only contribute a small part of the heat capacity of metals, but, as we will see below, they are almost entirely responsible for the thermal conductivity. In the above model, we used the principle of equipartition of the energy, which we borrowed from classical ideal gas theory. But, as Planck discovered in 1901, a vibrating system can only take up energy in quanta, the size of which is proportional to the vibration energy such that E = hν, where ν is frequency and h is the Planck constant. The chance that an atom vibrator can pick up an energy hν is proportional to e−hν/kT, and the average energy of a vibrating atom, at low temperature, may fall so low that the value of kT is now small compared with the size of the quantum hν, and the probability factor e−hν/kT is dramatically decreased. Therefore, DulongPetit is incorrect at low temperatures as vibrations of successively lower frequencies fail to become excited. Atoms in a crystal do not obey Maxwellian statistics at low temperatures, and one needs to invoke the Einstein or Debye law instead. The reason that electrons do not contribute to the heat capacity at room temperature is, just like in the case of electrical
conductivity, that they are fermions and cannot be treated as an ordinary MaxwellBoltzmann gas. At room temperature, only the very few electrons in the socalled MaxwellBoltzmann tail of the Fermi distribution can contribute to the heat capacity. Thus, at ordinary temperatures the electronic heat capacity is almost negligible, and it is the atomic vibration, i.e., the contribution of phonons, that dominates. In Figure 3.16 we show the experimental molar heat capacity as a function of temperature and the expectations for those values from classical theory and from the Einstein and Debye models, which are discussed at the end of this chapter. It is seen here that the electronic contribution Cv,el varies linearly with temperature.
Thermal Conductivity Heat conduction is the transfer of thermal energy from a hot body to a cold body. In a solid both electrons and phonons can move, and depending on the material involved, one or the other tends to dominate. We intuitively expect electrical and thermal conductivities somehow to be linked; from experience we know that, in general, good electrical conductors are also good thermal conductors. The connection between electrical and thermal conductivities for metals was first expressed in the WiedemannFranz law in 1853, suggesting that electrons carry thermal energy and electrical charge. Insulators are often transparent, and conducting
10–2
10–1
100
101
91
Al Cu Ag
Si
Fe Ge
SiO2
NaCl
Water
Rubber Nylon
Wood
Sulphur
Quantum Mechanics and the Band Theory of Solids
102
103
W/(mol·k)
Phonon conductors Electron conductors
FIGURE 3.17 Phonon and electron conductors.
metals are reflecting and shiny when polished. Most metals are shiny because when light strikes a metal, the light is scattered by the moving electrons. For an exception, think about diamond, which is a transparent insulator but conducts heat better than aluminum or copper. For a glaring difference between heat and electrical conduction, consider that electrical conductivity of materials spans 25 orders of magnitude, whereas thermal conductivity only spans about four orders. In metals, heat is mostly transferred by electrons, but in electrical insulators, there are few free electrons, so the heat must be conducted in some other way, i.e., lattice vibrations or phonons. Thus, materials are divided into phonon conductors and electron conductors of heat as illustrated in Figure 3.17. There is a major difference between heat conduction by electrons and by phonons; for phonons, the number changes with the temperature, but the energy is quantized, whereas for electrons, the number is fixed, but the energy varies. We will analyze now in more detail what that relation between electronic conductivity, σ, and thermal conductivity, κ is, and will discover that, when using classical models, the experimental results again cannot be properly explained. Recall the electrical result J = σE (Equation 2.2) dV and also J = σE = σ . The thermal equivalent for dx this expression is Fourier’s law for heat conduction, Q, which states that: Q KA
Th Tc dT KA L dx
(3.53)
with Th the hot temperature and Tc the cold temperature, κ the thermal conductivity, L the thermal conduit pathlength, and A its crosssectional area. From the first law of thermodynamics (heat conservation),
we know that the rate of heat conduction must equal the rate of change of energy storage: K
uT u2 T C v.el 2 ut ux
(3.54)
The specific heat capacity, in general, is made up of a phonon and an electron term (Cv = Cv,el + Cv,lat). In most metals, the contribution of the electrons to heat conductivity greatly exceeds that of the phonons, and the phonon term can be neglected (Cv = Cv,el). Because of electrical neutrality, equal numbers of electrons move from hot to cold as the reverse, but their thermal energies are different. Equations 3.53 and 3.54 only apply under the conditions that: t >> scattering mean free time of the energy carriers (τ) L >> scattering mean free path of the energy carriers (λ) These conditions break down for applications involving thermal transport in small length/time scales, e.g., nanoelectronics, nanostructures, NEMS, ultrafast laser processing, etc. (see below and Volume III, Chapter 7 on scaling). For now, however, we are interested in the relation between electronic conductivity, σ, and thermal conductivity, κ, for somewhat larger systems. To arrive at the expression for thermal conductivity, κ, we inspect Figure 3.18 and consider a metal bar [area A is a unit area (A = 1) here] with a temperature gradient dT/dx where we are interested in a small volume of material, with a length 2λ, with λ the mean free path between collisions. The idea is that an electron must have undergone a collision in this space and hence will have the energy/temperature of this location. To calculate the energy
92
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
E1
E2
Unit area
x x1
x0
x2
FIGURE 3.18 Fourier’s Law for heat conduction: we are interested in a small volume of material, with a length 2λ, where λ is the mean free path between collisions with the lattice.
flowing per unit time per unit area from left to right (E1), we multiply the number of electrons N crossing by the energy of one electron: energy
¥ dT ´ · 1 1 ¨ kT1 k © T0 L ¦ ¸ 2 2 ª § dx µ¶ ¹
number
1 nv dx 6
(3.55)
1 1 2 C v,el v dx L or also C v,el v dx T sine L v dx T (3.59) 3 3
As mentioned above, in most metals the conduction by electrons greatly exceeds that of the phonons; typically the phonon contribution at room temperature is only 1% of the electron contribution. In 1853, long before Drude’s time, Gustav Wiedemann and Rudolf Franz published a paper claiming that the ratio of thermal and electrical conductivities of all metals has almost the same value at a given temperature: 2
with vdx the drift velocity in the xdirection, and dT/dx a thermal gradient in the xdirection. We know that for charge neutrality the same number of electrons must flow in the opposite direction to maintain charge neutrality, but their energy per electron is lower. Based on: nv dx 1 ¥ dT ´ k ¦ T0 L µ 2 2 § dx ¶
(3.56)
the thermal energy transferred per unit time per unit area is: Q E1 E 2
nv dx dT kL 2 dx
(3.57)
Comparing this result with Equation 3.53 (with A = 1), we obtain: K
K
C mv 2 3¥k ´ K v,el 2 dx ¦ B µ T 2§ e ¶ S 3ne
nv dx 1 ¥ dT ´ E1 k ¦ T0 L 2 2 § dx µ¶
E2
This says that the thermal conductivity is larger if there are more electrons (n large), the electrons move faster (vdx large), and they move more easily (large λ with fewer collisions). Because NA k = R with R the ideal gas constant, N/NA = n (number of moles of electrons), and the electronic contribution to the molar specific heat capacity at constant volume, Cv,el, from Equation 3.52 is 3/2R. The bulk heat conductivity of a solid per mole (n = 1) can then be rewritten as:
1 nv dx kL 2
(3.58)
(3.60)
calculated through Drude’s application of classical 3 1 3 2 gas law: C v,el nk B and mv dx k B T . Ludwig 2 2 2 Lorenz realized in 1872 that this ratio scaled linearly with temperature, and thus a Lorenz number, L, was defined as: K y L ST
(3.61)
which is very nearly constant for all metals (at room temperature and above). A typical value for L, say for Ag, is 2.31 10 −8 WΩK−2 at 0°C and 2.37 10−8 WΩK−2 at 100°C (see Table 3.3). Although Equation 3.61 is the correct relationship, we now know that the value for L calculated from it is wrong. However, Drude, using classical values for the electron velocity vdx and heat capacity Cv,el, somehow got a number very close to the experimental value. But how lucky that Drude dude was: by a tremendous coincidence, the error in each term he made was about two orders of magnitude … in the opposite direction [the electronic Cv,el
93
Quantum Mechanics and the Band Theory of Solids
TABLE 3.3 Some Typical Lorenz Numbers −8
Lorentz force F = –qv × B
2
Lorenz Number L in 10 WΩK Metal Ag Au Cd Cu Ir Mo Pb Pt Sn W Zn
273 K 2.31 2.35 2.42 2.23 2.49 2.61 2.47 2.51 2.52 3.04 2.31
B
373 K 2.37 2.40 2.43 2.33 2.49 2.79 2.56 2.60 2.49 3.20 2.33
B F
y x
V=0
e
I
d
w
V = VH
(3.62)
But in Drude’s original paper, he inserted also an erroneous factor of two, as a result of a mistake in the calculation of the electrical conductivity. So he originally reported: L 2.24 s 10 8 W7K 2
z
v
is 100 times smaller than the classical prediction, but (vdx)2 is 100 times larger]. So the classical Drude model gives the prediction: L Drude 1.12 10 8 W7K 2
Coordinate system
(3.63)
The correct value for the Lorenz number, L, derived P 2 kB2 from quantum mechanics is or 2.45 × 10−8 3e 2 WΩK 2 (see Equation 3.340 below). So although Drude’s predicted electronic heat capacity was far too high (by a factor of 100!), his prediction of L made the free electron gas (FEG) model seem more impressive than it really was and led to a general acceptance of the model.
Hall Coefficients Conductivity measurements do not yield information about the sign of charge carriers; for this we need the Hall effect. The Hall effect uses current and a magnetic field to determine mobility and the sign of charge carriers. The Hall effect, discovered in 1879 by American physics graduate student (!) Edwin Hall, is simple to understand.1 With reference to Figure 3.19, consider a fairly strong magnetic field B (~2000 Gauss) applied perpendicular to a thin metal film (thickness is d and width is w) carrying a current I. The magnetic Lorentz force is
FIGURE 3.19 The Hall effect. Magnetic field B is applied perpendicular to a thin metal film sample carrying current I. VH is the Hall voltage.
normal to both the direction of the electron motion and the magnetic field. The path of the charge carriers shifts as a result of this Lorentz* force, and, as a consequence, the Hall voltage, V H = E y w (where E y is the Hall field strength), builds up until it prevents any further transverse displacement of electrons. In other words, the Hall field increases until it is equal to and opposite of the Lorentz force. The orientation of the fields and sample is illustrated in Figure 3.19. In mathematical terms, the above translates as follows. With both electric and magnetic fields present, a charge carrier with charge q experiences a Lorentz force in the lateral direction: FL q(v d s B z )
(3.64)
We do use the drift velocity vd of the carriers because the other velocities (and the forces caused by these components) cancel to zero on average. Note that instead of the usual term “electron,” the term “charge carrier” is used here because in principle an electrical current could also be carried by charged particles other than electrons, e.g., positively charged ions or holes (missing electrons). The vector product in Equation 3.64 ensures that the Lorentz force is perpendicular to vd and B z. For the geometry assumed in Figure 3.19, the Lorentz force FL has only a component in the ydirection, and we can use a *
This is the Lorentz we encounter again in Chapter 5 (Figure 5.50), not the Lorenz from the Lorenz number L.
94
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
scalar equation for the Lorentz force: F L = –qvdB z or with Equation 3.11 (where we replaced μe by μq for generality): FL = −qμqE x B z
RH
(3.65)
As more and more carriers are deflected by the magnetic force, they accumulate on one side of the thinfilm conductor, and this accumulation of charge carriers leads to the “Hall field” Ey that imparts a force opposite to the Lorentz force. The force from that electrical field Ey in the ydirection (which is of course q·Ey) must be equal to the Lorentz force with opposite signs. This way we obtain: FL qM q E x B z qE y or (3.66)
FL M q E x B z E y
The Hall voltage VH now is simply the field in ydirection multiplied by the dimension w in the ydirection (=wE y). It is clear then that the (easily measured) Hall voltage is a direct measure of the mobility μ of the carriers involved, and that its sign or polarity will change if the sign of the charges changes. It is customary to define a Hall coefficient, RH, for a given material as: RH y
Using Equations 3.10, 3.66, and 3.67, as well as Jx = σE x , we calculate RH as:
Ey J xBz
(3.67)
In other words, we expect that the Hall voltage, wEy, will be proportional to the current density Jx and the magnetic field strength B, which are, after all, the main experimental parameters (besides the trivial dimensions of the specimen): (3.68)
E y R HB z J x
(3.69)
When we calculate RH from our measurements and assume q = e (which Hall at the time did not know!), we can find n, the charge density. Also, the sign of VH and thus of RH tells us the sign of q! If RH is negative, the predominant carriers are electrons; if positive, they are holes. If both types of carriers are present, the Hall field will change its polarity depending on the majority carrier (Figure 3.20). Also from Equation 3.69 one sees that the lower the carrier density, the higher RH and thus the higher VH; this is a key to some very sensitive magnetic field sensors. For most metals the Hall constant is negative because electrons are majority carriers. But for Be and Zn, for example, there is a band overlap with dominant conduction by holes in the first band and fewer electrons in the second. As a result, RH is positive for these metals. Of course energy bands were not heard of yet, and the results of a positive RH were baffling at the time: how can we have q > 0 (even for metals!)? The Hall coefficient changes sign with the sign of the charge carrier and therefore provides an important method for investigating the electronic structure of the solid state. In particular, the positive Hall coefficients exhibited by metals such as magnesium and aluminum are a clear indication that a naive picture of a sea of conduction electrons is inappropriate because the majority carriers are clearly positively charged (and are, in fact, holes). The discrepancies between the FEG predictions and experiments nearly vanish when liquid metals are compared (see Table 3.4). This
B
B c
I
qvd × B vd
M q E x B z 1 M M qn S E xBz S qnM
qEH a (a)
c I
I ΔVH 0
qvd × B
I vd
qEH a
ΔVH 0
(b)
FIGURE 3.20 Electron and hole charge carriers in the Hall effect. When the charge carriers are negative, the upper edge of the conductor becomes negatively charged (a). When the charge carriers are positive, the upper edge becomes positively charged (b).
Quantum Mechanics and the Band Theory of Solids
95
TABLE 3.4 Discrepancies between the FEG Predictions for RH and Experiments Nearly Vanish When Liquid Metals Are Compared* RH (10−11 m3/As) n0
Solid
Liquid
FEG Value
Na Cu Ag Au Be Zn Al
1 1 1 1 2 2 2
−25 −5.5 −9.0 −7.2 +24.4 +3.3 −3.5
−25.5 −8.25 −12.0 −11.8 −2.6 −5 −3.9
−25.5 −8.25 −12.0 −11.8 −2.53 −5.1 −3.9
*This reveals clearly that the source of these discrepancies lies in the electronlattice interaction. Notice positive RH for Be and Zn.
reveals clearly that the source of these discrepancies lies in the electronlattice interaction of a solid. The Hall effect “oddities” will be properly explained once we have introduced quantum physics. We will also see that under special conditions of extremely low temperature, high magnetic field, and twodimensional electronic systems (2D electron gas, in which the electrons are confined to move in planes), the Hall resistance RH is quantized and increases as a series of steps with increasing magnetic field. These discrete energy levels are called Landau levels.
Blackbody Radiation Planck first discovered the discontinuous behavior that characterizes the atomic world in his analysis of the light spectra emitted from blackbodies in 1900. All substances, with thermal energy, radiate EM waves, and the radiation emanating from solids consists of a continuous spectrum of wavelengths. A blackbody (also cavity radiation) is a hypothetical object that is a perfect absorber or perfect emitter of radiation (Figure 3.21). “Blackbody” is an unfortunate name as the ideal radiating/absorbing body does not have to be black; stars and planets, to a rough approximation, are blackbodies! When a blackbody is heated, it first feels warm and then glows red or white hot, depending on the temperature. A typical spectrum of the radiated light intensity, brightness, or emittance of a blackbody is shown in Figure 3.22. Intensity is a measure of how much energy is emitted from an object per unit surface area per unit time at a given wavelength
FIGURE 3.21 Ideal blackbody (also cavity radiation). “Blackbody radiation” or “cavity radiation” refers to an object or system that absorbs all radiation incident on it and reradiates energy that is characteristic of this radiating system only, not dependent on the type of radiation that is incident on it. The radiated energy can be considered to be produced by standing wave or resonant modes of the cavity, which is radiating.
and in a particular direction. A blackbody of temperature T emits a continuous spectrum peaking at λmax. At very short and very long wavelengths there is little light intensity, with most energy radiated in some middle range frequencies. As the body gets hotter, the peak of the spectrum shifts toward shorter wavelengths (higher frequencies), but there is always a cutoff at very high frequencies. It was experimentally observed that the brightness peak position shifted with temperature as: TL max constant 2.898 s 10 3 mK (3.70) This is known as the Wien displacement law (see Figure 3.22). It was also known that the total energy, E, could be represented as the StefanBoltzmann law: E ST 4
(3.71) where the constant σ = 5.6704 × 10 W/m2·K4. Classical interpretation predicted something –8
5 × 1014
Emittance (W/m–3)
Metal
Wien’s law maxT = const
4 × 1014 8000 K
3 × 1014
7000 K 2 × 1014 6000 K
1 × 1014
5000 K 0
0
200
400 600 Wavelength (nm)
800
1000
FIGURE 3.22 Blackbody radiation spectra at four different temperatures.
96
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Toward the “ultraviolet catastrophe” 82
an tum Qu
ical
Planck Law
Class
Radiated intensity
c3
RayleighJeans Law kT
82 Curves agree at very low frequenices
c3
h h
e kT – 1
Frequency
FIGURE 3.23 Planck and RayleighJeans models for blackbody radiation.
altogether different; in the classical RayleighJeans model, instead of a peak in the blackbody radiation and a falling away to zero at zero wavelength, the measurements were predicted to go off scale at the short wavelength end as shown in Figure 3.23. Here is how the British physicists Lord Rayleigh and Jeans derived their model. They interpreted the blackbody radiation coming from a solid as electromagnetic radiation from oscillators that vibrate at every possible wavelength λ. In Figure 3.23 the radiated intensity, E(λ), in Js −1 m−3, is the energy distribution, i.e., the energy, E, at each λ. At equilibrium, the mean energy of all oscillators at temperature T is kT. The energy Eλ in a small interval dλ is then given by: E λ dλ = kTdn
(3.72)
where dn is the fraction of oscillators at the “average energy” in the dλ interval. From the Maxwell equations (see Chapter 5) one derives: dn 8P 4 dL L
(3.73)
Substituting this relation in Equation 3.72 leads to: ¨ 8P · E L dL kT © 4 ¸ dL ªL ¹ or also since ν = c/λ ¨ 8PN2 · E L dL kT © 3 ¸ dN ª c ¹
¨ 8PN2 · The term in brackets © 3 ¸ is the number of modes ª c ¹ per unit frequency per unit volume. The amount of radiation emitted in a given frequency range should be proportional to the number of modes in that range. The best of classical physics suggested that all modes had an equal chance of being produced, and that the number of modes increased proportionally to the square of the frequency. Equation 3.74 works at long wavelengths (see Figure 3.23) but fails at short wavelengths. This failure at short wavelengths is called the ultraviolet catastrophe; as λ decreases, Eλ goes to +∞. Even at very low T, the exponential curves in Figure 3.23 would have a huge value for visible light. Objects would be visible in the dark. The predicted continual increase in radiated energy with frequency (dubbed the “ultraviolet catastrophe”) did not happen. Nature knew better. The UV catastrophe attracted the attention of many physicists at the end of the nineteenth century, including Max Planck. Planck took the revolutionary step that led to quantum mechanics. He concluded that the available amount of energy could only be divided into a finite number of pieces among the atom oscillators in the cavity walls, and the energy of such a piece of radiation must be related to its frequency according to a new extremely important equation: E = hν
(3.75)
where h was a new constant now called the Planck constant. The quantization implies that a photon of blue light of given frequency or wavelength will always have the same size quantum of energy. For example, a photon of blue light of wavelength 450 nm will always have 2.76 eV of energy. It occurs in quantized chunks of 2.76 eV, and you cannot have half a photon of blue light—it always occurs in precisely the samesized energy chunks. Planck showed that the intensity I of radiation from a blackbody could be described by the function (now known as the Planck function):
(3.74) I(L ,T)
2hc 2 L5
1 (e
1 LkT
(3.76)
1)
Quantum Mechanics and the Band Theory of Solids
This Planck function was initially found empirically by trial and error but later derived by assuming the Planck constant and a Boltzmann distribution. Differentiating the Planck function with respect to wavelength one derives Wien’s displacement law— the wavelength of the maximum: L max
hc 4.965kT
Incident light Collector e– Emitter Vacuum tube
I
A
(3.77)
97
Ammeter
Power supply (Voltage V)
The constant hc/4.965kT agrees with the 2.898 × 10–3 m·K experimental value from Equation 3.70. Integration of the Planck function with respect to wavelength over all possible directions results in the total energy emitted per unit area per unit time from the surface of a blackbody (or absorbed per unit area per unit time by a body in a blackbody radiation field). This gives us back the StefanBoltzmann law (Equation 3.71): d
E ° E L ( T) 0
2P k 4 4 T ST 4 15c 2 h3
(3.78)
which also enables us to verify that the constant σ is indeed 5.6704 × 10 −8 W/m2·K4. Planck, interestingly, never appreciated how far removed from classical physics his work really was. He spent most of his life trying to reconcile the new ideas with classical thermodynamics. The Planck constant h was a bit like an “uninvited guest” at a dinner table; no one was comfortable with this new guest. But today we know that discontinuities in the nanoworld are meted out in units based on this Planck constant. This constant and its particular magnitude constitute one of the great mysteries in nature. It is the underlying reason for the perceived weirdness of the nanoworld, the existence of a “least thing that can happen” quantity—a quantum. The ubiquitous occurrence of discontinuities in the nanoworld constantly upsets our commonsense understanding of the apparent continuity of the macroscopic world.
Light as a Stream of Particles Photoelectric Effect The photoelectric effect, discovered by chance, by Heinrich Hertz and his student Hallwachs in 1888,
FIGURE 3.24 Experimental setup for studying the photoelectric effect.
is a process whereby light falling on negatively charged Zn, in an evacuated vessel, knocks electrons out of the surface as illustrated in Figure 3.24. The details of the photoelectric effect were in direct contradiction to the expectations of very welldeveloped classical physics of light waves, and the correct explanation by Einstein in 1905 marked one of the major steps toward quantum theory. Classical light wave theory predicts that the electrons in the metal will absorb radiation energy continuously. Once an electron has absorbed energy in excess of its binding energy, it will be ejected, and one would expect that a higher intensity would increase the chance that electrons are ejected. As illustrated in Figure 3.24, to test this model we introduce a metal collector plate that collects electrons and a circuit that may be closed to measure the current I. In this setup, a retarding or stopping potential, V0, may be applied to determine the kinetic energy of the electrons (eV0 = 1/2 mv2). The classical wave model implies that the stopping voltage V0 must be proportional to the intensity. Increasing frequency ν should not matter much, perhaps only causing a small decrease in current I, as a result of the rapid wave oscillations at high frequencies. With low intensity light, there should be a time delay to build up enough energy before current starts to flow. The results were unexpected; no electrons were ejected, regardless of the intensity of the light, unless the frequency exceeded a certain threshold characteristic of the bombarded metal (red light did not cause the ejection of electrons, no matter what the intensity). The electrons were emitted
98
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
immediately—no time lag. Increasing the intensity of the light increased the number of photoelectrons but not their maximum kinetic energy (a weak violet light would eject only a few electrons, but their maximum kinetic energies were greater than those for intense light of longer wavelengths). The kinetic energy of the ejected electrons varied linearly with the frequency of the incident radiation but was independent of the intensity, or: eV0( = kinetic energy of the electrons) = hν − Φ (3.79) where Φ, the photoelectric work function, is the energy lost by a surface when an electron is freeing itself from its environment. This cannot be explained by the Maxwell equations. If the charge of the electron is known, a plot of retarding or stopping voltage versus frequency of incident light, shown for three different metals in Figure 3.25, may yield a value for the Planck constant h. The electron charge was determined by Robert Millikan in 1909, and with that value and the slope of the lines in Figure 3.25, a value for h of 6.626 × 10−34 J∙s was calculated, identical to the one derived from the hydrogen atom spectrum and blackbody radiation (see above). The intercept with the frequency axis (at kinetic energy zero) is the threshold frequency, ν0, and the stop or retarding voltage axis intercept is the binding energy (–Φ) of the electron. The photoelectric phenomenon could not be understood without the concept of a light particle, eV0
Cs Li
i.e., a quantum amount of light energy for a particular frequency. Einstein’s paper explaining the photoelectric effect was one of the earliest applications of quantum theory and a major step in its establishment. The remarkable fact that the ejection energy was independent of the total energy of illumination showed that the interaction must be like that of a particle that gave all of its energy to the electron! This fit in well with Planck’s hypothesis that light in the blackbody radiation experiment could exist only in discrete bundles with energy. In quantum theory, the frequency, ν, of the light determines the energy, E, of the photons and E = hν, where h is Planck’s constant (h = 6.626069 × 10 −34 J·s) (Figure 3.26). This assumption explains quantitatively all the observations associated with the photoelectric effects. A photon hits an electron and is absorbed. The energy of the emitted electron is given by the energy of the photon minus the energy needed to release the electron from the surface. This explains the observance of a threshold value below which no electrons are emitted. Thus, it depends on the frequency of light falling on the surface but not on its intensity. It also explains why there is no time lag; a photon hits an electron, is absorbed by the electron, and the electron leaves. Higher intensity light contains more photons, and so it will knock out more electrons. However, if the frequency of the light is such that a single photon is not energetic enough to release an electron from the surface, then none will be ejected no matter how intense the light. Gilbert N. Lewis in 1926 called Einstein’s light particles photons. Just as the word photon highlights the particle aspect of an electron, the word graviton emphasizes
Ag
Retarding potential
Packet with energy E = h
Slope = h
0 Light frequency
Intercept = –
FIGURE 3.25 A plot of retarding or stopping voltage versus frequency of incident light. Slope is the Planck constant h. The intercept with the frequency axis (at kinetic energy zero) is the threshold frequency, ν0, and the stop voltage axis intercept is the binding energy.
c
FIGURE 3.26 Light as energy packets with an energy E = hν.
Quantum Mechanics and the Band Theory of Solids
the particle aspect of gravity, and gluon that of the strong nuclear force. The young Einstein, in 1905, was the first scientist to interpret Planck’s work as more than a mathematical trick and took the quantization of light (E = hν) for physical reality. He gave the uninvited dinner guest—the Planck constant h—a place at the quantum mechanics dinner table. What Einstein proposed here was much more audacious than the mathematical derivations by Planck to explain away the UV catastrophe. For a long time the science of optics had hesitated between Newton’s corpuscular hypothesis and Huygens’ wave theory. By the beginning of the nineteenth century the wave theory had become the dominant theory, largely because of the persistence of Augustin Fresnel (1788–1827), who described diffraction mathematically, and James Clerk Maxwell (1831–1879), who introduced the famous Maxwell equations in 1864 (Chapter 5). No wonder Einstein wrote at that time to one of his friends: “I have just published a paper about light, but I am sure nobody will understand it.” Einstein reintroduced a modified form of the old corpuscular theory of light, which had been supported by Newton but which was long abandoned. The particle nature of light was hard to swallow at the time, and it indeed still is. Remember the diffraction of xrays on a crystal described in Chapter 2. Diffraction is something that happens with waves, not with particles. Einstein’s light particles also negated the issue of “ether,” a medium required for wave propagation as in the case of sound waves (sound waves cannot propagate in a vacuum); light is perfectly happy traveling in a vacuum. How can we reconcile this duality of a photon as both wave and particlelike in nature? We will have to learn to think of the wave as the probability of finding the particle. For example, if we know the momentum of the particle exactly, we cannot say where it is, only where it is likely to be [the Heisenberg uncertainty principle (HUP)]. Compton Scattering The first strong support for the quantum nature of light came from monochromatic xray scattering on a graphite block. In 1922, Arthur Compton
99
FIGURE 3.27 Arthur Harry Compton (1892–1962).
(Figure 3.27), at Washington University in St. Louis, saw that the wavelength of xrays increases on scatterings off graphite, depending on the angle (Figure 3.28). This effect cannot be explained using wave theory of xrays. As first explained by Compton in 1923, a photon can lose part of its energy and momentum on scatterings with electrons in the graphite, and the resulting energy loss (or change in wavelength, Δλ) can be calculated from the scattering angle θ. The result is that some of the scattered radiation has a smaller frequency (longer wavelength) than the incident Compton scattering – – – –
–
–
– –
–
Valence electrons
–
– +++ + + +
–
–
–
–
L
– M
K –
–
–
–
– Incident photon (E0)
–
– Compton electron (Ee–)
–
–
–
1 1 < 2
1
Angle of deﬂection Scattered photon (Esc)
FIGURE 3.28 Compton effect. An incoming photon (E0) can inelastically scatter from an electron and lose energy, resulting in an outgoing scattered photon (Esc) with lower energy (Esc < E0).
100
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
radiation. This change in wavelength depends on the angle through which the radiation is scattered, and Compton concluded that an xray photon—or light in general—possesses momentum and thus behaves as a particle. Obviously, this was a big boost for the theory of light as composed of quanta. The three experiments that made the quantum revolution— blackbody radiation, the photoelectric effect, and the Compton effect—all indicate that light consists of particles. FIGURE 3.29 Democritus.
Quantum Mechanics to the Rescue Introduction Invoking quantum mechanics we can solve the many problems with classical theories we exposed in the previous sections. Central to quantum mechanics is Schrödinger’s equation, but before introducing Schrödinger’s equation, we must put down some more foundations. We start with Kelvin’s and Thomson’s plum pudding atom model, then review Rutherford’s and Bohr’s improved orbital atom models, emphasize the importance of the Balmer’s hydrogen emission lines in the discovery of the inner structure of an atom, and then we get baffled by de Broglie’s matter waves and Heisenberg’s uncertainty principle (HUP). There are four principal representations of quantum mechanics: Dirac’s Hamiltonian and quantum algebra representation; the matrix representation of Born, Heisenberg, and Jordan; Schrödinger’s wave equations; and Feynman’s sumoverhistories approach; the latter constitutes a fundamentally new way of looking at quantum theory. With the Schrödinger formalism of quantum mechanics we tackle the band model and revisit electrical and thermal conductivity and heat capacity.
Democritus suggested that all things are “composed of minute, invisible indestructible particles of pure matter.” According to the ancient Greeks, “atomos”* or atoms were all made of the same basic material, but atoms of different elements had different sizes and shapes. The sizes, shapes, and arrangements of a material’s atoms determined the material’s properties. For example, sourtasting substances were believed to contain atoms with jagged edges, whereas round atoms made substances oily. It was further believed that there were four elements that all things were made of: earth, air, fire, and water. This basic theory remained unchanged until the nineteenth century, when it first became possible to test the theory with more sophisticated experiments. Lord Kelvin and J.J. Thomson developed a “raisin cake” model of the atom (also called the plum pudding model, 1897), which incorporated Thomson’s negatively charged electrons as the raisins in a positively charged cake (Figure 3.30).
Bohr’s and Rutherford’s Atom The Greek philosopher Leucippus of Miletus, who lived around 400 BC, first proposed atomic theory of matter. His disciple, Democritus of Abdera, concluded that infinite divisibility of a substance belongs only in the imaginary world of mathematics and further developed his mentor’s atomic theory (Figure 3.29).
FIGURE 3.30 Kelvin’s and Thomson’s raisin cake.
*
Atomos in Greek means “unbreakable.”
101
Quantum Mechanics and the Band Theory of Solids Scattered particles
Beam of particles
Source of particles
Most particles are undeﬂected
Thin gold foil
Circular ﬂuorescent screen
FIGURE 3.31 The Rutherford experiment. Structure of atom experiments.
To check the Kelvin and Thomson model, Geiger and Marsden, working in Rutherford’s lab in 1911, directed a narrow beam of alpha particles, doubleionized helium atoms, of known energy onto a thin gold foil. A ZnS scintillation screen was used to record the striking alpha particles. Most particles went through the gold film undeflected, and some were deflected at small angles; however, they found that, once in a while, for about 1% of particles, the αparticles were scattered backward by the target (Figure 3.31). For a moving alpha particle to be scattered through a large angle, a considerable repulsive force must be exerted. To explain the backscattering, Rutherford proposed that the positive charge in a gold atom must be concentrated in a small region. Rutherford proposed in this way the first realistic model of the atom: he concentrated 99.99% of the mass of the atom in the nucleus, which is only 10−15 m across (Figure 3.32). In other words, the atom (and therefore matter in general) is composed of 99.9999999999999% empty space. The proportion
of nucleus to total atom size is obviously not drawn to scale in Figure 3.32. The problem is that according to classical models the Rutherford model cannot lead to stable atoms. Rutherford’s electrons are undergoing a centripetal acceleration and should radiate electromagnetic waves of the same frequency, socalled bremsstrahlung or “braking” radiation, leading to an electron “falling on a nucleus” in about 10−12 s! In the real world we have stable atoms, and atoms emit certain discrete characteristic frequencies of electromagnetic radiation. The Rutherford model is unable to explain these phenomena. It was the analysis of light emitted or absorbed by atoms and molecules that led the way to better and better atom models. Cold, dilute gases absorb light at characteristic and discrete wavelengths (absorption spectra), and hot gases emit light at discrete wavelengths while continuous light spectra result when hot solids, liquids, very dense gases, or blackbodies (see Figure 3.33) emit light at all wavelengths (emission spectra). (A) (a) (nm) 400
500
600
700
500
600
700
H Hg Ne (b) H (nm) 400 (B) Continuum for free electrons 4 3 H
2
H
H
Balmer lines Ly
Ly
13.6 eV
Ly Lyman lines
n=1 Ground state = lowest energy level
FIGURE 3.32 Rutherford’s atom. Matter is mostly empty space.
FIGURE 3.33 (Aa) Emission lines for H, Hg, and Ne; (Ab) Spectrum of sunlight with the hydrogen lines adsorbed out. (B) The hydrogen atom emission spectra with Balmer and Lyman lines for hydrogen.
102
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
When the light emitted from a hot gas is analyzed with a spectrometer, a series of discrete bright lines is observed. Each line has a different wavelength and color. This series of lines is the emission spectrum (Figure 3.33A). The absorption spectrum consists of a series of dark lines superimposed on the otherwise continuous spectrum. The dark lines of the absorption spectrum coincide with the bright lines of the emission spectrum. The continuous spectrum emitted by the sun passes through the cooler gases of the sun’s atmosphere. The various absorption lines can be used to identify elements in the solar atmosphere, and this led, for example, to the discovery of helium. Atomic hydrogen (one electron and one proton) in a gas discharge tube emits strongly at visible wavelengths Hα , Hβ , and Hγ. More lines are found in the ultraviolet region, and the lines get closer and closer until a limit is reached (Figure 3.33B). These same lines are also seen in stellar spectra from absorption in the outer layers of the stellar gas. There are four bright lines in the hydrogen emission spectrum, and in 1885, a Swiss teacher, Johann Balmer (1825–1898), guessed the following formula for the wavelength of these four lines: L 364.5 s 10 7
n2 (m) n2 4
(3.80)
where n = 3, 4, 5, and 6, which are now called the Balmer series. Equation 3.80 may be rewritten as the socalled Balmer formula as: ¥ 1 1 1´ RH ¦ 2 2 µ L §n k ¶
(3.81)
with positive n and k integers and n > k and RH the Rydberg constant for hydrogen with a measured value of 1.096776 × 107 m−1. With n = 1, we obtain the Lyman series in the UV; visible light is emitted in the Balmer series (n = 2), and with n ≥ 3 the infrared series are obtained (Paschen with n = 3, Brackett with n = 4, and Pfund with n = 5). The discrete emissions in Figure 3.33B suggest discrete energy levels, and Balmer’s formula suggests that the allowed energies are given by (RH/n2) (in case of hydrogen) (Figure 3.34). The “Great Dane,” Niels Bohr, explained the above results for the H emission spectra by introducing four quantum postulates in a model halfway
FIGURE 3.34 Some of the hydrogen emission lines.
between classical physics and quantum theory. He reasoned that if electrons orbit the nucleus in circles with radii restricted to certain values, then the energy also can only take on certain discrete values, i.e., if it is quantized and there is a lowest energy orbit, and the electron is not allowed to fall to a lower energy. The allowed states are called stationary states. When in these permitted orbits, contrary to classical theory, the electrons do not radiate (Postulate 1). Bohr also assumed that classical mechanics applies to electrons in those stationary states (Postulate 2). He recognized that there might be a link between stable orbits and the Planck’s and Einstein’s quantum relation between the quantized energy of a photon and its frequency, so he proposed that radiation absorption or emission corresponds to electrons moving from one stable orbit to another, i.e., ΔE = hν (where h is the Planck constant = 6.6 × 10−34 J·s) (Postulate 3). In classical physics, angular momentum (L) of an object in circular motion is defined as mass (me) multiplied by velocity (v), multiplied by the radius (r) of the orbit, i.e., L = mevr (or L = pr) (Figure 3.35). Bohr argued that allowed orbits are determined by the quantization of that angular momentum, L = nh/2π.
FIGURE 3.35 Momentum p for circular motion is mevr.
Quantum Mechanics and the Band Theory of Solids
In this expression n is called the principal quantum number, and the ground state corresponds to n = 1. So here Bohr postulated that it was not the atom that determined the Planck constant h, but h that determined the properties of atoms (Postulate 4)! Although this planetary kind of model has been shown to be mostly wrong, it makes for a very nice transition to fullfledged quantum mechanics. Bohr’s theory, with slight modifications, is used, for example, to estimate the binding energies of dopant atoms in Chapter 4 and to explain the energy of excitons in Chapter 5. Mathematically we can express Postulate 4 in vector notation as L = p × r = mevr, with v the tangential velocity and p the momentum of the electron (Figure 3.35). Bohr now combined his quantum model of the atom with Newton’s classical model of planetary orbits to calculate the radius of the hydrogen atom. The attractive force between the electron and the proton in a hydrogen atom is caused by the Coulomb force and is given as:
Rutherford could not explain the spectral lines in and Figures 3.33 and 3.34, but he did set up the energy balance for a H atom correctly: En (total energy) = KE (kinetic energy) + PE (potential energy)
E
r e 2 /4 PE 0 me v 2
F
e2 me v 2 r 4 PE 0 r 2
(3.83)
me v 2 m v2
me v 2 – e 0 2 2
E r
n=
0
n=5 n=4
– 0.544 eV – 0.850 eV
n=3
– 1.51 eV
n=2
– 3.40 eV
Excited state
0
r2
r1 Ground state
(3.86)
(3.87)
meaning that, because E < 0, the motion of the electron is not free: it is bound by the attractive force of the nucleus as illustrated in Figure 3.36. To free the electron (and ionize the atom), the electron must receive an amount of energy, called
E
r3
(3.85)
And substituting Equation 3.86 in Equation 3.85 results in:
(3.82)
Based on Newton (Postulate 2), we may write:
me v 2 e2
2 4 PE 0 r
The radial acceleration is a = v2/r, and with Newton’s Law (F = ma) this yields F = e2/(4πε0r2) = mv2/r, which, solving for r, results in:
E =
e 4 PE 0r 2
(3.84)
where the KE term depends on the velocity v and the PE term on the system (e.g., positional or electrostatic), or in the current case:
2
F
103
n=1
FIGURE 3.36 The electron is bound by the attractive force of the nucleus E < 0.
– 13.6 eV
104
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
ionization energy, that will bring its total energy up to zero. Although this concept of a negative energy is somewhat counterintuitive, it does make sense; if we say that an electron has zero energy when far removed from the nucleus, then the electrons that are attached to an atom have a negative amount of energy.
From Bohr model: n2
Lyman series (ultraviolet)
n1 E = hv = 13.6
1 1 – 2 eV n12 n2
c =—
n=3
The Quantum Numbers
2 2 n
e e r me 2 4 PE 0 me (n; /me rn ) 4PE 0n 2; 2
486.1 nm blue green
(3.88)
FIGURE 3.37 The Bohr atom with permitted radii. This Bohr model picture of the orbits has some usefulness for visualization, as long as it is realized that the “orbits” and the “orbit radius” just represent the most probable values of a considerable range of values.
with any integer value for n; by substituting the last two expressions in Equation 3.85, we obtain: En
rn
2
(3.89)
where a0 is the Bohr radius, and permitted orbits have radii r1 = a0, r2 = 4a0, r3 = 9a0 … for n = 1, 2, 3, … as shown in Figure 3.37. ; 2 4PE 0 , has a value of The Bohr radius, a 0 me e 2 −10 0.53 × 10 m. We are now also in a position to calculate Bohr orbit speeds vn: vn
me e 4 me e 4
En 32; 2 P 2 E 02n 2 16; 2 P 2 E 02n 2
2
n ; 4PE 0 n 2a 0 me e 2
n; ; e2 mrn nma 0 4Pn;E 0
me v 2 e2
2 4 PE 0 rn
¨ e2 · 1 e2 me ©
¸ 2 4 PE 0 n 2a 0 ª n; 4PE 0 ¹
Solving this expression for rn results in: 2
434.1 nm violet n=5 n=4
n=1
Paschen series (infrared)
Now we recall Bohr’s fourth postulate about the quannh or tization of angular momentum, L n me vrn 2P also me vrn n; with ; = h/2π. In the latter expression, n = 1, 2, 3, 4… and is called the principal quantum number; the ground state corresponds to n = 1. Thus, Ln is not only conserved but also constrained to discrete values by the quantum number n. This quantization of angular momentum is a crucial result and can be used in determining the Bohr orbit radii and Bohr energies. From the expression for r (Equation 3.86), we derive: rn
n=2
656.3 nm red
First or Principal Quantum Number n for the Level of Energy En
2
Balmer series (visible) 410.2 nm violet
(3.90)
With the latter two expressions, we are able to calculate the total energy of the electron, En, associated
and E 0
(3.91)
me e 4 E 02 32; 2 P 2 E 02n 2 n
e2 me 4 with a value of 13.6 8PE 0a 0 2(; 4 PE 0 )2
eV = 21.8 × 10 –19 J, sometimes called the Rydberg energy. The 13.6eV energy value for an electron in a hydrogen atom (with n = 1) is the energy required to remove an electron from that atom (see also Figure 3.33). The possible energy levels of the hydrogen atom are labeled by the values of the quantum number n. The lowest energy level occurs for n = 1; this is the most negative energy level and the ground state. As n progressively increases, the energy increases
Quantum Mechanics and the Band Theory of Solids
(becomes less negative) for the excited states of the hydrogen atoms, as is clear from Figure 3.36. E Using the expression E n 02 , we can now n invoke Bohr’s second postulate, which says that the photon energy is the difference in En values, and we derive Balmer’s formula: E n hN
¨1 hc 1· E 0 © 2 2 ¸ L n ¹ ªk
¨1 1· 1 E0 ¨ 1 1· e2
2¸
2¸ © © 2 2 hc ª n L k ¹ k ¹ 8PE 0 a 0 hc ª n
(3.92)
¨1 1· RH © 2 2 ¸ k ¹ ªn It was considered a big success for the Bohr model that it accounted for Balmer and other series and that the calculated RH agreed almost exactly (to within 0.1%) with the phenomenological value for the Rydberg constant for hydrogen, i.e., 1.096776 × 107 m−1. The model also gives an expression for the radius of the atom that increases with n2, the orbit speed that decreases with 1/n, and predicts the energy levels of a hydrogen atom that increase with −1/n2, and it can be extended to “hydrogenlike” atoms. Second Quantum Number l for Orbital Angular Momentum By 1914, Bohr had combined the quantum models of Planck and Einstein with the experimental work of Rutherford to provide a quantum model of the hydrogen atom, which fully explained the bright line spectra of hydrogen. To explain the spectra of more complicated atoms, other quantum numbers in addition to the principal quantum number n, defined by Bohr, had to be introduced. More detailed analysis of light spectra again led the way. Arnold Sommerfeld’s (1868–1951) first major contribution was to extend Bohr’s model to quantize all types of motion. He conceived elliptical atomic orbits by analogy to Johannes Kepler’s elliptical planetary orbits and described mathematically orbits with different elliptical shapes but the same value of the principal quantum number n. This gave a number of different stationary states, some with slightly smaller and some with slightly larger energies—and
105
hence multiple spectral lines—just as observed. The orbital angular momentum for an atomic electron can be visualized in terms of a vector model where the angular momentum vector is seen as precessing about a direction in space. Whereas the angular momentum vector has the magnitude shown in Figure 3.38, only a maximum of l units of = can be measured along a given direction, where l is the orbital quantum number. One of Sommerfeld’s other important contributions was to link quantum theory to relativity. If one calculates the speed of an electron moving around the nucleus of an atom a value of the order of 1000 km/s is found. This is small compared with the velocity of light but large enough to have to use relativistic mechanics (see Chapter 5). Using this approach Sommerfeld was able to work out the fine structure of the hydrogen spectrum—a result that was regarded as a triumph both for relativity and quantum theory. Third Quantum Number m, the Magnetic Number In the 1890s, Pieter Zeeman (1865–1943) had noticed that if a magnetic field B was applied to a hot gas, the emission lines were further split into yet a finer structure. Sommerfeld, in 1916, showed that this was because of the direction (i.e., the orientation) of the orbiting of the electron with respect to the magnetic field. Sommerfeld was able to account for this orientation effect with the addition of a magnetic quantum number, m, which was an integer (Figure 3.39). Although called a “vector,” the
FIGURE 3.38 The BohrSommerfeld atom. Sommerfeld introduced a second quantum number, l for elliptical orbitals. Spinup and spindown. Pauli’s fourth quantum number: the electron spin s (see text later this chapter and Figure 3.39).
106
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
FIGURE 3.39 The quantum number m describes how the direction of the angular momentum is quantized with respect to the direction of the magnetic field.
orbital angular momentum in quantum mechanics is a special kind of vector because its projection along a direction in space is quantized to values one unit of angular momentum (=) apart. In Figure 3.39 we show that the possible values that the “magnetic quantum number,” ml (for l = 2), can take are the values m = –2, –1, 0, +1, +2. Fourth Quantum Number s for Electron Spin More detailed measurements of the effects of a magnetic field on spectral line splitting showed yet further fine double splitting of the spectral lines. Wolfgang Pauli (1900–1958) explained this a little later, in 1921, by introducing yet another quantum number. While still a student, he proposed a fourth quantum number that he took to represent the electron spinning, not just in its orbit, but around its own axis. Because there are only two directions of spin, clockwise or spinup and counterclockwise or spindown, there are only two values for Pauli’s electron spin quantum number. No two electrons in an atom can have identical quantum numbers. This is an example of a general principle that applies not only to electrons but also to other particles of halfinteger spin (fermions). It does not apply to particles of integer spin (bosons). The two lowestenergy electron shells have an almost identical shape. Of the two, one shell is occupied or “filled” first with an electron that has an intrinsic magnetic direction that is opposite to the intrinsic magnetic field caused by the nucleus. The next shell has an electron with the
opposite magnetic direction. The DutchAmerican physicists Samuel Goudsmit and George Uhlenbeck discovered the intrinsic “spin” magnetism of the electron in the 1920s. It had been discovered years earlier that in a magnetic field, a beam of electrons splits into two beams (SternGerlach experiment). This fourth quantum number explains this phenomenon. It is believed to be caused by some internal circulation of the electron matter, in addition to its wave flow around the equator of the shell. The wave flow around the equator of the atom also produces atomic orbital magnetic effects. Some shells have no net orbital circulation, which is explained as the result of two equal and opposite counterrotating orbital waves. The magnetism of the nucleus itself is the result of the fundamental internal spin of the proton. Surprisingly, it turned out that the fourth quantum number, spin, s, had only half of the usual quantization value of h/2π, i.e., s = ±1/2 h/2π. Each quantum state, characterized by n, l, and m, is restricted to one electron of s = +1/2 and one electron of s = –1/2. Here classical analogies break down completely—a spin of a half implies the electron has to turn round twice to get back to where it started! The implications of Pauli’s exclusion principle are extremely profound. It is the restrictions imposed by Pauli’s exclusion principle—i.e., the fact no two electrons can be in the same quantum state—that prevents all the electrons from piling up into the lowest (n = 1) energy state, and hence stops all matter from collapsing! Pauli’s exclusion principle also implies that there is some sort of connectivity between the electron states in an atom: one electron must “know” which states all the other electrons are occupying to choose its own state! It is part of one of our most basic observations of nature: particles of halfinteger spin must have antisymmetric wave functions, and particles of integer spin must have symmetric wave functions. In Table 3.5 the different quantum numbers with their properties are summarized. The quantum numbers associated with the atomic electrons along with Pauli’s exclusion principle provide insight into the building up of atomic structures and the periodic properties observed. For a given principal number n, there are 2n2 different possible states.
Quantum Mechanics and the Band Theory of Solids
107
TABLE 3.5 Quantum Numbers and Their Properties The principal quantum number: n
The principal quantum number. Quantization of angular momentum: must be a positive integer (1, 2, 3, 4 … etc.).
The angular momentum quantum number: l
Related to the ellipticity of the orbit: must again be an integer but for a particular orbit can be no bigger than n (l = 0, 1, 2, 3 … n − 1).
The magnetic quantum number: m
Quantization of the orientation of the orbit with respect to a magnetic field: can be a positive or negative integer (m = −l, −l + 1, 0, 1, 2, … l) but must be no larger than –l ≤ ml ≤ 1.
The spin quantum number: s
The electron spin quantum number: must be +1/2 or −1/2.
n
Possible l
Possible m
Possible s
Spectroscopic Notation
Total States
1
0
0
±1/2
1s
2
K or 1st/2
2
0 1
0 −1,0,+1
±1/2 ±1/2
2s 2p
2 6
L or 2nd/8
3
0 1 2
0 −1, 0, +1 −2, −1, 0, +1, +2
±1/2 ±1/2 ±1/2
3s 3p 3d
2 6 10
M or 3rd/10
4
0 1 2 3
0 −1, 0, +1 −2, −1, 0, +1, +2 −3, −2, −1, 0, +1, +2, +3
±1/2 ±1/2 ±1/2 ±1/2
4s 4p 4d 4f
2 6 10 14
N or 4th/32
The Periodic Table of Dmitri Mendeleev (1834–1907) Most of the qualities of an atom are derived from the structure of its electron cloud with the nucleus in the hinterland. This includes most chemical, material, optical, and electronic properties. Not only did the quantum model of the atom proposed by Bohr, Sommerfeld, and Pauli explain atomic spectra, it also explained the periodic table itself (inside front cover plate)! Dmitri Mendeleev (1834–1907) had devised the periodic table by grouping together elements with similar chemical properties. The order of filling of electron energy states in an atom is dictated by energy, with the lowest available state consistent with Pauli’s principle being the next to be filled. The labeling of the levels follows the scheme of the spectroscopic notation. For each value of principal quantum number, one refers to a different shell: n = 1 for the K shell, n = 2 for the L shell, n = 3 for the M shell, and n = 4 for the N shell. Different values of l correspond to different subshells. For example, for n = 2 (K shell) we have two subshells, namely, 2s and 2p. For historical reasons,
Shell/Maximum Number of Electrons
the orbital quantum numbers l were given names associated with their appearance in spectroscopic emission and absorption patterns: l = 0 is given the letter s (for sharp), l = 1 is given the letter p (for principal), l = 2 is given the letter d (for diffuse), and l = 3 is given the letter f (for fundamental). Therefore, we can write the electronic occupation of an atom’s shell as nle, where n is the principal quantum number, l is the appropriate letter, and e is the number of electrons in the orbit. So, for example, nitrogen (N) with seven electrons has the configuration: 1s22s22p3. In chemistry, this is called the Aufbau (buildup) principle, from the German word for structure. As the periodic table of the elements is built up by adding the necessary electrons to match the atomic number, the electrons will take the lowest energy consistent with Pauli’s exclusion principle. The maximum population of each shell is determined by the quantum numbers, and the diagram in Figure 3.40 is a convenient way to illustrate the order of filling of the electron energy states. For a single electron, the energy is determined by the principal quantum number n, and that quantum
108
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
n=7 n=6 n=5 n=4 n=3 n=2 n=1
In the simplest picture, a metal has core electrons that are bound to the nuclei and valence electrons that can move through the metal. Insulators are formed from atoms with closed (totally filled) shells, e.g., inert gases:
7s 6s
6s
6s
5s
5s
5s
5s
4s
4s
4s
4s
3s
3s
3s
2s
2s
1s l=0
l=1
l=2 l=3
FIGURE 3.40 The periodic table of the elements is built up by adding the necessary electrons to match the atomic number.
number is used to indicate the “shell” in which the electrons reside. For a given shell in multielectron atoms, those electrons with lower orbital quantum number l will be lower in energy because of greater penetration of the shielding cloud of electrons in inner shells. These energy levels are specified by the principal and orbital quantum numbers using the spectroscopic notation. When you reach the 4s level, the dependence on orbital quantum number is so large that the 4s is lower than the 3d. Although there are minor exceptions, the level crossing follows the scheme indicated in the diagram, with the arrows indicating the points at which one moves to the next shell rather than proceeding to a higher orbital quantum number in the same shell. The quantum scheme gives a firm scientific basis for Mendeleev’s grouping: the chemical properties of the elements are defined by how nearly full or nearly empty a shell is. For example, full shells are associated with chemical stability (e.g., helium, neon, argon). Shells with a single electron or with one electron short of a filled shell are associated with chemical activity (e.g., sodium, potassium, chlorine, bromine). Most metals are formed from atoms with partially filled atomic orbitals, e.g., Na and Cu, which have the electronic structure: Na 1s 2 2 s 2 2p6 3s1 Cu 1s 2 2 s 2 2p6 3s 2 3d10 4 s1
He 1s 2 Ne 1s 2 2 s 2 2p6 or they form closed shells by covalent bonding as in the case of diamond. With principal quantum number n = 4, the 4f orbitals make their capricious appearance. Because electrons in these orbitals are less strongly held by the nucleus, it is easier to excite them, and they can exhibit a myriad of distinct energy states. This gives rise to the unusual optical and magnetic properties of the rareearth elements. Most atoms with odd atomic numbers (1, 3, 5…) have a very slight overall atomic magnetism because of the one electron spin (and some orbital magnetism in some elements), whereas most even atomic number (2, 4, 6…) atoms have no net electron spin magnetism, and thus approximately zero resulting atomic magnetism. Bohr’s Correspondence Principle Classical physics works for large systems; it is only at the atomic level that it fails. In 1923, Bohr proposed that any satisfactory quantum theory, then still being sought, should be in agreement with classical physics when the energy differences between quantized levels are very small or the quantum numbers are very large. This is the socalled Bohr correspondence principle. Let us consider the two main differences between the quantum theory and classical physics. The first difference is that whereas classical theory deals with continuously varying quantities, quantum theory deals with discontinuous or indivisible processes (e.g., the unit of energy packed in a quantum). The second difference is that whereas classical theory completely determines the relationship between variables at an earlier time and those at a later time, quantum laws determine only probabilities of future events in terms of given conditions in the past. The Bohr correspondence principle states that the laws of quantum physics must be so chosen that in the classical limit, where many quanta
Quantum Mechanics and the Band Theory of Solids
109
are involved (e.g., n is a large integer in E = nh), the quantum laws lead to the classical equations as an average. This requirement combined with indivisibility and incomplete determinism defines the quantum theory in an almost unique manner. In this chapter we will on a few occasions show how classical theory can be derived from an extension of quantum mechanics. An example of this principle that we may appreciate already is that of Newtonian mechanics as a special case of relativistic mechanics when the speed is much less than the speed of light (v Eg (for GaAs, Eg = 1.5 eV), making it an excellent optoelectronic material. The Fermi surface for Cu, shown in Figure 3.117, is a sphere entirely contained within the first Brillouin zone. Even if the free electron Fermi sphere does not intersect a BZ boundary, its shape can still be
affected at points close to the boundary where the energy bands begin to deviate from the free electron parabolic shape. This is the case with Cu, where in the directions, contact is made with the hexagonal Brillouin zone faces. Eight short “necks” reach out to touch the eight hexagonal zone faces. The Fermi surface shown in Figure 3.117 can extend throughout many unit cells if the necks in the directions are joined together with similar surfaces in adjacent cells. A section of such a continuous zone structure is shown in Figure 3.118. A magnetic field may close off these necks, a phenomenon that may be studied using cyclotron resonance. These necks are clearly evident from de Haasvan Alphen oscillations (http://www.lanl.gov/orgs/mpa/nhmfl/users/pages/ deHaas.htm and http://physics.binghamton.edu/Sei_ Suzuki/pdffiles/Note_dHvA.pdf) for magnetic fields in the directions, which contain two periods, determined by the extremal “belly” (maximum) and “neck” (minimum) orbits. The de Haasvan Alphen
FIGURE 3.117 Brillouin zone for Cu with free electron sphere bulging out in the directions to make contact with the hexagonal zone faces.
Quantum Mechanics and the Band Theory of Solids
169
1/ 2
¥ 2m*e E ´ derived earlier as k ¦ 2 µ (Equation 3.150). § ; ¶ For every kstate there is a corresponding energy state. Differentiating the latter expression with respect to energy leads to:
FIGURE 3.118 Continuous Fermi surfaces extending through adjacent unit cells in gold structures.
effect has its origin in the BohrSommerfeld quantization of the orbits of conduction electrons under the influence of a magnetic field. A measurement of the temperature dependence of the oscillation amplitude permits a determination of the cyclotron frequency or, equivalently, the electron mass. Density of States for Bulk Materials The DOS function G(E) is a property that quantifies how closely packed energy levels are in some physical system. It is usually expressed as a function of internal energy E, [G(E)], or as a function of the wave vector k, [G(k)]. The density of kstates, G(k), in the Fermi sphere drawn in Figure 3.111 is the number of allowed states between k and k + dk, i.e., the number of states between a sphere of radius k and a sphere of radius k + dk (analogous to the calculation of the density of states for gas molecules illustrated in Figure 3.7). In three dimensions the volume between the two shells, V is given by: Vdk 4Pk 2dk
(3.225)
The density of states G(k)3D is then derived by dividing this volume by the volume of a single energy state. From Figure 3.66b we recognize that each value of k occupies a volume V = (2π/L)3, so that the number of states per unit volume of kspace is 1/V or (L/2π)3. We also introduce a factor of two here from Pauli’s exclusion principle: each energy state can accommodate two electrons, or: G(k)3D dk 2
4 Pk 2dk ¥ 2P ´ ¦§ L µ¶
3
L3k 2 dk P2
(3.226)
To obtain the density of states in terms of the energy [G(E)3D], we use the relation between E and k,
¥ 2m* E ´ dk ¦ 2e µ § ; ¶
–
1 2
m*e dE ;2
(3.227)
The density of energy states G(E)3D, the number of allowed states between E and E + dE, is then obtained using the chain rule and dividing by L 3 (=V) because we want an expression per unit energy and unit volume: G(E)3D G(k)3D
dk k 2 dk dE P 2 dE
(3.228)
Thus, we calculate the density of states for a parabolic band in a bulk material (three degrees of freedom) as: 3
1 ¥ 2m* ´ 2 1 G(E)3D dE 2 ¦ 2 e µ E 2 dE 2P § ; ¶
(3.229)
for E ≥ 0. There are no available states at E = 0, and the effective mass of the electron takes into account the effect of the periodic potential on the electron. The minimum energy of the electron is the energy at the bottom of the conduction band (CB), Ec. For the valence band (VB), similar results hold. In the case that the origin of the energies is not chosen to be the bottom of the band (i.e., Ec ≠ 0), for the conduction band Equation 3.229 comes with an energy term (E – Ec)1/2, and in the case of the valence band the energy term is given as (Ev – E)1/2. Here the contributions from the light and heavyhole bands add to give the total DOS. Note that, just like the DOS in a 3D ideal gas (Equation 3.19), we obtain a square root dependence in energy E. This function is illustrated in Figure 3.119 (full line). Thus, in the case of free 3D motion, the electronic DOS has a smooth square root dependence on energy E with three continuously varying wave vectors k x , ky, and k z. This holds for materials that are large compared with the de Broglie wavelength (L1, L2, L3 > λDB). An important feature of nanostructure devices is that their DOS is very different from this expression, and
170
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
G(E)dE = 1 × [the number of states in the energy range from E to E + dE] V G(E)f(E)dE = 1 × [the number of ﬁlled states in the energy range from E to E + dE] V Density of states G(E)
kBT
1 Density of ﬁlled states G(E)f (E,T)
EF
Shaded area–ﬁlled states at T=0 2 EF
E
FIGURE 3.119 Density of states (DOS) (full line) and occupied states (shaded area filled at T = 0 K) around the Fermi energy [G(E)3D]. The density of filled states is marked with a broken line. As the temperature increases above T = 0 K, electrons from region 1 are excited into region 2.
this will turn out to have important consequences for their electrical and optical properties. Equation 3.229 gives us the number of possible electronic states of a large 3D device (L1, L2, L3 > λDB). To deduce how these states are occupied with electrons, we need to multiply the density of state function [G(E)3D] with the FermiDirac distribution function, fFD(E, T), which gives the probability that a state of energy E is occupied by an electron. The number of electrons with energies between E and E + dE is then written as: n(E)3D dE G(E)f FD (E)dE
(3.230)
where G(E)3DdE is the number of states between E and E + dE. This function is shown as a broken line in Figure 3.119. The integral of n(E)3DdE over all energies gives the total number of electrons n3D per unit volume (=n3D/V). From Equation 3.230, with f(E) = 1 (T = 0 K), the number density of filled states n3D is: d
EF
n 3D ° n(E)3DdE = ° G(E)3D f(E)dE or 0
0
3
EF
n 3D
° 0
3
1 ¥ 2m*e ´ 2 12 E dE 2P 2 ¦§ ; 2 µ¶
¥ 2m*e E F ´ 2 ¦§ ; 2 µ¶ 3P 2
Note that at T = 0, n(E)3D is zero for E > EF, so we only have to integrate from E = 0 to E = EF. In Figure 3.119 this integral corresponds to the shaded area. For a metal with a total number n3D of valence electrons per unit volume, we can now calculate the maximum energy (EF) and the maximum k value (k F). The maximum energy (the energy at the surface of the sphere) at T = 0 K is obtained by solving for EF:
(3.231)
;2 3P 2n 3D 2m*e
2 3
2
(0.365 eV nm2 )(n 3D ) 3 (3.232)
This Fermi level is the top of the collection of electron energy levels at absolute zero temperature, and it depends on the number of electrons per unit volume (n3D). Example numbers for Fermi energies for different metals can be found in Table 3.13. Because fermions cannot exist in identical energy states (see the exclusion principle), at absolute zero, electrons pack into the lowest available energy states and build up a “Fermi sea” of electron energy states. In this state (0 K), the average energy per electron in a 3D electron gas is calculated as: EF
Total Energy E av Number of Electrons
° EG(E)
dE
° G(E)
dE
3D
0 EF
3D
0
1 n 3D
(3.233)
EF
3 °0 EG(E)3DdE 5 E F
For Cu, for example, this average energy is 4 eV, huge compared with typical thermal energies of 0.025 eV (kT at 300 K). Contrast this result with that of a gas of molecules where a Boltzmann distribution leads to an energy E of zero at 0 K and of the order of kT at a temperature T! The total number N of kstates within the Fermi sphere can be calculated as: 4 3 Pk F k 3F v N 3 3 6P 2 ¥ 2P ´ ¦§ L µ¶
(3.234)
because each kstate occupies (2π/L)3 and the total 4 volume of the Fermi sphere equals Pk 3F. The ratio of 3
171
Quantum Mechanics and the Band Theory of Solids
these two gives the total number of states N, each of which accommodates two electrons; in other words, the density of states n3D(=N/V) at the Fermi level is:
n 3D
2N k 3F 2 V 3P
¥ 2m*e E F ´ ¦§ ; 2 µ¶
3 2
(3.235)
3P 2
giving us back Equation 3.231. Thus, the density of singleparticle states available per unit volume per unit energy of states at the Fermi level in an unrestricted (3D) electronic device is derived as:
From Equation 3.235, k F is given by: 1
k F (3nP 2 ) 3
which depends only on particle concentration n. We can now also ask, what is the speed in the highest occupied state EF? From k F, the Fermi wave vector, we calculate the velocity vF of the electrons on the Fermi surface, i.e., the Fermi velocity (see Equation 3.203, with group velocity vg = vF) as: vF
3
dn 3D G(E)3D (E E F ) dE
E=E F
1 2P 2
¥ 2m*e ´ 2 12 ¦§ ; 2 µ¶ E F (3.236)
This is a very important quantity as the rates of many processes are proportional to G(E). Increasing n3D, the density of electrons in 3D increases both EF (Equation 3.232) and G(E)3D (Equation 3.236). This is of course the same outcome as obtained in Equation 3.229, the only difference being that we replaced E with EF here. The result in Equation 3.236 can be simplified by comparing it with Equation 3.235 to obtain: G(E)3D (E E F )
dn 3D dE
E E F
3n 3D 2E F
(3.237)
What this means is that the density of singleparticle states available per unit volume and per unit energy of states at the Fermi level in 3D is 1.5 times the density of conduction electrons divided by the Fermi energy. Example 3.7: Calculate the Fermi energy EF of Na. Na has an atomic density of 2.53 × 1028 atoms/m3. We are assuming me = me*, i.e., h2 /2me= 1.505 eV.nm2. Answer: Sodium has one valence electron (3s) per atom, so the electron density is n = 2.53 × 1028/m3. Using Equation 3.232 we obtain: EF
1 h2 3P 2ne 4 P 2 2me
pF ;k F me me
2E F m*e
(3.239)
The Fermi velocity is the average velocity of an electron in an atom at absolute zero. This average velocity corresponds to the average energy given above (Equation 3.233). In Equation 3.239, pF is the Fermi momentum, i.e., the momentum of fermions at the Fermi surface, and with the expression for k F in Equation 3.238 we obtain: vF
; 3P 2n 3D m
1 3
(3.240)
We see that in 3D, the higher the electron density, the faster the electrons are moving. In the presence of an electrical field, all the electrons in a conductor move together, so the exclusion principle does not prevent the free electrons in filled states from contributing to the conduction. This is illustrated in Figure 3.120, where we show the Fermi function in one dimension versus velocity at an ordinary temperature. Over a wide range of velocities, the Fermi function equals 1, and speeds vF marked in this figure are given by Equations 3.239 and 3.240. The dashed curve represents the Fermi function after the electric field has been applied for a period t. f(E) No electric ﬁeld
With electric ﬁeld
2 3
1 1.505 eV nm2 3P 2 s 25.3 nm 3 4P2
(3.238)
2 3
–vF
3.31 eV
Obviously electrons in a metal have a very large kinetic energy, even at T = 0!
+vF
vx
FIGURE 3.120 The Fermi function versus velocity in one dimension for a conductor with (solid) and without (broken line) electrical field in the +xdirection. The effect is greatly exaggerated (see text).
172
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 3.12 Fermi Quantities* Fermi Quantity Fermi wave vector
Equation 3D k F (3P 2n)
Typical Value
1 3
2
~108 cm−1 2 3
; (3P 2n) ~1–10 eV 2m*e
Fermi energy
EF
Fermi wavelength
λF = 2π/kF
Fermi temperature TF = EF/kB Fermi momentum p = =kF ;k p vF * *F Fermi velocity me me
Few nanometers for metals, several tens of nanometers for semiconductors ~104–105 K
~108 cm/s
*All values at T = 0 K.
All the electrons have been shifted to higher velocities, but the net effect is equivalent to shifting electrons near the Fermi level only. A typical value for the Fermi velocity at 0 K is ∼106 m/s or 1000 km/s; as pointed out before, this is a surprising result because for a classical gas at 300 K 8k B T the thermal velocity v rms = 105 m/s (see Pm Equation 3.21) with a velocity that goes to zero at T = 0 K! The Fermi wavelength λF is given as 2π/kF; it represents the de Broglie wavelength associated with the Fermi wave vector kF. The Fermi temperature is the temperature TF at which kBTF = EF. Thus, it is the energy of the Fermi level of an assembly of fermions divided by Boltzmann’s constant. The quantity TF is not to be confused with the temperature of the electron gas. Below the Fermi temperature, a substance
gradually expresses more and more quantum effects of cooling. For temperatures much lower than the Fermi temperature, the average energy of the phonons of the lattice will be much less than the Fermi energy, and the electron energy distribution will not differ greatly from that at T = 0. We also recognize here that photons travel much faster than electrons! Photons travel at c = 3.0 × 108 m/s (in vacuum) versus electrons that travel at vF (Fermi speed) = 1.57 × 106 m/s (copper wire). The Fermi quantities we introduced in this section are summarized in Table 3.12, and in Table 3.13 we list calculated free electron Fermi surface parameters for some metals at room temperature.
Electronic Conductivity for Bulk Materials Drude, at the end of the nineteenth century, could not have known about the FermiDirac distribution. Electrons, being fermions, follow this distribution, and at room temperature it is almost the same as at absolute zero temperature, resulting in a velocity distribution for fermions very different from the one predicted by MaxwellBoltzmann statistics. Only electrons near the Fermi level contribute to electrical conductivity, and as a result of the wave nature of the electrons, they can pass through a perfect crystal without suffering any resistance at all. This means that the mean free path of an electron passing through a perfect crystal with all nuclei at rest is infinity rather than the interatomic spacing of the order of 1 nm assumed by Drude. In such an ideal crystal, a Bloch function ψk evolves into Y k $k x , and
TABLE 3.13 Calculated Free Electron Fermi Surface Parameters for Metals at Room Temperature Metal/Valency Cu(1) Ag(1) Au(1) Be(2) Mg(2) Zn(2) Al(3) Ga(3) In(3) Pb(4) Sn(4)
Electron Concentration n (cm−3)
Fermi Wave Vector (cm−1)
Fermi Velocity (cm s−1)
Fermi Energy EF (eV)
Fermi Temperature TF = EF /kB (in K)
8.45 × 1022 5.85 5.90 24.2 8.60 13.10 18.06 15.30 11.49 13.20 14.48
1.36 × 108 1.20 1.20 1.93 1.37 1.57 1.75 1.65 1.50 1.57 1.62
1.57 × 108 1.39 1.39 2.23 1.58 1.82 2.02 1.91 1.74 1.82 1.88
7.00 5.48 5.51 14.14 7.13 9.39 11.63 10.35 8.60 9.37 10.03
8.12 × 104 6.36 6.39 16.41 8.27 10.90 13.49 12.01 9.98 10.87 11.64
173
Quantum Mechanics and the Band Theory of Solids ky
F
kx kavg
FIGURE 3.121 Displacement of the Fermi surface with an applied electrical field. Collisions with thermal vibrations and defects (not stationary ions or other electrons, as Drude envisaged) stop the Bloch oscillations and cause electrons to settle to a drift velocity. See also Figure 3.71, where the Fermi factor in one dimension for a conductor with (solid) and without (broken line) electrical field in the + xdirection is shown.
when this electron state reaches the Brillouin zone at k = +π/a, it reenters the crystal at –π/a or we get resistanceless Bloch oscillations. In the absence of an electric field, the same number of electrons is moving in the ±x, ±y, and ±zdirections, so the net current is zero. But when a field E is applied, e.g., along the xdirection, the Fermi sphere in Figure 3.121, in the absence of collisions, is displaced at a uniform rate by an amount related to the net change in momentum, Δp x , of the free electron gas (FEG) as a whole. The equation of motion (Newton’s law) describes this situation as (see Equation 3.208): ¥ dk ´ dv x m ; ¦ x µ E x e F dt § dt ¶ * e
eE x t ;
k avg
k BZ z
The shift in Fermi sphere creates a net current flow because more electrons move in the + xdirection than the –xdirection. According to this model, the Fermi sphere moves with constant velocity in kspace. This means that the electron velocity increases indefinitely. This is of course not possible, and it is evident that scattering processes must limit the electron velocity and hence the finite electrical conductivity of metals. A viscous term must be introduced in the equation of motion. In a real crystal,
(3.243)
2P 2P z z 2 s 1010 m 1
10 a 3.00 s 10 m
The effect of the Fermi shift in Figure 3.121 are greatly exaggerated. If at t = 0 an electrical field is applied to a Fermi sphere centered at the origin of kspace, the sphere will move to a new position in a characteristic time between scattering events given by:
(3.241)
(3.242)
eE x T ;
The wave vector changes calculated from Equation 3.243 are very small changes; for example, with an electric field E of 1 V/m and with a value for the scattering time τ of ~10−14 s we calculate a value for k avg of ~15 m−1, a quantity very small compared with a BZ dimension, which we calculate as:
T
The quantity = k is the crystal momentum, and thus one can say that the force caused by the electric field is equal to the time derivative of the crystal momentum. Integrating the previous expression we obtain: k x (t) k x (0)
scattering events with a scattering time τ, involving collisions of electrons near the Fermi surface (these are the only ones that can move into empty states), prevent the observation of the ideal Bloch oscillations and oppose the electrical field effect so that the Fermi sphere reaches a steady state when the new center is displaced in the xdirection by an average wave vector:
L v avg
(3.244)
From Equation 3.243 the average velocity of the Fermi sphere is given by: v avg
;k avg * e
m
eE x T m*e
(3.245)
At the steady state the current density is then given as: ¥ ne 2E x T ´ J nev avg ¦ SE § m*e µ¶
[3.3][3.6]
where n is the electron density and: S
ne 2 T m*e
(3.7)
These are the same expressions as derived in Drude’s L (Equation model, but with τ given now as T v avg * 3.244) and me replacing me. The average velocity,
174
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
derived as v 8k B T (Equation 3.21) from the Pm Boltzmann distribution of speeds in Drude’s model, ;k avg eE T x* (Equation is replaced here by v avg * me me 3.245). In Drude’s model the mean free time between collisions of electrons with lattice ions, τ, is related eE T to the average velocity in v v dx x (Equation me 3.6) as: T
L a z vx vx
(3.246)
Drude assumed the electron mean free path, λ, to be equal to the lattice constant, a, which is of the order of 1 nm, in which case this equation yields a typical value for τ of about 10 −14 s. Based on Equations 3.7, 3.21, and 3.246, Drude then derived the following relationship for the resistivity: R
1 me v d m 2e 2 S ne L ne a
8kT Pme
(3.22)
Using the lattice constant, a, for the mean free path, this equation leads to values for the conductivity of a metal that are six times too small. Moreover, from Equation 3.22 the temperature dependence of the resistivity is determined by vdx , which in this model is proportional to T , whereas in practice the temperature dependence of the resistivity is represented by the empirical relationship: R R0 AT
(3.23)
where ρ0 is the resistivity at a reference temperature, usually room temperature, and α is the temperature coefficient. If the Boltzmann distribution function is applied to the electron gas, one thus immediately finds the velocity of the electron to change as T . According to Drude’s model, the mean free path is obviously temperatureindependent because it is calculated from the scattering crosssection of rigid ions (with lattice constant a). This results in a resistivity proportional to T , provided that the number of electrons per unit volume n is temperatureindependent (Equation 3.22). However, people at that time had been well aware that the resistivity of typical metals increases linearly with increasing temperature well above room temperature (Equation 3.23).
To be consistent with the Maxwell–Boltzmann distribution law, one then had to assume n to change as 1 in metals. This was not physically accepted, and T the application of the Maxwell–Boltzmann distribution to the electron system was apparently the source of the problem. In the quantum mechanical model, only a few electrons, all moving at the temperatureindependent very high Fermi velocity v F ~108 cm/s (Equation 3.239), carry the current, instead of all electrons moving at the average drift velocity vd (~0.1 cm/s) in Drude’s model (see p. 82 “Drude Fails”). Only electrons near the surface of the Fermi sphere find empty orbitals in which they can scatter. Electrons in the inner part of the Fermi sphere find no empty states with similar energy as those electrons near the Fermi sphere. Therefore, inner electrons cannot scatter, and those electrons do not contribute to the current transport process. Replacing vth with v F in Equation 3.8, one obtains a value for the resistivity that is 100 times larger than the experimental numbers—understandable because v F is 16 times larger than vth, and we know that the numbers obtained with vth were already six times too large. The resolution lies in the calculation of the mean free path λ; in a perfectly ordered crystal λ = ∞; in a real crystal, λ is determined by scattering phenomena. We need to replace the inner atomic distance a in Equation 3.22 with the quantum mechanics value for λ, the mean free path of the conduction electrons. Experiments have shown that the electrons can move surprisingly far without any interaction; the mean free electron pass can be up to 10 8 atom distances at low temperatures. Electrons are not scattered by the regular building blocks of the lattice because of the wave character of the electrons. Scattering mechanisms instead are: 1. Lattice defects (foreign atoms, vacancies, interstitial positions, grain boundaries, dislocations, stacking disorders), and 2. Thermal vibration of the lattice (phonons). Item 1 is more or less independent of temperature, whereas item 2 is independent of lattice defects but dependent on temperature. The mean free path
Quantum Mechanics and the Band Theory of Solids
now does not depend on the radius of the ions but rather on deviations of the ions from a perfectly ordered array such as seen from lattice thermal vibrations and the presence of impurities. The ion vibrations lead to an effective area A that results in an electron mean free path given as λ = 1/nion A. Lattice ions are basically points only, but their thermal vibration has them occupy an electron scattering area A = πr2, where r is the amplitude of the thermal vibrations. The energy of thermal vibration in a simple harmonic oscillator is proportional to the square of the amplitude of the vibration (r2). In other words, the area A is proportional to the energy of the vibrating lattice ions. From the equipartition theory we know that the average vibration energy is proportional to kT, so it follows that A is proportional to T and λ is proportional to 1/T. Because the mean free path is inversely proportional to tem1 perature at high temperatures, it follows that S t , T in agreement with the experimental evidence (Equation 3.23). This solves the issue of the wrong temperature dependence of the resistivity. We need to also calculate a correct absolute value for the resistance using the quantum mechanical mean free path. The quantum mechanical mean free path of the conduction electrons, say in Cu, is defined as: L vFT
(3.247)
where vF is the velocity at the Fermi surface, because all collisions involve only electrons near the Fermi surface. With Fermi velocities vF of typically 108 cm/s (see Table 3.13) and with roomtemperature resistivities for many metals of ρ ~ 1–10 μΩ·cm, the corresponding relaxation time is ~10 −14 s and the resulting averaged free electron path at room temperature is about 100 Å. So it is of the order of a few 10s to 100s of interatomic distances. At low temperatures for very pure metals the mean free path can actually be made as high as a few centimeters (τ ≈ 2 × 10−9 s at 4 K for very pure Cu). Compared with using the lattice constant, a, for the mean free path, this equation leads obviously to values for the conductivity that are 100 times higher—in agreement with experimental data. For a current J of 1 A/mm 2 in a conductor with an electron density of n = 1022 cm−3, we
175
calculate an average speed vavg of the Fermi sphere of J/ne ∼ 0.1 cm/s (see Equation 3.3), which is much less than the Fermi velocity v F ~ 108 cm/s. In a conductor, charges are always moving at the Fermi velocity, but the Fermi sphere moves much slower because electrons travel at fast Fermi velocities for a short average time, τ, and then “scatter” because of collisions with atom vibrations, grain boundaries, impurities, or material surfaces (especially in very thin films). The value for n(E)3D in J = − n(E)3Devavg (Equation 3.3) at T > 0 is obtained from Equation 3.230: n(E)3D dE G(E)3D f FD (E)dE 3
8P 2me 2 12 E h3
1 e
E EF kT
dE
(3.248)
1
For a large semiconductor, Equation 3.248 was illustrated in Figure 3.119 with a broken line. We will see below that G(E) depends strongly on dimensionality, so we also expect the current density to vary strongly with dimensionality. Quantum Wells: L1,2 > λ DB > L 3 Quantization As we saw earlier, devices that come with a length L that in one direction is comparable with the size of the electron de Broglie wavelength are known as quantum wells (1D confinement). A planar quantum well structure may be made from a thin region of a narrow gap semiconductor sandwiched between two layers of a wide bandgap semiconductor. We use for an example of such 1D confinement a quantum well made by sandwiching a layer of GaAs between two layers of Al xGa1x As, as shown first in Figure 3.59 and, simplified, reproduced in Figure 3.122. Growing two different semiconductors on top of each other, as illustrated, y x z
z L
FIGURE 3.122 A quantum well can be made, for example, by sandwiching a layer of GaAs between two macroscopic layers of AlxGa1xAs. This creates a layer in which the electrons (and holes) behave in a 2D way (see also Figure 3.59).
176
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
forms heterojunctions. The narrower bandgap GaAs material is enclosed by a material with a considerably larger bandgap to establish a potential barrier at the surface of the confined material. Because of the potential barrier, the motion of electrons and holes is restricted in one dimension (thickness L in the zdirection in this case) and is forced to occupy discrete states of energy instead of staying arbitrarily within an energy continuum. Hence quantization of the system occurs by shrinking the thickness of the GaAs layer. A 2D electron gas in the laboratory is really a 3D electron system in which the electron motion is strongly confined in one spatial direction but in which free motion is still allowed in the other two directions. At the interface of the semiconductors GaAs and Al xGa1x As a potential well is formed. The potential well is a result of charge transfer between the two materials and their conduction band offset (Ec), confining the electrons, and the motion of electrons perpendicular to the plane of the heterointerface (zaxis in Figure 3.122) is quantized. The composition x of the ternary semiconductor AlxGa1x As can be varied to control the electron barrier height. A good lattice match between GaAs and AlxGa1x As over a wide range of x values minimizes lattice strain at the interfaces. When the electron and holes are confined in the same layer, one talks about a type I quantum well; with electron and holes confined in different layers, one defines a type II quantum well. For the quantum well considered here, the Al xGa1x As layers are thick enough so that tunneling through these layers remains very limited. For an energy E smaller than the potential barrier V, the energy of an electron in the conduction band of a quantum well is given as:
represents the quantized energy in the zdirection (the thickness direction L of the GaAs film). This is the same expression we derived in Equation 3.156 for a finitesized 1D box with infinitely high potential walls. For quantization to be important, the difference between the electron energy levels should be much larger than the thermal energy kBT, that is, n 2h2 E n z * 2 k B T, where n z = 1, 2, 3 are the quan8me L z tum numbers labeling.the energy levels. E 0c is the energy corresponding to the bottom of the conduction band. Strictly speaking, the above expressions apply only to an infinitely deep potential well. However, we can use the same equations as long as En is well below the bottom of the conduction band of the wide band material. Using this condition, we find, for example, that in GaAs where m*e /me = 0.067, the levels are quantized at room temperature when L z = 150 Å. The third term on the right side of Equation 3.249 represents the kinetic energy of the electrons in the xy plane where they are free to move. The k zcomponent is absent in the last term of Equation 3.249 because the motion in this direction is quantized. Equation 3.249 reveals that for each value of the quantum number n, the values of wave vector components k x and ky form a 2D band structure. The wave vector k z in the zdirection, on the other hand, can only take on discrete values, k z = n zπ/L z. For each value of n there is a subband with n the subband index as illustrated in Figure 3.123. In this figure we show energy levels (bottoms of
E
E
nz = 3
h 2 (k 2x + k 2y ) n 2h2 E n (k x , k y ) E 0c z * 2 , n 0,1,2, 8m*e 8me L z (3.249) E1D (n z ) E1D (k x ,k y )
Subbands nz = 2
m*/πħ2
nz = 1
G(E) (in xy plane) k
with the wave function: Y n (x, y, z) Y n (z)e ik x x e
(a) ik y y
(3.250)
There is one quantized component in the zdirection and a “free” electron component in the xy plane. The second term on the right side of Equation 3.249
(b)
(c)
FIGURE 3.123 (a) Energy levels (bottoms of subbands) for a quantum well made by sandwiching a layer of GaAs between two macroscopic layers of AlxGa1x As (Lz is 150 Å). (b) Energy versus k (k 2x k 2y )1 2 for 2D electron gas in GaAs quantum well. (c) Density of states for quantum well structure (Harris, 2006.4)
Quantum Mechanics and the Band Theory of Solids
subbands), density of states for a quantum well structure, and energy versus k (k 2x k 2y )1 2 for the 2D electron gas in the GaAs quantum well. We can carry out an analogous argument for the holes in the valence band with the difference that their quantized energy is inverted and that we need to invoke m*h for the effective mass of the hole. For a quantum well, the lowestenergy bandtoband (interband) transition is now different from the bandgap (Eg) transition of the bulk semiconductor. It will occur at a higher energy level (shorter wavelength) between the lowest energy state for electrons in the conduction band (n = 1) and the corresponding state for holes in the valence band. This defines the effective bandgap for a quantum well as: E*g E 0c E 0v
1 ´ h2 ¥ 1 *µ 2 ¦ * 8L § me m h ¶
(3.251)
The shift to higher wavelengths is referred to as a “blue shift,” caused by quantization. Fermi Surfaces and Brillouin Zone for Quantum Wells In the case of a free 3D electron gas we appreciate that the surface of the Fermi sea is a sphere of radius k F connecting points of equal energy in kspace (see Figure 3.111). In 2D this becomes a circle connecting points of equal energy in 2D kspace. In Figure 3.124 we show the Fermi circles corresponding to 2D crystals with one, two, three, and four valence electrons per atom. In this figure we also show the 2D Brillouin zone (see square in dashed line), and we see how the free electron circle of a threevalent metal (red circle) cuts the Bragg planes k
located at π/a. The square shown in Figure 3.124 corresponds to the first Brillouin zone of a 2D square lattice (Figure 3.112b). Density of States for Quantum Wells The density of states for each subband of a quantum well (Figure 3.123c) can be found using an approach similar to the one we used above for a 3D density of states function, that is, by counting the number of states with wave vectors k between k and dk. In the case of 1D confinement of electrons we must find the number of kstates enclosed in an annulus of radius k + dk (see Figure 3.125). Each state occupies an area A of 2
¥ 2P ´ ¦§ L µ¶ . The area of the annulus, A, is given by: Adk 2Pkdk (3.252) Dividing the area of the annulus by the area occupied by a kstate, and remembering again to multiply by 2 for the electron spin states, we get for the number of states per unit area: G(k)2D dk 2
2Pkdk ¥ 2P ´ ¦§ L µ¶
k
2
L2 k dk P
(3.253)
Or, in terms of energy per unit area at an energy E (dividing by L2), the density of states for each subband is given as:
kdk G(E)2DdE P
2m*e E ¥ 2m*e E ´ ; 2 ¦§ ; 2 µ¶
–
1 2
m*e dE P; 2
m*e dE P; 2
(3.254) k
k
177
k k k
k
FIGURE 3.124 Free electron circles for 1, 2, 3, and 4 valence electrons. The free electron circle of a threevalent metal (red circle) cuts the Bragg planes located at π/a.
FIGURE 3.125 Density of states, G(k)2D, is the number of allowed states between k and k + dk, i.e., the number of states between a sphere of radius k and a sphere of radius k + dk.
178
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
* FIGURE 3.126 Filling of the first two subbands in a 2D structure. The first subband has a constant energy at me (a), * P; 2 and the second has a constant energy at 2me (b).4 P; 2
For this derivation we used Equation 3.227, which holds true for any dimensionality D of the problem. Importantly, in an ideal 2D system, the density of states is constant and does not depend on energy. The density of states in a 2D electron gas, in which only the lowest energy subband (n = 1 level Ez1) is occupied, is illustrated in Figure 3.126a, where we assume that the confinement is in the zdirection. For all electron energies up to Ez1 the density of states is zero because electrons cannot exist in the well at lower energies than this. Because of the freedom of motion in the plane of the hetero interface (with continuously varying wave vectors k x and ky in the xy plane), the energy levels that form in the potential well are highly degenerate. If the electron density is sufficiently low, then all electrons can be accommodated in the lowest level of the well, and the freedom of motion in the transverse direction is frozen out and the electron system effectively behaves as the ideal 2D one as described by Equation 3.254 with a single step in m* energy only with a constant value e2 . In the regime P; where only the lowest subband is occupied, increasing energy corresponds to increasing electron motion in the xy plane (kinetic energy). As the electron filling of the quantum well is increased, eventually electrons begin to fill the next transverse level of the potential well (Figure 3.126b). At this point we have two socalled 2D subbands occupied in the quantum well. To a good approximation, electrons in the two subbands may be viewed as forming two independent 2D electron gas systems. Thus, the density of states is double that which we would expect in the case where just a single subband is occupied. For each quantum state in
the quantum well, there will be a step in the density of states. The overall density of states is discontinuous, with a stepwise structure that is characteristic of quantum wells. Because of the summing over the different subbands, a more general description of a 2D system has Equation 3.254 modified as: G(E)2D
m*e ¤ H(E – En ) P; 2 n
(3.255)
where H(E − Ec) is the Heaviside step function.* It takes the value of zero when E is less than En and 1 when E is equal to or greater than En. En is the nth energy level within the quantum well. In Figure 3.127 we summarize the characteristics of a 2D density of states function G(E)2D. The energy spacing shown here increases with decreasing L; the thinner the 2D film, the more it approximates an ideal 2D gas with only one subband. The steplike behavior of a 2D density of states function G(E)2D implies that the density of states in the vicinity of the bandgap is much larger than in the case of a bulk semiconductor, where the value of G(E)3D goes to zero (E1 versus Eg). This makes for stronger optical transitions because a major factor G2D(E) E2 E1 Eg
E
Eg
z
E E1
E2
FIGURE 3.127 The density of states function for a quantum well. The solid black curve is that of a free electron. The bottom of the quantum well is at energy Eg. *
The Heaviside step function, H, also called the unit step function, is a discontinuous function whose value is zero for negative argument and one for positive argument.
Quantum Mechanics and the Band Theory of Solids
2
(transition matrix element H v,c a ). The enhanced oscillator strength of quantumconfined structures is put to good use in the fabrication of laser media for highly efficient and compact solidstate lasers (see Chapter 5). In Figure 3.128 we illustrate the boundstate energies for electrons in the conduction band and for holes in the valence band for a GaAs/Al xGa1x As heterojunction. If the GaAs layer is thin enough, bound states form as indicated here by dashed lines. For a perfect 2D electron gas, each bound state corresponds to a discontinuous jump in the electronic density of states function. The density of states function (DOS) can be investigated by measuring the absorption α of electromagnetic radiation associated with the excitation of an electron from the valence band to the conduction band. Because the wavelength of the radiation is long compared with the width of the well, transitions only occur between states for which the spatial variation of the wave function is similar; this leads to the selection rule Δn = 0 for the adsorption. Therefore, the allowed transitions are those indicated by the arrows AlxGa1xAs GaAs Electron bound states
AlxGa1xAs n=3
Conduction band edge
n=2 n=1
Possible photon absorption transitions Hole bound states (a)
n=1 n=2 n=3
Valence band edge
in Figure 3.128a. The frequency dependence of the absorption should reflect the steps in the DOS with the steps in the absorption expected to occur at frequencies ωn given by: ;W n E Cn E Vn
(3.256)
where ECn − EVn is the energy difference between the nth bound states in the conduction and valence bands. The measured adsorption spectra for GaAs layers of thickness 140, 210, and 4000 Å are shown in Figure 3.128b, and the expected step structure is clearly visible for the two thinner layers, with arrows indicating the frequencies at which steps are expected. Peaks at energies just a little below the predicted values mark the absorption. These results from the creation of an exciton, an electronhole bound state that is created when a photon is absorbed (see below for details). Because there is an attraction between the electron and the hole in an exciton, the photon energy required to create an exciton is lower than the predicted values that ignore such interactions. Thus, the difference in energy of the peak and the predicted absorption edge is a measure of the binding energy of the electronhole pair. An exciton, with an energy just below the bandgap, is clearly seen in the absorption curve for the 4000Å layers, but the steplike structure has disappeared, indicating that the DOS is a smooth curve as one expects for 3D behavior. Electronic Conductivity of Quantum Wells The circles shown in Figure 3.124 are the Fermi circles corresponding to 2D crystals with one, two, three, and
Lz Absorption intensity
in the expression for the probability of optical transitions is the density of states. The strength of an optical transition is often defined as the oscillator strength, and the oscillator strength of a quantum well in the vicinity of the bandgap is considerably enhanced compared with a bulk semiconductor. Below we will show how Fermi’s golden rule for absorption describes transition rates between levels in terms of the availability of states [density of states: G(E)], the availability of photons (intensity E0), and a “coupling strength” between the levels
179
(b)
n=4 n=2
n=3
4000 Å 210 Å
n=3 n=2
1.515 1.550
140 Å
1.600 1.650 1.700 Energy (ev)
FIGURE 3.128 (a) Heterojunction of GaAs and AlxGa1x As. If the GaAs layer is thin enough, bound states (dashed lines) form. When photons are absorbed, electrons are excited between these bound states. (b) The adsorption of light, measured as a function of photon energy for GaAs layers of thickness 4000, 210, and 140 Å. The arrows indicate the energies at which the onset of adsorption is expected to occur for transitions involving the nth bound state.
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Carrier distribution
180
Quantum wells (QWs) G(E) f(E)
n(E) Energy
FIGURE 3.129 Deformation of the free electron circle near Bragg planes, V(x) ≠ 0.
four valence electrons per atom. The circles represent surfaces of constant energy for free electrons [V(x) = 0], i.e., the Fermi surface for some particular value of the electron concentration. The total area of the filled region in kspace depends only on the electron concentration and is independent of any interaction of electrons with a lattice. In a solid more realistic shape of the Fermi surface depends on the lattice interaction of the electrons and will usually not be an exact circle in a lattice. There is a discontinuity introduced into a free electron Fermi circle any time it approaches a 2D Brillouin zone boundary. In Figure 3.129 we see how the shape of the Fermi circle is distorted near the surface if V(x) is not zero. Energy gaps appear at zone boundaries, and the Fermi surface intersects zone boundaries almost always perpendicularly. The crystal potential causes rounding of sharp corners on a Fermi surface. The volume enclosed by a Fermi surface only depends on electron density and not on details of the lattice interaction. In other words, the volume enclosed by a Fermi surface remains unchanged under the “deformations” just mentioned. The number of occupied states per unit volume in the energy range E to E + dE and with f(E) = 1 (T = 0) is calculated as: EF
d
n 2D ° n(E)2DdE ° G(E)2D [f(E) 1]dE 0
0
(3.257)
or EF
n 2D
m*e
° P; 0
2
dE
m*e E F P; 2
To calculate the current density for a 2D gas at a particular temperature we substitute the value for n(E)2D at T > 0 [and thus f(T) can then be different
FIGURE 3.130 Quantum wells (QWs). Density of states (DOS) (blue) and occupied states (red) around the Fermi energy for a quantum well. The FermiDirac function is f(E), and the product of f(E)G(E)2D = n(E)2D at T > 0.
from 1] in J = −n(E)2Devavg (Equation 3.3). The function n(E)2D for a given temperature T (>0) is shown as a red line in Figure 3.130. In the same graph we also show the FermiDirac function and the DOS function (blue). The form of the density of states function of a 2D gas can also be dramatically modified by a magnetic field, giving rise to very pronounced behavior in the conductance with the appearance of the socalled Landau levels. Quantum Wires: L1 > λ DB > L 2, 3 Quantization We saw earlier that when L becomes very small along two directions (2D confinement)—of the order of the de Broglie wavelength of an electron—one obtains a quantum wire where electrons can only move freely in one direction, i.e., along the length of the quantum wire as shown first in Figure 3.63 and, simplified, reproduced in Figure 3.131. These 1D electronic structures with 2D quantum confinement comprise nanowires, quantum wires, nanorods, and nanotubes. The starting point for the fabrication of one type of quantum wire is a 2D electron gas confined in one direction as discussed above. A 2D quantum gas that is very strongly confined at some interface and where we can assume that only the lowest subband of the electron gas is occupied, so that the motion transverse to that interface is frozen out. This is the situation we encountered for a y x z
FIGURE 3.131 A rectangular quantum wire.
Quantum Mechanics and the Band Theory of Solids
heterojunction with a very small L, so that Equation m* 3.254 is applicable [G(E)2D e2 (no summation of P; steps)]. To this strong confinement, a typically weaker, lateral confinement of the electrons is added by etching nanowires in the 2D quantum well. In Figure 3.131 we drew a rectangular quantum wire with a square crosssection; in reality nanowires will typically be much wider than they are thick (the xdirection is assumed to be the film thickness direction), so the quantum confinement is most severe in the xdirection. The reason for this discrepancy is that in micro and nanotechnology it is much easier to control a film’s thickness (x direction) than it is possible to control the lateral dimensions of a structure (y direction). Let us consider the 75nmwide quantum wires etched in a GaAs/Al xGa1x As heterojunction in Figure 3.132. The 2D electron gas formed at the heterointerface is confined here in a scale of just a few nanometers (in the thickness or x direction), and so its quantized energies are large in the x direction. The lateral confinement (y direction) of electrons in the 75nmwide wire is much weaker than this and its quantized energies are consequently much smaller. The weaker lateral confinement in the wires gives rise to a series of relatively closely spaced energy levels (see EY in Figure 3.132). Therefore, transport through the wire in the zdirection will involve electrons that occupy many of these lateral subbands. Thus, these structures in reality are quasi2D confined systems with free electron motion in one direction and two different types of confinement in the other two.
Ey E4
E3 y
E2 E1
FIGURE 3.132 75nmwide quantum wires etched in a GaAs/AlxGa1x As heterojunction. The confinement of electrons in the x and ydirections quantizes the electron energy into a set of discrete energies. The confinement in the xdirection is much stronger than in the ydirection.
181
For an idealized nanowire with a square cross section and the x = y dimensions in the nanoscale but continuous along the wire axis (zdirection), the energy dispersion function may be written as: E E n1 ,n 2 (k z )
; 2 k 2z 2m*e
(3.258)
with the wave function: Y( x, y, z) Y n1 ,n2 ( x, y)e ik yz
(3.259)
with n1 and n2 the quantum numbers labeling the eigenstates in the xy plane and k z the wave vector in the zdirection, and where we assume that the dispersion relation for the electron energy is parabolic. The energy term has again two contributions: one is 2 2 caused by the continuous band value ¥ ; kz ´ , and ¦§ 2m* µ¶ e the other term [E E n1, n 2 (k z )] is that of the quantized values of electrons confined in two dimensions as derived in Equation 3.158 (unconstrained direction is along the zaxis). Referencing energies to the conduction band edge, the latter expression may be rewritten as: E n1,n 2 (k z ) E 0c
h2 8m*e
¥ n12 n 22 ´ ; 2 k 2z ¦§ L2 L2 µ¶ 2m* e 1 2
(3.260)
0
where Ec is the bottom of the conduction band. The lowest subband is obtained for n1 and n2 = 1. The energy at the bottom of each subband (k z = 0) is simply given by: E n1,n 2 E c0
h 2 ¥ n12 n 22 ´ 8m*e ¦§ L21 L22 µ¶
(3.261)
If we choose the crosssection of the GaAs quantum wire containing the 2D confined electron gas to be equal to 100 × 100 Å, then the lowest energies in the two lowest subbands are equal to 0.112 eV and 0.280 eV. This is determined from Equation 3.261 for n1 = 1, n2 = 1 and n1 = 1, n2 = 2, respectively. In the case that the nanowire is much wider (ydirection) than it is thick (xdirection), the quantum confinement is most severe in the xdirection. Because in this case Ly >> Lx, the n2 levels form a staircase of small steps in the widely separated subbands corresponding to the various values for n1. Thus, confinement that is different in the x and y directions splits each
182
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
subband further up into a set of more narrowly spaced subbands. In Figure 3.133 we show band structure and density of states for a quantum wire with a square cross section; similar to the situation in quantum wells, subbands are formed, but in quantum wires with a rectangular crosssection multiple subbands form ; 2 kz2 at each eigenvalue E(nx ,ny), spread out as . 2m*e Fermi Surface of Quantum Wires Whereas Fermi surfaces in 3D and 2D electronic structures consist of a sphere and a circle, respectively, the Fermi surface of a strictly 1D electronic structure consists of just two points at +k F and –k F or ° dk = 2k F (where 2k F k F is the Fermi wave vector) or n1D = . This P unusual Fermi surface has some pretty significant consequences. In 1981, Hiroyuki Sakaki predicted that ideal 1D electrons moving at the Fermi level in quantum wires would require very large momentum changes (Δk = 2k F) to undergo any scattering. The result is that electron scattering is strongly forbidden. This is a consequence of the fact that in one dimension, electrons can scatter only in one of two directions: forward and 180° backward. With this large reduction in scattering, electrons should achieve excellent transport properties (e.g., very high mobility).
we use the same approach we took for the 3D and 2D cases. The kstate has now a length l of 2π/L, and we must find the number of kstates lying in a length of k + dk. The wire length difference, l, is given by:
The factor of two appears because the wave number could be either positive or negative, corresponding to the two directions along the wire. The resulting density of states per unit length of 1D kspace is obtained by multiplying by 2 for spin degeneracy and dividing by 2π/L: ¥ 2 ´ 2L G(k)1D dk 2 ¦ dk dk µ P § 2P /L ¶
1
¥ 2m* E ´ 2 derived earlier as k ¦ 2e µ (Equation 3.150) § ; ¶ and differentiate the latter expression with respect to energy: ¥ 2m* E ´ dk ¦ 2e µ § ; ¶
1 2
m*e dE ;2
(3.227)
1
2dk 1 ¥ 2m*e ´ 2 1 G(E)1DdE ¦ 2 µ dE 1 P P§ ; ¶ 2 E * 1 2me dE E hP
(3.264)
This is in sharp contrast with the behavior of a 3D electron gas where G(E)3D goes to zero at low energies, and two dimensions, where G(E)2D steps up to a constant value at the bottom of each 2D subband. Remembering that the group velocity is given as:
(2,1) Subbands (1,3) (2,1) (1,2)
dW dk which we found may also be written as: vg
(1,1) (in zdirection) kz
–
The density of energy states G(E)1D, the number of allowed states between E and E + dE, per unit energy and unit length (divide by L) is then obtained using the chain rule:
E
(2,2)
(nx,ny)
(3.263)
To obtain the density of states in terms of the energy [G(E)1D], we use again the relation between E and k,
Density of States Function for Quantum Wires For calculating the density of states for a quantum wire,
E
(3.262)
l 2
G(E)
FIGURE 3.133 Band structure and density of states for a quantum wire with a square crosssection.4
vg
(3.101)
1 ¨ dE · 1 or more generally v g k E(k) (3.202) ; ©ª dk ¸¹ ;
Quantum Mechanics and the Band Theory of Solids
we can rewrite Equation 3.264 now also in terms of the group velocity as:
G(E)1D E12 E11 Eg
E
1
G(E)1DdE
2 2dk 2 ¥ dE ´ ¦ µ dE dE (3.265) P P § dk ¶ P;v g (E)
Thus, for a 1D system the density of states is inversely proportional to the velocity! We will use this expression in vg when we derive the expression for the current through a nanowire. We will learn that in a nanowire the current is constant and proportional to the velocity and density of states (see further below Equation 3.269). If we add electrons to the nanowire, they initially fill only the lowest of the levels, say level (1,1) in Figure 3.133. As the energy is increased and remains less than level (1,2), the lateral motion remains frozen, and the increase in energy is transferred into motion along the length of the wire. The density of states in this level will then take the form predicted by Equation 3.265. However, in most situations the Fermi energy of the electrons in the wire is several times larger than the average spacing between the lateral energy levels in Figure 3.133, so several of these levels will be occupied, and each of these levels defines a corresponding 1D subband. The density of states within each subband is 1D, but the total density of states is obtained by summing over all subbands n. The summing over the individual subbands can be formulated mathematically as: 1
1
¥ 1 ´2 1 ¥ m* ´ 2 G(E)ID ¦ 2e µ ¤ L ¦ P § ; ¶ n § E E n µ¶
(3.266)
L is the unit step function (same as H in Equation 3.255). The density of states of a quantum wire 1
¥ 1 ´2 diverges as ¦ at each subband threshold § E En µ¶ and has the inverse energy dependence E−1/2 compared with the E1/2 dependence of a 3D electron gas (bulk semiconductor). The DOS of a quantum wire obviously has a more pronounced structure than does a 2D well, with a large number of subbands, each one starting as a peak. An immediate manifestation of a large G(E)1D at the bottom of each subband is again an increase of the strength of optical transitions or oscillator strength as compared with 3D and 2D electronic structures.
183
x,y
Eg
E E00
Enm
FIGURE 3.134 The density of states function for a rectangular quantum wire. The solid black curve is that of a free electron.
In Figure 3.134 we summarize the characteristics of a 1D density of state function G(E)1D. The axis of the rectangular wire is again in the zdirection, and quantization is in the x and ydirections. The peaks show the calculated density of states of a quantum wire over a range of energies where several different subbands become occupied. For comparison, the solid line shows the monotonic variation of the density of states expected for a 3D system. Electronic Conductivity of Quantum Wires Ohm’s law for macroscopic systems is given by V = IR, and in terms of conductance σ this is equivalent to σ = J/E (Equation 2.2). From the previous sections, we know that only electrons close to the Fermi level contribute to the conductance. From Bloch’s theorem, we also recall that in an ideal periodic potential, electrons propagate without any scattering—and thus no resistance at all—but that electron propagation in real materials does involve scattering. The origin of such scattering can be any source of disorder that disturbs the perfect symmetry of the lattice. Examples include defects and impurities, scattering from other electrons, and lattice vibrations (phonons). Because an electric current constitutes a movement of those “bumbling” electrons under an electric field, one expects that with nanostructures featuring dimensions comparable with the fundamental size of the electron, electrical properties will be strongly influenced by quantummechanical transport effects. Each of the discrete peaks in the density of states (DOS) in Figure 3.134 is caused by the filling of a new lateral subband. The peaks in the density of states functions at those energies where the different subbands begin to fill are called criticalities or Van Hove singularities. These singularities (sharp peaks) in the density of states function lead to sharp
184
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
where n1 is an empty band and n2 is a filled band. This can also be appreciated by considering that the density of states according to Equation 3.228 is given as G(E) = G(k)(dE/dk)−1, so that singularities emerge when dk/dE = 0 (for an example of such states, see the band diagram of Si in Figure 3.116, states at E1 and E2). The number of occupied states at T = 0 [where f(E) = 1] per unit volume in the energy range E to E + dE is again calculated from n(E)1D dE = G(E)1D [f(E) = 1]dE and one obtains:
k [E n1 (k) E n 2 (k)] 0
To calculate the number of occupied states at T > 0 per unit volume in the energy range E to E + dE, we use again n(E)1D dE G(E)1D f(E)dE, but because T is now > 0, f(E) might be different from 1. That function is shown as a red line in Figure 3.136. Consider now a quantum wire held between ideal contacts, as shown in Figure 3.137. In this very short 1D wire, the charge transport is assumed to be ballistic, i.e., electron transport without scattering, or the mean free path (λ) and device size (L) are comparable. Because the current carrying capacity of a 1D wire is finite, there must be a finite conductance even in the absence of scattering. Applying a voltage V
#
!
"
#
!
n1D ° n(E)1D dE 0
EF
° G(E)1D [f(E) 1]dE or n1D 0
EF
that n1D
° G(E)
1D
dE indeed equals
0
2k F P
(3.268)
2k F is easily P
recognized from the fact that: G(E)1DdE
2dk P
(3.265)
d
#
#
FIGURE 3.135 Van Hove singularities can be observed directly with scanning tunneling microscopy (STM). This is illustrated here for a metallic and semiconducting carbon nanotube. The DOS is shown in (a) and (b) and the differential conductance in (c) and (d). (From Dekker, C., Physics Today, 52, 22–28, 1999. With permission. 24)
Carrier distribution
!
(3.267)
"
!
peaks in optical spectra and can also be observed directly with scanning tunneling microscopy (STM). The STM tunneling current J as a function of bias V gives spatial and spectroscopic information about the quantum states of nanostructures. At low temperatures, the derivative of the current with respect to voltage is roughly proportional to the density of states of the sample weighted by the density of states at the STM tip position in other words a convolution of the DOS of the tip and the sample. Because dJ/dV ∼ DOS, the DOS is directly observed from an STM scan. This is illustrated in Figure 3.135 for a metallic and semiconducting carbon nanotube. The DOS is shown in Figure 3.135a and b, and the differential conductance is illustrated in Figure 3.135c and d. Metallic carbon tubes have a constant DOS around E = 0, whereas for semiconducting ones there is a gap at E = 0 (DOS = 0). Singularities occur because electron transitions accumulate at frequencies for which the bands n1,n2 are parallel, i.e., at frequencies where the gradient is equal to zero:
Quantum wires
G(E)
f(E) n(E) Energy
FIGURE 3.136 Quantum wires. Density of states (DOS) (blue) and occupied states (red) around the Fermi energy for a quantum wire. The FermiDirac function is f(E), and n(E) is the product of f(E) and G(E)1D at T > 0.
Quantum Mechanics and the Band Theory of Solids
FIGURE 3.137 A quantum wire held between ideal contacts. In this very short onedimensional wire, the charge transport is assumed to be ballistic with the mean free path (λ) and device size (L) comparable. Fermi level EF(1) = μ1 and Fermi level EF(2) = μ2 with EF(2) − EF(1) = qV, where q = −e for electrons and +e for holes. A net current flows between the two contacts for an applied bias V. A positive wave vector k is assumed with excess rightmoving electrons constituting the current.
over the wire has an excess of electrons moving in one direction only (left to right in the current case), so we assume a positive wave vector k with excess rightmoving electrons constituting the net current. The chemical potential μ of the electrons in the contacts, we recall, is equivalent to the Fermi level, and here we assign the contacts Fermi level EF(1) = μ1 and Fermi level EF(2) = μ 2 with EF(2) − EF(1) = qV, with q = −e for electrons and +e for holes. To calculate the current density for this 1D electron gas at T = 0, we must substitute the value for n(E)1D at T = 0 [where f(E) = 1] in J = −n(E)1D evavg (Equation 3.3), and EF
d
because n(E)1D ° n(E)1D dE ° G(E)1DdE, we can use 0
0
the expression for G(E)1D in terms of the group veloc2 ity, G(E)ID (Equation 3.265), resulting in: P;v g (E) E F (1)
J n(E)1D ev avg (E) e
°
v avg (E)n(E)1D d
E F (1) E F (2)
e
v avg (E)G(E)1D dE
°
E F (1) E F (2)
J e
°
v avg (E)
E F (1)
2 dE P;v g (E)
and
since v avg (E) v g (E) J
2e 2e 2 [E F (2) E F (1)] V h h
(3.269)
since EF (2) – EF(1) = qV, with q = –e for electrons and +e for holes.
185
For a macroscopic metal wire, the conductance decreases continuously as the diameter of the constriction is reduced. However, as the diameter becomes of the order of the Fermi wavelength, the conductance takes on integer values of the fundamental unit of conductance σ (= J/V) = 2e2/h. The conductance σ (= J/V) is fixed, regardless of length L of the conductor, and as a consequence there is no welldefined conductivity σ. This phenomenon is called quantized conductance (QC). What is remarkable is that in the case of a quantum wire the velocity cancels with the density of states, producing a current that depends only on the voltage and fundamental constants. As a consequence, the current carried by a subband is independent of the subband shape; it need not be parabolic, and the relation holds for all cases! The amount of current is dictated only by the number of modes (also called subbands or channels) M(EF), which are filled between μ1 and μ 2 with each mode contributing 2e2/h or: 2e 2 M(E F ) (3.270) h The corresponding quantized resistance is: S
R
h 1 2 2e M(E F )
(3.271)
As we increase the channel crosssection, the number of modes increases, so the resistance goes down. This quantized resistance R has a value of 12.906 kΩ and has allowed for the definition of a new practical standard for electrical resistance: the resistance unit h/e², roughly equal to 25.8 kΩ; the latter number is referred to as the von Klitzing constant RK (after Klaus von Klitzing, the discoverer of quantization of the Hall effect), and since 1990, a fixed conventional value RK –90 has been used in resistance calibrations worldwide. Resistance of a conductor, of course, decreases as the length of the channel decreases. But at some point it reaches a minimum, given by Equation 3.271, and decreases no further. This minimum resistance comes from the contact resistance, and the smaller the device, the more important this contact resistance. One might assume that this resistance can be eliminated by improving the contacts, but this simply is not true: there is a minimum contact resistance.
186
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Quantized conductance in a quantum wire is dramatically illustrated in Figure 3.138, where we show experiments involving quantum wires in a GaAs/ Al xGa1–x As heterostructure at very low temperatures (close to 0 K). A short quasi1D “wire” is formed here between two regions of a 2D electron gas as a negative gate voltage Vg applied to the metallic gates on the surface depletes the carriers in the underlying 2D electron gas in the GaAs (Figure 3.138a). Once the narrow constriction is reduced to a width d comparable with the electron Fermi wavelength λF (see Figure 3.138b) 1D quantization is obtained regardless of the wire length L. In the conductance voltage plot shown in Figure 3.138c, 14 quantized conductance steps of height 2e2/h are observed for a wire width d of 0.5 μm (see also Figure 3.138d). Each step corresponds to the occupancy of an additional subband or additional conductance channel in the quantum wire. In other words, M(EF) = 14. (a)
The conductance voltage plots in Figure 3.138d show that quantized steps are still clearly present for the 5μm wire, indicating ballistic transport, but wash away for 10μm wires because of crossover to diffuse transport. Thus, for this GaAs 1D system, the electron Fermi wavelength λF mean free path is between 5 and 10 μm. Long electron Fermi wavelengths λF are obviously key to integrating these 1D electronic nanostructures. An important experimental finding is that the conductance quantization is typically destroyed in narrow constrictions longer than a few hundred nanometers; ballistic transport cannot be preserved on length scales much longer than this. The reason for this is that as the constriction length is made longer, there is a greater probability of finding some disordered region (a barrier) that can disrupt ballistic transport by causing electron scattering. When we derived the conductance quantization (b)
Gate AlxGa1–xAs
2D
Narrow constriction; quasi1D (width d ~ Fermi wavelength λF)
Co
GaAs Twodimentional electron gas
Ballistic transport in 0.5 μm quantum wire
16 12 8 4 0
14
7
10
Conductance (2e2/h)
Conductance (2e2/h)
20
Ballistictodiﬀuse crossover
(d) 8
Conductance (2e
24
2/h)
(c)
2D
d
Co
nt
nt
ac
ac
t
t
L
5 0
–3
–2.5 –2 –1.5 VGate (V)
Metallic gate 2DEG
–3.0 –2.5 –2.0 –1.5 –1.0 –0.5 VGate (V)
1D
0.0
6 5 4 3 0.5μm 5μm 10μm
2 1 0
–1.0
–0.8
–0.6 –0.4 VGate/VGate
–0.2
FIGURE 3.138 Conductance quantization in a short channel electrostatically defined in a GaAs/AlxGa1–x As heterostructure. Measurements are carried out at very low temperatures (close to 0 K). (a) A negative gate voltage Vg applied to the metallic gates depletes the carriers in the underlying 2D electron gas. (b) Once the narrow constriction is reduced to a width d comparable to the electron Fermi wavelength λF, 1D quantization is obtained regardless of the wire length L. (c) In the conductance voltage plot, 14 quantized conductance steps of height 2e2 /h are observed for a wire width d of 0.5 μm. (d) Ballistic to diffuse transport crossover in GaAs quantum wires. The conductance voltage plots show that quantized steps are still clearly present for the 5μm wire, indicating ballistic transport, but wash away for 10μm wires because of crossover to diffuse transport. (From Sandia National Laboratory.)
Quantum Mechanics and the Band Theory of Solids
for a ballistic system we assumed a total absence of any scattering between the different 1D subbands. This allowed us to make a definite association between the direction of the carriers in the wire and the reservoirs from which they originated (see Figure 3.139). Such a distinction is no longer possible in the case where scattering occurs in the wire because electrons traveling in any particular direction may have originated from either reservoir. To compute the current that flows through such a disordered conductor, we now consider the probability that an electron incident in a given channel in one lead is transmitted into the other lead. Because of scattering in the sample an electron incident in some particular channel in the input lead will be transmitted into the different channels of the output lead with different probabilities. In the case in which a channel
is not perfectly conducting, e.g., there is some type of barrier in the channel, the conductance of that channel is then given by the quantum conductance times the electron transmission probability at the Fermi energy Tn(EF) through the barrier in that channel: S
2e 2 Tn (E F ) h
(3.272)
where Tn(EF) is given as: N
Tn (E F )
¤T
nm
(E F )
(3.273)
m 1
Here Tnm is the probability that an electron incident in mode n is transmitted into mode m in the output lead and the summation runs over the number (N) of occupied modes in the leads. Therefore, the probability Tn(EF) provides a measure of the degree of disorder in the conductor. This leads us to the socalled Landauer (1927–1999) formula, wherein the total current flow through the conductor is just the sum over all the occupied channels, which leads to the following expression for the conductance: S
187
J 2e 2 V h
N
¤ Tn n 1
2e 2 T h
(3.274)
NO SCATTERING
WITH SCATTERING
FIGURE 3.139 When there is no scattering in the wire, states are filled to higher energies in one direction than in the other.
where T is the total transmission coefficient of the conductor. A simple application of the Landauer formula is the problem of the ballistic quantum point contact that we considered earlier. In this case, each channel is perfectly transmitted, and the sum over the transmission probabilities in Equation 3.274 is replaced by the total number of channels M(EF); therefore, we recover the usual quantization condition given by Equation 3.270: S
2e 2 M(E F ) h
(3.270)
So we sum over the contributions of each subband and for perfect transmission of all the subbands T(EF) = M(EF) (which was 14 in Figure 3.138). When scattering is possible, however, the transmission coefficients Tn will no longer be equal to unity, and so the conductance quantization will not be observed. The Landauer equation can also be written in terms of transmission and reflection coefficients.
188
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Based on Equation 3.274, the resistance of a onechannel system [M(EF) = 1] can be rewritten as: Resistance (E F )
h 1 h ¨ 1 T(E F ) · ©1+ T(E ) ¸ 2 2e T(E F ) 2e 2 ª F ¹ h h R(E F ) 2 2 2e 2e T(E F )
quantized contact resistance scattering from barriers (3.275) inside channel where R(EF) = 1 − T(EF) is the reflection coefficient, and T(EF) + R(EF) = 1. Therefore, the resistance of the quantum wire is the sum of the quantized contact resistance and a second term, as a result of scattering from barriers in the channel. It is the latter term that is zero for a perfect conductor. At finite temperatures a thermal smearing out of the conductance staircase is observed because the FermiDirac energy distribution of electrons in the left and right leads must now be taken into account. This smearing out effect is observed in Figure 3.140, where the conductance voltage plots for the same type of quantum wires of Figure 3.138 are shown at 0.3 K, 0.6 K, 1.6 K, and 4.2 K. At the highest temperatures the staircase profile is almost lost as transport becomes more and more incoherent because of dephasing, resulting from inelastic scattering, phonons, etc. Quantum Dot: λ DB > L1, 2, 3 Quantization In quantum dots (QDs), generally consisting of 103 to 105 atoms and ranging from nanometers to tens of nanometers in size, dimensions are
CONDUCTANCE (2e2/h)
5 4 4.2 K 1.6 K
3 2
0.6 K
1
0.3 K
0
E n1 ,n 2 ,n3
h 2 ¥ n12 n 22 n 32 ´ 8m*e ¦§ L21 L22 L23 µ¶
(3.276)
where the quantum numbers n1, n2, and n3, each assuming the integral values 1, 2, 3,…, characterize quantization along the x, y, and zaxes, respectively. When considering the density of states for a zerodimensional (0D) electron gas, no free motion is possible: there is no kspace to be filled with electrons, and all available states exist only at discrete energies. Because carriers cannot move there is no ¥ ; 2k 2 ´ kinetic energy term ¦ here, only the quantized § 2m*e µ¶ energy terms survive. In Figure 3.142 we show the band structure and the density of states for a quantum dot. Quantum dots exhibit mesoscopic phenomena that are not observed in “simple” atoms. Mesoscale describes structures and behaviors at lengths between nanometers and 0.1 micrometers—too large for molecular or atomic characterization methods but too small to be fully characterized by their bulk behavior or to be modeled using continuum models. Phenomena at that scale, however, determine the properties of many scientifically and commercially important materials. Fermi Surfaces and Brillouin Zone for Quantum Dots There is no Fermi surface for quantum dots
0 0 0
smaller than the de Broglie wavelength of thermal electrons in all three directions (L1, L2, L3 < λDB). A quantum dot was first illustrated in Figure 3.67 and, simplified, is reproduced in Figure 3.141. Charge carriers in these “artificial atoms” are dimensionally confined in three directions (zero degrees of freedom), just like in an atom, and similarly have only discrete energy levels. The energy levels for an electron in a quantum dot are based on Equation 3.160, where we introduce the effective electron * mass me and, for generality, make the dimensions L1 # L2 # L3, to obtain:
–2.0
–1.6 –1.8 GATE VOLTAGE (V)
FIGURE 3.140 Conductance in number of units of 2e2 /h as a function of gate voltage (V) and at different temperatures. Same quantum wires as studied in Figure 3.138.
y x z
FIGURE 3.141 A cubic quantum dot.
Quantum Mechanics and the Band Theory of Solids
E
E
(2,1,1) (1,2,1) (1,1,2) Atomiclike levels: Artiﬁcial atoms
(1,1,1)
G(E)
(nx,ny,nz)
FIGURE 3.142 Energy levels and DOS of a quantum dot.4
because electrons are confined in all three directions (L1, L2, L3 < λDB) and cannot freely move. It is important to figure out for different solids at what length scale charge carriers become frozen in fixed energy states. The Fermi wavelength is a most important parameter for this as it tells us how finely a solid needs to be structured to have an impact on its electronic properties. The size of an electron in a solid is essentially its Fermi wavelength, λF = 2π/k F, with k F given by (3nπ2)1/3 (Equation 3.238), where n is the electron density. In most metals the electron density is very large (n > 1021 cm−3), and the value of the Fermi wavelength is consequently of the order of a few nanometers. In semiconductors, however, the lower carrier density (n < 1021 cm−3) gives rise to larger electron wavelengths of several tens of nanometers (see also Table 3.12). Therefore, confinement and quantization phenomena are visible in semiconductors already at dimensions greater than 200 nm, whereas in metals they typically are seen at 1–2 nm. This is one important reason why quantum effects have been observed mainly in semiconductor nanostructures, which have large Fermi wavelengths, rather than in metals, which have Fermi wavelengths comparable with a few crystal lattice periods only. We can also approach the difference in quantization effects between a metal and semiconductor nanoparticle from the point of view of the separation between adjacent energy levels. The average level spacing at the Fermi level between subsequent levels in a metal can be estimated from: $E n 1 n
1 2E F G(E)3D (E E F ) 3n 3D
(3.237)
189
For a spherical Au nanoparticle with a radius R = 2 nm, the average level spacing ΔE = En+1 − En is 2 meV only. In contrast, we calculate the energy separation between adjacent levels for a 2nm CdSe particle as 0.76 eV (see Volume III, Chapter 3). So obviously energylevel quantization is far more pronounced in semiconductor dots than in metal dots. Beyond the Fermi wavelength difference (or electron density difference) there are other reasons why semiconductors show quantum effects at a larger length scale: first, the energy level spacing—the energy difference En+1 − En—increases for lowlying states in a 3D potential well; second, the effective mass for electrons is smaller in semiconductors than in metals, and according to Equation 3.235 this also decreases the effective electron density n; and, third, the appearance of the plasmon oscillations of metal particles, described in Chapter 5 on photonics, often obscures quantization effects in metals. A Brillouin zone describes a material’s periodicity and is not defined for a quantum dot. Density of States Function for Quantum Dots Because band structure is no longer a term that has any relevance in a quantum dot, one describes the density of states for 0D (0 degrees of freedom) with a summation of delta functions δ(E) (sharp DOS peaks): G(E)0D 2¤ D(E E n )
(3.277)
n
where 2 is for the spin degeneracy. Such discrete atomlike densities of states are illustrated in Figure 3.143. The solid black curve is that of an electron in a large 3D semiconductor. As we just saw above, the relative importance of the quantum effect in a given system is determined
G0D(E) E
E112 E111 Eg x, y, z Eg
E E111 En1m
FIGURE 3.143 The density of states function for a quantum dot. The solid black curve is that of a free electron (see also Figure 3.119, full line), for example, in selforganized IIIV quantum dots (e.g., InAs/GaAs).
190
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
by the energy differences between the energy levels: ΔE = En+1 − En. Quantum size effects are only observable when this energy separation is larger than the thermal energy of the carriers (kT), so that adjacent subbands (e.g., the E111 and E112 levels in Figure 3.143) are differently populated. Electronic Conductivity of Quantum Dots To illustrate conduction through a quantum dot we introduce a type of quantum dot that is made by the electrostatic confinement of a 2D electron gas through a set of electrodes whose voltage can be varied at will. The specific example shown in Figure 3.144 is that of a lateral quantum dot (Figure 3.144a) made by applying a voltage on a set of gate electrodes (Figure 3.144b) to deplete the electrons in the underlying Al0.3Ga0.7As layer and thereby defining the lateral size of a quantum dot in the 2D electron gas at the Al0.3Ga0.7As/ GaAs heterojunction (Figure 3.144c). The potential well forms as a result of charge transfer between the (a)
Electrons travel in subsurface layer: Contact
Gate
Contact
two materials and their conduction band offset (Ec), and it confines the electrons so that the motion of electrons perpendicular to the plane of the heterointerface is quantized. The gate electrodes then further confine this 2D gas in the lateral direction to make a quantum dot (3D confinement). Any movement of electrons through a quantum dot requires the number of electrons in the dot to change one at a time. The Coulomb repulsion between electrons in the dot means that the energy of a dot containing N + 1 electrons is higher than one containing N electrons. This in turn requires extra energy to add an electron to the dot, and no current flows until increasing the voltage provides this energy. This is known as the Coulomb blockade. To better visualize the electronic transport through a quantum dot, consider a classical capacitor and compare it with a quantum dot between contact pins (Figure 3.145a). In the case of the macroscopic capacitor, the charge on the plates is given as Q = CV and the displacement current as I(t) = dQ/dt, and no charge can flow through this capacitor because the dielectric is an insulator. The electrostatic energy in the capacitor is then given as: d
GaAs
E
° V(t)I(t)dt 0
I (pA)
Ec = e2/2C
(c) + ++ ++ +++ + ++
Fermi energy
Doping layer Surface Al0.3Ga0.7As
GaAs
(3.278)
In the case of a quantum particle contacted by two measuring electrodes, one can envision that the contact points form a capacitor on either side of the quantum dot; if an electron is transferred by tunneling across these capacitors (Figure 3.145a), its Coulomb energy is changed by:
Negative voltage on gates depletes underlying electrons & deﬁnes dot cavity
(b)
Q2 2C
Only lowest subband occupied at low T
FIGURE 3.144 Electrostatically confined quantum dot in a 2D electron gas. (a) physical configuration. (b) gate electrodes and contacts. (c) energy diagram.
(3.279)
where it is assumed that the capacitors on either side of the quantum dot are identical. To ensure that thermal motion does not initiate a charge flow and an accompanying change in Ec, kT should be much smaller than the Coulomb blockade (kT kT) it reduces to: 2
¥ hN ´ ¥ hN ´ C v 3R ¦ µ exp ¦ § kT ¶ § kT µ¶
At low temperature the exponential term becomes dominant and controls the temperature variation of Cv. An exponential decay of Cv agrees with experimental data, except at very low temperatures, where Cv is proportional to T 3. Debye’s Heat Capacity Equation Debye retained the quantization of the atom oscillator energies introduced by Einstein but regarded them as coupled, where 3N modes now belong to the whole system rather than the N single atoms. In this model, because of the interconnections between atoms in a solid, the displacement of one or more atoms from their equilibrium positions gives rise to a set of mechanical waves propagating through the material. The amplitude of these “solid” waves is given by the displacements of the atoms from their equilibrium positions. The general Debye expression is:
¥ T´ C v 9R ¦ µ § QD ¶
QD 3 T
° 0
e4 x 4 ¥Q ´ dx 9RFD ¦ D µ (3.330) 2 x § T¶ (e 1)
where x = hν/kT and x max = hνD/kT and kθD = hνD with θD the Debye temperature. At high temperatures this expression again leads to DulongPetit, i.e., Cv = 3R, and at low temperatures (T θD, and for T > θD, Cv,lat is a constant, and at T 800°C) operation performed on semi
conductor wafers in an inert ambient. The heat treatment causes motion of dopant atoms in the direction of the concentration gradient (diffusion) and is used to drive dopant atoms deeper into the semiconductor. The dopants introduced in the substrate by a predeposition step are redistributed deeper into the substrate by such a drivein step. A twostep diffusion sequence is commonly used to form an np junction; during predeposition, a diffusion layer is formed under a constant surface concentration condition, which is followed by a drivein diffusion, or redistribution, under a constant total dopant condition. For most practical cases, the diffusion length (Dt)1/2 for the predeposition diffusion is much smaller than that for the drivein condition. Hence the predeposition profile can be treated as a delta function at the surface. This twostep junction formation is illustrated in Figure 4.24 with a predeposition from a constant source (erfc) and a limited source diffusion (Gaussian). The D in the above equations is the dopant diffusivity and is given by:
D D0 ( T0 )exp(
Surface concentration depends on temperature Increasing time Nx Distance from surface, x Boron source
Surface concentration decreases with time
Increasing time Nx Distance from surface, x O2 + N2
Drivein Impurity concentration, N(x)
Impurity concentration, N(x)
Predeposition
(4.29)
where Ea is the activation energy, whose value depends on the transport mechanism of the dopant
Ea ) kT
p+
p+
n
n
FIGURE 4.23 Normalized concentration versus normalized distance for the erfc and Gaussian functions. (a) Linear plot. (b) Semilog plot.
Predeposition
Drivein
FIGURE 4.24 Twostep junction formation with a predeposition from a constant source and a limited source diffusion.
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 4.3 Typical Values for D0 and Ea for Commonly Used Dopant Atoms D0 (cm2/s)
Element B Al Ga In P As Sb
Ea (eV)
10.5 8.00 3.60 16.5 10.5 0.32 5.60
3.69 3.47 3.51 3.90 3.69 3.56 3.95
Impurity concentration, n(x)
atoms. The diffusion coefficient, D0, is only a constant for a given reaction and concentration. In Table 4.3, typical values for D0 and Ea are given for commonly used dopant atoms. Dopant atoms take on several different ionization states and diffuse by several different mechanisms. The effective diffusion coefficient is the sum of the diffusivities of each species, which are in turn a function of temperature and dopant concentration. Hence, actual dopant concentration profiles deviate from the simple firstorder functions given above. The dopant diffusivities of phosphorus, arsenic, and boron in silicon at 1100°C are typically 2 × 10 –13, 1 × 10 –13, and 1 × 10 –13 cm2/s, respectively. Below the intrinsic carrier concentration (∼5 × 1018 cm–3 for Si at 1000°C), D is independent of the carrier concentration. Above the intrinsic concentration, the diffusion increases with carrier concentration and generally follows a power law as a result of the diffusion mechanism becoming point defect (vacancies and interstitials) assisted.
NS
ntype Gaussian proﬁle
ptype background concentration
NB
The point at which the diffused impurity profile intersects the background concentration is the metallurgical junction depth, xj. At that depth, the net impurity concentration is zero. In the case of a complementary error function, the depth is defined as: ¥N ´ x j 2 Dt erfc 1 ¦ B µ § NS ¶
¥N ´ x j 2 Dt ln ¦ s µ § NB ¶
(4.31)
The latter case is illustrated in Figure 4.25, where we show the diffusion of an ntype impurity in a ptype Si background substrate. It is important to remember that the concentration profile of the dopant in the semiconductor never changes abruptly (this would imply a zero or infinite flux), so diffusion always spreads impurities gradually around the edges of any mask. Lateral diffusion is ∼85% of the junction depth. This lateral diffusion continues every time the wafer is heated, resulting in an expanding die area. Besides lateral diffusion, diffusion doping also suffers from surface contamination interference, poor doping control, dislocation generation, and difficulty in creating ultrathin junction depths. Next, we will see that for each generation of IC technology, the trend has been to reduce the junction depth, which favors ion implantation (see comparison Table 4.4). NS – NB
ntype region NB ptype xj
xj (a)
(4.30)
When dealing with a Gaussian distribution, one obtains:
Net Impurity concentration, n(x)
232
Distance from surface, x
(b)
Distance from surface, x
FIGURE 4.25 Diffusion of ntype impurity into a ptype Si background substrate. Determination of xj in case of a Gaussian dopant distribution. Two representations are shown. In (a), the yaxis represents the impurity concentration; in (b), the yaxis represents the net impurity concentration (i.e., corrected for the background impurity concentration N B).
Silicon Single Crystal Is Still King
233
TABLE 4.4 Comparison of Thermal Diffusion and Ion Implantation Ion Implantation and Annealing Advantages Room temperature mask Precise dose control (1011–1016/cm2)
Solid/GasPhase Diffusion No damage created by doping Batch fabrication Cheaper
Accurate depth control Disadvantages Implant damage enhances diffusion Dislocations caused by damage may cause junction leakage Implant channeling may affect profile
Usually limited to solid solubility Low surface concentration hard to reach without a long drivein Low dose predeposition very difficult to achieve
Very expensive
Si Doping by Ion Implantation Ion implantation is the introduction of selected impurities (dopants) by means of highvoltage ion bombardment to achieve desired electronic properties in defined areas. Photolithography is used to mask the regions of the device where doping is not desired. For masking materials, most films used in the IC process can be used in the ionimplantation process—photoresists, SiO2, Si 3N4, metal film, etc.— in contrast with diffusion, where choices are much more limited. High energy ion beam implantation is a lowtemperature physical process and offers the advantage of being able to place ions at various depths in the sample, independent of the thermodynamics of diffusion and problems with solid solubility and precipitation. Ion implantation for doping was invented by Shockley in 1954. The technique is now very commonly used, with penetration depths in silicon of As, P, and B typically being 0.5, 1, and 2 μm at 1000 keV. A large range of extremely accurate doses is accessible: from 1011 to 1016/cm 2, and even buried (or retrograde) dopant profiles are possible. Unfortunately, however, ion beams produce crystal damage because the implant energy—between 30 and 100 keV—is thousands of times the silicon bond energy. Crystal damage can reduce electrical conductivity, but fortunately most of the damage can be eliminated by annealing at 700–1000°C, which is below the diffusion temperature. The anneal temperature is high enough for Si interstitial atoms to recombine with vacant
lattice sites and for the dopant atoms to move to substitutional lattice sites where they are electrically active. The combination of excellent spatial and dose control, as well as ease of manufacture, has led to widespread use of ion implantation. For the newest and future generation of complementary metal oxide silicon (CMOS) devices, which require highly doped, abrupt, and very shallow profiles (junction depths less than 30 nm!), the dopant diffusion step during annealing must be minimized. A beam of energetic ions implants charged dopant atoms into the silicon substrate. The acceleration energy and the beam current control the implantation depth and dopant concentration. The implanted dopant atoms enter unmasked regions in the silicon lattice at high velocity. The stopping mechanism of the ions involves nuclear collisions at low energy and electronic interactions at high energy. The acronyms associated with ion implantation include: ◾ Projected range, Rp: average distance traveled by ions parallel to the beam ◾ Projected straggle, Δ Rp: standard deviation or fluctuation in the projected range ◾ Lateral straggle, Δ R//: standard deviation or fluctuation in the final rest position, perpendicular to the beam (also called transverse straggle) ◾ Peak concentration, Np: concentration of implanted ions at Rp
234
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
In the absence of crystal orientation effects, the concentration profile, to a firstorder approximation, is Gaussian: 2 ¨ · 1 ¥ x Rp ´ ¸ © Ni ( x) N p exp ¦ © 2 § $R p µ¶ ¸ ª ¹
(4.32)
The range, Rp, is determined by the acceleration energy, the ion mass, and the stopping power of the material. Heavy ions do not travel as far into the crystal as light ions. They have a more narrow distribution (ΔRp) than light ions. The crystalline symmetry of the silicon lattice can have a dramatic impact on the implant profile. Once an ion enters a lattice channel, the small angle scattering events on the channel walls translate to ion penetration for a long distance before electron drag or a sharp collision stops the ion. Orientation of the substrate surface away from the plane perpendicular to the beam (tilt of 3–7°) prevents channeling, which can occur along crystal planes, ensuring better reproducibility of Rp. Ion channeling leads to an exponential tail in the concentration versus depth profile. This tail results from the crystal lattice and is not observed in an amorphous material. Channeling may also be prevented by creating a damaged layer on the Si wafer surface or by depositing a surfaceblocking amorphous layer such as an oxide. The three methods to limit ion channeling are compared in Figure 4.26. The total implanted dose (ions/cm2), Qi, can be either calculated by integrating the charges per unit time (current i) arriving at the substrate over time or also by integrating Equation 4.32 over all of x: d
Q i ° idt ° Ni ( x)dx 2P $R p N p
(4.33)
0
Oxide
Technologies studied to make the very shallow junctions needed in the latest CMOS devices are ultralowtemperature processing and rapid thermal annealing. For deep diffusions (>1 μm), implantation is used to create a dose of dopants, and thermal diffusion is used to drive in the dopant. Diffusion is a cheaper and more simplistic method than ion implantation but can only be performed from the surface of the wafers. Dopants also diffuse unevenly and interact with each other, altering the diffusion rate. Ion implantation is more expensive and complex. Ion implantation, however, except for annealing, does not require high temperatures and allows for greater control of dopant concentration and profile. It is an anisotropic process and therefore does not spread the dopant implant as much as diffusion. This aids in the manufacture of selfaligned structures, which greatly improve the performance of MOS transistors. Ion beams can implant enough material to form new materials, for example, oxides and nitrides, some of which show improved wear and strength characteristics. Ion implanters may be purchased from Varian Semiconductor (http:// www.vsea.com) and Eaton Corporation (http:// www.eaton.com). This equipment is very expensive, and usually service providers are used instead. In Table 4.4 we compare thermal diffusion and ion implantation.
Band Diagram of an Extrinsic Semiconductor In this section we establish the band diagram and carrier density for extrinsic semiconductors. The conductivity σ (Ωm)−1 is an intrinsic characteristic of a material and is independent of geometry. In extrinsic semiconductors, negative and positive charge carriers may contribute to the conductivity. In Chapter 3 we saw that the conductivity is
Damage
FIGURE 4.26 How to prevent ion channeling during implantation.
Tilt
Silicon Single Crystal Is Still King
the product of the number of free charges and their mobility [for electrons (e−) the mobility in cm2V−1s −1 is symbolized as μe (see Equation 3.10)]: σ = μene
(3.10)
The positive charge carriers (h+) are called holes as they correspond to an absence of electrons, and μh is their mobility. When both the concentration of holes (p) and the concentration of electrons (n) are considered, the conductivity σ of a solid is given as: σ = 1/ρ = e(μen + μpp)
(4.34)
where e is the electron charge, n is the electron concentration, and p is the hole concentration. In the case of a metal, we saw that resistance increases with temperature because the number of carriers remains the same but scatters more at higher temperatures. In a semiconductor, the resistance decreases as the temperature increases because more free carriers are generated (n and p increases). A semiconductor is called ntype when eμnn dominates the conductivity, in which case the majority of carriers are electrons, and the semiconductor is ptype if eμpp dominates, in which case the majority carriers are holes. By adding a donor atom (energy ED) to an intrinsic semiconductor at T = 0 K, an extra electron is bound to the positive charge on the donor atom. When the donor, at higher temperatures, ionizes,
+4 Si
+4 Si
+4 Si
+5 As
the neutral donor concentration ND converts to positively charged ND+. The electron bound to the positive ion is in an energy state, ED = Eg − ΔE, where ΔE is the binding energy. An electron that moves onto an acceptor atom has energy EA and coverts a neutral acceptor concentration NA into a negatively charged NA−. In Figure 4.27, we show donor ions (ED) energetically close to the bottom of the conduction band (EC) and acceptor ions (EA) close to the top of the valence band (EV). To estimate the Bohr’s radius and the binding energy (ΔE) involved in the donor holding onto its electron, we use the simple Bohr model for the hydrogen atom that was introduced in Chapter 3 but adapt the pertinent parameters to describe an impurity atom in a crystal rather than a hydrogen atom in vacuum. In Chapter 3 we calculated the Bohr radius of the hydrogen atom using Equation 3.89 as: a0 =
+4 Si
; 2 4 PE 0 me e 2
(3.89)
0.53 Å
For the binding energy involved, we use Equation 3.91: $E = E n
me e 4 2
2 2 0
32; P E n
2
E0 n2
(3.91)
With the Bohr radius equal to 0.53 × 10−10 m and n = 1, we get a value of 13.6 eV = 21.8 × 10 –19 J for
+4 Si q
235
Conduction electron
+4 Si
+4 Si
+4 Si
+4 Si
+3 B
+4 Si Hole +q
+4 Si
+4 Si
+4 Si
+4 Si
EC
Donor ions
EC Ei
Ei EV
+4 Si
Acceptor
Donor
ED
+4 Si
Acceptor ions
EA EV
FIGURE 4.27 Donors and acceptors in the Si lattice and their position in an energy band diagram. Here Ei stands for the Fermi level of the intrinsic material.
236
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology E T>0 T>0
EF fFD 1
ntype Si
Conduction band (partially ﬁlled)
EC EC EV
Valence band (partially empty
0
EF EV
ED
EC EF EV
EA ptype Si
FIGURE 4.28 Band diagram for intrinsic and extrinsic Si compared. Black is filled with electrons, and gray is empty.
the energy required to remove an electron from a hydrogen atom (see also Figure 3.36). For a typical solid, we saw in Chapter 3 one must replace me with the electron effective mass m*e ∼ 0.15 me and εr of 1 in the case of hydrogen with εr ∼ 15 for a typical semiconductor so that a 53Å Bohr radius is obtained from: a0 =
0.53 s E r * e
m /me
0.53 s 15 53 Å 0.15
(4.35)
and 9 meV is calculated for the binding energy of the electron to the donor atom from: *
$E
13.6 me 13.6 eV s 0.15 9 meV 2 (15)2 E r me
(4.36)
The ionization energy of the donor tells us how far below the conduction band the donor energy level is situated (ΔE = EC − ED). A similar calculation provides us with the distance above the valence band edge of the acceptor levels in a ptype material. This Bohrlike doping model assumes no interaction between dopant sites, i.e., a nondegenerate semiconductor. At T = 0 K, all electrons are in the lowest available energy states, and no electrons are excited from donor states (ND) into the conduction band (n = 0), but with a low binding energy of 9 meV at room temperature (kT ∼ 25 meV > ΔE = EC − ED) all of the donors will be ionized (ND+), and the number of free electrons in the conduction band n is given by: n ND ^ ND
(4.37)
This is the relevant regime for most electronics; note that the density of electrons is independent of temperature. Electrons do freeze out (i.e., return to
the valence band) if kT becomes too small to overcome the binding energy. From Equation 4.14 we calculate that: ¥N ´ E F E c k B T ln ¦ C µ § n ¶
(4.38)
where NC = 2.8 × 1019 cm−3 and n ∼ ND ∼1017 cm−3; we can see that the Fermi level is about 150 meV below the conduction band (∼6 kT). This situation is sketched in the middle panel of Figure 4.28, where we compare intrinsic silicon with ntype and ptype Si. Analogously, from Equation 4.15 we derive: ¥N ´ E F E v k B T ln ¦ v µ § p ¶
(4.39)
Some typical values for energy levels of impurities in Si are listed in Table 4.5. The Bohrlike doping model assumes no interaction between dopant sites; if adjacent dopant atoms are within 2 Bohr radii, then orbits overlap, and we are dealing with a degenerate semiconductor. This happens when ND (∼n) ∼ Nc or when NA (∼p) ∼ Nv. The degenerate semiconductor is then defined by EF ∼/> EC or EF ∼/< Ev. In these cases, the Fermi level is situated either inside the conduction or the valence band. TABLE 4.5 Some Typical Impurity Levels in Si Phosphorous, P Arsenic, As Boron, B Aluminum, Al Gallium, Ga Gold, Au
EC − ED = 44 meV EC − ED = 49 meV EA − EV = 45 meV EA − EV = 57 meV EA − EV = 65 meV EA − EV = 584 meV EC − ED = 774 meV
Silicon Single Crystal Is Still King
Oxidation of Silicon Oxidation Kinetics of SiSilica Is One of the Keys to Silicon’s Success Silicon owes a lot of its success to its stable oxide. By contrast, germanium’s oxide is soluble in water, and GaAs produces only leaky oxides. In IC design, silicon oxides, like other dielectrics, function as insulation between conducting layers, as diffusion and ion masks, as capping layers of doped oxides to prevent the loss of dopants, for gettering impurities, and for passivation to protect devices from impurities, moisture, and scratches. Doped oxides also act as a solidstate source of ions that can be diffused into a substrate at high temperatures. In micromachining, silicon oxides serve the same purposes but also very often act as sacrificial material. The stability and ease of formation of SiO2 on a Si surface was one of the reasons that Si replaced Ge as the semiconductor of choice in the late 1960s. Silica is the distinguishing feature of silicon versus other important semiconductor materials (see Table 4.6). Silica is inert to most chemicals, protects the Si surface, and forms a reasonably good diffusion barrier (although Si3N4 is much better in this respect). It is thermally stable up to 1600°C (Tm is 1830°C), easy to grow, and easy to pattern and etch selectively. In wet etching, HF preferentially etches SiO2, not Si, and in dry etching it can easily be plasma etched in CHF3. The material also makes for an excellent dielectric (insulator) with a 9eV bandgap, a dielectric strength of 107 V/cm, and a resistivity ρ of 1015 Ωcm. Silicon dioxide growth involves the heating of a silicon wafer in a stream of steam or in wet or dry oxygen/nitrogen mixtures (Figure 4.29) at elevated temperatures (between 600°C and 1250°C) in a TABLE 4.6 The Question of GoodQuality Native Oxides on Semiconductors Semiconductor (Bandgap) Si (1.1 eV) Ge (0.7 eV) GaAs (1.4 eV) SiC (~2.2 eV) GaN (~3 eV) Diamond (5 eV)
Native Oxide Yes No No No No No
237
horizontal or vertical quartz furnace. Dry oxide grows more slowly, but the oxide layers are more uniform, and there are also relatively few defects at the oxidesilicon interface. Defects interfere with the proper operation of semiconductor devices, and because a dry oxide has especially low surface state charges, it forms an ideal thin dielectric for MOS transistors (30–100 Å; see below). In wet oxides, hydrogen atoms, liberated by the decomposition of the water molecules during oxidation, produce imperfections that degrade the oxide quality somewhat. A major advantage of wet oxides includes their faster growth rate, making them useful for thick layers of field oxides (>3000 Å; see below). Silicon readily oxidizes, even at room temperature, forming a thin native oxide approximately 20 Å thick. The high temperature aids diffusion of oxidant through the growing surface oxide layer to the interface to form thick oxides quickly: Si + 2H2O (gas) → SiO2 + H2 (wet oxidation) Reaction 4.1 Si + O2 (gas) → SiO2 (dry oxidation) Reaction 4.2 Another gasphase oxidation method of Si is the pyrogenic method (Figure 4.29). Besides oxygen and nitrogen, the gas also contains hydrogen, which generates ultrapure steam. In the oxidizing gas stream, one also may add 2% HCl or Cl2; this helps to remove (getter) impurities by volatizing any metal impurities (AuCl3 and CuCl2). Oxidation setups Dry oxidation O2 N2
Furnace
Furnace
Wet oxidation
O2 N2 D1 H2O
Pyrogenic oxidation
Heating mantle
Furnace O2 N2 H2
FIGURE 4.29 Oxidation setups.
238
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
SiO2
Xox
Silicon
Silicon
SiO2
XS = 0.46Xox
Original Si interface
FIGURE 4.30 Silicon thickness converted, XS. Oxidation by inward diffusion of oxidant through the growing oxide to the interface.
The ratio of silicon thickness converted (Figure 4.30), XS, to resulting oxide thickness, Xox , is proportional to their respective densities: X S = 0.46Xox
F1 (gas) = h(C* − Cox) F2 (oxide) = D(Cox − Ci)/xox
(4.41)
F3 (reaction) = k sCi (see Figure 4.31) At equilibrium F1 = F2 = F3, and this yields the concentration of oxidant at the interface oxide/silicon, Ci, as: (4.42) C i ( X ox , k s , D, PG ) Oxide Xox
CGas
Silicon
F1 = h(C* – Cox) C* = H PGas F2 = D(Cox – Ci) / Xox F3 = ks Ci
Cox F1
F2
dX ox C i k s dt N
(4.40)
When 10,000 Å of oxide has grown, 4,600 Å of Si will be consumed; in other words, the amount of silicon consumed is 46% of the final oxide thickness. This relationship is important for calculating step heights that form in silicon microstructures. Very good adhesion to Si leads to volume expansion upward, resulting in compressive stress in the SiO2 film. All gasphase oxidation processes involve three steps in series: gasphase transport of oxidant to the surface (F1), diffusion through the existing oxide (F2), and the oxidation reaction itself (F3). The fluxes are:
Gas
where Xox = oxide thickness kS = Si oxidation rate constant, which is a function of temperature, oxidant, crystal orientation, and doping D = oxidant diffusivity, which is a function of temperature and oxidant PG = partial pressure of the oxidant in the gas phase C* = equilibrium oxidant concentration in the oxide = HPG, with H being Henry’s law constant The oxide growth rate is given by:
Ci X F3
FIGURE 4.31 Fluxes in the silicon oxidation reaction.
(4.43)
where N stands for the number of molecules of oxidant per unit volume of oxide (2.2 × 1022 cm–3 for dry oxygen and 4.6 × 1022 cm−3 for wet oxidation). Solution of this differential equation in the Bruce DealAndy Grove model for oxidation (1965) yields:
X ox (t)
· A ¨¥ tT ´ ¸ ©¦ 1 2 ·
1 µ 2 ©§ A / 4B ¶ ¹ ¸ ª ¹
(4.44)
where A and B are rate constants: A = 2D(1/k s + 1/h) (units of μm) B = 2DC*/N (units of μm2/h—parabolic rate constant) τ = (X i2 + AX i)/B h = gasphase mass transport coefficient in terms of concentration in the solid C* = equilibrium oxidant concentration in the oxide = HPG, with H being Henry’s law constant X i = initial oxide thickness The reason that wet oxide growth is much faster than dry oxidation can be found in the value for C* in the rate constant B. In dry oxygen at 1000°C, C*(O2) = 5.2 × 1016 cm−3, whereas at the same temperature in wet oxygen C*(H2O) = 3.0 × 1019 cm−3 (three orders of magnitude larger). This more than compensates for the fact that the diffusion coefficient of oxygen in SiO2 is larger than that of water [D(O2) > D(H2O)]. This general relationship for silicon oxidation is illustrated in Figure 4.32. From this figure it can be seen that for thin oxides [short
Silicon Single Crystal Is Still King
10
X0 A/2
X0 =
1 2
X0
10–1 0.1
=
t+ B(
B (t + ) A
)
1
2
X0 + AX0 = B (t + )
10 t+
100
1000
A2 / 4B
FIGURE 4.32 Silicon dioxide thickness versus growth time.
oxidation times with (t + τ) > τ and t >> A2/4B), we deduce from Figure 4.32 that the process is diffusion limited, and a parabolic law results: X ox (t ) B(t T)
(4.46)
where B is the parabolic rate constant. From Figure 4.32 we also conclude that oxide thickness versus growth time is initially linear when the oxidation reaction at the surface dominates but parabolic when the diffusion to the oxide/silicon interface dominates. A, B, and τ are strong functions of temperature and the gas ambient (wet vs. dry) and weak functions of orientation and doping (both type and level). The oxidation rate is also influenced by the presence of halogen impurities or hydrogen in the oxidizing gas, the oxidizing gas pressure, and the use of a plasma or a photon flux during oxide growth. For X0 < 200 Å, the oxidation is always faster than that predicted by the DealGrove model, and empirical models are used to fit the data. Even the substrate cleaning method influences the oxide thickness in this regime. The DealGrove model is also limited to the 700–1300°C temperature range and to the 0.1–25 atm pressure range. Short of using an ellipsometer to determine the oxide thickness (see Volume III, Chapter 6 on metrology), the silicon oxide thickness color table (Table 4.7) comes in handy. This table also lists some typical applications for oxides of various thicknesses. Charts showing the final oxide thickness as a function of temperature, oxidizing environment, and time are widely available.
TABLE 4.7 Oxide Color Table and Applications of Thermal Oxides: Observed Perpendicularly under Daylight Fluorescent Lighting Color Gray
239
Thickness (Å)
Application
Up to 100
Tunneling oxides in EEPROM (flash memories) and gate oxides (around 30 Å in 180nm CMOS)
Tan Brown Blue
500 700 800
Dark violetred violet Light bluemetallic blue Green Yellow Gold with slight yellow orange Orangemelon
1000
2800
4600
6500
Pad oxides Masking oxides during implant, diffusion, etc. Field oxide for isolation (e.g., LOCOS)
1500
3000
4900
6800
Field oxide for isolation (e.g., LOCOS)
1800 2100 2200
3300 3700 4000
5200 5600 6000
7200 7500
2500
4400
6200
240
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Some new types of oxidation under investigation include the growth of thick oxides at high pressures and the growth of ultrathin oxides ( (111) > (311) > (511) > (100), corresponding to an increasing activation energy that incorporates a term for the bond density in the plane, as well as one for the bond orientation. As might be expected, steric hindrance results in higher activation energy.4 In anisotropic wet etching, as we will discover in Volume II, Chapter 4, the sequence of the etch rates
242
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
is mostly reversed compared with that of oxidation. For example, a (100) plane etches up to 100 times faster than a (111) plane. It has been postulated that the slow etching of a (111) Si plane relative to a (100) plane may be because of its more efficient oxidation, protecting it better against etching than a (100) plane.5 In this interpretation—etching being an electrochemical process—one assumes that anodic oxidation, just like thermal oxidation, will occur faster at a (111) Si surface. To our knowledge, no evidence to support this theory has been presented as of yet. Moreover, Seidel et al.6 pointed out that the huge anisotropy in wet etching of Si could not be credited to the number of bonds available on different Si planes, as that number barely differs by a factor of 2 (see Volume II, Chapter 4). From the numbers observed, such an explanation could be valid for the anisotropy in thermal oxidation. There is no agreement, however, about the exact mechanism, and an understanding of the orientation dependence of the oxidation rate is still lacking. It has been attributed at various times to the number of SiSi bonds available for reaction and the orientation of these bonds, the presence of surface steps, mechanical effects such as stress in the oxide film, and the attainment of maximum coherence across the Si/SiO2 interface.4 It should also be noted that the oxidation rate sequence depends on temperature and oxide thickness—one more reason to take any model with a grain of salt.4 In Si, ntype dopants (As and P) at high concentrations (n++) lead to increases in oxidation rate, particularly at low temperatures. It is found that B/A is affected but that B remains unaffected. HoPlummer explained this phenomenon by postulating that point defects (vacancies) are being consumed during the volume expansion that accompanies Si oxidation.7,8 The oxidation rate is changed much less in case of highly borondoped (p++) wafers. Whereas boron atoms are taken up by the oxide, P and As pile up at the Si/SiO2 interface.9 Oxidation is also influenced by stress. Etched substrates exhibiting shaped structures oxidize at different rates than planar wafers. Oxide layers formed on silicon are under compressive stress, even in the planar case, and these stresses can be much larger on curved surfaces because the volume expansion
is dimensionally confined. For example, oxidation occurring in a confined corner, in which volume expansion is more difficult, is different from oxidation of a flat surface. Retardation of oxidation is very strong for sharp corners, i.e., for r small or 1/r large (e.g., a factor of two retardation in some cases). Retardation is also more pronounced for lower temperatures, and there are virtually no corner effects observed for 1200°C. Interior (concave) corners show more pronounced retardation effects than exterior (convex) corners. It is important to include stress when simulating oxide growth in the LOCOS process (see above). Si oxidation modeling using ATHENA software predicts the oxide shape much better when stress is included as a parameter (http://www.silvaco.com/ tech_lib/simulationstandard/1997/aug/a3/a3.html). In Volume III, Chapter 10 we show how oxidation sharpening is used to make sharp Si needle tips for scanning tunneling microscopes (STMs) and atomic force microscopes (AFMs; Volume III, Figure 10.12).
Nonthermal Methods for Depositing SiO2 Films Thermal oxidation involving the consumption of a thin layer of the Si surface results in excellent adhesion and good electrical and mechanical properties. It is an excellent technique when available. However, the thermal oxidation described in the previous section is by no means the only method available to implement a SiO2 film. Two nonthermal SiO2 deposition methods include electrochemical oxidation of Si and chemical vapor deposition. Electrochemical oxidation of Si has been studied (see, e.g., Schmidt10 and Lewerenz11) but has not led to commercial usage. Even though these anodic oxides are pinhole free, they exhibit many interface states. Madou et al.12 investigated mechanisms for anodic oxidation of Si and the introduction of oxide “dopants” into these anodically formed oxides. Such oxide dopants can be used as a source for doping of the underlying Si at elevated temperatures. Further study material on silicon oxidation can be found in Fair13 and Katz.4 Silicon dioxide is frequently used as an insulator between two layers of metallization. In such cases, some form of deposited oxide must be used rather
Silicon Single Crystal Is Still King
than grown oxides. Deposited oxides can be produced by various reactions between gaseous silicon compounds and gaseous oxidizers. Deposited oxides tend to possess low densities and large numbers of defect sites, meaning they are not suitable for use as gate dielectrics for MOS transistors but are acceptable for use as insulating layers between multiple conductor layers or as protective overcoats. For deposition of oxides at lower temperatures, we will learn in much more detail in Volume II, Chapter 7 that one may use lowpressure chemical vapor deposition (LPCVD), such as in the following reaction: SiH4 + O2 → SiO2 + 2 H2: 450°C
Reaction 4.3
Another advantage, besides the lower temperature, is the fact that one can dope an LPCVD silicon oxide film easily to create, for example, a phosphosilicate glass (PSG): SiH4 + 7/2 O2 + 2 PH3 → SiO2: P + 5 H2O: 700°C Reaction 4.4 Phosphorusdoped glass, also called Pglass or PSG, and borophosphosilicate glasses (BPSGs) soften and flow at lower temperatures, enabling the smoothing of topography. They etch much faster than SiO2, which benefits their application as sacrificial material in surface micromachining (see Volume II, Chapter 7).
Properties of Thermally Grown SiO2 A film of thermal SiO2 performs excellently as a mask against diffusion of the common dopants in Si. The diffusion coefficient, D, of boron at 900°C in SiO2 is 2.2 × 10 –19 cm2/s compared with 4.4 × 10 –16 in Si. For phosphorus, D equals 9.3 × 10 –19 cm2/s compared with 7.7 × 10 –15 in Si (from the common Si dopants, only Ga diffuses fast through the oxide with D = 1.3 × 10 –13). For some other elements, SiO2 forms a poor diffusion barrier. The amorphous oxide has a more open structure than crystalline quartz—only 43% of the space is occupied (see Figure 4.34). Consequently, a wide variety of impurities (especially alkali ions such as Na+ and K+) can readily diffuse through amorphous SiO2. Diffusion through the open SiO2 structure happens especially fast when the oxide is hydrated. One
243
Oxygen O 2.27Å
1.60Å Si
O
Silicon O
O (a)
(b)
(c)
FIGURE 4.34 (a) Basic structural unit of silicon dioxide. (b) Twodimensional representation of a quartz crystal lattice. (c) Twodimensional representation of the amorphous structure of silicon dioxide.
of the reasons for the poor performance of silicon dioxidebased ionsensitive fieldeffect transistors (ISFETs) in aqueous solutions can be traced back to the simple observation that SiO2 in water almost behaves like a sponge for ions.14 This is why, in such devices, SiO2 is often topped off with the ionic barrier material Si3N4. The use of SiO2 as a diffusion mask often stems from convenience; SiO2 is easy to grow, whereas Si3N4 cannot be put directly onto Si without problems. The quality of silicon dioxide depends heavily on its growth method. Dry oxidation at high temperatures (between 900 and 1150°C) in pure oxygen produces a better quality oxide than steam oxidation. Such a thermal oxide is stoichiometric, has a high density, and is basically pinhole free. Wet oxidation in steam occurs much faster but produces a lesser quality oxide, with water causing a loosening effect on the SiO2, making it more prone to impurity diffusion. Both types of oxidation are carried out in a quartz tube. Oxide thicknesses of a few tenths of a micrometer are used most frequently, with 1–2 μm being the upper limit for conventional thermal oxides. Addition of chlorinecontaining chemicals during oxidation increases the dielectric breakdown strength and the rate of oxidation while also improving the threshold voltage of many electronic devices.15 However, too high concentrations of halogens at high temperatures can pit the silicon surface. The
244
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
influence of chlorine, hydrogen, and other gases on the SiO2 growth rate and the resulting interface and oxide quality has been a fertile research field, a short summary of which can be found in Fair.13 It should be noted that for the IC industry, the electronic quality of the Si/SiO2 interface is expressed through low concentrations of interface trap states, low fixed oxide surface charges, low bulk oxide trapped charges, and mobile charges (impurity ions such as Li+, Na+, K+) (Figure 4.35);16 the interface quality is of little consequence in micromachining. In micromachining, the oxide is used as a structural element, a sacrificial layer, or a dielectric in a passive device, applications where the interface quality rarely matters. One notable exception is the aforementioned micromachined ISFET, where the electronic properties of the gate oxide are key to its functioning; a perfect oxide and oxide/semiconductor interface hold as much importance in this case as it does in the IC industry. Because of molecular volume mismatch and thermal expansion differences, a thermal silicon oxide is compressed. The compressive stress depends on the total thickness of the silicon dioxide layer and can
reach hundreds of MPa. Oxide films thicker than 1 μm can cause bowing of the Si wafer. Wet oxidation relaxes the compressive stress while speeding up the SiO2 growth. In Table 4.8, we review some of the more significant properties of thermally grown SiO2. The oxide is characterized by a variety of means reviewed in Volume III, Chapter 6 on metrology. Electrical tests are conducted to establish the capacitance (CV) at high and low frequencies to calculate the interface density, to measure dielectric breakdown, and for electrical stressing (with temperature ramp). Optical tests are carried out for thickness and optical constant determination using color (see Table 4.7), inter ferometry (needs calibrated substrate), and ellipsometry. Physical tests for thickness, surface quality, etc. involve profilometry, AFM, and crosssections by scanning electron microscopy (SEM)/ transmission electron microscopy (TEM). Oxidation furnaces may be purchased from Thermcraft (http://www.thermcraftinc.com/profile. html) and Tystar (http://www.tystar.com) (which makes Tytan Horizontal Furnace Systems; http:// www.tystar.com/furnace.htm).
SiO2
Transition region O2
SiO2
SiOx
Interface trap (a) states (Nit ~ 1015/cm2)
Si Si
Excess Si Interface trapped charge Qit
O2 Na+
SiO2
Mobile ionic charge Qm Bulk odxide trapped charge Qot Distance (z)
Fixed oxide surface charge Qf
(b) Fixed oxide surface charges (Nf ~ 2 × 1011/cm2) for dry O2 at 1100°C treatment and Nf ~ 2 × 1011 for wet (H2O at 1100°C treatment)
SiO2 Na+
Na+
Na+ Na+
SiO2 Na+
Na+ Si
SiO2
(c) Mobile impurity ions (Li+, Na+, K+) (Nm < 1012 ions)
(d) Charges trapped in the bulk oxide (Not may be positive or negative)
Si
FIGURE 4.35 Location of oxide charges in thermally oxidized silicon structures as defined by Bruce Deal. Q f and Q it are much lower for (100) silicon than for (111).
Silicon Single Crystal Is Still King
TABLE 4.8 Properties of Thermal SiO2 Property
SiBased Electronic Devices
Value
Density (g/cm3)
Introduction
2.24−2.27 (dry) and 2.18−2.20 (wet) 3.8−3.9 2 × 106 (dry) and 3 × 106 (wet) ∼8 1000
Dielectric constant Dielectric strength (V/cm) Energy gap (eV) Etch rate in buffered HF (Å/min) Infrared absorption peak (μm) Melting point (°C) Molecular weight Molecules/cm3 Refractive index Resistivity at 25°C (Ωcm)
9.3 ∼1700 60.08 2.3 × 1022 1.46 3 × 1015 (dry) and 3−5 × 1015 (wet) 1.0 2−4 × 109 (compressive) 0.014
Specific heat (J/g°C) Stress in film on Si (dyne/cm2) Thermal conductivity (W/cm°C) Thermal linear expansion coefficient (°C−1)
245
5 × 10−7 (0.5 ppm/°C)
The End of the Line for SiO2? In the following sections we learn about the gate oxide thickness crisis. The projected gate oxide thickness for 70 nm CMOS of 10–15 Å results in large tunneling currents (see Chapter 3) through the oxide. It is a challenge to find a replacement for thermal silicon dioxide with comparable dielectric properties. Oxides with high dielectric constant εr >> 3.9 are most desirable. Possible SiO2 replacements developed at present are silicon oxynitride (SiOx Ny), Al2O3, Ta 2O5, and Hf and Zr silicates.
The following active electronic devices will be reviewed in this section: diodes, specialpurpose diodes [including lightemitting diodes (LEDs), photodiodes, solar cells, Zener diodes, avalanche diodes, and tunneling (Esaki) diodes], and two types of transistors (bipolar and MOSFET). Si and Ge are the two most common single elements that are used to make diodes. A compound semiconductor that is commonly used is GaAs, especially in the case of LEDs because of its large direct bandgap. We analyze in some detail the scaling issues involved in the further miniaturization of Si MOSFETs, and in this context we introduce strained Si, which expands the prospect of continued Si use. Fundamental limits to MOSFET downscaling include not only electromagnetic, quantum mechanical, and thermodynamic effects but also technical and economic (practical) considerations. In the current volume Chapters 3 and 5 on quantum mechanics, and photonics, respectively and in Volume III, Chapter 3 on nanotechnology, alternative device operating principles that exploit the quantization effects, rather than being hampered by them, are investigated. These approaches include quantum wells, quantum wires, quantum dots, resonant tunneling diodes and transistors, superlattices, and molecular electronics.
Diodes Many semiconductor devices are based on the properties of the junction between ptype and ntype semiconductors (Figure 4.36). Russell Kohl at Bell Labs V(x) V0
p
n
p
n x
(a)
d0 (b)
d0
Idiﬀ
Idrift (d)
(c)
FIGURE 4.36 (a) p and n semiconductor before majority carriers cross the junction. (b) Motions of majority charge carriers across the junction uncover two spacecharge layers associated with uncompensated donor ions (to the right of the plane) and acceptors ions (to the left). (c) Associated with the space charge is a contact potential difference V0, which acts to limit the flow of majority carriers. (d) The diffusion of majority carriers across the junction produces a diffusion current, Idiff. The small concentration of minority carriers on either side of the junction moves in the opposite direction of the majority carriers, giving rise to a drift current, Idrift. In an isolated junction, the diffusion current is compensated for by the drift current, with the result that the net current through the junction is zero.
246
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
invented the solidstate pn junction diode in 1940. This device, when exposed to light, produced a voltage of 0.5 V across the junction and represented a stepping stone to the invention of the transistor (see Chapter 1). In a diode pn junction, electrons from the ntype diffuse into the ptype and holes diffuse the other way until the charge transfer builds up a big enough potential difference to halt the diffusion. As typical for diffusion, carriers flow from where there are many to where there are few. This motion of the majority charge carriers across the junction causes two spacecharge layers to form associated with the uncompensated donor ions (to the right of the junction) and acceptors ions (to the left of the junction). The interface where the p and ntype materials meet is called the metallurgical junction (Figure 4.36a). The two spacecharge regions form a depletion zone that is free of mobile charge carriers, with the ionized donor and acceptor ions fixed in their lattice sites. This double layer of opposite net electric charges is also called a dipole layer or a sandwich. A depletion layer, d0, typically extends a few micrometers on either side of the junction (Figure 4.36b). Associated with the space charge is a contact potential difference V0, which acts to limit the flow of majority carriers with a selfinduced electric field (103–105 V/cm), opposing further diffusion (Figure 4.36c). The diffusion of majority carriers across the junction produces the diffusion current, Idiff. A small concentration of minority carriers on either side of the junction moves in the opposite direction of the majority carriers and gives rise to a drift current, Idrift (Figure 4.36d). The electrical field is driving this current, not a concentration gradient. In a junction in equilibrium, the drift current compensates for the diffusion current, resulting in a net zero current through the junction. Even though there is no net current, electrons flow across the junction; it is just that the rates of flow in each direction are equal; such equilibrium is called dynamic equilibrium. In a real pn junction, the boundaries of the depletion zones are not as sharp as shown in Figure 4.36, but the contact potential curve is smooth with no sharp corners. The contact potential or barrier voltage, according to the Boltzmann relation, is given as: kT p p V0 ln e pn
(4.48)
where pp = hole concentration in the ptype material pn = hole concentration in the ntype material The term kT/e (= V T) is the thermal voltage (∼26 mV at room temperature). With pp ≈ NA and pn ≈ ni2/ND, where ni is the intrinsic carrier concentration, the barrier voltage can be approximated as: V0
kT N A ND ln e n i2
(4.49)
where NA = concentration of immobile acceptors on the pside of the junction ND = immobile donors on the nside of the junction For Si at room temperature, V0 is typically around 0.67 V (with NA = 1017 cm−3 and ND = 1015 cm−3). A typical width of the junction with these numbers is about 4 μm, and the electrical field E in this case is about 60 kV/cm. The majority carriers in the depletion layer disappear through recombination in which electrons and hole pairs annihilate each other. When equilibrium is reached, a single Fermi level characterizes the pn junction (Figure 4.37). The above describes a pn junction in an equilibrium situation. Now, we consider what happens when we apply a bias, as shown in Figure 4.38. When the pside of a pn junction is connected to the + terminal of a voltage source, and the nside to the – terminal, the majority carriers are repelled by their respective terminals toward the junction. This is called forward bias, and with such a bias the depletion layer becomes narrower (dF), and most electrons can go across the junction (right to left flow of electrons makes a positive current left to right because positive current flow is opposite of EC EF
ntype electrons EF
EV
ptype pn regions in equilibrium
EC EF EV
–– +– – + ++–– – + ++––– + ++–– ++ Depletion zone
FIGURE 4.37 A single Fermi level characterizes the whole pn junction in equilibrium.
Silicon Single Crystal Is Still King
247
FIGURE 4.38 (a) The forwardbiased connection of a pn junction, showing the narrowed depletion (dF) and the larger forward current IF. (b) The reverse (back)biased connection, showing the widening depletion zone (dB) and the small reverse (back) current I B.
the negative electron flow) (Figure 4.38a). With the shrinking of the depletion layer, the energy required for charge carriers to cross the depletion region decreases exponentially. Therefore, as the applied voltage increases, current starts to flow across the junction. The barrier potential of the diode is the voltage at which appreciable current starts to flow through the diode. The barrier potential varies for different materials. When connected in the opposite direction, the barrier gets higher, and practically no current flows. This is called back bias or reverse bias. The depletion layer is very wide (dB) when the reverse bias is high (Figure 4.38b). Very few electrons get into the depletion layer from the neutral
parts of the diode. Only electrons “produced” inside the depletion layer will move through it. A small leakage current, also saturation current, flows under these reversebiased conditions. A typical currentvoltage plot (I–V) for a diode is shown in Figure 4.39. Mathematically, the forward current (IF), with diffusion dominating, is described by an exponential as a function of the voltage. The reverse “leakage” current (IB), where drift dominates, is almost constant over most of the reverse voltage range (negative potentials in Figure 4.39). Combined we obtain: I I0 (e
eV HkT
1)
+I
Forwardbiased curve
120 100
80
60
40
Junction voltage
20
+V
–V
Breakdown voltage
0.4
Leakage current
Reversebiased curve
–I
FIGURE 4.39 Typical diode currentvoltage curve.
0.8
1.2
1.6
(4.50)
248
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
This equation is referred to as the Shockley equation. In it, η is the emission coefficient for the diode, which is determined by the way the diode is constructed and somewhat varies with diode current. For a silicon diode, η is around 2 for low currents and goes down to about 1 at higher currents. The reverse current, I0, depends on the number of electrons per second that “appear” in the depletion layer, not on the voltage. Only the temperature and the bandgap have an influence on I0. The simple Shockley equation does not explain the sudden increase of the leakage current at voltages above the breakdown voltage. We will explain this effect further below when discussing Zener and avalanche diodes. One important use for diodes is to convert alternating current into direct (unidirectional) current in power supply circuits. Diodes are also useful in some logic devices, and we can make some types of digital logic circuits using only diodes and resistors.
SpecialPurpose Diodes Introduction There are many types of specialized diodes. In this section we briefly introduce lightemitting diodes (LEDs), solar cells, Zener diodes, avalanche diodes, and tunnel or Esaki diodes. In Chapter 5 we discuss doublebarrier resonant tunneling diodes (DBRTs) and compare laser diodes with quantum well lasers. The existence of the zero point energy for confined electrons in a quantum well laser (see Chapter 3) makes a quantum well laser much more efficient than a diode laser. In a quantum well, there are no allowed electron states at the very lowest energies. What that means is that the lowest conduction state in a quantum well is broad so that many electrons can be accommodated. Similarly, the top of the valence band has plenty of states available for holes. This means that it is possible for many holes and electrons to combine and produce photons with identical energy for enhanced probability of stimulated emission (lasing) (see Chapter 5). Peltier diodes are described in Volume III, Chapter 8 on actuators. LightEmitting Diodes Electrons and holes can recombine in extrinsic semiconductors that have a substantial number of
electrons in the conduction band and many holes in the valence band. On recombination, energy conservation requires that photons and/or phonons be produced. The only place where there are enough electrons and holes to produce bright light is at the pn junction when a large current is flowing (i.e., in a forwardbiased pn junction). If the bandgap corresponds to the energy of a photon of visible light, then that type of radiation is produced. This is the lightemitting diode (LED), used extensively in electronic devices and cars as indicator lamps, as picture elements in color matrix displays for laptop computers, and so on. Being an indirect bandgap material, Si is currently not used for LEDs, and the most utilized material is direct bandgap GaAs (see Chapter 5). The earliest LEDs produced infrared or visible red light, but LEDs in yellow, green, and blue visible light colors are now available (Figure 4.40). These LEDs convert electrical input to light output. Greater difference in energy levels in the p and nsides of the diode produces greater energy change, and consequently higherfrequency, shorterwavelength light. A forwardbiased pn junction, showing electrons being injected into the ntype material and holes into the ptype material, is sketched in Figure 4.41. Light is emitted from the narrow depletion zone each time an electron and a hole combine across that zone. The ratio of generated photons to the electrons injected across the junction is called the quantum efficiency, which is a key measure of how well a light emitter is working. For highperformance III–V LEDs, the efficiency is around 10%. GaAs is a direct energy gap semiconductor with an energy gap of 1.424 eV in the nearinfrared portion of the electromagnetic spectrum. This semiconductor is often used in LED construction in combination with AlAs, an indirect energy gap semiconductor with an energy gap of 2.168 eV in the yellowgreen portion of the electromagnetic spectrum. As the mole fraction x of Al x Ga1−x As is raised from zero, the energy gap of the resulting compound increases from that of GaAs to that of AlAs. When the value of x is 0.45, the semiconductor switches from a direct energy gap to an indirect energy gap. GaAs and AlAs differ in lattice constants by less than 0.2% at 250°C, which allows for
Silicon Single Crystal Is Still King
Silicon (Si)
Indium nitride Gallium (InN) Gallium phosphide arsenide (GaP) (GaAs)
Gallium nitride (GaN)
Infrared
0
Diamond (C)
249
Aluminum nitride (AlN)
Ultraviolet
1 eV
2 eV
3 eV
4 eV
5 eV
6 eV
Binding energy of electron
InGaN Blue LED InGaN Green LED
200 μm
FIGURE 4.40 LEDs of all colors: the larger the difference in energy levels in the p and nsides of a diode, the shorter the wavelength of the light.
the growth of very highquality AlGaAs films on GaAs substrates. Molecular beam epitaxy (MBE) is a crystalgrowth technique in which material is deposited by evaporating individually controlled source materials onto a heated substrate in an ultrahigh vacuum chamber. The growth rates in MBE are very slow (0.1–2 mm/h). MBE is capable of producing highquality AlGaAs heterostructure devices with very uniform thickness and doping characteristics. Crystal growth of LEDs by metalorganic chemical vapor deposition (MOCVD) and liquidphase epitaxy (LPE) began in the late 1960s. By using MOCVD, it is easier to scale up to larger growth areas than with LPE, and the uniformity and surface morphology of MOCVD grown lasers are superior (MBE, LPE, and MOCVD are compared in Volume II, Chapter 7). Hole current R p Light
+ n
Light
Electron current
FIGURE 4.41 A lightemitting diode (LED): forward based pn junction, showing electrons being injected into the ntype material and holes into the ptype material.
The absorption coefficient for direct and indirect bandgaps was calculated using Fermi’s golden 1 rule as A(W) t G(E) t (;W E g ) 2 (Equation 3.301) and A(W) t G(E) t (;W E g p ;Np )2 (Equation 3.302) (with νp the phonon frequency and + for absorption and – for emission), respectively. Emission in an indirect bandgap semiconductor (e.g., Si) is a threeparticle interaction (1 electron + 1 photon + 1 phonon); therefore, the transition is unlikely, and such materials are poor light emitters. In silicon, few excited electrons generate photons, and most recombinations result in heat rather than light; thus, the quantum efficiency is poor. In other words, silicon as an indirect bandgap is a lousy light emitter: the probability that a phonon with just the right amount of momentum will meet an electron/hole pair is not very good. The occurrence of such a photongenerating transition in a III–V material is thousands of times more likely than in silicon. As a consequence, until recently, most people in the semiconductor industry would assure you that silicon is pretty much worthless at turning electricity into light, and as we just saw, LEDs and lasers are made of the more exotic III–V semiconductors. But these materials, including gallium arsenide, gallium nitride, and indium phosphide, are anywhere from 30 to 200 times more expensive than silicon. Moreover, the manufacturing infrastructure and knowhow about
250
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
making ICs from silicon is useless for making chips from III–V semiconductors. To connect the manufacturing of microprocessors with that of LEDs and lasers, one would like to develop cheap, integrated optoelectronics with all components made from silicon. In Chapter 3, we saw that one approach to getting more light out of silicon involves quantum confinement, with electron/hole pairs physically restricted to a small volume, typically less than 30 nm 3, or 300 times the size of a typical atom. This can be accomplished, for example, by embedding nanocrystals of silicon in an insulating silicon dioxide shell. Within such a nanocrystal, the energy levels of the valence and conduction bands differ significantly from those in bulk crystals, and in general, the smaller the nanocrystal, the larger the bandgap (blue shift). The latter represents an example of tuning a device’s optical properties by bandgap engineering, which is achieved in this case by the fine control of the nanocrystal’s growth during the manufacturing process. It turns out that quantum confinement also reduces silicon’s momentum problem, thus increasing the probability that injected electrons will produce photons. In confined silicon nanostructures, one observes a blue shift for the bandgap absorption onset, and some forbidden transitions become feasible. In other words, through nanotechnology, Si might yet be made into a good candidate for LEDs and lasers after all (another approach to make Si a better photonic material is seeding the silicon with lanthanide rare earth element ions, which give off light when electrically excited). One important reason to use LEDs is that they last longer, are brighter, and are more efficient than incandescent lights. LED lamps use as little as 10% of the electricity that an incandescent light uses and have lifespans of 100,000 h, which is more than 11 years of continuous use. A laser diode is made by putting an LEDtype structure in a resonant cavity formed by polishing the parallel end faces of the semiconductor (see Chapter 5). Photons bounce between the reflective ends, colliding with atoms and stimulating the emission of additional photons that are in phase with the others in the region. In a laser, the concentrated, active region bounded by
the reflective ends is known as the resonant cavity. Laser diodes are used in optical storage devices and for highspeed optical communication. As we already alluded to in Chapter 3, they are less efficient than quantum well lasers because more electrons and holes can be accommodated in the latter devices. This means that it is possible for many more holes and electrons to combine and produce photons with identical energy for enhanced probability of stimulated emission (lasing). Photodiodes and Solar Cells The photodiode is the inverse of the lightemitting diode (LED). Rather than giving off light it is sensitive to incoming light. Photons of energy Eg or greater create electron/hole pairs in the junction region. The electrons and holes are then swept out of the junction region by the electric field that exists before they can recombine. Photodiodes can be operated in two different modes, namely, the photovoltaic mode and the photoconductive mode. In the photovoltaic mode, like in a solar cell, the illuminated photodiode generates a voltage. However, the dependence of this voltage on the light intensity is rather nonlinear, and the dynamic range is typically small. Although the maximum sensitivity is not achieved, the area of the junction is large, and enough electron/hole pairs are produced so that significant solar energy can be taken from the device. In the photoconductive mode, one applies a reverse voltage to the diode (i.e., a back bias) and measures the resulting photocurrent. The dependence of the photocurrent on the light power can be very linear over six or more orders of magnitude of the light power. This type of diode is very sensitive and is used in CD players. The electron/hole pairs created by light in a photodiode result in an additional component of current flowing in the diode: eV
I I0 (e kT 1) Ioptical
(4.51)
with the first term the usual diode equation (Equation 4.50), and the second term the photocurrent, Ioptical, which is proportional to the light intensity. Photodiodes are constructed so their pn junction can be exposed to incoming photons
Silicon Single Crystal Is Still King
through a clear window or lens. To increase the volume in which radiation can be absorbed, positive intrinsic negative (PIN) diodes are often used. A PIN diode has a central undoped, or intrinsic, layer, forming a ptype/intrinsic/ntype structure. An internal electric field is maintained over a wider layer with the benefit that the depletion region now exists almost completely within the intrinsic region, which is a constant width (or almost constant) regardless of the reverse bias applied to the diode. This intrinsic region can be made large, increasing the volume where electron/hole pairs can be generated. For these reasons many photodetectors are based on PIN diodes. In solar cells, photons coming from the sun excite electrons in the valence band and raise them to the conduction band. Illumination of a pn junction produces hole pairs that diffuse to the depletion region. The minority carriers (electrons in ptype material) are swept across the depletion region and increase the reverse current. In these cells one tries to maximize the minority carrier lifetime, τ, so that long diffusion lengths, L = (Dτ)1/2, in excess of 100 μm, can be attained. In a ptype material, electrons are the minority carriers, and the number of electrons generated per unit area per second (generation rate G) in a ptype material within a diffusion length of the depletion layer is given as GL. The larger G and L, the more electrons reach the edge of the depletion layer, where they are collected by sweeping
251
them across the depletion layer, resulting in a current, Ioptical (see Equation 4.51), which is given by: (4.52)
Ioptical eGL
With a reverse bias applied to the solar cell, Equation 4.52 represents the increase in current with light intensity as illustrated in Figure 4.42b. The current is biasindependent as long as L >> d, with d the depletion layer thickness. The depletion layer thickness is the only voltagedependent parameter. Under open circuit conditions, no current is measured, and I in Equation 4.50 is equal to zero. On illumination, an open circuit voltage, Voptical, appears across the np junction: Voptical
kT Ioptical ln e I0
(4.53)
This open circuit voltage counteracts the flow of optically generated carriers, and the junction potential (V0; see Equation 4.48) is lowered so that an equal and opposite flow of electrons from ntype to ptype is established. Research interest in solar cells today, with soaring oil prices, is very high. Solar energy reaching the surface of earth is about 800 W/m2. The current problem with solar cells is not really the efficiency (20%) but rather the cost of production. Although it has come down by a factor of 100 in 50 years, it still has a factor of 2–5 to go to down to
Builtin electric ﬁeld 1000 W/m2 Conduction band
Photon
ptype Carrier generation
2
Current in A
e–
600 W/m2 1
Fermi level
200 W/m2
Valence band ntype
0 0 (b)
0,1
0,2 0,3 Voltage in V
0,4
0,5
h+ (a)
FIGURE 4.42 Illumination of a pn junction produces hole pairs that diffuse to the depletion region. The minority carriers (electrons in ptype materials) are swept across the depletion region and increase the reverse current (a). The higher the illumination intensity the higher the reverse current (b).
252
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
be competitive with fossil plants. Another problem is that no energy can be produced at night, so energy storage is needed to provide continuous service. The highest efficiency solar cells are made of silicon single crystals. These are difficult to manufacture and are expensive. The most popular alternatives are polycrystalline and amorphous Si thin films, as well as GaAs and several of its alloys. The latter are sensitive to different parts of the solar spectrum because they have different bandgaps. We detail progress in MEMS and NEMS applied to solar cells, including liquid junctionbased solar cells (the Gräetzel cell), in Volume III, Chapter 9 on power and brains in miniature devices. Zener, Avalanche, and Tunnel (Esaki) Diodes In the breakdown region in the diode currentvoltage curve in Figure 4.39, the diode exhibits a sudden increase in current. This is called the Zener breakdown, named for Dr. Clarence Melvin Zener of Southern Illinois University, inventor of the device. The Zener diode works at strong negative bias. If the reverse voltage is high enough to raise the top of the valence band on the pside above the bottom of the conduction band on the nside, then valence electrons can directly tunnel into the conduction band, and there is a sudden breakdown of the resistance (Figure 4.43). Zener diodes are used to regulate voltage: they do not allow voltage to go beyond the Zener breakdown point. They are equipped with cooling fins to keep them from melting under high voltage and high current (high power). Zener diodes
pside
Vext
p
n
nside
FIGURE 4.43 Band diagram for Zener diode: the top of the valence band on the pside is above the bottom of the conduction band on the nside, and valence electrons can directly tunnel into the conduction band, causing a sudden breakdown of the resistance. Also shown is the use of a reversebiased pn diode for a voltage clamping circuit. The current saturates to a value determined by the external circuit resistor, while the output voltage is clamped at the diode breakdown voltage.
are mostly used to produce an accurate reference voltage for measurement devices or analogdigital converters, and so on. Manufacturers set a precise breakdown voltage by careful doping, allowing the diode to be used as a precision voltage reference. Some devices labeled as highvoltage Zener diodes are avalanche diodes. Avalanche diodes conduct in the reverse direction when the reversebiased voltage exceeds the breakdown voltage. Avalanche diodes are electrically very similar to Zener diodes and are often mistakenly called Zener diodes, but they break down by the avalanche effect. This occurs when the reverse electric field across the pn junction causes a wave of ionization, reminiscent of an avalanche, leading to a large current. In this region, the high electric field in the middle of the depletion layer accelerates electrons that are produced there (by action of heat or light) so much that they garner enough energy to “dislodge” electrons from the valence band into the conduction band. When one energetic electron can “dislodge” two or more such electrons, it starts a “chain reaction” in which these electrons can produce even more conduction electrons. Avalanche diodes are designed to break down at a welldefined reverse voltage without being destroyed. Avalanche diodes are sensitive to very low radiation because of the “multiplication” of current by the avalanche effect. The difference between the avalanche diode (which has a reverse breakdown above about 6.2 V) and the Zener diode is that the channel length of the former exceeds the “mean free path” of the electrons, which means there are collisions between them on the way out. The only practical difference is that the two types of diodes have temperature coefficients of opposite polarities. Yet another specialpurpose diode is the tunnel diode (or Esaki diode), which, like the Zener diode, exploits tunneling across a potential barrier. The tunnel diode has the unusual characteristic that the current decreases with the applied bias voltage. Because of this negative resistance region at low voltage and its rapid response, it is capable of amplification, oscillation, and switching in electronic circuits at high frequencies. The Esaki or tunnel diode is designed from very heavily doped n and p regions. The high doping ensures a very large
Silicon Single Crystal Is Still King
253
FIGURE 4.44 The tunnel or Esaki diode. For explanation, see text.
electric field in the junction so that bandtoband tunneling is possible at all biasing conditions (see Figure 4.44). The discovery of the Esaki diode was very significant as it was the first quantum mechanical electronic device where electron tunneling was clearly manifested in semiconductors, and it opened up a new field of research: tunneling in solids. Esaki described the tunnel diode in his thesis in 1957 and received the 1972 Nobel Prize for it. Shockley was so impressed by Esaki’s work that at a symposium of the International Union of Pure and Applied Physics in Brussels in 1958, he announced (Figure 4.45):
With reference to Figure 4.44, the operation of the Esaki diode is as follows. When applying a small forward bias, electrons on the nside of the diode tunnel into holes on the pside. As that bias is increased, the band alignment enables yet more electrons to find holes to tunnel into, and the current increases (A). Beyond the point (B), empty states on the pside move higher in energy with respect to the electron energies on the nside. Eventually, at point C, there are no empty states (holes) available
The most beautiful demonstration of the Zener effect so far achieved is presented at this symposium by L. Esaki of Tokyo. Esaki has studied pn junctions which are very heavily doped on both sides, so that there is a builtin field of the order of 5 × 105 volt/cm. Under these conditions, current flows by the Zener mechanism even at zero voltage. Esaki finds that as forward bias is increased across the junction, this possibility of direct tunneling disappears and, as a consequence, he observes a predictable negative resistance region.
The tunnel diode couples tunneling with clever energy band alignment to create negative differential resistance as illustrated in Figure 4.44.
FIGURE 4.45 W. Shockley (age 48 years) and L. Esaki (age 33 years) in 1958 in Brussels for the symposium of the International Union of Pure and Applied Physics. This coincided with the World Expo held there.
254
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
for electrons to tunnel into. This causes the current to decrease to a minimum value. Eventually, the current increases again because the electrons and holes are able to overcome the reduced barrier because of their thermal distribution.
Transistors Introduction An integrated circuit (IC) is an electronic network fabricated in a single piece of a semiconductor material. In IC fabrication, the semiconductor surface is subjected to various processing steps in which impurities and other materials are added with specific geometrical patterns. The fabrication steps are sequenced to form 3D regions that act as transistors and interconnects that form the switching or amplification network. In this section, we detail different types of transistors. Transistors are threeterminal devices, where the current or voltage at one terminal, the input terminal, controls the flow of current between the two remaining terminals. In Chapter 1 we saw how the name “transistor,” a name coined by John R. Pierce, a scientist from Bell Laboratories, is a contraction of the terms trans and resistor. This term was adopted because it best describes the operation of the transistor—the transfer of an input signal current from a lowresistance circuit to a highresistance circuit. Basically, the transistor is a solidstate device that amplifies by controlling the flow of current carriers through its semiconductor materials. Electronic devices made up of transistors are more interesting and have more applications than diodes. Two types of transistors are widely used: the bipolar junction transistor (BJT), which is physically like two junction diodes back to back, and the fieldeffect transistor (FET), in which one uses the voltage on a control (gate) electrode to control the shape and hence the conductivity of a channel of one type of charge carrier in a semiconductor material. Only weeks after the point contact transistor was conceived by Shockley, Bardeen, and Brittain (see Chapter 1), Shockley came up with the BJT in 1948. Bardeen was the physicist; Walter Brittain, the experimentalist; and William Shockley, who became involved later in the development, was the instigator
and idea man. The team won the 1956 Nobel Prize in physics for their efforts. The transistor demonstrated for the first time that amplification in solids was possible. The device was initially known simply as the junction transistor, and it did not become practical until the early 1950s. The term bipolar was tagged onto the name to clarify the fact that both carrier types play important roles in its operation. Historically the eldest, it was in use for many years for large integrated devices and high speed at the expense of low density and higher power consumption. The dominance of BJTs through the 1960s and 1970s was quickly overwhelmed by the simplicity of the metal–oxide–semiconductor fieldeffect transistor (MOSFET) (in terms of both circuit design and fabrication processes) in the 1980s. This is especially true in the very large scale integration (VLSI) era. In a MOSFET, power consumption is very low, and the current flow depends on the majority carriers only; thus, it is unipolar. The BJT’s high current drive capability and superior analog performance continue to drive applications, however, and a recent trend is to combine the best of MOSFETs and bipolar devices in bipolar CMOS (BiCMOS) processes. BiCMOS is a type of IC that uses both bipolar and CMOS technologies. The logic gates are primarily made of CMOS, but their output stages use BJTs. Bipolar transistors consume more current (and therefore dissipate more power) but switch faster (see Table 4.9). Bipolar Transistors The BJT structure contains two pn diodes: one between the base and the emitter, and one between the base and the collector. There are many different types of transistors, but the basic theory of their operation is all the same. The three elements of the twojunction transistor are 1) the EMITTER, which gives off, or emits, current carriers (electrons or holes); 2) the BASE, which controls the flow of current carriers; and 3) the COLLECTOR, which collects the current carriers (Figure 4.46). Early BJTs were fabricated using alloying—a complicated and unreliable process (Figure 4.46a). Figure 4.46a, also shows the symbol used for a BJT transistor. The “planar process,” developed by Fairchild in the late 1950s, shaped the basic structure of the BJT, which is still seen even up to the present day. In the planar
Silicon Single Crystal Is Still King
255
TABLE 4.9 Bipolar, CMOS, and BiCMOS Compared Bipolar
CMOS
BiCMOS
Better analog capability
Highperformance analog
High power dissipation
Lower static power dissipation
Generally better noise performance and better highfrequency characteristics Improved I/O speed (particularly significant with the growing importance of package limitations in highspeed systems) Low packing density
Higher noise margins
Lower input impedance (high drive current) Low delay sensitivity to load Low voltage swing logic Higher current drive per unit area, higher gain High transconductance g Essentially unidirectional Higher switching speed
Lower power dissipation than purely bipolar technology (simplifying packaging and board requirements)
Flexible I/Os technology is well suited for I/O intensive applications
Higher packing density Lower manufacturing cost per device High input impedance (low drive current) High delay sensitivity to load (fanout limitations) Scaleable threshold voltage VT Low output drive current (issue when driving large capacitive loads) Low transconductance g Bidirectional capability (drain and source are interchangeable) A near ideal switching device
process, all steps are performed from the surface of the wafer (Figure 4.46b). A forwardbiased pn junction is comparable to a lowresistance circuit element because it passes a high current at a given voltage. In turn, a reversebiased pn junction is comparable to a high
Improved speed over purely CMOS technology
resistance circuit element. By using the Ohm’s law formula for power (P = I2R) and assuming the current is held constant, it can be concluded that the power developed across a high resistance is greater than that developed across a low resistance. Thus, if a crystal were to contain two pn junctions (one
Collector
Physical structure Base
n Metal contact
p n
Schematic symbol
Emitter C
(b)
C
E
B
n+ p n+ p− substrate
B (a)
E
FIGURE 4.46 Bipolar npn transistor made by alloying a BJT symbol (a) and a BJT made in a planar process (b).
256
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
forwardbiased and the other reversebiased), a lowpower signal could be injected into the forwardbiased junction and produce a highpower signal at the reversebiased junction. In this manner, a power gain would be obtained across the crystal. This concept is the basic theory behind transistor amplification. MOSFETS The most common fieldeffect transistor (FET) in both digital and analog circuits is the MOSFET. Nomenclature is different here than for a bipolar transistor with the base replaced by a gate (G), the emitter by a source (S), and the collector by a drain (D) (see Figure 4.47). The physical structure shown here consists of a ptype Si substrate, n+ source, n+ drain, a gate oxide (SiO2), a polysilicon gate, a chemical vapor deposition (CVD) oxide, and a contact metal 1 (usually Al). Notice that the effective gate length is shorter than the one drawn in the mask layout (Leff < Ldrawn) as a result of lateral doping effects. Silicon is the main choice of semiconductor used in MOSFET manufacture, but SiGe is also used more and more by some manufacturers (see page 269). Some other semiconductors such as GaAs are not useful in MOSFET manufacture because they do not form good insulating gate oxides. A thin oxide layer between the gate (e.g., a PolySi or socalled poly gate) and the semiconductor characterizes the MOSFET. This high resistivity oxide layer (ρ > 1016 Ωcm) prevents current flow from the semiconductor to the gate. Siliconbased MOSFETs rely on the extremely highquality interface between SiO2, the standard gate dielectric, and silicon. Physical structure
To understand a MOSFET, it is essential to recall the metal oxide semiconductor (MOS) capacitor fundamentals. In an idealized MOS capacitor, without any applied voltage, the metal work function, ϕm, is equal to the semiconductor work function, ϕs. Therefore, the Fermi level of the semiconductor, EFS, is aligned with the Fermi level of the gate, EFm. As a consequence, there is no band bending in any region of the MOS capacitor. We also assume here that the oxide is free of any charges, and the semiconductor is uniformly doped. In the example MOS structure in Figure 4.48a, we use a ptype semiconductor with a negative gate bias applied. With this negative gate bias (VGB), the gate charge, QG , is negative. Because charge neutrality must be preserved, a net positive charge, QC , is generated in the silicon substrate to counterbalance the negative charge on the gate. This is achieved by an accumulation of majority carrier holes under the gate (because we are dealing with a ptype semiconductor, the majority carriers are holes). The condition, where the majority carrier concentration is greater near the SiSiO2 interface compared with the bulk concentration, is called accumulation. Under this applied negative gate bias, the Fermi level of the gate is raised with respect to the Fermi level of the substrate by an amount qVGB. The energy bands in the ptype semiconductor are bent upward, bringing the valence band closer to the Fermi level, which is indicative of a higher hole concentration at the semiconductor surface right under the dielectric. Because no current flows through the device due to the presence of the insulating oxide layer, the Fermi level in the substrate
Layout representation
Schematic representation
CVD oxide Metal 1
Poly gate Source
Drain
Ldrawn
n+
Ldrawn
n+ Leﬀective
G
Wdrawn
D
S B
Gate oxide (b)
(c)
psubstrate (bulk) (a)
FIGURE 4.47 A MOSFET with nomenclature (a). The geometry of the areas on the Si surface is known as the layout of the chip (b). Schematic representation of a MOSFET (c).
Silicon Single Crystal Is Still King
257
Gate Oxide Substrate +Q (a) EFm
Ec Ei E Ev FS
(b)
QG < 0
x
QC > 0
–Q
QG < 0
+Q x
–Q
QC > 0
Ionized acceptors
(c) +Q
QG < 0 x –Q
QC > 0
Electrons
(d)
QG < 0
+Q x
QC > 0
–Q Ionized acceptors Electrons Accumulation
s < 0
VGB < VFB
QC > 0
Depletion
s > 0
VGB > VFB
QC < 0
Inversion
s > 0
VGB >> VFB
QC < 0
FIGURE 4.48 A MOS capacitor with a metal gate, an insulator, and a ptype semiconductor. (a) Accumulation; (b) depletion; (c) inversion; (d) strong inversion. Ei is the Fermi level for the intrinsic material, and EFS is that of the doped material (because it is a ptype material the Fermi level is close to the valence band).
(the semiconductor) remains invariant even with an applied bias. The applied gate voltage (VGB) divides between the gate dielectric and the semiconductor such that: VGB = Vox + Vs
(4.54)
where Vox and Vs are the voltages that drop across the oxide and the semiconductor, respectively. The bands in the oxide drop linearly over the bulk of the oxide thickness an amount equal to qVox , and the electric field in the oxide can be expressed as: Eox = Vox /tox
(4.55)
where tox is the oxide thickness. The amount of band bending in the semiconductor is principally located at the surface and is equal to qψσ, where ψσ is the
surface potential and is negative when the band bend is upward. When applying a positive gate bias VGB to counterbalance the positive gate charge, the holes under the gate are pushed away, leaving behind ionized, negatively charged acceptor atoms (N−A), which create a depletion region (Figure 4.48b). The charge in the depletion region of width W and area A is exactly equal to the charge on the gate to preserve charge neutrality [QG(+) = Qc(−) = −qN−A AW]. With a positive gate bias, the Fermi level of the gate is now lowered with respect to the Fermi level of the semiconductor. The bands bend downward, resulting in a positive surface potential. Under the gate, the valence band moves away from the Fermi level, which is indicative of hole depletion. When the band bending at the
258
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
surface is such that the intrinsic level (Ei) coincides with the doped semiconductor Fermi level (EFS), the surface region resembles an intrinsic material. The surface potential for this condition is given by: Y s FF
1 (E E F ) q i
(4.56)
with ϕF, the Fermi potential, given by: FF
kT N A ln q ni
(4.57)
where ni is the charge carrier density of the intrinsic material (see Equation 4.17: ni ≈ 1.5 × 1010 cm−3 at 300 K in pure Si). Applying a larger positive gate bias, the positive charge on the gate increases further, and thermally generated electrons start collecting under the gate. With these electrons, the intrinsic surface region begins to convert into an ntype inversion layer. The negative charge in the semiconductor is now composed of both ionized acceptor atoms in the depletion layer and free electrons in the inversion layer (Figure 4.48c). In this condition, the electron concentration at the surface is still less than the hole concentration in the neutral bulk of the semiconductor, and this regime is called weak inversion. The point where ψs = ϕF is defined as the onset of weak inversion. As the gate bias is further increased, the band bending also continues to increase. This causes the depletion region to become wider while the electron concentration in the inversion layer increases more and more. At the gate bias where the electron concentration in the inversion region is equal to the hole concentration in the bulk, a strong inversion layer is created (Figure 4.48d). The surface potential to achieve this strong inversion is given by: Y s = 2FF
2 (E E F ) q i
value for ψs. The maximum depletion layer width, Wd, at the onset of strong inversion is then given by: Wd
4FF E s qN A
In a real MOS device, the work function of the metal, ϕm, is not likely to be equal to that of the semiconductor, ϕs. Consider a MOS capacitor with ϕm < ϕs at zero gate bias. In this case, electrons in the metal reside at energy levels above the conduction band of the semiconductor. Thus, electrons will flow from the metal into the semiconductor until a potential counterbalances the difference in the work functions between the two plates of the MOS capacitor. This induces a negative charge under the gate dielectric, accompanied by a downward band bending and hence a preexisting positive surface potential ψms. With an external voltage, equal to this difference ψms, applied to the gate, the net charge in the semiconductor disappears, and the bands return to their flat position. This applied voltage is defined as the flatband voltage, VFB, and is expressed as: V FB = qψms = q(ϕs − ϕs)
(4.60)
The oxide and the semiconductor/oxide interface are not perfect, and another modification to the ideal picture of a MOS capacitor comes from charges that reside in the dielectric or at its interface. Such charges may originate from processing, defects in the bulk, or charges that exist at the interface between Si and SiO2 (for an overview of the type of oxide defects, see Figure 4.35). Charges in the bulk oxide, or at the interface, induce opposite charges in the semiconductor and the gate. This again causes the bands to bend up or down, and the flatband voltage has to be adjusted to take this into account. The flatband voltage can then be expressed as:
(4.58)
When the gate bias is increased beyond this value, new electrons in the inversion layer readily compensate extra positive charge on the gate and the depletion layer width does not further increase, and hence the band bending increases only very slightly. For simplicity, 2ϕF is generally taken as the maximum
(4.59)
VFB qFms
Qo C ox
(4.61)
where Qo is the oxide charge, and Cox is the oxide capacitance (we also have introduced ψms = ϕms). Defects located at the Si/SiO2 interface may not be fixed in their charged state, and the amount of charges may also vary with the surface potential of
Silicon Single Crystal Is Still King
the semiconductor. These defects are referred to as fast interface traps, and they impact the switching characteristics of MOSFETs. We now put a MOS capacitor between a source (S) and a drain (D). In Figure 4.49A we show an nchannel and a pchannel device. Both nchannel and pchannel MOSFETs are extensively used. In fact, CMOS IC technology relies on the ability to use both devices on the same chip. As shown in Figure 4.49B, to create an nMOSFET and a pMOSFET on the same ptype substrate, the pMOSFET must be provided with ntype well regions. Nwells are formed by ion implantation or by diffusion. Lateral diffusion limits the proximity between structures, and ion implantation results in shallower wells compatible with today’s fineline processes. Metal 1 makes contact to the nMOSFET and metal 2 to the pMOSFET. Metals in vias connecting to transistors are often made of tungsten metal plugs, and such plugs (A)
pMOSFET (pchannel)
(a)
Gate
Source
nMOSFET (nchannel) (b)
Drain
p+
Gate Source
p+
Drain
n+
n+
ntype silicon substrate
ptype silicon substrate
Drain
Drain
Gate
Gate
Substrate
Substrate
Source
Source (B)
Metal 2 Via
n+
Metal 1
nwell p+ ptype
FIGURE 4.49 (A) pMOS and nMOS with symbols. (a) pMOS with pchannel: a negative voltage is applied to the gate, thus attracting holes that form a channel between the two p + source and drain regions. (b) nMOS with nchannel: a positive voltage is applied to the gate, thus attracting electrons that form a channel between the two n + source and drain regions. (B) To create an nMOSFET and a pMOSFET on the same ptype substrate, the pMOSFET must be provided with an nwell.
259
are also used to fill vias between successive layers of metal (Cu or Al) (see Figure 4.62 and Volume III, Figure 4.3). Tungsten is used because of the extraordinarily good conformality of CVD from WF6. The tungsten in turn contacts the Si via an adhesion/barrier layer such as Ti/TiN. The Ti layer improves the W contact to the transistor and protects the underlying Si from attack by fluorine. Depending on the type of MOSFET (i.e., pchannel or nchannel), two different situations arise. The voltage applied between the gate and the substrate (VGS) generates an electric field through the oxide layer, creating an inversion channel under the gate oxide. In the case of a pMOSFET (with a pchannel) transistor, the ntype substrate is inverted to ptype in a thin layer under the gate oxide, and a ptype substrate is similarly inverted to ntype in an nMOSFET (with an nchannel) device. Because the inversion channel is of the same type as the source and drain, current can now pass from source to drain. The pMOS transistors are 2.5 times slower than nMOSFETs because of the mobility difference between electrons and holes. By varying the potential between the gate and substrate, the inversion channel in which current flows can be altered to control the magnitude of the current, or be turned off completely. Thus, the magnitude of the drain source current, ID, through the channel is controlled by the potential difference VGS applied between the source S and the gate G. The threshold voltage, VT, is the value of VGS where the drain current just begins to flow. From Figure 4.50 typical values range from 0.3 to 0.8 V. The drain current (ID) versus the voltage between drain and source (VDS) for different values of VGS is illustrated in Figure 4.51. As shown at low VDS, the drain current increases almost linearly with VDS, resulting in a series of straight lines with slopes increasing with VGS. At high VDS, the drain current saturates and becomes independent of VDS. Using the nMOSFET in Figure 4.52, the curves in Figures 4.50 and 4.51 are explained in a bit more detail. To make an nchannel MOSFET, as shown in Figure 4.52a, we diffuse donors in the source, drain regions (forming nregions) in an ptype substrate, and grow an oxide layer that acts as the gate oxide. With a small positive voltage on the drain and no
260
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology ID (a) (mA)
Gate
Drain
Source
L W
0.7 0.6
LEFF
0.5 Poly nactive
0.4
Gate oxide psub
Bulk
0.3 VDS = 2V
0.2
VDS
(b) VB
0.1
VGS IB
ID
IG
VT 0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
VGS
FIGURE 4.50 The value of VGS where the drain current, ID, just starts flowing is called V T or the threshold voltage.
bias on the gate, i.e., V DS > 0 and VGS = 0, the drain is a reversebiased pn junction. Conduction band electrons in the source region encounter a potential barrier determined by the builtin potential of the source junction. As a result, no electrons enter the channel region, and hence no current flows from the source to the drain. This is referred to as the “off” state and is illustrated in Figure 4.52b.
600
Linear region
Gate oxide Poly nactive psub Depletion region (electrically induced) VDS
(c) VB
VGS
IG
IB
ID
Saturation region VGS = +5 V
500 VGS = +4 V Drain current, ID (μa)
VDs
(d)
400
VGS VB
IB
IG
ID
VGS = +3 V
300
200
VGS = +2 V
100
VGS = +1 V
0 0
1
2 3 4 Drainsource voltage, VDS(volts)
5
6
FIGURE 4.51 The drain current, I D, versus the voltage between drain and source, VDS, for different values of VGS. The boundary between linear and saturation (active) modes is indicated by the upwardcurving parabola.
FIGURE 4.52 (a) nMOSFET. (b) Apply small VGS (VDS and VB assumed to be small). Depletion region electrically induced in channel, termed “cutoff” region of operation. (c) At a critical value of VGS, termed the threshold voltage (VT ), an inversion layer is created. The inversion layer supports current flow from D to S. The channel behaves as a thinfilm resistor. (d) With VDS, max > VGS − VT , the channel is flowing as much current as it can, so we call it pinched off (even though current continues to flow). The semiconductor bulk potential is VB.
261
Silicon Single Crystal Is Still King
With a small positive bias on the gate, band bending in the channel region (ψs > 0) brings the conduction band in the channel region closer to the conduction band in the source region, reducing the height of the potential barrier to electrons. At a critical value of VGS, termed the threshold voltage (VT), an inversion layer is created (see Figure 4.52c). The inversion layer supports current flow from D to S, and electrons can now enter the channel and flow from source to drain; we say that the transistor is on. In the low drain bias regime, the drain current increases almost linearly with drain bias, and like an ideal resistor it obeys Ohm’s law (see Figure 4.51). The channel resistance is determined by the electron concentration in the channel, which is a function of the gate bias. As the gate bias is increased, the slopes of the linear portion of the I–V characteristics in Figure 4.51 gradually increase as a result of the increasing conductivity of the channel. This region, where the channel behaves like a resistor, is called the linear region of operation. The drain current ID is given by: ID
1 W 2 M e C ox [2( VGS VT ) VDS VDS ] 2 L
(4.62)
The dimensions W, L can be identified from Figure 4.52a, and μe is the effective channel mobility of the electrons, which differs from the bulk electron mobility. For small VDS (VDS 200M transistors/chip
20 years
Triode Diode
Vacuum tube
1st Electric circuits
2016:
~10B transistors/chip
(b)
FIGURE 4.54 (a) History of electronics in the 20th century. In 100 years, the feature size was reduced by 1 million times. (b) Current and future (2016) transistors per chip.
Silicon Single Crystal Is Still King
Modern CMOS Beginning of submicron CMOS
1 m 100 nm 10 nm
Deep UV Litho
36 years of scaling history
90 nm in 2004
Every generation Feature size shrinks by 70% Transistor density doubles Wafer cost increases by 20% Chip cost comes down by 40% Generations occur regularly On average every 2.9 years over the past 34 years Recently every 2 years
1 nm 1970
1980
Density Speed Functionality Cost/bit
1990
2000
Presumed limit to scaling
2010
2020
Minimum feature size
100 m Motivation:
10 m
1
10 m
1K 1M
1 m
1G
100 nm
?
10 nm 1 nm
265
1950
1970
1990 2010 Year
2030 2050
FIGURE 4.55 Two versions of Moore’s first law. Scaling of minimum IC feature size.
lengths will be 7 nm (see Figure 4.55a). Technical limits are debatable and can be tackled, but fundamental limits are firm, and we discuss these ultimate limits first. Fundamental limits include electromagnetic, thermodynamic, and quantum mechanical limits. From the electromagnetic point of view, the speed of light fundamentally limits the electron transport along IC wiring to ∼60 ps/cm (τ > l/c).* In today’s technology, transmission times are getting longer than transistor switching times (now approaching 1 ps). In other words, as transistors are getting smaller and faster, onchip interconnects (wires) are not getting any shorter or faster! This means that a larger percentage of chip area is devoted to metal interconnects as transistors get smaller. The capacitance of the wires is also not decreasing nearly as fast as the transistor sizes (in practice τ ∼ RC ∼ l2, with R and C proportional to l; see also “Constant Field and Constant Voltage Scaling”). The fundamental thermodynamic limit of any electrical device used as a switch (like MOSFETs in computers) is the energy required to produce a binary transition that can be distinguished: independent of the system architecture one must be able to distinguish between logic 0 and 1. CMOS uses an irreversible process with an inevitable intrinsic dissipation of energy. The von NeumannLandauer17
*
It is important to note that the electric field propagates at the speed of light, but the electrons making up the electric current do not travel this fast themselves since they have mass. The individual electrons travel much more slowly. The electrons that go “into” one end of the wire are not the same electrons that “come out” of the other end.
formula sets the theoretical limit for scaling of the energy in all irreversible technologies as (at 300 K): Ebit > kT ln 2 ≈ 18 meV
(4.70)
It was Landauer who realized that with the binary value of a bit unknown, erasing that bit changes the logical entropy of the system from klog2 to klog1 = 0. If the physical representation of the bit is part of a thermalized distribution (so that thermodynamics does apply), then this bit erasure is associated with the dissipation of energy in a heat current of kTlog2 per bit. The practical performance of a MOSFET is limited by its thermodynamic energy efficiency, i.e., the useful work accomplished per unit energy dissipated. If a MOSFET consumes an amount of free energy E and performs N useful operations, the energy efficiency is given by: η = E/N
(4.71)
with η in units of operations per unit energy, or operations/s/W. Using the thermodynamic energy limit per bit from Equation 4.70, this would enable an energy efficiency of η = 3.5 × 1020 operations/s/W. In the case of 90nm VLSI technology, for minimal operations (e.g., conventional switching of a minimumsized transistor), E is on the order of 1 fJ (femtojoule) and η = 1015 operations/s/W. We see that the heat from the thermodynamic and logical entropy associated with a bit are currently five orders of magnitude lower than the electrostatic erasure energy. From classical physics we expect a transistor gate to be a perfect barrier where no electrons flow through, but from quantum physics (Chapter 3) we know that electrons are extended wavelike objects
266
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
that can “tunnel” through a thin gate, and this tunnel rate goes up exponentially as the gate gets thinner. MOSFET scaling is hampered by quantization of charge, which becomes important at a length scale of 10 nm in all materials, and energy level quantization, which becomes important in semiconductors also at a length scale of 10 nm and a factor of about 10 times lower for metals (see Chapter 3). The quantum mechanical limits on MOSFET scaling, based on the Heisenberg uncertainty principle (HUP), can be summarized as: $p x $x r x min
; $p x
h ; (see Equation 3.106) 2P ; 2me E bit
; 2me k B Tln2
1.5 nm (4.72)
which puts a fundamental limit on the integration density. So quantum mechanics allows for a very small switch indeed, but other factors, such as material temperature tolerance range or economics, will limit before this fundamental limit sets in. And also: $E$t r
h ; (see Equation 3.107) 2P
T ^ 0.04 ps or 25 Tbits/s
(4.73)
which sets a fundamental limit to switching speed. Constant Field and Constant Voltage Scaling Scaling of transistors may be achieved by reducing all dimensions (lateral and vertical) by 1/α. Suppose we scale down all transistor dimensions this way, including the gate oxide thickness (tox); then, to maintain the original electric field distribution, including the gate field, one must decrease voltages to 1/α and increase the channel doping by α. Typically 1/α = 0.7 (30% reduction in the dimensions). The scaling variables are summarized in Table 4.10. This is called constant field scaling because the electric field across the gate oxide does not change when the technology is scaled. If the power supply voltage is maintained constant, the scaling is called constant voltage. In this case, the electric field across the gate oxide increases
TABLE 4.10 Scaling of Variables Scaling Variables Voltage Gate length Gate width Gate oxide thickness Junction depth Channel doping
Before
After
V L W tox X N
V/α L/α W/α tox /α X/α Nα
as the technology is scaled down. Because of gate oxide breakdown, at less than 0.8 μm only “constant field” scaling is used. As an example, let us consider the consequences of a 30% scaling effort in the constant field regime (α = 1.43, 1/α = 0.7). ◾ Device/die area: W × L ⇒(1/α)2 = 0.49. In practice, microprocessor die size grows about 25% per technology generation! This is a result of added functionality. ◾ Transistor density: (unit area)/(W × L) ⇒ α2 = 2.04. In practice, memory density has been scaling as expected (not true for microprocessors…). ◾ Gate capacitance: W × L/tox ⇒ 1/α = 0.7 ◾ Drain current: (W/L) (V2/tox) ⇒ 1/α = 0.7 ◾ Gate delay: (C × V) / I ⇒ 1/α = 0.7 (see Figure 4.56) ◾ Frequency: α = 1.43 (see Figure 4.56). In practice, microprocessor frequency has doubled every technology generation (2–3 years)! ◾ The processing power (number of gates/area times speed): goes up as (unit area)/(W × L) × frequency ⇒ α3 = 2.92 ◾ Power: C × V2 × f ⇒ (1/α)2 = 0.49 ◾ Power density: 1/tox × V2 × f ⇒ 1 ◾ Active capacitance/unit area: Power dissipation is a function of the operation frequency, the power supply voltage, and the circuit size (number of devices). If we normalize the power density to V 2 × f, we obtain the active capacitance per unit area for a given circuit. This parameter can be compared with the oxide capacitance per unit area: 1/tox ⇒ α = 1.43. In practice, for microprocessors, the active capacitance/unit area only increases between 30% and 35%. Thus, the twofold improvement in logic density between technologies is not achieved.
Silicon Single Crystal Is Still King
goes up by E2, the gate leakage current increases, and transistors are more likely to fail. As pointed out earlier, higher transistor densities are only possible if the interconnects also scale. Typical wires have a capacitance of ∼0.2 fF/μm compared with 2 fF/μm for a typical gate capacitance. Reduced interconnect wire width leads to increased resistance, and denser interconnects also lead to a higher capacitance. For a wire interconnect, R and C are proportional to l, whereas the RC delay is proportional to l2. This leads to unacceptably great delays for long wires. To account for increased parasitics and integration complexity, more interconnection layers are added with thinner and tighter layers for local interconnections and thicker and sparser layers for global interconnections and power. One also breaks long wires into N shorter segments and drives each one with an inverter or buffer in socalled repeaters. In Table 4.11 constant field and constant voltage scaling of a MOSFET are compared.
Gate
1
Delay = 1
1
Freq = 1
Tox L Body
Source
Drain
1
Delay
Gate 0.7 Tox Source
0.7 L
0.49
0.7
Freq
Drain
Body
1 0.7
= 1.43
0.7
FIGURE 4.56 Scaling of delay and frequency in a MOSFET.
From the preceding, if we succeed in constant field scaling, the speed of the transistor goes up by α and the number of devices/area goes up by α2, the processing power (number of gates/area times speed) goes up by α3, and the heat generation/area (power density) remains unchanged (=1). Unfortunately, you cannot scale down voltage indefinitely. There are fixed voltage characteristics in MOSFETs, such as the 59mV/decade turnon current relation so the industry scales down voltage less aggressively than feature size and as a consequence the electric fields in the gate oxide have been increasing. If the electric field increases by E and the features are scaled down by α, then the doping goes up by E × α, the power density (heat)
Technical and Economic (Practical) Barriers to Downscaling and Possible Solutions Introduction Besides the fundamental limits to CMOS scaling (see above), there are several technical limits to consider, and ultimately the economics might decide the ultimate fate of CMOS. However, Si devices are the smallest devices currently available
TABLE 4.11 Constant Field and Constant Voltage Scaling of a MOSFET Parameter Supply voltage (V) Length (L) Width (W) Gate oxide thickness (tox)
Constant
Constant
1/α
1 1/α 1/α
1/α α
Electric field across gate oxide (E) Depletion layer thickness Gate area (Die area) Gate capacitance (load) (C) Drain current (Id)
1
Voltage
1/α 1/α 1/α
Junction depth (Xj)
Transconductance (g) Gate delay Current density DC and dynamic power dissipation Power density Powerdelay product
Field
1/α
Substrate doping (NA)
267
1/α α α
1/α 1/α2
1/α 1/α2
1/α 1/α
1/α α α 1/α2
1 1/α α
α3 α
2
1/α
α3
1 3
1/α
1/α
268
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
in the market, and there are no other candidates smaller than Si in the near future. Introducing new materials, structures, and processes will solve problems of downsizing. Mass Manufacturability and Economics As we scale down components, they have fewer atoms, electrons, and holes, and unless one has perfect control of the fabrication process, statistical fluctuations start coming in. Obviously MOSFET fabrication lines do not have perfect control, and statistical fluctuations get worse as the device gets smaller (the tyranny of small numbers). As a consequence, as transistors get smaller, there are greater variations in devicetodevice characteristics, such as gate threshold voltage (VT) and output current (ID). Combined with fundamental voltage fluctuations (Johnson noise) and current fluctuations (shot noise), this leads to a greater probability of errors. As onchip circuitry gets smaller and more complex, it is also increasingly sensitive to smaller defects. This lowers the yield and drives up costs even further. The demise of CMOS on technical grounds has been announced several times before.* However, it is more likely that one will hit an economic limit before the ultimate technical limit is reached. Because of increased sophistication of lithography tools, cost of IC fabrication lines is increasing exponentially with time (Moore’s second law) and is now in the multibilliondollar range (1967 cost of a silicon fabrication laboratory: $2 million; 2002 cost: ∼$3 billion; projected 2015 cost: ∼$100 billion). As an example of mass manufacturability and economics, consider resolutionenhancing techniques (RET) that enable subwavelength printing of MOSFETs (see Volume II, Chapters 1 and 2). Basically, RET is a set of optical wavefront engineering techniques that allows for the pattern transfer of features smaller than the lithography wavelength. Feature size scaling is now outpacing lithography wavelength advances, forcing design compromises and complex and costly optical wavefront management techniques. It is important to recognize that at less than 90 nm there is no yield without RET, but this unfortunately vastly increases *
In the late 1980s, 0.1 μm was called the “brick wall”; today 50 nm is called the “red brick wall” and 100 nm the “fundamental limit.”
mask costs and severely constrains design flexibility. Implementing all of these technology innovations may increase manufacturing and development costs to beyond the reach of all but a few global entities. This subwavelength crisis is summarized in Figure 4.57. A practical limit may thus be reached because of cost, reliability, and performance considerations. It is safe to say that it is not really known where that practical limit really lies, and, as remarked earlier, it is certainly too early to give up on Si. It is also clear that pushing CMOS to its ultimate limits will require revolutionary materials and device innovations that pose significant scientific and engineering barriers. These problems have caused more changes in IC technology and materials in the past 5 years than in the previous 40 years with work in SiGe, silicon on insulator (SOI), strained Si, alternative dielectrics, new metallization systems, and so on. Carrier Mobility Limitations The effective mobility of charge carriers in the channel of a MOSFET differs from bulk mobility as a result of additional scattering mechanisms associated with the channel surface, including interface charge scattering and surface roughness scattering. These mechanisms also tend to depend on the vertical electrical field as illustrated in Figure 4.58, where EEFF represents the effective electrical field. As gate length shrinks, mobility decreases, and increased doping is often used to combat this shortchannel effect. Another
10 Above wavelength 3.0 μm 2.0 μm 1.0 μm
1
Subwavelength
0.6 μm 436 nm
0.1
365 nm
0.35 μm 0.25 μm 0.18 μm Lithography wavelength 0.13 μm Silicon feature size
0.07 μm 0.05 μm
1980
1985
1990
1995
2000
FIGURE 4.57 The subwavelength crisis.
2005 2008
Silicon Single Crystal Is Still King 1000
Electron mobility/(cm2/Vs)
Strainenhanced mobility
100
0.80 μm 0.60 μm 0.35 μm 0.25 μm 0.18 μm Technology 0.13 μm node
10
EEFF/(MV/cm)
FIGURE 4.58 Mobility versus technology scaling trend for Intel process technologies. The xaxis is the effective electrical field EEFF. (From Thompson, S.E., M. Armstrong, C. Auth, M. Alavi, M. Buehler, R. Chau, S. Cea, et al. 2004. A 90nm logic technology featuring strainedsilicon. IEEE Trans Electron Devices 51:1790–7.49)
possible solution involves electron and hole mobility enhancement by using strained Si. This method increases mobility of electrons and holes in the channel of a FET by applying tensile (to increase electron mobility) or compressive strains (to increase hole mobility) to the channel. Strain alters the energy band structure and enables charge carriers to move with less resistance through silicon. The MOSFET channel is very close to the device surface, so that the strain must occur in the topmost ~0.01 μm of the silicon to realize a mobility enhancement in the channel. The effect of strain on mobility was noticed in the early 1950s, the exploitation of the phenomenon in an actual device was first carried out at MIT in the early 1990s (Gene Fitzgerald, who founded AmberWave in 1998). By August 2002, Intel used strained silicon in their HT Prescott P4 Processor. Models suggest that a strained silicon lattice can give hole mobilities up to 4× the unstrained value and electron mobilities up to 1.8× the unstrained value.18 One way to introduce strain in Si is to use a Si1xGe x crystal alloy substrate. Such an alloy is possible because both materials create diamondtype lattices and their lattice constants (a) are close. Vegard’s law determines the lattice constant of the alloy, which is a linear average between the lattice constants of Si (5.431 Å) and Ge (5.658 Å):
Silicon germanium
FIGURE 4.59 Formation of a strained Si lattice using an epitaxial straininducing template.
First, one introduces Ge in a Si lattice, and then the Si gate material is grown epitaxially using molecular beam epitaxy (MBE) on top of this Si1xGe x; the Si atoms align with the underlying lattice, causing a lattice strain in the silicon (see Figure 4.59). The electrons flow up to 70% faster through strained silicon, resulting in a 17% increase in transistor speed and a 34% reduction in power consumption. The SiGe devices market has grown more rapidly than was anticipated, and III–Vs producers are concerned about the switching from Si to SiGe instead of using GaAs in a number of key highspeed applications. With SiGe matching GaAs performance and beating it on cost, GaAs still edges out SiGe in terms of poweradded efficiency (PAE)* (typically 40% vs. > Tfin, top gate oxide thickness >> sidewall oxide, effective channel length Leff = Lgate + 2 × Lext thickness, effective channel width W = Tfin + 2 × Hfin.
Present MOSFET designs are planar, “buried” in the flat upper surface of the Si substrate. Each time you double circuit density by stacking, you can move a whole Moore’s law generation without using smaller features. But interconnection is tricky, as are connections to the outside world. It is also more difficult to make highperformance transistors from deposited films, and additional processing tends to spoil previous layers. Source and drain are getting too close for reliable performance, and the gate between them is getting harder to define. 3D techniques can extend microprocessor design for several more generations, but after that, a new design paradigm will be needed to deal with increasing errors and defects. The raised drain and source design in SOI approaches is a step in the right direction. In the FinFET approach, this concept is pushed even further; the transistor structure is put on top of the chip substrate as shown in Figure 4.65a. The term FinFET was coined by University of California, Berkeley researchers to describe a nonplanar, doublegate transistor built on an SOI substrate. The FinFET is a 3D device structure with a channel Si fin, sitting on the substrate, surrounded by a gate that effectively makes two to three gates in parallel. The gate wraps around the fin to form a very small channel. The Si fin has an insulator on the top, and the gate has oxide on either side (two channels). The current flows parallel to the device surface, and the channel width depends on the fin height (for dimensioning see Figure 4.65b). A lightly doped channel in a FinFET affords good gate control. Spacers are used to selfalign the gate to source/drain, and the fin
height can be used to increase the oncurrent, limited by aspect ratio. Many benefits arise from this design. Shortchannel effects are reduced, and there is very low leakage current, high on/off current ratio, low voltage operation, efficient gate design (less switching power), flexibility of using multiple fins for better performance, compatibility with current manufacturing processes, and scalability to sub10 nm. FinFET is the leading candidate set to replace the classic MOSFETs. It is based on a 3D architecture that uses double gates. It can be manufactured with very minor modifications to the current selfaligned process flow. However, there are many issues that have to be resolved before it can be used commercially. A 25nm transistor operating on just 0.7 V was demonstrated in December 2002 by the Taiwan Semiconductor Manufacturing Company. The “Omega FinFET” design, named after the similarity between the Greek letter omega and the shape in which the gate wraps around the source/drain structure, has a gate delay of just 0.39 ps for the ntype transistor and 0.88 ps for the ptype. In Figure 4.66, we sketch the predicted material and device evolution for the years 2004–2020. From the preceding, it appears that making Sibased MOSFETs smaller than 50 nm is not a problem. But the “ultimate” FET may not be made of silicon. Alternative approaches to fabricate logic switches, which we analyze in this volume Chapters 3 and 5 and in Volume III, Chapter 3 on nanotechnology, include molecular electronics, resonant tunneling diodes, and singleelectron transistors.
274
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Physical gate
Ultrathin SOI Doped channel
2004
2007
2010
2013
2016
2020
37 nm
25 nm
18 nm
13 nm
9 nm
6 nm
Highk gate dielectric
Strained Si, Ge, SiGe Raised source/drain
Halo Buried oxide Depletion layer Isolation Silicon substrate
Doublegate CMOS
FinFET
Top gate Channel
Buried oxide Isolation Silicon substrate
Channel Back gate Isolation
Gate
Source
Drain
Buried oxide
FIGURE 4.66 Evolving materials and device structures in MOSFET evolution. Halo from halo implant is a highangle implant of welltype dopant species introduced into the device after transistor gate patterning.
Physicochemical Properties of Si Introduction In the previous sections, we mostly focused on Si as an electronic material. In this section we are looking at all the other properties that make Si such an attractive IC, MEMS, and NEMS material. We first consider Si as a simple substrate, where the semiconductor only plays the role as a flat convenient passive substrate. Next, we investigate the mechanical, thermal, and optical properties of Si. We finish this section with a short commentary on Si’s biocompatibility.
Silicon as a Passive Substrate Any IC, MEMS, or NEMS device needs a substrate. In some cases that substrate acts as a passive support only and does not play any other role in the operation of the device it supports. The use of Si as a passive substrate is discussed in more detail in Volume III, Chapter 1, which focuses on comparing nonlithographybased (traditional) and lithographybased (nontraditional) manufacturing methods. In Volume III, Table 1.9, we show a performance comparison of passive substrate materials in terms of cost, metallization ease, and machinability. We will see there that silicon, because of its extreme flatness, relative low cost, and wellestablished coating procedures, is often the preferred passive substrate— especially for thin films. The disadvantages of
using Si substrates become more pronounced with increasing device size and low production volumes. An overwhelming determining factor for passive substrate choice is the final package of the device because the package often determines the volume and cost. Packaging is so important in the case of sensors that as a rule, their design should start from the package rather than from the sensor itself. For many mechanical sensor applications, singlecrystal Si (SCS), based on its intrinsic mechanical stability and the feasibility of integrating sensing and electronics on the same substrate, presents an excellent substrate choice. But, as we will see in Volume III, Chapter 1, for chemical sensors, Si, with few exceptions, is merely the substrate and as such is not necessarily the most attractive option.
Silicon in Mechanical Sensors Introduction In mechanical sensors, the active structural elements convert a mechanical external input signal (e.g., pressure, acceleration) into an electrical signal output (voltage, current, or frequency). The transfer functions in mechanical devices describing this conversion are mechanical, electromechanical, and electrical. In mechanical conversion, a given external load is concentrated and maximized in the active member of the sensor. Structurally active members are typically highaspectratio elements such as suspended
Silicon Single Crystal Is Still King
beams or membranes. Electromechanical conversion is the transformation of the mechanical quantity into an electrical quantity, such as capacitance, resistance, charge, and so on. Often, the electrical signal needs further electrical conversion into an output voltage, frequency, or current. For electrical conversion into an output voltage, a Wheatstone bridge (see Figure 4.75) may be used as in the case of a piezoresistive sensor, and a charge amplifier may be used in the case of a piezoelectric sensor. To optimize all three transfer functions, detailed electrical and mechanical modeling is required. One of (a)
Elastic
275
the most important inputs required for mechanical models is the experimentally determined, independent elasticity constants or moduli. In what follows, we describe in more detail what makes Si such an important structural element in mechanical sensors and present its elasticity constants. StressStrain Curve and Elasticity Constants Yield, tensile strength, hardness, and creep of a material all relate to the elasticity curve (the stressstrain diagram). Stressstrain curves for several types of materials are shown in Figure 4.67. For small
(b)
Plastic
Stress
Stress
y
TS (tensile strength)
M Ductile mild steel
F (fracture)
P Brittle Si P = proportional limit
0.002
Strain
(c)
Strain
10 60 8 50
6
40 30
b
4
Stress (MPa)
Stress (psi 10 3)
a
20 2 10
c 0
0
1
2
3
4 Strain
5
6
7
8
0
FIGURE 4.67 Typical stressstrain behaviors for different types of materials showing different degrees of elastic and plastic deformations. (a) Stressstrain curve for a typical material with the proportional limit P, and the yield strength σy, as determined using the 0.002 strain offset method. (b) Stressstrain curves for silicon and a ductile mild steel. The tensile strength (TS) of a metal is the stress at the maximum of the curve shown (M). Fracture is indicated by F. The various stages of a test metal sample are indicated as well. A high modulus material such as Si exhibits abrupt breakage; it is brittle with no plastic deformation region at all. (c) Stressstrain behavior for brittle (curve a), plastic (curve b), and highly elastic (elastomeric) (curve c) polymers.
276
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
strain values, Hooke’s law (1635–1702) applies, that is, stress (force per unit area, N/m 2) and strain (displacement per unit length, dimensionless) are proportional, and the stressstrain curve is linear, with a slope corresponding to the elastic modulus E (Young’s modulus, N/m2). This regime, as marked in Figure 4.67a, is the elastic deformation regime (typically valid for ε < 10−4). The magnitude of the Young’s modulus ranges from 4.1 × 104 MPa (Pascal, Pa = N/m2) for magnesium to 40.7 × 104 MPa for tungsten and 144 GPa for Invar,* whereas concrete is 45 GPa, aluminum is about 70 GPa, and elastomeric materials are as low as 10 −3 to 10−2 GPa. Silicon is a stiff and brittle material with a Young’s modulus of 160 GPa (Figure 4.67b). With increasing temperature, the elastic modulus diminishes. For isotropic media, such as amorphous and polycrystalline materials, the tensile stress, σa, or the applied axial force per unit area and the axial or tensile strain, εa, are related as: σa = Eεa
(4.75)
with εa given by the dimensionless ratio of (L2 – L1)/ L1 (ΔL/L1), that is, the ratio of the sample’s elongation to its original length. The elastic modulus may be thought of as stiffness or a material’s resistance to elastic deformation. The greater the modulus, the stiffer the material. A tensile stress usually leads to a lateral strain or contraction (Poisson effect), ε1, given by the dimensionless ratio of (D2 – D1)/D1 (ΔD/D1), where D1 is the original wire diameter and ΔD is the change in diameter under axial stress (see Figure 4.68). The Poisson ratio is the ratio of lateral over axial strain: N
E1 Ea
(4.76)
The minus sign indicates a contraction of the material. For most materials, ν is a constant within the elastic range and fluctuates for different types of materials over a relatively narrow range. Generally, it is on the order of 0.25–0.35, and a value of 0.5 is the largest value possible. The latter is attained by *
Invar, an alloy formed of nickel and iron, has an extremely small coefficient of thermal expansion at room temperature. Invar is often called for in the design of machinery that must be extremely stable.
FIGURE 4.68 Metal wire under axial or normal stress; normal stress creates both elongation and lateral contraction.
materials such as rubber and indicates a material in which only the shape changes, whereas the volume remains constant. Normally, some slight volume change does accompany the deformation, and, consequently, ν is smaller than 0.5. The Poisson ratios for metals are typically around 0.33 (e.g., aluminum and cast steel are 0.34 and 0.28, respectively). For ceramics, it is around 0.25, and for polymers it is typically between 0.4 and 0.5. In extreme cases, values as low as 0.1 (certain types of concrete) and as high as 0.5 (rubber) occur. For an elastic isotropic medium subjected to a triaxial state of stress, the resulting strain component in the xdirection, εx , is given by the summation of elongation and contraction: Ex
1¨ S N(S y S z )·¹ Eª x
(4.77)
and so on for the y and zdirections (three equations in total). For an analysis of mechanical structures, we must consider not only compressional and tensile strains but also shear strains. Whereas normal stresses create elongation plus lateral contraction with accompanying volume changes, shear stresses create shape
Silicon Single Crystal Is Still King
changes without volume changes (e.g., by twisting a body), that is, shear strains. The 1D shear strain, γ, is produced by the shear stress, τ, and has units of N/ m2. For small strains, Hooke’s law may be applied again: T G G
E 2 1 N
6
6
S m ¤ E mn E n and E m ¤ S mn S n
(4.81)
n 1
(4.78)
(4.79)
Crystal materials, whose elastic properties are anisotropic, require more than two elastic constants, the number increasing with decreasing symmetry. Cubic crystals, for example, require 3 elastic constants, hexagonal crystals require 5, and materials without symmetry require 2119,20 (see also Table 2.1). The relation between stresses and strains is more complex in this case and depends greatly on the spatial orientation of these quantities with respect to the crystallographic axes (see Chapter 2 on crystallography). Hooke’s law in the most generic form is expressed in two formulas: S ij E ijkl E kl and E ij S ijkl S kl
strains in terms of stresses. The tensor representations in Equation 4.80 can also be represented as two matrices:
n 1
where G is called the elastic shear modulus or the modulus of rigidity. For any 3D state of shear stress, three equations of this type will hold. Isotropic bodies are characterized by two independent elastic constants only because the shear modulus G, it can be shown,19 relates the Young’s modulus and the Poisson ratio as: G
277
(4.80)
where σij and σkl = stress tensors of rank 2 expressed in N/m2 εij and εkl = strain tensors of rank 2 and are dimensionless Eijkl = stiffness coefficient tensor of rank 4 expressed in N/m2 with at the most 3 × 3 × 3 × 3 = 81 elements Sijkl = compliance coefficient tensor of rank 4 expressed in m2/N with at the most 3 × 3 × 3 × 3 = 81 elements The first expression is analogous to Equation 4.75, and the second expression is the inverse, giving the
Components of tensors Eijkl and Sijkl are substituted by elements of the matrices Emn and Smn, respectively. To abbreviate the ij indices to m and the kl indices to n, the following scheme applies: 11 → 1, 22 → 2, 33 → 3, 23 and 32 → 4, 13 and 31 → 5, 12 and 21 → 6, Eijkl → Emn and Sijkl → Smn when m and n = 1, 2, 3; 2Sijkl → Smn when m or n = 4, 5, 6; 4Sijkl → Smn when m and n = 4, 5, 6; σij → σm when m = 1, 2, 3; and εij → εm when m = 4, 5, 6. Thus, with these reduced indices, there are six equations of the type: σx = E11εx + E12εy + E13εz + E14γyz + E15γzx + E16γxy (4.82) And hence there exist 36 moduli of elasticity or Emn stiffness constants. There are also six equations of the type: εx = S11σx + S12σy + S13σz + S14τyz + S15τzx + S16τxy (4.83) defining 36 Smn constants, which are called the compliance constants. It can be shown that the matrices Emn and Smn, each composed of 36 coefficients, are symmetrical (Emn = Enm and Smn = Snm); hence a material without symmetrical elements has 21 independent constants or moduli. Because of symmetry of crystals, several more of these may vanish until, for an isotropic medium, they number only two (E and ν). The stiffness coefficient and compliance coefficient matrices for cubiclattice crystals with the vector of stress oriented along the [100] axis are given as:
E mn
¨ E11 © ©E12 ©E © 12 ©0 ©0 © ©ª 0
E12 E11 E12 0 0 0
E12 E12 E11 0 0 0
0 0 0 E 44 0 0
0 0 0 0 E 44 0
0 · ¸ 0 ¸ 0 ¸ ¸ 0 ¸ 0 ¸ ¸ E 44 ¸¹
(4.84)
278
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
S mn
¨ S11 © ©S12 ©S © 12 ©0 ©0 © ©ª 0
S12 S11 S12 0 0 0
S12 0 S12 0 E11 0 0 S 44 0 0
0 0
0 0 0 0 S 44 0
· ¸ ¸ ¸ ¸ 0 ¸ 0 ¸ ¸ S 44 ¸¹ 0 0 0
(4.85)
In cubic crystals, the three remaining independent elastic moduli are usually chosen as E11, E12, and E44. The Smn values can be calculated simply from the Emn values. Expressed in terms of the compliance constants, one can show that 1/S11 = E = Young’s modulus, −S12/S11 = ν = Poisson’s ratio, and 1/S44 = G = shear modulus. In the case of an isotropic material, such as a metal wire, there is an additional relationship: E 44
E11 E12 2
(4.86)
With this expression the number of independent stiffness constants reduces to two. The anisotropy coefficient α is defined as: A
2E 44 E11 E12
(4.87)
making α = 1 for an isotropic crystal. For an anisotropic crystal, the degree of anisotropy is given by the deviation of α from 1. SCS has moderately anisotropic elastic properties,21,22 with α = 1.57, and very anisotropic crystals may have a value larger than 8. Brantley21 gives the nonzero Si stiffness components, referred to the [100] crystal orientation, as E11 = E22 = E33 = 166 × 109 N/m2, E12 = E13 = E23 = 64 × 109 N/m2, and E 44 = E55 = E66 = 80 × 109 N/m2: Sx
Ex 166(E11 ) 64(E12 ) 64(E12 ) 0 0 0 Sy Ey 64(E12 ) 166(E11 ) 64(E12 ) 0 0 0 Sz Ez 64(E12 ) 64(E12 ) 166(E11 ) 0 0 0 s 0 0 0 80(E 44 ) 0 0 T xy G xy 0 0 0 0 80(E ) 0 T xz G xz 44 0 0 0 0 0 80(E ) 44 T yz G yz
(4.88) with σ normal stress, τ shear stress, ε normal strain, and γ shear strain. The values for Emn in Equation 4.88 compare with a Young’s modulus of 207 GPa
for a low carbon steel. Variations on the values of the elastic constants on the order of 30%, depending on crystal orientation, doping level, and dislocation density, must be considered to have effects as well. In Volume II, Chapter 7, we learn that the Young’s modulus for polycrystalline silicon is about 161 GPa. From the stiffness coefficients, the compliance coefficients of Si can be calculated as S11 = 7.68 × 10–12 m2/N, S12 = –2.14 × 10 –12 m2/N, and S44 = 12.6 × 10 –12 m2/N.23 A graphical representation of elastic constants for different crystallographic directions in Si and Ge is given in Worthman et al.24 and is reproduced in Figure 4.69a–d displays E and ν for Ge and Si in planes (100) and (110) as functions of direction. Calculations show that E, G, and ν are constant for any direction in the (111) plane. In other words, a plate lying in this plane can be considered as having isotropic elastic properties. A review of independent determinations of the Si stiffness coefficients, with their respective temperature coefficients, is given in Metzger et al.25 Some of the values from that review are reproduced in Table 4.12. Values for Young’s modulus and the shear modulus of Si can also be found in Greenwood 26 and are reproduced in Table 4.13 for the three important crystal orientations. Residual Stress in SingleCrystal Si Most mechanical properties, such as the Young’s modulus, for lightly and highly doped silicon are identical. Residual stress and associated stress gradients in highly borondoped singlecrystal Si (SCS) present some controversy. Highly borondoped membranes, which are usually reported to be tensile, have also been reported as compressive.27,28 From a simple atomradius argument, a large number of substitutional boron atoms would be expected to create a net shrinkage of the lattice compared with pure silicon and that the residual stress would be tensile with a stress gradient corresponding to the doping gradient. For example, an etched cantilever would be expected to bend up out of the plane of the silicon wafer. Maseeh et al.28 believe that the appearance of compressive behavior in heavily borondoped singlecrystal layers results from the use of an oxide etch mask. They suggest that plastic deformation of the p + silicon beneath the compressively stressed oxide can explain the observed behavior. Ding et al.29 also
Silicon Single Crystal Is Still King ××
××
279
××
××
FIGURE 4.69 Elasticity constants for Si and Ge. (a) Young’s modulus as a function of direction in the (100) plane. (b) Young’s modulus as a function of direction in the (110) plane. (c) Poisson’s ratio as a function of direction in the (100) plane. (d) Poisson’s ratio as a function of direction in the (110) plane. (From Worthman, J. J., and R. A. Evans. 1965. J Applied Physics 36:153–56. With permission. 24)
found compressive behavior for nitridecovered p + Si thin membranes. These authors believe that the average stress in p + silicon is tensile, but great care is required to establish this fact because the combination of heavy boron doping and a hightemperature drivein under oxidizing conditions can create an apparent reversal of both the net stress (to compressive) and of the stress gradient (opposite to the doping gradient). A proposed explanation is that, at the oxide/silicon interface, a thin compressively stressed
layer is formed during the drivein, which is not removed in buffered HF. It can be removed by reoxidation and etching in HF, or by etching in KOH. The question of residual stress in polycrystalline Si is a heavily studied topic as we shall discover in Volume II, Chapter 7 on surface micromachining. Stress in thin polycrystalline films has dramatic effects on the reliable operation of surface micromachined mechanical elements (see also Volume II, Equation 7.29).
TABLE 4.12 Stiffness Coefficients and Temperature Coefficients of Stiffness for Si
Yield, Tensile Strength, Hardness, and Creep
Stiffness Coefficients in GPa Temperature Coefficient of (value in GPa = 109 N/m2) Young’s Modulus (10−6 K−1) E11 = 164.8 ± 0.16 E12 = 63.5 ± 0.3
E44 = 79.0 ± 0.06
−122 −162 −97
Source: Metzger, H., and F.R. Kessler. 1970. Der DebyeSears Effect zur Bestimmung der Elastischen Konstanten von Silicium. Z Naturf A 25:904.
As a material is deformed beyond its elastic limit, yielding or plastic deformation (permanent, nonrecoverable deformation) occurs. The point of yielding in Figure 4.67a is the point of initial departure from linearity of the stressstrain curve and is sometimes called the proportional limit indicated by a letter P. Young’s modulus of mild steel is ±30,000,000 psi, and its proportional limit (highest stress in the
280
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 4.13 Derived Values for Young’s Modulus and Shear Modulus for Si Crystal Orientation [100] [110] [111]
Young’s Modulus E (GPa)
Shear Modulus G (GPa)
Temperature Coefficient (10 –6 K−1)
129.5 168.0 186.5
79.0 61.7 57.5
–63 –80 –46
Source: Greenwood, J.C. 1988. Silicon in mechanical sensors. J Phys E Sci Instrum 21:1114.
elastic range) is approximately 30,000 psi.* Thus, the maximum elastic strain in mild steel is about 0.001 under a condition of uniaxial stress. This gives an idea as to the magnitude of the strains we are dealing with. A convention has been established wherein a straight line is constructed parallel to the elastic portion of the stressstrain curve at some specified strain offset, usually 0.002. The stress corresponding to the intersection of this line and the stressstrain curve as it bends over in the plastic region is defined as the yield strength, σy (see Figure 4.67a). The magnitude of the yield strength of a material is a measure of its resistance to plastic deformation. Yield strengths may range from 35 MPa (5,000 psi) for a soft and weak aluminum to more than 1,400 MPa (200,000 psi) for highstrength steels. The tensile strength is the stress at the peak of the stressstrain curve. This corresponds to the maximum stress that can be sustained by a structure in tension; if the stress is applied and maintained, fracture will result. Crystalline silicon is a hard and brittle material, deforming elastically until it reaches its yield strength, at which point it breaks. For Si, the yield strength is 7 GPa, equivalent to a 700kg weight suspended from a 1mm2 area. Both tensile strength and hardness are indicators of a metal’s resistance to plastic deformation. Consequently, they are roughly proportional.30 Material deformation occurring at elevated temperatures and static material stresses is termed creep. It is defined as a timedependent and permanent deformation of materials when subjected to a constant load or stress. Silicon exhibits no plastic deformation or creep below 500°C; therefore, Si sensors are very *
In the sensor area it is still mandatory to be versatile in the different unit systems especially with regard to pressure and stress. In this book we are using mostly Pascal, Pa (=N/m 2), but in industry it is still customary to use psi when dealing with metal properties, Torr when dealing with vacuum systems, and dyne/cm 2 when dealing with surface tension.
insensitive to fatigue failure when subjected to high cyclic loads. Silicon sensors have been cycled in excess of 100 million cycles with no observed failures. This ability to survive a very large number of duty cycles is because there is no energyabsorbing or heatgenerating mechanism caused by intergranular slip or movement of dislocations in silicon at room temperature. However, singlecrystal Si (SCS), as a brittle material, will yield catastrophically when stress beyond the yield limit is applied rather than deform plastically as metals do (see Figure 4.67b). At room temperature, high modulus materials, such as Si, SiO2, and Si3N4, often exhibit linearelastic behavior at lower strain and transition abruptly to brittlefracture behavior at higher strain. Plastic deformation in metals is based on stressinduced dislocation generation in the grain boundaries and a subsequent dislocation migration that results in a macroscopic deformation from intergrain shifts in the material. No grain boundaries exist in SCS, and plastic deformation can only occur through migration of the defects originally present in the lattice or of those generated at the surface. As the number of these defects is very low in SCS, the material can be considered a perfect elastic material at normal temperatures. Perfect elasticity implies proportionality between stress and strain (i.e., load and flexure) and the absence of irreversibilities or mechanical hysteresis. The absence of plastic behavior also accounts for the extremely low mechanical losses in SCS, which enable the fabrication of resonating structures that exhibit exceptionally high Qfactors. Values of up to 108 in vacuum have been reported. At elevated temperatures, and with metals and polymers at ordinary temperatures, complex behavior in the stressstrain curve can occur. Considerable plasticity can be induced in SCS at elevated temperatures (>800°C), when silicon softens appreciably and the mobility of defects in the lattice is substantially increased. Huff
281
Silicon Single Crystal Is Still King
and Schmidt 27 report a pressure switch exhibiting hysteresis based on buckling of plastically deformed silicon membranes. To eliminate plastic deformation of Si wafers, it is important that during hightemperature steps the presence of films that could stress or even warp the wafer in an asymmetric way, typically oxides or nitrides, be avoided.
Piezoresistors are indiﬀused at zones of maximum strain
Si
Piezoresistivity in Silicon Piezoresistance is the fractional change in bulk resistivity induced by small mechanical stresses applied to a material. Lord Kelvin discovered the effect in 1856. Most materials exhibit piezoresistivity, but the effect, Smith found in 1954, is particularly important in some semiconductors (more than an order of magnitude higher than that of metals).31 Monocrystalline silicon has a high piezoresistivity and, combined with its excellent mechanical and electronic properties, makes a superb material for the conversion of mechanical deformation into an electrical signal. The history of siliconbased mechanical sensors started with the discovery of the piezoresistance effect in Si (and Ge) more than four decades ago.31 The piezoresistive effect in semiconductor materials originates in the deformation of the energy bands as a result of the applied stress. The deformed bands change the effective mass and mobility of the charge carriers (electrons and holes), hence modifying the resistivity. The two main classes of piezoresistive semiconductor sensors are membranetype structures (typically pressure and flow sensors) and cantilever beams (typically acceleration sensors) with indiffused resistors (boron, arsenic, or phosphorus) strategically placed in zones of maximum stress (Figure 4.70). In Chapter 2 we saw how in a 3D anisotropic crystal, the electrical field vector (E) is related to the current vector, J, by a 3 × 3 resistivity tensor (see Equation 2.4).23 Experimentally, the nine coefficients always reduce to six, and the symmetric tensor, is given by: ¨ E1 · ©E ¸ © 2¸ ©ªE 3 ¸¹ Electric Field
¨ R1 ©R © 6 ©ªR5
R6 R2 R4
R5 · ¨ J1 · R4 ¸ © J2 ¸ ¸© ¸ R3 ¹¸ ª© J3 ¹¸
Resistivity Tensor
Si
FIGURE 4.70 Si membrane and Si cantilever with indiffused resistors.
For the cubic Si lattice, with the axes aligned with the directions, ρ1, ρ2, and ρ3 define the dependence of the electric field on the current along the same direction (one of the directions). The crosssensitivities, ρ4, ρ5, and ρ6, relate the electric field to the current along a perpendicular direction. The six resistivity components in Equation 4.89 depend on the normal (σ) and shear (τ) stresses in the material as defined earlier in this chapter. This can be represented as: ¥ 1´ R Rno stress $RS , T or S c ¦ µ Sno stress $S c S , T § R¶ (4.90)
(4.89)
Curren FIGURE 4.71 Piezoresistance in silicon.
282
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
where we use σc for conductivity to distinguish it from σ for the normal stress. For cubic crystals this can be written out as (see also Figure 4.71): ¨ $S c ,1 · ¨ P ¸ © 11 © © $S c ,2 ¸ © P12 © $S ¸ © © c ,3 ¸ © P12 © $S c ,4 ¸ © 0 © ¸ © © $S c ,5 ¸ © 0 © $S ¸ ©ª 0 ª c ,6 ¹
P12 P11 P12
P12 P12 P11
0 0 0
0 0 0
0 0 0 P 44 0 0
0 0 0 0 P 44 0
F
V
0 · ¨ S1 · ¸ © ¸ 0 ¸ ©S 2 ¸ 0 ¸ ©S3 ¸ ¸.© ¸ 0 ¸ © T1 ¸ 0 ¸ © T2 ¸ ¸ © ¸ P 44 ¸¹ ©ª T 3 ¸¹ (4.91)
Substituting the results of Equation 4.91 in Equation 4.89 one obtains the following three expressions for a large piece of bulk silicon: E1 RJ1 RP11S1J1 RP12 (S 2 S 3 )J1 RP 44 (J 2 T 3 J3 T 2 ) E 2 RJ 2 RP11S 2 J 2 RP12 (S1 S 3 )J 2 RP 44 (J1T 3 J 3 T1 ) E 3 RJ 3 RP11S 3 J 3 RP12 (S1 S 2 )J 3 RP 44 (J1T 2 J 2 T1 ) (4.92) For devices with finite dimensions, the influence of dimensional changes needs to be added through the Poisson ratio. Smith31 was the first to measure the resistivity coefficients for Si at room temperature. The coefficients are dependent on crystal orientation, temperature, and dopant concentration. Table 4.14 lists Smith’s results for the three remaining independent resistivity coefficients, that is, π11, π12, and π44 of [100]oriented Si at room temperature.31 The piezoresistance coefficients are largest for π11 in ntype silicon and π44 in ptype silicon, about –102.2 10 –11 and 138 10 –11 Pa–1, respectively. The piezoresistivity coefficients are related to the gauge factor (Gf ) by the Young’s modulus. The gauge factor, Gf, is the relative resistance change divided by the applied strain, or:
V
I
I F
F
F (a)
(b)
FIGURE 4.72 Longitudinal (a) and transverse (b) piezoresistors.
Gf
1 $R E R
(4.93)
The gauge factor of a metal strain gauge is typically around 2; for singlecrystal Si (SCS) it is 90; and for polycrystalline and amorphous Si, it is between 20 and 40. The contribution to resistance changes from stresses that are longitudinal (σ1) and transverse (σt) with respect to the current flow is given by (Figure 4.72): $R S l Pl S t P t R
(4.94)
where σ1 = longitudinal stress component, i.e., stress component parallel to the direction of the current σt = transversal stress component, i.e., stress component perpendicular to the direction of the current π1 = longitudinal piezoresistance coefficient πt = transversal piezoresistance coefficient The piezoresistance coefficients πl and πt for (100) silicon as a function of crystal orientation are reproduced from Kanda in Figure 4.73a for
TABLE 4.14 Resistivity and Piezoresistivity Coefficients at Room Temperature, Si Wafers and Doping Levels below 1018 cm−3 in 10−11 Pa−1
pSi nSi
ρ (Ωcm)
Direction
7.8
11.7
π11
π12
π44
+6.6
−1.1
+138.1
−102.2
+53.4
−13.6
πt
πl
0 −66.3 + 53.4 −17.6
0 71.8 −102.2 −31.2
Source: Smith, C.S. 1954. Piezoresistance effect in germanium and silicon. Phys Rev 94:42; and Khazan, A.D. 1994. Transducers and their elements. Englewood Cliffs, NJ: PTR Prentice Hall.
283
60
70
80
50
20 30 40 50 60 70 80 90 100 110
0
1
0 13 0 12
110
70
80
60
10
(010)
100
50
0 2010 90 1101009080706050403
0 13
50 0 13
0 12 110
100
10 20 30 40 50 60 70 80 90 100 11090
100
110
12
60
0
70
80
110
0 12 0
10 20 30 40 50 60 70 80 90 100 11090
9011010080 90 7060504030 2010
0
80
40
14
70
30
150
60
160
0
50
170
20
t
20
t
0
10
30
(110)
14
(010) 1101009080 70 60 50 40 30 20
40
150
(010) 0 20 30 40 50 60 70 80 90 100 110
0
170 40
10
170
160 30
20
(110)
160
150
20
30
(110)
150
0
14
10
0
(01 0) 11010090 80 70 60 50 40 30 20
1
14
(110)
40
160
13
(100)
(100)
170
100
Silicon Single Crystal Is Still King
(b)
(a)
FIGURE 4.73 Piezoresistance coefficients π1 and π t for (100) silicon in the (001) plane in 10 –12 cm2 dyne –1 or 10 –11 Pa –1. (a) For ptype. (b) For ntype. (From Kanda, Y. 1982. IEEE Trans Electr Dev 29:64. With permission.)
ptype and Figure 4.73b for ntype. 32 For lightly doped silicon (n or ptype < 1018 cm−3), the temperature coefficient of resistance for π1 and πt is approximately 0.25%/°C. It decreases with dopant concentration to about 0.1%/°C at 8 × 1019 cm−3. By maximizing the expression for the stressinduced resistance change in Equation 4.94, the achievable sensitivity in a piezoresistive silicon sensor is optimized. From Figure 4.73, the maximum longitudinal piezoresistive coefficient for ptype Si is πl,[111] = 93.5 × 10 −11 Pa−1 and for ntype Si it is πl,[100] = −102.2 10 −11 Pa−1 (this latter value is also found in Table 4.14).
The orientation of a sensing membrane or beam (Figure 4.74) is determined by its anisotropic fabrication. In ptype Si the piezoresistive coefficients are opposite in sign and comparable in magnitude, making them ideal for Wheatstone bridge detection (see Figure 4.75). The surface of the silicon wafer is usually a (100) plane; the edges of the etched structures are intersections of (100) and (111) planes and are thus directions. For pressure sensing, ptype piezoresistors are most commonly used. This is because the orientation of maximum piezoresistivity ()
Maximum surface stress Proof mass Substrate Flexure
Side view
Longitudinal Top view
1 –31.2 · 10–11 Pa–1
1 –17.6 · 10–11 Pa–1
1 71.8 · 10–11 Pa–1
1 –66.3 · 10–11 Pa–1
Transverse Top view
FIGURE 4.74 Bulk micromachined cantilever with longitudinal and transverse piezoresistors.
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Vb R1
284
For ntype resistors, π44 can be neglected, and we obtain:
A
$R P11 P12 S1 S t 2 R
R2
B A (100)
R3
R4
B
ptype resistors (b)
(a)
FIGURE 4.75 Measuring membrane resistance with piezoresistors. (a) Wheatstone bridge configuration of four indiffused piezoresistors. The arrows indicate resistance changes when the membrane is bent downward (into the page). (b) Maximizing the piezoresistive effect with ptype resistors. The A resistors are stressed longitudinally and the B resistors are stressed transversally. (Based on Peeters, E. 1994. Process development for 3D silicon microstructures, with application to mechanical sensor design. PhD diss., Katholieke Universiteit Leuven, Leuven, Belgium. With permission;2 and Maluf, N. 2000. An introduction to microelectromechanical systems engineering. Boston: Artech House. 34)
happens to coincide with the edge orientation of a conventionally etched diaphragm and because the longitudinal coefficient is roughly equal in magnitude but opposite in sign as compared with the transverse coefficient (see Figures 4.73a and 4.75b and Table 4.14).2 Piezoresistors oriented at 45° with respect to the primary flat, that is, in the direction, are insensitive to applied stress, which provides an inexpensive way to incorporate stressindependent diffused temperature sensors. Longitudinal and transverse piezoresistance coefficients are related to principal piezoresistance coefficients through coordinate transformation. With the values in Table 4.14, π1 and πt can be calculated numerically for other primary orientations. The longitudinal piezoresistive coefficient in the direction is π1 = 1/2(π11 + π12 + π44). The corresponding transverse coefficient is πt = 1/2(π11 + π12 – π44). From Table 4.14, we know that for ptype resistors π44 is more important than the other two coefficients, and Equation 4.94 is approximated by: $R P 44 Sl S t 2 R
(4.95)
(4.96)
Equations 4.95 and 4.96 are valid only for uniform stress fields or if the resistor dimensions are small compared with the membrane or beam size. When stresses vary over the resistors, they have to be integrated, which is conveniently done by computer simulation programs. More details on the underlying physics of piezoresistivity and its dependence on crystal orientation can be found in Kanda 32 and Middlehoek and Audet.33 To convert the piezoresistive effect into a measurable electrical signal, a Wheatstone bridge is often used. A balanced Wheatstone bridge configuration is constructed as in Figure 4.75a by locating four ppiezoresistors midway along the edges of a square diaphragm as in Figure 4.75b (location of maximum stress). Two resistors are oriented so that they sense stress in the direction of their current axes, and two are placed to sense stress perpendicular to their current flow. Two longitudinally stressed resistors (A) are balanced against two transversally stressed resistors (B); two of them increase in value, and the other two decrease in value on application of a stress. In this case, from Equation 4.95: $R z 70 10 11(S1 S t ) R
(4.97)
with σ in Pa. For a realistic stress pattern where σ1 = 10 MPa and σt = 50 MPa, Equation 4.97 gives us ΔR/R ≈ 2.8%.2 Thus, resistance change can be calculated as a function of the membrane or cantilever beam stress. By varying the diameter and thickness of the silicon diaphragms, piezoresistive sensors in the range of 0–200 MPa have been made. The bridge voltages are usually between 5 and 10 V, and the sensitivity may vary from 10 mV/kPa for lowpressure to 0.001 mV/kPa for highpressure sensors. A schematic illustration of a pressure sensor with diffused piezoresistive sense elements is shown in Figure 4.76. In this case, ptype piezoresistors are diffused into a thin epitaxial ntype Si layer on a ptype Si substrate.34
Silicon Single Crystal Is Still King Bondpad
{100} Si diaphragm
ptype diﬀused piezoresistor
Metal conductors ntype epitaxial layer
R11
R2
285
R3 ptype substrate and frame
{111}
Anodically bonded Pyrex substrate
Etched cavity Backside port
FIGURE 4.76 Schematic illustration of a pressure sensor with ptype diffused resistor in an ntype epitaxial layer. (Based on Maluf, N. 2000. An introduction to microelectromechanical systems engineering. Boston: Artech House.34)
$R z 53.10 11 s S t 102.10 11 s S 1 R
(4.98)
with σ in Pa. Based on Equation 4.98, with σt = 10 MPa and σ1 = 50 MPa, ΔR/R ≈ –4.6%. In the proposed stress pattern it is important to minimize the transverse stress by making the device truly uniaxial as the longitudinal and transverse stress components have opposite effects and can even cancel out one another. In practice, a pressure sensor with an estimated 65% gain in pressure sensitivity over the
more traditional configurations could be made in the case of 80% uniaxiality.2 Silicon as a Mechanical MEMS Material: Summary
>
Here we want to refine decision criteria about the choice of an “active substrate” for mechanical micromachining applications in which the substrate is involved in determining the mechanical performance of the device crafted from/on it. Mechanical stability is crucial for mechanical sensing applications. Any sensing device must be free of drift to avoid recalibration at regular intervals. Part of the 00
w2/λ, with w the diameter of the aperture and λ the wavelength of the light.
an interference pattern—a Fraunhofer diffraction pattern—is created (see also Figure 5.5). This diffraction pattern corresponds to a forward Fourier transformation. A lens, say, a microscope objective, is essential for image formation and acts to focus light from infinity to the “focal point” at a distance from the lens known as the focal length, f. Located at the focal point is the back focal plane of the lens where the diffraction pattern can be made visible on a screen, as shown in Figure 5.8. In Figure 5.8 we show how a gratinglike object is imaged and that a diffraction pattern can be seen in the back focal plane. The second stage of image formation takes place when the scattered radiation passes beyond the back focal plane of the lens and recombines to form an
What’s an Image? A major breakthrough in the understanding of image formation came in 1872, when Ernst Abbe (Figure 5.6) applied Fourier transforms to explain the phenomenon (Bragg, in 1939, applied Fourier analysis to xray crystallography; see Chapter 2). Image formation, according to Abbe’s theory, is a twostage, doublediffraction process: an image is the diffraction pattern of the diffraction pattern of an object. Consider an “ideal” lens system, in which an image depicts every detail of an object as shown in Figure 5.7. In the first stage of the image formation, light rays incident on the object are scattered, and
FIGURE 5.6 Ernst Abbe (1840–1905). The formula from Ernst Abbe expressing the maximum possible resolution from a light microscope on a monument erected by the University of Jena in Abbe’s memory.
304
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Eye
Eyepiece Image plane
Back focal plane Objective Object plane FIGURE 5.7 A lens is essential in image formation.
image. This is the back or inverse Fourier transform illustrated in Figure 5.9. The image formed by the lens does not exactly represent the real object because not all scattered radiation enters the lens and therefore cannot all be focused on the image plane. The more of the higher orders of the fringes in Figure 5.8 can be picked up, the higher the fidelity of the image. Thus, the basic description of image formation according to Fourier optics is that a Fourier transform of the object in the back focal plane of the lens is generated, and that propagation to the image plane produces another Fourier transformation—an inverse Fourier transform—i.e., the image. Here it may also be understood why Fourier image analysis is such a powerful method for analyzing a wide variety of periodic phenomena. The Fourier transform process separates the image processing into two stages: the information contained in the diffraction pattern in the first
Gratinglike object
stage reveals structural information in a straightforward manner and conveniently separates most of the signal and noise components and thus the transform may be manipulated and subsequently backtransformed in the second stage to produce a noisefiltered, better reconstructed image. Remember from our discussion on xray diffraction of crystals in Chapter 2 that because there is no lens in this case, no image of the crystal lattice is generated; instead, Fresnel diffraction patterns form at finite distances and Fraunhofer diffraction patterns at infinity. Thus, xray diffraction methods provide a direct way to display the decomposition of xrays in component waves (frequencies) in a forward Fourier transform. To get an image of the crystal one would need an xray focusing lens, which does not exist, or, as we do in practice, Fourier transform the diffraction pattern to get the real image of the crystal.
Image Resolution and Diffraction Limit Abbe’s Limit Besides recognizing how an image is formed, Ernst Abbe was also the first to characterize the resolution of an optical system. When an object illuminated in a microscope with coherent (inphase) light is an optical grating, the diffraction orders (N) of the grating are observed in the back focal plane of the objective, and these grating orders are then combined to form an image in the image plane (see Figures 5.7 and 5.8). The resolution of the resulting image depends on the number of grating orders that are transmitted through the optical system. Based
Microscope objective Order 2 Order 1
Order 0
Diﬀerent orders interfere at image plane
Order 1 Order 2
λ
Object plane
Back focal plane
Image plane
FIGURE 5.8 A gratinglike object is imaged, and in the back focal plane an interference pattern—a Fraunhofer diffraction pattern—is formed that corresponds to the forward Fourier transform of the object.
305
Photonics
!
$#
$#
%#
FIGURE 5.9 An inverse Fourier transform gives back the original image of Mickey Mouse on the left.
on imaging of gratings, Abbe, together with Carl Zeiss, published a paper in 1877 defining the physical laws that determined the resolving distance of an optical system. When imaging a grating with coherent light, the direction of diffracted rays is given by the grating formula: d
NL NL 2n sin Q 2NA
(5.1)
where d = grating spacing n = refractive index in image space λ = wavelength of the light N = diffraction order θ = angle of the ray of order N emerging from the grating NA = numeric aperture The grating spatial frequency (ν = 1/2d) corresponding to the firstorder (N = 1) diffracted peak is then given as: N
1 nsin Q 2d L
(5.2)
For imaging with a lens, the lens needs to be able to capture the light, so it is required that θ = θmax, where θmax is defined by the numerical aperture NA of the lens. The latter is given by: NA = nsin θmax
& "
!
FIGURE 5.10 Relationship between the object, image, focal length, and diameter of a lens to define the numerical aperture. An important application is projection lithography, where the image on the mask is imaged onto a photoresist (see Volume II, Chapter 1).
light; an NA of 1 means that the lens gathers all the light that falls onto it. Hence the numerical aperture characterizes the ability of a lens to transmit light. It is proportional to the size of the lens, lens diameter D, and inversely proportional to effective F number (F#), defined as f/D, or the focal length f divided by the lens diameter D: NA nsin Qmax
D 1 2f 2F
(5.4)
The assumptions here are a large F#, which implies that θ is small so that NA = sin θ ∼ tan θ ∼ θ, a situation called the paraxial approximation.* At angles larger than θmax, the imaging lens no longer captures light. Therefore, the highest grating spatial frequency that can be imaged by a coherent illumination system is given by: Nmax
(5.3)
This is illustrated in Figure 5.10, where the aim is to image a fine mask pattern onto a thin layer of photosensitive photoresist. The NA of the lens in a medium of refractive index n (1.0 in air) defines the angle of acceptance, 2θmax, of the cone of diffracted light from an object that the lens can accept. It lies between 0 and 1. An NA of 0 means that the lens gathers no
n sin Qmax NA 1 2dmin L L
(5.5)
Consequently, resolution R (defined here as dmin, i.e., slit or a line) in this case is given by: R dmin
*
L 2NA
(5.6)
To understand all the simplifications involved in this result consult Meinhart and Wereley (2003).53
306
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
A coherent wavetrain of many photons
An incohernt wavetrain of many photons
FIGURE 5.11 Spatial coherence of light.
In the case of incoherent illumination (see spatial coherence in Figure 5.11) of the same grating, each ray is diffracted by the grating and forms its own image in the wafer plane. The direction of the first diffraction peak (N = 1) for incoherent rays, incident at an angle i, is given by a more general grating equation: d
L L 2n (sin Q sin i) 2NA
the phenomenon. In 1872, Rayleigh proposed his resolution criterion based on this Airy pattern. This criterion defines two identical incoherent light sources, separated by a distance d, as resolved when the maximum of the Airy disc from one point source falls on the first zero of the intensity distribution of the Airy disc from a second point source. The diffraction for a circular aperture* is given as:
(5.7) ¥ PD sin Q ´µ µµ 2J1 ¦¦ ¦§ µ¶ L E and I E 2 ¥ PD sin Q ´µ ¦¦ µµ ¦§ µ¶ L
representing the path difference for light passing through adjacent slits. For light incident normal to the grating (sin i = 0), Equation 5.7 reduces to Equation 5.1. For image formation it is now required that both i and θ = θmax. Therefore: Nmax
1 2n sin Qmax 2NA 2dmin L L
(5.8)
or: R dmin
L 4NA
(5.9)
so that the resolution for incoherent light is twice better (smaller features can be resolved) than the resolution of coherent light. Rayleigh’s Limit The above imaging resolutions for coherent and incoherent light are theoretical limits. Let us calculate the practical limit to the resolution of a lens. Light passing through a circular aperture interferes with itself, creating ringshaped diffraction patterns known as an Airy pattern, which blurs the image (see Figures 5.13 and 5.14). It is named for George Biddell Airy, a British astronomer, who first explained
2
¨ ¥ PD sin Q ´ · µµ ¸ © 2J1 ¦¦ µµ ¸ © ¦§ L ¶¸ © © ¥ PD sin Q ´ ¸ µµ ¸ © ¦¦ © ¦§ µµ¶ ¸¸ L ©ª ¹ (5.10)
where E = electrical field I = intensity J1 = a Bessel function of the first kind of order 1 in x with x = πDsin θ/λ (see Figure 5.12) D = diameter of the aperture λ = wavelength of light The expression of I(r) is called the point spread function (PSF), and the radius of the Airy disc is derived from it. The PSF extends to infinity, but the “width” of the central intensity peak can be described from its first minimum where J1 is zero, i.e., at x = 3.8 (see Figure 5.12). The radius of the PSF(r), at a distance s of the aperture, is defined by the radius of the first dark ring in the image plane, corresponds to the radius of the Airy disc, and is calculated as: *
Exercise: In Chapter 2 we calculated the diffraction of xrays from a crystal (see Equation 2.39). Demonstrate that Equations 2.39 and 5.10 are identical expressions.
Photonics
307
Jn(x)
x
1 3
0.8 0.6
J0(x) J1(x)
J2(x)
J3(x)
0.4
J4(x)
J5(x)
0.2 2 2
4
6
8
10
x
–0.2 –0.4
1 (a)
(b)
FIGURE 5.12 (a) 1) pinhole, 2) lens system, and 3) point spread function (PSF). (b) Bessel functions.
J1 0 when x
PDsin Q 3.8 or, for small Q, L
1.22L D and since Q Q
r s
(5.11)
1.22Ls D Fraunhofer diffraction patterns are obtained by moving the screen far enough away from the aperture. To obtain the Fraunhofer diffraction pattern at the focal point of a lens, we set the lens against the aperture and use the focal length (f) of the lens as the aperture to screen distance (i.e., replace s with f in Equation 5.11), or: r
r
1.22Lf D
(5.12)
This is illustrated in Figure 5.13. Or, based on Equation 5.4, for an ideal lens system of focal length f, the Rayleigh criterion yields a minimum spatial resolution as: d
1.22L 2NA
(5.13)
In this expression d is the radius of the smallest object that the lens can resolve and also the radius of the smallest spot on which a collimated beam of
light can be focused. The Rayleigh criterion is illustrated in Figure 5.14. In Figure 5.15 we show a schematic of a single lens with diameter D imaging a small circular aperture. By definition, the magnification M of a lens is given by: M
Si S0
(5.14)
where S0 is the object distance and Si is the image distance. Combining this expression for magnification with the Gaussian lens formula we obtain: 1 1 1 f Si S0
(5.15)
S i (M 1)f
(5.16)
which leads to:
1.22 f/D
FIGURE 5.13 Image by a point source forms a circle with diameter of 2.44 λf/D (=2 × r) surrounded by diffraction rings (Airy pattern).
308
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
FIGURE 5.14 Rayleigh criterion: two light spots are considered resolved if the intensity minimum of one ¥ 1.22L ´ coincides with the maximum of the other ¦ d = . 2NA µ¶ §
where f is the focal length of the lens. If the object distance (S0) and the image distance (Si) are set equal to the focal lengths, the magnification can be written in terms of the focal lengths, or: M
Si f i S0 f0
(5.17)
In the case Si = S0 and f i = f0, the magnification M obviously equals 1. The F number (F#) of such a setup is then by definition given as F# = f0/D = f i/D (see Equation 5.4); its numerical aperture is NA0 = NA i = NA, and these factors are linked with the magnification M via: F
f0 f 1 1 (1 M)f i D D 2NA 0 2NA i D (5.18)
D is the diameter of the lens or the diameter of the light beam, whichever is the smaller of the two. The larger the NA of the projection lens in the lithography system of Figure 5.10, the greater the amount of light (containing diffraction information
FIGURE 5.15 Schematic of a single thin lens with aperture diameter, D. The object distance is S 0, and the image distance is Si. The point spread function through a circular aperture is the wellknown Airy function of width or diameter, d = 2.44Siλ/D (see Equation 5.13 with D = 2r).
of the mask) collected and subsequently imaged. Because the image is constructed from diffracted light, and the collection of higher orders of diffracted light enhances the resolution of the image, a larger NA, allowing a larger acceptance angle, results in a better lithography resolution. Therefore, for a set wavelength, the resolution in a lithography system has traditionally been improved by increasing the NA of the optical system. This is usually achieved by increasing the lens diameter D. Lately, work is also directed at increasing NA by increasing the refractive index n of the medium surrounding the imaging lens (Equation 5.3). The latter approach is exploited in immersion lithography, an advanced lithography approach with the potential to keep the semiconductor industry on track with Moore’s law. The physical limit to NA for lithography exposure systems using air as a medium between the lens and the wafer is 1 because the sine of any angle is always ≤1 and n = 1 for air. What happens, though, if a medium with a higher index of refraction is substituted for air, as is often done in microscopy, where oil is placed between the lens and the sample being viewed for resolution? Abbe and Zeiss developed these oil immersion systems using oils that matched the refractive index of glass. Thus, they were able to reach a maximum NA of 1.4, allowing light microscopes to resolve two points distanced only 0.2 μm apart. In Volume II, Chapter 1, we will further detail immersion lithography.
Refraction Snellius Law Geometric optics, also ray optics, has light propagate as “rays.” These rays are bent at the interface between two dissimilar media. The “ray” is an abstract object, perpendicular to the wavefronts of the electromagnetic (EM) waves. Geometric optics provides rules for propagating these rays through an optical system, revealing how actual wavefronts propagate. Ray optics is a significant simplification of optics and fails to account for many important optical effects, such as diffraction and polarization. The latter phenomenon will only be understood properly after we introduce Maxwell’s equations.
Photonics
Light refracts, which means that it bends when passing from one medium to another. Thus, refraction is the change in direction of a ray of light passing from one transparent medium to another one with a different optical density. When light enters a denser medium (say, water) coming from one that is less dense (say, air), it bends toward a line normal to the boundary between the two media as illustrated in Figure 5.16. The deviation is greater for shorter wavelengths. The ratio of the speed of the light going from one material into another material is proportional to the ratio of the sine of the angle of incidence and the sine of the angle of refraction as illustrated in Figure 5.16. This is the socalled Snellius law [1621; also Willebrord Snell (1580−1626)]: sin(i) n 1 sin(r ) n 2
(5.19)
with i being the angle of incidence and r the angle of refraction, n1 is the index of refraction of material 1, and n2 is the index of refraction of material 2. Two familiar examples to demonstrate refraction are a pencil in a glass of water (Figure 5.17) and a rainbow (Figure 5.18). In Figure 5.17 we show a pencil in a glass: first in an empty glass, then in one with water (positive refractive index), and then in a glass filled with a negative refractive index material. S
i Air
R
309
At the boundary between air and water, the light wave changes direction; its wavelength increases or decreases, but its frequency remains constant. We will see in the next section that the refractive index of a medium is related to the speed of light and that in a denser medium a “slowdown” of the light occurs relative to the speed of light in free space. When light slows down it appears bent. The case of negative refractive index water (Figure 5.17c) will be discussed further below under “The με Quadrant and Metamaterials.” A bright vividly colored rainbow as shown in Figure 5.18 is caused by dispersion of sunlight refracted by raindrops between 0.1 and 2 mm in diameter where geometric optics applies. Complex Mie scattering effects are important for smaller drops, which do produce white fog (see further below). The light is first refracted as it enters the surface of the raindrop, reflected off the back of the drop, and again refracted as it leaves the drop. This angle is independent of the size of the drop but depends a lot on its shape and refractive index.
Definition of Refractive Index Maxwell demonstrated that for electromagnetic (EM) waves the wave velocity v in a homogeneous, isotropic dielectric medium is determined by the magnetic permeability μ, and the dielectric constant (or permittivity), ε (for the detailed derivation see further below): 1 (5.20) v EM
H
Water r A
C
FIGURE 5.16 Snellius law illustrated: the ratio of the horizontal length, RH, to the diagonal, RA, is just the sine of the angle RAH, which is equal to the angle of incidence i measured from the line drawn perpendicular to the refracting surface at R. Likewise, the ratio RH/RC is just the sine of the angle of refraction RCH, or r. Thus, Snell’s ratio RC/RA is the same as (sin i)/(sin r).
FIGURE 5.17 Refraction illustrated. (a) Empty glass: no refraction; (b) typical refraction with pencil in water with n = 1.3; (c) what would happen if the refractive index were negative with n = −1.3 (see “The με Quadrant and Metamaterials”). (From Gennady Shvets, The University of Texas at Austin.)
310
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
FIGURE 5.18 A rainbow is caused by dispersion of sunlight refracted by raindrops.
For a wave traveling in free space (where we use the permeability and dielectric constant for vacuum μ0 and ε0 instead of μ and ε) v = c = 2.998 × 108 m/s. The “slowdown” factor, relative to free space, is by definition the refractive index n: n
c v
(5.21)
or also: n = εμ 2
(5.22)
For example, because the speed of light in air is v 1 E air M air (with the permeability and dielectric constant for air given by μair and εair, respectively), the refractive index of air is given by: n
E air M air
c v
E0M 0
1.003
(5.23)
For most materials μ/μ0 = 1, so the expression for n E air c is often written out as n ). In Chapter 3, v E0 2 1
2 1 = c
2 1
2 1 < c
we saw how the dielectric constant ε in the most general terms is a dielectric function dependent on both frequency (ω) and wave vector k: ε(ω,k). There is also a dispersion function for the magnetic permeability [μ(ω, k)]; thus, from Equation 5.23 we can expect the refractive index n to be frequencydependent as well. When a material is subject to an applied electric field E, the internal charge distribution is distorted, which generates an electric dipole moment per unit volume called the electric polarization P. After introducing the Maxwell equations, we will link the dielectric function to this polarization P and to the dispersion of the refractive index n for metals, semiconductors, and dielectrics. Dispersion of light is most familiar with respect to dispersion of white light on a prism. If a beam of white light enters a glass prism, what emerges from the other side is a spreadout beam of manycolored light. The various colors are refracted through different angles by the glass and are “dispersed,” or spread out.
Reflectance and Total Internal Reflectance To illustrate reflectance and total internal reflectance (TIR) we show a sequence of four images from ray optics in Figure 5.19. A light beam goes from medium 1 (say, water with refractive index n1) into a medium 2 (say, air with refractive index n2) at different angles θ1. When the light coming from the water strikes the surface, part will be reflected and part will be refracted. Measured with respect to the normal line perpendicular to the surface, the reflected light comes off at an angle equal to that at which it entered, whereas that for the refracted light is larger than the incident angle. In fact, the greater the incident angle, the more the refracted light bends away from the normal. 2 = 90°
2 1
1 = c
1 1
1 1
(b)
(c)
2 1
1
1
1 > c
1 1
(a)
(d)
FIGURE 5.19 Illustration of reflection and total internal reflectance (TIR). Material 1 (bottom) has the higher index of refraction (n1 > n2). For explanation of (a)−(d), see text.
Photonics
Thus, increasing the angle of incidence from the path shown in Figure 5.19a to the one shown in Figure 5.19b will eventually reach a point where the refracted angle is 90°, at which point the light appears to emerge along the surface between the water and air (Figure 5.19c). If the angle of incidence is increased further, the refracted light cannot leave the water (Figure 5.19d). It gets completely reflected. The interesting thing about TIR is that 100% of the light gets reflected back into the denser medium, as long as the angle at which it is incident to the surface is large enough. At a given critical angle when θ1 = θc TIR occurs (Figure 5.19c); the light cannot escape medium 1 with refractive index n1 anymore, except for some really weak evanescent wave. Any light incident at an angle θ1 > θc is also totally reflected (Figure 5.19d). Thus, TIR is an effect that combines both refraction and reflection. The critical angle, also called the Brewster angle, named after the Scottish physicist Sir David Brewster (1781−1868), is given by: sin Qc
n2 n1
(5.24)
A common and useful application of TIR is in fiberoptics to keep light beams focused inside a fiber without significant loss (see Figure 5.20). Further below, after launching the Maxwell equations, we calculate the reflectance R in terms of the refractive index n.
Light Polarization Polarized light is light that has its electric vector (E) oriented in a predictable fashion with respect to Light rays
311
the propagation direction. Ordinary white light is unpolarized and made up of numerous orthogonal electrical and magnetic field pairs (E, B) that fluctuate at all possible angles around the propagation direction. Even in short time intervals, it appears to be oriented in all directions with equal probability. Light is considered to be “linearly polarized” when it contains waves that only fluctuate in one specific plane (see Figure 5.21). Linear polarization “tries to” induce a linear charge motion, but the Lorentz force prevents this from being purely linear. For example, charge oscillation along the xaxis introduces a small Ey component (field rotation. Specifying the orientation of one of the field vectors (E or B) determines the polarization of the EM wave. The plane containing the Efield vector defines the polarization of the EM wave. Of course, the Bfield vector would then always lie in a plane perpendicular to this plane containing the Efield vector. But according to theoretical and experimental evidence, it is the electric vector (E) rather than the magnetic vector (B) of a light wave that is responsible for all polarization effects. Therefore, the electric vector of a light wave, for all practical purposes, can be identified as the light vector in this respect. The simplest way of producing linearly polarized light is by reflection from a dielectric surface. In the preceding section we learned that when light strikes a material such as glass, part of the light might get reflected and part of it refracted. Reflection also causes the light to become unpolarized, partially polarized, or completely polarized, depending on the angle at which the light strikes the surface, or the angle of incidence (see Figure 5.22). The light Vibration direction (VD) E Wavelength,
Total internal reﬂection
Travel direction (TD) B
Polarized light E
Core
Cladding
FIGURE 5.20 A fiberoptic is based on the principle of total internal reflectance.
Unpolarized light E E E E E
E
E
E E
E
F
FIGURE 5.21 Unpolarized and polarized light.
312
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
1
B
B
2 2
FIGURE 5.22 Reflection causes the light to become either unpolarized, partially polarized, or completely polarized, depending on the angle at which the light strikes the surface, or the angle of incidence. The angle θB is known as the polarizing angle, or the Brewster angle.
is unpolarized only if the incident light angle is 0°, which does not occur often. It is more common that polarization does occur, and the greater the angle of incidence, the greater the polarization. When the light strikes at an angle θB of 90° or perpendicular to the surface, the light is completely polarized. At this particular angle of incidence the reflectivity for light whose electric vector is in the plane of incidence becomes zero. Thus, the reflected light is linearly polarized at right angles to the plane of incidence. This angle θB is known as the polarizing angle, or the Brewster polarizing angle, because it was discovered by the same David Brewster of the critical angle θc (see previous section): tan QB
n2 n1
(5.25)
Certain natural materials absorb linearly polarized light of one vibration direction much more strongly than light vibrating at right angles. Such materials are termed dichroic. Tourmaline is one of the bestknown dichroic crystals, and tourmaline plates were used as polarizers for many years. Dichroic crystals were studied by Edwin Land in 1930; Land invented a polarizing material that would be called Polaroid and give a huge benefit to the camera industry. Polarization of light is also possible by refrac tion, in which case the light is bounced off of numerous surfaces, instead of only one. Often a stack of
thin films of a transparent material is used for this purpose. The beam of light that is refracted is continuously polarized because refraction causes polarization. Because of this polarization, the beam of light that is refracted is shown to increase in intensity. Polarization obviously occurs frequently: even the light from a rainbow is polarized because the angle of incidence of light off a water beam is similar to a Brewster angle. Other natural materials exist in which the velocity of light depends on the vibration direction. These materials are called birefringent. We will discuss these in more detail after we have introduced the Maxwell equations. Circular (and elliptical) polarization is possible because the propagating electric (and magnetic) fields can have two orthogonal components with independent amplitudes and phases (and the same frequency). The electric vector, at one point in time, describes a helix along the direction of wave propagation. Circular polarization may be referred to as right or left, depending on the direction in which the electric field vector rotates. The magnitude of the electric field vector is constant as it rotates. Circular polarization is a limiting case of the more general condition of elliptical polarization. A circularly polarized wave may be resolved into two linearly polarized waves, of equal amplitude, in phase quadrature (90° apart) and with their planes of polarization at right angles to each other. Such polarization occurs in chiral* materials, for example, with helical polarizable molecules in a solution.
Maxwell’s Equations Introduction As stated earlier, ray optics is a significant simplification of optics and fails to account for many important optical effects such as diffraction and polarization. The latter phenomena are only understood properly from Maxwell’s equations. Light
*
Definition of chirality by Kelvin: “I call any geometrical figure, or group of points, chiral, and say it has chirality, if its image in a plane mirror, ideally realized, cannot be brought to coincide with itself.”
Photonics
with its wave and particle character is not the easiest of natural phenomena to describe. Its ambivalent nature requires two complementary models for a satisfactory description of its properties. In Chapter 3, we mentioned how Dirac’s quantum field theory removed the paradox of particlewave duality: it showed that if a particle was probed in a way that was meant to demonstrate its particlelike properties, it would appear to be a particle, and if it was probed in a way that was meant to demonstrate its wavelike properties, it would appear to be a wave. Maxwell’s electromagnetic (EM) wave model, the topic of this chapter, follows logically from Dirac’s model and describes light as a continuous transfer of energy through space by a combination of waves of electrical and magnetic fields. The Scottish physicist James Clerk Maxwell (1831−1879) unified in one magnificent theory— four elegant equations—all that was known of electricity and magnetism. For the first time it became apparent that EM fields could travel through space, and the theory suggested the revolutionary concept that light was nothing but an EM wave itself. Maxwell’s equations are even more fundamental than Newton’s three laws of motion because they agree with Einstein’s relativity theory, whereas Newton’s laws do not. The refractive index of a material as introduced above comes about through the interaction of light with many, many atoms (1022 atoms/cm3), and it is impossible to describe the individual response of so many electrons and atoms. So we have to make do with “effective” materials properties, such as the refractive index, an average over many atoms. This works very well for many materials because atom spacings in solids are much smaller than the wavelength of the light at hand. For visible light, e.g., green light, a volume of λ3 corresponds to a volume of ∼ (500 nm)3 ∼ (5 10 −5 cm)3 ∼ 10 −13 cm3, and the number of atoms in such a volume ∼10 −13 × 1022 = 109! So working with spatially averaged fields will give good results in many cases. Before we launch into the Maxwell’s equations for plane wave EM radiation, we remind the reader of some important vector relations. Because both the electric field and the magnetic field have a direction, we describe light as vector fields. Two important
313
integral theorems we need for manipulating those equations are Gauss’ divergence theorem and Stokes’ theorem. We also introduce Ampère’s law, Gauss’ electric and magnetic laws, and Faraday’s law, as they are the foundation for Maxwell’s famous unifying equations.
Gauss and Stokes Theorems The first theorem we introduce, the divergence theorem, comes from vector calculus and is also known as Gauss’ (1777−1855) or Green’s (1783−1841) theorem. The divergence of a vector field is a scalar (a number) and represents the net outward flux per unit volume (one can think of it as a “source density”). The divergence theorem relates volume and surface integrals and expresses the fact that the volume integral of the divergence of any conservative vector (or tensor) field equals the total outward flux of the vector through the surface that bounds the volume (http://mathworld.wolfram.com/ConservativeField. html). More simply stated: the sum of all sources minus the sum of all sinks gives the net flow out of a region. Mathematically:
°
v
Adv
t° A ds s
(5.26)
where A is a vector field or tensor field (for example, A could be a stress tensor S or an electric field vec tor E); ds is a differential vector element of surface area S, with infinitesimally small magnitude and direction normal to surface S; and dv is a differential element of volume V enclosed by surface S. We remind the reader that in vector analysis ∇ ⋅ A is the same as div A. This equation applies to any volume V bounded by surface S. Effectively this comes down to saying that “field lines are conserved.” We see where field lines originate on the left side of the equation or count them as they leave through the surface on the right side of the equation (Figure 5.23). The second theorem we need to refamiliarize ourselves with is Stokes’ theorem, or the curl theorem. It is named after Sir George Gabriel Stokes (1819−1903), although the first known version of the theorem is by William Thomson (Lord Kelvin). Stokes’ theorem deals with the problem of a 3D
314
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology Surface (S)
ds
ds
Contour (C)
+ + ++ + + + + Q + + + V
dl
D
S
+
FIGURE 5.23 The divergence or Gauss’ theorem illustrated for the case where A is equal to D, the electric displacement which is related to the electric field E via a materialsdependent constant called the permittivity, ε (as given by the constitutive relation, D E E ; Equation 3.38 in Volume I). Consider a total amount of charge Q in a volume V bounded by the closed surface S. The area integral gives a measure of the net charge enclosed, and the divergence of the electric displacement gives the density of the sources (see Equations 5.34–5.36 below).
FIGURE 5.24 Illustrating Stokes’ law. S is an open surface bounded by a closed curve C.
With Gauss’ and Stokes’ theorems Maxwell’s equations can be transformed from differential format to integral, and vice versa.
Ampère’s Law, Gauss’ Electric and Magnetic Laws, and Faraday’s Law Ampère’s Law Ampère’s law states:
curve in space, and the line integral around such a curve; it relates a surface integral to a line integral:
° ( s A) ds t° S
C
A dl
The magnetic circulation around a closed loop is proportional to the net electric current flowing through the loop, including the actual flow of electric charge as well as the displacement current, which is the time derivative of the electric flux. The positive directions of circulation, current and flux are related by the righthand rule.
(5.27)
where S is an open surface bounded by a closed curve C, and dl is a differential vector element of path length tangential to contour C enclosing surface area S. The vector ds is an outward surface normal vector of magnitude ds. Stokes’ theorem says that if S is a surface in three dimensions having a closed curve C as its boundary, then the surface integral of the curl of a vector field over that open surface equals the closed line integral of the vector along the contour C bounding the open surface. Integrating the curl across a surface gives the same answer as integrating the tangential vector components along the line bounding that surface. Also, rotation in adjacent spots cancels out, and what is not canceled is present at the edge of the surface. This is a fairly remarkable theorem because S can be any surface bounded by the curve C and have just about any shape (Figure 5.24). We remind the reader that in vector analysis ∇ × A, rot A, and curl A are equivalent notations. Another way of saying this is that the curl of a field defines the “amount of rotation” in a field.
An electric current J running through a straight wire generates a magnetic field strength H (in A/m) around that wire (Figure 5.25). The integral of H along the circular path C is equal to the current I, which in turn can be obtained as the integral
H
S J D H
J
C D increasing when the capacitor is charged
FIGURE 5.25 Ampère’s law illustrated. The magnetic field is induced by electrical currents (J) and changes in electric field, uD (the displacement current is also called Maxwell’s ut displacement D).
Photonics
of the current density J across the crosssection of the wire:
t° H dI I ° J ds C
(5.28)
S
This is the original Ampère’s Law (1775–1836). Using Stokes’ theorem (Equation 5.27) we transform Equation 5.28 to:
° ( s H) ds I ° J ds S
(5.29)
S
From the latter expression it follows that: ∇×H=J
(5.30)
James Clerk Maxwell made an important correction to Ampère’s law; he recognized that a changing uD , is equivalent to a current J, and he electric field, ut uD the displacement current. The electric flux called ut density, also called Maxwell’s displacement D, is expressed in units of As/m2. The more general Ampere’s law, in which a changing electric field ¥ uD ´ ¦§ µ and a current (J) both produce a magnetic ut ¶ field (H), is then given as: sH J
uD ut
(5.31)
The electric displacement D, expressed in coulombs per square meter (C/m2) is related to the electric field E (in units of V/m) via the permittivity, ε (ω,k), as: D = ε(ω,k)E
(3.37)
The permittivity ε (As/Vm) is a scalar if the medium is isotropic or a 3 × 3 matrix otherwise, and its frequency dependence defines the socalled dielectric function, i.e., ε(ω,k). To obtain εr(ω,k), the relative dielectric response of a material, one divides by ε0 because ε(ω,k)/ε0 = εr(ω,k). Similarly, the magnetic field or flux density B is linked to the magnetic field strength H (in A/m) within the material through a second constitutive relation: B = μH
(5.32)
with μ = μ0μr and μr the dimensionless relative permeability. The magnetic permeability μ is a tensor
315
that reduces to a scalar in isotropic materials. The magnetic inductive capacity, μ, or permeability, is related to the ability of a medium, such as air, to store magnetic potential energy. The permeability of vacuum, μ0, is 1.257 × 10 −6 Hm−1, and in the case of air is μair = 1.260 × 10 −6 Hm−1. As in the case of the dielectric “constant” the response of the relative magnetic permeability μr of normal media to externally applied fields depends on the frequency of the field as well and on the wave vector, i.e., μr(ω,k). A third constitutive relation, the basis of Ohm’s law (V = IR), introduced in Chapter 2, links current density J (A/m2) to electrical conductivity σ (in A/Vm) of the material: J = σE
(2.2)
In the most general case, the electrical conductivity σ is a secondrank tensor and is also frequencydependent, i.e., σ(ω,k). For an isotropic material, σ becomes a scalar. Gauss’ Law for Electric Fields Gauss’ law for electric fields states: The net electric flux exiting a closed surface is proportional to the net electric charge enclosed by the surface.
Gauss’ law is an extended form of Coulomb’s law. Both Coulomb’s and Gauss’ laws relate electric fields to charges: charges make electrical fields. Consider a total amount of charge Q in a volume V bounded by a closed surface S. The electric charger Q equals the surface integral of the electric flux density over the closed surface S:
t° D ds Q S
(5.33)
With the divergence theorem this can be rewritten as:
t° D ds ° Ddv S
v
(5.34)
or also:
°
V
Ddv Q ° RV dv
(5.35)
V
and finally one obtains: ∇ ⋅ D = ρv
(5.36)
316
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
where ρV is the electric charge per unit volume (C/m3). For linear materials, D = ε E (Equation 3.38) and Equation 5.36 can be rewritten as: RV E E
(5.37)
From Equation 5.37 we can derive the socalled Poisson equation for the potential: Rv V E 2
(5.38)
because E = −∇V. In the case that the total charge density is zero, Equation 5.38 reduces to Laplace’s Equation: 2
∇ V=0
Faraday’s Law Faraday’s law states: The electric circulation (or emf) around a closed loop is proportional to the negative time derivative of the magnetic flux through the loop, where the positive circulation and flux directions are related by the righthand rule.
Faraday (1791−1867) discovered that a voltage V (or emf) is induced in a coil when a magnetic flux Φ [Webers (Wb)] in the environment changes with time, and he formulated a law stating that a changing magnetic field ¥ uB ´ produces an electric field (E): ¦§ ut µ¶
(5.39)
t°
C
marking a constant electric field.
uB ds S ut
E dl °
With Equation 5.27 (Stokes) we rewrite this expression as:
Gauss’ Law for Magnetic Fields Gauss’ law for magnetic fields states:
uB ds S ut
° ( s E) ds ° S
The net magnetic flux exiting a closed surface is always zero.
We know that magnetic poles always occur in pairs (north and south). Therefore, a magnetic field will be produced in space if there is a changing electric field, but this magnetic field is changing as the electric field is changing. A changing magnetic field produces an electric field that is changing—in other words, we have a selfperpetuating system. Because a single magnetic charge does not exist, the equivalent expression to Equation 5.33 for magnetism reads:
t° B ds 0 S
(5.40)
This means that the magnetic field lines must form closed loops, i.e., the mathematical formulation of the fact that the field lines cannot originate from somewhere or that there are no magnetic monopoles. Using Gauss’ theorem we obtain:
t° B ds ° S
V
Bdv 0
(5.41)
In other words: ∇⋅B=0
(5.43)
(5.42)
(5.44)
or: sE
uB ut
(5.45)
Finally, we introduce the continuity equation for the conservation of charge. Say that in a time dt, a charge dQ is lost from volume V; because of this flux of charge, a current density J leaves the surface element ds. We use the divergence theorem to convert the integral over the surface S into an integral over the volume V. We assume that the volume does not change, so only the charge density ρ in the volume changes. This leads to the continuity equation: uRV J 0 ut
(5.46)
From Equation 5.46 the current density flux flowing out of a closed surface equals the rate of decrease of the positive charge density. Example 5.1: Place some charges on a conductor with a conductivity σ; how long does it take for the charges to spread? From the continuity uR relation (Equation 5.46) we have J V . In ut the conductor we have Ohm’s law stating J = σE
Photonics
E 0
uR (Equation 2.2), and because S E V and ut ¥ R´ using Poisson’s equation ¦ E µ , the solu§ E¶ tion is: R R0 e
t T
° E ds 0
(5.47)
B 0
with the time constant τ = ε/σ With typical values for ε and σ one obtains a τ of 1.5 10 −19 s. Thus, charge density decays exponentially with time. For a very good conductor, charges flow instantly to the surface to form a surface charge density and (for timevarying fields) a surface current is established. Inside a perfect conductor (σ → ∞) and E = H = 0.
t° B ds 0
sE
C
Maxwell’s Elegant Summary
uE s B M 0 E0 ut
C
uE ds S ut
B dI M 0 E 0 °
S
uB ut
(5.50b)
(5.51a)
uB ds ut
Faraday
(5.51b)
where E (in V/m) is the electrical field strength and B (in Tesla, T, or kgA−1s−2) the magnetic flux density, and μ0 and ε0 the permeability and electric permittivity of free space, respectively; dl is a line element, and ds a surface element. The permittivity of free space, ε0, is 8.854 pF/m. The permeability of vacuum, μ0, is 1.257 10−6 H m−1. Vacuum is a linear, homogeneous, isotropic, and dispersionless medium. Except for a multiplicative scalar, electric and magnetic fields appear in these equations with remarkable symmetry, and this mathematical symmetry implies physical symmetry. We note here that the four Maxwell equations are not independent. In fact, the two divergence equations can be derived from the two curl equations. The timevarying Maxwell’s equations, in a medium and in the presence of charges and currents, in their differential and integrated forms are given as: sH J
t°
C
H dI
¥
° ¦§ J S
uD ut
uD ´ ds ut µ¶
Ampere
D RV
(5.48c)
(5.48d)
(5.49c)
(5.48a)
° D ds Q S
t°
E dI °
(5.49b) (5.50a)
Magnetic Gauss
S
t°
It was in 1864 that Maxwell summarized the above set of equations for all frequency ranges and size scales larger than atoms. He was the first to show that the four equations describing electric and magnetic fields could be rearranged to form a wave equation, with a speed of propagation equal to the speed of light. Maxwell also corrected Ampère’s law by introducing an additional term for the displacement current (changing electric fields act like currents, likewise producing magnetic fields; see above). The elegant modern mathematical formulation introduced here is by Oliver Heaviside (1850–1925), who in 1884 reformulated Maxwell’s equations using vector calculus. His more symmetric mathematical representation reinforces the physical symmetries between the magnetic and electrical fields. Maxwell’s equations, as remarked earlier, can be transformed from differential format to integral representation, and vice versa, by using the theorems from Gauss and Stokes. Remarkably, as we will see below, Maxwell’s equations are perfectly consistent with the transformations of special relativity. Maxwell’s equations in the absence of electric charge density ρ (in units of C/m3 = 0) and current J (in units of A/m2) in a vacuum in differential and integral form are:
(5.49a)
Electrical Gauss
S
317
Ampere (5.48b)
Electrical Gauss
B 0
(5.49d) (5.50c)
318
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
t° B ds 0
Magnetic Gauss
S
C
E dI °
S
uB ds ut
(5.51c)
Faraday
1. Diverging D fields relate to charges: ∇ ⋅ D = ρV 2. Diverging magnetic flux does not exist: ∇ ⋅ B = 0 The curl equations state that changes in magnetic fluxes give rise to electrical fields and changes in currents give rise to H fields or changing E field results in changing H field, which results in changing E field. . . . (Figure 5.26): 3. Rotating E fields relate to changing currents: uB sE ut 4. Rotating H flux lines relate to changing D, and several currents could be added (e.g., magnetiuD zation): s H J ut If we now consider solutions for timeharmonic electric and magnetic fields (e.g., sinusoidal) and replace the time derivative ∂/∂t by −iω [because u iWt e iWe iWt ], we arrive at the following ut Maxwell expressions: (5.48e) s H J iWD
C
H dI
°
S
J iWD
Ampere
D RV
° D ds Q S
Electrical Gauss
Magnetic ﬁeld
Magnetic ﬁeld
Magnetic ﬁeld
(5.51d)
where D [in coulombs per square meter (C/m2)] is the electric displacement, H (in A/m) is the magnetic field strength, J is current density (A/m2), Q (C) is the total charge, and ρV is the volume density of free electric charges (C/m3). Note that no constants such as μ0, ε0, μ, ε, c, χ … appear when the equations are written in this way. The divergence equations basically say that flux lines start and end on charges or poles:
t°
Electric ﬁeld
Electric ﬁeld
Curent
uB sE ut
t°
Electromagnetic wave
(5.50d)
(5.48f) (5.49e) (5.49f)
Direction
FIGURE 5.26 Changing E field results in changing H field, which results in changing E field.
B 0
t° B ds 0
(5.50e)
Magnetic Gauss
S
(5.51e)
s E iWB
t°
C
E dI iW ° B ds S
(5.50f)
Faraday
(5.51f)
Boltzmann was so impressed with Maxwell’s equation that he used a quotation from Goethe to describe them: “War es ein Gott der diese Zeichen schrieb?” (Is it a God who has written these signs?). These equations, together with the continuity equation (Equation 5.46), the Lorentz force* (Equation 3.64), and the constitutive equations for ε, μ, and σ, form the foundation of all macroscopic electromagnetic phenomena. In the case of no time variation (∂/∂t = 0), the Maxwell equations describe electrostatics and magnetostatics as summarized in Table 5.1. In the next section we will find that Maxwell’s equations allow for solutions that have the form of propagating plane waves, and that the wavelength is affected by the amount of polarization P of the material, leading to a refractive index n.
Plane Wave Solutions of Maxwell’s Equations Plane Wave Propagation Earlier we saw how electromagnetic (EM) plane waves are observed when moving far enough away from the source, just like dropping a rock in a pond and looking at waves a few hundred feet away from the *
An electric charge moving in the presence of an electric and a magnetic field experiences a vector force per unit charge that is equal to the sum of the electric field and the cross product of the velocity with the magnetic field.
Photonics
TABLE 5.1 Electrostatics (Capacitor Equations) and Magnetostatics (Inductor Equations) Magnetostatics ∇ ⋅ D = ρV ∇×E=0
∇⋅B=0 ∇×H=J
t° D ds Q
t° B ds 0
t°
t°
S
C
E dl 0
Electrical capacitance (in Farad) C = Q/V
both are zero) from the Maxwell equations. Taking the curl of Equation 5.51c leads to the homogenous vector wave equations (Equations 5.53 and 5.54) for electromagnetic (EM) radiation in such a medium we obtain: u( s B) ut L.H.S: ( E) 2E 2E ( E 0; Equation 5.49a) u 2E R.H.S: ME 2 (Equation 5.48c with u t J 0 and D EE and B MH)
S
C
s ( s E)
H dl I
Electric inductance (in Henry) L = Φ/I*
Φ is magnetic flux, and I is current.
*
impact point so that the wavefronts are essentially flat. When close enough to the EM source the radiated field must be considered mathematically spherical rather than planar. The first situation is called far field, and the second is near field (Figures 5.4 and 5.5). In Chapter 2, we defined a plane wave,* ei(krcot), as a wave that is constant in a plane perpendicular to k (in rad/m) and is periodic parallel to it. The wave number or wave vector k measures the number of wavelengths in a complete cycle; thus, it has a value of 2π/λ, and ω = 2πv = ck (free space) is the period of the wave. In the plane wave, equation r is the 3D position vector. A bit simpler: a plane wave is a continuous wave (CW) whose amplitude and phase are constant in the directions transverse to the propagation direction. We will now embark on a discussion of the interaction of light with materials. In optical experiments one measures reflectivity, transmission coefficient, luminescence, or light scattering to learn a great deal about energy band structure, impurities, phonons, defects, etc. In particular, optical measurements are used to determine the complex dielectric or complex conductivity, which is directly related to band structure.
or 2E ME
*
The complex exponential representation for periodic functions is convenient for adding waves, taking derivatives of wave functions, and so on. It is equivalent to a linear combination of a sine and cosine function because e iθ = cos θ + i sin θ (Euler’s formula).
u 2E u2 t
(5.52)
(5.53)
and similarly 2B ME
u 2B u2 t
(5.54)
For the lefthand side (L.H.S.) of Equation 5.52 we used the “BACCAB” rule.† Equations 5.53 and 5.54 represent wave equations for electromagnetic (EM) waves in bulk materials. In free space, μ and ε in these equations are replaced by μ0 and ε0. The 2 Laplacian ∇ operates on each component of E and B, so that the two vector equations (Equations 5.53 and 5.54) represent six 1D, homogeneous scalar wave equations. One of these expressions, the Ex component, in Cartesian coordinates, is written out as: u 2E x u 2E x u 2E x u 2E x EM ux 2 uy 2 uz 2 ut 2
(5.55)
Therefore, each component of the EM field (Ex , Ey, Ez, Bx , By, Bz) obeys a generic scalar differential wave equation of the type:
Wave Equations for a Medium without Charges or Currents We now derive the wave equations for plane wave propagation in a simple linear isotropic, homogeneous, nonconducting medium characterized by ε and μ without any charges or currents present (sourcefree region, i.e., a region where ρV and J
319
u29 u29 u29 1 u29 ux 2 uy 2 uz 2 v 2 ut 2
(5.56)
provided that the following important identity holds: v=
†
1
(5.20)
EM
We are taking advantage in this derivation of the “BACCAB” rule: A × (B × C) = B(A ⋅ C) − C(A ⋅ B), or in the current case: ∇ × (∇ × E) = 2 ∇(∇ . E) − (∇ . ∇)E = −∇ E.
320
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
The velocity v, the propagation speed of the wave, is solely determined by the medium. For a wave traveling in free space we substitute the values for μ0 and ε0 in Equation 5.20 and calculate the speed for all EM waves as v = c = 2.998 108 m/s. At the time of Maxwell, the values for μ0, ε0, and c were uncertain enough that the correspondence between c and Equation 5.20 was not all that definitive. However, it was close enough that Maxwell wrote in 1864: “This velocity is so nearly that of light that it seems we have strong reason to conclude that light itself (including radiant heat and other radiations) is an electromagnetic disturbance in the form of waves propagated through the electromagnetic field according to electromagnetic laws.” It is largely for this reason that this whole set of equations is named after Maxwell. When Heinrich Hertz (1857–1894) produced lowfrequency radio waves (lowfrequency light) and demonstrated that these waves were identical in all respects to light, save frequency, he confirmed Maxwell’s hypothesis. It was also Hertz who, in 1887, discovered the photoelectric effect (see Chapter 3). Maxwell’s equations show that electric and magnetic forces travel at a definite predicted speed—this is not instantaneous “action at a distance.” James Clerk Maxwell’s Treatise on Electricity & Magnetism (1873) is the last word on classical electricity and magnetism and ranks with Newton’s work as one of the great accomplishments of physics. Newton’s and Maxwell’s equations describe all “classical physics.” In Chapter 3 we introduced Bohr’s correspondence principle, according to which the predictions of the quantum theory must also cover the predictions of the classical theories of physics. In other words, the above equations derived here from Maxwell’s equations should also be a solution of Schrödinger’s equation. We demonstrated that this is so in Chapter 3, “Solution of the Wave Equation for Free Particles.”
equations to obtain the following two equivalent expressions (using the BACCAB rule again): s ( s E) ( E) 2E M
uJ u 2D uE u 2E
M 2 MS
ME 2 ut ut ut ut
2E MS
¥R ´ uE u 2E
ME 2 ¦ v µ ut § E¶ ut
(5.57)
uH u 2H
ME 2 0 ut ut
(5.58)
and similarly: 2H MS
In solving these equations, one often invokes the electric scalar and the magnetic vector potential. The magnetic vector potential A (in Weber per meter) is related to B as: B=∇×A
If one can find A for a given current distribution, then B can be obtained by taking the differential (curl) from A. This is similar to obtaining the electrical field E from the scalar electrical potential V (E = −∇V). Substituting Equation 5.59 into the differential Faraday expression (Equation 5.51a) gives: sE
To obtain the most general wave equations—in the presence of sources (charges, ρ) and a current (J) in a medium—we first combine the constitutive relations with the general timevarying Maxwell’s
u ( s A) or ut
(5.60)
uA s (E )0 ut The electric field intensity stems from both charge accumulations (through the −∇V term) and from the timevarying magnetic field (through the − uA term), ut or: E
Wave Equations for a Medium with Charges and Currents
(5.59)
uA
V ut
(5.61)
uA 0), this reduces back to ut the familiar E = −∇V, so that we can obtain E from V alone and B from Equation 5.59. With varying fields, E depends on both V and A. The inhomogeneous For the static case (with
Photonics
vector potential wave equation to be solved then becomes:
2 A MS
uA u2 A ME 2 MSV ut ut
(5.62)
Using the constitutive equations and substituting Equations 5.59 and 5.61 into 5.48e, we obtain: s s A MJ ME
u uA (
V) ut ut
(5.63)
or also: ¥ u A uV ´ MJ ¦¦ A ME µµµ 2 ¦ ut µ¶ ut §
(5.64)
By choosing the divergence of A such that: A ME
uV 0 ut
(5.65)
which is the socalled Lorentz condition for potentials (for static fields this condition becomes ∇ ⋅ A = 0). The Lorentz condition enables us to simplify Equation 5.64 to: u2 A A ME 2 MJ ut 2
(5.66)
This is the nonhomogeneous wave equation for vector potential A; solutions are waves traveling with 1 . The corresponding wave a velocity v equal to ME equation for the scalar potential V is obtained by substituting Equation 5.61 in Equation 5.49c, or:
E(V
uA ) RN ut
(5.67)
u R V ( A) N ut E
(5.68)
With the Lorentz condition (Equation 5.65) applied, this leads to: 2 V ME
u2 V R N 2 E ut
The Overall Solutions Are Plane Waves: E(r,t) = Emei(k ⋅ r – ωt) and B(r,t) = B ei(k ⋅ r – ωt) The solutions of the wave m equations for plane wave propagation in a simple linear isotropic, homogeneous, nonconducting medium (ρV and J both are zero) characterized by ε and μ (Equations 5.53 and 5.54) in one dimension (say with the E field propagating along the zaxis, the B field along y, and the propagation vector in the xdirection) are: E(r ,t) E m e i(k x x Wt ) and B Bm e i(k x Wt )
(5.69)
This result represents nonhomogeneous wave equation for the scalar potential V. Both wave equations
(5.70)
Rewriting these expressions in sines and cosines instead of the complex variable form (e x = cos x + i sin x), one obtains as the simplest form of a light wave: E = E msin(k x x − ωt) and B = Bmsin(k x x − ωt) (5.71) Generalizing for 3D, Equation 5.70 converts to: E(r ,t) E m e i(k r Wt ) and B(r ,t) Bm e i(k r Wt )
With ε constant this can be written out as: 2
(Equations 5.66 and 5.69) reduce to the Poisson’s equations in static cases. The above derived wave equations are the basis for modeling electromagnetic fields in microelectromechanical systems (MEMS) and nanoelectromechanical systems (NEMS). For more details on deriving and working with Maxwell’s equations, consult David K. Cheng’s Field and Wave Electromagnetics1 and Minoru Taya’s Electronic Composites.2 Plane Wave Solutions for Media without Charges or Currents
2
2 A ME
321
(5.72)
with r the 3D position vector and k a complex propagation constant, with the real part of it corresponding to the wave vector and the imaginary part corresponding to the absorption (analogous to our treatment of xrays in Chapter 2). The complex propagation constant k is obtained by substitution of this solution in the wave equations (see Equations 5.53 and 5.54). It should be noted that plane waves are not the only solutions to Maxwell’s equations; the differential
322
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
wave equation allows many solutions, including spherical waves. Constraints to the Plane Wave Solutions: E ⊥ k and B ⊥ k (I) Let us assess what we have so far: the sourcefree Maxwell equations (Equations 5.48a– 5.51a) were manipulated in such a way as to obtain the vector wave Equations 5.53 and 5.54, and solutions for these equations are given by E(r ,t) E m e i(k r Wt ) and B(r ,t) Bm e i(k r Wt ) (Equation 5.72). But we are not done yet: in addition to satisfying the vector wave equation, we must also verify these solutions satisfy the other Maxwell equations. We can write down lots of functions that satisfy the wave equations but that are not valid electromagnetic fields for the given boundary conditions (ρV and J both are zero). We first plug these proposed solutions into the divergence Equations 5.49a and 5.50a to find the following additional constraints: E 0 (Equation 5.49a) m k E 0
(5.73)
B 0 (Equation 5.50a) m k B 0
(5.74)
In other words, the divergence equations require that the electric and magnetic fields are orthogonal to the propagation direction: E ⊥ k and B⊥ k. The E and B fields have no component of vibration in the direction of propagation: there are no longitudinal components, or E and B are exclusively transverse in nature. Constraints to the Plane Wave Solutions: E ⊥ B ⊥ k (II) Let us now substitute these same solutions in the curl equations (Equations 5.48a and 5.51a) and establish how this adds the following constraints: s E
s B ME
uB (Equation 5.51a) }} m k s E WB ut (5.75) uE W (Equation 5.48a) }} mk s B 2 E ut c (5.76)
uE one of the curl equations: ut on the righthand side, we have the time derivative of E, pointing in the same direction as E because the time derivative does not change the vector’s direction. Consider s B ME
On the left, we have ∇ × B; this is perpendicular to B because the curl of any vector is orthogonal to that vector. Therefore, the first thing the curl equations tell us is that radiation’s electric and magnetic fields are orthogonal to each other. Second, the curl equations also require that E × B is parallel to the propagation vector k. In other words, the symmetry of Maxwell’s equations results in E ⊥ B ⊥ k as illustrated in Figure 5.1. In electromagnetic waves, the E and B fields are obviously intimately linked. To test this further, let us try out the solutions, E x E m e i(k x Wt) and B y Bme i(k x Wt) [E along the zaxis, B along the yaxis, and propa· gation direction k along the xaxis ¥¦¦ uE x 0´µµ¸ in µ¶¸ § ux ¹ Equation 5.51a, which leads to: sE
uB or ut
uB y uE z and thus E m (ik)e i(k x Wt) ux ut Bm ( iW)e i(k x Wt) or
(5.77)
Em W Bm k
For planar waves, k = 2π/λ and ω = 2πv = vk with v being the speed of the wave, and because E and B are in phase we conclude that E and B are related at any point in space by the velocity of the propagating wave: E W v B k
(5.78)
This relates the wave vector k, relating to phase variations in space, to ω, the angular frequency, relating to phase variations in time. In the case of a wave in free space, v = c = 2.998 × 108 m/s. Thus, boundary conditions for planar waves propagating in a medium without charges lead to Equation 5.78 expressing an important constraint for the proposed solution in a dispersion relation, i.e., a relation between the energy of the system and its corresponding momentum k (ω). In the case of free space, this is a linear function (ω = kc) with a slope c, the socalled light line (see Figure 5.27).
Photonics
Summarizing, we conclude that in a sourcefree region for timeharmonic signals Maxwell’s equations are reduced to two coupled curl equations, and these two curl equations combine to produce the wave equation for E or B. The eigenfunctions for these wave equations are plane waves described by propagation direction vectors called kvectors that have a length of 2π/λ and result in wave velocity v (the kvector is reciprocal to the space variation of the wavelength). The two curl equations have zero divergence, and this requires the vectors E and B to be perpendicular to the direction of propagation, whereas the E and B vectors must also be perpendicular to each other. In the section below on electromagnetic waves at boundaries, we will learn that to solve electromagnetic problems involving adjacent regions of different constitutive parameters, it is necessary to establish the boundary conditions that the field vectors E, D, B, and H must satisfy at the interfaces between the different optical materials. These boundary conditions, we will see, are established by applying the integral form of Maxwell’s equations to a small region at the interface of the contacting media. Plane Wave Solutions for Media with Charges or Currents We now substitute the timeharmonic electric field wave E(r ,t) E m e i(k r Wt ) = E m e ik r e iW t E r (r )e iW t in the most general wave equation for media with uE u2E
ME 2 (Equacharges and currents 2E MS ut ut tion 5.57). We will assume here nonmagnetic materials with μ = μ0 (remember that the magnetic permeability μ = μ0 ⋅ μr, where μr is the dimensionless relative permeability, which is 1 in this case) to obtain:
Substituting E r (r ) = E m e ik r in Equation 5.79 leads to the following constraint expressed in a new dispersion equation: k2
W2 E(W) v2
(5.80)
This is a relation between the wave vector k, related to phase variations in space, and ω, the angular frequency, related to phase variations in time. Note that a higher temporal frequency yields a higher spatial frequency, and a large permittivity will result in a large k (short wavelength). The “slowdown” factor of an electromagnetic wave in a material relative to free space is by definition the refractive c c index n (Equation 5.21). With n we can v v rewrite Equation 5.80 in terms of the refractive index n and the velocity of light in free space c as: n2 2 W or c2 n k W c k2
(5.81)
which in the case of free space with n = 1 simplifies back to ω = kc. Thus, the wave equation again imposes a constraint on the length of the kvector. Below we will analyze this dispersion relation in terms of the phase velocity of a wave (v p = ω/k = E/p) and the group velocity (vg = dω/dk = dE/dp) of that wave.
Characteristic Vacuum and Medium Impedance—η0 and η The vacuum impedance η0 is a universal constant relating the magnitudes of the electric and magnetic fields of electromagnetic radiation traveling through free space. From Equation 5.75: H0
2
323
E H
k 1 WM 0 M 0c WE E 0 c k
M0 E 0 (5.82)
2
E(r ) iWSE(r ) EW E(r ) W2 E(r ) 2 E(W)E(r ) v 2
with an effective dielectric contstant: iS E(W)) 1 W
(5.79)
which equals 376.73 ohms. More general, for a uniform plane wave the ratio of the magnitudes of E and H is the intrinsic impedance of the medium and is designated η. Again from Equation 5.75 it follows: H
E H
k WM WE k
M E
(5.83)
324
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Like the velocity of propagation, the intrinsic impedance is independent of the source and only determined by the properties of the medium.
vg
Dispersion Relations in Vacuum and in Media
k
In Vacuum In physics, the dispersion relation is the relation between the energy of a system and its corresponding momentum. Here we analyze the dispersion relation ω(k) from Equation 5.81 in terms of the phase velocity of a wave (v p = ω/k = E/p) and the group velocity (vg = dω/dk = dE/dp). Remember that the phase velocity of a wave (v p = ω/k = E/p) is not necessarily the same as the group velocity (vg = dω/dk = dE/dp) of that wave. Two velocities must be defined when dealing with multiple waves, with the phase velocity corresponding to the speed of the highfrequency components and the group velocity to the speed of a localized envelope. Also, the phase velocity of the wave is the rate at which the phase of that wave propagates in space, or it is the velocity at which the phase of any one frequency component of the wave propagates and the group velocity we saw earlier also corresponds to the light “particle” speed (Chapter 3). Because the group velocity vg is given as dω/dk, we calculate: vg
dv p dW d (kv p ) v p k dk dk dk
(5.84)
dv P = In a nondispersive medium such as a vacuum dk 0, the group and phase velocity is the same (v p = vg), or: W dW vp vg c k dk
FIGURE 5.27 The dispersion relation—the relation between the energy of the system and its corresponding momentum k(ω)—is a linear function of ω in the case of vacuum with a slope c = vg = vp.
In a Medium Dispersion occurs when the phase velocity vp depends on k (or λ), i.e., the group velocity does not equal the phase velocity (see Equation 5.85): dv p x 0 or v g x v p dk
(5.86)
A wave packet or group velocity with vg = dω/dk less than the phase velocity v p = ω/k is illustrated in Figure 5.28 for a case where vg = v p/2. We can rewrite the group velocity (vg = dω/dk) of light in a medium also in terms of refractive index n and the velocity of light c. For the group velocity we then derive for the most general case: vg
dW c dk n
c EM
(5.87)
c and n(W)2 EM vg (Equations 5.21 and 5.22), and the dispersion relation then becomes: where we used the fact that n(W)
k(W)
W n(W)W W EM c vg c
(5.88)
(5.85)
This is of course the same result we obtained earlier as a constraint when substituting a planar wave [E(r ,t) E m e i(k r Wt) ] in the wave equation for free uE space 2E ME 2 (Equation 5.53). Thus, the disu t persion relation—the relation between the energy of the system and its corresponding momentum k(ω)—is a linear function of ω with a slope c = vg = v p in the case of vacuum as shown in Figure 5.27.
We will use this important equation to construct a με quadrant to classify all materials according to their magnetic permeability μ and their dielectric constant (or permittivity) ε. From Equation 5.88 we can also calculate the group velocity vg as a function of the refractive index: vg
c c/n Wdn Wdn n 1 dW ndW
(5.89)
Photonics
325
positive for most frequencies (vg < vp). The exception is in regions of anomalous dispersion, regions that are not only dispersive but also absorbing, that is, near a resonance. To explain these anomalous regions we will introduce the Lorentz model further below. We can summarize the frequency dependence of the refractive index n shown here as follows:
λ0 y(x, t)
◾ Low frequencies: All transitions contribute their lowfrequency response ⇒ high n. ◾ Between resonances: n slowly increases = “normal dispersion.” ◾ Close to resonances: n rapidly decreases = “anomalous dispersion.” ◾ Above resonance, contribution vanishes ⇒ n(ω) mostly because of higher resonances. ◾ At high frequencies (∼xray wavelengths) n approaches 1. We more often think of the refractive index in terms of wavelength, so let us write the group velocity also in terms of the vacuum wavelength λ0. Using the chain rule we can write: dn dn dL 0 dW dL 0 dW
(5.91)
Now λ0 = 2πc/ω and:
2Pc
2Pc
L 02 dL 0 2 dW 2Pc W2 ¥ 2Pc ´µ ¦¦ µµ ¦§ L 0 µ¶
(5.92)
Substituting this in Equation 5.89, we obtain: FIGURE 5.28 A wave packet or group velocity with vg = dω/dk less than the phase velocity vp = ω/k with vg = vp/2. Phase velocity vp is marked by blue arrows, and the group velocity vg is marked with red dots.
and finally: vg
vp W dn 1 ndW
vg
c c/n Wdn L dn n 1 0 dW ndL 0
(5.93)
Right and LeftHanded Materials (Metamaterials) (5.90)
The group velocity vg equals the phase velocity when dn/dω = 0, such as in vacuum. Otherwise, because n usually increases with ω, dn/dω > 0 and vg is less than the phase velocity vp. This is illustrated in Figure 5.29, where we plot the refractive index as a function of ω. We see that the refractive index is
From Maxwell’s equations we derived that for planar waves with a positive μ and ε, the vectors E and H and k do constitute a right set of vectors and thus one defines righthanded materials (RHMs) as illustrated in Figure 5.30a. The direction of E × H is called the beam or ray direction. In vacuum and for most materials the “righthand rule” relates E, H, and k because normally
326
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
" #
!
!
!
!
FIGURE 5.29 Refractive index n as a function of frequency ω: n(ω). The refractive index is positive, so vg < vp for most frequencies! The exception is in regions of anomalous dispersion, absorbing regions near a resonance.
μ > 0 and ε > 0. But in 1968, Victor G. Veselago postulated that if the permittivity ε and permeability μ of materials are negative simultaneously, there is no violation of any fundamental physical rules, and the materials will have special optical properties.3 For a material with μ and ε negative, the vectors E and H and k form a left set of vectors, and one refers to them as lefthanded materials (LHMs) (Figure 5.30b). For lefthanded materials n(ω)2 = εμ (Equation 5.22) is modified to: n(W) p EM which for E 0 and M 0 (5.94) n(W) EM So we are forced by Maxwell’s equations to choose a negative square root for the refractive index. Because no naturally occurring material or compound has ever been demonstrated with both ε and μ negative, Veselago wondered whether this apparent asymmetry in material properties was just (a) If
then and is a right set
of vectors:
(b) If
then and is a left set of
vectors:
FIGURE 5.30 (a) Righthanded (RHM) and (b) lefthanded materials (LHM).
happenstance or perhaps had a more fundamental origin. From 1996 onward, strong theoretical and experimental evidence started emerging that lefthanded materials, now called metamaterials, could be fabricated (at least in the RF range, not yet in the optical range). In Figure 5.17 we show a picture of a drinking straw in a glass with a negative refractive index water n = −1.3 and observe an apparent bending of the straw in the opposite direction of what we are used to in the case of “normal” water. We will detail metamaterials further below. Whereas in conventional materials properties derive from their constituent atoms, in metamaterials properties derive from their constituent units. These units can be engineered as we please.
Birefringence—Double Refraction In the daily world we are most familiar with EM waves or light that propagates according to the righthand rule (k is in the E × H direction) as illustrated in Figure 5.30a. Materials in which this is the case are isotropic media, and the dielectric constant ε in the constitutive relation (D = ε E; Equation 3.38) in this case is a scalar. Glass is an example of an isotropic material because it does not matter how light passes through it. The characteristics of the glass are such so that it has no different effects on the light even though the direction of the beam varies. In nature one also has materials in which the direction of k is not exactly along the E × H direction; the angle between the two is then smaller than 90°. In mathematical terms, this means k ⋅ (E × H) > 0. These are optically anisotropic media, such as birefringent calcite crystals (CaCO3), quartz, ice, sugar,
Photonics
and so on. Birefringence, also called double refraction, was first observed and explained in the 17th century after sailors visiting Iceland brought back to Europe transparent calcite crystals (Iceland spar) that showed double images of objects that were viewed through them (Figure 5.31). The effect was first explained by the Dutch physicist Christiaan Huygens (1629–1695), who called the effect double refraction that involved an ordinary and an extraordinary wave. The extraordinary ray is so named because it does not exhibit ordinary Snellius law (Equation 5.19) behavior on refraction at the crystal surface. As light travels through an anisotropic material, such as calcite, the electromagnetic waves become split into two principal vibrations, which are oriented mutually perpendicular to each other and perpendicular to the direction that the waves propagate. The wave whose electric vector vibrates along the major axis is termed the ordinary or slow wave because the refractive index for this wave is greater than the refractive index for the other wave. The wave vibrating perpendicular to the slow wave is termed the fast or extraordinary wave. The dielectric tensor in the constitutive Equation 3.38 (D = εE) in the case of an optically anisotropic material with a single optical axis (calcite, quartz, or any tetragonal, hexagonal, or rhombohedral crystal) is a tensor of rank two given by: ¨ E xx © E ©0 ©ª 0
0 E xx 0
0· ¸ 0¸ E zz ¸¹
(5.95)
In a crystal like this there exists a single optical axis, the ordinary optical axis, where light propagation is
327
isotropic. In all other directions, two orthogonally polarized waves with different velocities do propagate; these are called the extraordinary rays. Birefringence is widely used in optical devices, such as liquid crystal displays, light modulators, color filters, wave plates, optical axis gratings, and so on. In Volume III, Chapter 6 on metrology we encounter the phenomenon in both ellipsometry (measures the polarization of light), and in Volume II, Chapter 10 (Figure 10.8), we compare birefringence of polymer MEMS structures made with different replication techniques to evaluate their stress levels. Birefringence should not be confused with dichroism, which itself has two related but distinctly different meanings in optics. A dichroic material is either one that causes visible light to be split up into distinct beams of different colors, or one in which light rays having different polarizations are absorbed by different amounts. Light that passes through an isotropic crystal is absorbed in the same way in all directions, but in an anisotropic crystal, the light is absorbed differently, depending on its direction of travel through the crystal. Isotropic colored crystals show no color change as they are rotated in plane polarized light, whereas anisotropic crystals show a distinct change in color when they are viewed in different directions. An anisotropic crystal may produce a number of different colors, known as pleochroism. When only two colors are observed, it is called dichroism. Such devices include mirrors and filters, usually treated with optical coatings, which are designed to reflect light over a certain range of wavelengths and transmit light that is outside that range. An example is the dichroic prism, used in some camcorders, which uses several
Birefringent crystal n2
Extraordinary Optical axis
Unpolarized ray
Ordinary n1
FIGURE 5.31 As light travels through an anisotropic material, such as calcite, the electromagnetic waves become split into two principal vibrations. In this double diffraction mode, an ordinary and an extraordinary wave are involved that are oriented mutually perpendicular to each other and perpendicular to the direction that the waves propagate.
328
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
coatings to split light into red, green, and blue components for recording on separate chargecoupled device (CCD) arrays. This kind of dichroic device does not usually depend on the polarization of the light. The second meaning of dichroic refers to a material in which light in different polarization states traveling through it experiences a varying absorption. The term came about because of early observations of the effect in crystals such as tourmaline. In these crystals, the strength of the dichroic effect varies strongly with the wavelength of the light, making them appear to have different colors when viewed with light having differing polarizations. This is more generally referred to as pleochroism, and the technique can be used in mineralogy to identify minerals. Dichroic crystals were researched by Edwin Land in 1930, who invented a polarizing material that would be called Polaroid and result in a huge benefit to the camera industry. The material he invented was herapathite (iodoquinine sulfate), in which the effect is not strongly dependent on wavelength, and so the term dichroic is something of a misnomer but still used.
Energy and Momentum and Electromagnetic Waves
may also write it out in terms of magnetic field B to obtain: U
U
1 B2 1 E0E 2 2 M0 2
(5.98)
Writing the total energy out in terms of both E and B, we derive: U E 0 E 2 E 0 EcB
E 0 EB E0M 0
E0 EB M0
S
1 dU EB A dt M0
(5.100)
The direction of S is along k and perpendicular to E and B for righthanded materials; for lefthanded materials, k is still perpendicular to E and H (we can use B or H because B = μH) but opposite the Poynting vector as shown in Figure 5.32. Mathematically more correct, the Poynting vector is usually written out as: S
1 (E s B) M0
(5.101)
Because S, E, and H always form a righthanded set, two types of substances can be identified: righthanded substances with S parallel to k, and lefthanded substances with S antiparallel to k (see also Figure 5.30). Because k denotes the direction of phase velocity (v p = ω/k = E/p) and S denotes the direction of group velocity (vg = dω/dk = dE/dp), in righthanded materials phase velocity (along k) E
(5.96)
Righthanded
E* k
From Equation 5.78, E/B = c, and because (e0μ0) 1/c, we can rewrite Equation 5.96 as: Total energy E 0 E
2
−1/2
=
(5.97)
The E field and the B field each contribute half of the total energy in an electromagnetic wave. As we just wrote out the total energy in terms of the E field, we
(5.99)
Now let us get back to the Poynting vector S: the energy the wave transports per unit time per unit area is given by:
Energy in EM—The Poynting Vector Electromagnetic waves transfer energy from one place to another. The Poynting vector S describes that energy flux (Jm−2 s−1). It is named after its “inventor,” the English physicist John Henry Poynting (1852–1914). The vector S points in the direction of energy flow, and its magnitude is the power per unit area crossing a surface normal to it. The total energy, U, in an EM wave is the sum of the electrical and magnetic contributions:
B2 M
S
k, S H
Lefthanded
H* (a)
(b)
FIGURE 5.32 The phase velocity (along k) and group velocity (along the Poynting E × H vector) are in the same direction (a) but in lefthanded materials. The group and phase velocities are in opposite directions (b) (see also Figure 5.30).
Photonics
and group velocity (along the Poynting E × H vector) are in the same direction. In lefthanded materials, group and phase velocity are in opposite directions. The lefthanded substances have negative group velocity that occurs in anisotropic systems or when there is spectral dispersion. We delve into these matters deeper when we discuss metamaterials in more detail further below.
$P
$P
$U c
(5.102)
with ΔU the energy absorbed by the material over a time Δt and c the speed of light. If in contrast the radiation is completely reflected, the momentum transfer becomes twice as large, or: $P
2$U c
(5.103)
For intermediate cases between total absorption and total reflection, one generalizes Equations 5.102 and 5.103 to read:
(5.104)
Because a real surface will always absorb and reflect some of the energy, κ is a constant between 1 and 2. From Newton’s second law we can calculate the force and the pressure. The average rate of energy in the beam is related to the Poynting vector by: dU A SA (E s B) dt M0
Momentum of EM: Radiation Pressure Because magnetic waves carry energy, see above, they also deliver punch or momentum to a surface they are reflected off or absorbed in (think about a sun sail; Figure 5.33). The force they exert on the material as a result is given by F = dP/dt. The force per unit area exerted by electromagnetic waves is called radiation pressure. Maxwell predicted the existence of radiation pressure and showed that if a beam of electromagnetic radiation is fully absorbed by a material, then the momentum transfer is given by:
K$U c
329
(5.105)
with A the crosssection of the object that the beam is hitting. The radiation pressure is given by: P
F 1 dP 1 dU S A A dt Ac dt c
if light is fully absorbed and P
(5.106)
2S c
if light is fully reflected Laser tweezers are another example dramatically illustrating the utility of radiation pressure (Figure 5.34). With optical tweezers one can manipulate nanometer and micrometersized dielectric particles by relying on the small forces contained in a highly focused laser beam (even a single atom can be manipulated!. Arthur Ashkin and colleagues first demonstrated laser tweezers in 1970 at Bell Labs.4 With forces in the pN range optical tweezers can be used to manipulate and move small objects, measure small forces, and build up structures of small particles. The “Lilliputian” optical force pulls the object toward the focal volume of the beam, and
FIGURE 5.33 Sun sail. Sunlight striking the sail creates a force that pushes the spaceship away from the sun, much as the wind propels a sailboat.
330
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology Specimen plane Objective Laser Optical trap
(a)
Laser light
y
Fgradient x
Fscattering z
(b)
FIGURE 5.34 Laser tweezers—an example of the use of radiation pressure. (a) The beam is focused through a microscope objective. The beam waist, contains a very strong electric field gradient. Dielectric particles are attracted along the gradient to the region of strongest electric field, which is the center of the beam. (b) This spot creates an “optical trap” which is able to hold a small particle at its center. The forces felt by this particle consist of the light scattering and gradient forces due to the interaction of the particle with the light.
by moving the focal volume of the beam one can cause the object to move. In Figure 5.34a we show a laser beam focused by a microscope objective into a small spot on a specimen (e.g., a nanoparticle). This focussed spot constitutes an “optical trap” capable of holding a small particle at its center. In Figure 5.34b we illustrate how exactly such an optical trap works. Two forces are shown to be at play : 1) Fscattering which is the scattering force and points in the direction of the incident light (z, see axis), and 2) Fgradient, which is the gradient force, due to the gradient nature of the Gaussian light intensity profile (xy plane). As we just learned, light carries momentum and momentum is proportional to its energy in the direction of its propagation. A change in direction of the incoming light by reflection or refraction, results in a change of the momentum of the incoming photons. That momentum change, conservation of momentum dictates, causes the dielectric particles in the path of the light to undergo an equal and opposite momentum change and this is what causes a force to act on particles. When the light of a Gaussian laser beam interacts with a small particle, the light rays are bent (two example rays are illustrated in Figure 5.34b). Summing all the forces results in a resultant
force for Fscattering (zdirection) and one for Fgradient (xy plane). With the contribution to Fscattering of the refracted rays larger than that of the reflected rays a restoring force is created along the zaxis, and a stable trap is established. In modern equipment the image of the trapped particle can be projected onto a quadrant photodiode to measure nmscale displacements. A continuous wave (CW), lowpower laser was used to “optically trap” individual bacteria and protozoa. Steven Chu, who was at Stanford at the time, showed that lasers could be used to manipulate molecules. He and his team famously attached polystyrene beads at the end of DNA and pulled on the beads to stretch the DNA molecule. Others have used laser tweezers to study kinesin motors (see Volume III, Figure 2.33). Laser scissors were in use earlier than laser tweezers.5 Laser scissors are shortpulsed and highirradiance (energy reaching the surface in a given amount of time) beams, whereas tweezers are continuous and of low irradiance. The CW lasers can cause a 1.15–1.45°C increase per 100 mW of laser power. If the heat dissipation is inefficient, the laser can produce 10 times that power. Therefore, in the case of tweezers, the target must be transparent to not store significant energy.
The Complex Refractive Index n c and the Complex Wave Vector k As we saw above, at optical frequencies, electric fields in homogeneous media have solutions of the form E E me i(k x x Wt ) and B Bm e i(k x x Wt ) (E along the zaxis, B along the yaxis, and k along the xaxis; see Equation 5.70). For nonmagnetic materials with μ = μ0, this results in a dispersion equation k 2 = c W2 E(W) (Equation 5.80), and with n this can 2 v v n2 also be expressed as k 2 2 W 2 (Equation 5.81). c This dispersion relation for the case where the refractive index n is a real number correctly describes transparent materials. To describe a material that is also absorbing and features the anomalous regions we typically observe in plots of the refractive index as a function of frequency (see, for example, Figure 5.29), we need to introduce a complex wave vector k and a complex refractive index nc.
Photonics
n 2P W with a c L/n real refractive index n must be replaced by a complex n 2P wave vector k c W with a complex c L / nc refractive index nc. Thus, the real wave vector k
The complex refractive index nc is given as: n c n + iK
(5.107)
with n the refractive index and κ the extinction coefficient of the material. It follows that the dispersion Equation 5.81 then is transformed as:
E x ( x,t) E m ( x , W)e
¥ Wn ´ WK x WK µ x i ¦§ ¶ c c
damping/ absorption
e
331
(5.109)
propagation
which represents a traveling damped wave (Figure 5.35). The optical intensity of this electromagnetic wave is calculated as: 2
I t E I0 e
2WK x c
I0 e Ax
(5.110)
KW 4 PK c L 2kK. Note that α > 0 means absorption and α < 0 means gain (see lasers at the end of this chapter), and a propagation coefficient is defined as ¥ W´ B ¦ µ n kn . The complex wave vector in §c¶ Equation 5.108 can be written out in terms of this absorption coefficient α and the propagation coefficient β as: with the absorption coefficient A 2
k(W) p
(n + iK)W c
(5.108)
The KramersKrönig relation links the real and complex parts of the complex refractive index (i.e., the refractive index n and κ the extinction coefficient). If you know one, you can calculate the other one. The macroscopic quantities n and κ in Equation 5.108 will now be derived from the microscopic functions χ and εr, i.e., from the complex electric susceptibility and the complex permittivity, respectively. Substituting the complex wave vector in the proposed wave solution (Equation 5.70), we obtain:
k k a ik aa B i
(5.111)
The real part of the complex wave vector (k) is k′ = β and the imaginary part k′′ = α/2; in other words, the real part of the complex wave vector corresponds
FIGURE 5.35 A traveling damped wave.
A 2
332
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
to the propagation coefficient and the imaginary part corresponds to the absorption coefficient of the material. Substituting the complex wave vector, written out in this format, into the proposed wave solution [E = E mei(k ⋅ x−ωt)] (for simplicity we have dropped the sub x for the wave vector k), we obtain:
E x ( x,t) E m ( x,W)e k aax e i k ax Wt A
x
E m ( x,W)e 2 e iBx Wt absorption
(5.112)
propagation
for transparent materials κ
(5.143)
Note that the reflection coefficient r in Equations 5.136 and 5.138 can be positive or negative, depending on the relative sizes of the intrinsic impedances of the two media. The transmission coefficient t, on the other hand, is always positive (see Equations 5.137 and 5.139). Importantly, Equations 5.136–5.139 also hold when the media are dissipative, i.e., when η1 and/or η2 are complex. A complex r (or t) means that a phase shift is introduced at the interface on reflection (or transmission). Reflection and transmission are related by: t(ω) = 1 + r (ω)
(5.144)
The same boundary conditions derived above require the components of the complex wave vector k (see Equation 5.111) parallel to the surface to be the same on both sides of the boundary. When a sinusoidal plane wave, with angular frequency ω and propagation wave vector k, travels in the xdirection in a linear dielectric with a scalar permittivity and no free charge or currents present, any dissipative process leads to phase lag and a complex wave vector. Thus, a transmitted wave in a medium is attenuated because, by the dispersive relation for electromagnetic waves, the wave vector in the medium is related to the incident k in vacuum by (n + iκ)k, or the incident wave, E i ( x ) E im e i(k x Wt), is modified to:
E mt E m exp [i(n iK)k x Wt)] exp ( Kk x) exp [i(nk x Wt)] (5.145) attenuation propagation Continuity of E and B at the interface (surface of i r t the medium) dictates that E m E m E m (Equation 5.133), or: kE im kE rm (n iK)kE mt or E im E rm (n iK)(E im E rm )
(5.146)
(n iK 1)E im (1 n iK)E rm Thus, we obtain for the reflectivity at normal incidence: r(W)
E rm ¥ n iK 1 ´ n c 1 E im ¦§ n iK 1 µ¶ n c 1
(5.147)
But the quantity measured in experiments is reflectance R, defined as the ratio of the reflected intensity to the incident intensity (see above), or:
R(W)
E rm E im
2 2
2
(n 1)2 K 2 n 1 c nc 1 (n 1)2 K 2
(5.148)
When R = 0, there is no reflection, and this occurs with n = 1, κ = 0, and R = 1 when either n or κ becomes large. It is difficult to measure the phase θ(ω) of the reflected wave, but it can be shown that it can be calculated from the measured reflectance R(ω) if this is known over all frequencies. With both R(ω) and θ(ω) known we can use Equation 5.148 to calculate n(ω) and κ(ω). Above we saw that n(ω) and κ(ω) are related to the complex dielectric function εr as: n c (W) n(W) iK(W)
E ra (W) iE raa(W) (5.113 and 5.115)
Thus, plugging the values for n(ω) and κ(ω) in Equation 5.113 we obtain the complex dielectric function. The values for the refractive index n and extinction coefficient κ are not independent; they are linked by the KramersKrönig relations. The KramersKrönig relations enable us to find the real part of the response of a linear passive system if we know
337
Photonics
TABLE 5.3 Optical Coefficients
TABLE 5.4 Semiconductors: Transparency Range (T), Bandgap Wavelength, and Refractive Index
Relative Dielectric Constant
εr = 1 + χe(ω) Crystal
na
( Era )2 ( Eraa )2 Era 2
Imaginary part of refractive index
naa
(Era )2 (Eraa )2 Era 2
Absorption coefficient
A 2
W naa c
Reflectivity
r(W )
¥ n iK 1´ nc 1 Erm ¦ i Em § n iK 1µ¶ nc 1
Real part of refractive index
Reflectance
R(W )
r m i m
2
2
Ge Si GaAs CdTe CdSe ZnSe ZnS
2
E  (n 1) K E 2 (n 1)2 K 2
the imaginary part of the response at all frequencies, and vice versa: d
n(W) 1
1 K(W a) P° dW a P d W a W d
K(W)
(5.149)
1 n(W a) 1 P° dW a P d Wa W
where P denotes the Cauchy principal value. Either of these equations, plus a knowledge of R(ω) at all frequencies, permits one to disentangle the separate values of n(ω) and κ(ω). The previous discussion makes it clear that the refractive index of a semiconductor can also be determined from a sometimes more practical transmission measurement. In Table 5.3 we summarize the important optical coefficient properties deduced so far. In Table 5.4 we list a number of semiconductors with their transparency range, the refractive index, and the wavelength corresponding to their bandgap. Example 5.3*: Surface reflectance R of Ge. At 400 nm the complex refractive index nc for Ge = 4.141 + i2.215. Calculate the 1) wave propagation speed v, 2) absorption coefficient α, and 3) reflectance R. 1. v = c/n = 2.998 × 108/4.141 = 7.24 × 107 m/s 2. α = 4π × 2.215/400 × 10 −9 = 6.96 × 107 m−1 (4.141 1)2 2.2152 3. R = 47.1% (4.141 1)2 2.2152 *
All three examples are from Mikael Mulot’s class notes.
Transparency Range (μm)
λg (μm)
n
1.8–23 1.2–15 1.0–20 0.9–14 0.75–24 0.45–20 0.4–14
1.8 1.1 0.87 0.83 0.71 0.44 0.33
4.00 3.42 3.16 2.67 2.50 2.41 2.20
Example 5.4: Transmittance T through Si. The reflectance of a 10μmthick Si slice at 633 nm = 35% and α = 3.8 × 10 −5 m−1. Calculate the transmittance T. For αl = (3.8 × 10 −5)(10 × 10 −6) = 3.8. As a result we obtain for T = (1 − R)2e−αl = (1–35%)2e−3.8 = 0.0095. Example 5.5: Reflectance R and absorption coefficient α of NaCl. The complex relative dielectric constant at 60 μm for NaCl is −16.8 + i91.4. Calculate 1) α and 2) R: n
1 2
16.8 ( 16.8)2 91.42 6.17
1 16.8 ( 16.8)2 91.42 7.41 2 4 PK 4 P s 7.41 1.55 s 106 m 1 we derive for A L 60 s 10 6
1. With K
2. R
(6.17 1)2 7.412 76.8% (6.17 1)2 7.412
Bulk, Surface, and Localized Plasmons: Plasmonics Introduction Plasmons are electron density waves that can carry huge amounts of data and that can be squeezed into miniscule metal structures, holding the promise of a new generation of superfast computer chips, ultrasensitive molecular detectors, microscopes with improved subwavelength resolution (nearfield scanning optical microscopes; NSOMs), better exploitation of nonlinear optics, sensitive optical studies of surfaces and interfaces, fabrication of an infinite variety of brightly colored metal nanoparticles,
338
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
better lightemitting diodes, higherresolution lithography, and perhaps even the possibility of altering the electromagnetic field around an object as to render it invisible (cloaking). In 2000, Harry A. Atwater from Caltech gave the name of “plasmonics” to this promising emerging field.6 In Chapter 3 we saw how a metal may exhibit collective longitudinal oscillations of the free electron gas density, often at optical frequencies. A plasmon is a quantum of a plasma oscillation that is excited by passing an electron through a material or by reflecting an electron or a photon off a material. It is a result of the quantization of the plasma oscillations just as photons and phonons are quantizations of light and sound waves, respectively. In other words, reflected or transmitted electrons/photons lose an amount of energy that equals an integral number of times the plasmon energy. A plasmon can also couple with a photon to create a plasma polariton. The most discussed types of polaritons are phononpolaritons, resulting from the coupling of an infrared photon with an optical phonon; excitonpolaritons, resulting from the coupling of visible light with an exciton; and surface plasmonpolaritons, resulting from the coupling of surface plasmons with light. Plasmons can be observed experimentally using electron energy loss spectroscopy (EELS). In EELS, electrons are accelerated to a defined energy and are then shot onto a thin foil of the material under investigation. The number and energy of the transmitted electrons are measured. These electrons are able to excite plasmons, which then appear as a more or less sharp dip in the number of transmitted electrons at an energy loss equal to the plasma frequency.
bulk plasmon frequency ωp, defined as W p
ne 2 me E 0
(Equation 3.41), and at frequencies above ωp, the metal becomes transparent and dielectriclike, whereas below it is reflective and conductive. The bulk plasmon resonance of silver, for example, occurs at = ωp = 3.76 eV. In Figure 5.27, we saw that the dispersion relation, the relation between the energy of the system and its corresponding momentum k(ω), in a vacuum, is a linear function of ω with a slope c = vg = v p (velocity of light = group velocity = phase velocity). The straight line in Figure 5.27 is referred to as the light line. We also established that the dispersion relation in a medium is no longer a straight W n(W)W W line but is given by: k(W) EM vg c c (Equation 5.88). If we consider a highly conductive system, where the damping factor γ is very small, the real component of the dielectric constant W 2p E ra (W , k) z 1 2 (Equation 3.44) dominates with W W 2p G the imaginary component E raa(W , k) z 3 (Equation W 3.45) tending to zero. In other words, Equation 3.44 is the expression for the dielectric constant when only the conduction electrons contribute, and damping is neglected. The Drude model, in this case, predicts a monotonous decrease of E r (W , k) for decreasing frequency, and experiments confirm that E ra (W , k) becomes zero when ω = ωp in such case (see Figure 3.9. When E ra (W) becomes zero at ω = ωp, the material supports free longitudinal collective modes for which all electrons oscillate in phase. The dispersion relation for bulk plasmons from Equation 5.88 is then given as:
Bulk Plasmons In Chapter 3 we explained electron oscillations in a metal using the Drude model of metals. In the Drude model the metal is treated as a 3D crystal of positively charged ions with a delocalized electron gas moving in a periodic potential of this ion grid, i.e., as a plasma. Based on that model, we calculated the complex dielectric constant of the bulk · ¨ W2 plasma as E(W , k ) E 0 ©1 2 p ¸ (Equation 3.40). (W iG W) ¸¹ ©ª The plasma exhibits resonance absorption at the
W 2 W 2p c 2 k 2
(5.150)
as shown in Figure 5.39, where we also mark the light line (ω = ck). It is clearly seen that when ω is less than ωp there is no propagating solutions and the wave vector is imaginary. Surface Plasmons Surface plasmons are those plasmons that are confined to surfaces and that interact strongly with light, resulting in a polariton. They occur at the interface of a vacuum or a material with a positive
Photonics
!
FIGURE 5.39 Dispersion of bulk plasmon. The light line is also marked (vphase = c).
dielectric constant (a dielectric) and that of a negative dielectric constant (usually a metal or doped dielectric) (Figure 5.40). Surface plasmons are a subset of the “eigenmodes” of the free electrons in a metal or doped dielectric, with the electronic oscillations being excited parallel to the surface of the metal and a surrounding dielectric. Because all electrons may participate in the oscillations, plasmons can interact strongly with light of the right frequency. With wave vectors much smaller than the Fermi wave vectors of metals, these wave modes can be described by Maxwell’s equations. Quantum mechanical considerations only are necessary for the shortest plasmon wavelengths. At lowsurface plasmon wave vectors, the behavior of these surface modes can be understood intuitively. In this regime, they are essentially transverse in character, and these transverse fields generate a polarization in the dielectric, which is aligned with the stimulating field. In the metal, however, the polarization is in the opposite direction of the applied field owing to its negative dielectric constant. Now the stimulating field is creating equal and opposite electric displacements (D), in phase with
339
each other across an interface. These opposing electric displacements serve to attract and confine the current to the interface, thus generating the collective electron oscillations of the surface plasmon. Figure 5.41 illustrates vertical and horizontal polarized waves. In vertical polarization (spolarization from the German senkrecht), the E field is perpendicular to the plane of incidence. In horizontal polarization (ppolarization), the E field is parallel to the plane of incidence. Starting from the Maxwell’s equations, we derive the characteristics for the plasmonic system shown in Figure 5.42a. Light that is ppolarized (see Figure 5.41) will create polarization charges at the interface as illustrated in Figure 5.42b. These charges give rise to surface plasmon modes. With an spolarized incident radiation no such polarization charges are created at the interface; thus, these EM waves cannot excite surface plasmon modes. We assume that the free current J is zero, that the relative permeability (μr) of both media to be unity, and that the wave is propagating in the xdirection. The EM field of surface plasmons propagates on the surface in the xdirection. The Hy is the magnetic field in the ydirection of the incident ppolarized wave. Thus, the components of the E and H fields are E = (E x , 0, Ey) and H = (0, Hy, 0), and the interface between the metal and dielectric is at z = 0. As we saw above, the constraints imposed on the transverse E and H field components at a boundary are that: E1x E 2x H1y H2y
(5.151)
FIGURE 5.40 Surface plasmons at metal/dielectric interface.
Illustrating vertical and horizontal polarized waves.
FIGURE 5.41 The ppolarization: E field is parallel to the plane of incidence, and spolarization: E field is perpendicular to the plane of incidence (German senkrecht = perpendicular).
340
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology Dielectric 1 E1z
Z E1
z=0
H1y
E1x Dielectric
y
E
~ei(kxxt)
x
Wave propagating in xdirection
z Metal 2
Hy +++
+++
X
Metal (b)
(a)
FIGURE 5.42 (a) Surface plasmons a subset of the “eigenmodes” of the free electrons in a metal. Electronic oscillations being excited parallel to the surface of the metal and a surrounding dielectric. The local field intensity depends on the wavelength. (b) Polarization charges are created at the interface between two materials.
i.e., the components of the E and H fields are continuous across the interface from metal to insulator. It is also informative to look at the boundary condition for the normal component of the D field: D1z D2z
(5.152)
H1 (0, H1y , 0)e i(k1x x k1z z Wt)
(5.154)
E1 (E1x , 0, E1y )e i(k1x x k1z z Wt)
which can be rewritten as:
and for the metal:
E 0 E 0z P1z E 0 E 0z P2z n
Thus, a suggested solution for the surface plasmon mode of wave propagation in the dielectric may be written as:
n
(5.153)
H 2 (0, H 2y , 0)e i(k 2x x k 2z z Wt)
(5.155)
Creation of the polarization charges
E 2 (E 2x , 0, E 2y )e i(k 2x x k 2z z Wt)
If one of the contacting materials is a metal, the electrons respond to the polarization by the ppolarized light (Figure 5.42, right), and this gives rise to surface plasmon modes. To model these waves we are looking for a localized surface mode, decaying into both materials as shown in Figure 5.43a, where the exponential dependence of the field Ez is shown. The decay in the two media is characterized by the penetration depth, i.e., the depth at which value of Ez falls to 1/e ≈ 1/κz (see Equations 5.111 and 5.112: k ∼ k′′ ∼ α ∼ κ (because the absorption coefficient α = 2κω/c = 2kκ, with κ the extinction coefficient).
Substituting these suggested solutions in Maxwell’s equations and applying the continuity boundary conditions, i.e., k1z = k 2z (because continuity holds for both E and H: Equation 5.151), we find the following additional constraint for the wave vector:
(a)
~eikzz; kz = iz Intensity
(b)
k1x k1z
E1 E 2 k1z k 2z
(5.156)
From the vector diagram in Figure 5.43b, we see that n1k is given as: 2 2 (n1k)2 k1x k1z or also E1(W , k)
W2 2 2 k1x k1z c2 (5.157)
Dielectric 1
and this enables us to establish the sign of k z: n1k
k1z
n k
2
2
k1x
2
2 2x
1
(5.158) z
Metal 2
FIGURE 5.43 (a) We are looking for a localized surface mode, decaying into both materials so that k z has to be imaginary; (b) n1 is the dielectric constant of the dielectric.
k 2z
n k 1
k
because k1z and k 2z are of opposite signs, the condition in Equation 5.156 will be satisfied only if ε1 and
Photonics
ε2 are of opposite signs as well. This is the case when one material is dielectric, ε1 > 0, and the second material is metal, ε2 < 0. It also follows from this equation, because k1z and k 2z must both be imaginary, that:
n k
2
1
k
2 1k
k
2 2x
0
so that k1x n1k
(5.159)
and:
n k
2
2
0
so that k 2x n 2 k
(5.160)
The condition in Equation 5.160 is always satisfied for metals because: 2 E2k 2 k 2x
(5.161)
with ε2 for a metal > ω0, the real part of the dielectric constant becomes zero (ε′ = 0). Also note that ε′ drops below zero between ω0 and ωp. When approaching ω0 from below, ε′ starts rising to reach a maximum at $W W W 0 G/2 and a minimum at $W G /2. The peak (a Lorentzian line shape) in the imaginary part of the dielectric function (ε′′) occurs at ω = ω0 and has a full width at half maximum (FWHM) of γ (see Figure 5.57, inset). The quality factor (Q) of the resonance Q = ω0/γ is a measure of the dissipation of the system. For an isolated molecule the damping parameter can be interpreted as the inverse of the lifetime of the excited quantum state. This is consistent with the Heisenberg uncertainty principle 1 h h z (HUP) ($E$t z ; Equaor $t z 2P$N 2P 2P.h$N tion 3.107). If an absorption line is dampened solely by the natural lifetime of the state, one refers to natural broadening. This is also the peak that is so characteristic for bound electrons (see the example of Ag with bound delectrons in Figure 5.64). If one knows the ωdependence of the dielectric function, then the ωdependence of the refractive index can be calculated. From the relationship between the complex refractive index and the complex dielectric constant (Equations 5.115, 5.116, and 5.117), the real and imaginary parts of the complex refractive index nc as a function of ω were plotted in Figure 5.57b. Comparing Figure 5.57a and b, one recognizes that the real part of the refractive index n(ω) approximately follows the frequency dependence of
E ra (see Equation 5.118) and that the extinction coefficient κ more or less follows εr′′(ω)/2n (see Equation 5.116). This correspondence is more and more exact if κ > ω0, n gradually rises, and above the highestfrequency resonance (usually in the deep UV/soft xray region) tends toward 1, and the group velocity vg becomes equal to the velocity of light c; in other words, the light moves through this medium as if it were moving through a vacuum. In the region between ω0 and ωp, n is small over the same region where ε is negative. At low frequencies (ω ωp), in other words, TART. These regions become more distinct the smaller γ and the larger ωp. As expected for smaller damping γ, the curves are narrower and have larger maximum values. The reflectance is much higher and has sharper edges. The high R starts around ω0 and falls near ωp. This is because κ >> n in
Photonics (A) (a)
0
= 4,
p=
8 and = 1
(b)
10
0
= 4,
p=
357
8 and = 0.3
20
Re ( )
Re ( )
Im ( )
Im ( )
0
0 −20
−10
−40
0
4
2
8
6
10
12
0
2
4
6
8
10
12
0
2
4
6
8
10
12
6
8
10
12
6
4
n( )
n( ) ( ) ( )
2
4
( ) 2
2
( ) p
2
p
0
0
0
2
4
6
8
10
12
1
1
R( ) 0.5
R( ) 0.5
0
0 0
2
0
(B)
= 4,
4
p=
6
8
10
12
0
2
8 and = 0.3
6
n( )
4
( ) 2
4
Four distinct spectral regions ( ) p
Transmissive Absorptive Reﬂective Transmissive
2
0
0
2
4
T
6 A
8
10
12
(frequency ranges are approximate) The regions are more distinct for smaller and larger p.
T
R
< 0 − /2 − γ/2 < < 0 + γ/2 < < p > p
1
R( ) 0.5
0
0
2
4
6
8
10
12
FIGURE 5.61 (A) Compare the real and imaginary parts of a dielectric function as a function of ω, the real and imaginary parts of the refractive index n as a function of ω, and the reflectivity from air at normal incidence for γ = 1 (broad resonance, a) and γ = 0.3 (narrow resonance, b). (B) We have colored in four distinct spectral regions, marked with T for transmissive, A for absorptive, R for reflective, and T for transmissive again—TART. We have plotted also a scaled version of α by plotting 2ωκ scaled to ωp.
358
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
the reflecting band. Above ω0, n is well below unity. Above ωp, n rises, but only in the highfrequency limit does n approach unity. Local Field Corrections The calculations of the dielectric constant we have discussed until now are valid for a rarefied gas with a low density of atoms. In “dense optical media,” such as solids, there are other factors that we have to consider. In a real solid, atoms may feel a field from an incident light beam, but they also experience an induced field from the surrounding atoms. In other words, the local field E L is the sum of a field without matter E 0 and an induced dipolar field E dipole from all the other surrounding atoms, or: E L E 0 E dipole
(5.203)
In our discussions of dipole oscillators in solids, we should have been using E L not E 0! The degree of polarization in a solid is related to the structure of the material. As a consequence, dielectric behavior in electrostatic and alternating electric fields depends on both static and dynamical properties of the solid. The local electric field can be calculated according to the crystal structure by the method of Clausius and Mossotti. For example, for cubic structures the ClausiusMossotti equation reads (e.g., see Ashcroft and Mermin, SolidState Physics, p. 539): EL E0
P , 3E 0
(5.204)
which is larger than E 0. Similar relations can be derived for any solid. For a solid consisting of atoms of type j with a concentration Nj, we then derive for the polarization P: ¥ P ´ P E 0 ¤ N jE L C j,e E 0 ¤ N j ¦ E 0 C j,e 3E 0 µ¶ § j j E 0 ¤ N jC j,e E 0 j
¤N C j
j
j,e
¥P´ ¦§ 3 µ¶ (E r 1)E 0E 0 (5.205)
fj e2 . But we know ¤ 2 E 0 me j (W 0,j – W 2 – iWG j ) that D = ε0E + P, D = ε0εrE, and P = ε0(εr − 1)E, and
where C j,e
this way we obtain the ClausiusMossotti (CM) relation: (E 2 1) NC j,e 2 3 (E 2)
(5.206)
This relation links the polarizability to the dielectric constant. Using εr = n2 we find the socalled LorentzLorenz relationship: C j,e (n 2 1) N 2 3 (n 2)
(5.207)
And we find that the refractive index approximately follows the formula: Er 1 n2 1 Ne 2 2c E r 2 n c 2 3E 0 me
¤ (W j
2 0,j
fj
W 2 iWG j ) (5.208)
We follow with some examples from the n, κ database (http://www.ioffe.ru/SVA/NSM/nk/index). In Figure 5.62a we show the refractive index n and absorption index κ versus photon energy for silicon. At visible frequencies, i.e., below the resonance, Si is “transmissive.” But the high refractive index of Si still yields high reflectivity (30–50%), and all visible frequencies are reflected strongly, so Si appears as a grayish reflector throughout the visible spectrum (1.7–3.2 eV) “gray metallic.” In Figure 5.62b we show the refractive index for two common dielectrics (Si3N4 and SiO2). Dielectrics typically exhibit one resonance only, and at low frequencies they are transmissive. The resonances are typically in the UV range associated with electron polarization. There is an additional resonance in the IR range for polar materials resulting from nuclear motion and orientation (see Figure 5.63). We come back to describe these polar materials in more detail further below. To design a material with a high dielectric constant, we choose ions with high polarizability and a high density of them. Example 5.6: Estimation of εr(ω = 0) for Si The reflectance R of Si increases sharply at about 3 eV, and we may take this as an estimate for ω0. Hence ω0 ≈ 3 × 1.6 × 10−19 = 4.53 × 1015 rad/s. Because W p2 W p2 Er ( W ) 1 2 , , so if E ( W 0 ) 1 r W 20 W 0 W 2 iG W
Photonics 7 Refractive index n Absorption index
Refractive index n
6
5.0
5
4.0
4
3.0
3
2.0
Absorption index
(a)
359
2 1.0 1 1
(b)
2
3 4 5 Photon energy hv (eV)
2.8
6
7
0.0
1.65
2.6
Refractive index n
Refractive index n
2.7 2.5 2.4 2.3 2.2 2.1
Si3N4 2
4 5 6 3 Photon energy hv (eV)
7
1.55 1.50 SiO2
1.45
2.0 1
1.60
8
1
2
3 4 5 6 Photon energy hv (eV)
7
FIGURE 5.62 Examples from the n, κ database (http://www.ioffe.ru/SVA/NSM/nk/index.html#A3B6). (a) Refractive index n and absorption index κ versus photon energy for silicon. (b) The refractive index for two common dielectrics (Si3N4 and SiO2). The color bands in the three figures roughly mark the visible spectrum (1.7–3.2 eV).
Ultraviolet
we can determine ωp, we can estimate εr(ω = 0).
Infrared
Visible
Absorption coeﬃcient α Electronic transitions No transitions
Atomic vibrations
Now we remember that W p ne2 /E 0m , and because each Si atom has four valence electrons, n = 4NSi ≈ 4 × 2 1028 m−3. This gives us an estimate of ωp ≈ 1.6 × 1016 rad/s (corresponding to about 10.5 eV), and hence εr(ω = 0) ≈ 14. This compares to a measured value for εr(ω = 0) of 12, so our approximations are reasonable.
Optical Properties of Metals
Refractive index n
Introduction 0.01
0.1
1
10
100
Wavelength λ (μm)
FIGURE 5.63 The absorption coefficient and the index of refraction versus wavelength for a generic polar insulator. As we derived earlier: A 2kK .
The Drude model implies that only the plasma frequency ωp dictates the appearance of metals. This works indeed for many metals, say for aluminum, but it does not explain why copper is red, gold is yellow, and silver is colorless. In fact, the appearance
360
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
(a) 100 Al
60 Au
40 20 0 200 nm
Ãp = 15.8 eV
< p 1.0 0.8
Reﬂectance
Reﬂectance %
80
(b)
Experimental data for Al
0.6
> p
0.4 = 0 = 8.0 fs
0.2
Ag
0.0 500 nm 1 m 2 m Wavelength
5 m
0
5
10 Energy [eV]
15
20
FIGURE 5.64 (a) Reflectance curves of Ag, Au, and Al. (b) Reflectance versus energy for an ideal metal with zero damping (γ = 0) and experimental data for aluminum. See also Example 5.8.
of these metals is characterized by a different edge in the reflectance spectrum (see Figure 5.64a), but the fact is that these three metals have the same number of valence electrons, so according to the Drude model they all should have been the same. Moreover, the calculated plasma frequency for all three should lie at about 9 eV, well outside the visible region, so the Drude plasma frequency cannot in itself account for the colors of Cu and Au. Colored metals have interband transitions in the visible that remove particular frequencies from the reflected spectrum. The combined effects of the free electrons and the bound delectrons influence the reflectance properties of the metal in these cases. In Chapter 3, we pointed out that in a metal where both bound electrons [εB(ω)] and conduction electrons [εr(ω)] contribute to the dielectric constant, an effective dielectric constant εEff(ω) must be defined as: E Eff (W) E B (W) E r (W)
(3.48)
Whereas the Drude model explains the free electron contribution [εr(ω)] to E Eff (W), the bound electron effect [E B (W)] can only be treated by the Lorentz model. Based on the DrudeLorentz model, we will now review optical properties of bulk metals (3D) and metals in reduced dimensionalities in plasmonics. Reflectance and Absorption of Electromagnetic Waves in Metals Reflectance of Conductors Metals can be treated as plasmas because they contain equal numbers of fixed positive ions and free electrons. In Figure 5.64a, we
plot the reflectance R of Al, Au, and Ag as a function of wavelength. In Figure 5.64b, we show the reflectance of an ideal metal and that of aluminum versus the energy of the incoming radiation. A characteristic feature of all metals is that they are shiny as a result of the interaction of light with the free electrons (plasma excitations) and that their reflectance is close to 100% (R = 1) below the plasma frequency ωp but much smaller at higher ω. At low frequencies, metals with plenty of free carriers are very good reflectors. The free carriers can respond rapidly, on a time scale of an AC cycle, so as to screen the external applied AC fields. Earlier we calculated the normal incidence reflectance for any material as: R(W)
E rm E im
2 2
2
nc 1 (n 1)2 K 2 nc 1 (n 1)2 K 2
(5.148)
If we consider a lightly damped (highly conductive) system, where the damping factor γ tends to zero (an ideal metal would come with zero damping γ = 0), the real components of the dielectric constant W 2p E ra (W , k) z 1 2 (Equation 3.44) dominate because W W 2p G the imaginary component E raa(W , k) z 3 (Equation W 3.45) tends to zero. For the complex refractive index in this case we can write: n c (W)
E ra (W) 1
W 2p W2
(5.209)
Substituting this expression in Equation 5.148 for the reflectance R, we see that when ω < ωp, nc is imaginary, R = 1, and the metal is shiny (say, up to
361
Photonics
the nearinfrared). At higher frequencies (visible and UV), with ω > ωp, nc turns real, the reflectance R suddenly falls (for ω → ∞, R → 0), and metals are transparent in the UV. It follows from the expression for the plasma frequency of an FEG in a metal ne 2 [W p (Equation 3.41)] that the higher the me E 0 conductivity (n larger), the higher the plasma frequency. And indeed, plasma frequencies ωp are in the optical range (UV) for metals and in the terahertz to the infrared region for semiconductors and insulators (see also Table 3.2). Without any damping (γ = 1/τ = 0), the reflectivity R equals 1 and then drops very steeply (see rectangular box in Figure 5.64b). Introducing some damping, R becomes less than 1, and the reflectance decrease is less severe (see Figure 5.64b where we used τ = 8.0 fs, a value calculated for aluminum; see also Example 5.8). When the conduction electrons can no longer move rapidly enough to screen the external applied field on the time scale of an AC cycle, only the core electrons bound to the atoms can contribute to the dielectric response; the metal behaves now as a transparent dielectric. The frequency at which the metallictodielectric transition occurs is the plasmon frequency ωp. At ω = ωp, the real part of the dielectric constant becomes zero. Hence nc(ωp) = 0, which means the phase velocity tends to ∞. (This occurs in the anomalous dispersion regions shown in Figure 5.29.) Another way to describe this is that the wavelength, λ = 2πc/ncω → ∞ as ω → ωp. This means that all the electrons are oscillating in phase throughout the propagation length of the material. Absorption and Penetration Depth of Electromagnetic Radiation in Conductors Optical measurements of the complex dielectric constant εr(ω,k) of a plasma are equivalent to AC conductivity measurements. This can be gleaned from a comparison of the dielectric function of a free electron plasma with its AC conductivity. In Chapter 3 we calculated for the AC conductivity of a plasma: S(W)
ne 2 ¥¦ 1 ´µ µµ ¦ µ me ¦¦ 1 ¦¦ iW µµµ §T ¶
(based on Equation 3.30)
and for the complex dielectric constant we derived: · E(W, k) ¨© ne 2 ¸ 1 2 © E0 me E 0 (W iG W) ¸¹ ª
E r (W, k)
(based on Equation 3.40) Comparing these expressions we note that: E r (W , k) 1
iS(W) E0W
(5.210)
At very low frequencies (ω c, is faster than the speed of light, but the latter does not correspond to the velocity of a real physical propagation of any physical quantity. A wave that propagates in the medium with the dispersion relation 2
2
2 2
W W P c k is also shown, as is the region of longitudinal plasma oscillation. The yellow area is the forbidden frequency gap. (Based on Kittel.)
¥ ck ´ phonons W . However, in polar materials, ¦ E(d) µ¶ § light, close to the vibrational resonance frequencies (ω ∼ 1014 rad/s), does interact with the transverse optical phonon modes, and εr starts to vary strongly so that ω versus k is not a straight line anymore as evident from Figure 5.84. At large k wave vectors (k > 105 cm−1), we derived ck a positive photonlike solution with W (just E(d) like in Figure 3.158b) and a negative phononlike mode with a singularity at ω = ωT. With ω approaching ωT, the index of refraction increases, and the group and phase velocities of the wave slow down (decreasing slope of the dispersion curve) to a value close to that of the lattice modes (AT mode). The wave now propagates as a strongly coupled polarizationelectric field wave, with a velocity characteristic of the lattice transverse acoustic mode. At small k vectors (k 0, we are dealing with absorption, and with α < 0, we have a gain g (so g = −α is used for negative absorption). The increase of intensity in a laser is much greater than can be obtained by spontaneous emission mechanisms. The threshold of a laser is the state where the gain just equals the cavity losses. For electrically pumped lasers this corresponds to a certain threshold current Ith.
Quantum Mechanics and Lasers Quantum Confinement Lasers work because of the quantum properties of photons—one photon tends to cause another to be emitted—and one photon cannot be distinguished from another (they are bosons; see Chapter 3). If there are many excited atoms, the photons can “cascade,” and very intense, collimated light is emitted, forming a beam of precisely the same color of light. Because photons cannot be distinguished, which atom emitted a given photon is completely uncertain, but that also means that the direction and energy of the photons can be very certain.
Current
Top mirror (99.0% reﬂective) Laser cavity (Length = )
Oxide layer Gain region
Bottom mirror (99.9% reﬂective)
– (a)
(b)
FIGURE 5.147 Comparison of an edgeemitting laser diode (a) and a vertical cavity surfaceemitting laser (VCSEL) (b).
Photonics
In a quantum well, we saw in Chapter 3, there are no allowed electron states at the very lowest energies (zeropoint energy). What that means is that the lowest allowed conduction state in a quantum well is broad so that many electrons can be accommodated. Similarly, the top of the valence band has plenty of states available for holes. This means that it is possible for many holes and electrons to combine and produce photons with identical energy for enhanced probability of stimulated emission (lasing), making the quantum well laser much more efficient than a diode laser. The two important reasons that better lasers are enabled with lowerdimensionality semiconductors is the quantum confinement of carriers, which leads to a concentrated density of states, and a sharper energy distribution. The carrier distribution is given by n(E) = G(E)f(E) (see Equation 3.230), and bulk semiconductors have a broad carrier distribution compared with lowerdimensional semiconductor structures. Arakawa and Sakaki predicted significant increases in the gain and decreases in the threshold current Ith of semiconductor lasers using QDs or boxes in the active layer of the laser.50 The gain g predicted by Asada et al.51 for 3D, 2D, 1D, and 0D semiconductor structures is shown in Figure 5.148. Quantum Cascade Lasers Esaki was not only the originator of the Esaki tunnel diode, covered in Chapter 4, but also the originator 104 Ga0.47In0.53As/InP T 300K in 1 s 1018cm3
Gain (cm1)
Box 100 100 100Å3 Wire 100 100Å2 103
QW ﬁlm 100Å Bulk
1.2
1.3
1.4 1.5 Wavelength ( m)
1.6
1.7
FIGURE 5.148 Gain for 3D, 2D, 1D, and 0D semiconductor structures proposed by Asada et al.51
1957 Bipolar
427
1969 Unipolar E2 E1
Esaki tunnel diode
Doublebarrier resonant tunnel diode
Superlattice Lowdimensional quantum structure
FIGURE 5.149 Esaki inventions from the 1957 Esaki tunnel diode to the doublebarrier resonant diode to the superlat tice. In bipolar devices, electrons and holes are involved; in unipolar devices, only one type of charged particle is involved.
of superlattices (1969) and doublebarrier resonant tunneling diodes (1974). The resonant tunnel diode has even more spectacular characteristics than the Esaki tunnel diode and constitutes one of the possible contenders to replace CMOS technology. In Figure 5.149 we summarize the intellectual path followed by Esaki and colleagues in going from the first tunnel diode to the doublebarrier resonant tunnel diode and finally to lowdimensional quantum structures. Before arriving at the superlattice concept, Esaki and Tsu examined the feasibility of structural formation of potential barriers and wells that were thin enough to exhibit resonant tunneling (see Figure 5.149). Resonant tunneling in quantum mechanics is an effect observed in quantum wells that are coupled to electron reservoirs by thin tunnel barriers and corresponds to a resonant enhancement of transmission that is seen whenever the energy in the reservoirs matches one of the quantized values in the well. With barriers that are thin enough, an electron with energy lower than that of the height of the barrier can tunnel through the barrier, as long as there is an empty state of the same energy level waiting on the other side. The well is then “in resonance.” Resonant tunneling can be compared to the transmission of an EM wave through a FabryPérot resonator. The doublebarrier resonant tunneling diode shown in Figure 5.150 is a variant of the tunnel diode of Chapter 4, with thin barrier layers of GaAlAs and a GaAs quantum well with sharp interfaces and layers with a width comparable with the Schrödinger wavelengths of the electrons
428
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
A E0
EF
B
eVB
Current
Energy
n+–GaAs GaAIAs GaAs GaAIAs n+–GaAs
C
eVC
A
Distance
C
B
Voltage
FIGURE 5.150 Semiconductor resonant tunneling diode: device schematic and current voltage plot.
permitting resonant behavior. In the device schematic we see that the contacts/leads are made of highly doped ntype GaAs (n+ GaAs) and that two thin GaAlAs barrier layers (e.g., 20Å thick) enclose a thin GaAs well region (e.g., 50Å thick). The narrower bandgap material GaAs is enclosed by the considerably larger bandgap of GaAlAs to establish potential barriers at the surface of the GaAs well. Because the GaAs well is thin, the motion of electrons and holes is restricted in one dimension and is forced to occupy discrete states of energy instead of staying arbitrarily within an energy continuum. With a low bias applied, the quantized energy level in the well Eo is situated above EF, and no current flows (A in the schematic and the current voltage plot). At a medium bias, the level in the well has lined up with the conduction band, and current flows (B in the schematic and the current voltage plot). At yet higher bias, the energy level in the well is now situated below the bottom of the conduction band, and the current decreases (C in the schematic and the current voltage plot). The current voltage plot is typical for a tunnel diode (see Figure 5.150), but whereas the Esaki diode is a bipolar device (two types of charge carriers are involved: electrons and holes) and features relatively large dimensions, the resonant tunnel diode is a unipolar device (only one type of charge carrier) with layers that have a thickness comparable with the Schrödinger wavelengths of the electrons.
A superlattice is a material with periodically alternating layers of different substances. Such structures possess periodicity both on the scale of each layer’s crystal lattice and on the scale of the alternating layers. Quantum superlattices are a type of superlattice featuring arrays of periodic quantum structures: quantum wells, quantum dots, or quantum wires. Esaki and Tsu first proposed research on such artificially structured materials in 1960 to the Army Research Office (ARO). They envisioned engineered semiconductor superlattices based on a periodic structure of alternating layers of semiconductor materials with wide and narrow bandgaps using highprecision heteroepitaxial deposition methods such as molecular beam epitaxy (MBE) and metalorganic chemical vapor deposition (MOCVD) and involving III–V semiconductors. Although the proposal was favorably received by ARO, Physical Review rejected their first paper on the basis that it was “too speculative” and involved “no new physics.” In some circles, the ARO proposal was criticized as impossible to implement in practice. The main objection being that a humanmade structure with compositional variations on the order of a few nanometers would be thermodynamically unstable because of interdiffusional effects. Fortunately, it turned out that interdiffusion is negligible at the temperatures involved, and innovations and improvements in epitaxial techniques such as MBE and MOCVD made it possible to prepare highquality heterostructures
Photonics
the bandgap of GaAs is 1.43 eV, whereas it is 1.79 eV for Al xGa1−x As (x = 0.3). Thus, the electrons and holes in GaAs are confined in a 1D potential well of length L in the zdirection. Two or more quantum wells side by side give rise to a multiple quantum well (MQW) structure. This is called a compositional superlattice. An artificial periodic potential in a semiconductor crystal can also be fabricated through periodic ntype and ptype doped layers as shown in Figure 5.151B. Such a superlattice is called a doping superlattice. When the individual quantum wells are widely separated, the wave functions of the electrons and holes remain confined within the individual wells, and the array can be treated as a set of isolated quantum wells. Noninteracting MQWs like this are used to enhance/amplify absorption or emission of photons compared with what is possible with a single quantum well. In lasing, for example,
with predesigned potential profiles and impurity distributions with dimensional control close to the interatomic spacing. This great precision opened up the mesoscopic quantum regime to practical experimentation. Because a 1D potential could now be introduced along with the growth direction in the laboratory, famous examples in the history of 1D mathematical physics, including the abovementioned resonant tunneling (1930s), KrönigPenney bands (1931), Zener bandtoband tunneling (1934), and so on, all of which had remained textbook exercises, could for the first time be practiced in the laboratory. The superlattice example shown in Figure 5.151A is formed by a periodic array of quantum wells produced by the growth of alternate layers of a widebandgap (AlGaAs) and narrower bandgap (GaAs) semiconductors in the growth direction. At 300 K,
(A)(b)
AlxGa1–xAs
GaAs AlxGa1–xAs
AlxGa1–xAs
GaAs AlxGa1–xAs
Z
AlxGa1–xAs
AlxGa1–xAs
GaAs
Multiple quantum wells
Quantum well GaAs
(A)(a)
429
Compositional superlattice
Electron energy
Conduction band
Energy gap
Eg1
Eg2
Valence band D
l 2
l
3l 2
5l 2
2l
3l
Distance x (B)
Doping superlattice
Electron energy
Conduction band +++ +++ Energy gap–E–g
+ –––
–––
+ –––
Valence band
FIGURE 5.151 (A) Superlattice formed by a periodic array of quantum wells produced by the growth of alternate layers of wider bandgap (AlGaAs) and narrower bandgap (GaAs) semiconductors in the growth direction. Schematics of the arrangement (a) and the energy bands of multiple quantum wells (b). This is a compositional superlattice. (B) Artificial periodic potential in a semiconductor crystal made through periodic ntype and ptype doped layers. Such a superlattice is called a doping superlattice.
430
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
the stimulated emission is amplified by photons transversing through MQWs, with each well acting as an independent lasing medium. One of the most interesting applications of superlattices is the quantum cascade laser. In the April 1994 issue of Science, Faist, Capasso, Sivco, Sirtori, Hutchnson, and Cho of AT&T Bell Labs reported a new type of farinfrared laser called the quantum cascade laser.52 The idea of this superlattice device was first proposed by Rudolf Kazarinov (who is now with AT&T Bell Labs) and Robert Suris of A. F. Ioffe Institute in 1971 (http://www.mtmi.vu.lt/legacy/ pf k/funkc_dariniai/nanostructures/super lattice. htm). The Bell Labs’ work thus represents a real breakthrough that had been anticipated for almost a quarter of a century. Unlike quantumconfined lasers, which involve interband transitions between the conduction band and valence band, these quantum cascade lasers involve transitions of electrons between the various subbands (minibands) corresponding to different quantized levels of the conduction band. Because only electron transitions are involved, one refers to these types of lasers as unipolar lasers. There could be ∼50 quantum wells in an MQW laser geometry. The barrier layers are very thin (1–3 nm), and an excited electron may emit 25–75 photons as it cascades down the ladder of subbands in the conduction band. Quantum cascade lasers have been demonstrated for wavelengths between 3 and 20 μm, which is useful for sensing atmospheric pollution. Quantum cascade lasers, operating on intraband transitions and emitting in
the midinfrared region, are used, e.g., for trace gas analysis. In what follows we clarify how these bands within the conduction band come about. If the thickness of the widebandgap barrier layer in Figure 5.151 is small enough so that electrons may tunnel through, then the situation becomes similar to what happens when individual atoms are brought together in a crystal. To understand the interaction between these very closely spaced quantum wells better, we follow the thinking of Esaki and Tsu. Let us bring a set of N quantum wells together as shown in Figure 5.152. These wells consist again of alternate layers of GaAs (well) and AlGaAs (barriers). First, consider two wells in this array only, each with their own set of quantized levels En and labeled with their own quantum numbers n = 1, 2, 3, along the confinement direction (the growth direction). Reducing the separation between these two wells allows the wave functions to overlap, and the same (degenerate) energy levels En of the two wells now form two new states: En(1) and En(2) (just as we saw in Chapter 3 when bringing atoms together), where En(1) = En – Δn and En(2) = En + Δn. The magnitude of the splitting 2Δn depends on the level En. The higher the energy En, the more the wave function extends into the energy barrier between the wells, allowing for stronger interaction between the wave functions in those wells and leading to a larger splitting Δ n. Bringing N wells together, instead of only two, increases the energy degeneracy for all N wells, producing N levels closely spaced in a socalled miniband. In the
Z GaAs AIGaAs
E2 E1 Ec GaAs
AIGaAs
Ev Substrate
Multiple quantum well (GaAs/AIGaAs)
Z Energy bands of MQW
FIGURE 5.152 Schematic of formation of minibands in a superlattice consisting of alternate layers of GaAs (well) and AlGaAs (barriers).
Photonics
case illustrated in Figure 5.152, individual levels E1 and E2 in the quantum wells are split into two minibands; the higherenergy miniband has a greater bandwidth than the lowerenergy miniband for the reason explained above (larger splitting for higherenergy levels). Just as in a crystal where the periodic atomic potential leads to band formation in a superlattice, an artificial, humanmade periodical potential causes the formation of minibands. Thus, the introduction of the 1D superlattice potential perturbs the band structure of the host materials, yielding a series of narrow subbands and forbidden gaps that arise from the subdivision of the Brillouin zone into a series of minizones. Most semiconductor devices are operated based on the interband transitions, namely, between the conduction and valence bands. These devices are usually bipolar involving a pn junction. A new class of devices is based on the transitions between the subbands or minibands in the conduction or valence bands as described here. These intraband devices are unipolar and are faster than the intraband devices. Today a wide variety of engineered structures have been developed that exhibit extraordinary electronic transport and optical properties that do not exist in any natural crystals. This new degree of freedom offered in semiconductor research through advanced materials engineering has inspired many ingenious experiments, resulting in observations of not only predicted effects but also totally unknown results, and it appears that nearly half of all semiconductor physicists in the world are working now in this area. In addition to being used in quantum cascade layers, superlattice structures have been used in field effect transistors, where several quantum wells provide parallel conducting channels, increasing the device currentcarrying capabilities and hence the output power. Superlattices are also used for photodetectors and for novel LEDs. Photonic Crystal and Lasers Earlier in this chapter we listed as an important benefit of photonic crystals the ability to control spontaneous emission and to modify the state density and group velocity of light by creating structure defects. We pointed out that these structures could be used to create novel, highly efficient lasers that emit light
431
in a very narrow wavelength range. Point defects in photonic crystals act as highQ resonator cavities and have been used in lowthreshold photonic crystal lasers. In photonic lasers, only the wavelength that matches the wavelength of the defect mode is amplified because it can propagate freely through the material. The intensity of the propagating light increases as it undergoes successive reflections and travels back and forth through the photonic crystal. Meanwhile, light at other wavelengths is trapped within the photonic crystal and cannot build up. This means that the laser light is emitted in a narrow wavelength range that is directly related to the geometry of the microcavity.
Questions Questions by Chuan Zhang, UC Irvine 5.1: In a traditional lithography system using
iline (365 nm) wavelength, the numerical aperture is NA = 0.8. Can we use this system to fabricate a pattern with a minimum line width of 65 nm? List several ways of increasing the resolution of the lithography system. 5.2: A beam of light with a wavelength of 500 nm goes through an aperture that has a diameter of 0.1 mm and generates an Airy disk on the image plane very far from the aperture. If the diameter of the Airy disk is 50 mm, what is the distance between the aperture and the image plane? If the distance becomes 3 times longer, then what would the size of the Airy disk be? 5.3: A beam of monochromatic red light with a frequency of 500 terahertz and a wavelength of 600 nm goes from vacuum into a piece of glass with an incidence angle of 30°. After getting into the glass, the wavelength of the light becomes 450 nm. What is the angle of refraction? 5.4: A beam of monochromatic light with a frequency of 500 terahertz and a wavelength of 600 nm transmits in water, which has a refractive index of 1.333, and then the light is totally internally reflected at the interface
432
5.5:
5.6:
5.7:
5.8:
5.9:
5.10:
5.11:
5.12: 5.13:
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
of water and an unknown material with an incident angle 60°. What is the minimum possible wavelength of that light when it is transmitted in the unknown media? Make a comparison between righthanded and lefthanded materials. List the two most important applications for lefthanded materials. A stationary proton with an electric charge of 1.60217653·10 −19 C and a mass of 1.6726·10 −27 kg is accelerated to 0.8c under an electric field intensity of E0 = 1·106 V/m; what is the weight of the particle at this speed and how long did it take to reach the final speed? In an optical microscope, if we replace the light source (⎣ = 550 nm) of visible light with ultraviolet (⎣ = 275 nm), what is the percentage increase of resolution? If the numeral aperture in air is 0.8, what is the smallest distance between two parallel lines that can be resolved with the ultraviolet light source? And what if we immerse the lens system into an oil medium with a refractive factor of 1.5? A beam of light has a wavelength of 500 nm in air. After crossing through another medium, its wavelength becomes 200 nm. Assuming the difference of permeability between this medium and air is very small, what is the relative dielectric constant for this medium? The refractive index of a crystal is 1.7, dn/d⎣ = –0.15 um–1; what is the ratio of phase velocity to group velocity for light with a wavelength of 400 nm? What is the optical phenomenon called light polarization? A beam of light becomes completely polarized after being reflected from the interface between water and an unknown medium. We know the incident angle is 60°. What is the refractive index of the unknown medium? How does an optical fiber work? Explain why fiber losses increase if the fiber is bent? How can plasmonics avoid the bending problem? How can surface plasmons be excited? What are some applications? What is the difference between a direct bandgap and indirect bandgap semiconductor?
Which one has a higher photon absorption and electron transition possibility? For optoelectronic applications, which kind of semiconductor is preferred? 5.14: Compare the similarities and differences between photonic crystals and metamaterials. 5.15: Why is there a resolution limit for traditional lenses? How does a superlens made from negative refractive index material exceed that limit? 5.16: What is Raman scattering? Compare Raman spectroscopy with infrared (IR) spectroscopy. 5.17: As the size of a metal particle becomes
smaller and smaller, will there be any changes in its color? Explain why. 5.18: Why is the sky blue, while clouds are white? 5.19: Show that in the Maxwell equation Δ × H = uD Jc all three terms have the same dimenut sions. 5.20: If an eye has a pupil opening (lens diameter) of 4 mm, can it resolve two point sources of 600 nm light (direct or reflected) that are 5 mm apart and 10 m away? Does the eye’s resolving ability improve if the pupil enlarges to 5 mm?
References 1. Cheng, D. K. 1989. Field and wave electromagnetics. 2nd ed. Boston: AddisonWesley. 2. Taya, M. 2005. Electronic composites. New York: Cambridge University Press. 3. Veselago, V. G. 1968. The electrodynamics of substances with simultaneously negative values of ε and μ. Sov Phys Usp 10:509–14. 4. Ashkin, A. 1970. Acceleration and trapping of particles by radiation pressure. Phys Rev Lett 24:156–59. 5. Berns, M. W., and D. E. Rounds. 1970. Cell surgery by laser. Scientific American 222: 98–103. 6. Atwater, H. A. 2007. The promise of plasmonics. Scientific American 296:56–63. 7. Greene, B. 1999. The elegant universe. New York: W.W. Norton. 8. Parker, B. 1987. Search for a supertheory: from atoms to superstrings. New York: Plenum Press. 9. Faraday, M. 1858. The Bakerian lecture: experimental relations of gold (and other metals) to light. Philos Trans Royal Soc London 147:145–81. 10. Padovani, S., C. Sada, P. Mazzoldi, B. Brunetti, I. Borgia, A. Sgamellotti, and A. Giulivi. Copper in glazes of renaissance luster pottery: nanoparticles, ions, and local environment. J Appl Phys 93:10058–63.
Photonics 11. Bohren, C. F., and D. R. Huffman. 1983. Absorption and scattering of light by small particles. New York: John Wiley and Sons. 12. Gans, R. 1915. Fortpflanzung des Lichts durch ein inhomogenes Medium. Ann Physik 352:709–36. 13. Link, S., and M. ElSayed. 1999. Size and temperature dependence of the plasmon absorption of colloidal gold nanoparticles. J Phys Chem B 103:4212–17. 14. Westcott, S. L., S. J. Oldenburg, T. R. Lee, and N. J. Halas. 1998. Formation and adsorption of clusters of gold nanoparticles onto functionalized silica nanoparticle surfaces. Langmuir 14:5396–401. 15. Chen, J., B. Wiley, Z.Y. Li, D. Campbell, F. Saeki, H. Cang, L. Au, J. Lee, X. Li, and Y. Xia. 2005. Gold nanocages: engineering their structure for biomedical applications. Adv Mater 17:2255–61. 16. Maier, S. A., M. L. Brongersma, and H. A. Atwater. 2001. Electromagnetic energy transport along arrays of closely spaced metal rods as an analogue to plasmonic devices. Appl Phys Lett 78:16–18. 17. Frenkel, J. 1931. On the transformation of light into heat in solids. I. Phys Rev Lett 37:17–44. 18. Frenkel, J. 1931. On the transformation of light into heat in solids. II. Phys Rev 37:1276–94. 19. Gross, E. F. 1956. Optical spectrum of excitons in the crystal lattice. Il Nuovo Cimento 3:672–701. 20. Gustav, M. 1908. Beiträge zur Optik Trüber Medien, Speziell Kolloidaler Metallösungen. Ann Physik 330:377–445. 21. Jeanmaire, D. L., and R. P. V. Duyne. 1977. Surface Raman spectroelectrochemistry. Part I. Heterocyclic, aromatic, and aliphatic amines adsorbed. J Elecroanal Chem 84:1–20. 22. Shalaev, V. M. 1999. Nonlinear optics of random media: fractal composites and metaldielectric films. Berlin: Springer. 23. Laserna, J. J. 1993. Combining fingerprinting capability with trace analytical detection: surfaceenhanced raman spectometry. Anal Chim Acta 283:607–22. 24. Kneipp, K., H. Kneipp, V. B. Kartha, R. Manoharan, G. Deinum, I. Itzkan, R. R. Dasari, and M. S. Feld. 1998. Detection and identification of a single DNA base molecule using surfaceenhanced raman scattering (SERS). Phys Rev E57:R6281–84. 25. John, S. 1987. Strong localization of photons in certain disordered dielectric superlattices. Phys Rev Lett 58:2486–89. 26. Yablonovitch, E. 1987. Inhibited spontaneous emission in solidstate physics and electronics. Phys Rev Lett 58:2059–64. 27. Ho, K. M., C. T. Chan, and C. M. Soukoulis. 1990. Existence of a photonic gap in periodic dielectric structures. Phys Rev Lett 65:3152–55. 28. Yablonovitch, E., and T. J. Gmitter. 1989. Photonic band structure: the face centered cubic case. Phys Rev Lett 63:1950. 29. Ozbay, E. 1994. Micromachined millimeterwave photonic bandgap crystals. Appl Phys Lett 64:2059–61. 30. Lehmann, V., and H. Foll. 1990. Formation mechanism and properties of electrochemically etched trenches in ntype silicon. J Electrochem Soc 137:653–60. 31. Grüning, U., V. Lehmann, S. Ottow, and K. Busch. 1996. Macroporous silicon with a complete twodimensional photonic band gap centered at 4.9 μm. Appl Phys Lett 68: 747–49. 32. Campbell, M., D. N. Sharp, M. T. Harrison, R. G. Denning, and A. J. Turberfield. 2000. Fabrication of photonic crystals for the visible spectrum by holographic lithography. Nature 404:53–56.
433
33. Vlasov, Y. A., X. Z. Bo, J. C. Sturm, and D. J. Norris. 2001. Onchip natural assembly of silicon photonic bandgap crystals. Nature 414:289–93. 34. Joannopoulos, J. D. 2008. Photonic crystals: molding the flow of light. Princeton, NJ: Princeton University Press. 35. Coen, S., A. H. Chau, R. Leonhardt, J. D. Harvey, J. C. Knight, W. J. Wadsworth, and P. S. Russell. 2001. Whitelight supercontinuum generation with 60ps pump pulses in a photonic crystal fiber. Opt Lett 26:1356–58. 36. Cubukcu, E., K. Aydin, E. Ozbay, S. Foteinopoulou, and C. M. Soukoulis. 2003. Electromagnetic waves: negative refraction by photonic crystals. Nature 423:604–05. 37. Research Highlights. 2007. Invisibility cloak in sight. Nature 444:4–5. 38. Pendry, J. B., A. J. Holden, D. J. Robbins, and W. J. Stewart. 1998. Low frequency plasmons in thinwire structures. J Phys Condens Matter 10:4785–809. 39. Pendry, J. B., A. J. Holden, W. J. Stewart, and I. Youngs. 1996. Extremely low frequency plasmons in metallic mesostructures. Phys Rev Lett 76:4773–76. 40. Pendry, J. B., A. J. Holden, D. J. Robbins, and W. J. Stewart. 1999. Magnetism from conductors and enhanced nonlinear phenomena. IEEE Trans Microwave Theory Techn 47:2075–84. 41. Wiltshire, M. C. K., J. B. Pendry, I. R. Young, D. J. Larkman, D. J. Gilderdale, J. V. Hajnal. 2001. Microstructured magnetic materials for RF flux guides in magnetic resonance imaging. Science 291:849–51. 42. Shelby, R. A., D. R. Smith. and S. Schultz. 2001. Experimental verification of a negative index of refraction. Science 292:77–79. 43. Smith, D.R., and N. Kroll. 2000. Negative refractive index in lefthanded materials. Phys Rev Lett 85:2933. 44. Smith, D. R., W. J. Padilla, D. C. Vier, S. C. NematNasser, and S. Schultz. 2000. Composite medium with simultaneously negative permeability and permittivity. Phys Rev Lett 84:4184–87. 45. Shalaev, V. M., W. Cai, U. K. Chettiar, H. K. Yuan, A. K. Sarychev, V. P. Drachev, and A. V. Kildishev. 2005. Negative index of refraction in optical metamaterials. Opt Lett 30:3356. 46. Soukoulis, C. M., S. Linden, and M. Wegener. 2007. Negative refractive index at optical wavelengths. Science 315:47–49. 47. Notomi, M. 2000. Theory of light propagation in strongly modulated photonic crystals: refraction like behavior in the vicinity of the photonic band gap. Phys Rev B 62:10696–705. 48. Fang, N., and X. Zhang. 2003. Imaging properties of a metamaterial superlens. Appl Phys Lett 82:161. 49. Fang, N., H. Lee, C. Sun, and X. Zhang. 2005. Subdiffractionlimited optical imaging with a silver superlens. Science 308:524–37. 50. Arakawa, Y., and H. Sakaki. 1982. Multidimensional quantum well laser and temperature dependence of its threshold current. Appl Phys Lett 40:939–41. 51. Asada, M., Y. Miyamoto, and Y. Suematsu. 1986. Gain and the threshold of threedimensional quantumbox lasers. IEEE J Quant Electron QE22:1915–21. 52. Faist, J., F. Capasso, D. L. Sivco, C. Sirtori, A. L. Hutchinson, and A. Y. Cho. 1994. Quantum cascade laser. Science 264:553–56. 53. Meinhart, C. D., and S. T. Wereley. 2003. The theory of diffractionlimited resolution in microparticle image velocimetry. Meas Sci Technol 14:1047. 54. Pendry, J. B. 2000. Negative refraction makes a perfect lens. Phys Rev Lett 85:3966.
6 Fluidics Outline Introduction Macroscale Laws for Fluid Flow Breakdown of Continuum Theory in Fluidics Forces at Interfaces Mixing, Stirring, and Diffusion in Low Reynolds Number Fluids Chemical Reactions in Microchambers—Microreactors Fluid Propulsion Electrowetting Centrifugal Fluidic Platform—CD Fluidics Scaling in Analytical Separation Equipment Acknowledgments Questions Further Reading References
Angry Sea at Naruto Ando Hiroshige, 1830
Observe the motion of the surface of the water, which resembles that of hair, which has two motions, of which one is caused by the weight of the hair, the other by the direction of the curls; thus the water has eddying motions, one part of which is due to the principal current, the other to random and reverse motion. Leonardo da Vinci, 1510 The current nano hype makes us forget that already Sir Isaac Newton described nanoscale phenomena, the socalled Newton rings (left; no, that is not spaghetti he is looking at). Newton also very clearly formulated experiments of microfluidics by describing experiments with capillary flow between parallel glass plates (below). So, neither nano nor micro are [sic] really very novel it seems!
Based on an editorial by Andreas Manz and Harpal Minhas for Lab on a Chip
These [natural] laws may have originally been decreed by God, but it appears that he has since left the universe to evolve according to them and does not now intervene in it. Stephen Hawking A Brief History of Time 435
436
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Introduction
Macroscale Laws for Fluid Flow
Fluid mechanics (fluidics) is the study of motion of fluids (liquids and gases) and the forces associated with that motion. In Chapter 6 we introduce fluidics, compare various fluidic propulsion mechanisms, and discuss the influence of miniaturization on fluid behavior. Our treatment deals with macroscale, microscale, and nanoscale fluidic phenomena. Given the current academic and industrial interest, fluidics in miniaturized analytical equipment is detailed in this chapter as well. Example applications we discuss include electroosmotic pumping systems, diffusive separation systems, micromixers, DNA amplifiers (PCR), compact disc diagnostic platforms, and cytometers. Newton and da Vinci aside (see insets above), fundamental work on the physical behavior of f luids in micro and nanomachined structures only started in the early 1980s. In the micro and nanodomain, many factors seem to upset the old f luidics continuum order: NavierStokes equations (NSEs), with noslip boundary conditions at the f luid interface, cannot always be applied, and slip f low, creep f low, intermolecular forces, etc., start suggesting molecularbased f low models instead. For gases, breakdown of macroscale physics is readily recognized, and some molecularbased modeling progress has been made. For liquids, with molecules much more closely packed, modeling has proven to be much more elusive. Microfluidics and nanofluidics present researchers with exciting future applications. These include the characterization of individual molecules (e.g., reading the base sequence in DNA by feeding the molecule through a nanopore), studying the kinetics of very fast reactions, isolating a molecule in a nanometric space for detection purposes, further increasing the role of surfaces in catalytic reactions, manipulation of single molecules, labeling and studying of conformational changes of single molecules, applying intense electrical or magnetic fields to control chemical reactions, constructing hybrid systems by assembling biomolecules in NEMS structures, etc.
Definition of Fluids and Types of Flow A fluid, in our common experience, is a substance that has volume but no shape; that is, a fluid is a material that cannot resist a shear force or shear stress without moving.1 The two most important parameters characterizing a fluid are density and viscosity. Density or specific mass, ρ, of a fluid is the mass per unit volume (in kgm−3), and dynamic viscosity, η, is the fluid property that causes shear stresses when the fluid is moving; without viscosity there would be no fluid resistance. Dynamic viscosity is measured as kg/ms (SI system), that is, Pa·s or Poiseuille (Pl)*, and is given as the ratio of shear stress, τs, to shear rate, Γs: H
Ts 's
(6.1)
The dynamic viscosity of air is 1.85 × 10−5 kg/ms, and for water it is 10−3 kg/ms. Equation 6.1 can be better understood from an inspection of Figure 6.1, in which we illustrate two large plates, of area A, separated by a fluid layer of uniform thickness, d. When one of the two plates is moved in a straight line relative to the other at an average velocity V, the shear force required for obtaining V is given by τzx (=F/A = force/area in N m−2, i.e., Pa): F V T zx H d A
(6.2)
and V/d corresponds to the shear rate Γs (velocity gradient in s−1). The first subscript in τzx is in the direction normal to the shearing force (z), and the second x = Vt F = zx A B
E
C
F
V d V
Steady state
d
A
D
FIGURE 6.1 Schematic of shearing experiment. *
In the CGS system it is measured in poise (1 poise or P = 10 –1 N·sm–2) and 1 Pl = 10 P.
Fluidics
subscript is in the direction of the force (x). Equation 6.2 can be generalized as: T zx H
dV dz
N
Bingham plastic
Shear stress
Shear thinning
(6.3) Yield stress
This relationship is known as Newton’s Law of viscosity, and it relates the velocity gradient in the fluid to the shear stress. Thus, viscosity refers to friction between layers. The normal component of stress (Fn) for a fluid at rest is called the pressure, and the tangential component (Ft) is the shear stress (Figure 6.2). A solid can resist applied shear by deforming, and the stress is proportional to the strain, but a fluid deforms continuously under applied shear, and the stress is proportional to strain rate. The kinematic viscosity, ν in m2/s, or also myria (=10,000) Stokes (ma St, where the Stokes is the CGS unit, 1 m2/s = 104 St), is the ratio of the absolute viscosity to density given by: H R
(6.4)
Its value is 1.43 × 10 –5 m2/s for air and 10–6 m2/s for water. For Newtonian fluids such as water and air, the shearing stress and the velocity are linearly related so that the viscosity is only a function of the nature of the fluid.2 For nonNewtonian fluids such as milk and blood,* the viscosity is also a function of the velocity gradient (see Figure 6.3). Most often, the viscosity in these cases diminishes when the velocity gradient increases, and these types of materials are called pseudoplastics. A Bingham plastic
437
Newtonian Shear thickening
Shear strain rate
FIGURE 6.3 Newtonian and nonNewtonian fluids compared. The viscosity usually diminishes when the velocity gradient increases, and these types of materials are called pseudoplastics.
is a viscoelastic material that behaves as a rigid body at low stresses but flows as a viscous fluid at high stress. Once a critical shear stress (or “yield stress”) is exceeded, the material flows as a Newtonian fluid. NonNewtonian flow behavior of fluids can offer real advantages. Paint, for example, should be easy to spread, so it must have a low viscosity at the high shear caused by the paintbrush. Many cleaning fluids and furniture waxes have similar properties. The causes of nonNewtonian flow depend on the colloid chemistry of the particular product. The fundamental laws governing fluid motion are the socalled NavierStokes equations (NSEs) (see Navier and Stokes in Figure 6.4). The NSEs are 3D vector equations and represent the differential forms of three equations: 1) the conservation of mass, 2) the conservation of linear momentum, and 3) the conservation of energy (this third equation
Normal to surface Force acting F on area dA
Fn
dA
Ft
Tangent to surface
FIGURE 6.2 Pressure and shear stress in a fluid. *
Although serum is a Newtonian fluid, the presence of red blood cells makes whole blood nonNewtonian. The same is true for mayonnaise; the oil in it is Newtonian, but the emulsion with yolk makes it nonNewtonian.
(a)
(b)
FIGURE 6.4 (a) French mathematician L. M. H. Navier (1758–1836) and (b) English mathematician Sir G. G. Stokes (1819–1903) formulated the NavierStokes equations by including viscous effects in the equations of motion.
438
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
that makes up the complete set of NSEs will not be separately derived here). The NavierStokes equations are applicable to the description of the motion of a fluid volume at an arbitrary location in a flow field at any instant of time. One often classifies flows as a means to simplify the assumptions governing the partial differential NavierStokes equations. Lower dimensional flows reduce the complexity of analytical and computational solutions. We start by introducing the NSEs and show how they simplify depending on the type of flow. Next we derive two of the actual NSEs. 1. The Conservation of Mass Equation. The continuity equation in differential form is given as: uR RV 0 ut
(6.5)
Mass is neither created nor destroyed; there are no sources or sinks, or the net inflow rate, i.e., (inflow − outflow), must equal the accumulation rate. For one direction (e.g., the xdirection with velocity component u) this yields:
uR u Ru 0 ux ut
(6.6)
A flow is classified as incompressible if the density remains constant. For an incompressible fluid ¥ ´ uR ¦§ R constant or ut 0µ¶ , this results in: u 0 (for 1D) and V 0 (for 3D)
(6.7)
Note that the above is true even for unsteady flows. Liquid flows typically are incompressible, but gas flows are compressible, especially at high speeds. The Mach number, Ma = V/c, is the ratio of flow velocity to the speed of sound (c) and may be regarded as the ratio of inertial forces to elastic ones. The Mach number is a good indicator of whether compressibility effects are important (Figure 6.5). 2. The Conservation of Momentum. In vector notation, the conservation of momentum is given as: R
uV R V V p H 2 V Rg ut a b c d e
(6.8)
FIGURE 6.5 Ma = V/c. With Ma < 0.3 (∼100 m/s), incompressible; with Ma < 1, subsonic; with Ma = 1, sonic; with Ma > 1, supersonic; and with Ma >> 1, hypersonic.
where g is the gravitational acceleration, p is the driving pressure, and t is time. The gravitational acceleration is related to the gravitational potential Ω as g = −∇Ω. Each term in Equation 6.8 has the dimension of {m/L 2t 2}. The term a is the local acceleration of the fluid element. For a steady flow this term is zero. Steady flow implies no change at any point with time; transient terms in the NSE are then also zero: uV uR 0 ut ut
(6.9)
Transients usually describe a starting or developing flow (Figure 6.6). A change in coordinate system (e.g., Cartesian, cylindrical, spherical) may facilitate the mathematical treatment. For example, from Figure 6.6, for a fully developed pipe flow, velocity V(r) is a function of radius r, and pressure p(z) is a function of distance z along the axis. The next term in Equation 6.8 is the term b, which represents the convective acceleration of the fluid particle, and it predicts how the flow differs from one location to the next at the same instant of time. Uniform flow has no convective acceleration. The c term is the pressure acceleration caused by the “pumping” action. The d term is the viscous deceleration term resulting from the fluid’s frictional resistance. The e term is the acceleration caused by gravity (weight). Regions where frictional effects are dominant are called viscous regions. They usually are close to solid surfaces (Figure 6.7). Regions where frictional forces are small compared with inertial or pressure forces are called inviscid. Such fluids are
Fluidics Developing velocity profile, V(r, z)
439
Fully developed velocity profile, V(r)
r
z
FIGURE 6.6 From a developing velocity profile to a fully developed velocity profile.
considered to be ideal, and in that case the d term in Equation 6.8 can be neglected: R
uV R V V p Rg ut
(6.10)
This expression is known as the Euler equation of motion. Even though this relation is simpler than the NavierStokes, an analytical solution is still not generally possible because the advective accelerations make the equations nonlinear. Internal flows (e.g., inside a pipe), as illustrated in Figure 6.6, are dominated by the influence of viscosity throughout the flow field, whereas in external flows, viscous effects are limited to the boundary layer and wake as illustrated in Figure 6.8. In the case of very slow fluid motion, the total acceleration term (a + b) as well as the acceleration caused by gravity (e) are zero. Equation 6.8 then reduces to the equation for Stokes flow or creep flow: p H 2 V
(6.11)
This equation applies when dealing with very viscous fluids, capillary flow, and certain molten metals. Flows are also distinguished as being laminar, turbulent, or transitional, as shown in Figure 6.9. An important concept in fluidics concerns the idea of streamlines. A streamline is a path traced out by a
Inviscid flow region
FIGURE 6.8 External flow. Viscous effects are limited to the boundary layer and wake around the object in the flow.
massless particle as it moves with the flow. Velocity is tangent to a streamline at every point. In the laminar case, the fluid motion is highly ordered with smooth streamlines. In the case of turbulence, one has a highly disordered fluid motion characterized by velocity fluctuations and eddies. In the transitional case, one obtains a flow that contains both laminar and turbulent regions. We will see below that it is the Reynolds number, Re = ρVL/η, that is the key parameter in determining whether a flow is laminar or turbulent. A rotational flow is one where streamlines close in on themselves while in an irrotational flow the streamlines do not close in on themselves.
Boundary Conditions Continuum Hypothesis In a continuum all quantities are defined everywhere and vary continuously from point to point. To understand this better, consider an “average” density, ρ, averaged over a fluid “particle” with volume L3 as illustrated in Figure 6.10. For the “average density,” it
Laminar
Transitional
Viscous flow region Inviscid flow region
FIGURE 6.7 Inviscid and viscous regions in a liquid flow.
Turbulent
FIGURE 6.9 Laminar, transitional, and turbulent streamlines.
440
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Molecular ﬂuctuations
System size variations
Local value of the density
L1
L2
L3
L
FIGURE 6.10 Schematic representation of the variation of instantaneous density of the fluid particle with respect to its volume.
holds that ρ = N·m/L3, with N the number of molecules and m the mass of each molecule. The continuum assumption fails when the sampling volume becomes too small. For the smallest particle size (L1), molecular fluctuations may cause density variations. Also, for large volume elements, of the scale of the system itself (L3), density can evolve because of spatial variations caused by changes in, for example, pressure (e.g., shocks) or temperature. It is only in the intermediate, “mesoscopic” size regime (L2), the plateau in Figure 6.10, where it is possible to establish equations of fluid flow assuming a continuous medium. The continuum hypothesis thus assumes that in the L2 regime (with L1 1 such as silicone oils (Pr = 10 to 107). Convection: Newton’s Cooling Law Fourier’s Law, as explained above, describes heat transport in solids through conduction. Convection heat transfer is the mode of energy transfer between a solid surface and an adjacent liquid or gas that is in motion, and it involves the combined effects of conduction and fluid motion. In Figure 6.28 we show velocity and temperature variation of air flowing over a hot substrate and illustrate the difference between forced and natural convection. In Newton’s Cooling Law, the heat flux between a solid surface at temperatures Ts and the bulk temperature of a fluid, T∞, is proportional to the temperature difference, the exposed area A, and the convective heat transfer coefficient h:
q hA Ts Td Velocity variation of air
V
T∞
Air flow
(6.62)
T Temperature variation of air
Qconv A
Ts Hot block
Forced convection
Natural convection Air
Air Hot egg
Hot egg
FIGURE 6.28 Velocity and temperature variation of air flowing over a hot substrate, and the difference between forced and natural convection.
452
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
The units of h are W/m2K. For most experiments, h is related to the fluid velocity u, or h ∼ u, which in turn is proportional to l−1. As in the case of conductive heat transfer, 10 times reduction in size will give 10 times reduction in heat transfer. It is important to keep in mind that the energy exchange at the solid/ fluid interface is by conduction and that this energy is then convected away by fluid flow. Convective heat transfer also can be discussed in terms of the Nusselt number (William Nusselt, 1882– 1957), the dimensionless heat transfer coefficient: Nu = hL/κ
(6.63)
with L (in W/mK) the characteristic length and κ the thermal conductivity of the solid, so this number may be viewed as the ratio of convection to conduction for a layer of fluid. With Nu = 1, we have pure conduction, and higher values mean that heat transfer is enhanced by convection. In a boundary layer situation, L is the thickness of the boundary layer. To determine a numerical value for Nu in a forced convection situation, one uses the relationship Nu = α (Re)β (Pr)γ, and for a free convection at low velocity Nu = α(Re)β(Pr)γ (Gr)δ . The parameters α, β, γ, and δ in this last expression are determined by the experimental setup. From the dimensionless numbers— the Reynolds number (Re), the Prandtl number (Pr), and the Grashof number (Gr)—Re has the dominant effect on h. The Grashof number Gr is defined as: Gr
L3R2 gB$T H
(6.64)
with L the characteristic length (m), ρ the density (kg/m3), g the acceleration resulting from gravity (9.080665 m/s2), β the coefficient of volumetric expansion (K−1), ΔT the temperature difference between the wall and the surrounding bulk (°C), and η is the viscosity (Pa·s). The Grashof number is a ratio between the buoyancy forces and viscous forces. Typical values of the convection heat transfer coefficient h (W/m2K) are shown in Table 6.2. Radiation The third mode of heat transmission is the result of electromagnetic wave propagation, which occurs both in fluidic media and in an absolute vacuum (Figure 6.29).
TABLE 6.2 Typical Values of the Convection Heat Transfer Coefficient h [W/m2K] Free convection Gases Liquids
h 2–25 50–1,000
Forced convection Gases Liquids
25–250 50–20,000
Convection with phase change Boiling or condensation
2,500–100,000
Radiation is the energy emitted by matter that is at a finite temperature. Radiant heat transfer is proportional to the fourth power of the absolute temperature, whereas we learned that conduction and convection are linearly proportional to temperature differences. The fundamental StefanBoltzmann’s law E = σT 4 (Chapter 3): E = 5.67 × 10−8 T 4
(3.71)
where T is the absolute temperature, and the constant is independent of surface, medium, and temperature. The ideal emitter, or blackbody, is one that gives off radiant energy according to Equation 3.71. All other surfaces emit somewhat less than this amount, and the thermal emission from many surfaces (gray bodies) can be represented by: E E 5.67 s 10 8 T 4
(6.65)
where ε, the emissivity of the surface, ranges from zero to one. Example 6.4: Thermal Problem in Miniaturization Let us apply the insights gathered so far to a simple practical problem, i.e., the calculation of Person 30°C Fire 900°C Air 5°C Radiation
FIGURE 6.29 Example of radiation heat.
Fluidics
the thermal time constant associated with the sudden transfer of an object from one temperature to another. The heat flow into a material of volume V0, at a uniform temperature T0, through boundary surface A, when the volume is suddenly immersed in an environment of temperature T∞, is equated to the rate of increase of the internal energy of the material in volume V0, or:
q hA T0 Td Rcp V0
dT dt
(6.66)
Solving this differential equation gives us the temperature of the solid as a function of time: ¥ h! ´
¦ µt T Td Rc V e § p 0¶ T0 Td
(6.67)
The term on the left represents the dimensionless temperature, and it can be verified that the temperature in the solid decays exponentially with time and that the shape of the curve is determined by the time constant τc given by: Tc =
Rcp V0 hA
(6.68)
To develop a feeling for the above expression, we compare how fast a Ni rod of 0.5in. diameter and one with a 50μm radius come to equilibrium with their surroundings. For a cylinder, with V0 = πr2l and A = 2πrl, the above equation transforms to: Tc =
Rcpr 2h
(6.69) m−3,
Assuming h = 10 W/m K, ρ = 8900 kg and − 1 cp = 0.44 J kg /K gives a τc = 1.24 s for the bigger cylinder. If we assume equilibration with the surrounding temperature, T∞, in 4 τc, equilibration is reached in 5 s. For the 50μm Ni rod, equilibrium is reached after 0.039 s. 2
Biot’s Number When a solid body is placed in a surrounding of a different temperature, the body heats up or cools down, and internal temperature gradients that cause thermal stresses are set up. The dimensionless number that characterizes the magnitude of the established thermal gradient is the Biot number (Bi), the ratio of the average surface heat/transfer coefficient for convection from the entire surface (h), to
453
the conductivity of the solid (κ), for a characteristic dimension L, or: Bi
hL K
(6.70)
As L becomes smaller, the Biot number goes down. For Bi 1, convective and inertial forces do. Similarity of flow will always be maintained if the Reynolds number has an identical value for the bodies being considered.6 In laminar flow the resistance, caused by intermolecular viscous forces, is proportional to velocity, with turbulence the resistance, generated along the channel perimeter and related to channel shape, particle size, and concentration is proportional to the square of the velocity. Laminar flow is characterized by smooth flow of fluid in layers that do not mix: such flow also is called streamline flow. Turbulent flow is characterized by eddies and swirls that mix layers of fluid together. At sufficiently high velocity, a fluid flow can change from streamline to turbulent flow. The onset of turbulence can be found from the Reynolds number. If Re = 2000 or below, the flow is streamline; if 2000 < Re < 3000, the flow is unstable; and if Re = 3000 or above, the flow is turbulent.
1010
Reynolds number
454
105
100
10−5
Whale Tuna Dragonﬂy Squid Cabbage butterﬂy Goald beetle Houseﬂy
Paramecium Spermatozoa
DC 10 Benjamin Franklin (an aeroplane) Submarine
Eel Honeybee
Nematoda
Bacteria 1 nm
1 μm
1 mm
1 km
Size
FIGURE 6.30 Reynolds number for mobile machines in their fluidic environment as a function of their size.
A tiny rotor blade in an airfilled, 10μmwide capillary will only be able to rotate in milliseconds rather than microseconds. The consideration of moving small things in water is even more daunting, because water is like syrup to the submerged micromachine. Fluid systems in the microdomain are damped heavily and exhibit slow response times. In Figure 6.30, the Reynolds number for mobile machines in their fluidic environment is plotted as a function of size (length), and Table 6.3 lists some additional example Reynolds numbers. Bacteria must be seen as truly autonomous micromachines. Swimming in an aqueous environment, such small vessels are up against the tide with an Re of 10 −5 (see Table 6.3). Mechanical engineers have avoided designing such machines, but that is exactly how nature has done it, and bacteria are the most abundant life form on Earth.
Friction Factor Example 6.5: Equation 6.71 may be used to calculate the Reynolds number for the flow of air (η = 1 × 10–6 m2s−1) and water (η = 15 × 10–6 m2s−1) in a 50μmdiameter capillary. Assuming a velocity V = 500 × 10–6 ms−1 (10 times the diameter of the pipe per second), we obtain 0.0016 for air and 0.025 for water. Both are considerably less than 1, indicating that if fluids behave as a continuum, as is assumed in classical fluids, microsystems will operate in a viscousdominated Stokes regime.
We touched upon frictional resistance when discussing a falling sphere and when deriving pipe flow. When a fluid flows through a fluidic channel it experiences frictional resistance, and as a consequence, useful mechanical energy is degraded into unusable heat energy. Knowledge of frictional characteristics is vital for the design of any fluidic system. For a tube of circular crosssection, friction loss or head loss can be determined in terms of shear stress at the wall, τ: T
$pL 41
(6.72)
Fluidics
TABLE 6.3 Example Reynolds Numbers and Hydrodynamic Layer Thickness Description
Re
Earth’s tectonic plates (100 km at 10−8 m/s, kinematic viscosity is 1020 m2/s) Glacier Bacteria in water (1 μm at 10 μm/s and kinematic viscosity ν in water = 10−6 ma St) Sperm cells in semen A small marble falling in honey Fish in a tropical aquarium Human swimmer Bird Car (1.5 m long at 90 km/h, kinematic viscosity ν in air = 15 × 10−6 ma St)
10−23
FIGURE 6.31 Friction in pipe flow (τ = FD/A).
10−11 10−5
it is used mostly for heat transfer problems in pipe flow. In other words (see also Volume III, Equation 7.27 with τ = FD/A):
10−3 10−2 102 105 106 2.5 ×106
Airplane taking off at 300 km/h, 9m wingspan Pleasure boat (10m long at 21.6 km/h or 1,166 knots, and kinematic viscosity υ in water = 10−6 ma St) Large fish in the ocean
CD
50 × 106
Size of δ, hydrodynamic boundary layer (mm) ∼0.9 1.2
60 × 106
1.3
108
where l is the length of the tube in meters and L is the internal diameter of the pipe. With reference to Figure 6.31, Equation 6.72 is easily derived from the fact that the force balance is given by: p
455
PL2 PL2 p $p TPLl or 4 4 $pL T 4l
The shear stress, τ, at the wall is a function of five independent parameters: τ = f(η, ρ, V, L, k). The surface roughness of the pipe is given as k and can be described as a length. With five independent variables, the solution is very complex. However, the complexity can be reduced by use of only two nondimensional variables. The nondimensional shear stress, called the friction coefficient or Fanning friction factor, CD, can be tabulated as a function of the Reynolds number and surface roughness k only. The Fanning friction factor CD is defined as 2τ/ρV2 and
FD 1 2 RV A 2
¥ RVL k ´ T f¦ , 2 § H L µ¶ RV 2
(6.73)
with k/L the relative surface roughness. Civil engineers replace the Fanning friction factor frequently with the Moody friction factor, CM, related to CD as: C M 4C D
8T RV 2
(6.74)
Yet differently, Coulson and Richardson define the friction factor as τ/ρV2.9 The friction factor for pipe flow of all incompressible Newtonian fluids is a unique function of the Reynolds number. This is a very important insight. Only two groups of variables need to be studied experimentally to obtain a relation that is universally valid for a wide class of fluids, geometries, and flow parameters. For a smooth pipe, Equation 6.73 reduces to CD = f(Re) only. In laminar flow, we calculate from Equation 6.54 that the pressure drop, Δp, is given as: Q8Hl ¥ Q ´ with L 2R and V 2 ¦ PR § PR 2 µ¶ 32HlV L2
$p
(6.75)
Q is the volumetric flow rate, and from the balance of forces (see Equation 6.72): T
$pL 8HV 4l L
(6.76)
For macroscopic laminar flow in long tubes, the friction factor, CD, thus correlates to the Reynolds number as: CD
¥ RVL ´ T H 16 f¦ 16 2 µ RVL R e § H ¶ RV 2
(6.77)
456
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
where CD is a constant (for Re < 2200), also called the Poiseuille number, that depends on the crosssectional shape but typically has a value of 16 for tube flow (see linear part of curve in Figure 6.32). Compare this with a Fanning friction factor for a sphere of 24 (see Figure 6.16). In case the Moody friction factor, CM, for pipe flow is plotted, the slope is 64 instead. The friction factor can be regarded as the ratio of the net imposed external force to the inertial force. Figure 6.32 represents Re versus friction factor CD for different pipe sizes, relative pipe roughness, densities, and a broad range of viscosities.1 Data from all pipe sizes and the entire viscosity range overlap and cover more than four decades in Re. At Reynolds numbers below 2200, the viscous shear effects are so large they balance the driving effect of the pressure, and a laminar, creeping, or Stokes flow condition results. For this type of flow, acceleration is negligible. Stokes flow is obtained either by a slow flow, that is, V is small, L is small, or η is large. It is in this regime that Equation 6.54, the HagenPoiseuille equation, is valid. At large enough Reynolds numbers, above 4000, a laminar flow becomes unstable and eventually turns turbulent. The region between 2100 and 4000 is a transition region, where transition depends on the size and frequency of disturbances inherent to the type of flow, the roughness of
k/L = 9.86 × 10−4 " = 1.98 × 10−3 " = 3.97 × 10−3 " = 8.34 × 10−3 " = 1.63 × 10−2 " = 3.34 × 10−2
CD
2×10−2
1×10−2 f=16/Re smo oth
2×10−3
4 6 8 2 103
4 68 2 104
Re
tube s
4 68 2 105
k L
FIGURE 6.33 Schematic of a pipe wall of uniform, regular roughness.
the boundaries, temperature, boundary flexibility, etc. For turbulent flow, the friction factor/Reynolds number dependence is weaker, but no simple theory exists and we must rely on experimental results. An empirical equation for turbulent flow is f = 0.079 Re–1/4.1,5 The onset of turbulent flow, as is obvious from Figure 6.32, is related to the relative roughness of the pipe wall. As illustrated in Figure 6.33, the relative roughness is represented by the dimensionless group k/L. The larger that ratio, the earlier turbulence starts. For micromachined tubes, one might expect a large k/L and turbulence to kick in quickly. But some simple calculations show that the Reynolds numbers are so low that turbulence is not likely to be observed in microsystems even with a large k/L. Boundary Layers The primary resistance to heat transfer and mixing by convection is controlled within a thin layer of stagnant fluid adjacent to the immersed body. In this hydrodynamic boundary layer, the flow velocity, V, varies from zero at the surface, that is, the noslip condition, to the value in the bulk of the fluid, that is, V∞. A quantity δ, the upper limit of the boundary layer, corresponds to the layer thickness when V has reached 0.99 V∞. For laminar flow around an object of length L, δ is given by: Dz
4 68 2 106
FIGURE 6.32 The Reynolds number, Re, is plotted versus friction factor, CD, for different pipe sizes, densities, and a broad range of viscosities. Data from all pipe sizes and the entire viscosity range overlap. Different relative roughness factors k/L (caused by sandroughened pipes) cause different onsets for turbulence. (From Denn, M. M. 1980. Process fluid mechanics. Englewood Cliffs, NJ: Prentice Hall. With permission.)
L VL N
z
L Re
(6.78)
As the Reynolds number gets larger, the boundary layer gets thinner. From Figure 6.34 we can deduce how Equation 6.78 comes about. From the continuity equation it follows that: uv uu uy ux
(6.79)
Fluidics
Equation 6.81 the last term remains, and we obtain Equation 6.78:
y (x)
x
V
457
u L
¥ u2u u2u ´ uu uu 1 u pd v N ¦ 2 2 µ or R ux ux uy uy ¶ § ux 2
¥L´ N L ¦§ D µ¶ VL ^ 1 or D ^ Re
FIGURE 6.34 Boundary layer dimensions.
The scaling of the term, ∂u/∂x, goes as V/L. If the length scale in the direction normal to the body is denoted as δ, i.e., the boundary layer thickness, and the normal velocity scale is denoted as U, it follows from the estimate ∂v/∂y ∼ U/δ that: U^
D V L
(6.80)
The streamwise equation of momentum balance, with p the pressure, and the scaling of each term annotated, is then given as:
Example 6.6 1. For a car being driven at 90 km/h (with ν = ±15 × 10 −6 ma St), the thickness of the hydrodynamic boundary layer is about 1 mm (see Table 6.3 for other examples). 2. In Volume II, Chapter 7, in the section on chemical vapor deposition (CVD), we calculated the average boundary layer thickness over a substrate on which a thin film is deposited, using the boundary layer model from Prandtl (Volume II, Equation 7.13) and obtained: D=
¥ u2 u u2 u ´ uu uu 1 up v N¦ 2 2 µ u uy ¶ ux uy R ux § ux V2 , L
V2 , L
V V2 V , N 2, N 2 L L D
multiply by L /V 2 to obtain: 2
1, 1, 1,
N ¥ L´ N ,¦ µ VL § D ¶ VL
1, 1, 1,
1 ¥ L´ 1 ,¦ µ Re § D ¶ Re
or also,
2
(6.81)
2L
When a fluid at one temperature flows along a solid surface that is at another temperature, a thermal boundary layer develops in addition to the hydrodynamic boundary layer. The thickness of the thermal boundary of a solid object in a fluid medium depends on the velocity of the fluid over the solid surface and the properties of the fluid medium. The equation to estimate the thermal boundary layer thickness, δ T, is given by: DT z
The case of interest here is that of a large Reynolds number (but not so large as to cause turbulence), so that 1/Re 7λ. Consequently, the boundary between the microscale and macroscale
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
regimes equals L = 7λ for the conduction across a layer, where L is the layer thickness and λ the mean free path of the dominant carrier of heat. Given the dimensions of a phonon at least 10 times smaller than λ of a gas at atmospheric pressure, we might not observe deviations from the NavierStokes equations in liquids until the dimensions of the containing vessels are in the 100Å range. Maps for heat transfer regimes in microstructures, immediately showing whether a certain heat transport in a given device can be analyzed with macroscale theory, have been developed.17 Slip in Liquids Deviations from the NavierStokes equations in liquid are more difficult to demonstrate than in a gas. Liquids do not have a welladvanced molecularbased theory as dilute gases; for example, there is no Knudsen number for liquids, and the concept of a mean free path in a liquid is very different than for a gas. Gravesen et al.13 in 1993 reviewed some of the literature describing deviations from NavierStokes equations in liquid flow in narrow channels but could not find enough consistency in the data to conclude that there was a breakdown of the macrotheory. More clarity has emerged since 1993. In controlled experiments, generally with dimensions of microns or smaller, apparent violations of the noslip boundary condition clearly have been demonstrated in liquids. We usually assume that viscosity in liquids is independent of the dimensions of the flow channel. However, experiments by Harley et al.18 suggest that in microchannels liquid flow takes on values as much as an order of magnitude greater than that expected from a constant viscosity. Pfahler et al.12 similarly measured a flow significantly higher than expected from macrotheory when using isopropanol and silicone oil. Israelachvili19 showed that the apparent viscosity of a liquid is the same as that in the bulk once the film is thicker than a dozen molecular layers (∼5 nm); below that thickness the viscosity grows by several orders of magnitude. Tretheway et al.,20 using a 30 × 300μm channel made hydrophobic with a 2.3nmthick monolayer of octadecyltrichlorosilane, measured fluid slip velocities within 450 nm of the wall of about 10%
of that in the center instead of zero. This slip condition has the effect of increasing the total volume flow. In the case of a hydrophilic surface, velocity profiles remained consistent with Stokes flow and the wellaccepted noslip boundary (see Figure 6.38). Slip of liquids was also measured with hexadecane flowing over an atomically smooth surface, such as mica, that again was made nonwettable by deposition of a hydrophobic monolayer.21 From the above, we conclude that slip causes a “shift” in the velocity profile. It also has been established that slip increases with the contact angle,22 decreases with increasing surface roughness,22 and increases with viscosity and driving rate.23 In flow channels approaching molecular diameters, “molecular” effects turn yet more dramatic. When the channel is less than 10 molecular diameters, of the order of a few nanometers, the fluid loses its liquidlike behavior and assumes some solidlike characteristics.24 The structure of the molecules changes from a random order to a discrete number of ordered layers, with an “apparent” viscosity of the fluid 105 times the “regular” viscosity. The molecular time scale for molecules in these nanotubes slows down by a factor of 1010.25 In Figure 6.39, the friction force between two parallel plates, separated by a few Velocity proﬁles 25.0
Position from wall (microns)
462
20.0
15.0
10.0
5.0
0.0 0.0
0.2
0.4
0.6
0.8
1.0
Streamwise velocity (normalized)
FIGURE 6.38 Measurement of slip length. Square symbols: hydrophilic coating (L s = 0), triangle symbols: hydrophobic coating (L s = ∼1 μm). The velocity at 450 nm from the wall was measured at 10% from that in the middle of the flow (instead of 0). (Tretheway, D. C., and C. D. Meinhart. 2002. Apparent fluid slip at hydrophobic microchannel walls. Phys Fluids 14: L9.)
Fluidics
n=1
40
n=2
sit i
10
on
20 n=3 0 0 1
Tra ns
itio
n
30
n=2
Tr an
Frictional Force (mN)
50
2
Time (minutes)
FIGURE 6.39 Friction forces between two parallel plates. (Ho, C. M. 2001. 14th IEEE International Conference MEMS, Interlaken, Switzerland, 375.)
molecular layers of OMCTS (octamethylcyclotetrasiloxane), sliding with respect to each other while the distance between them decreases (horizontal axis), is shown. Two very striking features are apparent. First, the frictional forces increase in a stepwise fashion as the distance between the plates is reduced and settles on a stable value corresponding to an integer number of molecular layers (1, 2, or 3). Second, a sawtooth behavior is observed, corresponding to a stickstick motion of the plates when the molecular layers are rearranging themselves while moving with respect to each other. When working with macromolecules such as DNA and proteins in nanochannels, effects as described here are to be expected. Instead of continuum theory, molecular dynamics methods are used to study interfaces at the molecular level. In molecular dynamics one integrates Newton’s equations of motion for each individual particle. A commonly used force between the interacting molecules is the LennardJones force introduced in Chapter 7 (Equation 7.22).
463
is termed the interfacial tension (in units of N/m or also J/m2), whereas for interfaces involving solids, it is called “surface energy.” We start by illustrating the surface forces at the liquid/gas interface, i.e., surface tension. Next we study the solid/liquid interface to elucidate beading of droplets and capillary action.
Surface Tension Many of the properties of a liquid, including surface tension, capillary action, and beading, are caused by cohesion and/or adhesion of molecules. In liquids, the rearrangement after creating a new interface is very fast, and the surface tension is an equilibrium value. Liquids and gases are separated by a meniscus and differ only in density, not structure. Molecules at the surface of a liquid experience forces around and below, whereas molecules in the middle are attracted from all sides, so the net attraction on molecules at the top is downward (Figure 6.40). Increasing the surface area results in more molecules that are exposed and a higher overall energy, so the surface area tends toward the smallest possible area to reduce the overall energy of the system. A liquid thus arranges itself to have less surface area. Water forms spherical drops because a sphere exhibits less surface to volume. The energy required to break through the surface of a substance or to spread a drop of the substance out into a film is the surface tension. Fluids behave as though they have a surface composed of an elastic skin that is always in tension. Surface tension, with reference to Figure 6.41, is the amount of energy Surface
Interior
Forces at Interfaces Introduction Molecules condense when attractive intermolecular bond energies are comparable with or greater than their thermal (i.e., kinetic) energy. These condensed materials have a surface: a transition region between condensed phase [S(olid) or L(iquid)] and a gas phase. An interface is a region between two condensed phases. At interfaces, atoms and molecules possess energies and reactivities significantly different from those of the same species in the bulk. That imbalance leads to surface free energy. The imbalance of forces at a gas/liquid interface usually
FIGURE 6.40 The molecular origin of surface tension. Molecules at the surface of the liquid experience forces around and below, whereas molecules in the middle are attracted from all sides, so the net attraction on molecules at the top is downward.
464
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
required to stretch or increase the surface area of a liquid by a unit area. The force exerted by a planar film supported on a rectangular frame with one movable bar of length l, as shown in Figure 6.41, is given by: Fs = 2Gl
(6.88)
The factor of two is introduced because the liquid film has two surfaces. The work required to create new surface area is then: W 2 G ld and 2G
dW dA
(6.89)
An interfacial energy γ is associated with any interface between two phases (J m−2) (also called a surface tension: Nm−1). An increase in area increases the system’s free energy, which is not thermodynamically favorable. Water has the highest surface tension of all common liquids.
Drops and Bubbles
Fin Fout Fsurface 0 pin Pr 2 pout Pr 2 G 2Pr 0 (pin pout )Pr 2 G 2Pr 2G 2G or also $p r r
(6.90)
In this example there is only one liquid/gas surface. For a soap bubble, with two liquid/gas surfaces, the force will be twice as great. Atoms of liquid on the surface of a small droplet are held less tightly compared with atoms on a flat 2A Fs l
Surface tension force Pin 2r
FIGURE 6.42 Pressure difference across a curved surface.
liquid surface. High curvature effectively reduces the coordination number of the surface atoms, making them easier to evaporate. This is manifested as an increase in the vapor pressure p of a liquid droplet compared with that of a bulk liquid p0 and is described in the Kelvin equation. In the case of a positive curvature, the liquid in drops has a higher vapor pressure than in the bulk. In the case of negative curvature, it has a lower vapor pressure than in the bulk (e.g., liquid in pores). The Kelvin equation for a droplet is given as: ln
The forces on a liquid sphere (say, a drop of water) of radius r can be calculated as follows. Balance of forces in Figure 6.42 requires that ¤ F 0. So we can write:
pin pout
Pout
Fs
p 2G V p0 R Tr
(6.91)
In this equation: r = the drop radius γ = the surface tension V = the molar volume of the liquid R = the gas constant T = the absolute temperature From Equation 6.91 the vapor pressure p relative to the bulk p0 can be calculated as: ¥ 2G V ´ p p0 exp ¦ µ § R Tr ¶
(6.92)
Evaporation of a droplet of diameter d at time t is given as: d 2 d02 Bt
(6.93)
where d0 is the initial diameter, and β is a constant independent of drop size. The time it takes for the drop to disappear is then:
Fw
t
d02 B
(6.94)
d
FIGURE 6.41 The work involved in expanding a liquid film by 2A (=2dl).
The latter scales as l2, and clearly miniaturization favors faster evaporation. Fast evaporation of small
Fluidics
¤G 0
G—Gas L—Liquid S—Solid
Contact angle
LG
SG
G
c S
465
LS
L
LG cos C = C
FIGURE 6.43 The horizontal force balance between these three interfacial tensions represents Young’s equation.
liquid droplets often poses a considerable problem in MEMS. A droplet ejected from a small nozzle might evaporate before it reaches the substrate, which makes storing small amounts of chemicals on a liquid platform very cumbersome for the same reason.
Wetting and Contact Angle–Beading on Solid Surfaces We now introduce a solid surface in a liquid and define adhesion forces and wetting of a solid surface. From the previous section we know that increasing the surface area of any liquid requires work, and this effort per unit surface area is the liquid’s surface tension (with a unit of N/m and symbol γ). When liquid of a sessile drop comes in contact with both a solid and a gas, as shown in Figure 6.43, a contact angle θc of between 0 and 180° is set up. Three interfacial tensions come into play: γSG , the solid/gas interface tension; γSL , the solid/liquid interface tension; and γLG , the liquid/ gas interface tension. The horizontal force balance between these three interfacial tensions represents Young’s equation:
G LS G LG cos Qc G SG 0 G LS G LG 2Pr cos Qc G SG 0
(6.95)
G LS G LG G LG cos Qc 0 2Pr
G LS G LG G LG cos Qc G c 2Pr where θc is the contact angle. The critical surface tension γc is an intrinsic characteristic of the surface. Liquids with γ < γc completely wet the surface (θ = 0º). Liquids with γ > 90º are said to not wet the surface (γLS > γSG). The surface of plant leafs, especially of the lotus flower (Nelumbo nucifera), the symbol of purity in some Asian religions, can show extreme hydrophobicity or superhydrophobicity to water. This makes the deposition of water drops on their surface almost impossible (large water contact angles θ > 150°) (Figure 6.44). Such hydrophobic surfaces also show a remarkable selfcleaning effect. Even after emerging from mud, the lotus leaves do not retain dirt when they unfold. The prospect of selfcleaning surfaces is obviously of significant commercial interest. Two botanists, Barthlott and Neinhuis, from the University of Bonn, discovered the reason for this selfcleansing effect.27 The general opinion used to be that the smoother a surface, the less dirt and water adhere to it. However, when inspected with an SEM, lotus leaves show a combination of nano and microstructures that make for a rough surface at the micro and nanoscale. The explanation for the resulting effect lies in two physical characteristics of the
FIGURE 6.44 Extreme hydrophobicity of lotus plant leafs. The far right photo represents a commercial application of the Lotus Effect; i.e., a BASF aerosol spray for paper, wood, leather, etc., makes those materials superhydrophobic.
466
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
lotus leaf, i.e., the properties of these microstructures repel water, and the nanostructures found on top of the microstructures are made of waxy materials that are poorly wettable. The combination of the chemistry, the nanostructures, and the nonadherence of dirt and water to the microrough surface is what Barthlott and Neinhuis named the Lotus Effect. The roughness of a surface improves the wettability for hydrophilic surfaces (θ < 90°). A drop on such a surface will appear to sink into the hydrophilic surface. For hydrophobic surfaces (θ > 90°) the wettability decreases as it gets energetically too expensive to wet a rough hydrophobic surface. The result is an increased waterrepellency. Energetically the best configuration for the drop is then on top of the roughness spikes like “a fakir on a bed of nails” (Figure 6.45). A droplet on an inclined superhydrophobic surface rolls off instead of sliding. When the droplet rolls over a contamination, the particle is picked up from the surface, and the energy of absorption into the rolling droplet is higher than the surface stiction force between the dirt particle and the surface. Usually the force needed to remove a particle is very low because of the minimized contact area between the particle and the surface. As a result, the droplet cleans the leaf by rolling off the surface (Figure 6.46). See also Volume III, Chapter 3, page 144 “Superhydrophobicity and the Lotus Effect”.
Capillary Action The beading, illustrated in Figure 6.44, occurs when a polar substance is placed on a nonpolar surface and cohesive forces compete with adhesive forces. There is also a competition between adhesive and cohesive forces in capillary action. If adhesive forces are greater than cohesive forces, the liquid surface is attracted to
FIGURE 6.46 Selfcleaning behavior of a superhydrophobic surface by droplets rolling off instead of sliding off. (From http://lotusshower.isunet.edu/the_lotus_effect.htm.)
its container more than the bulk molecules. Therefore, the meniscus is Ushaped (e.g., water in glass) (Figure 6.47Aa left). If cohesive forces are greater than adhesive forces, the meniscus is curved downward (Figure 6.47Aa right). In capillary action, liquids rise spontaneously in a narrow tube (Figure 6.47Ab). We are all familiar with water being sucked up by a hydrophilic capillary (e.g., in a glass capillary) as a result of positive capillarity. Less evident from daily experience is that water may have to be pushed up in the case of a hydrophobic capillary as a result of negative capillarity (e.g., in a Teflon tube). Figure 6.47B illustrates the two types of capillarity schematically. In the positive capillarity case, liquid in a capillary rises as to seek a lower interfacial energy. The liquid will rise until it lifts a column of liquid balancing the energy reduction gained by rising. The energy reduction by rising over a distance l in the capillary is given by (γSG – γSL) 2πrl. In this expression, r is the capillary radius, and the work performed in raising the liquid column is given by Δpπr2l, with Δ p the pressure difference between the top and bottom of the raised column. By equating these two energies, we can deduce the pressure drop across a liquid/gas interface in a small capillary as: $p
(a)
(b)
FIGURE 6.45 (a) A droplet on a hydrophilic rough surface seems to sink into the gaps. (b) A droplet on a rough hydrophobic surface sitting on the spikes. (From http:// lotusshower.isunet.edu/the_lotus_effect.htm.)
(G SG G SL ) 2S L cos Qc r r
(6.96)
where it has been assumed, as is generally the case, that γLG = σL (the surface tension of the liquid). The pressure produced by wetting, calculated from this expression for typical values of the gas/liquid surface tension (γLG = σL = 0.073 N/m at room temperature and 0.058 N/m at 100°C) and a capillary radius of 10 μm, is in the range of 0.01 MPa. This is roughly the same as achieved with piezoelectric pumps, which are much larger in size.
Fluidics
Capillary forces scale with l1, and as we will see in Volume III, Chapter 7 on scaling, the smaller the exponent of l, which is 1 in this case, the more favorable the scaling. The Kelvin equation for a liquid in a cylinder (say, in a pore of a solid) as shown in Figure 6.47 is, in analogy with Equation 6.91 for a droplet, given as: ln
p G V p0 R Tr
(6.97)
In this equation: r = the cylinder radius γ = the surface tension V = the molar volume of the liquid R = the gas constant T = the absolute temperature
2G f r
(6.98)
Mixing, Stirring, and Diffusion in Low Reynolds Number Fluids Stokes or low Reynolds number flow, we saw above, occurs when Re >b
(b)
1 ns 1 nm Laminar chaotic ﬂow
FIGURE 6.51 The concept of chaotic advection. (a) Two flows come together in a small conduit and only limited mixing takes place. (b) Laminar chaotic advection reduces the time it takes to mix in a microchamber.
Inlet 2
Inlet 1
FIGURE 6.52 Mixer configuration for chaotic advection in the microdomain. Two fluids entering the inlet ports laminate at the first horizontal junction, producing two sidebyside fluid streams. Successive vertical separation and horizontal reuniting of fluid streams increase the number of laminates with each stage and, thus, the contact area between the two fluids.
compared with 3 × 10−6 cm2/s for fluorescein), and one might need to look for alternatives for inducing fast mixing because pure diffusional mixing is now too slow. This is an important, current technological challenge, for example, in the design and manufacture of fast DNA and protein arrays for molecular diagnostics: assays in arrays need to be married with a small, simple fluidic manifold, whereas reaction rates in the microfluidic chambers holding the arrays must remain high, despite low Reynolds numbers and high Péclet numbers.
Red blood cell
Viral DNA
Ribosome
Glucose
1 μm Diffusion length
1 mm
FIGURE 6.53 Diffusion times and lengths in the lab and on a chip.
where D is the diffusion coefficient, x the distance over which a species has diffused, and t is the average time between collisions. From this equation, the diffusional mixing time is of the order x2/D. Miniaturization, as illustrated in Figures 6.53, can thus be expected to lead to smaller diffusive mixing times (scales with l2). To help things along, in passive mixer designs the interfacial area is increased to reduce diffusion length. This may be accomplished using sinusoidal, squarewave, or zigzag channels. As illustrated in Figure 6.54, the smaller the distance between regions of different concentration, the larger the diffusive flux. Multilaminated flow downscales the diffusion length. Mixing as illustrated in Figure 6.55 can also be improved on by using a fractal approach, a design akin to how nature uses passive mixing (Figure 6.55). In nature, only the smallest animals rely on diffusion for transport; animals made up of more than a few cells cannot rely on diffusion anymore to move materials within themselves. They augment transport with hearts, blood vessels, pumped lungs, digestive tubes, etc. These distribution networks (a) Not fully mixed yet
a
b
a>>b
(b) Fully mixed already
Passive Micromixers Several passive micromixer designs aim at reducing the diffusion path length. We start this analysis from the EinsteinSmoluchowski equation: x 2 2Dt
(6.100)
FIGURE 6.54 (a) Two flows come together in a small conduit and only limited mixing takes place. (b) The smaller the distance between regions of different concentration, the larger the diffusive flux. Multilaminated flow downscales the diffusion length.
470
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
T^
w2 D
(6.101)
The necessary mixing length of the mixer is estimated by assuming that the two fluids at a velocity of Q/wb, with Q the total flux, require a length Lm to achieve mixing, or: Lm ^
(a)
n=0
1
2
3
4 ....N
(b)
FIGURE 6.55 (a) The branching structures found in mammalian circulatory and respiratory systems have, through natural selection, evolved over many millennia to their current state of minimizing the cost function associated with the amount of biological work required to operate and maintain the system. (b) Biomimetic microfluidic device used for studying concentration gradients in a network of branching serpentines, in which three dyes are injected at the top before combining in a single channel at the bottom. (Whitesides, G. M. 2003. The “right” size in nanobiotechnology. Nat Biotech 21:1161–65.)
typically constitute fractals. Fractals are an optimal geometry for minimizing the work lost as a result of the transfer network while maximizing the effective surface area (see Volume III, Chapter 9). In Figure 6.56 we demonstrate a Tshaped diffuser/ mixer, where two fluids A and B enter a Tshaped intersection. Beyond the T, the width of the collection channel is reduced. In the narrowed rectangular crosssection of the fluidic structure, with width w and height b, the diffusive mixing time is proportional to:
Qw bD
(6.102)
At a fixed height b, narrowing the channel width w can reduce the length Lm to achieve mixing in a shorter time. Two adjoining laminar flows A and B in a Tdiffuser/mixer may be used as a filter as we illustrate in Figure 6.57. As the two parallel laminar flows contact, diffusion may extract one compound from one stream into the other. This way, components with higher diffusivity can be extracted from a sample stream (say, A) into a second diluent flow (say, B). This simple system does not require a membrane and is somewhat akin to field flow fractionation. Example applications include competitive immunoassays, determination of diffusion coefficients, and reaction kinetics parameters. Diffusive extraction is also the underlying principle of the Hfilter, illustrated in Figure 6.58. This continuous filter consists of two Tdiffuser/mixers: one for mixing and one for separation. In the Hfilter a proper design of a microfluidic channel allows for controlled extraction of analytes with high diffusion coefficients from components of the sample with lower diffusion A
B
Fluid A Mixing section
z
w b 1
w Fluid B
FIGURE 6.56 Tshaped diffuser/mixer, forcing fluids to mix by diffusion in a constriction of the microchannel. The length of the constriction is l, the width is w, and the height is b (unchanged from the wide channel section).
FIGURE 6.57 Tdiffuser/mixer used as a filter. (Ismagilov, R. F., A. D. Stroock, P. J. A. Kenis, and G. Whitesides. 2000. Experimental and theoretical scaling laws for transverse diffusive broadening in twophase laminar flows in microchannels. Appl Phys Lett 76:2376–78.)
Fluidics
471
w
Solution D1
t> D2τ. Typical values are λ = 10 μm, w = 40 μm, and t = 5 s. Applications of the Hfilter include cell lysis, nonmotile sperm separation, extracting a wide range of analytes from the mucins in saliva, etc. For a final example of a passive mixer in low Reynolds number fluids, we return to chaotic advection mixing. A first example of this type of mixing was illustrated in Figure 6.52. As a second example we use the herringbone micromixer developed by Stroock et al. (2002),34 shown in Figure 6.60. In this mixing approach, staggered herringbone microgrooves in the bottom of a flow channel in the
pw (a)
m
h
c u
uc
h d cu
w
y = 3 cm
z
FIGURE 6.59 Design parameters of the Hfilter. The fixed residence time in the transverse channel provides a “diffusion window” for the fastest components in one stream to diffuse to the other parallel stream and thus be separated.
z
h h
100 m
(c)
3 cm 200 m
Cycles 15: Cycle 15:
x
2/q 0 cycles:
1/2 cycle:
z
1 cycle:
y = 3 cm
y (b)
m
x
100 m
FIGURE 6.60 Micromixing by generating chaotic advection: the staggered herringbone mixer. By patterning grooves in the bottom of a microchannel, secondary flows are promoted that stretch and fold fluid elements, increasing areas with concentration gradients and so increase diffusive mass transport and mixing. In (a) no grooves are patterned, and parallelflowing separated fluids undergo almost no mixing. By patterning grooves in several configurations, different secondary flows are promoted with smaller (b) or larger (c) mixing effects. (Stroock, A. D., S. K. W. Dertinger, A. Ajdari, I. Mezi, H. A. Stone, and G. M. Whitesides. 2002. Chaotic mixer for microchannels. Science 295:647–651.)
472
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology Δx0
Δx
Stretch
l0
Δx
Fold
Diffuse
Stir
n=0 1 fold
n=1 2 folds
FIGURE 6.61 Mixing and stirring in low Reynolds number fluids is like kneading dough.
ydirection promote secondary rotating velocities (vx, vz). The underlying process for this type of efficient mixing, even in very viscous flow, is depicted in Figure 6.61 and is called the “baker’s transformation. The main property of this transformation is that fluid pair elements will separate exponentially in “chaotic advection.” As illustrated in Figure 6.62, the width of the fluid folds (Δx) decreases exponentially, and the length of the interface (l) grows exponentially: $ x(n) $ x 0 (2) n and (6.103)
l(n) l 0 (2)n The mixing length Lm was estimated as34:
(6.104)
L m z w log Pe
where w is the channel width, and Pe, the Péclet number, is calculated from the width and average flow velocity. This estimation, confirmed by experiments, leads to mixing lengths several tens of times larger than the width w for Péclet numbers on the order of 105. Active Mixers One also can use active perturbation to create timedependent flows so that chaotic advection can occur. Different sources can be employed: pressure,
Stretch
Fold
n=2 4 folds
FIGURE 6.62 The baker transformation. Chaotic advection.
ultrasonic/piezoelectric, electrohydrodynamic, electroosmosis, and mechanical stirring. The mixing in the narrow section of the Tdiffuser/ mixer in Figure 6.56, for example, can be dramatically improved through hydrodynamic focusing, the technique used in cell and particle flow sorting. Two side flows “squeeze” or “hydrodynamically focus” an inlet flow. By using hydrodynamic focusing, the diameter of a central liquid jet can be reduced to just a few nanometers, which allows for mixing within this kind of beam in the tens of microseconds. This work, by Knight et al.,35 is illustrated in Figure 6.63. The diameter of the jet (Wf) in the collection channel (Wc) is controlled by the ratio of the flow rates coming out of the three channels that bring the fluids together at the intersection. Knight et al. showed that with flow ratios of >100, Wf can be made to be around 30 nm. Applications of hydrodynamic focusbased mixing include the study of fast reaction kinetics (like protein folding), which depend on fast mixing of reactants.
Side wc wf
Inlet
10 μm
10 μm Side
FIGURE 6.63 Geometry of a hydrodynamic focusing structure allowing for the reduction of the size of the jet and thereby enabling effective mixing transverse to the jet. (Knight, J. B., A. Vishwanath, J. P. Brody, and R. H. Austin. 1998. Hydrodynamic focusing on a silicon chip: mixing nanoliters in microseconds. Phys Rev Lett 80:3863–66.)
Fluidics
FIGURE 6.64 Principle of PPy/Au actuator. Mixing is achieved by activation of PPybased actuators in microchannels.
Another active mixing approach pursued by the Madou group at the University of California, Irvine, involves the use of gold/polypyrrole actuators. Small rectangular gold/polypyrrole bilayer structures make for little flaps that can be made to move by biasing the polypyrrole with respect to a counter electrode in the same solution (see Figure 6.64). These actuators have been used to promote flows around a sensor in close proximity to the flapping bilayers. In doing so, convective mass transport is achieved, and the response in the sensor is increased over diffusive limits. Arrays of these mixing flaps
473
have been fabricated as well with individual actuators ranging in dimensions from several millimeters to a few micros (see Casadevall i Solvas, X. 2009. Active micromixing and invivo protection of sensors with gold/polypyrrole actuators. PhD diss., University of California, Irvine, Irvine, CA; and Casadevall i Solvas, X., R. A. Lambert, L. Kulinsky, R. H. Rangel, and M. J. Madou. 2009. Au/PPy actuators for active micromixing and mass transport enhancement. Micro and Nanosystems 1:2–11). The idea of the flexible flaps presented above is based on biomimetics. In 1977 Purcell, discussing swimming of microorganisms in fluids at very low Reynolds numbers,36 presented the physical requirements that would allow microsystems to move (or propel fluids) in the microdomain (Figure 6.65). A simple singlehinged, rigid system (Figure 6.65a) would permanently move back and forth from its initial to its final position without accomplishing any real progress. To circumvent this limitation, multiplehinged systems (Figure 6.65b) and flexible propelling structures (Figure 6.65c) can be used. Both configurations can be implemented easily with
!
!
! !
!
"$%&#
"#
FIGURE 6.65 Swimming of microorganisms in fluids at very low Reynolds numbers. A simple singlehinged, rigid system (a) would permanently move back and forth from its initial to its final position without accomplishing any real progress. To circumvent this limitation, multiplehinged systems (b) and flexible propelling structures (c) can be used. (Purcell, E. M. 1977. Life at low Reynolds number. Am J Phys 45:3–11.)
474
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
the flexible gold/polypyrrole actuators shown in Figure 6.64. In microvolumes of fluid, because of the flexible nature of these actuators and the possibility to actuate several of them simultaneously, these devices could be used to promote flows of sufficient complexity for chaotic advection to develop, and so enhance mixing in a targeted, isolated fashion, minimizing device and reagent volumes. For a good review and an excellent comparison of active and passive micromixing, see Nguyen and Zhigang.37 The summarizing comparison between active and passive mixing in Figure 6.66 is borrowed from this review.
Damköhler Numbers
Chemical Reactions in Microchambers—Microreactors Introduction The ultimate objective of passive and active micromixers in many instances is to speed up a chemical reaction by enhancing the mass transport to reaction sites in a chemical microreactor. As pointed
(A)
Passive micromixing
(a)
(b)
out earlier, this finds a key application in the development of faster DNA and protein arrays for molecular diagnostics. These array assays need to be accommodated in a small reaction chamber, whereas reaction rates must remain high, despite low Reynolds numbers and high Péclet numbers. Because of these chemical reactions, the earlier described equations for fluid motion now need to be expanded with terms that take into account the generation (source) or consumption (sink) of reagents dissolved in the fluid. The proper design of chemical microreactors leads to faster and more sensitive assays.
(c)
Diffusive transport is captured by Fick’s second law (see Equation 4.21 in Chapter 4), stating that the flux gradient ¨ DF(x ,t) · is proportional to the change of ©ª Dx ¸¹ the concentration with time. For a diffusion coefficient D, which is independent of position, this equation can be written for 3D using the ∇ operator as:
(B)
(d)
Active micromixing
(a)
(b) GND
(c) Mixing chamber (e)
(f )
(g)
(i)
(j)
(k)
(l)
(m)
(h)
(e)
(n)
(d) Mixing chamber
GND
(f ) GND
(g)
FIGURE 6.66 Comparing passive (A) and active (B) micromixing. Passive micromixers: modified Tesla structure (A) (a), Cshape (A) (b), Lshape (A) (c), connected outofplane Lshapes (A) (d), twisted microchannel (A) (e), other designs of twisted channel (A) (f–h), slanted ribs (A) (i), slanted grooves (A) (j), staggeredherringbone grooves (A) (k), and patterns for surface modification in a micromixer with electrokinetic flows (A) (l–n). Active micromixers: serial segmentation (B) (a), pressure disturbance along the mixing channel (B) (b), integrated microstirrer in the mixing channel (B) (c), electrohydrodynamic disturbance (B) (d), dielectrophoretic disturbance (B) (e), electrokinetic disturbance in the mixing chamber (B) (f), and electrokinetic disturbance in the mixing channel (B) (g). (Nguyen, N. T., and W. Zhigang. 2005. Micromixers—a review. J Micromech Microeng 15:R1–R16.)
Fluidics
uC D 2 C ut
(6.105)
For steadystate conditions the concentrations are constant in time, and there is no change in the mass stored with time, or ∇ 2C = 0 (Laplace’s equation). If, besides diffusion, we also consider convective or advective transport (mass flux due to the velocity V of the flow), we need to add a term: uC D 2C CV ut
(6.106)
Expanding the advective term we obtain: uC D 2C VC CV ut
(6.107)
For transport in a steadystate flow field ∇V = 0, so that: uC D 2C VC ut
(6.108)
uC D 2C V C r ( kC) ut
and their definition varies according to the system under consideration. A global definition for the Damköhler number is: Da
(6.109)
where r is the net mass produced or consumed per unit volume per unit time (moles/L 3t). For each species in the system an Equation 6.109 is required. The general form of the r term is r = kC, that is, r is the product of concentration and a reaction rate coefficient, k. Depending on the type of reaction, r takes on different forms; in a first order–type reaction (e.g., encountered in radioactive decay), r = −λC, where λ is a decay constant. In the case of second order kinetics, with reagents A and B, r = −kC ACB. One can distinguish between two extreme cases depending on the Damköhler numbers. The Damköhler numbers (Da) are dimensionless numbers used to relate chemical reaction time scales to other phenomena occurring in a system. They are named after the German chemist Gerhard Damköhler, 1908–1944. There are several Damköhler numbers,
TC TM
(6.110)
where τC is the characteristic time of the chemical reaction, and τM is the mixing time that can be controlled by hydrodynamics or by diffusion. So a small Damköhler number refers to a very slow chemical reaction compared to all other processes. Introducing a dimensionless concentration C* (dividing C by an arbitrary concentration Cr); a dimensionless time t* (dividing t by an arbitrary time tr); and dimensionless lengths x*, y*, and z* (by dividing by the characteristic length L), we nondimensionalize Equation 6.109 as: ¨ L2 · uC* ¨ kL2 · ¨ VL · 2 * C* C
© ¸ © ¸ C* ©ª D ¸¹ ª D ¹ ª Dt r ¹ ut * Fourier
In case the velocity of the fluid is zero, we recover the diffusion equation. Finally, when reactions take place, we add a term for production (source) or removal (sink) of chemicals. This results in:
475
or Fo
Péclet
Damköhler
uC* 2C * PeC* PeDa IC * ut*
where Da I
kL V
and also Fo
uC* 2C* Pe$C* Da IIC * ut*
kL2 where Da II D
(6.111)
The Fourier number Fo (L2/Dtr) is a dimensionless quantity that can be used to characterize a diffusion length for a particular time. For example, if D = 10−9 m2/s and t r = 1 year, then the diffusion length is about 0.18 m. The first Damköhler number (DaI = kL/V) measures the tendency for reaction versus advective transport. The second Damköhler number (DaII = kL 2/D) measures the tendency of reaction relative to the tendency for diffusive transport. With a small DaI or DaII, convection and/or diffusion is much faster than chemical reaction, and the concentration in the reactor is uniform. The system is reaction ratecontrolled, and convection and/or diffusion have no influence. With a large DaII, the chemical reaction is very fast so that the concentration, say
476
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
on an electrode, might fall to zero, and the system is transportlimited. Since the Biot number (see above) will tend to decrease for microdevices, it is expected that microchemical reactors will have nearly uniform temperatures. Thus, the wall effects will be very important from the point of view of keeping a hightemperature reaction going. The tendency will therefore be for the presence of small Damköhler numbers (weak reaction) due to heat losses through the reactor walls that reduce the reaction rate and consequently increase the chemical time, while the small dimensions reduce the diffusion time. For a general chemical reaction A → B of nth order, the Damköhler number is defined as: 1 t Da kC n 0
(6.112)
where k = kinetics reaction rate constant C0 = initial concentration n = reaction order t = time
Electrochemical Reactions Here we set up an expression for the current on an electrochemical sensor with transport of electroactive species to and from the electrode by diffusion, migration, and convection. From Fick’s first law (Equation 4.20) we derive for the flux or current resulting from electroactive species i: J i (x ) Di
DC i ( x ) DF
z i Mi FC i Ci V( x) D(x ) Dx
Diffusion
Migration
molecules to a positively charged electrode, the solution must have a low conductivity as otherwise the field does not penetrate the liquid (see Chapter 7). As we learn in Chapter 7, to obtain reliable analytical data on amperometric electrochemical sensors, the migration term needs to be minimized in favor of the diffusion and convection terms. This, we will learn, is accomplished by the addition of an indifferent electrolyte suppressing the migration of the electroactive species of interest. In Table 6.5 we summarize the important transport phenomena determining the response of an electrochemical sensor. Electrochemicals are studied in detail in Chapter 7 where they are also compared with optical sensors.
Convection (6.113)
where Ji = flux of species i in mol/cm2 s zi = charge number of species i in eq/mol μi = mobility of species i in cm2mol/Js Ci = concentration of species i in mol/cm3 ϕ = electrostatic potential in V F = the Faraday constant Di = diffusion coefficient of species i in cm2/s V = fluid velocity in cm/s In this expression for an electrochemical reaction, the new term we consider is migration transport. For migration of species, say negatively charged DNA
Fluid Propulsion Introduction Many options present themselves for fluid propulsion, including mechanical means, dc and ac electrokinetics, acoustic pumping, electrowetting, centrifugal, electrohydrodynamic and magnetohydrodynamic, etc. Acoustic, electrohydrodynamic, and magnetohydrodynamic pumping techniques are reviewed in Volume III, Chapter 8 on actuators, and in Volume III, Chapter 1 we compare and summarize the most important new pumping methods and their MEMS integration (see Volume III, Table 1.8). In the current section we detail the theory behind dc and ac electrokinetics, electrowetting, and centrifugal fluidics.
Electrokinetic Effects—Direct Current (DC) Introduction to Electrophoresis and ElectroOsmosis An electrical field works on both charged particles in a fluid and on the fluid itself when the fluid is placed in a narrow capillary with electrically charged walls. The force on the particles in the fluid leads to electrophoresis; the force on the fluid in a narrow column leads to electroosmosis. Both phenomena are of great importance in miniaturization science: electrophoresis for separation of compounds and electroosmosis for movement of fluids. Mathematically, it does not make a difference whether the fluid passes a charged wall or a charged particle moves through a fluid.
Fluidics
477
TABLE 6.5 Transport Phenomena on an Electrochemical Sensor Transport
Migration
Response to Acts on Flux density (from Equation 6.113) J=
Diffusion
Potential gradient Ions only
zFMC
uF ux
mobility
Concentration gradient All solutes uC
D ux
Convection Pressure gradient Solutes + solvent CV
diffusivity
Relationship between μ and D
Einstein derived a simple relation between D and μ as: D = μRT
Combining migration with diffusion flux
¨ uC zF uF · J D © C ª ux RT ux ¸¹ (NernstPlanck flux equation using the Einstein relation between D and μ.)
Conservation law
uC uJ ut ux for planar transport uC uJ 2J ut ur r for spherical transport
Electrophoresis Electrophoresis is the migration of ions in a separation medium under the influence of an electric field. An ion with charge q (Coulombs) in an electric field E (Vm−1) feels an acceleration force qE (Newtons). A steadystate speed is reached when the accelerating force (qE) equals the frictional force generated by the separation medium, or: qE f VE
(6.114)
where f = the friction coefficient or friction factor V E = the electrophoretic steadystate speed of the ion The expression for the electrophoresis velocity VE of a charged species in a separation medium can then be written as: VE M E E
(6.115)
with μE (m2/V/s) the electrophoretic mobility (= q/f) and E the applied electrical field. The friction coefficient for a spherical particle of radius r moving through a fluid of viscosity η, we learned from
Equation 6.26, is given by 6πηr, and its electrophoretic mobility consequently equals: ME
q 6PHr
(6.116)
The frictional coefficient f depends on the size of the molecule in free solution. For a solid sphere f is given by 6πηr, so that f ∼ MW1/3 because r ∼ MW (where MW is molecular weight). Other models are more appropriate for differently shaped molecules, as summarized in Table 6.6. According to the freedraining coil model, a randomly coiled polymer chain in motion hardly interacts with the solvent within it at all. DNA is a good example of a freedraining coil with each unit of the polymer contributing equally to the friction created by its movement through a fluid. Because the charge q is proportional to N (number base pairs), and f ∼ (MW)1 ∼ N, we conclude that: ME
q constant f
(6.117)
As a consequence, DNA strands of varying size cannot be separated by electrophoresis in solution.
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 6.6 Friction Factor f for Variously Shaped Molecules Model
!
Proportionality f ∼ (MW)1/3 f ∼ (MW)1/2 f ∼ (MW)4/5 f ∼ (MW)1
Sphere Random coil Long rod Freedraining coil
MW = molecular weight.
This is why we need to perform electrophoresis in a porous or tortuous material such as a gel. In this case, the solute moves snakelike through the polymer pores. In this model, the frictional term is f ∼ N2. This leads to: ME
q N 1 z 2 z f N N
(6.118)
which is the type of behavior normally observed in DNA electrophoresis. The difference in ion mobility gives rise to a separation in bands of the various solutes, and the narrower the bands, the better the separation. Traditionally, electrophoresis was carried out on columns packed with gels (e.g., a polyacrylamide gel) or on gelcovered plates (Figure 6.67). Electrophoresis in narrow capillaries, as shown in Figure 6.68, was pioneered by researchers such !
"
FIGURE 6.67 Gel electrophoresis.
478
"
FIGURE 6.68 Capillary electrophoresis schematic. A sample may be injected in the capillary through pressure application (e.g., a syringe) on the sample vial or suction at the outlet of the capillary. A more elegant solution for sample introduction is through electroosmotic pumping, discussed below. The chart recorder in this case plots absorbance (Ab at 280 nm) versus time.
as Virtanen38 and Jorgenson,39 who recognized important advantages of this approach. Performing electrophoresis in smalldiameter capillaries allows the use of very high electric fields because the small capillaries efficiently dissipate the heat that is produced. Increasing the electric fields produces very efficient separations and reduces separation times. Capillaries are typically of 50μm inner diameter and 0.5 to 1 m in length. The applied potential is 20 to 30 kV. Because of electroosmotic flow (see next section), all sample components migrate toward the negative electrode. A small volume of sample (10 nL) is injected at the positive end of the capillary, and the separated components are detected near the negative end of the capillary. CE detection schemes include absorbance (see the example in Figure 6.68), fluorescence, electrochemistry, and mass spectrometry. The capillary also can be filled with a gel, which eliminates the electroosmotic flow. Separation is accomplished as in conventional gel electrophoresis, but the capillary allows higher resolution, greater sensitivity, and online detection. To cool the capillary during electrophoresis, a Peltier device, forced air convection, or a flowing liquid bath may be used. ElectroOsmosis Capillary electrophoresis to some degree always is accompanied by electroosmosis. The inside wall
Fluidics
Neutral

+ +
Net positive charge Net negative charge
+

+

+
+
+  + +  + + + + + + + +      +   +     +
+

+
+
+

+
Anode
Bulk solution (cations = anions) Diﬀuse part of double layer (rich in cations) Surfacebound O and tightly adsorbed cations Fused silica
(a)
+
479
+ +
+


+
+
+  + +  + + + + + + +    +   + +    +
+
+

+
Net ﬂow toward cathode
+
– Cathode
(b)
+
–
Anode
Cathode
(c)
Electroosmotic velocity proﬁle
FIGURE 6.69 A schematic diagram showing the origin of electroosmotic flow. (a) Electric double layer is created by negatively charged silica surface and excess cations in the diffuse part of the double layer in the solution near the wall. The wall is negative, and the diffuse part of the double layer is positive. (b), Predominance of cations in diffuse part of the double layer produces net electroosmotic flow toward the cathode when an external field is applied. (c) Electroosmotic velocity profile is uniform over more than 99.9% of the crosssection of the capillary. Capillary tubing is required to maintain constant temperature in the liquid. Temperature variation in larger diameter tubing causes bands to broaden.
of a fused silica capillary is covered with silanol groups (SiOH). Silanol groups have a pK a near 2 and consequently carry a negative charge (SiO −) at pH > 2. Positive compensating charges (cations) are either in an immobile layer immediately adjacent to the glass surface, the Stern layer, or in the diffuse part of the double layer, referred to as the GouyChapman layer. The GouyChapman layer stretches a bit further out into the solution, ∼10 nm further away when the ionic strength of the medium in the capillary is 1 mM.* In a tangential electric field, excess cations in the mobile part of the diffuse double layer are attracted to the cathode, and this imparts a pumping action onto the whole fluid column, which moves toward the cathode (Figure 6.69).40 This pumping describes electroosmotic or also electroendosmotic flow.
*
For a binary electrolyte in aqueous solution, the doublelayer thickness ranges from 3 to 300 nm for electrolyte concentrations of 10 −2 to 10 –6 M, respectively.
The electroosmotic velocity, VEOF, is given by: VEOF M EOF E
(6.119)
where μEOF = the electroosmotic mobility E = the applied electrical field The electroosmotic mobility (q/f ) is given by: M EOF
E6 PH
(6.120)
where ε = the dielectric constant ζ = electrokinetic or zeta potential η = is the fluid viscosity The structure of the electrical double layer (EDL) is detailed in Chapter 7. Here we list some of the most salient features of the EDL model. A thin layer of liquid along the capillary wall never moves; liquid movement begins only at a shear plane in the diffuse double layer at a distance, x 0, away from the wall. The electrokinetic potential ζ (from which all electrokinetic effects can be derived) represents
480
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
the value of the electrostatic potential, ψ, at x 0. Its value at any point is determined from the profile of the electrostatic potential as a function of distance from the capillary wall into the moving fluid (see Figure 7.25). The thickness δ of the diffuse layer itself is defined as the distance from the immobile Stern layer to a point at which the electrostatic potential has dropped to 37% of the zeta potential. The amount and type of ionic species in the solution can greatly influence the zeta potential; for example, the larger the concentration of added indifferent electrolyte in the moving solution, the smaller the ζ (see Figure 7.25). The zeta potential of an aqueous solution in contact with glass can have a magnitude as high as 100 mV.3 Besides pH and ionic strength, surface impurities also might affect the electrokinetic potential, and all conspire to make electroosmosis a rather difficult pumping mechanism to control. Despite these barriers, several new miniaturized bioanalytical products based on electrokinetic effects are now on the market (e.g., visit www.nanogen.com and www. calipertech.com). Most product applications concern genomic analysis; medical and environmental diagnostics have not been able to garner the same amount of funding today. Generalizing, Equations 6.115 and 6.119 may be expressed as: V M a E or
V Ld / t V / L t
(6.121)
where V = the velocity of ions or fluid column μa = the apparent mobility (i.e., the vector sum of electroosmotic and electrophoretic mobilities) E = the electric field strength L d = the length of the column from injection to detector t = the time required for solute to migrate from the injection point to the detector V = the applied voltage between the two ends of a capillary with total length Lt As pointed out earlier, mathematically, electroosmosis and electrophoresis are indistinguishable: either the charge moves through the medium or the medium moves through the charged capillary. In the case of electroosmosis, ζ is the electrokinetic
potential at the capillary wall; in the case of electrophoresis, it is the electrokinetic potential at the charged particle. In absolute terms, electroosmotic mobility generally is larger than electrophoretic mobility. Under typical experimental conditions, say for DNA separations (300 V/cm), the electroosmotic mobility of DNA molecules within fused silica capillaries is 1.25 to 3 times larger than their electrophoretic mobility. In some cases electroosmosis is undesirable; for instance, in gelfilled capillaries the gel may ooze out of the capillary or positively charged proteins may adsorb onto the capillary walls. Electroosmosis may be suppressed by chemical modification of the capillary surface with a neutral EOFsuppressing polymer (e.g., by coating with polyacrylamide41 or methyl cellulose). By the adjustment of the buffer pH and/ or buffer concentration, or by the application of a radial electric field, the EOF also may be modulated by the user.40 The latter may change both the magnitude and the polarity of the zeta potential. In the section below on scaling in analytical separation techniques, we will further detail advantages and disadvantages of miniaturizing electrophoresis and electroosmosis and separation equipment in general. Flow Profiles The flow through a separation media such as a capillary may be a consequence of an applied pressure (i.e., hydrodynamic) or of an applied field (i.e., electroosmotic). In a pressuredriven system, an external pump provides the pumping force. As shown in Figure 6.70a, a crosssection of a hydrodynamic velocity flow profile driven by a pressure difference between the ends of a column is parabolic (see Equation 6.46 and Figure 6.22). It is the fastest at the center and slows to zero at the walls. When injecting a solute, the parabolic flow profile makes for a less attractive analytical tool, as it causes band broadening (see also the section below on scaling in separation techniques). Electroosmosis, in which the driving force is generated very close to the capillary wall, gives a uniform flow over more than 99.9% of the crosssection of a capillary column, as shown in Figure 6.70b. The speed of the flow falls off immediately adjacent to the capillary wall. To illustrate
Fluidics
481
Hydrodynamic ﬂow Buffer Pump
“Parabolic ﬂow”
(a) Sample waste
Electroosmotic ﬂow Sample –
+ “Plug ﬂow”
Injection valve
(b) Separation channel
FIGURE 6.70 A hydrodynamic velocity profile (a) compared with an electroosmotic velocity profile (b).
this with a practical example, in a typical DNA electrophoresis experiment, the double layer δ is around 30 Å thick, and x0 (see Figure 7.25) is even thinner. Compared with the inner diameter of a capillary of 50 μm, the region of velocity variation is negligible. Flat flow profiles are expected when the capillary radius is greater than about 7 times the doublelayer thickness. The rapid flow of buffer and analyte with a flat velocity profile is attractive, as it can be used to pull all analytes, regardless of their mobility, past a detector without contributing significantly to band broadening. In hydrodynamic injection of a sample in a capillary, the injected volume is derived from the volumetric flow rate, Q, in m3s–1. The flow rate Q, of an incompressible fluid with viscosity η (N/s/m2) in a capillary with inner diameter d (m) and total length of the capillary Lt (m), resulting from an applied pressure Δ p (N m−2), is calculated from HagenPoiseuille’s Law (Equation 6.54) as: Q
$pPd 4 128HL t
(6.54)
This equation applies for laminar flow of a fluid through a capillary. To obtain the volume, V, the volumetric flow rate Q is multiplied by t, where t is the injection time: V Qt
(6.122)
Conventional pumps must generate extremely high pressures when narrow capillary diameters are used, and they are not well suited for the delivery of small samples. This is where electroosmotic pumping comes in.
2 mm
Waste
FIGURE 6.71 Microchip used for highspeed electrophoretic separations. Inset: Enlargement of the injection valve and separation channel. (Based on Jacobson, S. C., C. T. Culbertson, and J. M. Ramsey. 1998. Solidstate sensor and actuator workshop. Hilton Head Island, SC: Transducers Research Foundation.)
Electrokinetic Injection Electrokinetic injection is popular in micromachined fluidics (see Figure 6.71), but it is more generally applied in capillary gel electrophoresis, in which the liquid is too viscous to allow for hydrodynamic injection. In electrokinetic injection, a capillary is dipped in sample solution, and a voltage is applied between the ends of the column. The moles of each ion, moli, absorbed into the capillary in t seconds are given by: ¥ K ´ mol i M a ¦ E b µ tPr 2C i § Ks ¶
(6.123)
where μa = the apparent mobility of the analyte E = the applied electric field r = the radius of the capillary Ci = the sample concentration (molm−3) κb/κs = the ratio of the conductivities of the buffer and the sample Electrokinetic injection leads to sampling bias, because a disproportionately large quantity of the species with higher electrophoretic mobility migrates into the tube and can cause problems for
482
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
quantitative analysis. Moreover, electroosmotic flow rates tend to change over time because the zeta potential changes over time, thus leading to changes in μa in Equation 6.123. Below, we will see that certain types of electroosmotic injection methods in miniaturized flow channels avoid this type of sample biasing and aging effects. Micromachined Capillary Electrophoresis Equipment Planar Fluidic Networks In freeflow, traditional capillary electrophoresis work by Jorgenson et al.,42 electroosmotic flow rates of 1.7 mm s −1 were reported, certainly fast enough for many analytical purposes. The technology for generating this flow rate does not involve moving parts and is easily implemented in micromachined channels. Using micromachined channels in a substrate instead of glass capillaries offers the potential for mass production, the choice of many materials (e.g., different plastics besides glass), and the integration of many processing steps on one chip. One needs only one electrode in the reservoirs at each end of the different flow channels, and these electrodes may be thin films deposited on the substrate or needle electrodes inserted into the reservoirs from above (bedofnails approach). Harrison et al.43 achieved electroosmotic pumping with flow rates up to 1 cm s −1 in 20μm capillaries micromachined in glass. Compared with conventional capillary electrophoresis, where separations usually are in the order of 10–20 min, microfabricated electrokinetic devices are capable of producing high quality separation in seconds or even submilliseconds as first demonstrated by Jacobsen et al.44,45 In Figure 6.71 we show a schematic of the microchip used by Jacobson et al.46 for submillisecond electrophoresis using a field strength of 53 kV cm–1 and a separation length of 200 μm. Two dyes, rhodamine B (RB) and dichlorofluorescein (DCF), were resolved in 0.8 ms using this system.47 The earliest patents describing electrophoresis and electroosmosis in a micromachined channel with side branches in a planar substrate are by Pace (filing date June 1988)48 and by Soane et al.49 (priority filing date Feb 28, 1990). The latter is the more generic patent of the two, as it covers all insulating substrates for making fluidic channels, whereas the former patent is
confined to Si. Si, besides being expensive, is a semiconductor and needs to be coated with an insulator before it can be used in an electrokinetic application. When using SiO2 as the insulator, the oxide tends to break down and age rapidly in contact with water, making Si far from ideal as a substrate for an electrokinetic device. As far back as 1991, Manz et al.50 demonstrated the injection, mixing, separation, and reaction of fluids in a manifold of micromachined flow channels without the use of mechanical valves. Manz et al.51 described a set of reservoirs connected by an Hlike pattern of capillary channels etched into a glass substrate. This setup is schematically reproduced in Figure 6.72. Application of a voltage between reservoir 1 (sample) and reservoir 4 (injection waste) results in flow of sample across the center of the H. Subsequent application of a potential between reservoir 2 (carrier) and reservoir 5 (waste) directs the geometrically confined sample plug from the center bar of the H into the elongated leg of the H, that is, into the separation channel and toward the detector. By applying a potential between reservoirs 1 and 4 for an extended period of time, the composition of the fluid plug in the center of the H will be identical to that of the sample, thus avoiding the bias errors described under electrokinetic injection above. In addition, because the injected volume is geometrically defined, the amount of injected sample is reproducible and independent of changes in the electroosmotic flow over time. The key to the tightest possible valving of liquids at intersecting capillaries in a manifold, as shown in Figure 6.72, is the suppression of convection and diffusion effects. Harrison et al.43 demonstrated that these effects can be well controlled by appropriate and simultaneous application of voltages to the intersecting channels. Fast separations in micromachined fluidics are possible by confining the smallest possible sample plug at an intersection.52,53 Ramsey achieved this by controlling the voltages at all four terminals of a simple cross structure, as shown in Figure 6.73, and pinching the plug at the intersection. In this way, the injected sample plug is of the order of the channel width. In the pinched injection mode demonstrated in Figure 6.73, analyte is pumped electrophoretically and electroosmotically from reservoir 1 to 2 (left to right) with mobile phase from reservoir 3 (top) and
Fluidics Carrier Sample or buﬀer 2 1
Detector
Analyte 1
10 mm
483
Buffer 3 Waste 2
Intersection 5 5 Waste
Carrier or buﬀer 3 4 Injection Waste
250 μm
Separation Column 6 Buffer 4
Load 1. 90% 2. 0% 3. 90% 4. 100%
Run 50% 50% 100% 0%
FIGURE 6.73 Pinched injection. Load and run modes (see text). (Based on Ramsey, J. M. 2000. Lockheed Martin Energy Research Corporation. US Patent 6,010,607.) FIGURE 6.72 Schematic drawing of an electrokinetic injection process using a branched microflow system. Layout of the glass chip with integrated sample injector. Channel crosssections: 50 × 12 (thin channels) and 250 × 12 μm (broad channels), respectively. After application of a high voltage between reservoirs 1 (sample) and 4 (injection waste), the geometrically defined injection volume (double“T” injection, circled area) is filled by electrophoretic migration of the sample ions. After loading is completed, application of a high potential between reservoirs 2 (buffer) and 5 (waste) drives the injected sample plug into the separation channel and causes electrophoretic separation of the sample components. The detection is based on laserinduced fluorescence (LIF). The Tintersection where the selected sample zones are withdrawn is enlarged in the circled image. (Based on Effenhauser, C. S., A. Manz, and H. M. Widmer. 1995. Manipulation of sample fractions on a capillary electrophoresis chip. Anal Chem 67:2284–87.)
reservoir 4 (bottom) traveling to reservoir 2 (right). The appropriate voltages, as indicated in Figure 6.73, are applied to reservoirs 1, 3, 2, and 4, whereas reservoir 2 is grounded, thereby spatially constricting the analyte in the injection cross or intersection 5. This plug can be injected into the separation column 6 by applying a bias between electrodes 3 and 4 (4 is grounded now) while the potential of reservoirs 1 and 2 is kept at half the value of reservoir 3. The above plumbing examples are simple; more complex manifolds exist that enable serial and more complex analytical procedures. These procedures include flow injection analysis, metering, mixing,
reaction, dilution, aliquoting, pre and postcolumn derivatization, addition of masking agents, and preconcentration (perhaps using isoelectric focusing techniques; see below). An interesting manifold configuration by Burggraf et al.55 involves synchronized cyclic capillary electrophoresis (SCCE). In this technique a sample, through a sequence of voltage applications, is cycled through a loop made up of intersecting capillaries; after each pass the sample gets separated better into its constituent compounds.55 A single electrokinetic channel can only be optimized to a point; once an optimum critical channel length and a minimal dead volume detector and injector have been designed (see scaling in analytical separations), other means to improve throughput must be implemented. For example, to obtain high throughput with integrated fluidics, one important need is for serialtoparallel converters.56 Optimal Size of Fluidic Channels—Scaling With 1mmwide conduits and flow velocities not greater than a typical centimeterpersecond range, the Reynolds numbers for flow are so low that all flow is laminar. Mixing then occurs solely by diffusion, and the time required for molecules to travel a distance x is given by τ = x 2/2D (see Equation 6.100). For homogeneous flow to be established, bringing two streams of different compositions together at a Yjunction requires that the molecules diffuse over
484
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
500 μm (onehalf of the channel width). For a molecule such as fluorescein with a D of 3 × 10−6 cm2/s, this process will take 400 s, and with a flow velocity of 1 cm/s, the channel must be 4 m long before the mix has homogenized. Reducing the channel width to 70 μm and using the same flow rate, mixing is established in 2 s over a distance of 2 mm only. This suggests an upper limit of about 100 μm for the channel width, based on the need for fast mixing by diffusion. At very small dimensions, another limitation lurks. Assume that one wants to detect an analyte at 1 nM concentration in a cubic micrometer volume. The number of molecules in that small volume is only 0.6 (see also Volume III, Table 7.5). In other words, about half of the time nothing there will be detectable. Singlemolecule detection is possible, for example, with fluorescence burst counting as demonstrated by Haab et al.57 and Wahl et al.,58 but it is far from common; 1000 molecules is a much more comfortable number with which to work. To have about 1000 molecules available in a 1nM solution (a quantity readily detected), a volume of 12 μm3 is needed. So, for optimal detection chamber dimensions should not be much smaller than 10 μm. With a channel crosssection of 2 × 10–3 mm2 and a flow velocity between mm/s and cm/s the flow rate is in the nL/s range. Often, flow control must be within 1% or 1 pL/s. This tight tolerance is impossible to reach with today’s micropumps, which cannot provide accurate control in the nL/s range. With electrokinetics flow control better than 1% is easily achieved.19 Isoelectric Focusing Isoelectric focusing (IOF) is the migration of charged particles (electrophoresis) under pH gradients to a location in the buffer, where they have zero net charge (isoelectric point). The pH gradient is set up between a cathode and an anode with the cathode at the higher pH.59 This ingenuous process simultaneously concentrates and separates. Individual charged species, such as proteins, are rendered immobile as electrophoresis pushes them into the pH gradient until they arrive at the pH that renders them neutral, that is, at their isoelectric point (Ip) or isoelectric pH (IpH). Small amphoteric molecules (called ampholytes), which comprise a multitude of varying Ips, form the pH gradient. The ampholytes in an agarose or polyacrylamide gel carry a net charge, and a linear
pH E
Green ﬂuorescent protein Phycoerythrin Allophycocyanin
X
FIGURE 6.74 Isoelectric focusing (IOF).
pH gradient is built up when an electric field is applied in the socalled prefocusing step (see Figure 6.74). In this brief treatment of the subject, we are particularly interested in the advantages and disadvantages of downscaling a static IOF system compared with downscaling a traditional electrophoresis system. The focusing effect of the electrical force is counteracted by diffusion, which is directly proportional to the analyte (e.g., proteins) concentration gradient in the zone. At steady state, a balance between electrophoresis and sample diffusion holds and can be described by: CME D
dC dx
(6.124)
where C = the sample concentration dC/dx = the concentration gradient E = the applied field strength D = the diffusion coefficient μ = the electrophoresis mobility At steady state, this differential equation yields a Gaussian [C(x) = C0exp (−x 2/2σ2)] for the concentration distribution, resulting in individual bands with bandwidth σ: dx dpH S p ¥ dM ´ E¦ § dpH µ¶ D
(6.125)
As the values of E and d(pH)/dx increase, the distribution width decreases. At a separation of 3σ, bands are considered resolvable, and the minimum pH separation between adjacent zones is described as:
485
Fluidics
$pHmin $L min
dpH dpH 3S dx dx
(6.126)
V
The resolving power is deduced by setting ΔpH equal to ΔpI and replacing σ with Equation 6.125: $pImin 3
DdpH ¥ dM ´ ¦§ dpH µ¶ V
(a) Generic electrophoresis:
(6.127)
To arrive at Equation 6.127, we also substituted the electric field E by V/L, with V the applied potential and L (= dx) the length of the separation medium. From this equation, the minimum resolvable isoelectric point difference between adjacent focused bands is independent of L and dependent only on individual protein characteristics, the total pH difference, and the applied potential.60 With pH and voltage gradient held constant, a sharper pH gradient (i.e., a shorter column) thus is expected to lead to a better separation. Exceptionally short columns might enable shorter analysis time and imaging of the entire separation with an inexpensive line array chargecoupled device (CCD).60 In principle IOF downscales better than capillary electrophoresis, where the capillary length determines the resolution (see further below under scaling in analytical equipment). The maximum allowable temperatures dictate the minimum IOF separation length. Higher temperatures decrease the viscosity in an exponential fashion, thereby increasing the diffusivity of the sample. As the separation channel is shortened below 1 mm, Herr et al.60 calculate a 23% increase in diffusivity compared with macroscale IOF (the macroscale device in the comparison is 20 cm long, and both have a 50μm diameter channel). As a compromise, this research group chose an 8mmlong channel. In Figure 6.75 capillary electrophoresis and capillary isoelectric focusing are compared. Open Electrophoresis Electrokinetics can be exploited to guide and manipulate charged particles (DNA, RNA, PCR amplicons, polynucleotides, proteins, enzymes, antibodies, nanobeads, and even micron scale semiconductor devices) on a planar chip equipped with an array of closely spaced planar metal film electrodes.61 The ability to produce welldefined electric fields with such electrode
–
+
ab b ca
" Later... V –
+
c a a bb c a c b
In capillary electrophoresis, because of high surface:volume ratio, electroosmotic ﬂow becomes signiﬁcant: V –
+
+O+ +O+ +O+ +O+ +O+ +O+ +O + +O+
+
S

!
!
(b) Isoelectric focusing: V – c a b c ba c a b
a
c
b c a
+ Dilute acid
Ampholytes are selected to encompass the pI’s of proteins of interest. As gradient forms, protein charge is determined. If positive (pH below protein pI), the protein moves toward cathode; if negative (pH above protein pI), toward anode. Later... V –
b
pH bb
c c c
+ Dilute acid
Regardless of which direction protein initially moves, as it approaches the region where pH equals its pI, it loses net charge, and ceases to move.
FIGURE 6.75 (a) Generic electrophoresis. (b) Isoelectric focusing (IOF).
arrays (see, e.g., the Nanogen DNA array; Volume II, Chapter 8, Example 8.2) enables one to electrophoretically transport those charged particles to or from any microlocation on the surface of the device submerged in the analyte solution. This socalled open electrophoresis technique does not use fluidic conduits but closely spaced, individually addressable
486
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
electrodes. We explore this topic further below when using the Nanogen DNA array for dielectrophoresis (DEP) and in Volume III, Chapter 4 on packaging, assembly, and selfassembly, where we use the same chip for electric fielddriven assembly.
Electrokinetic Effects—Alternating Currents (AC) Introduction The AC electrokinetic effects we discuss here are dielectrophoresis (DEP), electrorotation (ROT), and traveling wave dielectrophoresis (TWD). Pohl introduced the term dielectrophoresis in 1951 to describe the motion of particles caused by dielectric polarization effects in nonuniform electric fields.63,64 The effect was first recorded more than 2500 years ago, when it was discovered that rubbed amber attracts bits of fluff and other matter. Electrorotation is the rotation of particles in rotating electric fields, and traveling wave dielectrophoresis describes the translational movement of particles exposed to traveling electric fields.65 In electrophoresis, motion of a particle is determined by a net intrinsic electrical charge carried by that particle. In dielectrophoresis, on the other hand, motion is determined by the magnitude and polarity of charges induced in the particle by an applied field. In electrophoresis, direct current (DC) or lowfrequency electric fields, usually homogeneous, are applied; in dielectrophoresis, on the other hand, alternating current (AC) fields of a very wide range of frequencies (in principle, there is no upper limit) are used, and the field must be inhomogeneous.66 The dielectrophoresis effect can be understood with reference to Figure 6.77. A particle placed in an electric field becomes electrically polarized as a result of partial charge separation, which leads to
Surface Electrophoresis As a further extension of the open electrophoresis concept, consider Wickramasinghe’s use of AFM tips for molecular manipulation.62 Applying a field between an AFM tip and a conductive surface, DNA electrophoresis over the shaft of the AFM tip was demonstrated at unprecedented speeds (104 times faster than CE) (Figure 6.76). We saw earlier that in free solution electrophoresis, DNA behaves as a freedraining coil, so that both charge and hydrodynamic drag scale linearly with molecular size (Equation 6.117). This is why DNA sequencing is not normally possible in free solution. Traditional DNA sequencing is done in a gel or polymer matrix, which presents a series of obstacles or obstructions, providing friction that depends on molecular size. Small DNA molecules migrate more easily through the pores of the gel, and thus have greater electrophoretic mobility than large DNA molecules. In the AFM case, electrophoretic separation of molecules such as DNA takes place in the nanometerthick water films covering the shaft of the AFM tip (Figure 6.76A). In this layer, the Debye screening length is greater than the water film thickness, and surface charges are not screened totally by the water molecules. This might explain these encouraging results. (A)
(B) 4x104
Chemical derivatization
(b)
Metallic coating
E
Mobility [cm2/Vs]
(a)
3
2
1
0
0
20
40
60
80
100
N bases
FIGURE 6.76 DNA electrophoresis. (A) (a) AFM setup and (b) AFM tips. (B) DNA mobility as a function of base pair number.
487
Fluidics (a)
(b) + Lower field
+ Lower field
Higher field
Higher field
–
– + + – + + – + – + + – +
+
–
+
– – + – – – + – – + –
– – + – + – – + – –
Particle less polarizable Dipole direction + Movement
–
+
+ – + + – + – + + – +
Particle more polarizable Dipole direction – + Movement
FIGURE 6.77 Negative (a) and positive (b) dielectrophoresis.
an induced dipole moment. The dipole moment is a consequence of the generation of equal and opposite charges (+q and −q) at the boundary of the particle. This induced surface charge is only about 0.1% of the net surface charge normally carried by cells and microorganisms and is generated within about a microsecond. In a nonuniform electric field, the field on one side of the particle will be stronger than that on the other side, and a net dielectric force, FDEP, is exerted. The magnitude of the induced dipole depends on the polarizability of the particle with respect to that of the medium. If a suspended particle has polarizability higher than the medium, the dielectrophoresis force will push the particle toward regions of higher electric field in socalled “positive dielectrophoresis.” In negative dielectrophoresis, the medium has a higher polarizability than the suspended particles, and the particles are driven toward regions of low field strength. Dielectrophoresis causes a motion of neutral matter by polarization of the neutral matter in a nonuniform electric field. The method is particularly suited for the separation, aggregation, selective trapping, manipulation, and identification of cells and microorganisms.66 Dielectrophoresis Force Spherical particles of radius r and complex permittivity εp, suspended in a fluid of absolute complex
dielectric permittivity εm, are subject to a dielectric force given by: FDEP 2Pr 3 E m A r E 2
(6.128)
where ∇E2 = the gradient of the square of the electric field (rms, or root mean square value) quantifying the nonuniformity of the electric field ∇ = the del vector operator αr = the real component of the ClausiusMossotti factor, that is, the effective polarizability of the particle with respect to its suspending medium; the latter term may thus be written as: ¥ E*p E*m ´ A r Re ¦ µ § E *p 2 E*m ¶
(6.129)
In the above expression: Re = “the real part of” ε*p and ε*m = the complex dielectric properties of the particle and its medium, with ε* = ε − jσ/ω, in — —— which j = √−1 ε = permittivity σ = conductivity ω = angular frequency of the applied field (ω = 2πf)
488
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
For a vacuum, which has no mobile charges, ε is 1, and for a conductor, it is infinite. Because ε*p − ε*m can be positive or negative, depending on the relative magnitudes of ε*p and ε*m, controlled movement from and to areas of high electric field strengths is possible. In other words, a material with a higher dielectric constant will experience a force tending to move it into a stronger electric field, displacing a material with a lower dielectric constant in the process. A positive value for αr in Equation 6.129 implies a positive DEP force; a negative value produces a negative DEP. Because the field E in Equation 6.128 appears as ∇E2, reversing the bias does not reverse the DEP force. Ac voltages in a frequency range from 500 Hz to 50 MHz have been used. Based on Equation 6.129, one recognizes that the factor αr is frequencydependent. At low frequencies polarizability mainly is determined by the conductivity, and at high frequencies it is determined by the permittivity. Theoretically, the value of αr may be between +1.0 and −0.5. Key in dielectrophoresis is the presence of a material of substantially different dielectric constant from its surroundings. In an aqueous conductive solution, ions shield the dielectric material from the external applied field. Varying the field in time reduces the shielding effect of the ions somewhat. If the mobile dielectric materials are embedded in a sufficiently low resistance medium, then the dielectrophoresis effect can be much more readily observed. For a rigorous derivation of Equation 6.128, we refer to Huang et al.67 and Wang et al.68 Using DEP, individual biological cells have been moved and positioned by altering the ac frequency
so as to switch from a “capture” mode using positive DEP to “release” mode using negative DEP.69 Particles can also be separated using DEP. This is illustrated in Figures 6.78 and 6.79. Figure 6.78a reveals how cell type A switches from negative to positive DEP at a changeover frequency of about 105 Hz. From Figure 6.78b we learn that there is a frequency range above 105 Hz where cell type B displays negative dielectrophoresis, whereas A exhibits positive dielectrophoresis. This means that one cell type will move to higher electric field regions, while the other cell type will do the opposite, effectively separating the two types of cells. This effect is exploited in Figure 6.79, where we separate Listeria from whole blood. An array of 100planar Pt electrodes [the Nanogen chip (see Volume II, Chapter 8, Example 8.2)] is used in this experiment. In the first panel, blood contaminated with Listeria is placed over the chip. In the second panel, a 10kHz, 10Vpp ac signal is applied, driving the red blood cells to low electric field regions (i.e., between the Pt electrodes) and the Listeria to high electric field regions (i.e., on the Pt electrodes). In the third panel we wash off the red blood cells, leaving the Listeria highly enriched on the Pt electrodes where they stick better than the red blood cells on the insulating regions (Si3N4) between the Pt electrodes. In the fourth panel only Listeria is left on the chip. Finally, in the fifth panel, we release the Listeria by removing the bias and washing again. In Table 6.7 we summarize some pros and cons of using dielectrophoresis for particle separation. (b)
(a)
0.8
0.8
0.6
Positive DEP
0.4
DEP response
DEP response
0.6
0.2 0 –0.2
Crossingover frequency
–0.4 Negative DEP –0.6 102
104
0.4
Sample A
0.2 0 –0.2 Sample B
Separation frequency region
–0.4 106 Frequency
108
1010
–0.6
10 5
10 6 Frequency
FIGURE 6.78 Dielectrophoresis: how to separate particle A from particle B. (a) Cell type A switches from negative to positive DEP at a change over frequency of about 105 Hz. (b) Above 105 Hz cell type B displays negative DEP, whereas A exhibits positive DEP.
Fluidics
489
Listeria
FIGURE 6.79 Dielectrophoretic separation of Listeria from whole blood.
One problem associated with traditional methods of DEP separation highlighted in Table 6.7 is that the DEP force, which is proportional to ∇E2, rapidly decays as the distance from the planar electrodes increases. As a consequence, a common problem to most current dielectrophoresis devices using planar electrodes is the incapability to achieve high throughputs and high efficiencies. With a given flow channel crosssection, many targeted particles might flow over the planar electrodes without experiencing a force, its mean distance to the electrode surface being too long, making it necessary to reflow the same sample several times. This has prevented DEP from being used in highvolume applications. To correct this problem, the author’s University of California, Irvine, team is using 3D electrodes to reduce the mean distance of any targeted particle contained in a channel or chamber to the closest electrode surface, as illustrated in Figure 6.80. Numerical simulations demonstrating such advantage were obtained
by Park,70 and the experimental verification was carried out by MartinezDuarte.71 The 3D electrodes are implemented using the CMEMS process detailed in Volume III, Chapter 5 (page 266 “Microfabrication of Carbon: CMEMS Process”). In 3D CMEMS dielectrophoresis, carbon 3D structures up to several hundreds of micrometers high are implemented as electrodes in the flow channel. An example of 65μmhigh posts is shown in Figure 6.81. The difference in trapping efficiency of yeast cells, when only flowing the sample once, between 2D and 3D electrodes increases as flow rate increases, with the 2D efficiency always being lower as shown in Figure 6.82. Microfabricated 3D electrodes also have been implemented by Wang72 and Voldman,73 who used electroplated gold electrodes for particle separation, applying the lateral field established by the electrodes that form the channel side walls and for particle trapping for cytometry purposes, respectively. More
TABLE 6.7 Pros and Cons for Particle Separation by Dielectrophoresis Pros
Cons
Intrinsic dielectric properties are taken advantage of No immunolabeling involved No narrow channels to clog Simple and low cost Easy to scale down or scale up Can move even semiconductor components
Speed: clinical sample requires ml volume (1) Throughput: can only separate two types of cells (2) Selectivity/sensitivity
1) This problem may be solved using 3D volumetric DEP methods (described next). 2) This problem could be solved by using an array of signal generators.
490
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
(a) Traditional 2D electrodes Particle not experiencing DEP
(b) 3D electrodes Particle experiencing DEP
FIGURE 6.80 (a) In traditional 2D DEP, many particles might flow by without experiencing any DEP force. (b) In 3D DEP, the mean distance from the particle to the electrode surface decreases; thus, the number of particles experiencing DEP force greatly increases.
therapy, sample purification, drug screening, water analysis, and many other applications may become possible in the future. Throughput refers to inducing DEP on as many particles as possible without consideration of selectivity between targeted and nontargeted particles. This is also known as maximal retention efficiency.77 Selectivity refers to how well one can induce DEP to a targeted particle without affecting nontargeted ones. It is also referred to as maximal purification efficiency.77 Traveling Wave Dielectrophoresis If, instead of using a stationary electric field, as is used in DEP, a particle is subjected to a moving electric field, the particle can be moved by an effect known as traveling wave dielectrophoresis, or TWD. To produce these traveling waves, electrode !!%#
recently, Iliescu74 has used complex microfabrication techniques to obtain 3D doped silicon electrodes in a multistep process. In a nontraditional way, LapizcoEncinas et al.75 have induced DEP on bacteria and proteins using insulator volumetric microelectrodes, in a technique that has become known as insulator DEP. The main concept behind this approach is the use of two metal electrodes, excited by thousands of volts, to generate a uniform electric field between them, which is then disrupted and turned nonuniform by the insulator structures in between. Another truly 3D DEP approach is that of Fatoyinbo et al.,76 who use a drilled conductorinsulatorconductor laminate to obtain wells with electrodes all along the top and bottom surfaces of the laminate. The final goal is to improve throughput and efficiency in DEP devices for a commercial product featuring high selectivity at high flow rates. Immediate applications might include cell enrichment for cell
Madou 5.0kV 12.0mm x600 SE(M) 2/20/07 12.15
50.0um
FIGURE 6.81 Carbon posts (65 μm high) for use as electrodes in CMEMS dielectrophoresis (CMEMS DEP).
! &"$
FIGURE 6.82 Higher retention efficiency at all flow rates are obtained with 3D DEP compared with 2D DEP. The difference between them sharply increases with flow rate. (MartinezDuarte, R., H. A. Rouabah, N. G. Green, M. Madou, and H. Morgan. 2007. Proceedings of the Eleventh International Conference in Miniaturized Systems for Chemistry and Life Sciences: microTAS 2007. Paris.)
Fluidics
270°
0°
90°
180°
270°
0°
90°
180°
270°
0°
10 μm
Channel
20 μm
Electrical connections Insulating layer
90°
180°
270°
0°
90°
180°
270°
0°
90°
180°
Track
FIGURE 6.83 TWD setup. Electrode structures for producing traveling electric fields along channels or tracks. When addressed with sinusoidal voltages of the phase sequences shown, a traveling field is established by the propagation direction indicated by the arrow. The characteristic dimensions shown are suitable for manipulating yeast, erythrocytes, and parasites such as Cryptosporidium, for example. Correspondingly larger or smaller dimensions are required for larger bioparticles (e.g., white blood cells, plant cells, pollen) or smaller ones (e.g., bacteria, viruses), respectively. (Burt, J. P. H., R. Pethig, and M. S. Talary. 1998. Microelectrode devices for manipulating and analysing bioparticles. Trans Inst MC 19:1–9. With permission.)
geometries with tracks of electrodes in a channel, as shown in Figure 6.83, may be used. In this arrangement, electrodes are fabricated on a bottominsulating substrate, and a second insulator layer is used to define a channel along the length of the electrode track. Another set of four electrodes is then deposited on this second insulator layer, and vias are used to link every fourth electrode together and to provide external connections. The four electrodes are addressed with sinusoidal voltages of 90° phase separation (0°, 90°, 180°, and 270°). The used phase quadrature voltages are equal in amplitude (around 1 to 5 V peakpeak) and of a frequency range from about 1 kHz to 10 MHz. TWD provides conveyor tracks over which particles, suspended by negative dielectrophoresis, are moved. By changing the magnitude and frequency of the energizing voltages, the speed and direction of particles in the channel can be controlled.65
491
TWD, in combination with DEP, enables selective and nonselective trapping of particles. The selective trap only holds desirable subpopulations, whereas a nonselective trap retains all particles from a fluid flow. Particles moving in a channel by TWD may be captured nonselectively and held immobile by suddenly changing the frequency and phases of the applied voltages so as to encourage positive dielectrophoresis. By returning to a TWDtype of field, all the particles, or a subset of them, can be made to resume their movement along the channel. In the case of selective trapping, the TWD remains in effect, and trapping is accomplished by the choice of the electric field frequency. The frequency may be chosen such that some particles are levitated by negative dielectrophoresis and thus keep on moving under the influence of the TWD, whereas others are captured by positive dielectrophoresis and are immobilized at the electrode surfaces.65 Particle Levitation The gravitational settling force pulls down a spherical particle with radius r and mass density γ1, suspended in a fluid with mass density γ2, and is given by: Fg
4 3 Pr ( G 2 G 1 )g 3
(6.130)
where g is the gravitational acceleration vector. A particle will hover above the electrode surface when the opposing gravitational and negative dielectrophoretic forces balance: FDEP Fg 0
(6.131)
Or, from Equations 6.128 and 6.130: 2(G 2 G 1 )g 3 E m A r E 2
(6.132)
From Equation 6.132, levitation is independent of particle size, as both DEP and gravitational force scale as l3. Levitation height only depends on the intrinsic properties of the particle, such as permittivity, conductivity, and mass density. By working at very high frequencies, where the polarizability factor primarily depends on the permittivity rather than the conductivity, levitation may also be made independent of the conductivity of the solution. A quantitative
492
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
estimate of the levitation height requires knowledge of how the factor ∇E2 varies as a function of height h above the electrode plane. Rousselet et al.79 derived the following relationship between ∇E2 and h: E 2 AV 2 exp( hk)
(6.133)
where V = applied voltage A = constant k = another constant inversely proportional to the width of the electrodes79 Combining this expression with Equation 6.132, the expression for stable levitation height is derived as: h
1 ¨ 3 E m A r AV 2 · ln © ¸ k ª 2(G 2 G 1 )g ¹
(6.134)
This type of dielectrophoretic levitation was demonstrated, for example, with latex beads and interdigitated electrodes of widths and separations ranging from 5 to 40 μm, with ac signals of 0–10 V (rms) in the frequency range 1 kHz to 10 MHz. Maximum levitation was observed at 1 MHz. At this frequency it was confirmed experimentally that levitation height was independent of particle size and solution conductivity.79 It also was shown that red blood cells could be separated from latex beads easily. Whereas the erythrocytes were attracted to the electrodes by positive dielectrophoresis, the latex particles levitated and could be separated by flowing liquid over the surface. By deenergizing the electric field, the red blood cells also could subsequently be removed by flowing more liquid.79 Particles possessing different dielectric properties levitate at different heights in a flat fieldflowfractionation (FFF) chamber through the balance of DEP and gravitational forces.68 The different particles are levitated into streamlines with different velocities, as shown in the parabolic flow profile illustrated in Figure 6.84, and can be separated this way. Even continuous separation of particles is possible.80
FIGURE 6.84 Fieldflow fractionation (FFF). Outline of the combined DEPFFF separation procedure. Particles with different dielectric properties or density are levitated by negative dielectrophoresis to different planes of the parabolic velocity profile of the liquid flowing through the chamber. (Rousselet, J., G. H. Markx, and R. Pethig. 1998. Separation of erythrocytes and latex beads by dielectrophoretic levitation and hyperlayer fieldflow fractionation. Colloids Surfaces A 140:209–16. With permission.)
using four electrodes positioned at right angles to one another and energized with phasequadrature signals of frequencies between 50 Hz and 100 MHz. The ROT torque acting on a particle positioned in the center of this electrode assembly is given by: TROT 4P r 3E m A i E 2
(6.135)
where αi is the “imaginary part” of the ClausiusMossotti factor. As with impedance spectroscopy, there is a direct relationship between the real and imaginary components of the ac electrokinetic effect, so that the electrorotation frequency spectrum can be calculated from the measured dielectrophoresis response, and vice versa. In Figure 6.85 the frequency variations of αr and αi for viable and nonviable yeast cells are shown. The polarity and peak values of αi are determined by the rate of change of αr. The frequency dependence of magnitude and polarity of αr and αi is the basis of the three ac electrokinetic applications discussed here. Rotation analysis chambers in a biofactoryonachip are used to monitor dielectric properties of particles.65 Electrorotation has been shown to be a sensitive method for monitoring the physiological viability of cells.82
Electrorotation Electrorotation (ROT) is the imaginary component of the ac electrokinetic effect, whereas its real component is the aboveintroduced dielectrophoresis (DEP). The rotating electric field usually is generated
Scaling Considerations Depending on particle size, different forces compete with the DEP force. For example, a typical biological cell with a radius of 1 μm and a density of
Fluidics
FIGURE 6.85 Alpha plots. The frequency variations of the real and imaginary polarizability parameters αr and αi of Equations 6.128 and 6.135 for viable (a) and nonviable (b) yeast cells in a suspending medium of conductivity 0.8 mS/m. Only the nonviable cells will exhibit traveling field dielectrophoresis (in the frequency range f1) and thus the viable cells will remain immobilized at the electrodes. (Burt, J. P. H., R. Pethig, and M. S. Talary. 1998. Microelectrode devices for manipulating and analysing bioparticles. Trans Inst MC 19:1–9; and Talary, M. S., J. P. H. Burt, J. A. Tame, and R. Pethig. 1996. Electromanipulation and separation of cells using travelling electric fields. J Phys D Appl Phys 29:2198–203. With permission).
1.05 kg m−3 suspended in an aqueous solution at room temperature feels both the gravitational and the Brownian force of around 2 × 10−15 N each. For the DEP force to dominate, it should be at least 10 times larger than these competing forces; to affect this, ∇E2 must be around 9 × 1012 V2m−3 (with an α of 0.5).66 Both the DEP and the gravitational effect scale as l3, and, with increasing particle size, no scaling advantage of one over the other emerges. With submicrometer particles, on the other hand, the randomizing Brownian effect, being proportional to l−1, becomes the dominating force competing with DEP. With particles below 0.1 μm, for example, values for ∇E2 greater than 1017 V2m−3 are required to make the DEP force 10 times larger than the Brownian. This requires field strengths in excess of 106 Vm−1, and at a suspending medium conductivity higher than 0.1 Sm−1, these high fields cause local heating, leading to hydrodynamic effects. The latter interfere with the DEP effect of submicron particles significantly.66 Moreover, at these fields cell damage might become an issue. Müller et al.83 used submicronscale electrodes to achieve DEP levitation and trapping of
particles as small as 14 nm, but, as predicted, hydrodynamic effects interfered significantly. Downscaling of the electrodes is very favorable in dielectrophoresis. By using thin film metal electrodes rather than wire or pin electrodes, one approaches the size of the typical particles to be separated. In Figure 6.86, the expression for ∇E2 for the specific represented electrode configuration is given. Maintaining the applied voltage at 1 V rms and reducing the radius of curvature 100fold produces a 1000fold increase in ∇E2. Lower voltages can thus be used to produce the same DEP force on a particle in the same relative position. Despite the small crosssectional area of the electrodes, the volume of liquid they energize is very large by comparison, so that heat produced by the electrical current is efficiently dissipated, and, moreover, surface electrochemical processes are reduced.66 Applications In a 1983 patent, Batchelder84 describes the use of dielectric forces to selectively position, transport,
493
E
r
FIGURE 6.86 Two particles located in a nonuniform electric field, generated in this example by electrodes of spherical geometry and radii of curvature Ri and Ro. Different dipole moments m (depicted as separated microcharges q) are induced in each particle. Particle a is more polarizable than the surrounding medium and is directed by positive dielectrophoresis toward the high field at the inner electrode, whereas particle b is weakly polarizable and moves toward the lowfield region at the outer electrode under the influence of negative dielectrophoresis. The force causing this motion is proportional to ∇E2, described by the equation in the figure, where s is the distance of the particle from the inner electrode, V is the applied (rms) voltage, and r0 is a unitradius vector. (Pethig, R., and G. H. Markx. 1997. Applications of dielectrophoresis in biotechnology. TIBTECH 15:426–32. With permission.)
494
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
mix, and react one or more chemicals within a reaction chamber. The Batchelder patent was ahead of its time in terms of vision for microfluidics and constituted a laboratoryonachip (LOC) long before academics introduced the buzzword. The emphasis in this patent is on the dielectrophoresis mechanism, and little is said about micromachining. Although metal electrodes are patterned with lithography techniques, the reaction chambers are made with more traditional manufacturing methods. Once microelectrode technology and MEMS made their entry, it became apparent that dielectrophoresis would be a promising tool for the selective manipulation and separation of cells, bacteria, viruses, and perhaps even biomacromolecules such as DNA and proteins. A limitation may be cell damage, electroporation, and electrofusion, which start at field strengths of 1–3 × 105 Vm−1. However, in dielectrophoresis, the field is rarely higher than 105 Vm−1. In practice, no irreversible cell damage has been reported in DEP experiments.66 Another possible limitation is that of particles being smaller than 10 nm; these might be too difficult to manipulate because of the hydrodynamic effects interfering with the DEP force. Batch and continuous separation of particles has been achieved through positive and negative DEP in FFF chambers. A typical DEPFFF separation chamber is shown in Figure 6.87 and consists of two glass plates spaced a small distance (typically 99.2% are obtained.85 Electrorotation is used, for example, to determine the dielectric properties of human leukocyte
Dielectrophoretic separation chamber Valve 2
Cell type 1 (nonviable cells)
Cell type 2 (viable cells)
Valve 1
Pump 2
Pump 3
Pump 1 Microscope slide with interdigited, castellated electrodes
Cell mixture
FIGURE 6.87 Outline of a continuous dielectrophoretic separation system. Valves, frequency generators, and pumps are all under computer control. (Markx, G. H., and R. Pethig. 1995. Dielectrophoretic separation of cells: continuous separation. Biotech Bioeng 45:337–43. With permission.)
subpopulations.86 Pethig et al.65 are experimenting with combinations of DEP, ROT, and TWD elements on a single substrate to make a socalled biofactoryonachip.
Electrowetting Electrical control of interfacial tension between a liquid and a solid provides another means of fluid pumping without moving mechanical parts. Altering the apparent surface tension at the solid/liquid interface becomes possible by applying a potential over the interface. This phenomenon is known as electrowetting and is described by the Lippmann equation: G SL G max
SL
Er E0 ( V Vpzc )2 2D
(6.136)
where Vpzc represents the potential of zero charge max for the solid/liquid (electrolyte) interface, and G SL is the surface tension corresponding to V = Vpzc. The thickness of the diffusion layer in the solution is given by δ, and εr and ε0 are the relative permittivity of the solution and the permittivity of vacuum, respectively. A voltage applied across the interface will alter the surface tension and cause the liquid to move within the capillaries. The flow velocities achieved with electrocapillary pressure are several centimeters per second or nearly two orders of magnitude higher than the velocities achieved by electroosmotic pumping.87
Fluidics
Surface tension becomes important only when dimensions drop well below 1 mm. As in the case of electroosmotic pumping, subtle uncontrollable changes at the solid/electrolyte interface make this actuation principle difficult to control and electrolyte specific. Light has been used to control the wettability of the surface of certain photoresponsive materials. The exact mechanisms of the surface wettability changes of these materials on illumination still are being debated; however, it is generally accepted that the effect is caused by a photoelectrochemical reaction at the surface.88 With ZnO, UV irradiation is responsible for generating electronhole pairs on its surface. These holes react with the lattice oxygen to form surface oxygen vacancies in a process described by Zhang et al.89 in the following equations:
495
for example, showed changes of contact angle from 109° before to 5° after UV exposure for a droplet of water on a ZnO surface. Other wide bandgap semiconductor oxides, such as Ta 2O5, TiO2, indium–tin oxide, In TaO4, and In2O3, also exhibit optowetting. These materials reverse their characteristic and tend to go back to their hydrophobic state if the UVexposed sample is placed in a dark room; over time the hydroxyl groups absorbed on the defect sites are replaced by oxygen atoms. This is because the surface is thermodynamically unstable after the hydroxyl absorption, and oxygen is more strongly bonded on the defect site than a hydroxyl group. Because there is some degree of reversibility, these semiconductors show promise as a wettability switch for future microfluidic applications.
ZnO 2hN m 2h 2e
Centrifugal Fluidic Platform—CD Fluidics
O2 h m O 1 O h m O2 V0 (oxygen vacancy) 2
Introduction Reaction 6.1
In ambient air, water and oxygen from the surroundings compete with lattice oxygen to dissociatively absorb on those vacancies. In solution the defect sites, however, kinetically favor the absorption of hydroxyl groups over oxygen,90 and with the surface attracting more hydroxyl (−OH) groups, the surface becomes more hydrophilic. This switch from a hydrophobic to a hydrophilic surface has been extensively documented. Sun et al.,91
An attractive approach to fluid propulsion is centrifugation in fluidic channels and reservoirs crafted in a CDlike plastic substrate as shown in Figure 6.88. The centrifugal force caused by the rotation of the CD results in the release and flow of reagents and analytes. No external pumps and valves are needed— fluidic flow can be controlled by the spinning rate. The centrifugal force generated in such an instrument overcomes (depending on the rotation speed) the capillary forces in the fluidic network and moves fluid in a valveless manner from reservoir chamber
LabCDTM reader
LabCDTM disc
Analysis optics
Drive motor Cuvette Informatics
Spectrophotomeric read cuvette Fluidics manifold
CD optics
FIGURE 6.88 Centrifugal platform on a CD. The name LabCD™ was introduced by Gamera, the first fluidic CD company (now defunct).
496
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
to reaction chamber and eventually to a waste site. A whole range of fluidic functions, including valving, mixing, metering, sample splitting, and sample separation, has been implemented this way.92 Such analytical functions make for a laboratoryonadisc with applications in diagnostics and drug discovery. Analytical measurements may be fluorescent or absorption based, and informatics embedded on the same disc could provide testspecific information (merging of fluidics with informatics). Prototyping methods of this microfluidic platform are covered in Volume III, Chapter 5 on selected new materials and processes for MEMS and NEMS. In Volume II, Chapter 10 on replication techniques and LIGA, we cover manufacturing of the fluidic CD. The aspect of the CD platform we are interested in here is the physics behind its operation and the comparison of CD fluidics to mechanical, osmotic, and acoustic pumping.
Centrifugal Platform Operation In a centrifugal platform, the centrifugal force provides the pumping force, whereas hydrophilic and hydrophobic valves are used to inhibit flow. In Figure 6.89a, we show a schematic of a centrifugal platform together with relevant parameters; Figure 6.89b and c demonstrates two types of hydrophobic valves, and Figure 6.89d is a hydrophilic or capillary valve. For a hydrophobic CD surface, to make a valve, a flow restriction can be made in the flow channel by (a)
(b)
reducing its radius from r1 to r2. A positive pressure is then needed to push the fluid across this restriction. From Equation 6.96, the pressure p is determined by r, the radius of the capillary, and the required pressure Δ p to overcome a sudden narrowing in capillary tubing is calculated from Equation 6.96 as: ¥ 1 1´ $p 2S L cosQc ¦ µ § r1 r2 ¶
(6.137)
Equation 6.137 is independent of the length of the restriction and flow rate. Once the capillary downstream is wetted, the pressure needed to continue flow is given by Equation 6.54 (HagenPoiseuille’s Law). These hydrophobic restrictions can be used as passive valves in fluidic networks: by setting the pumping pressure below the pressure associated with the restriction, no flow will take place unless the pumping pressure is increased. Mixers, diluters, sample splitters, and sample integrators have been built using passive hydrophobic valving in combination with an external mechanical pump.93 Of course, the same principles can be applied in combination with centrifugal, electrokinetic, or acoustic pumping. As shown in Figure 6.89c, one can also create a hydrophobic valve by locally changing the hydrophobicity of the surface, i.e., by locally increasing θc. In the case of a contact angle less than 90° (a hydrophilic surface), to make a valve the capillary is widened, which leads to the need of increased pressure as more energy is required now to wet a larger surface area (Figure 6.89d). (c)
(d)
Center of CD Hydrophobic zones
Δr
r Δr L Liquid
Hydrophobic valves
Capillary valve
FIGURE 6.89 Centrifugal platform on a CD. (a) CD platform, (b and c) hydrophobic valves, and (d) hydrophilic capillary valve.
497
Fluidics
Assuming a capillary valve, when spinning the CD, the two opposing forces at work can be described as follows (see Figures 6.89a and 6.90). The pumping force (Pc) caused by spinning of the disc is given by: dPc RW 2r dr
(6.138)
where ρ = the density of the liquid ω = the angular velocity of the CD platform r = the distance between a liquid element and the center of the CD Integration of Equation 6.138 from r = R1 to r = R 2 gives: $Pc RW 2 (R 2 R 1 )
R 2 R1 RW 2 $R R 2
(6.139)
The capillary force (Ps) caused by interface tension is given by: $Ps
G cosQc C A
(6.140)
where γ = the interface tension θc = the contact angle (in a practical example θc may be 61.5°) A = the crosssection area of the capillary C = the associated contact line length The burst frequency is the frequency at which the fluidics are released from their reservoirs. The
liquid will be released when Δ Pc is greater than Δ Ps; consequently, the burst frequency calculated from Equations 6.139 and 6.140 is given by: 1 2
1
¥ ´2 ¥ G cos Qc C ´ G cos Qc fb r ¦ 2 ¦ µ (6.141) 2 § P R R $R 4 A µ¶ § P R R $R dH ¶ Here dH is the socalled hydrodynamic diameter of the channel. Example 6.8: TwoPoint Calibration Disc As an early first example of the use for the CD fluidic platform, the author and his team, by appropriately choosing the channel diameter and reservoir dimensions and locations, designed an automated twopoint optrode calibration system, capable of five sequential fluid movement steps as shown in Figure 6.91a and b. The liquid flows in the order of calibrant 1, wash 1, calibrant 2, wash 2, and sample to an optrode chamber by increasing the rotating speed (see Figure 6.91a for the placement of these fluidic chambers, top figure is an actual photograph of the CD and the bottom is a schematic). Figure 6.91b shows the calculated burst frequencies of the reservoirs in the twopoint calibration platform. The same optrode chamber is used for measuring calibrants and sample to eliminate artificial system errors common with devices using separate chambers for measuring sample and calibrants. To demonstrate the functionality of this twopoint calibration system, we deposited a potassium ion selective membrane in the optrode chamber using a microdrop delivery setup. The membrane was composed of poly(vinyl chloride) (PVC), valinomycin (ionophore), dioctyl sebacate (plasticizer), potassium tetrakis(4chlorophenyl) borate, and chromoionophore for detection at a 640nm wavelength. The slope (sensitivity) of a doseresponse curve (absorption of the 640nm wavelength vs. concentration) was determined by the measurements of calibrant 1 and calibrant 2.94 The ion concentration of unknown samples was then deduced from this calibration curve. Example 6.9: The CD Platform as a Microscope
FIGURE 6.90 Schematic illustration of fluid propulsion in centrifugal microfluidics.
Horacio Kido and Jim Zoval from the author’s research team recognized that the optical
498
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Sample Second wash Second calibration
First wash
First calibration
Calculated burst frequency (rpm)
Waste
Optical sensor
Center of disc Sample Wash 2 Calibrant 2 Wash 1 Calibrant 1 Optrode
1200 1000 800 600 400 1 Sample
Waste
(a)
5 2 3 4 Wash 2 Calibrant 2 Wash 1 Calibrant 1 Reservoirs (b)
FIGURE 6.91 Twopoint calibration of an optrode on a CD. (a) Functional diagram and photo of a twopoint calibration unit on a CD. (b) A plot of calculated burst frequencies.
disc drive is a sophisticated laser scanning microscope designed to characterize and identify micrometersized features at a rate of about a megahertz (Figure 6.92). By taking the voltages from the photodetector and sending them to a computer using a fast A/D converter, an image of what is on the disc can then be reconstituted using simple graphics software. It does not matter whether the image is a pit in the CD (see Figure 6.92) or objects placed on the disc (see Figure 6.93).
Compact Disc Objective lens 1/4 Wave plate
Beam splitter
Laser
Cylindrical lens
Quadrant photodetector
Low High Voltage
FIGURE 6.92 Using the CD as a microscope.
Time
Example 6.10: Using the Coriolis Force on the CD On a spinning CD, the Coriolis force can be used to switch fluid flow between two reservoirs depending on the direction of the CD’s rotation. The Coriolis force, we remember, is a fictitious force exerted on a body when it moves in a rotating reference frame. It is called a fictitious force because it is a byproduct of a coordinate transformation. To understand the Coriolis force
Fluidics
499
Coriolis force thus can be used to switch fluid flow between a left reservoir and a right reservoir depending on the direction of the CD rotation (Figure 6.94b).
DNA array
Gnat wing
Some other applications of the CD, including cultivation of C. elegans worms, can be found in the References.95,96 A recent review article on CD fluidics can be found in Madou et al.97 In Table 6.8 we compare four popular fluidic platforms: mechanical, osmotic, centrifugal, and acoustic. This table should be read together with the more detailed Table 1.8 from Chapter 1 in Volume III. For more background on the physics behind acoustic fluidics see Volume III, Chapter 8 on actuators.
White blood cells
FIGURE 6.93 Images from the CD microscope.
on the CD, it is convenient to rewrite the NavierStokes equation (Equation 6.8) in a rotating reference frame. This results in an expression for the Coriolis force given as:
FCoriolis 2R u s u
(6.142)
The formula implies that the Coriolis force is perpendicular both to the direction of the velocity of the moving mass and to the frame’s rotation axis. In this expression, ρ is the fluid density, ω is the angular velocity vector, and u is the flow velocity vector. The Coriolis force is transverse to the CD radius and acts to transport the fluid stream left or right depending on the direction of the CD rotation (see Figure 6.94a). The
Scaling in Analytical Separation Equipment Introduction When incorporating sensors in microfluidics one finds that most sensing techniques scale poorly in the microdomain. As we analyze in Chapter 7, different detection schemes exhibit different signal scaling factors. For example, in an amperometric technique, in which an analytical current is the signal, the output exhibits a (l2) scaling (i.e., proportional to the area of the electrode); an optical absorption technique scales as (l3), and potentiometric techniques are, in principle, sizeindependent. In general we find that most detection methods are less sensitive
Inlet
r
FCoriolis –w x u
dH
A left reservoir
r
A right reservoir
FCoriolis u CCW rotation (a)
(b)
FIGURE 6.94 Coriolis force for flow switching. (a) Forces shown on a disc rotating at the angular velocity vector ω pointing into the paper plane. When this disc spins in the counterclockwise direction, the Coriolis force switches the fluid in the channel to the left, and when this disc spins in the clockwise direction, the fluid moves to the right. (b) When the CD rotates counterclockwise (CCW), the Coriolis switching valve diverts fluid to the waste reservoir (left reservoir), and when the CD rotates clockwise, fluid is diverted to the extraction chamber (right reservoir).
500
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 6.8 Comparison of CD Fluidics with Mechanical, Osmotic, and Acoustic Pumping (see also Table 1.8 , Chapter 1 in Volume III)
Mechanical (e.g., with Johnson and Johnson’s blister pouch HIV test; see Figure 1.12 in Volume III, Chapter 1) − Scales as l3 + No contact of sample with electrodes + Generic (all types of sample can be used) + Innovation in the blister pouch + Solves liquid and vapor valving − Difficult to further miniaturize − Difficult to multiplex Electrokinetic (electroosmosis) (e.g., with the microchip in Figure 6.71 used for highspeed electrophoretic separations) + Scales as l2 − Highvoltage source is not convenient − Many parameters influence propulsion force − Not generic (only limited types of samples can be used) − Mixing difficult to implement − Sample contact with capillary walls modifies the electroosmotic force (EOF) + First products on the market / Solves liquid valving but not for vapors! + Better for highthroughput screening and smaller samples Centrifugal (e.g., with the twopoint calibration CD in Figure 6.91) + Scales a bit better than l3 + Compatible with a wide range of samples + Mixing easy to implement + Sample preparation easier than with an electrokinetic setup + Simple and inexpensive CD player for drive + No fluid contact + Established + Generic / Solves liquid valving elegantly but not vapor valving + Most functions demonstrated + Cell work easier + Better for diagnostics Acoustic (e.g., with White’s flexural plate wave device; see Volume III, Chapter 8) + Scales as l2 + No fluidic contact − Research and development phase + Generic − Does not solve valving yet − ZnO technology to implement the acoustic transducer still difficult to reproduce − Easy to further miniaturize
when used in microchambers in microfluidic platforms. In this chapter, we saw already that all flow in small tubes is laminar (making mixing a challenge), that evaporation from small droplets is very fast, and that surface tension in the microdomain becomes
very appreciable. These represent mostly negative aspects associated with scaling down any analytical equipment involving fluid handling. Positive attributes of miniaturizing such equipment are the savings on expensive reagents, short analysis times, and
Fluidics
fast heating/cooling (e.g., for PCR), which all dictate small devices. We now look into one class of analytical equipment involving fluid handling, namely, separation equipment, with some more detail. Electrophoresis, as described earlier in this chapter, is only one of many separation techniques used in analytical chemistry; other methods include gas chromatography (GC) and many varieties of liquid chromatography. Miniaturization in electrophoresis and chromatography has been a study topic for many years. The goal is not only to separate smaller amounts of chemical compounds, but theory also predicts that a reduction in dimensions of the separation column should result in an enhancement of analytical performance, such as a shorter separation time and more efficient heat dissipation.98,99 To put recent advances in miniaturization of separation devices in context, we need to reconsider the fundamentals of separation methodology. The following theoretical analysis will shed light on scaling laws applicable to analytical separation systems. We closely follow the derivations presented by Manz et al.98 One principal goal of separation techniques is to create the narrowest possible separation bands, w, to increase the separation efficiency. Several mechanisms contribute to band broadening, each with its own standard deviation σ, and we need to understand each of the contributing mechanisms to appreciate the effect of miniaturization on separation performance.
Commonly Used Terms in Separation Chemistry Analytical separation of compounds often is affected by forcing the sample compounds, suspended in a carrier medium or mobile phase, through a selectively absorbing medium or stationary phase immobilized in some sort of flow channel. The mobile phase in chromatography may be a liquid or a gas. The stationary phase (the one that stays in place inside the flow channel or column) is most commonly a viscous liquid coated on the inner side of a capillary tube or on the surface of solid particles packed in the column. Alternatively, the solid particles in the column may form the stationary phase themselves. To force the sample and carrier phase (i.e., the eluent), through the column, either
501
a pressure or electrical gradient, respectively, defining chromatography techniques and electrophoresis techniques, can be employed. The fluid emerging from the column is called the eluate, and the process of passing liquid or gas through a chromatography column is called elution. The partitioning of solutes between the mobile and stationary phases gives rise to separation of the various components in the sample. Columns are either packed or open tubular. A packed column is filled with particles as the stationary phase or the particles are coated with the stationary phase. An open columnar column is a narrow capillary in which the inside wall itself forms the stationary phase or a stationary phase is coated on that wall. The center of an open tubular column is hollow. Based on the mechanisms of interactions of the solute with the stationary phase, different types of chromatography are distinguished: adsorption, partition, ion exchange, molecular exclusion (also called gel filtration), and affinity chromatography.100 An electrochemical or optical detector, in the case of liquid chromatography, or a thermal conductivity detector (TCD) or flame ionization detector (FID), in the case of gas chromatography, may detect solutes eluted from a column. A chromatograph is a graph showing the response of such a detector as a function of elution time (Figure 6.95). Ideally, a solute applied as an infinitely narrow band at the inlet of a separation column emerges with a Gaussian shape at the outlet. In less ideal circumstances, the band becomes asymmetric. Different compounds are retained for different amounts of time, called retention times (tr), onto the immobilized medium through which they are forced. Retention time tr is the time needed after injection of the mixture for each component to reach the detector. The retention time for a solute often is corrected for the time it takes the unretained mobile phase (e.g., air) to travel through the column (tm). This socalled adjusted retention time t′r may be written as: t ra t r t m
(6.142)
For any two components 1 and 2, the relative retention, α, is given as: A
t ra 2 t ra1
(6.143)
502
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
t´r Detector response
tr
tm
Injection time
Air
Octane
Unknown
Nonane
Time
FIGURE 6.95 Schematic gas chromatogram showing measurement of retention times.
in which t′r2 > t′r1 so that α is always larger than 1. The larger the α, the better the separation between compounds 1 and 2. The relative retention is independent of flow rate and is used to identify compounds, even when the flow rate has changed between experiments. For each compound in the column, the capacity factor, k′, is defined as: ka
tr tm tm
(6.144)
A larger capacity factor signifies a compound better retained onto the column. The capacity factor in Equation 6.144 corresponds to the ratio of time the solute spends in the stationary phase over the time it spends in the mobile phase. The latter ratio in turn is based on the partition coefficient K, an equilibrium constant defined by the ratio of the concentration Cs of solute in the stationary phase over Cm, the concentration of the solute in the mobile phase: ka
V C s Vs K s Vm C m Vm
(6.145)
where Vs is the volume of the stationary phase and Vm the volume of the mobile phase. From Equations 6.143–6.145, we can conclude that: A
t ra2 k 2a K 2 t ra1 k1a K1
(6.146)
The relative retention of two solutes is proportional to the ratio of their partition coefficients. Two factors contribute to the efficiency of separation of components on a column. One is the difference in elution times between peaks; the other is the width of the peaks. Different compounds in an
applied sample on a column separate into bands, and the further apart they are, the better the separation performance of the setup. The resolution of two peaks is defined as: resolution
$t r $Vr w av w av
(6.147)
in which Δtr or Δwr is the separation between peaks in units of time (t) or volume (V), and wav is the average width of the two peaks in corresponding units. A band of solute in a column invariably spreads as it travels through a separation medium and emerges at the detector with a standard deviation σ; the narrower the bands (w), the better the resolution.
Band Broadening in the Column Individual solute bands in a column generally assume symmetric concentration profiles that can be described in terms of a Gaussian distribution curve and its standard deviation, σx. The Gaussian curve is given by: x2
C
m e 4 Dt 4PDt
(6.148)
where D = diffusion coefficient (m2/s) (104 faster in gases than in liquids) m = moles per unit crosssectional area C = concentration (mol m−3) t = time x = distance along the column (total length Lt) from the center of the band (at the band center, x = 0)
Fluidics
The standard deviation of this distribution curve, σx, is used to describe the bandwidth length and is given by: (6.149)
S x 2Dt
i.e., the width at time t of a band progressing in the column. If a solute moves a distance x at the linear flow rate ux (m s −1), the time it has been on the column is t = x u x–1 (when x = Lt, then t = t r). Or we can write that: x ¥ 2D ´ S 2Dt 2D x Hx u x ¦§ u x µ¶ 2 x
(6.150)
and: H
S 2x x
(6.151)
In this equation, plate height H (also called the height equivalent to a theoretical late) is the proportionality constant between the variance (σ2) of the band and the distance it has traveled (x). Thus, plate height is simply a quantity relating the width of a band to the distance traveled through the column. The number of theoretical plates, N, in the entire column is the total length Lt divided by the plate height: N
2 t 2 x
2 t 2
16L L t Lx L 2 H Sx S w
(6.152)
because x = L and σ = w/4. The above analysis can be made more generic; the bandwidth parameter, σ, for a flow channel can be expressed not only in terms of length in m (σx, see above) but also in terms of time in s (σt), and volume in m3 (σv). Rewriting Equation 6.152 with L and w (or σ) in units of time instead of length leads to: N
16t 2r ¥ t r2 ´ w 2 ¦§ S 2 µ¶
(6.153)
where tr is the retention time of the peak, and w is the width at the base of the peak in units of time. The smaller the H and thus the larger the N, the narrower the bands and the better the separation. Plate heights are ∼0.1 to 1 mm in gas chromatography (GC), ∼10 μm in highperformance liquid chromatography (HPLC), and 2000 0.21 4.2 0.94 0.47 2.1
220 0.56 70 3.3 0.8 16 1.5
700 0.56 22 0.33 0.08 5 49
220 1.4 70 52 1.2 16 0.075
700 1.4 22 5.2 12 5 2.4
0.41 3.3
1.3 3.3
4.1 3.3
5.1
5.1
5.1
5.1
Note: Obtained with capillary electroosmotic (EC), liquid (LC), and supercritical fluid chromatography (SFC). Assumed constants are diffusion coefficients 1.6 × 10−9 m2/s (LC, EC) and 10−8 m2/s (SFC); viscosities of the mobile phase 10−3 Ns/m2 (LC, EC) and 5 × 10−5 Ns/m2 (SFC); electrical conductivity of the mobile phase 0.3 S/m (EC); electrical permittivity × zeta potential, 5.6 × 10−11 N/V (EC); and heating power 1.1 W/m (EC). Source: After Manz, A., E. Verpoorte, C. S. Effenhauser, N. Burggraf, D. E. Raymond, D. J. Harrison, and H. M. Widmer. 1993. Miniaturization of separation techniques using planar chip technology. HRC J High Resol Chromatogr 16:433–36; and Manz, A., N. Graber, and H. M. Widmer. 1990. Miniaturized total chemical analysis systems: a novel concept for chemical sensing. Sensors Actuators B B1:244–48.
506
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
number (pressure drop), systems are easier to compare because all reduced parameters remain constant regardless of the size of the system.107 First, we define some of these reduced parameters in terms of those variables that can be assumed constant over the entire range of interest, including inner capillary diameter (d), mobile phase viscosity (ηm), average diffusion coefficient (Dm) of the sample in the mobile phase, and a Poiseuille number, C, of 32 for a circular crosssection. The diameter, d, is also the characteristic length here. With those constants, other quantities can be grouped into dimensionless forms—for example, volume, V; column length, L; linear flow rate, u; retention time, t; and pressure drop, Δ p. A reduced volume parameter, for example, is obtained by division through d3. Thus, one obtains: S V w 3 and s v 3v d d
(6.161)
Similarly, timerelated parameters such as the migration time, t0; the retention, t, for a compound with a capacity factor k′; and the time bandwidth, σt, can be reduced to their dimensionless terms, known as Fourier numbers, in the following fashion: T0
t 0 Dm d
2
,T
tDm d
2
k a 1 , and s
t
S t Dm d2
S 1 H , h , and s x x d d d
(6.163)
9
(6.164)
UEX Hm Dm
(6.165)
with ζ the zeta potential. Both Bodenstein numbers, describing the reduced pressure and voltage, can be rewritten as the socalled flow equations: (6.166)
9 LPe
in electroosmotic and electrophoretic flow, and: (6.167)
0 LPe
for pressuredriven chromatography. Also, the Fourier numbers can be further simplified as: L L and T k a 1 Pe Pe
(6.168)
The equations for reduced plate height, h, and the Péclet number, Pe, lead to the following simplified Golay equation for band broadening in pressuredriven flow, neglecting the third term (C) in Equation 6.155: h
2 1 6k a 11k a 2 Pe 2 Pe 96 1 k a
(6.169)
for a fielddriven flow we simply obtain: h
2 Pe
(6.170)
The reduced bandwidth is then given by: s 2x Lh
(6.158)
which represents the average linear flow rate divided by the absolute value of the average rate of diffusion
$pd 2 uL HmDm & Dm
The Bodenstein number thus represents the average linear flow rate divided by the absolute value of the average rate of longitudinal diffusion, Dm/L. In this expression, Φ is the Poiseuille number (32 for a circular crosssection). The applied voltage can be reduced to the “electrical” Bodenstein number, Ψ:
T0
where λ is the socalled reduced length. The linear flow rate of a nonretained component or the mobile phase is reduced to the Péclet number, Pe, given earlier as: ud Pe Dm
0
(6.162)
The first expression describes the ratio of the time required for a molecule to migrate in a fielddriven flow through the capillary from end to end to the time required to diffuse from wall to wall. The second term defines the analogous expression for chromatography. Terms with a length dimension are reduced by dividing by d: L
orthogonal to the direction of flow, Dm/d. The applied pressure can be reduced to the socalled Bodenstein number as:
(6.171)
and the plate number by: N
L Pe and N L h 2
(6.172)
Fluidics
507
TABLE 6.10 Reduced Parameter Set for the Example Separation Systems in Table 6.9 CE
Capillary LC
Capillary SFC
Number of theoretical plates, N Analysis time, t (k′ = 5) (min) Capillary inner diameter, dc (μm) Capillary length, L (cm) Reduced length, λ Péclet number (reduced flow rate), Pe Fourier number (reduced retention time), τ
Parameter
100,000 1 24 6.5 2700 100 28
100,000 1 2.8 8.1 29,000 14 2100
100,000 1 6.9 20 29,000 14 2100
Bodenstein number (reduced pressure decrease), ∏ Electric Bodenstein number (reduced voltage decrease), ψ
— 260,000
400,000 —
400,000 —
CE = capillary electrophoresis; LC = liquid chromatography; SFC = supercritical flow chromatography. Source: Manz, A., E. Verpoorte, C. S. Effenhauser, N. Burggraf, D. E. Raymond, D. J. Harrison, and H. M. Widmer. 1993. Miniaturization of separation techniques using planar chip technology. HRC J High Resol Chromatogr 16:433–36; and Manz, A., N. Graber, and H. M. Widmer. 1990. Miniaturized total chemical analysis systems: a novel concept for chemical sensing. Sensors Actuators B B1:244–48.
It can be recognized here how the number of theoretical plates is in a way representative of the Péclet number of the system. From Equations 6.172 and 6.163, the smaller Dm, the higher the number of plates, and the larger the velocity and the length of the column, the more the separation is “efficient.” With these reduced parameters, the examples of Table 6.9 now are compared again in Table 6.10. We conclude that the values for the reduced variables for LC and SFC are identical, regardless of differences in capillary diameter, lengths, diffusion coefficients, and viscosities. This can be used conveniently to deduce the influence of changing the capillary diameter on retention time, pressure, and signal bandwidth for a given number of theoretical plates and
a single set of reduced parameters, as illustrated in Table 6.11. The scaling for diffusioncontrolled separations, in which the time scale is proportional to d2, is summarized in Table 6.12. All reduced parameters remain constant regardless of the size of the system; that is, hydrodynamic diffusion, heat diffusion, and molecular diffusion effects behave in the miniaturized system as in the original large system. Reducing the characteristic length d (i.e., the tube diameter) by a factor of 10 makes for a 100times faster analysis. The pressure required is 100 times higher, and, more importantly, the voltage requirements remain unchanged in electrophoresis/electro osmosis systems. Miniaturization in diffusioncontrolled
TABLE 6.11 Calculated Parameter Set for an Open Tubular Column LC System Diameter d (μm)
Length, L (m) Time, t (min) Pressure, ∆p (atm) Peak, σx (μm) Peak, σt (ms) Peak, σv (pl)
1
2
5
10
20
Reduced Parameter
0.45 0.12 8700 450 7.4 0.35
0.9 0.5 2200 890 30 2.8
2.3 3 350 2200 190 44
4.5 12 87 4500 740 350
9 50 22 8900 3000 2800
λ = 450,000 t = 11,800 ∏ = 17,000,000 sx = 447 st = 12 sv = 354
Note: One million theoretical plates at zero retention (Péclet number Pe = 38). Assume diffusion coefficient is Dm = 10−3m2s. Source: Manz, A., E. Verpoorte, C. S. Effenhauser, N. Burggraf, D. E. Raymond, D. J. Harrison, and H. M. Widmer. 1993. Miniaturization of separation techniques using planar chip technology. HRC J High Resol Chromatogr 16:433–36; and Manz, A., N. Graber, and H. M. Widmer. 1990. Miniaturized total chemical analysis systems: a novel concept for chemical sensing. Sensors Actuators B B1:244–48.
508
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 6.12 Proportionality Factors for Some Mechanical Parameters in Relation to the Characteristic Length, d, in a DiffusionControlled System DiffusionControlled System Space, d Time, t Linear flow rate, u Volume flow rate, F Pressure drop (laminar flow) ∆p Voltage (electroosmotic flow), U Electric field, U/L Reynolds number, Re Péclet number, reduced flow rate, Pe Fourier number, reduced elution time, τ Bodenstein number, reduced pressure, ∏ Reduced voltage, ψ
d d2 L/d d L/d2 Constant L/d Constant Constant Constant Constant Constant
Source: After Manz, A., E. Verpoorte, C. S. Effenhauser, N. Burggraf, D. E. Raymond, D. J. Harrison, and H. M. Widmer. 1993. Miniaturization of separation techniques using planar chip technology. HRC J High Resol Chromatogr 16:433–36; and Manz, A., N. Graber, and H. M. Widmer. 1990. Miniaturized total chemical analysis systems: a novel concept for chemical sensing. Sensors Actuators B B1:244–48.
systems leads to a higher rate of separation while maintaining separation efficiency. Separation efficiency in capillary electrophoresis, in terms of theoretical plates per second, can be estimated from Equations 6.170 and 6.172: N
9 tU 2
(6.173)
where Ψ is the reduced voltage so that N is proportional to U, the applied voltage; the higher the applied voltage, the higher the number of theoretical plates. The voltage cannot be increased too much though, because heat evolution quickly becomes the limiting factor. In standard capillary electrophoresis, the maximum allowable heat generation is about 1 W/m. Because of the higher surfacetovolume ratio in micromachined channels, heat dissipation is faster, which permits higher electric fields than in standard capillary electrophoresis. For now, we will admit 1 W/m as an upper limit even for micromachined capillaries. Keeping the power per unit length constant means: P UI const L L
(6.174)
where I is the current through the capillary. The resulting upper limit for the voltage is then determined by the geometry of the capillary in terms of the reduced characteristic length (λ = 1/d):
Umax t L
(6.175)
The plate number N can thus reach values up to Nmax, where: Nmax t L
(6.176)
The minimum migration time is given by: t0 t
L2 U
(6.177)
and: t min t L2d
(6.178)
The maximum number of plates obtainable per second is then given by: Nmax 1 t 2 2 t min L d
(6.179)
clearly demonstrating the benefits of reducing the inner diameter of the capillary for rapid separation in capillary electrophoresis. The reduced height, h, of a chromatographic system according to Equation 6.169 shows a minimum, hmin, at an optimum reduced flow rate, Peopt (Péclet number). To reduce losses in pressure drop and to minimize analysis time, one must operate close to this optimum. Analogous to Equation 6.172, we can write the maximum number of theoretical plates as:
Fluidics
Nmax
L hmin
(6.180)
where hmin is constant for optimum Péclet number, Peopt, at a fixed capacity factor k′. This makes Equation 6.180 for pressuredriven chromatography equivalent to Equation 6.176 for electrophoresis. Equations 6.178 and 6.179 are also equally valid for capillary electrophoresis and capillary chromatography. The reduced parameter analysis shows that a downscale of 1/10 of the original size (diameter of a tube) reduces the related time variables (analysis time, required response time of a detector) to 1/100. The pressure requirements increase by a factor of 100, but the voltage requirements (for electrophoresis/electroosmosis) remain constant. The main advantage of capillary electrophoresis is thus higher speed of separation with a comparable efficiency.108
Example 6.11: Droplet Microfluidics In a new branch of microfluidics, a rich variety of droplets are made by emulsification in microfluidic systems. Dropletbased microfluidics allows for independent control of each droplet, thus generating microreactors that can be individually transported, mixed, and analyzed.109 The generation of droplets involves the disruption of interfacial forces between two streams of immiscible fluids either via flowinduced shear forces or other surface forces (e.g., electrowetting, dielectrophoresis). An oftenused breakup method of streams of immiscible fluids is in the confined geometry of a microfluidic Tjunction (see Figure 6.56). For a detailed theoretical treatment of droplet formation in a Tjunction, we refer to the work by De Menech et al.110 The droplets thus formed can be filled with reagents to perform bioassays in discretized femtoliter to nanoliter volumes separated by immiscible fluids as opposed to more conventional microfluidics, where reactions are not confined either spatially or temporally within the microchannels. Rapid mixing is possible because there is relative fluid motion between the immiscible fluids at the droplet interfaces that create recirculation of flows inside the droplets. The sizes of the droplets are extremely monodisperse (within 2%) and
509
can be controlled over a wide range (typically 1–100 μm in diameter).111–115 Because of high surface area to volume ratios at the microscale, heat and mass transfer times and diffusion distances are shorter, facilitating faster reaction times. Because multiple identical microreactor units can be formed in a short time, parallel processing and experimentation can easily be achieved, allowing large data sets to be taken efficiently and enabling high throughput screening and syntheses. Droplet microfluidics also offers greater potential for increased throughput and scalability than continuous singlephase flow microfluidics. In the past 5 years, several groups have used digital microfluidics to form irregular particles,116 double emulsions,117 hollow microcapsules,118 and microbubbles.74,119–123 As a curious return to fluidic logic (see the fluidic logic chips from 1965 in Volume III, Figure 1.2), MIT’s Neil Gershenfeld et al.124 are building rudimentary bubblebased logic devices. They constructed an entire family of chips modeled on the architecture of existing digital circuits that mimic the functions of electronic components: logic gates (AND/OR/NOT), memory, and even a microfluidic ring oscillator constructed from three AND gates (see Figure 6.96). These digital microfluidic devices show the nonlinearity, gain, bistability, synchronization, cascadability, feedback, and programmability required for scalable universal computation. Instead of using high and low voltages to represent a bit of information, the presence or absence of a bubble is used. This means that a bubble can not only carry some kind of payload—say a therapeutic drug or chemical reagents (see above)—but
FIGURE 6.96 A bubble microfluidic ring oscillator constructed from three AND gates.
510
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
it also can carry information at the same time. The bubble chips are 100 times slower than an average microprocessor, but among other uses they could enhance the memory capabilities of microfluidic chips: thousands of reagents could be stored on a single chip—much like conventional data storage technology—using counters to dispense exact amounts and builtin logic circuits to deliver the reagents to targeted spots. They could also be used to sort biological cells in assays and to make programmable print heads for inkjet printers, for example. With increasing complexity in largescale microfluidic processors, bubble logic provides an onchip process control mechanism integrating chemistry and computation.
scale? How can one enhance good mixing of two chemicals in a microreactor? 6.4: A lawn sprinkler consists of two arms equipped with nozzles at right angles which rotate about a pivot in a horizontal plane. Assuming the flow rate through each nozzle equals Q and the nozzle’s exit area is A, find the velocity of the water leaving the nozzle, in two cases: (a) There is no friction at the pivot. (b) There is a constant frictional torque Tf at the pivot.
Q
Acknowledgments Special thanks to Dr. Suman Chakraborty (Indian Institute of Technology Kharagpur), Dr. Nahui Kim (University of California, Irvine), and Marleen Madou.
Questions Questions by Omid Rohani, UC Irvine
6.1: We partially fill an open vessel with a liquid and rotate it at a constant angular velocity ω about a vertical axis. After some time the liquid also rotates at the same angular velocity as the vessel and the surface of the liquid develops into a steady shape. What is the equation that describes the free surface of the liquid? 6.2: Consider the flow of blood through a micro or nano channel. List 4 assumptions that introduce potential errors when modelling blood flows through such a micro channel using the NavierStokes equations. 6.3: What conclusions can one draw regarding liquid flows in micro and nano channels based on the currently available data in the literature? What do you know about turbulence in the macro scale and in the micro and nano
r r Q
6.5: Derive an equation for the flow rate Q as a dp , H for fully developed function of U, b, dx Couette shear flow, where U is the velocity of a moving plate and b is the height of the channel between this moving plate and a fixed bottom plate. We will assume that the flow is in the xdirection and b is in the ydirection. dp The viscosity is represented by η and is the dx pressure gradient in the xdirection. 6.6: What are the advantages of microfluidics? Give an example application. 6.7: Compare the breakdown of continuum theory for gasses and liquids. 6.8: What techniques can be implemented for mixing two reagents in the microscale (in low Reynolds number liquids)? 6.9: Given is a mixture of two proteins of similar molecular mass. Protein A comes with a MW = 12,400 and a pI = 10.7 and protein B has a MW = 12,800 and a pI = 7.5 (pI is the isoelectric point). You are told that capillary zone electrophoresis, CZE, is the best way to separate these two proteins.
Fluidics
6.10:
6.11:
6.12:
6.13:
6.14:
6.15:
6.16:
6.17:
(a) Do you agree with the suggestion of using CZE or would you employ another method? Briefly support your decision and your choice of separation method. (b) Explain the principle behind capillary electrophoresis and draw a schematic illustrating its operation. (c) What will be the elution order if you perform the separation using a buffer with a pH of 5.0? Why? When do the macroscopic laws of gas flow begin to fail and when does the noslip condition cease to apply? Explain some of the changes in the behavior of a liquid when the channel diameter decreases to below ten molecular diameters (the channel diameter of the order of a few nanometers). What is electrophoresis? Explain why DNA strands of varying size cannot be separated by electrophoresis in a free solution. Describe how electroosmotic phenomena can cause a pumping effect in a fused silica micro capillary. Using the HagenPoiseuille law for flow rate, explain why conventional pumping is not useful for the delivery of small samples? What pumping method do you suggest for delivery of small samples? How does this method change the flow profile? In a centrifugal fluidic platform (CDfluidics), what constitutes the pumping force, and how are valves for liquids implemented? A simple and accurate viscometer can be made from a length of capillary tubing. If the flow rate and pressure drop are measured, and the tube geometry is known, the viscosity can be computed. A test of a certain liquid in a capillary viscometer gave the following data: flow rate: 880 mm3/s; tube diameter: 500 μm; tube length: 1 m; pressure drop: 1.0 MPa. Determine the viscosity of the liquid. The accepted transition Reynolds number for flow in a circular pipe is Re ≈ 2300. For flow through a 6 cm diameter pipe, at what velocity will this occur at 20°C for (a) airflow and (b) water flow?
511
6.18: List five electrokinetic effects taken advantage of in the MEMS field and list one application for each approach. 6.19: Why are more theoretical plates achievable in capillary electrophoresis than in the following separation techniques? (a) Slab electrophoresis (b) Liquid chromatography 6.20: Compare/contrast how separation is achieved in chromatography and electrophoresis. 6.21: List 6 different methods to propel fluids through micro channels. 6.22: Why is there a lower limit to the size of an uncharged particle one can move with dielectrophoresis (~14 nm) and not on the size of a charged particle one can move in electrophoresis? What types of particles (size and charge) can one move with electroosmosis? 6.23: If a 100 bp long DNA is to be sequenced in a microfabricated channel, calculate the length of a channel needed to get single base pair separation. What voltage (E field) would you pick to perform the separation in a polyacrylamide gel. Make the necessary assumptions! The width and height of the channel is 20 μm × 20 μm. Thanks to Dr. Rashid Bashir, Purdue University. 6.24: Demonstrate that δ/δT ~ Pr1/2.
Further Reading Abraham, S., E. H. Jeong, T. Arakawa, S. Shoji, K. C. Kim, I. Kim, and J. S. Go. 2006. Microfluidics assisted synthesis of welldefined spherical polymeric microcapsules and their utilization as potential encapsulants. Lab Chip 6:752–56. Anna, S. L., N. Bontoux, and H. A. Stone, 2003. Formation of dispersions using “flow focusing” in microchannels. Appl Phys Lett 82:364–66. Belder, D. 2005. Microfluidics with droplets. Angewandte Chemie 44:3521–22. Cubaud, T., M. Tatineni, X. Zhong, and C. M. Ho. 2005. Bubble dispenser in microfluidic devices. Phys Rev E 72:4. Cubaud, T., and C. M. Ho. 2004. Transport of bubbles in square microchannels. Phys Fluids 16:4575–85. Fair, R.B., 2007. Digital microfluidics: is a true labonachip possible? Microfluidics Nanofluidics 3:245–81. Forsberg, F., J. B. Liu, D. A. Merton, N. M. Rawool, and B. B. Goldberg. 1995. Parenchymal enhancement and tumor visualization using a new sonographic contrast agent. J Ultrasound Med 14:949–57.
512
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
Garstecki, P., I. Gitlin, W. DiNuzio, and G. M. Whitesides. 2004. Formation of monodisperse bubbles in a microfluidic flowfocusing device. Appl Phys Lett 85:2649–51. Gerdts, C. J., V. Tereshko, M. K. Yadav, I. Dementieva, F. Collart, A. Joachimiak, R. C. Stevens, P. Kuhn, A. Kossiakoff, and R. F. Ismagilov. Timecontrolled microfluidic seeding in nLvolume droplets to separate nucleation and growth stages of protein crystallization. Angewandte Chemie 45:8156–60. Goldberg, B. B., J. S. Raichlen, and F. Forsberg. 2001. Ultrasound contrast agents. London: Dunitz Ltd. Gordillo, J. M., Z. Cheng, A. M. GananCalvo, M. Márquez, and D. A. Weitz. 2004. A new device for the generation of microbubbles. Phys Fluids 16:2828–34. Gunther A., and K. F. Jensen. 2007. Multiphase microfluidics: from flow characteristics to chemical and materials synthesis. Lab Chip 7:935. Hettiarachchi, K., E. Talu, M. L. Longo, P. A. Dayton, and A. P. Lee. 2007. Onchip generation of microbubbles as a practical technology for manufacturing contrast agents for ultrasonic imaging. Lab Chip 7:463–68. Jensen, K., and A. P. Lee. 2004. The science and applications of droplets in microfluidic devices. Lab Chip 4:31N–32N. Kobayashi, I., K. Uemura, and M. Nakajima. 2007. Formulation of monodisperse emulsions using submicronchannel arrays. Colloids Surfaces A Physicochem Eng Aspects 296:285–89. Liu, K., H. J. Ding, J. Liu, Y. Chen, and X. Z. Zhao. 2006. Shapecontrolled production of biodegradable calcium alginate gel microparticles using a novel microfluidic device. Langmuir 22:9453–57. Nisisako, T., S. Okushima, and T. Torii. 2005. Controlled formulation of monodisperse double emulsions in a multiplephase microfluidic system. Soft Matter 1:23–27. Nisisako, T., and T. Torii. 2007. Formation of biphasic Janus droplets in a microfabricated channel for the synthesis of shapecontrolled polymer microparticles. Adv Mater 19:1489–93. Sakai, S., I. Hashimoto, and K. Kawakami. 2007. Agarosegelatin conjugate for adherent cellenclosing capsules. Biotech Lett 29:731–35. Sakai, S., I. Hashimoto, and K. Kawakami. 2006. Usefulness of flow focusing technology for producing subsievesize cell enclosing capsules: application for agarose capsules production. Biochem Eng J 30:218–21. Song, H., D. L. Chen, and R. F. Ismagilov. 2006. Reactions in droplets in microfluidic channels. Angewandte Chemie 45:7336–56. Tan, Y. C., V. Cristini, and A. P. Lee. 2006. Monodispersed microfluidic droplet generation by shear focusing microfluidic device. Sensors Actuators B Chem 114:350–56. Teh, S.Y., R. Lin, L. Hung, and A. Lee. 2008. Droplet microfluidics. Lab Chip 8:198–220. Utada, A. S., E. Lorenceau, D. R. Link, P. D. Kaplan, H. A. Stone, and D. A. Weitz. 2005. Monodisperse double emulsions generated from a microcapillary device. Science 308:537–41. Wei, K., and S. Kaul. 1997. Recent advances in myocardial contrast echocardiography. Curr Opin Cardiol 12:539–46. Woodward, A., T. Cosgrove, J. Espidel, P. Jenkins, and N. Shaw. 2007. Monodisperse emulsions from a microfluidic device, characterised by diffusion NMR. Soft Matter 3:627–33. Xu, J. H., S. W. Li, Y. J. Wang, and G. S. Luo. 2006. Controllable gasliquid phase flow patterns and monodisperse microbubbles in a microfluidic Tjunction device. Appl Phys Lett 88:3.
Yobas, L., S. Martens, W. L. Ong, and N. Ranganathan. 2006. Highperformance flowfocusing geometry for spontaneous generation of monodispersed droplets. Lab Chip 6:1073–79. Zheng, B., C. J. Gerdts, and R. F. Ismagilov. 2005. Using nanoliter plugs in microfluidics to facilitate and understand protein crystallization. Curr Opin Struct Biol 15:548–55. Zheng, B., L. S. Roach, and R. F. Ismagilov. 2003. Screening of protein crystallization conditions on a microfluidic chip using nanolitersize droplets. J Am Chem Soc 125: 11170–71. Zhou, C. F., P. T. Yue, and J. J. Feng. 2006. Formation of simple and compound drops in microfluidic devices. Phys Fluids 18:14.
References 1. Denn, M. M. 1980. Process fluid mechanics. Englewood Cliffs, NJ: Prentice Hall. 2. Potter, M. C., and J. F. Foss. 1982. Fluid mechanics. Okemos, MI: Great Lakes Press. 3. Barron, A. E., and Blanch, H. 1995. DNA separations by slab gel and capillary electrophoresis: Theory and practice. Separation and Purification Methods 24:1–118. 4. White, F. M. 1994. Fluid mechanics. New York: McGrawHill. 5. Allen, T. J., and R. L. Ditsworth. 1972. Fluid mechanics. New York: McGrawHill. 6. Granger, R. A. 1995. Fluid mechanics. New York: Dover Publications. 7. Ozisik, M. N. 1977. Basic heat transfer. New York: McGrawHill. 8. Corcoran, P., H. V. Shurmer, and J. W. Gardner. 1993. Integrated tin oxide sensors of low power consumption for use in gas and odour sensing. Sensors Actuators B B15–16:32–37. 9. Coulson, J. M., and J. F. Richardson. 1999. Chemical engineering. New York: Pergamon. 10. Stokes, G. G. S. 1851. On the effect of the internal friction of fluids on the motion of pendulums. Trans Cambridge Phil Soc 9:8–106. 11. Poiseuille, J. L. M. 1840. Experimental investigations upon the flow of liquids in tubes of very small diameter. Rheological Memoirs 1. 12. Pfahler, J., J. Harley, and H. Bau. 1991. ASME 1991: micromechanical sensors, actuators, and systems. Atlanta: ASME, 49–60. 13. Gravesen, P., J. Branebjerg, and O. S. Jensen. 1993. Microfluidics: a review. J Micromech Microeng 3:168–82. 14. Liu, J., and Y.C. Tai. 1995. Proceedings: IEEE micro electro mechanical systems (MEMS ’95). Amsterdam: IEEE, 209–15. 15. Arkilic, E. B., K. S. Breuer, and M. A. Schmit. 1994. Applications of microfabrication to fluid mechanics. Chicago: ASME, 57–66. 16. Wong, C. C., D. R. Adkins, G. C. FryeMason, M. L. Hudson, R. Kottenstette, C. M. Matzke, J. N. Shadid, and A. G. Salinger. 1999. Proceedings: microfluidic devices and systems II. Santa Clara, CA: SPIE, 120–29. 17. Flik, M. I., B. I. Choi, and K. E. Goodson. 1991. ASME 1991: micromechanical sensors, actuators, and systems. Atlanta: ASME, 31–46.
Fluidics 18. Harley, J., H. Bau, J. N. Zemel, and V. Dominko. 1989. Proceedings: IEEE micro electro mechanical systems (MEMS ’89). Salt Lake City, UT: IEEE, 25–28. 19. Israelachvili, J. N. 1986. Measurement of the viscosity of liquids in very thin films. Colloid Interface Sci 110:263–71. 20. Tretheway, D. C., and C. D. Meinhart. 2002. Apparent fluid slip at hydrophobic microchannel walls. Phys Fluids 14:L9. 21. Pit, R., H. Hervet, and L. Léger. 2000. Direct experimental evidence of slip in hexadecane: solid interfaces. Phys Rev Lett 85:980–83. 22. Zhu, Y., and S. Granick. 2001. Ratedependent slip of Newtonian liquid at smooth surfaces. Phys Rev Lett 87:096105. 23. Craig, V. S., J. Neto, and C. Williams. 2001. Sheardependent boundary slip in an aqueous Newtonian liquid. Phys Rev Lett 87:054504. 24. Israelachvili, J. N. 1992. Intermolecular and surface forces: with applications to colloidal and biological systems (colloid science). New York: Academic Press. 25. Gee, M. L., P. M. McGuiggan, J. N. Israelachvili, and A. M. Homola. 1990. Liquid to solidlike transitions of molecularly thin films under shear. J Chem Phys 93:1895–906. 26. Ho, C. M. 2001. 14th IEEE International Conference MEMS, Interlaken, Switzerland, 375. 27. Barthlott, W., and C. Neinhuis. 1997. The purity of sacred lotus or escape from contamination in biological surfaces. Planta 202:1–8. 28. Colgate, E., and H. Matsumoto. 1990. An investigation of electrowettingbased microactuation. J Vac Sci Technol A8:3625–33. 29. Kenis, P. J. A., R. F. Ismagilov, and G. M. Whitesides. 1999. Microfabrication inside capillaries using multiphase laminar flow patterning. Science 285:83–85. 30. Aref, H. 1984. Stirring by chaotic advection. J Fluid Mech 143:1–21. 31. Whitesides, G. M. 2003. The “right” size in nanobiotechnology. Nat Biotech 21:1161–65. 32. Ismagilov, R. F., A. D. Stroock, P. J. A. Kenis, and G. Whitesides. 2000. Experimental and theoretical scaling laws for transverse diffusive broadening in twophase laminar flows in microchannels. Appl Phys Lett 76:2376–78. 33. Brody, J. P., P. Yager, R. E. Goldstein, and R. H. Austin. 1996. Biotechnology at low Reynolds numbers. Biophys J 71:3430–41. 34. Stroock, A. D., S. K. W. Dertinger, A. Ajdari, I. Mezi, H. A. Stone, and G. M. Whitesides. 2002. Chaotic mixer for microchannels. Science 295:647–651. 35. Knight, J. B., A. Vishwanath, J. P. Brody, and R. H. Austin. 1998. Hydrodynamic focusing on a silicon chip: mixing nanoliters in microseconds. Phys Rev Lett 80:3863–66. 36. Purcell, E. M. 1977. Life at low Reynolds number. Am J Phys 45:3–11. 37. Nguyen, N. T., and W. Zhigang. 2005. Micromixers—a review. J Micromech Microeng 15:R1–R16. 38. Virtanen, R. 1974. Zone electrophoresis in a narrowbore tube employing potentiometric detection. Acta Polytech Scand 123:1–67. 39. Jorgenson, J. W., and K. D. Lukacs. 1981. High resolution separations based on electrophoresis and electroosmosis. J Chromatogr 218:209–14. 40. Barron, A. E., and H. Blanch. 1995. DNA separations by slab gel and capillary electrophoresis: theory and practice. Separation Purification Methods 24:1–118.
513
41. Cobb, K. A., V. Dolnik, and M. Novotny. 1990. Electrophoretic separations of proteins in capillaries with hydrolytically stable surface structures. Anal Chem 62:2478–83. 42. Jorgenson, J. W., and E. J. Guthrie. 1983. Liquid chromatography in opentubular columns. J. Chromatog 255: 335–48. 43. Harrison, D. J., Z. Fan, K. Fluri, and K. Seiler. 1994. Technical digest: 1994 solidstate sensor and actuator workshop. Hilton Head Island, SC. 44. Jacobson, S. C., R. Hergenröder, A. W. Moore, and J. M. Ramsey. 1994. Technical digest: 1994 solidstate sensor and actuator workshop. Hilton Head Island, SC. 45. Jacobson, S. C., J. Kutter, C. Culbertson, and J. Ramsey. 1998. Micro total analysis systems ‘98. Banff, Canada, 315. 46. Jacobson, S. C., and J. M. Ramsey. 1998. Microchip structures for submillisecond electrophoresis. Microchip structures for submillisecond electrophoresis. Anal Chem 70: 3476–80. 47. Jacobson, S. C., C. T. Culbertson, and J. M. Ramsey. 1998. cstate sensor and actuator workshop. Hilton Head Island, SC. 48. Pace, S. 1990. E. I. Du Pont De Nemours & Co. US Patent 4,908,112. 49. Soane, D. S., and Z. Soane. 1998. Soane Biosciences . US Patent 5,750,015. 50. Manz, A., J. C. Fettinger, E. Verpoorte, H. Ludi, H. M. Widmer, and D. J. Harrison. 1991. Micromachining of monocrystalline silicon and glass for chemical analysis systems: a look into next century’s technology or just a fashionable crazy? Trends Anal Chem 10:144. 51. Manz, A., D. J. Harrison, E. M. J. Verpoort, J. C. Fettinger, A. Paulus, H. Ludi, and H. M. Widmer. 1992. Planar chips technology for miniaturization and integration of separation techniques into monitoring systems: capillary electrophoresis on a chip. J Chromatogr 593:253–58. 52. Ramsey, J. M. 1999. Lockheed Martin Energy Systems. US Patent 6,001,229. 53. Ramsey, J. M. 2000. Lockheed Martin Energy Research Corporation. US Patent 6,010,607. 54. Effenhauser, C. S., A. Manz, and H. M. Widmer. 1995. Manipulation of sample fractions on a capillary electrophoresis chip. Anal Chem 67:2284–87. 55. Burggraf, N., A. Manz, E. Verpoorte, C. S. Effenhauser, H. M. Widmer, and N. F. de Rooij. 1994. A novel approach to ion separation in solution: synchronization cyclic capillary electrophoresis (SCCE). Sensors Actuators B 20:103. 56. Bousse, L., A. R. KopfSill, and J. W. Parce. 1998. Systems and technologies for clinical diagnostics and drug discovery. Ed. G. E. Cohn. San Jose, CA: SPIE. 57. Haab, B. B., and R. A. Mathies. 1998. Systems and technologies for clinical diagnostics and drug discovery. Ed. G. E. Cohn. San Jose, CA: SPIE. 58. Wahl, M., R. Erdmann, K. Lauritsen, and H.J. Rahn. 1998. Systems and technologies for clinical diagnostics and drug discovery. Ed. G. E. Cohn. San Jose, CA: SPIE. 59. Righetti, P. G. 1990. Immobilized pH gradients: theory and modelling. Amsterdam: Elsevier. 60. Herr A. E., J. I. Molho, J. G. Santiago, T. W. Kenny, D. A. Borkholder, G. J. Kintz, P. Belgrader, and M. A. Northrup. 2000. Technical digest: 2000 solidstate sensor and actuator workshop. Hilton Head Island. 61. Heller, M. J., A. H. Forster, and E. Tu. 2000. Active microelectronic chip devices which utilize controlled electrophoretic fields for multiplex DNA hybridization and other genomic applications. Electrophoresis 21: 157–64.
514
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
62. Martin, Y., and H. K. Wickramasinghe. 1987. Magnetic imaging by “force microscopy” with 1000 Å resolution. Appl Phys Lett 50:1455–57. 63. Pohl, H. A. 1951. The motion and precipitation of suspensoids in divergent electric fields. J Appl Phys 22:869–71. 64. Pohl, H. A. 1978. Dielectrophoresis. Cambridge, UK: Cambridge University Press. 65. Pethig, R., J. P. H. Burt, A. Parton, N. Rizvi, M. S. Talary, and J. A. Tame. 1998. Development of biofactoryonachip technology using excimer laser micromachining. J Micromech Microeng 8:57–63. 66. Pethig, R., and G. H. Markx. 1997. Applications of dielectrophoresis in biotechnology. TIBTECH 15:426–32. 67. Huang, Y., X. B. Wang, F. F. Becker, and P. R. C. Gascoyne. 1997. Introducing dielectrophoresis as a new force field for fieldflowfractionation. Biophys J 73:1118–29. 68. Wang, X.B., J. Vykoukal, F. F. Becker, and P. R. C. Gascoyne. 1998. Separation of polystyrene microbeads using dielectrophoretic/gravitational fieldflowfractionation. Biophys J 74:2689–701. 69. Suehiro, J., and R. Pethig. 1998. The dielectrophoretic movement and positioning of a biological cell using a threedimensional grid electrode system. J Phys D Appl Phys 31:3298–305. 70. Park, B. Y., and M. J. Madou. 2005. 3D electrode designs for flowthrough dielectrophoretic systems. Electrophoresis 26:3745–57. 71. MartinezDuarte, R., H. A. Rouabah, N. G. Green, M. Madou, and H. Morgan. 2007. Proceedings of the Eleventh International Conference in Miniaturized Systems for Chemistry and Life Sciences: microTAS 2007. Paris. 72. Wang, L., L. Flanagan, and A. P. Lee. 2007. Sidewall vertical electrodes for lateral field microfluidic applications. J Microelectromech Systems 16:454–61. 73. Voldman, J., M. L. Gray, M. Toner, and M. A. Schmidt. 2002. A microfabricationbased dynamic array cytometer. Anal Chem 74:3984–90. 74. Iliescu, C., L. Yu, G. Xu, and F. E. H. Tay. 2006. A dielectrophoretic chip with a 3D electric field gradient. J Microelectromech Systems 15:1506–13. 75. LapizcoEncinas, B. H., B. A. Simmons, E. B. Cummings, and Y. Fintschenko. 2004. Dielectrophoretic concentration and separation of live and dead bacteria in an array of insulators. Anal Chem 76:1571–79. 76. Fatoyinbo, H. O., D. Kamchis, R. Whattingham, S. L. Ogin, and M. P. Hughes. 2005. A highthroughput 3D composite dielectrophoretic separator. IEEE Trans Biomed Eng 52:1347–49. 77. Becker, F. F., X. B. Wang, Y. Huang, R. Pethig, J. Vykoukal, and P. R. C. Gascoyne. 1994. The removal of human leukaemia cells from blood using interdigitated microelectrodes. J Phys D Appl Phys 27:2659–62. 78. Burt, J. P. H., R. Pethig, and M. S. Talary. 1998. Microelectrode devices for manipulating and analysing bioparticles. Trans Inst MC 19:1–9. 79. Rousselet, J., G. H. Markx, and R. Pethig. 1998. Separation of erythrocytes and latex beads by dielectrophoretic levitation and hyperlayer fieldflow fractionation. Colloids Surfaces A 140:209–16. 80. Markx, G. H., and R. Pethig. 1995. Dielectrophoretic separation of cells: continuous separation. Biotech Bioeng 45:337–43. 81. Talary, M. S., J. P. H. Burt, J. A. Tame, and R. Pethig. 1996. Electromanipulation and separation of cells using travelling electric fields. J Phys D Appl Phys 29:2198–203.
82. Goater, A. D., J. P. H. Burt, and R. Pethig. 1997. A combined travelling wave dielectrophoresis and electrorotation device applied to the concentration and viability determination of cryptosporidium. J Phys D Appl Phys 30:L65–69. 83. Müller, T., S. Fiedler, T. Schnelle, K. Ludwig, H. Jung, and G. Fuhr. 1996. Biotech Tech 10:221–26. 84. Batchelder, J. S. 1983. Method and apparatus for dielectrophoretic manipulation of chemical species. US Patent 4,390,403. 85. Huang, Y., J. Yang, X.B. Wang, F. F. Becker, and P. R. C. Gascoyne. 1999. The removal of human breast cancer cells from hematopoietic CD34+ stem cells by dielectrophoretic fieldflowfractionation. J Hematother Stem Cell Res 8:481–90. 86. Yang, J., Y. Huang, X. Wang, X.B. Wang, F. F. Becker, and P. R. C. Gascoyne. 1999. Dielectric properties of human leukocyte subpopulations determined by electrorotation as a cell separation criterion. Biophys J 76:3307–14. 87. Prins, M. W. J., W. J. J. Welters, and J. W. Weekamp. 2001. Fluid control in multichannel structures by electrocapillary pressure. Science 291:277–80. 88. Asakuma, N., T. Fukui, M. Toki, K. Awazu, and H. Imai. 2003. Photoinduced hydroxylation at ZnO surface. Thin Solids Films 445:284–87. 89. Zhang, Z., H. Chen, J. Zhong, G. Saraf, and Y. Lu. 2007. Fast and reversible wettability transitions on ZnO nanostructures. J Electr Mater 36:895–99. 90. Feng, X., L. Feng, M. Jin, J. Zhai, L. Jiang, and D. Zhu. 2004. Reversible superhydrophobicity to superhydrophilicity transition of aligned ZnO nanorod films. J Am Chem Soc 126:62–63. 91. Sun, R. D., A. Nakajima, A. Fujishima, T. Watanabe, and K. Hashimoto. 2001. Photoinduced surface wettability conversion of ZnO and TiO2. Thin films. J Phys Chem B 105:1984–90. 92. Madou, M. J., and G. J. Kellogg. 1998. Systems and technologies for clinical diagnostics and drug discovery. Eds. G. E. Cohn and A. Katzir. San Jose, CA: SPIE. 93. McNeely, M. R., M. K. Spute, N. A. Tusneem, and A. R. Oliphant. 1999. Microfluidic devices and systems II. Eds. C. H. Ahn and A. B. Frazier. Santa Clara, CA: SPIE. 94. Madou, M. J., Y. Lu, S. Lai, Y.J. Juang, L. J. Lee, and S. Daunert. 2000. Technical digest: 2000 solid sensor and actuator workshop. Hilton Head Island, SC. 95. Kim, N., C. M. Dempsey, C. J. Kuan, J. V. Zoval, E. O’Rourke, G. Ruvkun, M. J. Madou, and J. Y. Sze. 2007. Gravity force transduced by the MEC4/MEC10 DEG/ENaC channel modulates DAF16/FoxO activity in Caenorhabditis elegans. Genetics 177:835–45. 96. Kim, N., C. M. Dempsey, J. V. Zoval, J. Y. Sze, and M. J. Madou. 2007. Automated microfluidic compact disc (CD) cultivation system of Caenorhabditis elegans. Sensors Actuators B Chemical 122:511–18. 97. Madou, M. J., J. Zoval, G. Jia, H. Kido, J. Kim, and N. Kim. 2006. Lab on a CD. Ann Rev Biomed Eng 8:601–28. 98. Manz, A., E. Verpoorte, C. S. Effenhauser, N. Burggraf, D. E. Raymond, D. J. Harrison, and H. M. Widmer. 1993. Miniaturization of separation techniques using planar chip technology. HRC J High Resol Chromatogr 16:433–36. 99. Manz, A., N. Graber, and H. M. Widmer. 1990. Miniaturized total chemical analysis systems: a novel concept for chemical sensing. Sensors Actuators B B1:244–48. 100. Nölting, B. 2005. Methods in modern biophysics. Berlin: Springer.
Fluidics 101. Harris, D. C. 1999. Quantitative chemical analysis. New York: W. H. Freeman. 102. Golay, M. J. E. 1958. Gas chromatography. New York: Academic Press. 103. Taylor, G. I. 1953. Dispersion of soluble matter in solvent flowing slowly through a tube. Proc Roy Soc A 219:186–203. 104. Wong, C. C., D. R. Adkins, G. C. FryeMason, M. L. Hudson, R. Kottenstette, C. M. Matzke, J. N. Shadid, and A. G. Salinger. 1999. Microfluidic devices and systems II. Santa Clara, CA: SPIE. 105. Molho, J. I., A. E. Herr, B. P. Mosier, J. G. Santiago, T. W. Kenny, R. A. Brennen, and G. Gordon. 2000. A low dispersion turn for miniaturized electrophoresis. Technical digest: 2000 solidstate sensor and actuator workshop, Hilton Head, SC. 106. Culbertson, C. T., S. C. Jacobson, and J. M. Ramsey. 2000. Technical digest: 2000 solidstate sensor and actuator workshop. Hilton Head, SC. 107. Manz, A., and W. Simon. 1987. Potentiometric detector for fast highperformance opentubular column liquid chromatography. Anal Chem 59:74–79. 108. Manz, A., J. C. Fettinger, E. Verpoorte, and H. Ludi. 1991. Micromachining of monocrystalline silicon and glass for chemical analysis systems: a look into the next century’s technology or just a fashionable craze. Trends Anal Chem 10:144–49. 109. Fair, R. B. 2007. Digital microfluidics: is a true labonachip possible? Microfluid Nanofluid 3:245–81. 110. De Menech, M., P. Garstecki, F. Jousse, and H. A. Stone. 2008. Transition from squeezing to dripping in a microfluidic Tshaped junction. J Fluid Mech 595:141–61. 111. Anna, S. L., N. Bontoux, and H. A. Stone. 2003. Formation of dispersions using “flow focusing” in microchannels. Appl Phys Lett 82:364–66. 112. Zhou, C. F., P. T. Yue, and J. J. Feng. 2006. Formation of simple and compound drops in microfluidic devices. Physi Fluids 18:14. 113. Tan, Y. C., V. Cristini, and A. P. Lee. 2006. Monodispersed microfluidic droplet generation by shear focusing microfluidic device. Sensors Actuators B Chem 114:350–56.
515
114. Woodward, A., T. Cosgrove, J. Espidel, P. Jenkins, and N. Shaw. 2007. Monodisperse emulsions from a microfluidic device, characterised by diffusion NMR. Soft Matter 3:627–33. 115. Yobas, L., S. Martens, W. L. Ong, and N. Ranganathan. 2006. Highperformance flowfocusing geometry for spontaneous generation of monodispersed droplets. Lab Chip 6:1073–79. 116. Nisisako, T., and T. Torii. 2007. Formation of biphasic Janus droplets in a microfabricated channel for the synthesis of shapecontrolled polymer microparticles. Adv Mater 19:1489–93. 117. Nisisako, T., S. Okushima, and T. Torii. 2005. Controlled formulation of monodisperse double emulsions in a multiplephase microfluidic system. Soft Matter 1:23–27. 118. Utada, A. S., E. Lorenceau, D. R. Link, P. D. Kaplan, H. A. Stone, and D. A. Weitz. 2005. Monodisperse double emulsions generated from a microcapillary device. Science 308:537–41. 119. Gordillo, J. M., Z. D. Cheng, A. M. GananCalvo, M. Marquez, and D. A. Weitz. 2004. A new device for the generation of microbubbles. Phys Fluids 16:2828–34. 120. Garstecki, P., I. Gitlin, W. DiLuzio, G. M. Whitesides, E. Kumacheva, and H. A. Stone. 2004. Formation of monodisperse bubbles in a microfluidic flowfocusing device. Appl Physi Lett 85:2649–51. 121. Cubaud, T., and C. M. Ho. 2004. Transport of bubbles in square microchannels. Phys Fluids 16:4575–85. 122. Cubaud, T., M. Tatineni, X. L. Zhong, and C. M. Ho. 2005. Bubble dispenser in microfluidic devices. Phys Rev E72:4. 123. Hettiarachchi, K., E. Talu, M. L. Longo, P. A. Dayton, and A. P. Lee. 2007. Onchip generation of microbubbles as a practical technology for manufacturing contrast agents for ultrasonic imaging. Lab Chip 7:463–68. 124. Prakash, M., and N. Gershenfeld. 2007. Microfluidic bubble logic. Science 315:832–35. 125. Hagen, G. H. L. 1839. III Über die Bewgung des Wassers in engen cylindrischen Röhren, Poggendorfs Annalen der Physik und Chemie 2(46):423–42.
7 Electrochemical and Optical Analytical Techniques
Outline
Electricity
Introduction Physics
Intermolecular Forces Electrochemistry
Chemistry
Electrochemistry
Material Science
Mathematics
Optical Spectroscopy Comparison of Optical versus Electrochemical Sensors
The History of Electrochemistry (calendar from http://www.basinc.com).
Questions References
(a)
(b)
(a) Shrimp vomiting a bioluminescent substance toward a predator. (b) Firefly exhibiting bioluminescence.
Introduction In all electrochemical and many optical sensors, molecules interact with a solid surface and generate an analytical signal that can be used to identify and sometimes quantify an unknown analyte. This chapter begins with a detailed study of the nature of the attractive and repulsive forces 517
518
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
at an interface between a liquid and a solid (mostly in the form of small particles and bulk electrodes). Forces at the liquid/solid interface are the same as those that control the interaction between liquid molecules but are modulated by the presence of the solid. Intermolecular nonbonding forces between molecules, ions, or molecules and ions are much weaker than intramolecular bonding forces, such as covalent bonds within a molecule. Nevertheless, intermolecular forces sum to an impressive total binding energy, often several hundreds of kilojoules per mole, when many are present within a macromolecule or in a solid. The intermolecular forces we will study include the classical (coulomb) electrostatic forces, van der Waals interactions, and the quantum mechanical Casimir force. These forces, when exerted between individual molecules, extend typically over a few nanometers only, but when molecules come together into condensed phases, the force range at the surface is extended to several tens of nanometers. Intermolecular forces explain the electrical double layer (EDL) at the interface of liquid/solid surfaces, surface tension, viscosity, vapor pressure, boiling points, and many other important phenomena, including DNA hybridization and selfassembly. Hydrophilic and hydrophobic interactions, also based on intermolecular forces, are treated in Chapter 6 on fluidics. Electrochemistry is the study of reactions taking place at the interface of a solid conductor and an electrolyte. Using sensor examples, we introduce some of the most important concepts in electrochemistry, i.e., the EDL, potentiometry, voltammetry, two and threeelectrode systems, Marcus theory of electron transfer, reaction rate and diffusion ratecontrolled electrochemical reactions, and ultramicroelectrodes (UMEs). We also learn how different materials, such as metals, semiconductors, solid electrolytes, and mixed conductors, exposed to a solution offer the possibility for building different types of electrochemical sensors. Besides insights in electrochemical sensor construction, this section prepares the reader for an appreciation of the role of electrochemistry in the manufacture of microelectromechanical systems (MEMS) and nanoelectromechanical systems (NEMS), i.e., in electrochemical machining as covered in
Volume II, Chapter 4 (electrochemical etching, a subtractive technique) and Volume II, Chapter 8 (electrochemical deposition, a forming technique). We conclude the electrochemistry section with more electrochemical sensor examples, including ionsensitive fieldeffect transistors (ISFETs), potentiometric and amperometric immunosensors, and glucose sensors. Many researchers use MEMS and NEMS to miniaturize optical components or whole instruments for absorption, luminescence, or phosphorescence measurements. The latter techniques, like the electrochemical methods reviewed, constitute a branch of analytical chemistry, a branch that is concerned with the production, measurement, and interpretation of electromagnetic data arising from either emission or absorption of radiant energy by matter. We compare the sensitivity of the various optical sensing techniques and analyze how amenable they are to miniaturization (scaling laws). We end this chapter by comparing the merits and problems associated with electrochemical and optical measuring techniques.
Intermolecular Forces Introduction For the nonchemist, a few simple chemistry concepts are recalled here. A covalent bond, holding a molecule together, is a bonding or intramolecular force, whereas the attraction between molecules is a nonbonding or intermolecular force. Ionic chemical bonding results from the maximization of the electrostatic forces between large numbers of cations and anions in ionic solids. Intermolecular forces between molecules, between ions in solution, or between molecules and ions are much weaker than intramolecular forces (e.g., leading to a binding energy of only 16 kJ/mol vs. 431 kJ/mol for HCl) (see Figure 7.1). Covalent bonds (300–400 kJ/mol) determine molecular architecture, whereas noncovalent bonds, typically 10–100 times weaker, determine molecular conformations. Being individually weak, noncovalent interactions nevertheless sum to an impressive total, often several hundreds of kilojoules per mole, when many are present within a given
Electrochemical and Optical Analytical Techniques Covalent bond (strong)
Intermolecular attraction (weak)
FIGURE 7.1 In a HCl molecule, there is a bonding or intramolecular bond that is covalent and strong and a nonbonding or intermolecular hydrogen bond that is weak.
macromolecule, between macromolecules in a solution, or between the building blocks making up a solid. The intermolecular energy term (used in the analytical calculations involving energy) usually includes the classical (coulomb) electrostatic and van der Waals interactions. The nonbonding forces we will analyze below are: ◾ Chargecharge interactions (Coulomb’s law in a dielectric medium) ◾ Permanent and induced dipole interactions (van der Waals interactions): t Chargedipole interactions t Dipoledipole interactions t Chargeinduced dipole interactions t Dipoleinduced dipole interactions t Dispersion (induced dipoleinduced dipole) interactions ◾ Hydrogen bonds: donor groupacceptor group interactions (a very important case of dipoledipole interactions) ◾ Casimir force: a quantum mechanical effect (a special type of van der Waals interaction, i.e., the retarded van der Waals force also known as the CasimirPolder force) Hydrophilic versus hydrophobic interactions, a very important group of van der Waals interactions, were treated in Chapter 6 on fluidics. In Table 7.1 we compare bonding and nonbonding forces. Properties controlled by intermolecular forces include vapor pressure, boiling point, molecular crystals, protein folding, colloidal stability, rheological behavior, selfassembly, surface tension, viscosity,
519
and so on. To understand how important intermolecular forces are, the two following quotes help: The very existence of condensed phases of matter is conclusive evidence of attractive forces between molecules, for in the absence of attractive forces, the molecules in a glass of water would have no reason to stay confined to the glass… Anthony J. Stone The Theory of Intermolecular Forces (1996) The most important forces dictating the properties of biomolecules are the nonbonded [intermolecular] interactions… Alexander D. MacKerell, Jr. Journal of Computational Chemistry (2004)
In other words, in the absence of ionic bonding and interatomic or intermolecular forces, all matter would exist in the gas form, even at 0 K. Thus, intermolecular forces play a crucial role in many of the properties of liquids, gases, and solids. When a substance melts or boils, the intermolecular forces are broken (not the covalent bonds), and when a substance condenses, intermolecular forces are formed. Intermolecular forces at a solid/liquid interface are the same forces that control the interaction between the constituent molecules of the solution modulated by the presence of foreign molecules at the solid/liquid interface. In this section, we establish the operational range of these forces and find that forces between individual molecules typically only extend over a few nanometers. However, when molecules come together into condensed phases, the force range at the surface is extended to several tens of nanometers. A couple of examples of intermolecular forces at work follow. When intermolecular forces are weak, little energy is required to overcome them. Consequently, boiling points are low for such compounds. The vapor pressure of a liquid depends on intermolecular forces such that, when the intermolecular forces in a liquid are strong, the vapor pressure is low. The boiling point is related to vapor pressure and is lowest for liquids with the weakest intermolecular forces. Surface tension increases with increasing intermolecular forces, and because surface tension
520
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 7.1 Comparison of Bonding (Intramolecular), Ionic, and Nonbonding (Intermolecular) Interactions Force
Model
Basis of Attraction
Energy (KJ/mol)
Example
Bonding Ionic
Cation–anion
400–4000
NaCI
Covalent
Nucleishared e– pair
150–1100
H—H
Metallic
Cations–delocalized electrons
75–1000
Fe
Iondipole
Ion charge–dipole charge
40–600
Hbond
Polar bond to H–dipole charge (high EN of N,O,F)
10–40
Diploebond
Dipole charges
5–25
Ioninduced dipole
Ion chargepolarizable e– cloud
3–15
Dipoleinduced dipole
Dipole chargepolarizable e– cloud
2–10
Dipersion (London)
Polarizable e– cloud
0.05–40
Nonbonding (intermolecular)
is the energy needed to reduce the surface area of a liquid, it is necessary to pull molecules apart against the intermolecular forces of attraction (cohesion) to increase surface area. Viscosity increases with increasing intermolecular forces because increasing these forces increases the resistance to flow. Other factors, such as the possibility of molecules tangling together, can also affect the viscosity. Liquids with long molecules that tangle together are expected to have higher viscosities. Intermolecular forces explain all the data of the liquids listed in Table 7.2, and we will learn in the pages that follow and elsewhere in the book that they explain many other important phenomena, from DNA hybridization to selfassembly. Many observed phenomena in nature have their basis in intermolecular forces! For example, in Volume III, Chapter 7 on scaling laws, we will
learn that the gecko’s ability to walk on ceilings is due to van der Waals attractive forces between the spatulae (1 billion of them) on the gecko’s feet and the wall. This example shows how shortrange forces can have longrange (macroscopic) effects. Intermolecular forces exert their influence especially in the micro and nanoworld. In the nanoworld, gravitational forces are negligible, and forces such as van der Waals and the quantum mechanical Casimir force take over. At distances less than a micrometer, the Casimir force (a special type of van der Waals force) becomes the dominant force between two neutral objects in a vacuum. In Volume III, Chapter 8 on actuators, we calculate that two plates with an area of 1 cm 2 separated by a distance of 1 μm have an attractive Casimir force of about 10 −7 N. At separations of 10 nm, the Casimir effect produces the equivalent of 1 atm. Obviously,
Electrochemical and Optical Analytical Techniques
521
TABLE 7.2 Properties of Some Liquids at 20°C Substance Water, H2O Carbon dioxide, CO2 Pentane, C5H12 Glycerol, C3H8O3 Chloroform, CHCl3 Carbon tetrachloride, CCl4 Bromoform, CHBr3
Molecular Weight (amu)
Vapor Pressure (mmHg)
Surface Tension (J/m2)
Viscosity (kg/m · s)
18 44 72 92 119 154 253
1.8 × 101 4.3 × 104 4.4 × 102 1.6 × 10−4 1.7 × 102 8.7 × 101 3.9 × 100
7.3 × 10−2 1.2 × 10−3 1.6 × 10−2 6.3 × 10−2 2.7 × 10−2 2.7 × 10−2 4.2 × 10−2
1.0 × 10−3 7.1 × 10−5 2.4 × 10−4 1.5 × 100 5.8 × 10−4 9.7 × 10−4 2.0 × 10−3
Intermolecular forces explain the data of the liquids in this table.
this is a force to reckon with in MEMS and NEMS devices.
Interparticle Interaction Energy (U) and Interaction Forces (F) The interaction energy between two particles (atoms or molecules) is defined as the pair potential (energy), U(r), which depends on the intermolecular separation, r. The force, F(r), between the two particles is obtained as the negative of the gradient of the pair potential: F(r )
dU(r ) dr
(7.1)
At very large separations (as r → ∞), the interparticle interaction is negligible (U → 0, F → 0). At shorter separations, the particles attract (F < 0, particles are pulled together). A dimer is more stable than the two isolated particles, hence U(r) < 0. At very short separations (r → 0), the particles repel each other (F > 0, particles are pushed apart). At r = re, U(r) is at its minimum (Umin), and the interparticle force, F = 0. This is summarized in Figure 7.2. The diagram in Figure 7.2 shows the total potential energy between two particles. A power law with r raised to the exponent –n generally models the intermolecular potential energy function:
For the case of attractive interactions, U(r) < 0, whereas for repulsive interactions, U(r) > 0. To understand the exact shape of the curve in Figure 7.2, we must introduce the exact equations for repulsive and attractive potentials first. The most important repulsive term corresponds to the limit of compressibility of matter. At short internuclear separations, there are both electrostatic repulsions between the atomic nuclei and between the electrons (both valence and core) on neighboring atoms. The latter is based on the Pauli exclusion principle. The Pauli exclusion principle is quantum mechanical in origin and only allows for two electrons with opposite spin per energy level. The importance of the Pauli principle was exemplified in Chapter 3, where we saw that without the Pauli principle all material would collapse! The total shortrange repulsive interaction is generally modeled by steep 1/r12 dependence on interatomic distance (Figure 7.2, left
U>0 (unstable)
U re
U(r ) Cr n
C rn
(7.2)
where C is a constant. The general expression for F(r) is then: F(r )
nC r n1
(7.3)
F>0 (repulsive force)
F σ, intermolecular forces become inefficiently weak and do not contribute to UTotal; however, with n < 3, the size of the system L becomes important. The latter is the case, for example, for gravity (distant planets and stars) and Coulomb interactions where n = 1, i.e., both are very longranged forces that fall off very slowly. For n ≥ 3, the intermolecular potential becomes important and is the reason why bulk properties of a material are sizeindependent (water boils at the same temperature in a cup as it does in a bucket) unless we go to submicrometer size distances, where properties of material change as intermolecular forces start taking over. The Paulibased repulsive interaction, for example, is very short ranged (n = 12).
Coulomb Interactions
r
FIGURE 7.3 Coulomb interaction between two point charges or monopoles.
Q1Q 2 ). In Equation 4PE 0 E 7.5, Q1 = z1e, where e is the magnitude of the electron charge (1.602 × 10−19 C) and z1 is an integer value. In the denominator, ε0 is the permittivity of free space (8.854 × 10−12 J−1 C2 m−1), and ε is the relative permittivity of the medium between the ions (ε = 1 in a vacuum or ε > 1 in a gas or liquid). In the case of repelling like charges U(r) is positive, and in the case of attracting opposite charges U(r) is negative. This Coulomb interaction potential is additive when charges are grouped in crystals. With ions in solution, the Coulomb interaction is modulated by the dielectric constant of the medium. Highly polar solvents have high dielectric constants. Water, for example, has a dielectric constant ε = 78 (at interfaces this number is much lower as movement of the water dipoles is more restricted). This leads to a large reduction in the Coulombic potential between ions in polar solvents and can lead to the solvation or hydration of a salt in a solution (Figure 7.4). The hydration of cations and anions is responsible for the high solubility of many ionic compounds in water. When molecules are in close contact, U(r) is typically ∼10−18 J, corresponding to about 200–300 kT (where k is the Boltzmann constant and T the temperature in Kelvin) at room temperature. To contrast (Equation 7.2 with n = 1 and C =
Na+
The Coulomb electrostatic interaction potential between two charges (Figure 7.3) is represented by the following equation: Q1Q 2 4 PE 0 E r
Q1
H2O
Types of Interparticle Interaction Forces
U(r )
Q2
Cl–
Hydrated Na+ ion
Hydrated Cl– ion
(7.5) FIGURE 7.4 Solvation power of water. NaCl dissolution.
Electrochemical and Optical Analytical Techniques
m2
523
m1 r
FIGURE 7.5 Gravitational interaction between two molecules.
this Coulomb interaction with the gravity interaction of molecules (Figure 7.5), consider that the gravitational interaction energy is given by: U(r)
gm1m 2 r
(7.6)
This is equivalent to Equation 7.2 with n = 1 and C = gm1m2. In this expression the gravitational constant g = 6.67 × 10−11 Nm2kg−1, and for molecules in contact this leads to a negligible gravitational interaction energy U(r) of about 10−52 J compared with 10−18 J for the Coulomb interaction energy. The Coulomb interaction is an electrostatic interaction, i.e., such an interaction may occur between charged atomic or molecular species (ions = monopoles) or between asymmetric charge distributions in neutral molecules (e.g., dipoles, quadrupoles, etc.). A dipole is an asymmetric charge distribution in a molecule, where there is no net charge; however, one end of the molecule is negative (partial charge = −q) relative to the other (partial charge = +q). Molecules may possess higherorder electric multipoles, arising from their nonspherical charge distributions (Figure 7.6). Each type of multipole has an associated multipole moment: the monopole moment is the charge of the atom/ molecule; the dipole moment is a vector whose magnitude is the product of the charge (q) and distance (λ) between the charge centers (μ = qλ). Higherorder multipole moments have tensor properties. A polar molecule is one that possesses a permanent dipole moment: there is an asymmetric charge distribution, with one end of the molecule relatively negative (−q) with respect to the other (+q). The interaction energy between a stationary point charge Q2 and a permanent fixed dipole μ1 separated by a distance r is given as (Figure 7.7): U(r )
Q 2M1 cos Q 4 PE 0 E r 2
FIGURE 7.6 Electric quadrupole. Four charges, two positive and two negative. The arrows depict the electric fields, and the lines are the equipotential surfaces.
with Q2 = z2e in units of C and μ1 (q1λ) in units of Cm [often expressed in Debye (D), where D = 3.336 10−30 Cm]. The interaction energy now depends on the orientation of the dipole relative to the charge (θ) and the sign of the charge. In the case of a permanent dipole that can freely rotate, one obtains a new expression:
U(r )
Q 22M12
(7.8)
6(4 PE 0 E)2 kTr 4
with k being the Boltzmann constant. Notice that temperature dependence now appears in the denominator. One example of this type of interaction is the condensation of water (μ = 1.65 D) caused by the presence of ions in water. During a thunderstorm, ions are created that nucleate raindrops in thunderclouds (ionic nucleation). When an electric charge (i.e., an ion = electric monopole) or asymmetric charge distribution (e.g., Na+
Iondipole interaction –
+
I– +
(7.7) FIGURE 7.7 Iondipole interaction.
–
524
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
dipole, quadrupole, etc.) gives rise to an electric field (E) that causes the polarization of neighboring nonpolar atoms or molecules, an induced dipole is created. The magnitude of the induced dipole is: M AE
(7.9)
where α is the polarizability of the neutral atom or molecule. Polarizability is the ease with which the electron distribution in the atom or molecule can be distorted. Polarizability increases as the number of electrons increases and as the electron cloud becomes more diffuse (larger molecules). An ioninduced dipole interaction energy is given as: U(r )
Q12A 2 2(4 PE 0 E)2 r 4
(7.10)
Van der Waals Forces To explain deviations from ideal gas behavior (equation of state by Boyle and GayLussac: PV = RT), van der Waals, in 1873, proposed a modification to the equation of state of a gas as follows: a ´ ¥ ¦§ P 2 µ¶ V b RT V
(7.11)
This new expression accounted for the fact that molecules have a finite volume (b) and that there is an attractive force between these molecules (a). This relation correctly predicts gas behavior over a wider pressure range. The attractive intermolecular forces between gas molecules are now known as van der Waals forces. The three types of interactions that constitute van der Waals forces are summarized in Table 7.3. The exponent n = 6 indicates that these types of van der
Waals forces are short range. The attractive interactions between dipoles, quadrupoles, and between permanent multipoles are sometimes named after Keesom. Another source of attraction is induction (i.e., polarization), which is the interaction between a permanent dipole or multipole on one molecule with an induced dipole or multipole. This interaction is named after Debye. The third type of attraction, London forces, is named after the GermanAmerican physicist Fritz London, who himself called it dispersion forces. This is the only attraction experienced by noble gas atoms, but it is operative between any pair of molecules, regardless of their symmetry. London dispersion forces are weak intermolecular forces that arise from the attractive forces between transient dipoles (or multipoles) in molecules without permanent dipole (or multipole) moments. We will see that the London component is often the most dominant interaction from the three interactive forces. DipoleDipole Interactions—Keesom The expression for the interaction energy of two fixed dipoles, μ1 and μ2, that are not coplanar (i.e., there is an angle ϕ between them) is calculated as: M12M 22 f (Q1 , Q2 , F)
U(r )
4 PE 0 Er 3
where r is the distance between the centers of mass of the two molecules. The expression for two freely rotating dipoles, the socalled Keesom equation, is given as: U(r )
M12M 22 3(4 PE 0 E)2 kTr 6
TABLE 7.3 Types of van der Waals Forces Interaction Component
(7.12)
Origin of Interactions
Equation M12M 22 3( 4 PE 0 E)2kTr 6
Keesom
Dipoledipole
Debye (induction)
Dipoleinduced dipole
U(r )
London (dispersion)
Induced dipoleinduced dipole
U(r )
U(r )
M12A 2 ( 4 PE 0 E)2r 6
3A 2hN 4( 4 PE 0 E )2r 6
(7.13)
Electrochemical and Optical Analytical Techniques
Here a temperature dependence of the interaction energy appears. Dipoledipole interactions are generally weak. These dipoledipole interactions become significant when two interacting dipoles approach each other closely, e.g., in O δ− —Hδ+, Nδ− —Hδ+, Fδ− —Hδ+, etc. Such strong dipoledipole interactions are the underlying reason for the wellknown hydrogen bonds (see below). The electrostatic interaction between higherorder multipoles can be treated in an analogous fashion to that described here for dipoledipole interactions. The distance dependence of the interaction energy between an npole and an mpole (assuming no molecular rotation) is given as: U(r) t p
1 r
DipoleInduced Dipole Interactions—Debye An induced dipole interacts in an attractive fashion with a fixed, permanent dipole (μ1). The inductive interaction energy between the fixed permanent dipole (μ1) associated with molecule 1 and the induced dipole on molecule 2 (which has no fixed dipole but has certain polarizability α2 and is a distance r away from molecule 1) is given by:
M12A 2 1 3 cos 2 Q 2 6
2(4 P E 0 E) r
(7.15)
TABLE 7.4 Interaction Energies between an nPole and an mPole Interaction Energies for… Monopolemonopole (coulomb) Monopoledipole Dipoledipole Dipolequadrupole Quadrupolequadrupole
In the case where the permanent dipole is free to rotate, the socalled Debye interaction energy results: U(r )
M12A 2 (4 PE 0 E)2r 6
(7.16)
As the direction of the induced dipole follows that of the permanent dipole, the effect survives even if the permanent dipole is subjected to thermal reorientations. Debye interactions are thus independent of temperature. Dipoles (and higher multipoles) may also be induced by neighboring molecules featuring permanent charges (monopoles) or by highorder multipoles. Similar expressions can be derived for the interactions between these permanent and induced multipoles.
(7.14)
( n m 1)
where n and m are the orders of the multipoles: n, m = 1 (monopole), 2 (dipole), 3 (quadrupole), 4 (octopole), etc. (Table 7.4). It is noted that the higher the order of the multipole, the shorter ranged the interaction is, i.e., the more rapidly it falls off with distance.
U(r )
525
U(r) ∝ r−1 U(r) ∝ r−2 U(r) ∝ r−3 U(r) ∝ r−4 U(r) ∝ r−5
Induced DipoleInduced Dipole—Dispersive or London Forces The intermolecular forces between nonpolar molecules and closed shell atoms (e.g., rare gas atoms such as He, Ne, and Ar) are the “London” or dispersion forces, attractive forces that arise as a result of temporary dipoles, which are induced in atoms or molecules (Figure 7.8). Keesom and Debye interactions require the presence of at least one permanent dipole, but London interactions do not. Hence, London interactions exist between all molecules. It is also generally the dominant contribution to van der Waals forces. The London interaction component was known for a long time, but the theory only evolved after the development of quantum mechanics. Nonpolar molecules exhibit London forces because electron density moves about a molecule probabilistically. There is a high chance that the electron density will not be evenly distributed throughout a nonpolar molecule. When an uneven distribution occurs, a temporary multipole is created, which may interact with other nearby multipoles. London forces are also present in polar molecules, but they are usually only a small part of the total interaction force. This phenomenon is the only attractive intermolecular force between neutral atoms (e.g., helium) and is the major attractive force between nonpolar molecules (e.g., nitrogen or methane). Without London forces, there would be no attractive force between noble gas atoms, and they could not then be obtained in a liquid form.
526
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
FIGURE 7.8 Induced dipoleinduced dipole interaction. Dispersion or “London” forces in helium atoms (a) before the dipole and (b) with the dipole.
A general expansion for the attractive energy resulting from these dispersion forces can be written as: «C C C C º U(r ) ¬ 66 88 1010 ! nn » r r r ¼ r
(7.17)
where the Cn terms are constants and r is the interatomic distance. The first term represents the instantaneous dipoledipole interaction and is the dominant variable; therefore, the higher terms (which contribute less than 10% of the total dispersion energy) are often omitted when calculating dispersion energies. A reasonable approximation to the dispersion energy is found in the London formula (derived by London in 1930, based on a model by Drude), in which the dispersion energy between two identical atoms/molecules is given as: U(r )
C6 r6
3A 2 hN 4(4 PE 0 E)2r 6
(7.18)
where α is the polarizability and hν is the ionization energy of the atom/molecule. The polarizability α is squared in Equation 7.18 because the magnitude of the instantaneous dipole depends on the polarizability of the first atom/molecule. The strength of the induced dipole (in the second atom/molecule) also depends on α. When molecules are in close contact, U(r) is typically ∼10−21–10−20 J/mol, corresponding to about 0.2–2 kT at room temperature, which is a comparable magnitude to the thermal energy. London forces become stronger as the atom (or molecule) in question becomes larger. This is because of the increased polarizability of molecules with larger, more dispersed electron clouds. London forces provide molecular level reasoning that at room temperature small molecules such as Ar, He,
and CH4 are gases, whereas larger molecules, like hexane and decane, are liquids, and yet even larger molecules are solids. Interactions involving charged species (e.g., ions) tend to be stronger than polarpolar interactions. All intermolecular forces are anisotropic (except those between two noble gas atoms), which means that they depend on the relative orientation of the molecules. The induction and dispersion interactions are always attractive, but the electrostatic interaction changes sign on rotation of the molecules (can be attractive or repulsive, depending on the mutual orientation of the multipoles). When molecules are in thermal motion, as they are in the gas and liquid phase, the electrostatic forces are diminished to a large extent because the molecules thermally rotate and thus probe both repulsive and attractive parts of the potential. The thermal averaging effect is much less pronounced for induction and dispersion forces. Further below we will see that the Londonvan der Waals forces are related to the quantum mechanical Casimir effect introduced in Chapter 3 (Figure 3.69). The latter is sometimes referred to as the retarded van der Waals force. Example of DipoleDipole Interaction: Hydrogen Bonding Earlier we saw that weak dipoledipole interactions can become significant when two interacting dipoles approach each other closely, e.g., in Oδ− —Hδ+, Nδ− —Hδ+, Fδ− —Hδ+, and so on. Such strong dipoledipole interactions are the underlying reason for hydrogen bonds. Hydrogen bonding is an intermolecular linkage of the form X—H—Y, where a hydrogen atom is bound to one electronegative atom (e.g., X=N, O, F) and interacts with a second electronegative atom (Y) that has an available pair
Electrochemical and Optical Analytical Techniques
of free electrons. For example, X—H is the hydrogen bond donor (e.g., O—H, peptide N—H), and Y is the hydrogen bond acceptor (e.g., :O, :N, peptide C=O). The donor is, in this case, an acid (proton donor), whereas the acceptor is a base (proton acceptor). A hydrogen bond is stronger than most other nonbonded interactions. Typical hydrogen bond strength is 10–40 kJ mol−1 (about 10% of a covalent bond). A rare strong Hbond may be 60 kJ mol−1 when the donor and acceptor are very close for significant orbital overlap. Hydrogen bonding is especially strong when H is attached to F, O, or N because these three elements all have high electronegativity and are small enough to get close to. Most biological Hbonds are ∼2.8 Å (e.g., O—H…O is 2.7 Å and O—H…N is 2.9 Å). Water forms hydrogen bonds: the O—H bonds act as Hbond donors, and the O lone pairs act as Hbond acceptors (Figure 7.9). The proton in the water molecule is unshielded and makes an electropositive end to the bond, which explains the partial ionic character of the hydrogen bond. Most of the unique properties of water are the result of this hydrogen bonding and its polar nature. Water, we saw above, is a good solvent for ionic species because it has a high dielectric constant. Each molecule of water in the solid state (ice, see Figure 7.10) is engaged in 4.0 hydrogen bonds (accepting two and donating two), and each molecule of water in the liquid state is engaged in approximately 3.4 !
!
!
FIGURE 7.9 Hydrogen bonding in water. The structure of a water molecule (a) makes it a perfect hydrogen bond donor (b) and acceptor (c).
527
FIGURE 7.10 In ice, water molecules form an Hbonded network that fully satisfies the Hbonding potential (4 per H2O).
hydrogen bonds that are transitory in nature. With fewer hydrogen bonds, the oxygen atoms may on average be closer to each other (denser). About 15% of Hbonds break when ice melts. As a consequence, water is denser than ice. The hydrogen bond endows specificity to an interaction as particular atoms are required as donors and acceptors. It also imposes geometrical constraints; hydrogen bonds, like covalent bonds, are highly directional. The X—H—Y bond is optimally a straight line (see Figure 7.9c), where the donor H bond tends to point directly at the acceptor electron pair. The major component (around 80%) of a hydrogen bond is electrostatic, whereas other contributions are inductive and dispersion forces. It is the latter forces that impose the directionality in the direction of the acceptor lone pair. Hydrogen bonding plays a very important role in biology, being responsible for the structural organization of proteins and other biomolecules. Actually, the existence of life on Earth is a direct consequence of the hydrogen bonding present in water and the wide temperature range over which water remains liquid (0–100°C). Also, the tetrahedral threedimensional (3D) structure of ice and the local structure of liquid water is a consequence of hydrogen bonding. We will come back to hydrogen bonding in discussions on protein folding, DNA, and selfassembly
528
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
(Volume III, Chapters 2−4). In the gas phase, the optimal Hbond strength between water molecules is ∼23 kJ mol−1. The Hbonding in condensed phases of water is cooperative (nonadditive), and the strength of Hbonding increases with increasing number of water molecules, as this increases the polarization of the O—H bonds. This is observed as an increase in the average dipole moment (μ) per water molecule, which increases from 1.85 D (isolated H2O) to 2.4−2.6 D (liquid H2O at 0°C). In Table 7.5, we summarize what we have learned about intermolecular forces thus far. We describe the type of interaction, give a model and an example, and list the distance dependence of the energy.
to combine them to describe the exact shape of the curve in Figure 7.2 for the total potential energy of interaction between two neutral atoms or polar molecules as a function of the distance between them. In combining forces, one typically groups the attractive forces between polar and nonpolar molecules in the socalled van der Waals force. This refers to all electrostatic induction and dispersion interactions between polar and nonpolar molecules, varying as r −6. From Table 7.3, van der Waals forces include Keesom (dipoledipole), Debye (dipoleinduced dipole), and London dispersive interactions (induced dipoleinduced dipole). These shortrange forces (n = 6) can all be expressed as: U(r)
The LennardJones Potential Having introduced the equations for repulsive and attractive intermolecular forces we are now ready
C r6
(7.19)
The most important component of the van der Waals force, as seen earlier, is the London term.
TABLE 7.5 Intermolecular Energy Dependence on Distance for Various Types of Interactions Type of Interaction
Model
(a) Chargecharge Longestrange force; nondirectional (b) Chargedipole (fixed) Depends on orientation of dipole (c) Dipoledipole Depends on mutual orientation of dipole (d) Chargeinduced dipole Depends on polarizability of molecule in which dipole is induced (e) Dipoleinduced dipole Depends on polarizability of molecule in which dipole is induced (f) DispersionLondon forces Involves mutual synchronization of fluctuating charges (g) Fermi repulsion Occurs when outer electron orbitals overlap (h) Hydrogen bond Charge attraction + partial covalent bond
+
q– q+
q– q+
+
q– q+
q– q+
q– q+
−
NH3
–
q– q+
1/r
O
+
+
Dependence of Energy on Distance
Example
O
C
H + – NH3 q O q+ H q–O Hq+ q– H + O q H H
NH3
q– q+
q–O Hq+ q– q+ H q+
q–
q– q+
q+
q–
1/r6
1/r6
1/r12
– –
q–
1/r3
1/r4
+
q– q–
q+
1/r2
Length of bond fixed
N
H
O
C
Electrochemical and Optical Analytical Techniques
Regardless of other interactions found within a complex system of atoms and molecules, there will almost always be a contribution from van der Waals forces. Taking into account both repulsive and attractive interactions, a good approximation to the total potential energy of interaction between two neutral atoms or polar molecules is given by the LennardJones potential: U(r)
B C
r12 r 6
(7.20)
The C/r6 term is the attractive van der Waals term, also known as the dispersive term (Equation 7.19). The term B/r12 describes the hardcore repulsion, also known as Fermi repulsion, and stems from the Pauli exclusion principle. Atoms are treated here as hard spheres with diameter σ [in the extreme; d
¥ S´ U(r) = ¦ µ ]. This leads to a potential expression of §r¶ the following form: «® ¥ S ´ 12 ¥ S ´ 6 º® U(r ) 4 E ¬ ¦ µ ¦ µ » §r¶ ® ® § r ¶ ¼
«® ¥ S12 ´ ¥ S 6 ´ º® dU 24 E ¬ 2 ¦ 13 µ ¦ 7 µ » dr ® § r ¶ § r ¶ ¼®
In Equation 7.21, ε is the depth of the energy well and σ is the separation at which U(r) = 0. The equilibrium separation, i.e., the position of the m inimum in U(r), occurs at re = 21/6 × σ [U(r) = −ε]. The van der Waals’ radii (σ) of atoms, which is the size of an atom or the preferred distance atoms will pack to if no other significant interactions occur, may be calculated from this equation. The increase in ε when going from lighter to heavier rare gases reflects the increase in the attractive dispersion forces because of the higher polarizability that occurs as a result of the lower effective nuclear charge experienced by the outer electrons in the heavier rare gas atoms. As molecules are larger and (usually) more polarizable than rare gas atoms, typical binding energies caused by dispersion forces are of the order ε ≈ 10 kJ mol−1 per intermolecular interaction. The interactive attraction forces are the derivative of the van der Waals term, and these contributions (polar or nonpolar) all decrease as 1/r7. In all cases, substituting numerical values in Equation 7.22, these forces do not exceed a range of a few nanometers.
(7.21) Example 7.1:
as illustrated in Figure 7.11. The force between the two molecules is derived from the LennardJones potential as: F(r )
529
The magnitude of the dispersion energy for two methane molecules separated by 0.3 nm is approximately −4.7 kJ mol−1, i.e., ε ≈ 4.7 kJ mol−1.
(7.22)
Calculating Interaction Forces between Surfaces and Particles Introduction
U(r)
ULJ + r–12
0 σ
re ULJ – r–6
Thus far, we have mainly discussed intermolecular forces at work between various types of molecules. Now we turn our attention to the detailed nature of the attractive and repulsive forces at an interface between a liquid and a solid. Based on this knowledge, we will be ready to introduce the electrode/ liquid interface and the electrochemical principles that enable electrochemical sensors. Van der Waals Forces on Solid Surfaces
ε r
FIGURE 7.11 The LennardJones potential.
Van der Waals forces for molecules, we saw, vary as 1/r7 (Equation 7.22), with r being the distance between them. In 1937, Hamaker calculated the
530
SolidState Physics, Fluidics, and Analytical Techniques in Micro and Nanotechnology
TABLE 7.6 Hamaker Constants H for Various Materials in 10−20 J Material 6HSiC tetraZrO2 βSi3N4 αAl2O3 Y2O3 MgO MgAl2O4 SiO2
Vacuum
Medium Water
nDodecane
25 20 18 15 13 12 13 6.5
13 8.8 7.0 5.2 4.0 3.2 3.5 0.83
1 6.8 5.0 3.6 2.6 1.9 2.1 0.15
Example 7.2: Considering only van der Waals attraction, what is the force and energy of adhesion between two particles of radius 1 μm with H = 10−19 J? (L0 = 3 Å). The force of adhesio